1,126 112 18MB
English Pages [546] Year 2020
Table of contents :
Preface to the Second Edition
Preface to the First Edition
Contents
About the Author
Abbreviations
1 Introduction
1.1 Epitaxy
1.1.1 Roots of Epitaxy
1.1.2 Epitaxy and BulkCrystal Growth
1.2 Issues of Epitaxy
1.2.1 Convention on Use of the Term ``Atom''
1.2.2 Assembly of Atoms
1.2.3 Tasks for Epitaxial Growth
References
2 Structural Properties of Heterostructures
2.1 Basic Crystal Structures
2.1.1 Notation of Planes and Directions
2.1.2 Wafer Orientation
2.1.3 FaceCentered Cubic and Hexagonal ClosePacked Structures
2.1.4 Zincblende and Diamond Structures
2.1.5 Rocksalt and CesiumChloride Structures
2.1.6 Wurtzite Structure
2.1.7 Thermal Expansion
2.1.8 Structural Stability Map
2.1.9 Polytypism
2.1.10 Random Alloys and Vegard's Rule
2.1.11 VirtualCrystal Approximation
2.2 Elastic Properties of Heterostructures
2.2.1 Strain in One and Two Dimensions
2.2.2 ThreeDimensional Strain
2.2.3 Hooke's Law
2.2.4 Poisson's Ratio
2.2.5 Pseudomorphic Heterostructures
2.2.6 Critical Layer Thickness
2.2.7 Approaches to Extend the Critical Thickness
2.2.8 Partially Relaxed Layers and Thermal Mismatch
2.3 Dislocations
2.3.1 Edge and Screw Dislocations
2.3.2 Motion of Dislocations
2.3.3 Dislocation Network
2.3.4 Dislocations in the fcc Structure
2.3.5 Dislocations in Diamond and Zincblende Structures
2.3.6 Dislocation Energy
2.3.7 Dislocations in the hcp and Wurtzite Structures
2.3.8 Antiphase Domains
2.3.9 Mosaic Crystal
2.4 Structural Characterization Using XRay Diffraction
2.4.1 Bragg's Law
2.4.2 The Structure Factor
2.4.3 The Reciprocal Lattice
2.4.4 The Ewald Construction
2.4.5 HighResolution Scans in the Reciprocal Space
2.4.6 ReciprocalSpace Map
2.5 Problems Chapter 2
2.6 General Reading Chapter 2
References
3 Structure of Organic Crystals
3.1 Building Blocks in Organic Crystals
3.1.1 Bonding in Organic Crystals
3.1.2 SmallMolecule Crystals
3.1.3 Polymers
3.2 SubstrateLayer Relation and Defects of Organic Crystals
3.2.1 SubstrateLayer Relation of Organic Crystals
3.2.2 Ordered Pentacene Layers
3.2.3 Defects in SmallMolecule Crystals
3.2.4 Defects in Polymers
3.3 Problems Chapter 3
3.4 General Reading Chapter 3
References
4 Electronic Properties of Heterostructures
4.1 Bulk Properties
4.1.1 Electronic Bands of Zincblende and Wurtzite Crystals
4.1.2 Strain Effects
4.1.3 Spontaneous Polarization and Piezoelectricity
4.1.4 Temperature Dependence of the Bandgap
4.1.5 Bandgap of Alloys
4.2 Band Offsets
4.2.1 ElectronAffinity Rule
4.2.2 CommonAnion Rule
4.2.3 Model of Deep Impurity Levels
4.2.4 InterfaceDipol Theory
4.2.5 ModelSolid Theory
4.2.6 Offsets of Some Isovalent Heterostructures
4.2.7 Band Offset of Heterovalent Interfaces
4.2.8 Band Offsets of Alloys
4.3 Electronic States in LowDimensional Structures
4.3.1 Dimensionality of the Electronic DensityofStates
4.3.2 Characteristic Scale for Size Quantization
4.3.3 Quantum Wells
4.3.4 Quantum Wires
4.3.5 Quantum Dots
4.4 Problems Chapter4
4.5 General Reading Chapter4
References
5 Electronic Properties of Organic Semiconductors
5.1 Band Structure of Organic Crystals
5.1.1 Highest Occupied and Lowest Unoccupied Molecular Orbitals
5.1.2 Bands and Bandgaps in Organic Crystals
5.1.3 Excitons in Organic Crystals
5.2 Transport in Organic Semiconductors
5.2.1 Polarons
5.2.2 Mobility of Carriers in Organic Semiconductors
5.3 Interfaces in Organic Semiconductors
5.3.1 OrganicOrganic Heterointerface
5.3.2 OrganicMetal Interface
5.4 Problems Chapter 5
5.5 General Reading Chapter 5
References
6 Thermodynamics of Epitaxial LayerGrowth
6.1 Phase Equilibria
6.1.1 Thermodynamic Equilibrium
6.1.2 Gibbs Phase Rule
6.1.3 Gibbs Energy of a SingleComponent System
6.1.4 Phases Boundaries in a SingleComponent System
6.1.5 Driving Force for Crystallization
6.1.6 TwoComponent System
6.2 Crystalline Growth
6.2.1 Homogeneous ThreeDimensional Nucleation
6.2.2 Heterogeneous ThreeDimensional Nucleation
6.2.3 Growth Modes
6.2.4 Equilibrium Surfaces
6.2.5 TwoDimensional Nucleation
6.2.6 Island Growth and Coalescence
6.2.7 Growth without Nucleation
6.2.8 Ripening Process After Growth Interruption
6.3 Problems Chapter 6
6.4 General Reading Chapter 6
References
7 Atomistic Aspects of Epitaxial LayerGrowth
7.1 Surface Structure
7.1.1 The Kink Site of a Kossel Crystal
7.1.2 Surfaces of a Kossel Crystal
7.1.3 Relaxation and Reconstruction
7.1.4 ElectronCounting Model
7.1.5 Denotation of Surface Reconstructions
7.1.6 Reconstructions of the GaAs(001) Surface
7.1.7 The Silicon (111)(7times7) Reconstruction
7.2 Kinetic Process Steps in Layer Growth
7.2.1 Kinetics in the TerraceStepKink Model
7.2.2 Atomistic Processes in Nucleation and Growth
7.2.3 Adatoms on a Terraced Surface
7.2.4 Growth by Step Advance
7.2.5 The EhrlichSchwoebel Barrier
7.2.6 Effect of the EhrlichSchwoebel Barrier on Surface Steps
7.2.7 Roughening of Surface Steps
7.2.8 Growth of a Si(111)(7times7) Surface
7.2.9 Growth of a GaAs(001) β2(2times4) Surface
7.3 Selforganized Nanostructures
7.3.1 StranskiKrastanow Island Growth
7.3.2 Thermodynamics Versus Kinetics in Island Formation
7.3.3 Wire Growth on Nonplanar Surfaces
7.4 Problems Chapter7
7.5 General Reading Chapter7
References
8 In Situ Growth Analysis
8.1 Surface and Ambient Probing
8.2 In Situ Ambient Analysis
8.2.1 Quadrupole Mass Spectrometry
8.2.2 Optical Ambient Probing
8.3 SurfaceSensitive Diffraction Techniques
8.3.1 Reflection HighEnergy Electron Diffraction (RHEED)
8.3.2 Grazing Incidence XRay Diffraction (GIXD) and Reflection
8.4 Optical in Situ Surface Probes
8.4.1 Pyrometry
8.4.2 Deflectometry
8.4.3 Reflectance and Ellipsometry
8.4.4 ReflectanceDifference Spectroscopy
8.5 Problems Chapter 8
8.6 General Reading Chapter 8
References
9 Application of Surfactants
9.1 The Surfactant Effect
9.1.1 Concept of SurfactantMediated Growth
9.1.2 Evidence for the Surfactant Effect
9.1.3 SurfactantMediated Ge/Si Epitaxy
9.1.4 SurfactantMediated Epitaxy of III–V Semiconductors
9.2 Models of SurfactantAssisted Epitaxy
9.2.1 Thermodynamic Considerations
9.2.2 Kinetic Approach
9.2.3 The Diffusion—Deexchange—Passivation (DDP) Model
9.2.4 Exchange Pathways in SurfactantMediated Epitaxy
9.3 Conclusion
9.4 Problems Chapter 9
9.5 General Reading Chapter 9
References
10 Doping, Diffusion, and Contacts
10.1 Doping of Semiconductors
10.1.1 Thermal Equilibrium CarrierDensities
10.1.2 Solubility of Dopants
10.1.3 Amphoteric Dopants
10.1.4 Compensation by Native Defects
10.1.5 Hydrogen Compensation and Passivation
10.1.6 DX Centers
10.1.7 FermiLevel Stabilization Model
10.1.8 Delta Doping and Modulation Doping
10.2 Diffusion
10.2.1 Diffusion Equations
10.2.2 Diffusion Mechanisms
10.2.3 Effective Diffusion Coefficients
10.2.4 Disordering of Heterointerfaces
10.3 MetalSemiconductor Contact
10.3.1 Ideal Schottky Contact
10.3.2 Real MetalSemiconductor Contact
10.3.3 Practical Ohmic MetalSemiconductor Contact
10.3.4 Epitaxial Contact Structures
10.4 Problems Chap.6
10.5 General Reading Chap.6
References
11 Methods of Epitaxy
11.1 LiquidPhase Epitaxy
11.1.1 Growth Systems
11.1.2 Congruent Melting
11.1.3 LPE Principle
11.1.4 LPE Processes
11.2 Metalorganic VaporPhase Epitaxy
11.2.1 Metalorganic Precursors
11.2.2 The Growth Process
11.2.3 Mass Transport
11.3 Molecular Beam Epitaxy
11.3.1 MBE System and Vacuum Requirements
11.3.2 Beam Sources
11.3.3 Uniformity of Deposition
11.3.4 Adsorption of Impinging Particles
11.4 Problems Chapter 11
11.5 General Reading Chapter111
References
12 Special Growth Techniques
12.1 Selective Area Growth
12.1.1 Principle of Selective Area Growth
12.1.2 Conditions for Selectivity
12.1.3 Selective Area Growth of Faceted Structures
12.1.4 Epitaxial Lateral Overgrowth (ELO)
12.2 Vapor–Liquid–Solid Growth of Nanowires
12.2.1 Outline of the VLS Method
12.2.2 Growth of Si Nanowires
12.2.3 Growth of III–V Nanowires
12.3 Atomic Layer Epitaxy and Related Techniques
12.3.1 Atomic Layer Epitaxy (ALE)
12.3.2 MigrationEnhanced Epitaxy (MEE)
12.3.3 Atomic Layer Deposition (ALD)
12.4 Deposition of Organic Crystals
12.4.1 Methods of Organic Layer Deposition
12.4.2 Epitaxy of Organic Semiconductors
12.5 General Reading Chapter 12
References
Appendix
Index
Fundamental Physical Constants
Graduate Texts in Physics
Udo W. Pohl
Epitaxy of Semiconductors Physics and Fabrication of Heterostructures Second Edition
Graduate Texts in Physics Series Editors Kurt H. Becker, NYU Polytechnic School of Engineering, Brooklyn, NY, USA JeanMarc Di Meglio, Matière et Systèmes Complexes, Bâtiment Condorcet, Université Paris Diderot, Paris, France Sadri Hassani, Department of Physics, Illinois State University, Normal, IL, USA Morten HjorthJensen, Department of Physics, Blindern, University of Oslo, Oslo, Norway Bill Munro, NTT Basic Research Laboratories, Atsugi, Japan William T. Rhodes, Department of Computer and Electrical Engineering and Computer Science, Florida Atlantic University, Boca Raton, FL, USA Susan Scott, Australian National University, Acton, Australia H. Eugene Stanley, Center for Polymer Studies, Physics Department, Boston University, Boston, MA, USA Martin Stutzmann, Walter Schottky Institute, Technical University of Munich, Garching, Germany Andreas Wipf, Institute of Theoretical Physics, FriedrichSchillerUniversity Jena, Jena, Germany
Graduate Texts in Physics publishes core learning/teaching material for graduate and advancedlevel undergraduate courses on topics of current and emerging ﬁelds within physics, both pure and applied. These textbooks serve students at the MS or PhDlevel and their instructors as comprehensive sources of principles, deﬁnitions, derivations, experiments and applications (as relevant) for their mastery and teaching, respectively. International in scope and relevance, the textbooks correspond to course syllabi sufﬁciently to serve as required reading. Their didactic style, comprehensiveness and coverage offundamental material also make them suitable as introductions or references for scientists entering, or requiring timely knowledge of, a research ﬁeld.
More information about this series at http://www.springer.com/series/8431
Udo W. Pohl
Epitaxy of Semiconductors Physics and Fabrication of Heterostructures Second Edition
123
Udo W. Pohl Institute of Solid State Physics Technische Universität Berlin Berlin, Germany
ISSN 18684513 ISSN 18684521 (electronic) Graduate Texts in Physics ISBN 9783030438685 ISBN 9783030438692 (eBook) https://doi.org/10.1007/9783030438692 1st edition: © SpringerVerlag Berlin Heidelberg 2013 2nd edition: © Springer Nature Switzerland AG 2020 This work is subject to copyright. All rights are reserved by the Publisher, whether the whole or part of the material is concerned, speciﬁcally the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting, reproduction on microﬁlms or in any other physical way, and transmission or information storage and retrieval, electronic adaptation, computer software, or by similar or dissimilar methodology now known or hereafter developed. The use of general descriptive names, registered names, trademarks, service marks, etc. in this publication does not imply, even in the absence of a speciﬁc statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. The publisher, the authors and the editors are safe to assume that the advice and information in this book are believed to be true and accurate at the date of publication. Neither the publisher nor the authors or the editors give a warranty, express or implied, with respect to the material contained herein or for any errors or omissions that may have been made. The publisher remains neutral with regard to jurisdictional claims in published maps and institutional afﬁliations. This Springer imprint is published by the registered company Springer Nature Switzerland AG The registered company address is: Gewerbestrasse 11, 6330 Cham, Switzerland
Preface to the Second Edition
The book Epitaxy of Semiconductors has been well received by students and the scientiﬁc community. The ﬁrst edition focused concisely on the very basics and omitted quite a number of important aspects. In the second edition, I therefore added a few new chapters and also amended the initial text. The new parts comprise the emerging ﬁeld of organic semiconductors with their speciﬁc peculiarities and the important in situ analysis of epitaxial growth, which is today routinely implemented in commercial growth systems for online monitoring and control. A chapter on the application of surfactants is added, illustrating an additional means to control growth and pointing out the effect of kinetics. One new chapter is dedicated to special techniques, which are applied by all major epitaxy methods MOVPE, MBE, and LPE. Selective area growth is widely employed in nanostructure fabrication and epitaxial lateral overgrowth to create layers with areas of low defect density; migrationenhanced epitaxy is used to improve the performance of MBE, and vaporliquidsolid growth is a popular and versatile method for fabricating nanowires with high quality. I would like to thank my colleagues for critically reading parts of the new manuscript: Armin Dadgar (Univ. Magdeburg), Mario Dähne (TU Berlin), Norbert Esser (ISAS Berlin), and Kolja Haberland (LayTec Berlin). I am indebted to Nigel Mason (Oxford, UK) for stimulating the inclusion of in situ sensing, and I appreciate encouraging comments I received from Ganesh Balakrishnan (Univ. Albuquerque, NM). Berlin September 2019
Udo W. Pohl
v
Preface to the First Edition
Epitaxy—the growth of a crystalline layer on a crystalline substrate—represents the basis for the fabrication of semiconductor heterostructures and devices. Textbooks on semiconductor physics and devices usually describe the design of a heterostructure and subsequently measured data of a respective realization. The chain between these end points requires to solve many basic problems related to physics and technology. Such steps are generally described in specialized literature focusing on diverse aspects. Students and researchers starting in the ﬁeld need to study papers and books on quite speciﬁc problems in a wide ﬁeld. This textbook attempts to bridge the gap between wellestablished books on semiconductor physics on one side and texts on completed heterostructures like semiconductor devices on the other. The book is based on a onesemester course held at Technical University of Berlin for undergraduate and graduate students in physics and engineering physics. It is primarily addressed to the nonspecialist with some basic knowledge in solid state and semiconductor physics. The ﬁeld of epitaxy is rapidly evolving and includes many materials and growth techniques. The text, therefore, focuses on basics and important aspects of epitaxy, emphasizing particularly the physical principles. Problems are illustrated for important semiconductors with zincblende or wurtzite structure. The subject matter ﬁrst covers the properties of heterostructures. Structural aspects implying elasticity and strain relaxation by dislocations are addressed as well as electronic properties including band alignment and electronic states in lowdimensional structures. Then, the thermodynamics and kinetics of epitaxial layer growth are considered, introducing the driving force of crystallization and paying special attention to nucleation and surface structures. Instructive examples are given for selforganized growth of quantum dots and wires. Afterward, aspects of doping, diffusion, and contacts are discussed. Eventually, the most important methods used for epitaxial growth are introduced: metalorganic vaporphase epitaxy, molecularbeam epitaxy, and liquidphase epitaxy.
vii
viii
Preface to the First Edition
I am grateful to my students, who consistently engaged me in discussions about fundamentals of epitaxy and stimulated an active motivation to write this book. I am also indebted to A. Krost for critical manuscript reading, and I appreciated the cooperation with C. Ascheron, Springer Science+Business Media. Berlin July 2012
Udo W. Pohl
Contents
1
Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1 Epitaxy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1.1 Roots of Epitaxy . . . . . . . . . . . . . . . . . 1.1.2 Epitaxy and BulkCrystal Growth . . . . . 1.2 Issues of Epitaxy . . . . . . . . . . . . . . . . . . . . . . . 1.2.1 Convention on Use of the Term “Atom” 1.2.2 Assembly of Atoms . . . . . . . . . . . . . . . 1.2.3 Tasks for Epitaxial Growth . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
1 1 1 4 4 4 5 6 10
2
Structural Properties of Heterostructures . . . . . . . . . . . . . . . . . 2.1 Basic Crystal Structures . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1.1 Notation of Planes and Directions . . . . . . . . . . . . . 2.1.2 Wafer Orientation . . . . . . . . . . . . . . . . . . . . . . . . . 2.1.3 FaceCentered Cubic and Hexagonal ClosePacked Structures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1.4 Zincblende and Diamond Structures . . . . . . . . . . . 2.1.5 Rocksalt and CesiumChloride Structures . . . . . . . . 2.1.6 Wurtzite Structure . . . . . . . . . . . . . . . . . . . . . . . . 2.1.7 Thermal Expansion . . . . . . . . . . . . . . . . . . . . . . . . 2.1.8 Structural Stability Map . . . . . . . . . . . . . . . . . . . . 2.1.9 Polytypism . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1.10 Random Alloys and Vegard’s Rule . . . . . . . . . . . . 2.1.11 VirtualCrystal Approximation . . . . . . . . . . . . . . . 2.2 Elastic Properties of Heterostructures . . . . . . . . . . . . . . . . . 2.2.1 Strain in One and Two Dimensions . . . . . . . . . . . . 2.2.2 ThreeDimensional Strain . . . . . . . . . . . . . . . . . . . 2.2.3 Hooke’s Law . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2.4 Poisson’s Ratio . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2.5 Pseudomorphic Heterostructures . . . . . . . . . . . . . .
. . . .
. . . .
. . . .
13 13 13 15
. . . . . . . . . . . . . . .
. . . . . . . . . . . . . . .
. . . . . . . . . . . . . . .
16 17 19 19 20 22 23 25 29 30 30 31 32 35 36
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
ix
x
Contents
2.2.6 Critical Layer Thickness . . . . . . . . . . . . . . . . . . . . 2.2.7 Approaches to Extend the Critical Thickness . . . . . 2.2.8 Partially Relaxed Layers and Thermal Mismatch . . 2.3 Dislocations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3.1 Edge and Screw Dislocations . . . . . . . . . . . . . . . . 2.3.2 Motion of Dislocations . . . . . . . . . . . . . . . . . . . . . 2.3.3 Dislocation Network . . . . . . . . . . . . . . . . . . . . . . . 2.3.4 Dislocations in the fcc Structure . . . . . . . . . . . . . . 2.3.5 Dislocations in Diamond and Zincblende Structures 2.3.6 Dislocation Energy . . . . . . . . . . . . . . . . . . . . . . . . 2.3.7 Dislocations in the hcp and Wurtzite Structures . . . 2.3.8 Antiphase Domains . . . . . . . . . . . . . . . . . . . . . . . 2.3.9 Mosaic Crystal . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4 Structural Characterization Using XRay Diffraction . . . . . . 2.4.1 Bragg’s Law . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4.2 The Structure Factor . . . . . . . . . . . . . . . . . . . . . . . 2.4.3 The Reciprocal Lattice . . . . . . . . . . . . . . . . . . . . . 2.4.4 The Ewald Construction . . . . . . . . . . . . . . . . . . . . 2.4.5 HighResolution Scans in the Reciprocal Space . . . 2.4.6 ReciprocalSpace Map . . . . . . . . . . . . . . . . . . . . . 2.5 Problems Chapter 2 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.6 General Reading Chapter 2 . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . .
40 44 47 49 49 50 52 54 56 57 61 64 65 67 67 68 70 72 73 76 79 83 83
3
Structure of Organic Crystals . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Building Blocks in Organic Crystals . . . . . . . . . . . . . . . . 3.1.1 Bonding in Organic Crystals . . . . . . . . . . . . . . . . 3.1.2 SmallMolecule Crystals . . . . . . . . . . . . . . . . . . . 3.1.3 Polymers . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 SubstrateLayer Relation and Defects of Organic Crystals . 3.2.1 SubstrateLayer Relation of Organic Crystals . . . . 3.2.2 Ordered Pentacene Layers . . . . . . . . . . . . . . . . . . 3.2.3 Defects in SmallMolecule Crystals . . . . . . . . . . . 3.2.4 Defects in Polymers . . . . . . . . . . . . . . . . . . . . . . 3.3 Problems Chapter 3 . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4 General Reading Chapter 3 . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . .
. . . . . . . . . . . . .
. . . . . . . . . . . . .
87 87 88 90 96 97 97 100 103 107 109 111 111
4
Electronic Properties of Heterostructures . . . . . . . . . . . . . 4.1 Bulk Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1.1 Electronic Bands of Zincblende and Wurtzite Crystals . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1.2 Strain Effects . . . . . . . . . . . . . . . . . . . . . . . . 4.1.3 Spontaneous Polarization and Piezoelectricity .
. . . . . . . . . . . . .
. . . . . . . 115 . . . . . . . 115 . . . . . . . 115 . . . . . . . 117 . . . . . . . 123
Contents
xi
4.1.4 Temperature Dependence of the Bandgap . . . . . . 4.1.5 Bandgap of Alloys . . . . . . . . . . . . . . . . . . . . . . . 4.2 Band Offsets . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2.1 ElectronAfﬁnity Rule . . . . . . . . . . . . . . . . . . . . . 4.2.2 CommonAnion Rule . . . . . . . . . . . . . . . . . . . . . 4.2.3 Model of Deep Impurity Levels . . . . . . . . . . . . . 4.2.4 InterfaceDipol Theory . . . . . . . . . . . . . . . . . . . . 4.2.5 ModelSolid Theory . . . . . . . . . . . . . . . . . . . . . . 4.2.6 Offsets of Some Isovalent Heterostructures . . . . . 4.2.7 Band Offset of Heterovalent Interfaces . . . . . . . . . 4.2.8 Band Offsets of Alloys . . . . . . . . . . . . . . . . . . . . 4.3 Electronic States in LowDimensional Structures . . . . . . . 4.3.1 Dimensionality of the Electronic DensityofStates 4.3.2 Characteristic Scale for Size Quantization . . . . . . 4.3.3 Quantum Wells . . . . . . . . . . . . . . . . . . . . . . . . . 4.3.4 Quantum Wires . . . . . . . . . . . . . . . . . . . . . . . . . 4.3.5 Quantum Dots . . . . . . . . . . . . . . . . . . . . . . . . . . 4.4 Problems Chapter 4 . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.5 General Reading Chapter 4 . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5
6
Electronic Properties of Organic Semiconductors . . . . . . . . . 5.1 Band Structure of Organic Crystals . . . . . . . . . . . . . . . . 5.1.1 Highest Occupied and Lowest Unoccupied Molecular Orbitals . . . . . . . . . . . . . . . . . . . . . . 5.1.2 Bands and Bandgaps in Organic Crystals . . . . . . 5.1.3 Excitons in Organic Crystals . . . . . . . . . . . . . . . 5.2 Transport in Organic Semiconductors . . . . . . . . . . . . . . . 5.2.1 Polarons . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.2.2 Mobility of Carriers in Organic Semiconductors . 5.3 Interfaces in Organic Semiconductors . . . . . . . . . . . . . . . 5.3.1 OrganicOrganic Heterointerface . . . . . . . . . . . . 5.3.2 OrganicMetal Interface . . . . . . . . . . . . . . . . . . 5.4 Problems Chapter 5 . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.5 General Reading Chapter 5 . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . .
128 129 133 134 135 136 137 139 139 140 143 144 145 149 151 156 161 169 170 170
. . . . . 177 . . . . . 177 . . . . . . . . . . . .
. . . . . . . . . . . .
. . . . . . . . . . . .
. . . . . . . . . . . .
178 180 185 187 188 190 197 198 200 201 203 203
Thermodynamics of Epitaxial LayerGrowth . . . . . . . . . . . . . . 6.1 Phase Equilibria . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.1.1 Thermodynamic Equilibrium . . . . . . . . . . . . . . . . . 6.1.2 Gibbs Phase Rule . . . . . . . . . . . . . . . . . . . . . . . . . 6.1.3 Gibbs Energy of a SingleComponent System . . . . 6.1.4 Phases Boundaries in a SingleComponent System .
. . . . . .
. . . . . .
. . . . . .
207 207 208 211 212 216
. . . . . . . . . . . .
xii
Contents
6.1.5 Driving Force for Crystallization . . . . . . . . . . 6.1.6 TwoComponent System . . . . . . . . . . . . . . . . 6.2 Crystalline Growth . . . . . . . . . . . . . . . . . . . . . . . . . . 6.2.1 Homogeneous ThreeDimensional Nucleation 6.2.2 Heterogeneous ThreeDimensional Nucleation 6.2.3 Growth Modes . . . . . . . . . . . . . . . . . . . . . . . 6.2.4 Equilibrium Surfaces . . . . . . . . . . . . . . . . . . 6.2.5 TwoDimensional Nucleation . . . . . . . . . . . . 6.2.6 Island Growth and Coalescence . . . . . . . . . . . 6.2.7 Growth without Nucleation . . . . . . . . . . . . . . 6.2.8 Ripening Process After Growth Interruption . . 6.3 Problems Chapter 6 . . . . . . . . . . . . . . . . . . . . . . . . . 6.4 General Reading Chapter 6 . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7
. . . . . . . . . . . . . .
. . . . . . . . . . . . . .
. . . . . . . . . . . . . .
. . . . . . . . . . . . . .
218 221 227 227 230 233 235 241 244 246 247 248 249 249
Atomistic Aspects of Epitaxial LayerGrowth . . . . . . . . . . . . . . 7.1 Surface Structure . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.1.1 The Kink Site of a Kossel Crystal . . . . . . . . . . . . . 7.1.2 Surfaces of a Kossel Crystal . . . . . . . . . . . . . . . . . 7.1.3 Relaxation and Reconstruction . . . . . . . . . . . . . . . 7.1.4 ElectronCounting Model . . . . . . . . . . . . . . . . . . . 7.1.5 Denotation of Surface Reconstructions . . . . . . . . . . 7.1.6 Reconstructions of the GaAs(001) Surface . . . . . . . 7.1.7 The Silicon (111)(7 7) Reconstruction . . . . . . . . 7.2 Kinetic Process Steps in Layer Growth . . . . . . . . . . . . . . . 7.2.1 Kinetics in the TerraceStepKink Model . . . . . . . . 7.2.2 Atomistic Processes in Nucleation and Growth . . . 7.2.3 Adatoms on a Terraced Surface . . . . . . . . . . . . . . . 7.2.4 Growth by Step Advance . . . . . . . . . . . . . . . . . . . 7.2.5 The EhrlichSchwoebel Barrier . . . . . . . . . . . . . . . 7.2.6 Effect of the EhrlichSchwoebel Barrier on Surface Steps . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.2.7 Roughening of Surface Steps . . . . . . . . . . . . . . . . 7.2.8 Growth of a Si(111)(7 7) Surface . . . . . . . . . . . . 7.2.9 Growth of a GaAs(001) b2ð2 4Þ Surface . . . . . . 7.3 Selforganized Nanostructures . . . . . . . . . . . . . . . . . . . . . . 7.3.1 StranskiKrastanow Island Growth . . . . . . . . . . . . . 7.3.2 Thermodynamics Versus Kinetics in Island Formation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.3.3 Wire Growth on Nonplanar Surfaces . . . . . . . . . . 7.4 Problems Chapter 7 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.5 General Reading Chapter 7 . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . .
. . . . . . . . . . . . . . .
. . . . . . . . . . . . . . .
251 251 252 253 255 256 259 261 266 268 268 269 274 276 280
. . . . . .
. . . . . .
. . . . . .
282 284 287 290 292 293
. . . . .
. . . . .
. . . . .
299 301 303 305 305
. . . . . . . . . . . . . .
. . . . . . . . . . . . . .
. . . . . . . . . . . . . .
Contents
8
9
xiii
In Situ Growth Analysis . . . . . . . . . . . . . . . . . . . . . . . . . . 8.1 Surface and Ambient Probing . . . . . . . . . . . . . . . . . . 8.2 In Situ Ambient Analysis . . . . . . . . . . . . . . . . . . . . . 8.2.1 Quadrupole Mass Spectrometry . . . . . . . . . . . 8.2.2 Optical Ambient Probing . . . . . . . . . . . . . . . 8.3 SurfaceSensitive Diffraction Techniques . . . . . . . . . . 8.3.1 Reﬂection HighEnergy Electron Diffraction (RHEED) . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.3.2 Grazing Incidence XRay Diffraction (GIXD) and Reﬂection . . . . . . . . . . . . . . . . . . . . . . . 8.4 Optical in Situ Surface Probes . . . . . . . . . . . . . . . . . . 8.4.1 Pyrometry . . . . . . . . . . . . . . . . . . . . . . . . . . 8.4.2 Deﬂectometry . . . . . . . . . . . . . . . . . . . . . . . . 8.4.3 Reﬂectance and Ellipsometry . . . . . . . . . . . . 8.4.4 ReﬂectanceDifference Spectroscopy . . . . . . . 8.5 Problems Chapter 8 . . . . . . . . . . . . . . . . . . . . . . . . . 8.6 General Reading Chapter 8 . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . .
. . . . . .
. . . . . .
. . . . . .
. . . . . .
. . . . . .
. . . . . .
311 311 314 314 317 320
. . . . . . . 320 . . . . . . . . .
. . . . . . . . .
. . . . . . . . .
323 324 325 326 329 335 338 340 340
Application of Surfactants . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.1 The Surfactant Effect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.1.1 Concept of SurfactantMediated Growth . . . . . . . . . 9.1.2 Evidence for the Surfactant Effect . . . . . . . . . . . . . . 9.1.3 SurfactantMediated Ge/Si Epitaxy . . . . . . . . . . . . . 9.1.4 SurfactantMediated Epitaxy of III–V Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.2 Models of SurfactantAssisted Epitaxy . . . . . . . . . . . . . . . . . 9.2.1 Thermodynamic Considerations . . . . . . . . . . . . . . . . 9.2.2 Kinetic Approach . . . . . . . . . . . . . . . . . . . . . . . . . . 9.2.3 The Diffusion—Deexchange—Passivation (DDP) Model . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.2.4 Exchange Pathways in SurfactantMediated Epitaxy . 9.3 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.4 Problems Chapter 9 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.5 General Reading Chapter 9 . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . .
. . . . .
345 345 345 347 349
. . . .
. . . .
353 356 356 358
. . . . . .
. . . . . .
361 364 367 367 369 369
. . . . . . .
. . . . . . .
373 374 375 380 384 385 388
10 Doping, Diffusion, and Contacts . . . . . . . . . . . . . . . . . 10.1 Doping of Semiconductors . . . . . . . . . . . . . . . . . 10.1.1 Thermal Equilibrium CarrierDensities . . . 10.1.2 Solubility of Dopants . . . . . . . . . . . . . . . 10.1.3 Amphoteric Dopants . . . . . . . . . . . . . . . . 10.1.4 Compensation by Native Defects . . . . . . . 10.1.5 Hydrogen Compensation and Passivation .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . . . .
. . . . . . .
. . . . . . . . .
. . . . . . .
. . . . . . . . .
. . . . . . .
. . . . . . . . .
. . . . . . .
. . . . . . .
xiv
Contents
10.1.6 DX Centers . . . . . . . . . . . . . . . . . . . . . . . . . . 10.1.7 FermiLevel Stabilization Model . . . . . . . . . . . 10.1.8 Delta Doping and Modulation Doping . . . . . . . 10.2 Diffusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.2.1 Diffusion Equations . . . . . . . . . . . . . . . . . . . . 10.2.2 Diffusion Mechanisms . . . . . . . . . . . . . . . . . . 10.2.3 Effective Diffusion Coefﬁcients . . . . . . . . . . . . 10.2.4 Disordering of Heterointerfaces . . . . . . . . . . . . 10.3 MetalSemiconductor Contact . . . . . . . . . . . . . . . . . . . 10.3.1 Ideal Schottky Contact . . . . . . . . . . . . . . . . . . 10.3.2 Real MetalSemiconductor Contact . . . . . . . . . 10.3.3 Practical Ohmic MetalSemiconductor Contact . 10.3.4 Epitaxial Contact Structures . . . . . . . . . . . . . . 10.4 Problems Chapter 10 . . . . . . . . . . . . . . . . . . . . . . . . . . 10.5 General Reading Chapter 10 . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . .
389 391 393 398 398 402 404 407 411 411 415 418 420 422 423 424
. . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . .
427 428 429 432 433 436 439 440 442 447 453 453 456 461 463 464 465 466
12 Special Growth Techniques . . . . . . . . . . . . . . . . . . . . . . . 12.1 Selective Area Growth . . . . . . . . . . . . . . . . . . . . . . 12.1.1 Principle of Selective Area Growth . . . . . . . 12.1.2 Conditions for Selectivity . . . . . . . . . . . . . . 12.1.3 Selective Area Growth of Faceted Structures 12.1.4 Epitaxial Lateral Overgrowth (ELO) . . . . . .
. . . . . .
. . . . . .
. . . . . .
. . . . . .
. . . . . .
. . . . . .
. . . . . .
. . . . . .
469 470 470 471 476 480
11 Methods of Epitaxy . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.1 LiquidPhase Epitaxy . . . . . . . . . . . . . . . . . . . . . 11.1.1 Growth Systems . . . . . . . . . . . . . . . . . . . 11.1.2 Congruent Melting . . . . . . . . . . . . . . . . . 11.1.3 LPE Principle . . . . . . . . . . . . . . . . . . . . . 11.1.4 LPE Processes . . . . . . . . . . . . . . . . . . . . 11.2 Metalorganic VaporPhase Epitaxy . . . . . . . . . . . 11.2.1 Metalorganic Precursors . . . . . . . . . . . . . 11.2.2 The Growth Process . . . . . . . . . . . . . . . . 11.2.3 Mass Transport . . . . . . . . . . . . . . . . . . . 11.3 Molecular Beam Epitaxy . . . . . . . . . . . . . . . . . . . 11.3.1 MBE System and Vacuum Requirements . 11.3.2 Beam Sources . . . . . . . . . . . . . . . . . . . . 11.3.3 Uniformity of Deposition . . . . . . . . . . . . 11.3.4 Adsorption of Impinging Particles . . . . . . 11.4 Problems Chapter 11 . . . . . . . . . . . . . . . . . . . . . . 11.5 General Reading Chapter 11 . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . .
Contents
12.2 Vapor–Liquid–Solid Growth of Nanowires . . . . 12.2.1 Outline of the VLS Method . . . . . . . . 12.2.2 Growth of Si Nanowires . . . . . . . . . . . 12.2.3 Growth of III–V Nanowires . . . . . . . . 12.3 Atomic Layer Epitaxy and Related Techniques . 12.3.1 Atomic Layer Epitaxy (ALE) . . . . . . . 12.3.2 MigrationEnhanced Epitaxy (MEE) . . 12.3.3 Atomic Layer Deposition (ALD) . . . . . 12.4 Deposition of Organic Crystals . . . . . . . . . . . . 12.4.1 Methods of Organic Layer Deposition . 12.4.2 Epitaxy of Organic Semiconductors . . . 12.5 General Reading Chapter 12 . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
xv
. . . . . . . . . . . . .
. . . . . . . . . . . . .
. . . . . . . . . . . . .
. . . . . . . . . . . . .
. . . . . . . . . . . . .
. . . . . . . . . . . . .
. . . . . . . . . . . . .
. . . . . . . . . . . . .
. . . . . . . . . . . . .
. . . . . . . . . . . . .
. . . . . . . . . . . . .
. . . . . . . . . . . . .
485 486 488 491 499 501 501 502 505 506 509 513 514
Appendix . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 521 Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 527 Fundamental Physical Constants . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 535
About the Author
Dr. rer. nat. Udo W. Pohl, professor of experimental physics, studied physics in Aachen and Berlin, Germany, and received his Ph.D. degree in 1988 from the Technical University of Berlin, where he is currently principal investigator in the Institute of Solid State Physics. He is a member of the German Physical Society, participated in international conference committees, and has given keynote addresses at international conferences. Since the early 1990s he has given lectures on semiconductor physics and epitaxy. In 2009, he was appointed Adjunct Professor of Physics at Technical University of Berlin. He is series editor of Materials Sciences, has authored over 200 journal articles and conference papers, the books Epitaxy of Semiconductors and—together with Prof. Dr. Karl W. Böer—Semiconductor Physics, thirteen book contributions, and patents. His current research interests include physics and epitaxy of semiconductor nanostructures and devices.
xvii
Abbreviations
0D 1D 2D 3D ACS AIP APS AVS bcc BEP CB CBE CVD DAS DBR DOS ELO EMA EXAFS fcc FET FWHM GSMBE hcp hh HRTEM HRXRD HUC LEED LED
zerodimensional onedimensional twodimensional threedimensional American Chemical Society American Institute of Physics American Physical Society American Vacuum Society—The Science & Technology Society bodycentered cubic beam equivalent pressure conduction band chemical beam epitaxy chemical vapor deposition dimer adatom stackingfault (model) distributed Bragg reflector density of states epitaxial lateral overgrowth (also: ELOG) effective mass approximation extended Xray absorption ﬁnestructure facecentered cubic ﬁeldeffect transistor full width at half maximum gassource molecular beam epitaxy hexagonally closed packed heavy hole highresolution transmission electron microscopy highresolution Xray diffraction half unit cell lowenergy electron diffraction lightemitting diode
xix
xx
lh LPE MBE ML MOCVD MOMBE MOVPE MRS MWQ PL PLE PVD QD QW QWR RHEED rms RSC SEM si SIMS SL slm so STM TEC TEM TLK TSK UHV VB VCA VCSEL ViGS VPE Wiley XPS XRD XSTM ZB
Abbreviations
light hole liquid phase epitaxy molecular beam epitaxy monolayer metalorganic chemical vapor deposition metalorganic molecular beam epitaxy metalorganic vaporphase epitaxy Materials Research Society multiple quantum well photoluminescence photoluminescence excitation (spectroscopy) physical vapor deposition quantum dot quantum well quantum wire reflection highenergy electron diffraction root mean square Royal Society of Chemistry scanning electron microscopy semiinsulating secondary ion mass spectrometry superlattice standard liters per minute spinorbit, also splitoff scanning tunneling microscopy thermal expansion coefﬁcient transmission electron microscopy terraceledgekink (model) terracestepkink (model) ultrahigh vacuum valence band virtual crystal approximation verticalcavity surfaceemitting laser virtual gap states vapor phase epitaxy John Wiley and Sons Xray photoelectron spectroscopy Xray diffraction crosssectional scanning tunneling microscopy zincblende
Chapter 1
Introduction
Abstract This introductory chapter provides a brief survey on the development of epitaxial growth techniques and points out tasks for the epitaxy of device structures. Starting from early studies of alkalihalide overgrowth in the beginning of the 20th century, basic concepts for lattice match between layer and substrate were developed in the late 1920s, followed by the theory of misfit dislocations introduced about 1950. Major progress in epitaxy was achieved by technical improvements of the growth techniques, namely liquid phase epitaxy in the early, and molecular beam epitaxy and metalorganic vapor phase epitaxy in the late 1960s. Current tasks for epitaxial growth are often motivated by needs for the fabrication of advanced devices, aiming to control carriers and photons.
Most semiconductor devices fabricated today are made out of a thin stack of layers with a typical total thickness of only some µm. Layers in such a stack differ in material composition and may be as thin as a single atomic layer. All layers are to be grown with high perfection and composition control on a bulk crystal used as a substrate. The growth technique employed for coping with this task is termed epitaxy. In the following we briefly consider the historical development and illustrate typical issues accomplished using epitaxy.
1.1 Epitaxy 1.1.1 Roots of Epitaxy Crystalline solids found in nature show regularly shaped asgrown faces. The faces of a zinc selenide crystal grown from the vapor phase in the lab are shown in Fig. 1.1a. Mineralogists found that the angles between corresponding faces are always the same for different samples of the same type of crystal. They concluded already in the 18th century that such regular shapes originate from a regular assembly of identical building blocks forming the crystal as indicated in Fig. 1.1b. In the early 19th century mineralogists noticed that naturally occurring crystals sometimes grew together with © Springer Nature Switzerland AG 2020 U. W. Pohl, Epitaxy of Semiconductors, Graduate Texts in Physics, https://doi.org/10.1007/9783030438692_1
1
2
1 Introduction
(a)
(b)
(111) (001)
(111)
(100)
Fig. 1.1 a ZnSe bulk crystal with {100} and {111} growth faces. b Faces formed from regularly repeating building blocks described around 1800 [3]. The complete shape of the displayed rhombdodecahedron is indicated by red lines
a unique relationship of their orientations [1]. A first successful artificial reproduction of this effect in a laboratory was reported by Moritz L. Frankenheim in 1836 [2]. He demonstrated a parallel oriented growth of sodium nitrate NaNO3 from solution on a freshly cleaved calcite crystal CaCO3 . First systematic studies on the crystal growth on top of another crystalline material were reported by Thomas V. Barker starting 1906 [4]. At that time growth from solution and optical microscopy were the only readily developed techniques for growth and characterization of samples, respectively. Baker investigated a large number of NaCltype alkali halides like chlorides, bromides, iodides, and cyanides of, e.g., rubidium and cesium. He placed a drop of saturated solution of one halide onto a freshly cleaved surface of another halide and observed the nucleation of a crystalline structure under a microscope. Crystals of the solute appeared as a rule in a few seconds, but sometimes nucleation was too rapid to be observed or difficulties arose due to a greater solubility for the crystal than for the dilute dropped on top. He concluded that crystalline growth of alkali halides was more likely to occur if the molecular volumes of the two intergrowing materials were nearly equal. We note that such conditions often imply a similar size of the building blocks mentioned above and consequently a small misfit of the lattice constants of the two materials. The discovery of Xray diffraction (1912) and electron diffraction (1927) by crystals had a strong impact on the knowledge about crystal structure. When Louis Royer made his seminal comprehensive studies with a wide variety of layers and substrate materials in 1928, he could precisely report on the effect of substrate crystal structure on the crystalline orientation of the layer [5]. Royer introduced the term epi
1.1 Epitaxy
3
taxy from the Greek epi (epi, upon, attached to)—taxis (taxis, arrangement, order) and concluded general rules for epitaxy. He noted that oriented growth occurs only when it involves the parallelism of two lattice planes which have lattice networks of identical or quasiidentical form and closely similar spacing. More precisely, he found that the differences between the latticenetwork spacing (lattice parameters) for growth of alkali halides upon other alkali halides or mica (minerals of the form X Y23 Z4 O10 (OH, F)2 ) should be no more than 15%. Such geometrical considerations are still prominent today, though it was established later that epitaxy may also occur for much larger misfits. In the 1930s, G. I. Finch and A. G. Quarrell concluded from a study of zinc oxide on sputtered zinc that the initial layer is strained in order to attain lattice matching parallel to the interface [6]. The layer latticeparameter vertical to the interface was also considered to be changed to maintain approximately the bulk density. They named this phenomenon pseudomorphism. Though later the experimental evidence was pointed out to be by no means conclusive [1], the concept of pseudomorphic layers proved to be of basic importance for epitaxial structures. The introduction of the theory of misfit dislocations at the interface between the substrate and the layer by F. C. Frank and Jan H. van der Merve in 1949 [7–9] extended the pseudomorphism approach and predicted a limit for the misfit of pseudomorphic growth. The incorporation of edge dislocations allows to accommodate misfit strain and consequently makes epitaxy possible also for structures with larger misfit. Conclusive experimental evidence for this was provided by John W. Matthews and coworkers in the 1960s [10, 11]. Thin metal layers on singlecrystal metals with low misfit proved to grow pseudomorphic, while misfit dislocations were generated in thicker layers with a density depending on layer thickness. Later also conditions not included in the mentioned concepts like, e.g., interface alloying or surface energies were found to significantly affect epitaxial growth. The emerging semiconductor industry in the early 1960s had a strong impact on the interest in epitaxy. In addition, advancements in the technique of producing high vacuum and pure materials, and progress in experimental techniques like electron microscopy and Xray diffraction allowed to efficiently develop methods for epitaxial growth. Liquidphase epitaxy enabled epitaxial growth of multilayered device structures of high complexity like separateconfinement semiconductor lasers. The advancement of this technology was facilitated by its similarity to the wellstudied growth of bulk singlecrystals from seeded solution. In the 70s the more sophisticated methods of molecularbeam epitaxy [12] and metalorganic vaporphase epitaxy emerged. These techniques opened up epitaxy far from thermodynamic equilibrium and hence fabrication of structures with atomically sharp interfaces, which cannot be produced near equilibrium. Understanding and control of the epitaxial growth techniques was significantly advanced by the application of insitu studies of the nucleation and growth process, and by the development of computational techniques. In the late 80s the modern techniques attained a maturity to get in the lead of device massproduction. Today a large variety of electronic, optoelectronic, magnetic, and superconducting layer structures are fabricated using epitaxial techniques, including structures of reduced dimensionality on a nanometer scale.
4
1 Introduction
1.1.2 Epitaxy and BulkCrystal Growth Crystal growth in an epitaxial process proceeds basically in the same way as conventional growth of bulk crystals. In epitaxy, however, layer and substrate differ in the nature and strength of the chemical bond. Moreover, both materials may have a different crystal structure and generally have an unequal lattice parameter—at least if the temperature is varied. We may therefore say that crystals differ energetically and geometrically in epitaxy [13]. Crystalline deposition of different materials on each other is also termed heteroepitaxy. Such a definition does obviously not apply for the epitaxial deposition on a substrate of the same material. The process is usually referred to as homoepitaxy (sometimes also autoepitaxy). Let us consider a simple example to illustrate that there may still be a difference to conventional crystal growth. Epitaxy of electronic devices is usually performed on doped substrates and often starts by depositing a layer of the same material termed homoepitaxial buffer layer. Doping often alters the lattice parameter without significantly changing the chemical bond in bulk material. A ptype doping of, e.g., silicon with boron to a level of 2 × 1019 cm−3 induces a change of the lattice parameter by −1%. An undoped layer on a doped substrate of the same material will hence not differ energetically but geometrically. This provides a clear distinction of homoepitaxy from conventional crystal growth. According to this differentiation deposition of a layer of the same kind and doping like the substrate underneath should be termed crystal growth instead of epitaxy. Following the general usage we will, however, use the term homoepitaxy less strictly. Deposition of a layer of the same material as the substrate is usually just one of many layers to follow in the growth process of a device structure. Furthermore, fabrication of bulk crystals is usually performed applying a different growth regime than in epitaxy, allowing for much higher growth rates. Accordingly also different experimental setups are employed. The term homoepitaxy will be used here for deposition of the same material as the substrate, just to distinguish from heteroepitaxy.
1.2 Issues of Epitaxy 1.2.1 Convention on Use of the Term “Atom” Solids are composed of atoms, which may be charged due to the character of the chemical bond. When used in a general way in this book, the word “atom” denotes both, an atom or an ion. Uncharged atoms are hence for simplicity usually not distinguished from charged atom cores in, e.g., ionic crystals or metals unless explicitly pointed out.
1.2 Issues of Epitaxy
5
Fig. 1.2 Gradual circular arrangement of 48 iron adatoms on a copper surface assembled using a lowtemperature scanning tunnelling microscope. Interference ripples originate from electron surface states. From [15]
1.2.2 Assembly of Atoms Epitaxy denotes the regular assembly of atoms on a crystalline substrate. By inventing the scanning tunneling microscope (STM) a particular means has been developed to control the assembly of single atoms for forming an ordered structure. The method uses the finite force an STM tip always exerts on an adsorbed atom (adatom) attached to the surface of a solid [14]. The magnitude of the force can be tuned by adjusting the voltage and the position of the tip. Since generally less force is required to move an atom across a surface than to pull it away the tip parameters can be set to allow for positioning an individual adatom while it remains bound to the surface. The example given in Fig. 1.2 shows iron atoms on a (111) copper surface. The initially disordered Fe atoms were carefully positioned at chosen locations. May such procedure also be applied to deposit an epitaxial layer onto a substrate? Imagine a skillful operator placing one atom per second exactly on the correct site of a layer. For typically about 1015 sites per cm2 such procedure requires 31 Mio. years for a single atomic layer being deposited on one cm2 . The fabrication of epitaxial structures hence requires other methods. The problem of growing a layer by the assembly of single atoms is comparable to the issue of describing the behavior of a gas by formulating the equation of motion for each atom. This cannot be accomplished for exceedingly large ensembles like a considerable fraction of 6 × 1023 atoms present in one mole. The approach of kinetic theory of gases hence solely describes averages of certain quantities of the vast number of atoms in the ensemble, concluded from the behavior of one single atom. These averages correspond to macroscopic variables. We will basically follow a comparable approach. In epitaxial growth we seek to establish favorable conditions for atoms of a nutrient phase to finding proper lattice sites in the solid phase. The macroscopic control parameters are governed by both thermodynamics and kinetics, and their effect depends on the materials and the applied growth method.
6
1 Introduction
1.2.3 Tasks for Epitaxial Growth Semiconductor devices control the flow and confinement of charge carriers and photons. To fulfill its task a device is composed of crystalline layers and corresponding interfaces with different physical properties. Epitaxy is employed to assemble such layer structure. The precise control of the growth process in epitaxy requires the accomplishment of issues with quite different nature. We consider the example of a semiconductor devicestructure to illustrate a number of tasks addressed during fabrication and indicate the connection to respective chapters of this book. The addressed concepts basically apply also for insulators and metals. In this book we focus on semiconductor materials. The demand for increasing datarate capacity in datacommunication networks raised the need for suitable optical interconnects, particularly for light sources. Verticalcavity surfaceemitting lasers (VCSELs) have characteristics meeting ambitious requirements of fiber communication and meanwhile emerged from the laboratory to the marketplace. VCSEL devices are also widely used in computer mice due to a good shape of their optical radiation field. A VCSEL is a semiconductor laser, which emits the radiation vertically via its surface—in contrast to the more common edgeemitting lasers. Like any laser it consists of an active zone where the light is generated, overlapping with a region where the optical wave is guided. Light is generated by recombination of electrons and holes which are confined in quantum wells (MQW, multiple quantum well). The generated photons contribute to the light wave which travels back and forth in an optical FabryPérot resonator built by two mirrors, and a small fraction representing the laser radiation is allowed to emerge from the top mirror. Since the resonator in a VCSEL is very short, the reflectivity of the mirrors must be very high (R > 99%) to maintain lasing oscillation. They hence are made from distributed Bragg reflectors (DBR) of many pairwise 41 λ/n thick layers with a difference in the respective refractive index n, λ being the operation wavelength. If the index step n is low many pairs are required (a few tens). The basic design of a VCSEL is given in Fig. 1.3. The realization of a semiconductor device is a complex process. The basic design layout is determined by a number of operation parameters like, e.g., the emission wavelength for an optoelectronic device. Already at this stage materials aspects play an important role. Obviously a widebandgap semiconductor material, e.g., must be used in the active region if the device is to radiate at high photon energy. The design stage comprises simulation work on electrical, optical, and other properties of the device depending on the employed materials and the specific purpose of the device. The design eventually yields a list of materials composition, thickness, and doping for each individual layer in the entire layer stack to be epitaxially grown. The crystalline epitaxial growth on a singlecrystalline substrate requires a welldefined relationship of the substrate structure with respect to that of the layers grown on top. For this purpose the spacing of the atoms parallel to the interface between substrate and the layers of the device structure on top has to accommodate. Since the lateral lattice constants never match perfectly and the total layer thickness of the
1.2 Issues of Epitaxy Fig. 1.3 Schematic of a verticalcavity surfaceemitting laser indicating the sequence of differently alloyed and doped semiconductor layers
7
light output
pcontact pDBR mirror MQW
cavity
nDBR mirror nbuffer layer nsubstrate ncontact
device structure is generally much below the substrate thickness, epitaxial layers are elastically strained. Chapter 2 introduces into the structural and elastic properties of epitaxial layers and points out a critical limit for such strain. As a consequence of overcritical stress, plastic relaxation occurs by the introduction of misfit dislocations. Prominent species of such dislocations for the important crystal structures zincblende and wurtzite are treated. Prior to the growth of the device layers usually a buffer layer is grown on the substrate. This layer is introduced to keep defects located at the interface to the substrate and dislocations originating from large misfits away from the device layers. A further challenge occurs from a large change of composition within a layer sequence. The device depicted in Fig. 1.3 comprises Bragg mirrors, which require a large step of the refractive index between consecutive quarterlambda thick layers. A large index step of the layer pairs in the mirror stack is connected not only to a large difference of the fundamental bandgap of the layers, but usually also to a large difference of lattice constants. To keep the strain below the critical limit, layers with a composition mix of materials are used to maintain the lattice constant while changing the refractive index. The change of lattice constant in mixed layers and means to compensate the total strain in a layer stack are also considered in Chap. 2. Organic semiconductors are increasingly applied in (opto) electronic devices. Their structure differs substantially from that of their inorganic counterparts and is discussed in Chap. 3. Organic semiconductors comprise smallmolecule crystals and polymers; they both feature weak intermolecular forces, yielding usually highly defective crystals with a close molecule packing. The structure of a thin smallmolecule film often deviates from the bulk structure and depends on the film thickness and on the interaction to the substrate. The exact register of substrate and layer lattices commonly observed for inorganic heterostructures is usually not found for organic layers. The new epitaxial coincidence modes occuring in such structures and their relation to intra and intermolecular elasticity are outlined in Chap. 3. Various kinds
8
1 Introduction
of defects are described, including the prevailing vacancies and grain boundaries between singlecrystal domains. Strain and interfaces between layers with different bandgap affect the electronic properties of the layer structure. In Chap. 4 the effect of strain on valence and conductionband states is outlined. Furthermore, the consequence of alloying on the fundamental bandgap is considered. The contact of two semiconducting layers raises the question how the uppermost valence bands mutually align. Models treating this problem and effects of interface composition are reviewed in Chap. 4. The band discontinuities determine the confinement of charge carriers in a sandwich structure and are also affected by strain. This is particularly important for the active layers which are usually formed by quantum wells as depicted in Fig. 1.3. Structures with a reduced dimensionality—quantum wells, quantum wires, and quantum dots—form the active core of many advanced devices. Chapter 4 points out the basic electronic properties of such quantum structures to indicate the required dimensions, which have to be realized in the epitaxial growth process. In organic semiconductors the highest occupied und lowest unoccupied molecular orbitals (HOMO and LUMO) form the valence and conduction bands. Chapter 5 considers the special properties of these bands originating from the molecular structure, and the consequences for the electronic properties. The environment of a charge carrier in an organic crystal experiences a strong structural and electronic relaxation. The resulting strongly bound Frenkel excitons and the pronounced polaron character of mobile carriers are pointed out, and the transport properties are discussed. The band alignment at interfaces with organic semiconductors depends sensitively on molecule charge and orientation. In many cases the classical electronaffinity rule known from Chap. 4 yields a good description of the heterojunction between two organic solids. The effect of molecule orientation is discussed in Chap. 5, and also the band alignment for a contact to a metal is treated. Growth occurs at some deviation from thermodynamic equilibrium. Epitaxy is a controlled transition from the gas or liquid phase to a crystalline solid. The nature of the driving force depends on the particular material system and growth conditions. Chapter 6 introduces into the thermodynamics of growth for simple oneand twocomponent systems. Nucleation of a layer, epitaxial growth modes, and a thermodynamic approach to surface energies are described. Even though epitaxial growth processes may occur under conditions far from equilibrium, thermalization times of atoms arriving from the nutrition phase on the surface can be much less than the time required to grow a single monoatomic layer. In such cases thermodynamic descriptions are often successfully applied to model the growth process. For the device structure illustrated in Fig. 1.3 thermodynamics may constitute limits for the stability of mixed crystals used to meet the requirements for lattice constants, bandgaps, band alignments, and doping. In such cases epitaxy may still be possible in a restricted temperature range. The fabrication of atomically sharp interfaces between two dissimilar solids requires a significant deviation from equilibrium to suppress interdiffusion. This is particularly important for quantum structures like the active layers in the VCSEL structure shown in Fig. 1.3, usually realized using multiple quantum wells. Under
1.2 Issues of Epitaxy
9
such nonequilibrium conditions growth is strongly affected by kinetic influences. Kinetics and atomistic aspects of epitaxial growth are addressed in Chap. 7. A kinetic description of nucleation and layer growth accounts for the detailed steps atoms experience on the growing surface. They depend on the structure of the surface, where the arrangement of atoms may differ substantially from that found in the solid bulk underneath. Such surface reconstructions are specific for the given material and change with growth conditions—they are pointed out for specific examples. Growth modes depending on strain or specific surface states are often employed in epitaxy to fabricate lowdimensional structures by selforganized processes. The basics of such selforganized formation of quantum dots and quantum wires is considered in Chap. 7. VCSEL devices like that depicted in Fig. 1.3 are also fabricated using quantum dots in the active region, formed in the selforganized StranskiKrastanow growth mode. The online analysis of a layer structure already during its epitaxial growth is a prominent tool for the development of device structures and for ensuring runtorun reproducibility. Sensors for the in situ measurement of sample temperature, growth rate, strain, and other parameters of the growth process are considered in Chap. 8. The data are deduced by probing the sample surface, or from the analysis of the ambient in the vicinity of the growing sample using mass spectrometry or optical spectroscopy. Most online tools discussed in Chap. 8 are applicable to all major growth techniques, and some of them can even resolve the growth of a single monolayer. Prominent techniques for the in situ analysis of epitaxy comprise structural analysis by diffraction methods and various optical probes; besides pyrometry techniques such as deflectometry, reflectometry, ellipsometry, and others are addressed providing both chemical and structural information. The surface energy can be modified during epitaxy by surfaceactive species referred to as surfactants. Chapter 9 discusses how the threedimensional island growth occurring during mismatched heteroepitaxy can be suppressed, yielding smooth twodimensional growth for an appropriate combination of surfactant and semiconductor material. During growth the surfactant layer floates on the semiconductor layer; altered adatom diffusivity and nucleation rate are considered, and processes for strain relaxation in the epitaxial layer are pointed out. Chapter 9 also introduces models treating both kinetic and thermodynamic effects, and highlights the prominent role of the passivation of step edges at nucleating monolayer islands. For specific examples exchange pathways of adatoms and surfactant atoms are discussed. Electronic and optoelectronic devices require control of charge carriers in semiconductors and a contact of the semiconductor structure to a metal for a connection to the electric circuit. Chapter 10 gives a brief introduction to problems in epitaxy connected to doping and contact fabrication. For a given semiconductor material thermodynamics may impose limits in the doping level originating from restricted solubility of the dopants, an amphoteric behavior of the dopants, or compensation by native defects. Nonequilibrium epitaxial growth may relieve some restrictions. Growth far from equilibrium also enables deltalike doping profiles, used to fabricate devices employing a twodimensional electron gas with a high mobility. Doping and
10
1 Introduction
heterostructure composition profiles may be affected by redistribution of atoms due to diffusion phenomena. Mechanisms of diffusion in semiconductors are considered and examples are given for dependences on the ambient atmosphere and on the kind of doping. Ohmic contacts between semiconductor and metal are a classical subject, but epitaxy also enables the growth of specific contact structures to achieve a low contact resistance. Some examples are outlined in Chap. 10. Various techniques for epitaxial growth have been established and are described in Chap. 11. The first method which attained maturity to produce complex devices was liquidphase epitaxy. It operates close to thermodynamic equilibrium and may hence be well described by thermodynamics. More versatile control is achieved using the more sophisticated methods of molecularbeam epitaxy and metalorganic vaporphase epitaxy, which both operate far from thermal equilibrium. They hence both allow for a control of layer thickness down to a fraction of a single atomic layer and are used to fabricate devices with quantum structures in the active region. The two methods are also employed in VCSEL production on a large scale. Chapter 12 addresses special techniques applied using common epitaxial methods. In selective area growth an epitaxial layer is grown only in selected parts of a substrate, defined by windows in a mask. The conditions for selectivity are pointed out, and the effects of the mask and the crystallographic orientation on the growth rate are discussed. Epitaxial lateral overgrowth of the mask is highlighted as an important application. In the following section vaporliquidsolid (VLS) growth is introduced as a prominent method to fabricate semiconductor nanowires with high performance. Controlled axial and radial growth enabling the fabrication of axial and coreshell heterostructures is pointed out, and the very large critical thicknesses for coherent epitaxy is discussed. Techniques with an alternately pulsed supply of gaseous precursors are considered next, comprising atomic layer epitaxy (ALE) or deposition (ALD), and the related migration enhanced epitaxy (MEE). The MEE mode of MBE leads to an increased lifetime of adatoms, enabling particularly sharp interfaces and doping profiles. ALD of amorphous or polycrystalline layers is widely used in semiconductor technology due to an exceptional conformality and thickness control on nonplanar surfaces. Chapter 12 concludes considering the epitaxial deposition of organic crystals using organic molecular beam deposition or organic vaporphase deposition. Differences with respect to inorganic layer deposition is discussed, and the demanding nucleation issues are emphasized.
References 1. D.W. Pashley, A historical review of epitaxy, in Epitaxial Growth (Part B), ed. by J.W. Matthews (Academic Press, New York, 1975), pp. 1–27 2. M.L. Frankenheim, Über die Verbindung verschiedenartiger Krystalle. Ann. Phys. 113, 516 (1836). (On the interface of different crystals, in German) 3. M. L’Abbé, R.J. Haüy, Traité Élémentaire de Physique, 3rd edn. (Mme. V. Courcier, Libraire Pour Les Sciences, Paris, 1821) (in French)
References
11
4. T.V. Barker, Contributions to the theory of isomorphism based on experiments on the regular growths of crystals on one substance on those of another. J. Chem. Soc. Trans. 89, 1120 (1906) 5. L. Royer, Recherches expérimentales sur l’epitaxie ou orientation mutuelle de cristaux d’espèces différentes. Bull. Soc. Fr. Minéral. Cristallogr. 51, 7 (1928). (Experimental investigation on the epitaxy or mutual orientation of crystals of different species, in French) 6. G.I. Finch, A.G. Quarrell, The structure of magnesium, zinc and aluminium films. Proc. R. Soc. Lond. A 141, 398 (1933) 7. F.C. Frank, J.H. van der Merve, Onedimensional dislocations. I. Static theory. Proc. R. Soc. Lond. A 198, 205 (1949) 8. F.C. Frank, J.H. van der Merve, Onedimensional dislocations. II. Misfitting monolayers and oriented overgrowth. Proc. R. Soc. Lond. A 198, 216 (1949) 9. F.C. Frank, J.H. van der Merve, Onedimensional dislocations. III. Influence of the second harmonic term in the potential representation, on the properties of the model. Proc. R. Soc. Lond. A 200, 125 (1949) 10. W.A. Jesser, J.W. Matthews, Evidence for pseudomorphic growth of iron on copper. Philos. Mag. 15, 1097 (1967) 11. W.A. Jesser, J.W. Matthews, Pseudomorphic growth of iron on hot copper. Philos. Mag. 17, 595 (1968) 12. J. Orton, T. Foxon, Molecular Beam Epitaxy: A Short History (Oxford University Press, Oxford, UK, 2015) 13. I.V. Markov, Crystal Growth for Beginners (World Scientific, Singapore, 2003) 14. D.M. Eigler, E.K. Schweizer, Positioning single atoms with a scanning tunnelling microscope. Nature 344, 524 (1990) 15. Details and the last STM image are reported in M.F. Crommie, C.P. Lutz, D.M. Eigler, Confinement of electrons to quantum corrals on a metal surface. Science 262, 218 (1993). Image originally created by IBM Corporation, http://www.almaden.ibm.com/vis/stm/corral.html
Chapter 2
Structural Properties of Heterostructures
Abstract Structural properties of epitaxial layers are pointed out in this chapter with some emphasis on zincblende and wurtzite crystals. After a brief review on perfect, polytype, and mixed bulk crystals we focus on elastic properties of pseudomorphic strainedlayer structures. Then the concept of critical layer thickness is introduced, and dislocations relieving the strain in epitaxial layers are presented. Xray diffraction—the standard tool for structural characterization—is outlined at the end of the chapter.
2.1 Basic Crystal Structures Atoms in an ideal solid have a regular periodic arrangement, which represents a minimum of total energy. The structure of such a crystalline solid is described by a lattice, which constitutes the translational periodicity, and a basis, which represents the atomic details of the recurring unit cell. In 1848 Auguste Bravais showed that there are only 14 lattices in threedimensional space. These 14 Bravais lattices may be divided into 7 crystal systems, which differ in shape of their unit cell as shown in Table 2.1. The given unit cells reflect the symmetry of the structures. In most cases they are not primitive, i.e., they are larger than the smallest possible unit cell and contain more than one basis. Some important crystal structures are pointed out explicitly in this chapter.
2.1.1 Notation of Planes and Directions Lattice planes and directions in crystals are generally denoted by triplets of integer numbers h, k, l called Miller indices. To determine the Miller indices of a given plane, first a coordinate system is constructed using base vectors of the unit cell (regardless of being primitive or not). Then the intersection points of the plane with the axes are determined in units of the lattice constants, i.e., as multiples of the base vectors. Finally the reciprocal of these three values are expanded to the smallest set of integer © Springer Nature Switzerland AG 2020 U. W. Pohl, Epitaxy of Semiconductors, Graduate Texts in Physics, https://doi.org/10.1007/9783030438692_2
13
14
2 Structural Properties of Heterostructures
Table 2.1 The seven crystal systems and the 14 Bravais lattices. a, b, and c are lattice vectors spanning the unit cell; α, β, and γ are angles between these vectors System Unit cell Bravais lattices Symmetry axes Cubic
a = b = c, α = β = γ = 90◦
Simple cubic, bodycentered cubic, facecentered cubic
Tetragonal
a = b = c, α = β = γ = 90◦
Rhombohedral
a = b = c, α = β = γ = 90◦
Simple tetragonal, bodycentered tetragonal Rhombohedral
Hexagonal
a = b = c, α = β = 90◦ , γ = 120◦ a = b = c, α = β = γ = 90◦
Orthorhombic
Monoclinic
Triclinic
a = b = c, α = γ = 90◦ , β = 90◦ a = b = c, α = β = γ , α, β, γ = 90◦
Hexagonal
Simple orthorhombic, basecentered orthorhombic, bodycentered orthorhombic, facecentered orthorhombic Simple monoclinic, facecentered monoclinic Triclinic
4 threefold axes parallel to the diagonals of the unit cell 1 fourfold axes of rotation or inversion parallel to c 1 threefold axes of rotation or inversion parallel to a + b + c 1 sixfold axes of rotation or inversion parallel to c 3 mutually perpendicular twofold axes of rotation or inversion parallel to a, b, and c
1 twofold axes of rotation or inversion, e.g. parallel to b None
values. Example: A plane intersects the three axes of a cubic coordinate system at (3, 1, 2) yielding the reciprocals (1/3, 1, 1/2), and consequently the Miller indices (2, 6, 3). Different kind of brackets are used to distinguish between various planes, directions, and lattice points: (hkl) {hkl} [hkl] hkl hkl
a specific plane, normal parentheses a set of crystallographically equivalent planes, curly brackets a specific direction, square brackets a set of equivalent directions, cuspid brackets the position of a specific lattice point.
¯ means [−h −k l]. PosiFinally, negative values are denoted by a bar on top, e.g., [h¯ kl] tion and nomenclature of some important lowindex planes in cubic and hexagonal lattices are depicted in Fig. 2.1. In the hexagonal system usually the four MillerBravais indices are used, i.e., hktl. The index t refers to a third vector a3 in the base plane of the unit cell and
2.1 Basic Crystal Structures
15 [001]
Fig. 2.1 Position of important planes and their Miller indices for cubic and hexagonal lattices
(001)
[001]
[001]
(010)
[010] [100]
(100)
[00.1]
[21.0] c plane
(111)
(110)
(00.1)
[12.0]
[00.1]
(11.0)
a plane
[00.1]
(10.0)
m plane
depends on the indices of the vectors along a1 and a2 shown in Fig. 2.4d by the relation t = −(h + k), i.e., a3 = −(a1 + a2 ). MillerBravais indices of a plane are defined by the primes referring to the reciprocals of intercepts of the plane with all four axes. For indexing planes the index t is redundant and commonly replaced by a dot. Sometimes this dot is dropped and the Miller indexing system is used, so that indices of cubic and hexagonal lattices look similar. For directions the relation between the fourindex and threeindex systems is more complicate, because the third index cannot just be left out. The conversion of any direction u a1 + v a2 + t a3 + w c = u a1 + v a2 + w c between the fourindex MillerBravais system and the (primed) threeindex Miller system is given by the relations u = 2u + v u = 13 (2u − v ) v = 2v + u v = 13 (2v − u ) 1 t = − 3 u + v = −(u + v) w = w w = w . After conversion to relative primes. The MillerBravais all indices must be reduced ¯ , 12 ¯ 10 ¯ , and 1120 ¯ directions hence correspond to the Millerindexed 21¯ 10 indexed [100], [010], and [110] directions, respectively. The directions of the hexagonal system given in Fig. 2.1 refer to the commonly used convention.
2.1.2 Wafer Orientation Thin slices of bulk semiconductor crystals referred to as wafers are used for growth of epitaxial layers. Wafers made of Si, GaAs, and InP with surfaces vicinal to {100},
16
2 Structural Properties of Heterostructures PF
[011]
(100)
[011]
[011]
SF
PF
[010] EJ option
SF
(100) SF
[001] SF [011] US option
(100) ptype
(100) ntype
(111) ntype
(111) ptype SF
PF 110
PF 110
PF 110
PF 110
SEMI standard
Fig. 2.2 Semiconductor wafers with standard flat orientations according to various options. PF and SF denote primary and secondary flats, respectively. The arrows along [010] and [001] refer to the coordinate system of the two wafers on the left hand side, the primary flat in the SEMI standard is located on a {110} plane
{111}, and {110} are most common and produced by cutting an onaxis crystal at the appropriate angle. Their cleavage planes are discussed in Sect. 2.1.4. The wafers are usually of circular shape with 2–6 in. diameter (silicon up to 300 mm) and 300 up to 1000 µm thick (depending on diameter). Information on the orientation of the crystallographic axes and the dopant type (ntype, ptype, or undoped) are indicated by location and number of flats, features machined at the perimeter of the wafer. Primary or major (orientation) flats and shorter secondary or minor (identification/index) flats are used according to different standards. Common standards are the EJ (Europe/Japan), US, and SEMI options. Figure 2.2 shows some wafer geometries of semiconductors with cubic structure along with crystallographic orientations.
2.1.3 FaceCentered Cubic and Hexagonal ClosePacked Structures The facecentered cubic and the hexagonal structure are often found in metals, and the most important semiconductors crystallize in the related diamond, zincblende, or wurtzite structures. Let us consider the atoms as spheres, which do not prefer any direction of bonding. If such atoms are closely arranged in a plane, each one has contact to six next neighbors, cf. Fig. 2.3a. The atoms form a hexagonal net plane, which we label plane B. To obtain a closely stacked threedimensional arrangement, atoms within a plane A on top of plane B must be arranged similarly, starting with an atom above the interstice of three Batoms. Note that only 3 of the 6 hexagonally arranged interstices of B are occupied by atoms in plane A. Hence there are two alternatives for a plane C below plane B: Their atoms either use the interstices not used above in plane A, or they are arranged similar to plane A. These two different structures are referred to as facecentered cubic (fcc, stacking sequence ABC ABC along the [111] stacking direction) and hexagonal closepacked (hcp, sequence AB AB). Note that both structures have the same stacking density with 74.1% space filling.
2.1 Basic Crystal Structures
17
(a)
(b)
[001]
[111]
A
B [010]
C
[100]
Fig. 2.3 a Hexagonal net planes in a closedpacked crystal structure. and + denote locations of atoms in the planes above and below, respectively, forming the fcc structure shown in (b). b Facecentered cubic structure. A, B, and C label different hexagonal lattice planes in a facecentered cubic lattice
(a)
(b)
[001]
[010]
[010]
a
(c)
[001]
[100]
(d)
[001]
c
[010] [100]
c
[100]
a1
a
a2
Fig. 2.4 The crystal structures of a zincblende, b rocksalt (NaCl), c cesium chloride (CsCl), and d wurtzite
Figure 2.3b shows that the ABCstacked atoms are located on a cubic lattice, with additional atoms centered on the six faces of the cube (the contour of the front half of the fcc unit cell is only partially drawn for clarity). This is not the case in the unit cell of the hcp structure, represented by the dark spheres in Fig. 2.4d.
2.1.4 Zincblende and Diamond Structures Many solids are composed of more than one kind of atoms. Crystal structures of some important binary bulk compounds with an at least partial ionic bond are given in Table 2.2. Some of these solids may crystallize also in another structure as noted in Table 2.3. ZnS and CdSe, e.g., have also a stable high temperature phase (here wurtzite), which may be preserved at room temperature by suitable growth conditions. Using epitaxy also structures which differ from that of the stable bulk crystal may be stabilized.
18
2 Structural Properties of Heterostructures
Table 2.2 Stable crystal structures of AB compounds composed of either group II and VI, or group III and V elements. W, ZB, and Gr denote wurtzite, zincblende, and graphite structure, the compound marked by a star does not exist. From [1] Cation Anion group VI Cation Anion group V group group III II O S Se Te N P As Sb Be Mg Zn Cd
W NaCl W NaCl
ZB NaCl ZB W
ZB NaCl ZB ZB
ZB W ZB ZB
B Al Ga In
Gr W W W
ZB ZB ZB ZB
ZB ZB ZB ZB
* ZB ZB ZB
In the zincblende structure, the basis of the primitive unit cell consist of two atoms, which generally have different polarity. Their location is at (0, 0, 0) and (1, 1, 1) × a/4, a being the lattice constant (cf. Fig. 2.4a). We will refer to these atoms as cations and anions (like zinc and sulfur in ZnS). The zincblende structure is composed of an fcc lattice of cations (represented by, e.g., dark spheres in Fig. 2.4a) and an fcc lattice of anions. √ These two sublattices are displaced by a quarter of the cube diagonal, i.e. by ( 3/4) × a. As a result, each ion is tetrahedrally surrounded by four ions of opposite polarity as depicted in Fig. 2.4a. The zincblende structure has no center of inversion, in contrast to the related diamond structure introduced below. 110 planes of the zincblende structure contain an equal number of cations and anions, arranged along zigzag chains. Since their charges balance, 110 crystal faces are nonpolar. Crystals may usually be well cleaved parallel to nonpolar planes, a fact used, e.g., in laser devices made from zincblende semiconductors to fabricate resonator facets by cleaving along two parallel 110 planes: Zincblende wafers with ¯ form side facets perpendicular to the (100) orientation scribed along [011] and [011] wafer surface and perpendicular to each other. In contrast, 100 and 111 planes contain only one kind of ions and hence form polar faces. The [111] direction is not ¯ direction. In AB compounds like zincblende ZnS ( A an B equivalent to the [1¯ 1¯ 1] generally denoting cations and anions, respectively, not to be confused with layer labels), wafers with (111) surface have a cationterminated Aface and an opposing anionterminated Bface, which can be distinguished, e.g., by different chemical etching behavior. Typical compounds with zincblende structure are ZnS, GaAs, InP, and CuCl. If the atoms on the two fcc sublattices are identical, we obtain the diamond structure (consider all atoms in Fig. 2.4a to be blue). The diamond structure has a center of inversion at the midpoint of each connection line between two next neighbors. Crystal faces of this structure are nonpolar, crystals may also be cleaved parallel to planes differing from 110. Elements crystallizing in diamond structure are C (diamond phase), Ge, Si, and Sn (α phase). In Si and Ge primary cleaving planes are 111 planes: They produce less dangling bonds than 110 planes upon cleaving.
2.1 Basic Crystal Structures
19
¯ form {111} side facets Si wafers with (100) orientation scribed along [011] or [011] inclined to the wafer surface by an angle of 54.7°.
2.1.5 Rocksalt and CesiumChloride Structures The cubic rocksalt structure (also termed sodiumchloride structure) shown in Fig. 2.4b is composed of two fcc lattices for √ cations and anions, respectively, displaced by half of the cube diagonal, i.e., by ( 3/2) × a. The two ions of the basis are located at (0, 0, 0) and (1, 1, 1) × a/2. As a result, each ion is octahedrally surrounded by six ions of opposite polarity. Their charges balance on 100 crystal faces, which are hence nonpolar and build cleavage planes of this structure. Compounds which crystallize in rocksalt structure are, e.g., NaCl, KCl, AgBr, FeO, PbS, MgO, and TiN. The cesiumchloride structure depicted in Fig. 2.4c consists of a simple cubic lattice with a diatomic base. The two ions are located at (0, 0, 0) and (1, 1, 1) × a/2, similar to the rocksalt structure. Typical compounds with cesiumchloride structure are CsCl, NH4 Br, TlCl, AgZn, AlNi, and CuZn.
2.1.6 Wurtzite Structure The wurtzite structure shown in Fig. 2.4d is composed of two hcp sublattices, one for cations and one for anions. In the ideal structure these sublattices are displaced by u = 3/8c along the [00.1] direction, c being the vertical lattice parameter. The ideal ratio of vertical and lateral lattice parameters is c/a = (8/3)1/2 = 1.633. The primitive unit cell contains 1/3 of the volume of the usually applied unit cell of Fig. 2.4d and is spanned by the vectors a1 , a2 , c; its basis comprises four atoms with two anions and two cations. The wurtzite structure has no center of inversion. The u/c ratio of wurtzitetype crystals often deviates from the ideal value 0.375, and likewise the c/a ratio. The deviation gives rise to a macroscopic spontaneous polarization (Sect. 4.1.3), which can cause strong internal electric fields—e.g. in groupIII nitrides up to 3 MV/cm [2]. Lattice parameters for some crystal structures are listed in Tables 2.3 and 2.4. In wurtzite crystals the zigzag chains of bonding lie within a nonpolar 11.0 plane (Fig. 2.6, a plane Fig. 2.1). It is a cleavage plane perpendicular to the (00.1) c plane. The top face of the unit cell represents the polar (00.1) plane. It is often referred to as basal plane, i.e., a plane which is perpendicular to the principal axis (c axis) in a hexagonal or tetragonal structure. The [00.1] ¯ the (00.1) face is made up of cations and, e.g., direction is not equivalent to [00.1]; ¯ face ((00.1) ¯ N in in GaN referred to as (00.1) Ga face, while anions build the (00.1) GaN).
20
2 Structural Properties of Heterostructures
Table 2.3 Lattice parameters of existing and hypothetical tetrahedrally coordinated crystals [1]. Italicized numbers are theoretical results from pseudopotential calculations, E WZB is the calculated energy difference between wurtzite and zincblende structures at T = 0 Solid Wurtzite Zincblende E WZB a (Å) (meV/atom) a (Å) c (Å) c/a u/c GaN InN AlN
3.192 3.095 3.545 3.536 3.112 3.099
5.196 5.000 5.703 5.709 4.980 4.997
1.628 1.633 1.609 1.615 1.600 1.612
3.912
6.441
1.647
0.374
3.979 3.823 3.777 4.137 4.121
6.497 6.261 6.188 6.716 6.682
1.633 1.638 1.638 1.624 1.621
0.376
3.800 2.51 2.490
6.269 4.12 4.144
1.650 1.641 1.665
0.378
−11.4
0.374 0.374
3.539
25.3
0.381
AlAs
CdS
0.375 0.377
Si C
−9.9
4.983 5.431 4.365 5.653 5.654 5.660 5.620 5.410 5.345 5.818 5.811 5.431 5.392
0.380
GaAs
ZnS
4.531 4.364
−18.4 12.0 5.8 3.1 −1.1 11.7
2.1.7 Thermal Expansion Epitaxy is performed at temperatures far above room temperature to provide sufficient mobility of adatoms on the growing crystal surface. Typical growth temperatures are around 600 °C, but materials may require substantially lower or higher temperatures (e.g., compound semiconductors containing Hg below 200 °C or nitrides well above 1000 °C). Cooling after epitaxy over a wide range to room temperature or cryogenic temperatures is accompanied by a significant diminution of the lattice constant due to anharmonic terms of the crystal potential. The difference in the thermal expansion of substrate and layer materials may induce large strain in the structure, leading to bending of the substrate and, in case of tensile strain, to cracks in the epitaxial layer. Large differences in the thermal expansion of layers within a heteroepitaxial structure may hence seriously affect structural properties and lead to the requirement of inserting suitable buffer layers to accommodate the thermal mismatch. Within the thermal range of interest usually the description of a temperaturedependent lattice parameter a(T ) by a linear thermal expansion coefficient (TEC) α is applied according to
2.1 Basic Crystal Structures
21
Table 2.4 Linear thermal expansion coefficients and lattice parameters of some cubic and hexagonal semiconductors at 300 K. Data reported in literature have significant scatter, particularly for hexagonal structures. Listed values represent some mean data Semiconductor Lattice parameter (Å) Thermal expansion coefficient (10−6 K−1 ) a c αa αc GaAs AlAs InAs GaP AlP InP ZnS ZnSe CdTe Si Ge SiC (3C) SiC (6H) GaN AlN InN ZnO Al2 O3
5.6535 5.661 6.058 5.4509 5.4635 5.8690 5.410 5.668 6.484 5.4310 5.6576 4.3596 3.0806 3.189 3.112 3.533 3.249 4.758
– – – – – – – – – – – – 15.1173 5.186 4.982 5.693 5.207 12.991
5.7 5.2 5.1 4.8 ∼5 4.7 7.1 ∼7.4 4.9 2.6 5.7 2.8 4.2 ∼4.5 ∼4.2 ∼3.8 ∼4.7 ∼8.1
– – – – – – – – – – – – 4.7 ∼4.0 ∼5.3 ∼2.7 ∼2.9 ∼7.3
a(T ) − a(T0 ) = α × (T − T0 ). a(T0 ) Usually room temperature is taken as reference temperature T0 . The thermal change of volume is in general anisotropic and α is consequently a second rank tensor. It is described by three components αi the principal axes of which are along those of the strain tensor (Sect. 2.2.2). Along a principal axis the respective component αi is defined by 1 ∂a . αi = a ∂T P For cubic crystals the three components αi are identical and the expansion coefficient becomes a scalar. Crystals with a hexagonal structure have two independent components, namely αa = α⊥ perpendicular to the c axis and αc = α along the c axis. Linear expansion coefficients of semiconductors are typically of the order mid 10−6 K−1 . Data for some semiconductors are given in Table 2.4. The thermal expansion is actually not a linear function of temperature. The expansion coefficients depend on temperature and are usually positive quantities. Below
22
2 Structural Properties of Heterostructures
Table 2.5 Coefficients for a polynomial fit of the temperature dependent lattice parameter a(T ) of some cubic semiconductors; the reference temperature is T0 = 300 K Semiconductor
A
B (10−6 K−1 )
C (10−9 K−2 )
D (10−12 K−3 )
Range (K)
GaAs
−1.47 × 10−3
4.239
2.916
−0.936
200–1000
Si
−0.71 × 10−3
1.887
1.934
−0.4544
293–1600
Ge
−1.533 × 10−3
4.636
2.169
−0.4562
293–1200
100 K semiconductors with zincblende or diamond structure show a commonly not observed negative thermal expansion [3, 4]. Above 300 K coefficient values slightly increase if the temperature is raised. An empirical relation by a polynomial fit is sometimes applied to account for the temperature dependence of the thermal expansion. In a specified temperature range the lattice parameter is then described by a(T ) = a(T0 ) 1 + A + BT + C T 2 + DT 3 , where T0 is the reference temperature (generally 300 K) and T is the absolute temperature in K. Values for some cubic semiconductors are given in Table 2.5.
2.1.8 Structural Stability Map Rules to predict crystal structures of solids from properties of atoms require firstprinciple calculations with a high degree of accuracy, because the difference in equilibrium energies of a given compound in two closely related structures is often less than 0.1% of the cohesive energy. In the corresponding problem of the regularities of the periodic table of the elements, a scheme with the two integral coordinates principal and orbital quantum number was found. Starting from classical approaches using atomic radii and Pauling’s electronegativity, today some largely universal schemes for predicting the structural stability of many intermetallic compounds of the form A x B y , of spbonded An B p−n ( p = 8 or 2, . . . , 6) semiconductors and insulators, and of highTc superconductors have been suggested. The success rate generally exceeds 95%, and domains of different overlapping structure types could be related to polymorphic structural forms [1, 5–8]. Most schemes use orbital radii coordinates R, which are linear combinations of the s and porbital radial functions R A and R B of the atoms building the AB compound: Rσ (A, B) = R pA + RsA − R pB + RsB , Rπ (A, B) = R pA − RsA + R pB − RsB .
(2.1a) (2.1b)
2.1 Basic Crystal Structures 5
NaCl
4
R (a0)
Fig. 2.5 Structural stability map for binary AB compounds, calculated using atomic orbital radial functions in units of the Bohr radius. NaCl, W, ZB, and Gr denote sodiumchloride, wurtzite, zincblende, and graphite structures, respectively. The misaligned cross in the zincblende range marks a NiAs structure, the triangles cinnabar (HgS) structure. From [1]
23
W
3 2 1
ZB
Gr
0 0.5
0
0.5
1
R (a0)
1.5
2
Rσ provides a measure of the size difference between atoms A and B, and roughly scales with ionicity. Rπ scales with the atomic s and p energy difference and measures to some extent sphybridization. Figure 2.5 shows a structural stability diagram for binary compounds of the form An B 8−n like GaIII AsV , using radii of (2.1a)–(2.1b) at which the allelectron atomic radial orbitals r × Rnl (r ) have their outer maxima. Zincblende and wurtzite are the most common crystal structures of binary semiconductors. For these structures the orbital radii coordinates given in (2.1a)–(2.1b) were used to calculate the equilibrium energy difference E W−ZB between the ideal wurtzite and the zincblende structure, cf. Table 2.3. Calculated structural deviations from ideal wurtzite are small, the energy gain due to such relaxations is generally smaller than 1 meV per atom (except for AlN, −2.7 meV) [1]. The study confirms the phenomenological correlation, that wurtzitestable compounds have smaller c/a ratios than the ideal value, while zincblende and diamondstable compounds have larger ratios. As a further rule of thumb, a large difference in electronegativity and atomic radii of atoms A and B favor the wurtzite structure.
2.1.9 Polytypism Small values of equilibrium energy differences between wurtzite and zincblende structure E WZB given in Table 2.3 indicate an intrinsic low stability of the crystal structure of some solids. In fact many solids may crystallize in multiple crystal structures having identical stoichiometries, a phenomenon called polymorphism. Wurtzite and zincblende are two structures of a onedimensional polymorphism referred to as polytypism. For a graphic representation of such polytypes of tetrahedrally coordinated AB compounds a plot of the cationanion zigzag chains, which lie in the (11.0) plane of the hexagonal lattice and in the (110) plane of the zincblende lattice,
24
2 Structural Properties of Heterostructures
3C
4H
A
C
A
C
B
B
B
A
C
A
C
B
B
B
A
C
A
B
C
c
B A A B C A B C
6H
c
A
C
C
B
B A
A A B C A B C
A B C A B C A
Fig. 2.6 Stacking sequences of binary AB compound polytypes depicted in the (11.0) plane of the hexagonal lattice. Labels A, B, and C on the horizontal axis refer to atom sites, while such labels on the vertical axis denote net planes as shown in Fig. 2.3b
is useful. Figure 2.6 shows three prominent polytypes, the zincblende 3C structure, and the two structures 4H and 6H. The number in the notation refers to the periodicity, while C and H designate a cubic and hexagonal structure, respectively. Using this notation, the wurtzite structure is labeled 2H. There are numerous such polytypes known from some compounds, more than, e.g., 100 for ZnS and about 170 for SiC; they build cubic (3C), hexagonal (H), and rhombohedral (R) structures. All these modifications have the same lateral lattice constant a in the representation chosen above, while c is an integer multiple of the layer thickness. All polytypes may be considered as mixtures of 3C and 2H. The 4H modification is then composed equally of cubic ( ABC next neighborhood) and hexagonal (AB A) bonds. The notation of a given polytype by periodicity is not unambiguous, e.g., periodic stacks of ABC AC B and ABC B AB form inequivalent hexagonal 6H modifications. The different polytypes of a given compound have widely ranging physical properties. The bandgap energy generally becomes greater as the wurtzite component increases, see Table 2.6. The number of atoms within a unit cell and that of inequivalent atom sites increases with the size of the unit cell, and consequently also the number of phonon branches. The electron mobility of the high symmetry 3C polytype may be higher due to reduced phonon scattering. Furthermore, a particular doping impurity on inequivalent sites has different electronic properties due to a more cubic or hexagonal environment.
2.1 Basic Crystal Structures
25
Table 2.6 Physical properties of some polytypes, arranged in increasing order of wurtzite character. The number of atoms refers to the primitive unit cell, E g denotes the bandgap energy at 2 K. Data from [9–11] Polytype 3C 15R 6H 4H 2H Space group symmetry Atoms per unit cell Inequivalent sites SiC E gX (eV) a (Å) c (Å) ZnS E g (eV) a (Å) c (Å) GaN E g (eV) a (Å) c (Å)
Td 2 1 2.390 4.349 3.85 5.410 – 3.21 4.50 –
C3v 10 5 2.906 3.08 37.70
C6V 12 3 3.023 3.081 15.117
C6V 8 2 3.265 3.073 10.053
3.83 46.88
3.82 18.72
3.81 12.46
C6V 4 1 3.330 3.076 5.048 3.91 3.823 6.260 3.503 3.189 5.185
A selfcontained theory explaining the origin of polytypes with up to more than 100 planes within a period does not yet exist. The occurrence of long periods is often associated with dislocations (Sect. 2.3), e.g., screw dislocations which induce spiral growth. In such case the periodicity is determined by the step height of the growth spiral. Shortperiod polytypes may be stabilized by growth conditions given by temperature, pressure or gasphase composition, due to different minima in the formation energy.
2.1.10 Random Alloys and Vegard’s Rule Mixing two or more solids to an alloy, i.e., a solid solution, is an old technique to modify properties of materials. Alloys with two, three, or four components are called binary, ternary or quaternary alloys, respectively. In substitution alloys atoms of comparable size are simply substituted for one another in the crystal structure. Such alloys are routinely made from semiconductors to engineer properties like lattice parameter or bandgap. Metals may also form interstitial alloys, where atoms of one component are substantially smaller than the other and fit into the interstices between the larger atoms. Usually a random mixing of the atoms on the semiconductor latticesites of the alloy is intended. Limits in the miscibility of the components or ordering effects in the alloy may, however, lead to significant deviations from a random distribution and consequently to altered physical properties of the alloy. There are three extreme cases occurring in alloy formation.
26
2 Structural Properties of Heterostructures
• Random alloy: The probability of an atom next to a given atom in an A x B1−x alloy is x for an Aatom and (1 − x) for a Batom. This is the case usually wanted for applications. • Ordered alloy: Atoms in the alloy have a regular periodic structure. The crystal structure is then given by placing at each site of the Bravais lattice a multiatomic base, yielding translational symmetry of the Bravais lattice in the alloy. Examples are βbrass with alternating Cu and Zn atoms along [111] or CuPt structure of In1−x Gax P at x ≈ 0.5. Since ordering requires a specific ratio in the number of the atom types forming such alloys, they are also referred to as stoichiometric alloys. • Phase separation: Atoms of type A and B do not mix and are located at different regions in the solid. We consider the technologically important random alloy in more detail. We assume two compound semiconductors AC and BC having the same crystal structure, A and B representing cations and C an anion. Alloying leads to a semiconductor A x B1−x C with a mixture of A and B atoms on the cation sublattice, while all sites on the anion sublattice remain occupied by C atoms. Since the alloying forms a binary sublattice (the unmixed materials AB and AC are already binary compounds themselves) such alloys are called pseudobinary (often also referred to as ternary, though in a true ternary all components mix on the same lattice). The concept may be extended to compounds A x B1−x C y D1−y usually termed quaternary compound. The composition parameter x in the pseudobinary alloy A x B1−x C denotes that on the average an anion C has x neighbors of type A and a fraction of 1 − x neighbors of type B. A number of properties of true alloys are expected to scale by a smooth interpolation between the two endpoint materials. This is usually well fulfilled for the lattice constant. The empirical rule called Vegard’s rule [12] states that a linear interpolation exists, at constant temperature, between the crystal lattice constant of an alloy and the concentrations of the constituent elements. The lattice constant aalloy from two materials A and B with the same crystal structure and lattice constants a A and a B , respectively, is hence given by aalloy = xa A + (1 − x)a B .
(2.2a)
The lattice constant of a (pseudobinary) ternary alloy with a mixture of compounds AC and BC is given by the same relation putting a A and a B to a AC and a BC , respectively. The linear relationship also holds for quaternary alloys. For compounds of the type A x B y C1−x−y D the interpolation yields aalloy = xa AD + ya B D + (1 − x − y)aC D .
(2.2b)
The lattice parameter for alloys of the type A x B1−x C y D1−y , where atoms A and B mix on one sublattice and atoms C and D on another sublattice, is calculated from the ternary parameters a ABC , a AB D , a AC D , and a BC D ,
2.1 Basic Crystal Structures
27
x(1 − x)[ya ABC (x) + (1 − y)a AB D (x)] + y(1 − y)[xa AC D (y) + (1 − x)a BC D (y)] , x(1 − x) + y(1 − y) (2.2c) a ABC (x) = xa AC + (1 − x)a BC ,
aalloy =
a AB D (x), a AC D (y), and a BC D (y) accordingly.
Fig. 2.7 Mean cationcation distance dc in Zn1−x Mnx Se for varying Mn concentration x. The distance dc increases linearly with x according to Vegard’s rule also across a change of crystal structure. From [15]
cationcation distance d dcc (Å)
Using Vegard’s rule (2.2a)–(2.2c) lattice matching to a substrate lattice parameter is achieved using an appropriate composition x (and y) of materials with a larger and a smaller lattice parameter. Example: In0.53 Ga0.47 As for epitaxy on InP (aInAs = 6.0584 Å, aGaAs = 5.6533 Å, aInP = 5.8688 Å). It must be noted that the adjustment of lattice parameters by alloying is accompanied by a change of the bandgap energy and other properties. Often the composition is rather chosen for obtaining a desired band gap in the alloy. In a quaternary alloy lattice parameter and bandgap energy can be adjusted independently (Sect. 4.1.5). Note that exact lattice matching is generally met only for a given temperature, because the lattice parameter varies as the temperature is changed (e.g., from growth temperature to room temperature) and different materials like substrate and layer have usually different thermal expansion coefficients (cf. Sect. 2.1.7). For stable two and threedimensional centralforce networks (e.g. triangular net or fcc lattice) Vegard’s rule was derived from quite general assumptions [13]. Deviations from the linear relation are always found in metallic alloys [14], but they are in practice usually negligible in miscible semiconductor alloys. Vegard’s rule is therefore routinely used to measure the composition of a studied alloy from its lattice parameter aalloy using, e.g., Xray diffraction. Vegard’s rule may more generally apply for the average interatomic distances in solids if structural changes without change of the coordination number occur in an alloy. The example given in Fig. 2.7 shows the nextneighbor distance on the cation sublattice in the diluted magnetic semiconductor Zn1−x Mnx Se with magnetic Mn2+ ions substituting the nonmagnetic Zn2+ cations. For a fraction exceeding x ≈ 0.3 the crystal structure changes from zincblende to wurtzite. The c/a ratio of wurtzite √ ZnMnSe is close to the ideal value of 8/3, indicating a close relationship to an ideal close packing arrangement [15]. The type of coordination does not change across
4.2
Zincblende
Wurtzite
4.1 Powder data Single crystal data
4.0 0.0
0.5
Mn concentration xx
1.0
28
2 Structural Properties of Heterostructures
the region in which the alloy changes between the crystal structures, which both are based on a closest packing of spheres. Such factors favor compliance with Vegard’s rule. The simple linear relation of the concentrationweighted average bond length expressed by Vegard’s rule (2.2a), (2.2b) suggests that the chemical bond of atoms in an alloy smoothly changes between the values of the endpoint materials. Such assumption is the premise of the virtualcrystal approximation (VCA) discussed below (Sect. 2.1.11). In real semiconductors this is not compelling. Experiments like extended Xray absorption fine structure measurements (EXAFS) [16, 17] show that bond lengths in a semiconductor alloy are actually much closer to those of the endpoint materials. The bond length calculated using Vegard’s rule originates essentially from the weighted average of alternating bonds [18]. The difference between Vegard’s rule and actual bond lengths is illustrated for the pseudobinary alloy Ga1−x Inx As. Both GaAs and InAs crystallize in zincblende structure. They are miscible over the entire range and form a random alloy. In Xray diffraction (XRD) measurements the lattice constant of this alloy is found to vary linearly with the In composition x according to Vegard’s √ rule. This behavior is shown in terms of the measured cationanion bond length 3 × a/4 in Fig. 2.8a (squares) [19]. In contrast, a measurement of the local bond length using EXAFS demonstrates that actually two different types of bonds exist in the alloy: shorter Ga–As bonds and longer In–As bonds, yielding in average a bond length varying
(a)
In  As 4.32
2.55
CationCation distance (Å) Anionanion distance (Å)
Nearneighbor distance (Å)
2.60
XRD VCA
2.50
Ga  As 2.45 0.0
0.2
0.4
0.6
0.8
In concentration xx
1.0
(b) 4.24
As  In  As
Ga  In
4.16
VCA
In  In 4.08
Ga  Ga
4.00 0.0
As  Ga  As 0.2
0.4
0.6
0.8
1.0
In concentration xx
Fig. 2.8 a Cationanion nearneighbor distance as a function of In mole fraction in Ga1−x Inx As alloys. Circles and squares refer to EXAFS and XRD data, respectively, the dotted line is the cation√ anion bond length ( 3 × a/4) according to the virtualcrystal approximation (VCA), calculated from the Xray lattice constant. b As–As secondneighbor distance corresponding to As–Ga–As and As–In–As bonds (black circles) and Ga–Ga, In–In, and Ga–In secondneighbor distances, denoted by gray triangles, squares, and circles, respectively. The dotted line represents values expected c 1983 APS from the VCA. Reproduced with permission from [16],
2.1 Basic Crystal Structures
29
linearly with composition. Figure 2.8a shows that the actual individual bond lengths are close to those of GaAs and InAs, and that they vary only little. Consequently the two secondnext neighbor distances of anions As–Ga–As and As–In–As given in Fig. 2.8b differ and remain almost constant for all compositions x. This is not the case for the secondnext neighbor distances of cations depicted with gray symbols in the figure. The distances of atoms on the cation sublattice are all within ∼0.05 Å of the linear interpolation suggested by Vegard’s rule and the VCA considered below. Distances of In–In are above, Ga–Ga below, and Ga–In very close to the VCA line given in Fig. 2.8b. It should be noted that the bimodal nearneighbor distance shows a quite small width of the distribution, whereas all secondnearest neighbor distributions are rather broad [16]. The data demonstrate that the atomic scale structure of Ga1−x Inx As alloys features a nearneighbor distribution which consists of two well defined distances. In contrast, the secondnearest neighbor mixed cation distances exhibit a single broadened distribution, and the corresponding common anion distribution is bimodal. The cation sublattice hence approaches a linearly interpolated VCA lattice, while the anions suffer a local displacement from the average position in the lattice. The origin of this behavior was explained in terms of differences in the distortion energy and the consequential mixing enthalpy [20].
2.1.11 VirtualCrystal Approximation The virtualcrystal approximation (VCA) assumes an ideal hypothetical crystal to model the properties of a random alloy formed by atoms A and B on a (sub) lattice. In a VCA crystal atoms A and B are replaced by a single kind of atoms C whose properties are assumed as a linear average of those of A and B. The virtual alloy made of pseudoatoms C has hence a crystal structure common to the crystals made of either A or B atoms with a linearly averaged crystal potential. The assumption strongly reduces computational complexity and leads to a great popularity of the approach. The VCA has been applied to semiconductor alloys within various schemes like the semiempirical pseudopotential method or the empirical tightbinding method. A VCA crystal contains solely a single type of bonds and yields the linear relationship of lattice parameters in the alloy expressed by Vegard’s rule (2.2a)–(2.2c). The approximation succeeded in calculating a number of problems like the fact of an optical bandgap bowing discussed in Sect. 4.1.5. It must be noted that properties depending on local differences in the potentials of individual atoms like charge redistribution or polarization are precluded in the VCA approach. Effects arising from such differences as atomAlike and atomBlike features, also referred to as chemical disorder, are not correctly described by the VCA approach.
x 0
x+ x ∇
x x+u ∇ ∇
u
x
u
∇
0
∇
Fig. 2.9 Deformation of a dilatable string in an unstrained (top) and strained state (bottom). The origin is assumed to be fixed
2 Structural Properties of Heterostructures
∇
30
x+ u
2.2 Elastic Properties of Heterostructures An epitaxial layer with a chemically different composition and potentially also a different structure compared to the substrate represents a heterostructure. If the interface does not contain structural defects, the layer—and to some minor extent also the substrate—are strained, because the lattice parameters of layer and substrate will generally differ due to differences in bond lengths and thermal expansion coefficients. The elastic properties of the heterostructure can, to a very good approximation, be determined using continuum mechanics, i.e., a macroscopic theory. To assess the effect of the structural and thermal misfits, we first consider the macroscopic effect of stress on the deformation of solids in general. An introduction into this classical subject may be found in, e.g., [21, 22].
2.2.1 Strain in One and Two Dimensions Stress leads to a deformation (strain) of a solid. For a onedimensional problem the effect of strain on a dilatable string is illustrated in Fig. 2.9. A point at an arbitrary position x is displaced by u. In homogeneous stretching u is a linear function of x, and the section x is strained to x + u. The strain of the section x can now be defined as e = du/d x. It is a dimensionless quantity and small compared to 1. We now extend the problem to the twodimensional strain of a plane sheet. Here, the strain is specified by the four quantities ei j = du i /d x j for i, j = 1, 2.
(2.3)
The quantities ei j can be regarded as components of a secondrank tensor described by a 2 × 2 matrix. Without any distortion all components are expected to vanish. This is, however, not fulfilled for components defined in such a way; a simple rigidbody rotation leads to nonzero offdiagonal components. To meet the condition of zero components at zero distortion, the tensor is expressed as a sum of a symmetrical and an antisymmetrical tensor, yielding components ei j = εi j + εi j . Only the symmetrical part
2.2 Elastic Properties of Heterostructures
εi j =
31
1 (ei j + e ji ) = ε ji 2
(2.4)
is defined as the strain (the antisymmetrical components are εi j = 21 (ei j − e ji ) = −ε ji ). The twodimensional strain tensor then reads ε=
1 (e 2 12
e11 1 (e + e21 ) 2 12
+ e21 )
e22
.
(2.5)
In absence of a rotation, the diagonal components ε11 and ε22 directly measure the extensions or compressions per length along the x and yaxes, respectively. The offdiagonals ε12 = ε21 measure the shear strain. The antisymmetrical tensor contains only the two offdiagonal elements 21 (e12 − e21 ) and describes a pure solidbody rotation potentially connected to the deformation of the area. The deformation of an area (x1 , x2 ) in the plane sheet is given by (x1 + u 1 , x2 + u 2 ) with the two displacement components u i =
∂u i ∂u i x1 + x2 = ei1 x1 + ei2 x2 for i = 1, 2. ∂ x1 ∂ x2
2.2.2 ThreeDimensional Strain The description of threedimensional strain is a generalization of the former cases. The three diagonal components εii = eii (i = 1, 2, 3) = εx x , ε yy , εzz , are the tensile or compressive strains. They occur along the x, y, and zaxis, respectively, if no rotation is connected to the deformation. The sum of the diagonal components yields the relative change of volume originating from the strain, V εii . = V i=1 3
(2.6)
In the offdiagonal elements the quantities ei j describe rotations similar to the twodimensional case. e12 describes an anticlockwise rotation about the zaxis, e21 = −e12 . Similarly, e13 and e23 describe rotations about the y and xaxes, respectively. The offdiagonal terms of ε are again symmetrized and represent shear strains, εi j =
∂u j 1 ∂u i , + 2 ∂ xj ∂ xi
yielding the threedimensional strain tensor
(2.7)
32
2 Structural Properties of Heterostructures
⎡
e11 1 ε = ⎣ 2 (e12 + e21 ) 1 (e + e31 ) 2 13
1 (e 2 12
+ e21 )
e22 1 (e 2 23
+ e32 )
1 (e 2 13 1 (e 2 23
⎤ + e31 ) + e32 ) ⎦ .
(2.8)
e33
Since the strain tensor is symmetric, only 6 of the 9 components are independent. The 6 independent components are often written according to the Voigt notation in form of a 6 × 1 matrix for short. This symbolic vector is formed by the index substitution 11 → 1, 22 → 2, 33 → 3, 23 and 32 → 4, 31 and 13 → 5, and 12 and 21 → 6, yielding ⎛ ⎞ ε1 ⎜ ε2 ⎟ ⎤ ⎡ ⎜ ⎟ ε11 ε12 ε13 ⎜ ε3 ⎟ ⎟ ⎦ ⎣ (2.9) ε = ε12 ε22 ε23 → ε = ⎜ ⎜ ε4 ⎟ . ⎟ ⎜ ε13 ε23 ε33 ⎝ ε5 ⎠ ε6 In the Voigt notation the shear components of the strain tensor are usually defined in terms of an engineering convention instead of the physical convention used above. engin. The engineering quantities are εi j = 2εi j , i = j. This allows for writing Hooke’s law in the simple notation with reduced indices (2.10). A 3 × 3 matrix composed of engin. and the diagonals εii of ε does, however, not form a tensor, the offdiagonals εi j because such array does not transform according to the rules of a secondrank tensor [21]. This must be considered if the strain occurs not along the principal directions. We briefly consider the threedimensional stress, which gives rise to the strain treated above. Similar to the strain ε all stress components are combined in a symmetric second order stress tensor σ , which often is likewise written in form of a vector. Any stress may be composed of three components: uniaxial stress, shear stress, and hydrostatic stress. Uniaxial tensile or compressive stresses σx x , σ yy , and σzz , act along the axes x, y, and z, respectively. They are built by force pairs acting normal to the surfaces (see Fig. 2.10) and have the unit of a force per area, i.e., N/m2 or Pa. If the forces act tangentially, they create a shear stress and are labeled σx y , σ yz , and σx z . The first and second index denote the axis of force direction and the normal of the surface where the force acts, respectively. In the Voigt notation the same index substitution is used as that applied for the strain, but no factor of 2 is put into the offdiagonal elements.
2.2.3 Hooke’s Law If the strain is not too large, the interaction potential of the atoms in the solid is well described in the harmonic approximation, and we obtain a linear relationship between stress and resulting strain. For the analogous problem of a spring, Robert Hooke stated in the 17th century that the force exerted by a mass attached to a spring is
2.2 Elastic Properties of Heterostructures
33
(b)
(a)
x
(c)
xy xx
l
y x
l
xx
yy
zz
l
Fig. 2.10 Deformation of a solid by a uniaxial stress, b shear stress, and c hydrostatic stress
proportional to the amount the spring is stretched. In the generalized Hooke’s law the constant of proportionality in the onedimensional case is replaced by the elasticity stiffness tensor C. C is a fourthorder tensor comprising 34 = 81 components Ci jkl . By considering all symmetries present in crystalline solids, the number of nonzero components is reduced to 36. C is usually written according to Voigt’s notation in form of a 6 × 6 matrix by putting Ci jkl = Cmn (i, j, k, l = 1, 2, 3; m, n = 1, . . . , 6). Using the Voigt notation for stress and strain defined in (2.9) and accordingly the 6 × 6 matrix representation for C, Hooke’s law reads ⎞ ⎛ C11 σ1 ⎜ σ2 ⎟ ⎜ C21 ⎜ ⎟ ⎜ ⎜ σ3 ⎟ ⎜ C31 ⎜ ⎟=⎜ ⎜ σ4 ⎟ ⎜ C41 ⎜ ⎟ ⎜ ⎝ σ5 ⎠ ⎝ C51 σ6 C61 ⎛
C12 C22 C32 C42 C52 C62
C13 C23 C33 C43 C53 C63
C14 C24 C34 C44 C54 C64
C15 C25 C35 C45 C55 C65
⎞⎛ ⎞ ε1 C16 ⎜ ε ⎟ C26 ⎟ ⎟⎜ 2 ⎟ ⎜ ε3 ⎟ C36 ⎟ ⎟ ⎜ engin. ⎟, ⎜ ⎟ C46 ⎟ ⎟ ⎜ ε4engin. ⎟ ⎠ C56 ⎠ ⎝ ε5 engin. C66 ε6
(2.10)
engin.
where εi denotes shear components of the strain according to the engineering convention. Equation (2.10) may be written σ = Cε for short. The inverse relation is given by the compliance matrix S = C−1 , yielding ε = Sσ . In Voigt’s notation of S some factors appear, which are not necessary in C [21]: Smn = Si jkl when m and n are 1, 2, or 3; Smn = 2Si jkl for either m or n being 4, 5, or 6; Smn = 4Si jkl when both m and n are 4, 5, or 6. A particular stress component is given by σi =
6 k=1
Cik εk ,
(2.11)
34
2 Structural Properties of Heterostructures
where εk denotes the engineering quantities when k > 3. The components of the elasticity matrix C are called (second order) elastic stiffness constants. C is a symmetric engin. with matrix, which has at most 21 independent coefficients. The factor of 2 in εk respect to εk had to be introduced in order to write Hooke’s law in this simple form with reduced indices. If we write (2.11) in the initial full tensor notation σi j =
3 3
Ci jkl εkl ,
(2.11a)
k=1 l=1
we obtain for the offdiagonals the summands Ci jkl εkl + Ci jlk εlk (k = l). In the shorter matrix notation (2.11) the corresponding summands Cmn εn (n = 4, 5, 6) only appear once. The missing factor of 2 is therefore put into the offdiagonal elements by introducing the engineering convention. The procedure has the disadvantage that it applies only for strain along the principal axes for the usually listed constants Cmn , e.g., along the [001] direction. For other orientations (2.11a) needs to be rotated to obtain a transformed elasticity tensor Ci jkl [23]. We return to the simplified C matrix of (2.10) with 21 independent coefficients. For crystal structures with high symmetry, many of these coefficients are 0. In addition, some coefficients are related to others. Any cubic crystal structure has only 3 independent elastic stiffness coefficients, namely C11 , C12 , and C44 . This strong reduction originates basically from the equivalence of the three cubic axes. Any hexagonal crystal structure has 5 independent coefficients. As an example, the matrix notations of the elasticity tensors of a cubic and a hexagonal structure are given by ⎛
Ccubic
Chexagonal
C11 ⎜ C12 ⎜ ⎜ C12 =⎜ ⎜ 0 ⎜ ⎝ 0 0 ⎛ C11 ⎜ C12 ⎜ ⎜ C13 =⎜ ⎜ 0 ⎜ ⎝ 0 0
⎞ C12 C12 0 0 0 C11 C12 0 0 0 ⎟ ⎟ C12 C11 0 0 0 ⎟ ⎟, 0 ⎟ 0 0 C44 0 ⎟ 0 0 0 C44 0 ⎠ 0 0 0 0 C44 C12 C13 0 0 C11 C13 0 0 C13 C33 0 0 0 0 C44 0 0 0 0 C44 0 0 0 0
0 0 0 0 0
C11 −C12 2
⎞
(2.12)
⎟ ⎟ ⎟ ⎟. ⎟ ⎟ ⎠
Values of Cmn for some solids are listed according to the engineering notation in Table 2.7. For isotropic solids only 2 independent stiffness constants exist, describing the response on axial and shear stress. For such materials C is given by the cubic matrix in (2.12), putting C44 = 21 (C11 − C12 ). The two independent elastic constants are called Lamé constants μ = G = C44 and λ = C12 . G is the shear modulus. Often any other two constants are used, and a number of relations exist to express their dependences.
2.2 Elastic Properties of Heterostructures
35
Table 2.7 Elastic stiffness constants of some cubic and hexagonal solids at room temperature, given in units of 1010 Pa. Column 2 denotes structures as discussed in Sect. 2.1, values for carbon (C) refer to the diamond modification Material Structure C11 C12 C13 C33 C44 Au [24] Al [25] W [25] Mg [24] NaCl [24] CsCl [24] C [9] Si [9] ZnS [9] ZnSe [9] GaAs [9] AlAs [9] InAs [9] GaN [26] AlN [26] InN [26] ZnO [27]
fcc fcc bcc hcp NaCl CsCl D D ZB ZB ZB ZB ZB W W W W
19.0 10.9 51.5 5.9 4.9 3.7 107.6 16.6 9.8 9.0 11.9 11.9 8.3 39.0 39.6 22.3 20.6
16.1 6.3 20.4 2.6 1.3 0.9 12.5 6.4 6.3 5.3 5.4 5.7 4.5 14.5 13.7 11.5 11.7
– – – 2.1 – – – – – – – – – 10.6 10.8 9.2 11.8
– – – 6.2 – – – – – – – – – 39.8 37.3 22.4 21.1
4.2 2.8 15.6 1.6 1.3 0.8 57.7 8.0 4.5 4.0 6.0 5.7 4.0 10.5 11.6 4.8 4.4
If the elastic properties of isotropic solids are expressed in terms of components of the compliance matrix S, the two independent components are S11 = 1/E and S12 = −ν/E; S44 = S55 = S66 then equals (2 + 2ν)/E. E is Young’s modulus (also referred to as elastic modulus) and represents the ratio stress/strain, and ν is Poisson’s ratio considered below. The two quantities are related to the Lamé constants by E=
μ(2μ + 3λ) , μ+λ
ν=
λ . 2(μ + λ)
2.2.4 Poisson’s Ratio Virtually all common materials undergo a transverse contraction when longitudinally stretched, and a transverse expansion when longitudinally compressed. The quotient of such deformations is a material property termed Poisson’s ratio ν: ν = −(transverse strain/longitudinal strain) for a uniaxial tensile stress applied in longitudinal direction. It is usually a positive quantity, though also negative Poisson’s ratios were reported for novel foam structures called antirubber which have interatomic bonds realigning with deformation [28]; for more information see [29].
36
2 Structural Properties of Heterostructures
For isotropic solids comprising polycrystalline materials ν is given by the ratio of the two independent stiffness constants C11 /C12 . For nonisotropic materials like any crystalline solid ν depends on the stress direction. For cubic materials and stress along an axis of the unit cell, the ratio is ν = C12 /(C11 + C12 ), for other axes and symmetries the relation gets more bulky [30]. Values for Poisson’s ratios range between 0.5 (incompressible medium) and −1 (perfect compressibility), values for ordinary materials are between 0.25 and 0.3 for common semiconductors, 0.45 for Pb, and 0.33 for Al.
2.2.5 Pseudomorphic Heterostructures We consider a free standing crystalline structure consisting of two layers, which have a common interface as delineated in Fig. 2.11. We assume the layers to have the same cubic crystal structure, but—in absence of the common interface—different unstrained lattice constants a and thicknesses t labeled a1 , t1 , a2 , and t2 , respectively. If the difference in lattice constants is not too large (say, below 1%), the layers may form an interface without structural defects and adopt a common inplane lattice constant a parallel to the interface, with an intermediate value a1 > a > a2 . Since a
is smaller than the relaxed (unstrained) lattice parameter a1 , layer 1 is compressively strained in lateral direction (i.e., parallel to the interface) by the contact to layer 2. Layer 1 consequently experiences a distortion also in the vertical direction to approximately maintain its bulk density. The vertical lattice constant a1⊥ of the strained layer 1 is hence larger than the unstrained value a1 . Vice versa layer 1 exerts a laterally tensile stress on layer 2, leading likewise to a vertical strain a2⊥ < a2 . Such a heterostructure is called pseudomorphic, and the layers are designated coherently strained.
layer 1 kompressive strain
a1
layer 2 tensile strain
a2 a
Fig. 2.11 Schematic of a heterostructure consisting of two layers with a common interface. a is the common lateral lattice constant, a1⊥ and a2⊥ denote the vertical lattice constants of the strained layers 1 and 2
2.2 Elastic Properties of Heterostructures
37
In the strained cubic heterostructure illustrated in Fig. 2.11, the strain in the two lateral directions, say x and y, is equal, εx x = ε yy = ε . Such a biaxial strain results in a tetragonal distortion. Since the structure is assumed to be freestanding, no force is applied along the zdirection. The stress tensor component σzz is thus always zero. Inserting the cubic elasticity tensor (2.12) into Hooke’s law (2.10) and setting up (2.11) for σzz , we obtain a relation between the diagonal strain components and hence between ε and ε⊥ : σzz = 0 = C12 εx x + C12 ε yy + C11 εzz , C12 εx x + C12 ε yy 2C12 =− εx x , C11 C11 ε⊥ = −D001 ε .
εzz = −
(2.13)
The distortion factor D001 is given in (2.17) also for other orientations of the interface. Vertical strain εzz = ε⊥ and lateral strain ε virtually always have opposite sign, since common stiffness constants Ci j are positive quantities. The volume of the unit cell is usually not preserved during deformation: The effect of the counteracting strain perpendicular to the interface does not fully compensate the inplane strain. In the case of a tetragonal distortion no inplane shear strain occurs, the respective offdiagonal elements of the strain tensor are hence zero. According to (2.6) the volume change is given by the trace of the strain tensor, V /V = εx x + ε yy + εzz .
(2.14)
The inplane lattice constant a of the pseudomorphic heterostructure (Fig. 2.11) is given by a balance of the elastic strain minimizing the strain energy [31], a G 1 t1 + a G 2 t2 = a 1 G 1 t1 + a 2 G 2 t2 , a 1 G 1 t1 + a 2 G 2 t2 . a = G 1 t1 + G 2 t2
(2.15)
G denotes the shear modulus and depends on the crystal structure and the crystallographic orientation of the interface plane. a and t are the unstrained lattice parameter and the thickness of the respective layer. For a cubic structure, like e.g. zincblende, the shear moduli G i of layers 1 and 2 are given by i i (1 − Di /2), + 2C12 G i = 2 C11 with the distortion factors D of the respective orientations
(2.16)
38
2 Structural Properties of Heterostructures
D001 =
2C12 , C11
D110 =
C11 + 3C12 − 2C44 , C11 + C12 + 2C44
D111 =
2C11 + 4C12 − 4C44 . C11 + 2C12 + 4C44
(2.17)
The factors D represent the ratios −εi⊥ /εi for the respective orientations of the interface, i.e., the ratios of normal and lateral strains for a biaxial deformation. The assumption of a constant ratio in strained layers is based on the assumed validity of Hooke’s law (2.10). It should be noted that distortions along 110 or 111 reduce the crystal symmetry in a way that the atomic positions in the unit cell are not uniquely determined by strain. The shifts originate from changes in the bond strengths: Strain along [111] in zincblende or diamond structures, e.g., makes the [111] bond inequivalent to the ¯ [11 ¯ 1], ¯ and [11¯ 1] ¯ bonds, leading to a static displacement of the sublattices. other [1¯ 11], Introducing √ an internal strain parameter ξ [32], the [111] bond is elongated by (1 − ξ )ε44 a 3/4. ξ = 0 and 1 correspond to perfectly strained positions and rigid bond lengths, respectively [33]. Using the constants D also the vertical change of the unit cell in layer i can be calculated, (2.18) ai⊥ = ai 1 − Di (a /ai ) − 1 . It should be noted that a and a⊥ represent the actual lattice constants only for the (001) orientation of the interface plane. For other orientations these quantities express the change of the unit cell dimensions under strain. The lateral and vertical strains of layer i are related to the respective strained lattice parameters by a
− 1, ai ai⊥ = − 1, ai
εi =
(2.19a)
εi⊥
(2.19b)
where the quantity ai denotes the unstrained lattice constant of layer i. In a corresponding hexagonal structure with a basalplane interface, the lattice constants a and c of the considered layer are inserted into a and a⊥ of (2.19a), (2.19b), respectively. Using analogous insertions made to obtain (2.13), the relation reads for hexagonal structures 2C13 ε . (2.19c) ε⊥ = − C33
2.2 Elastic Properties of Heterostructures
39
Pseudomorphic Layer A thin epitaxial layer grown on a much thicker substrate is described by considering t1 /t2 → 0 in (2.15). We see that then a = a2 . The unstrained lattice constant aL of the layer (a1 in (2.15)) laterally adopts the lattice constant of the substrate aS (a2 in (2.15)) at epitaxial growth and can be varied using different substrates. The substrate remains virtually unstrained due to its large thickness, and the misfit (or, lattice mismatch) f between the two crystals is usually expressed by
f =
aS − aL . aL
(2.20a)
It must be noted that also other definitions for the lattice mismatch are used in literature, particularly the relations f alternative1 =
aL − aS aS
(2.20b)
f alternative2 =
aL − aS . aL
(2.20c)
and
Note the change in sign of the alternative relations with respect to (2.20a). If we compare (2.20a) with (2.19a), we notice that the misfit is equal to the lateral strain of the epitaxial layer: f = ε . This applies for coherent growth, i.e., growth with an elastic relaxation of the strain without formation of defects. Such a layer is called pseudomorphic. f may have either sign as illustrated in Fig. 2.12 by comparing a compressively and a tensely strained layer.
(a)
aL > a S
a
layer
substrate
aL < aS
(b)
a
aS
Fig. 2.12 Biaxially strained layers (yellow atoms) on substrates (blue atoms) with another lattice constant aS . In a the unstrained lattice constant of the layer aL is larger than aS , and the layer is compressively strained in lateral direction; in b the layer is tensely strained
40
2 Structural Properties of Heterostructures
2.2.6 Critical Layer Thickness A strained solid like the layers considered in Fig. 2.12 contains a strain energy per volume E/V . The differential work of deformation for a small increment of strain is given by 6 1 dE = σi dεi . (2.21) V i=1 Integration of (2.21) using (2.11) yields the elastic energy density of a strained solid, 1 E = Cik εi εk . V 2 i=1 k=1 6
6
(2.22)
For a cubic material (2.22) reads 1 E 2 = C11 εx2 x + ε2yy + εzz + 2C12 (ε yy εzz + εzz εx x + εx x ε yy ) V 2 2 2 + εx2y , + C44 ε yz + εzx
(2.23)
with the three respective terms of hydrostatic, uniaxial, and shear strains. We see that the homogeneous energy density increases quadratically with strain in the harmonic approximation of Hooke’s law. If a cubic, biaxially strained pseudomorphic layer is considered, which is allowed to elastically relax according to Poisson’s ratio, the elastic energy density is given by [34] 1+ν E , = 2Gε 2 AtL 1−ν
(2.24)
A, tL , G, ε , and ν being the area, the strained layer thickness, the shear modulus, the inplane strain parallel to the interface, and Poisson’s ratio of the layer, respectively. According to (2.24) the areal density of the elastic strain energy in the layer E/A increases linearly with the layer thickness tL and quadratically with ε , i.e., the misfit f for a pseudomorphic layer. Areal strain energy is hence accumulated as the layer thickness increases. At some critical thickness tc this energy is larger than the energy required to form structural defects which plastically relax the strain. Such defects are dislocations, the nature of which is studied in more detail in Sect. 2.3. The plastic relaxation reduces the overall strain, but at the same time the dislocation energy increases from zero to a value determined by the particular dislocation. Quite a few models were developed to calculate the critical thickness tc of a pseudomorphic epitaxial layer depending on the misfit f with respect to the substrate. They all consider some energy balance or, equivalently, a balance of forces or stresses, by comparing the amount of homogeneous strain energy relaxed by the introduction of a particular defect with the energy cost associated with the formation of this defect.
2.2 Elastic Properties of Heterostructures
41
Fig. 2.13 Scheme of a dislocation introduced into a layer, that plastically relaxes the strain. Layer and substrate are represented by yellow and blue atoms, respectively. The inserted extra plane is shown in cross section and represented by the dashed red line
Basic early work by Frank, Van der Merve, and coworkers described the plastic relaxation by an array of parallel, equally spaced misfit dislocations (Sect. 2.3.6) [35–37], or by a twodimensional grid of such dislocations at the interface [38– 41]. A more simple approach for predicting the critical thickness was developed by Matthews and Blakeslee [42, 43]. The model considers the force on a threading dislocation penetrating from the substrate through the epitaxial layer, which creates a dislocation at the interface and gives rise to a comparable scenario as considered by Van der Merve and coworkers. The general picture is outlined below, assuming a structural lattice defect that can relax the strain of the layer by a plastic deformation. Such a dislocation formed by, e.g., the insertion of an extra lattice plane in the layer is depicted in Fig. 2.13. The end of the additional halfplane near the interface of the heterostructure builds a dislocation line with a locally highly strained region. The formation of this dislocation requires a formation energy E D . This energy cost is balanced by the elastic relief of homogeneous strain energy in the layer lattice outside the core region of the dislocation line. Whether or not plastic relaxation occurs in the epitaxial layer depends on the minimum of the elastic energy E I at the interface. E I is given by the sum of homogeneous strain energy E H in the layer (denoted E in (2.24)) and dislocation energy E D . The dislocation energy E D depends on the particular geometry and the amount of plastic relaxation as expressed by the Burgers vector (Sect. 2.3). The remaining mismatch f of the (partially) relaxed layer refers to an average lattice constant of the layer. In the presence of dislocations f is less than the natural misfit, which is defined by the unstrained lattice constants in (2.20a)–(2.20c) and denoted f 0 in the following. To a good approximation f is given by the sum of f 0 and the lateral strain
42
2 Structural Properties of Heterostructures
E/A
100
50 15
ε
f0
Fig. 2.14 Areal energy densities occurring at a biaxially strained layer with a thickness of 15, 50 and 100 times the substrate lattice constant. ε denotes lateral strain, f 0 = −0.36 % is the assumed natural misfit. The black, gray, and light gray curves are homogeneous strain, strain at the interface, and dislocation energy, respectively. The arrow denotes an energy minimum of a thick layer attained by plastic strain relaxation
ε=
aL − aL,0 aL,0
which normally has opposite sign; aL,0 denotes the unstrained lattice parameter of the layer. The dependence of E I from ε is then given by E I /A = E H /A + E D /A, E H /A ∝ tL ε2 ,
(2.25)
E D /A ∝ ε + f 0 . The relation for the interface energy given by (2.25) is illustrated in Fig. 2.14 for a GaAs0.9 P0.1 layer on GaAs substrate with a natural misfit f 0 = −0.36% and a thickness below, just at, and above the critical value for plastic relaxation [40]. The homogeneous strainenergy density disappears at zero strain and increases quadratically with ε (black curves), while the dislocation energy density gets zero at f = ε + f 0 = 0 (light gray curves). In any case the energy density at the interface E I /A (gray curves) tends to attain a minimum. The criterion for the critical thickness tc is [44] (2.26) ∂(E I /A)/∂ ε = 0, evaluated at ε =  f 0 . For tL > tc the homogeneous strain of the layer gets larger than the natural misfit  f 0 , and dislocations introduce a strain of opposite sign, thereby reducing ε and hence E I /A. The critical thickness is usually inverse to the natural misfit in a wide range, cf. Fig. 2.15. For the evaluation of the critical thickness in a given heterostructure the geometry of the strainrelaxing dislocations must be specified. We consider the example of a semiconductor layer with diamond (or zincblende) structure and accommodating
2.2 Elastic Properties of Heterostructures 6
10
Critical thickness tc (aS)
Fig. 2.15 Critical thickness of a biaxially strained layer with diamond or zincblende structure in units of the substrate lattice constant as for the introduction of accommodating 60° dislocations. From [40]
43
diamond
5
10
60°, =0.25
4
10
3
10
2
10
1
10
6
10
5
10
4
10
3
10
2
10
1
10
1
Natural misfit f0
60° dislocations, which are most prominent in such solids and are treated in detail in Sect. 2.3. We assume a biaxially strained layer with a given Poisson ratio ν. Taking the dislocation energy E D from (2.36), the energy at the interface E I (2.25) reads E I /A = E H /A + E D /A ε + f 0 (1 − ν cos2 α) ρR 1+ν + bG ln . = 2Gtε2 1−ν 2π(1 − ν) sin α cos β b
(2.27)
The strain denotes the inplane components ε = εx x = ε yy = ε , and the geometry of the dislocation is expressed in terms of the absolute value b of its Burgers vector b, the angle α between the Burgers vector and the dislocation line vector, and the angle β between the glide plane of the dislocation and the interface. R is the cutoff radius defining the boundary of the strain field produced by the dislocation core, and the factor ρ accounts for the strain energy of the dislocation core and is on the order of unity. We now apply condition (2.26) to the interface energy (2.27) and put R = tc , because the first dislocations are expected to appear if the cutoff radius is equal to the critical layer thickness. This gives the relation [40] ρtc (1 − ν cos2 α) ln . tc = b 8π  f 0 (1 + ν) sin α cos β b
(2.28)
The critical thickness tc can be calculated numerically from this transcendent equation for a given natural misfit f 0 . If the geometrical parameters of the √ 60° dislocation are inserted for the considered geometry, b = a/2 × [101] = a/ 2, α = 60◦ , β = 54.7◦ , and assuming ρ = 4 for the dislocations and ν = 0.25 for layer, we obtain the dependence of tc shown in Fig. 2.15 [40]. The geometry of the 60° dislocation in zincblende crystals is depicted in Fig. 2.25b. Consideration of another geometry yields a different prefactor of ln in (2.28), producing a vertical shift of the curve in Fig. 2.15.
44
2 Structural Properties of Heterostructures
The dependence given in Fig. 2.15 follows approximately the relation tc ∼ 1/ f 0 . It should be noted that the actual degree of plastic relaxation does not solely depend on the misfit, but also on the growth procedure: Kinetic barriers for the generation and movements of misfit dislocations may lead to significantly larger values of the critical thickness than expected from equilibrium calculations. For metal layers, the experimentally determined values agree reasonably well with the predictions of equilibrium theory. For semiconductor layers, however, much larger values were observed. Equilibrium considerations are still useful to provide a reasonable measure for the lower limit of the critical layer thickness.
2.2.7 Approaches to Extend the Critical Thickness Epitaxy of heterostructures free of dislocations (at least within the diffusion length of charge carriers) is of particular importance for electronic and optoelectronic applications. Dislocations introduce local inhomogeneities, giving rise to a short lifetime and nonradiative recombination of charge carriers in semiconductors. Furthermore, piezoelectric effects associated with local strains change electronic properties. Dopants may precipitate at dislocations or strongly change diffusion characteristics. Fast degradation of devices often is connected to the action of dislocations. In device fabrication the reduction of the dislocation density in the active region below a level usually defined by the diffusion length of charge carriers is therefore an important issue. Typical values in semiconductor industry are in the range below 102 cm−2 for Si and 102 –103 cm−2 for III–V arsenides. Nitride semiconductors have much higher values in the range 104 –106 cm−2 for lasers and 107 –109 cm−2 for LEDs and electronic devices. A number of concepts is applied to extend the critical thickness beyond the limit given by the natural misfit. In many cases alloying of the layer materials by mixing crystals of different lattice constants is used to closely match the substrate lattice constant. The lattice constants of alloys are generally found to vary linearly with composition, a relation expressed by Vegard’s rule (Sect. 2.1.10). Since simultaneously the bandgap of the alloy varies, this may require mixing of more than two components with counteracting effects on bandgap and lattice constant (Sect. 4.1.5). Growth of such ternaries or quaternaries sometimes encounters thermodynamic limits, stimulating the search for alternatives. Buffer Layer A widely applied method to reduce the dislocation density of latticemismatched heterostructures is the introduction of a buffer between the epitaxial structure and the substrate [45]. Such layers or layer stacks confine misfit dislocations in a region
2.2 Elastic Properties of Heterostructures
45
below the active part and should in particular suppress the penetration of dislocation lines, i.e., the threading dislocations. A simple approach for a buffer is a uniform buffer layer (thick, µm range) with a high defect density near the interface to the substrate. The density of threading dislocations in a mismatched layer is usually found to decrease inverse to its thickness due to reactions of dislocations with opposite sign. Such buffer layers are referred to as metamorphic. They are to a large extend plastically relaxed and their lattice parameter approaches the unstrained value at the surface. Due to the thermal mismatch with respect to the substrate there will always remain some strain below growth temperature. A thick uniform buffer layer is also called virtual substrate. The approach of a uniform buffer grown at low temperature is widely applied in nitride growth on sapphire [46, 47]. This systems is strongly structurally and thermally mismatched, giving rise to peeling off and cracking of epitaxial GaN layers grown without buffer. The basic idea is the deposition of a nitride layer with poor crystallinity at a low temperature where adatom mobility is low, and a subsequent crystallization by an annealing step. The interface to the substrate then contains numerous defects making the buffer compliant to accommodate misfits, while the surface consists of well oriented crystallites which can coalesce during overgrowth. It should be noted that the epitaxial layer may have a different crystallographic orientation or a different crystal structure than the substrate. A prominent example is the prevalent growth of wurtzite (hexagonal) GaN on basal plane corundum (trigonal) αsapphire Al2 O3 . The [00.1] directions (or (00.1) planes, respectively) of GaN and ¯ direction Al2 O3 coincide, but the [10.0] direction of GaN is parallel to the [11.0] of the Al2 O3 substrate [48, 49]. This corresponds to a rotation of the epitaxial unit cell by 30° about the [00.1] caxis as compared to that of the substrate. General matching conditions for any pair of crystal lattices and any orientation may be found by considering interface translational symmetry [50]. The two lattices match if the two twodimensional lattices, formed by the crystal translations of the paired lattices parallel to the common interface, have a common superlattice. Such geometrical lattice match may induce epitaxial growth, but interface chemistry will always play a major role. A drawback of the uniform relaxed buffer layer is the large thickness required to obtain a threadingdislocation density suitable for devicegrade material of the epitaxial structure grown on top. In zincblende semiconductors a typical bufferlayer thickness on the order of some µm is required to achieve a high quality for device growth. In wurtzite layers grown along the common [0001] direction the reduction of dislocation density is less efficient, and thicker uniform buffers are needed [51]. Another approach is the graded buffer consisting of a continuously (or stepwise) change of the lattice constant by alloying with consecutively changing alloy parameters. Usually a linear grading of the composition—and consequently also of the lattice mismatch—is applied. Such a buffer is expected to have a uniform volume density of misfit dislocations throughout its thickness; this is in contrast to the high dislocation density of a uniform buffer (or layer) near the interface to the substrate, decreasing with increasing separation to the interface, see Fig. 2.16. The critical thickness tc of a
46 Fig. 2.16 Transmission electron micrograph of a 1.8 µm thick ZnTe layer grown on (001)oriented GaAs, imaged along the [110] direction. Inset: Diffraction pattern from the ZnTe/GaAs interface region. Reproduced with permission c 1993 Elsevier from [62],
2 Structural Properties of Heterostructures
(a)
(b)
ZnTe
GaAs
400 nm
graded buffer exceeds that of a uniform buffer, and above tc the density of threading dislocations at the surface is lower. An empirical model indicates that this density is proportional to the concentration gradient and also to the applied growth rate, if the gliding process of dislocations is not significantly impeded [52]. Growth conditions should hence favor the glide of threading dislocations to create the longest possible strainrelieving misfit segments, e.g., by a high growth temperature. For a review on various graded buffer layers see [53]. A more sophisticated approach is the socalled dislocation filtering using a strainedlayer superlattice. Multilayer structures with either alternating strain or alternating elastic stiffness were employed. Strains in the superlattice may cause bending of dislocation lines, leading to a meandering in alternating strain fields. Bending is also promoted when a dislocation line enters an elastically softer layer. The bending of dislocation lines increases the probability for defect reactions and favors annihilation. The thickness of the individual layers in the superlattice must be below the critical value for that particular layer, because the layers should induce a bending of dislocation lines without introducing new dislocations. Epitaxial Lateral Overgrowth A conceptual different approach is epitaxial lateral overgrowth (ELO or ELOG) [54, 55]. In the ELO process the substrate is first covered with an amorphous mask layer (e.g., SiO2 ) which contains windows. In subsequent epitaxy, growth is controlled to occur only in the windows. When the layer thickness exceeds that of the mask, the mask is laterally overgrown. Since defects from the interface between substrate and layer cannot penetrate through the mask, the overgrowth region has a very low defect density. ELO growth requires a growth anisotropy with the lateral growth rate well exceeding the vertical rate; furthermore, nucleation and growth on the mask must be prevented. ELO is an application of selective area growth and discussed in detail in Sect. 12.1.4.
2.2 Elastic Properties of Heterostructures
47
Compliant Substrate Concepts discussed so far use thick substrates which define the lateral lattice constant of the heterostructure in pseudomorphic growth. Considering (2.15), the critical layer thickness can be largely extended by using a thin and therefore compliant substrate [56–58]. The strain is then distributed between epilayer and substrate. For a sufficiently thin, freestanding substrate the epitaxial layer can virtually be arbitrarily thick. Compliant substrates were implemented using various approaches. The compliant substrate is generally composed of a thin compliant layer, which is mechanically decoupled from a thicker substrate required for handling. On a small area thin freestanding membranes with a support at the side were realized. Approaches for larger area use various methods for bonding the thin layer to the mechanically stable support, in particular oxide bonding, borsilicateglassbonding, and twistbonding. Reviews on this topic are given in [59, 60].
2.2.8 Partially Relaxed Layers and Thermal Mismatch The increase of elastic strain energy in a latticemismatched epitaxial layer up to a critical thickness tc was pointed out in Sect. 2.2.6. If the layer thickness exceeds tc misfit dislocations are formed in the layer and the strain is partially or, in sufficiently thick layers, fully relieved. We consider a cubic crystal. Usually strain relief of a biaxially strained and partially relaxed layer is symmetric and the two independent lateral lattice constants remain equal. The relief of strain may then be described by a strain parameter γ , a − aS , (2.29) γ =1− aL − aS aS and aL being the unstrained (natural) lattice constants of substrate and layer, respectively, and a the lattice constant of the layer in its strained state parallel to the interface. The fully strained pseudomorpic layer then corresponds to γ = 1 (a = aS ), and γ = 0 to the fully relaxed layer (a = aL ). Usually partial strain relief leads to a graded strain profile, i.e., γ is not constant throughout the layer. The density of threading dislocations is approximately invers to the layer thickness and is modeled for semiconductors with fcc (and related zincblende) structure in [61] and for wurtzite structure in [51]. An example is given in Fig. 2.16. The image shows a strongly mismatched zincblende ZnTe layer (aL = 6.123 Å at Tgrowth = 350 ◦ C) grown on GaAs substrate (aS = 5.665 Å at 350 °C, f = −7.5%) [62]. Dark lines indicate dislocation lines which form a dense network extending approximately 300 nm from the interface. Most of them are inclined by about 55° to the interface, equal to the angle of the intersection line of {111} planes with the (110) image plane. The angle indicates the occurrence of 60° dislocations (Sect. 2.3.5). The density of dislocations decreases as the ZnTe layer thickness grows, leading to regions with much lower
48
2 Structural Properties of Heterostructures
(a) (b)
Energy (eV)
Reflectivity
2.795
2.800
2.805
2.78
2.79
2.80
Energy (eV)
2.81
2.82
5
0
5
10
15
20 x10
4
Strain ε
Fig. 2.17 a Reflectivity spectra of free excitons in ZnSe/GaAs epitaxial layers which were grown at different temperatures. The lowest spectrum refers to a ZnSe bulk crystal. From [64]. b Energies of free lighthole (Xlh ) and heavyhole (Xhh ) excitons in differently prepared ZnSe samples on GaAs substrate (squares) and ZnSe layers released from the substrate (circles). The triangle at the crossing point marks the exciton energy measured with a bulk crystal. Reproduced with permission c 1992 Elsevier from [63],
defect density above 600 nm. The inset in Fig. 2.16 shows a diffraction pattern from the interface region, consisting of the superimposed response from the two zincblende crystals GaAs (outer points of each reflection due to a smaller lattice constant) and ZnTe. The pattern proves the epitaxial relation of layer and substrate. The decreasing defect density for increased layer thickness is accompanied by a progressive strain relief (γ → 0) and consequently by a gradual approach of the layer lattice constants a and a⊥ toward the unstrained value aL . It must be noted that the unstrained lattice constant varies as the temperature is changed (e.g., from growth temperature to room temperature, Sect. 2.1.7), and that different materials (e.g., substrate and layer) have different thermal expansion coefficients. An example of different builtin strains in ZnSe epilayers grown at different temperatures on GaAs is given in Fig. 2.17. The lattice mismatch (2.20a) at room temperature is f = −0.27%, inducing laterally a biaxial compressive strain in the layer. The studied ZnSe layers were thicker than the critical thickness tc (∼ =150 nm) considered in Sect. 2.2.6 and were thus partially relaxed. Since the thermal expansion coefficient of GaAs is substantially smaller than that of ZnSe (∼5.7 × 10−6 K−1 compared to ∼7 × 10−6 K−1 at RT, respectively), the ZnSe lattice contracts more pronounced when the heterostructure is cooled from growth temperature to the applied measurement temperature. The strain may be evaluated from the splitting of the valence band, reflected in the splitting of the free exciton (Sect. 4.1.2). The measurement of the freeexciton states in Fig. 2.17a shows that different strain states exist in samples
2.2 Elastic Properties of Heterostructures
49
which were prepared at different growth temperatures between 320 °C (molecular beam epitaxy) and 450 °C (hot wall epitaxy) [63, 64]. The exciton reflectionloops progressively split and shift to lower energy as the growth temperature is increased, indicating increasing tensile strain. The strain state was calculated from the difference of thermal expansion coefficients times the difference between growth and measurement temperature. The measurement of the nearsurface strain state Fig. 2.17b derived from reflectivity spectra recorded at 1.6 K reveals a large range of values including also negative strain, i.e., still compressive inplane strain of the ZnSe layer at 1.6 K. The crossing point agrees well with the energy of the unsplit free exciton of a ZnSe bulk crystal.
2.3 Dislocations A crystalline defect is any region where the microscopic arrangement of atoms differs from that of a perfect crystal. Defects are classified into point defects, line defects, and surface defects, depending on whether the imperfect region is bounded in three, two or one dimensions, respectively. There is a very large variety of defects in solids, and for many of such imperfections their presence is a general thermal equilibrium phenomenon. We will focus on only two important kinds of defects, namely dislocations and substitutional impurities. The latter are point defects, which particularly govern electronic and optical properties of semiconductors and are studied in Chap. 10. In the following some basic properties of dislocations are outlined. More details are found in, e.g., [65, 66]. Examples are particularly considered for the fcc and hcp structures and their related important zincblende and wurtzite structures.
2.3.1 Edge and Screw Dislocations Dislocations are line defects which are present in virtually any real crystal. Dislocation densities in actual crystals range typically from 102 cm−2 in good semiconductors to 109 cm−2 in metals or highly defective semiconductors. The vector along the dislocation line, i.e., along the core of the dislocation, is called line vector l. A dislocation is characterized by l and the Burgers vector b. b is the dislocationdisplacement vector and determined by a closed path around the dislocation core, the Burgers circuit. The procedure to find b is illustrated in Fig. 2.18. The Burgers vector completes the path around the dislocation line with respect to a similar path within a perfect reference crystal. According to the righthand screw convention, the Burgers circuit is formed clockwise around the dislocation line, when looking in the positive sense of the line vector (in Fig. 2.18 l points into the plane of projection; in many structures an arbitrariness in the sense of l cannot be avoided). If the path incloses more than one dislocation, the resulting Burgers vector is given by the sum of the Burgers vectors of all single dislocations.
50
2 Structural Properties of Heterostructures
(a)
(b)
b
b
l
l
Fig. 2.18 a Edge dislocation and b screw dislocation. b and l denote the Burgers vector and the dislocationline vector, respectively
There are two basic types of dislocations, edge dislocations and screw dislocations. In an edge dislocation b is perpendicular to l. Such a dislocation may be formed by the insertion of an extra halfplane spanned by l and b × l, see Fig. 2.18a. In a screw dislocation b is parallel to l. This kind of dislocation is built by a shift of one part of the solid by an amount b as shown in Fig. 2.18b. Most dislocations occurring in solids are of mixed character with an edge component and a screw component. They are generally denoted by specifying the angle between b and l. Pure edge dislocations obey b · l = 0, for pure screw dislocations b · l = b (for a righthanded screw, −b otherwise). The Burgers vector along a dislocation line is constant, if the dislocation line is a straight line; consequently the type of dislocation does not change in this case. However, the type of dislocation and hence also the angle between Burgers vector and line vector change if the dislocation line bends.
2.3.2 Motion of Dislocations Geometrical considerations show that a dislocation line can neither begin nor end within the crystalline solid [65]. A dislocation line therefore either forms a closed loop within the crystal, or it begins and ends at an interface or grain boundary of the crystal. If a force acts on the crystal, the dislocation line can move along specific slip planes through the crystal. This process requires the breaking of bonds and is hence thermally activated. Since the position of individual atoms changes only a fraction of the lattice constant during such movements, the required energy is quite small. The presence of dislocations thereby accounts for the fact that real solids withstand much smaller shear strengths against slipping of atomic planes than perfect crystals would do (factor ∼10−4 ). Two kinds of dislocation movements are distinguished: Glide and climb processes. They are illustrated in Fig. 2.19. During gliding the dislocation moves in the direction of the Burgers vector by turning crystal planes as illustrated in Fig. 2.19a. Such shear displacement is termed glide when it is produced by a single dislocation, and slip
2.3 Dislocations
(a)
51
shear
(b) norm
norm
shear
Fig. 2.19 Edge dislocation performing a a gliding process and b a climbing process. σ shear and σ norm indicate shear and normal stresses acting on the solid, the yellow line in (a) indicates the glide plane
when it is produced by a number of dislocations. The total number of atoms and lattice sites is conserved in such motions. For pure edge dislocations the process can only occur along slip planes which contain both the Burgers vector and the dislocation line. Pure screw dislocations can glide along any plane, since l and b are parallel. Climbing is a motion out of the glide plane; it occurs within a plane, which contains the dislocation line but is perpendicular to the Burgers vector. Climbing is accompanied by a material transport, i.e., emission or absorption of interstitials or vacancies (point defects) moving to or from the dislocation core, as indicated in Fig. 2.19b. The symbol to represent a general dislocation is ⊥. For an edge dislocation the upwards pointing arm of the inverted T points to the direction of the added or removed material. The total geometry of a dislocation is specified by the glide plane in addition to the Burgers vector and the line vector; this set is referred to as slip system. Slip planes in a crystal are usually planes with closest packing of atoms; they have largest separation. In zincblende semiconductors these are {111} planes, see Fig. 2.3. Dislocation lines in real crystals are not straight lines; they contain short segments, where the dislocation line is displaced on an atomic scale. A kink is formed when part of the dislocation is shifted within the same glide plane by one lattice plane from its original position (Fig. 2.20a, b). Such a kink does not impede glide of the dislocation. If the dislocation line moves from one atomic slip plane to another a jog is formed (Fig. 2.20c, d). Jogs are segments of the dislocation line that have a component normal to the glide plane. If this sement extends over more than one interplanar spacing it is termed superjog. The jog on a screw dislocation has an edge component; it can only glide in the plane containing the dislocation line before and
52
2 Structural Properties of Heterostructures
(c)
(a) b
b
(d)
(b) b
b
Fig. 2.20 Dislocation line with a kink (a, b) and a jog segment (c, d) on a scew (b, d) and an edge dislocation (a, c). The glide plane is marked in yellow
after the jog (paper plane in Fig. 2.20d). Both kinks and jogs can nucleate in pairs on an initially straight dislocations line. Such pairs (of opposite sign) are formed by thermal fluctuations in the crystal and can initiate movement of the dislocation line. If the last line of atoms along an edge dislocation is removed, e.g., by diffusion to the crystal surface, then the dislocation has climbed by one atomic spacing. A climb is a motion out of the glide plane. However, the diffusion of only a few atoms from the edge is more likely. This results in a climb of only a fraction of the dislocation, with a jog to the undisturbed part. Climb by nucleation of jog pairs is equivalent to dislocation motion in perpendicular direction by nucleation of kink pairs. Widening of the distance between jog pairs usually requires diffusion of the interspacing line of atoms to the surface.
2.3.3 Dislocation Network Section 2.2 outlined how a strained epitaxial layer of a pseudomorphic heterostructure may relax strain energy by introducing a misfit dislocation. The process of this plastic strain relaxation is now considered in more detail. To reduce the tensile or compressive strain in an overcritical epilayer with thickness t > tc , the introduction or omission of a lattice plane is favorable, respectively, creating a dislocation line at the layer/substrate interface. Since the dislocation line can neither begin nor end within a crystal, its ends must lie at the surface. There exist two possibilities which fulfill this condition [42]. One mechanism is based upon a dislocation line with a suitable
2.3 Dislocations
53
Fig. 2.21 Generation of a misfit dislocation network (c) at the interface between layer (upper part) and substrate (lower part, blue) from (a) a preexisting threading dislocation of the substrate and (b) from the nucleation of a dislocation half loop
Fig. 2.22 Plan view transmissionelectron microcraph of a 2 µm thick Si layer on (001)oriented GaP substrate. The parallel and closely spaced fringes denoted S originate from a stacking fault. Reproduced with permission from [67], c 1987 AIP
(b)
(a) 2
(c)
1
1 2
S
1 m
Burgers vector already existing in the substrate and terminating at its surface. As illustrated in Fig. 2.21a the dislocation is replicated in the layer and forms a threading dislocation, i.e. a dislocation penetrating the layer. Under the action of coherency strain the dislocation line bends and glides along the interface (from position 1 to 2). Thereby a strainrelaxing misfit segment of the dislocation line is created at the interface. Another mechanism is the nucleation of a dislocation half loop at the layer surface, illustrated in Fig. 2.21b. The half loop represents the border of an extra plane (in tensely strained layers), which expands and glides towards the interface over slip planes. Both mechanisms lead to the formation of a dislocation network at the interface (Fig. 2.21c). The average spacing p of the parallel line segments at the interface is given by (2.33). The formation of a dislocation network at the layer/substrate interface of incoherent (plastically relaxed) epilayers may be observed in plan view microcraphs due to the accompanying strain field at the dislocation core. An example for an epitaxial layer with 0.5% natural misfit at growth temperature is given in Fig. 2.22.
2 Structural Properties of Heterostructures
(a) [001]
D ] [10 1
1] [21
[010]
D
[12
[12
1]
[110]
B
]
1 [21
1]
[112] [10 1]
] [10 1
[112]
A
1] [21
C
0] [11
[100]
C
1] [121 ] [21 [110]
1] [01
D
B
0] [11
A
[112]
(b)
[112]
54
[12
[110]
1]
D
Fig. 2.23 Thompson’s reference tetrahedron a in the fcc unit cell and b in a planar development showing the different crystallographic directions
2.3.4 Dislocations in the fcc Structure The facecentered cubic and hexagonally closepacked structures are the two most common structures for metallic elements and—as constituents of the related zincblende and wurtzite structures—also for important semiconductors (Sect. 2.1). For these structures we consider simple reference schemes to denote Burgers vectors of possible dislocations and stacking faults. Figure 2.23 represents Thompson’s tetrahedron used for fcc structures [68]. The side faces of the tetrahedron are the four equivalent {111} faces, which lie parallel to the corresponding closepacked planes of the fcc structure and represent the possible glide planes. The edges point towards 110 directions and correspond to the six glide directions denoted AB, etc. They √ represent vectors of the type 21 a 110 with length a/ 2, which are primitive translations of the fcc structure. Dislocations with such a Burgers vector are termed perfect dislocations. Vectors from a corner to the midpoint of a side facet are of the type a 112 and are labeled Aβ, etc. Dislocations with a Burgers vector which does not 6 correspond to primitive translations (like Aβ) are referred to as partial dislocations. Partial dislocations lead to a change in the ABC stacking order of the {111} planes of the fcc structure. The resulting planar defects are referred to as stacking faults. Possible Burgers vectors of dislocations in the fcc structure and the notation of the corresponding dislocation type are given in Table 2.8. Notations with two pairs represent the sum vector, e.g., D B/C A ≡ DC + B A yields [100]. The energy of a dislocation is generally proportional to the square of the absolute value of its Burgers vector. A dislocation with Burgers vector b can, therefore, lower its strain energy and divide into two (or more) partial dislocations with Burgers vectors b1 and b2 , if Frank’s rule is satisfied: b1 2 + b2 2 < b2 .
(2.30)
The common validity of Frank’s rule originates from the weak dependence of the line energy of a dislocation on its character (edge or screw type or mixed). In any case
2.3 Dislocations
55
Table 2.8 Burgers vectors and types of dislocations in the fcc structure, a is the lattice constant of the unit cell Burgers vector Burgers vector Type of dislocation b2 (Thompson’s notation) (crystallographic notation) (×36/a 2 ) 1 2 a110 1 3 a111 1 6 a112 1 6 a110 1 3 a100 1 3 a110 1 6 a013 1 6 a123
AB Aα Aβ αβ δα/C B δ D/Cγ δγ /B D δ B/Dγ
Perfect Frank partial Shockley partial StairRod partial StairRod partial StairRod partial StairRod partial StairRod partial
18 12 6 2 4 8 10 14
E dislocation /length ∝ const × Gb2 , where G is the shear modulus and the constant differs by less than a factor of 2. Only dislocations with the shortest Burgers vectors are stable. Perfect dislocations with shortest Burgers vectors in the fcc structure are of the type 21 a011. Such a dislocation tends to dissociate into two (stable) partial dislocations with shorter Burgers vectors. From Thompson’s tetrahedron Fig. 2.23 we read, e.g., AD = Aβ + β D, or a ¯ ¯ a a ¯ ¯ ¯ [101] = [10 2] + [2¯ 1¯ 1]. 2 6 6 This dislocation reaction describes the dissociation of a perfect dislocation into two energetically favorable Shockley partial dislocations, cf. Table 2.8. The process is illustrated in Fig. 2.24. The dislocation line of the perfect dislocation AD splits into two lines of the partial dislocations. Since their Burgers vectors are not lattice vectors, they lead from a lattice site to a crystallographic not equivalent site: They produce a stacking fault. The two dislocation lines border a strip of stacking faults which keeps
(a)
l
b
b1
D
(b) l1
b2
AD A
l2
3.8 nm
Fig. 2.24 a Dissociation of a perfect dislocation into two Shockley partial dislocations. b Highresolution transmission electron micrograph of a stackingfault ribbon in Ge bounded by two Shockley partial dislocations, the double arrow indicates the stacking fault width expected from the c 1998 Elsevier stacking fault energy. Reproduced with permission from [69],
56
2 Structural Properties of Heterostructures
the partial dislocations together at some equilibrium distance and forms a socalled extended dislocation. In the stackingfaulted region the regular ABC ABC stacking order is changed by removal or insertion of one layer, e.g., to AB ABC. The three equivalent 110 directions and four equivalent {111} planes of a cubic semiconductor crystal yield 12 slip systems, collectively denoted a2 110 {111}. Dislocations on these slip systems comprise pure edge, pure screw, and mixed 60◦ dislocations.
2.3.5 Dislocations in Diamond and Zincblende Structures The diamond and zincblende structures result from the fcc structure by adding to each atom on the ABCstacked fcc lattice one atom of another type in the distance a [111], i.e., a corresponding abcstacking. This yields a total Aa BbCc stacking, 4 with different kind of atoms (charges) on the two sublattices in zincblende (Sect. 2.1). Dislocations in semiconductors which crystallize in diamond or zincblende structures are therefore also described using Thompson’s tetrahedron. Mismatched layers of such semiconductors generally show larger values of the critical thickness for plastic relaxation and slower relaxation of the elastic strain than metal films. This is due to a lower mobility of dislocations in semiconductors and a consequently reduced length of misfit segments along the interface. Furthermore, the larger perfection of semiconductor substrates necessitates the nucleation of new dislocations, instead of, as in metal films, glide of preexisting ones or heterogeneous nucleation at precipitates. The three main types of perfect dislocations in diamond and zincblende semiconductors with a2 110 Burgers vectors are edge dislocations, screw dislocations, and 60°mixed dislocations. The 60◦ mixed type is the most common perfect dislocation, because the edge type has a high core energy and the screw type cannot relax tetragonal mismatch which arises from (001)oriented heterostructure growth. The screw dislocation and 60°mixed dislocation in zincblende structure are illustrated in Fig. 2.25. The respective dislocations of the diamond structure are obtained when all atoms are considered to be equal. There are two different sets of dislocations due to the Aa BbCc doublelayer atomic arrangement. Dislocations of the shuffle set (or type I) have glide planes lying between layers of the same index, e.g., Aa. Gliding of shuffleset dislocations requires breaking of one bond per atom. Dissociation of perfect dislocations of such set into partials is not favorable, because it would produce a stacking fault of the type Aa BbCbCc Aa with a high energy of the CbC sequence. Furthermore, the partial dislocations cannot glide like a perfect dislocation. On the other hand, dislocations of the glide set (or type II) dissociate into partials which are glissile by, e.g., forming a stacking fault of the type Aa BbAa BbCc. Gliding of perfect glideset dislocations requires breaking of three bonds per atom; they are much more mobile than shuffleset dislocations, though. Dissociation and interactions of these dislocations are identical to those of the fcc structure. A glideset dislocation can transform to the shuffle set and vice versa by climb. Dislocations in the zincblende structure require a further distinction with respect to those in diamond structure, because the dislocation line
2.3 Dislocations
57
(b)
(a)
b
l
b l
[111]
[001]
[111] Fig. 2.25 Perfect dislocations in the zincblende structure: a Screw dislocation, b 60° dislocation. ¯ The [001] direction shown in (b) lies in the plane spanned by [111] and [1¯ 11]
C B
b
B
c b a
b
c C
a
A C
A
a
b B c C b B
a
B A
c b a
C
C B
Fig. 2.26 Dissociated perfect dislocation with a bounded stacking fault in zincblende structure ¯ viewed along [110]
¯ may either lie on a row of anions or cations. Dislocations with l parallel to the [110] direction are termed α type. Their core comprises cations in the shuffle set and anions in the glide set. Accordingly, β type dislocations have a dislocation line along the [110] direction with anions in the shuffle set and cations in the glide set. The dissociation of a perfect zincblende 60° dislocation with type II glide plane into an extended dislocation of a stacking fault bounded by two Shockley partial dislocations is shown in Fig. 2.26. This scheme corresponds to the stacking fault ribbon imaged in Fig. 2.24, if all atoms are considered to be of the same kind to obtain the diamond structure.
2.3.6 Dislocation Energy Near a dislocation atoms are displaced from their equilibrium positions which they occupy in a perfect crystal. A corresponding cost of elastic energy is required to
58
2 Structural Properties of Heterostructures
produce the dislocation and is referred to as dislocation energy E D . To obtain an estimate for E D we first consider the simple case of a screw dislocation in an isotropic continuum forming a coaxial cylinder as depicted in Fig. 2.27 [65]. The dislocation is produced by a shear displacement in the z direction across the x z glide plane and assumed to increase uniformly with the angle ϕ. Displacements of this dislocation are given by u x = u y = 0, and u z = b × ϕ/(2π ) = b/(2π ) × tan−1 (y/x). The only nonzero stresses of such displacement are σx z = −Gb/(2π ) × y/(x 2 + y 2 ), and σ yz with y in the enumerator being replaced by −x. G is the shear modulus and b the length of the Burgers vector. In polar coordinates the stress reads σϕz = Gb/(2πr ), and the strain resulting from Hooke’s law is εϕz = εzϕ = σϕz /(2G) = b/(4πr ). The strain field has a pure shear character and decays with 1/r from the dislocation line l. The elastic energy per length L follows 2 , yielding from the integration of the elastic energy density E/V = 2Gεϕz
isotropic
E screw L
= rc
R
2 2Gεϕz r dr dϕ =
Gb2 ln(R/rc ). 4π
(2.31)
The lower bound rc denotes the radius of the dislocation core. At a distance r from the center of the dislocation below a value rc the linear elastic theory cannot be applied. A somewhat arbitrary cutoff parameter ρ is often used to account for the nonlinear elastic energy and dangling bonds in the core, where rc = b/ρ with ρ ≈ 2, . . . , 4. Sometimes in literature instead of using ρ a constant is added to the logarithm term of (2.31), yielding (ln(R/b) + const) instead of ln(ρ R/b); const = 1(= ln(e)) is then isotropic usually applied. The divergence of E screw /L for an infinite upper bound R indicates that the dislocation does not have a specific characteristic energy, but depends on the size of the solid. An appropriate choice for R is the shortest distance of the dislocation line to the surface or, in case of a solid with many dislocations of both signs, roughly their mutual average distance.
Fig. 2.27 Screw dislocation along the axis of a cylinder
z r
ϕ b x
l
y
2.3 Dislocations
59
The strain field of an edge dislocation comprises all kind of strains. Considering the edge dislocation Fig. 2.18a with an inserted lattice plane above the line vector l, the strain field has dominant compressive and tensile hydrostatic components above and below l, respectively. At the right and left hand side of l we find predominantly shear strains of opposite sign, and on the diagonals compressive and tensile axial components. In isotropic media the tensile stress in radial direction σrr and that along the circumference σr ϕ should be proportional 1/r and change sign by exchanging x and y. A continuummechanical deduction of the stress field of the edge dislocation yields σrr = σϕϕ = −Gb/(2π(1 − ν)) × sin ϕ/r , and σr ϕ = Gb/(2π(1 − ν)) × cos ϕ/r isotropic for the shear stress [65]. Integration leads to the elastic energy per length E edge /L, which, apart from an additional factor 1/(1 − ν), has the same form as that of the screw dislocation (2.31). The considerations likewise apply for anisotropic media, where the particular geometry examined introduces additional terms. In a dislocation with mixed character the strain fields of the screw and edge components superimpose. We consider the example of the prominent 60° dislocation in crystals with diamond or zincblende structure, introduced at a (001) interface between a substrate and a layer to accommodate misfit strain. The angle α between line vector and Burgers vector enters the elastic energy per unit length, yielding [40] Gb2 ρR sin2 α Eα = cos2 α + ln . L 4π (1 − ν) b
(2.32)
To evaluate the strain energy E D of all dislocations in a layer, their total number has to be considered. Figures 2.21 and 2.22 illustrate that the strain in a layer which exceeds the critical thickness is actually accommodated by a network of dislocations, which in many cases form a more or less regular grid at the interface. The average spacing p in such an array of parallel misfit dislocations is related to the actual misfit f . We consider the strongly mismatched, relaxed heterostructure depicted in Fig. 2.28 to obtain an expression for p. In Fig. 2.28 the lateral distance p comprises n planes of the substrate and (n + 1) planes of the layer (here aL < aS ). The lateral spacing between the depicted planes of the substrate is then given by aS = p/n, and that of the layer planes is aL = p/(n + 1). Taking the definition of the misfit f from (2.20a) we obtain for aL < aS f =
aS − aL = aL
p n
p n+1 p n+1
−
=
1 . n
If aL > aS there are only n − 1 layer planes for n substrate planes, yielding aL = p/(n − 1). Insertion into (2.20a) then leads to f = −1/n ( f < 0). The spacing p of the parallel misfit dislocations is hence p = naS =
aS . f
(2.33)
The inverse of p is the (linear) density of the dislocations illustrated in Fig. 2.28.
60
2 Structural Properties of Heterostructures
1
2
... n+1 layer interface substrate
1 p
2 ... n
Fig. 2.28 Equally spaced dislocations accommodating the strain in the layer of a mismatched, relaxed heterostructure. The lines represent lattice planes which lie perpendicular to the image plane and contain the dislocation line. Lattice planes in substrate and layer are drawn black and gray, respectively
[111]
AlN
Si
(a)
(b)
2 nm
2 nm
[110] Fig. 2.29 Equally spaced step dislocations at the interface between an AlN(0001) epilayer and the Si(111) substrate. a Highresolution transmissionelectron micrograph taken along the [11 −2] axis of Si. b The fastFourier filtered image shows the Si(−110) and the AlN(−2110) net planes, c 1999 Elsevier respectively. Reproduced with permission from [70],
A dense regular spacing of dislocations may occur, if a large lattice mismatch f between epilayer (lattice spacing dL ) and substrate (dS ) is accommodated by a coincidence lattice fulfilling the condition m × dS ≈ n × dL with small integer numbers m and n. The remaining mismatch is in this case f = (m × dS − n × dL )/n × dL . An example is given in Fig. 2.29. The lateral lattice constant of the AlN epilayer (dL = 3.11 √ Å) is much smaller than that of the (111)oriented Si substrate (dS = 5.43 Å/ 2 = 3.84 Å), yielding a natural misfit (dS − dL )/dL = 0.23. By introducing one edge dislocation into each unit cell of the coincidence lattice on the epilayer side with a ratio m : n = 4 : 5 the mismatch is reduced to f = −0.01 [70]. The edge dislocation was more recently considered being composed of the ¯ edge component each and edge components of two 60◦ dislocations with 21 1010 opposite screw components [71]; there are three such equivalent 60◦ dislocations
2.3 Dislocations
61
¯ lying in the (0001) basal plane. These dislowith Burgers vectors of type 13 1120 cations create a regular triangular network of misfit dislocations at the AlN/Si(111) interface. Coincidence relations play a prominent role in organic epitaxy discussed in Sect. 3.2.1. The elastic dislocation energy E D per area A of a network of dislocations at the interface is 2 E disloc ED = . (2.34) A p L The factor 2 accounts for the two independent lateral directions assumed here to be equivalent, and E disloc /L is the energy per length of one dislocation, like, e.g., (2.32). If the degree of relaxation is anisotropic, as was observed for, e.g., 60° dislocations ¯ directions, (2.34) splits into a in zincblende type layers along the [110] and [110] sum with two periods pi and two related E disloc,i /L i . An explicit relation of (2.34) also comprises the angle β between the glide plane containing the Burgers vector and the interface. β is related to the angle α between line vector l and Burgers vector b, and also to the substrate plane spacing aS according to aS = b sin α cos β.
(2.35)
Using (2.32), (2.33), and (2.35) yields a general relation for the dislocation energy of a layer containing a dislocation network [40], ε + f 0 (1 − ν cos2 α) ρR ED = bG ln . A 2π(1 − ν) sin α cos β b
(2.36)
The geometrical parameters for the 60° dislocation are the length of the Burgers vector b = a/2 × [101], the angle between Burgers vector and line vector α = 60◦ , and the angle between the {111} glide planes and the considered (001) interface plane β = 54.7◦ . The critical thickness of a strained epitaxial layer accommodated by such misfits is given by the implicit relation (2.28), the solution of which is depicted in Fig. 2.15.
2.3.7 Dislocations in the hcp and Wurtzite Structures In the hcp structure the triangular bipyramid given in Fig. 2.30 is a widely used reference construction for classifying dislocations [77]. In this representation basal¯ 10]), ¯ BC = a2 , and C A = a3 . The plane lattice vectors are labeled AB = a1 (= 13 [12 lattice vector c (= [0001]) is given by T S, the line σ S = T σ = 21 c does not represent ¯ 13], ¯ and a lattice vector. Further vectors of interest are T S + AB = c + a1 = 13 [12 ¯ Aσ = 1 [0110]. 3
62
2 Structural Properties of Heterostructures
Fig. 2.30 Triangular bipyramid used as reference system to describe dislocations in the hcp structure
S C A
B T
In crystals with hcp structure the closepacked basal planes are the most frequently observed glide planes. Dislocations with a slip vector of the type AB operating on these (0001) planes are therefore of particular importance. For vectors lying in the basal plane it is sufficient to use the base of the bipyramid as a reference system. As an example we consider the dissociation of a perfect glide dislocation with vector AB into Shockley partial dislocations. From the reference bipyramid we read AB = Aσ + σ B.
(2.37)
The partial dislocation Aσ changes the layer sequence from the ordinary abab stacking to a bcbc sequence as illustrated in Fig. 2.31. The second partial σ B in (2.37) restores the initial order. Thereby a stackingfault ribbon bound by two partials is created, comparable to the case shown in Figs. 2.24 and 2.26. Another kind of such a ribbon is formed from the same perfect glide dislocation if the order of the partial dislocations is reversed, i.e. AB = σ B + Aσ. (2.38) In this case the ribbon contains layers stacked in an acac sequence, cf. Fig. 2.31b. Both kinds of ribbons have the same energy, although they are crystallographically distinguishable. The wurtzite structure is formed from the hcp structure by adding to each atom a further atom of another kind, shifted by 38 c along [0001], cf. Sect. 2.1. Dislocations in the resulting Aa Bb Aa Bb stacking are described in the same framework as those of the hcp structure. The basic edge and screw dislocations in a wurtzite crystal are shown in Fig. 2.32. Panel (a) shows a highresolution transmissionelectron micro¯ determined from graph of a pure edge dislocation with a Burgers vector of 13 [1120], the Burgers cycle marked by open circles. The inserted plane is perceived by viewing the image at a glancing angle from the lower left corner. This type of threading
2.3 Dislocations
63
(a)
(b)
a
b
A
c AB
b
a
AB c
a b a b a b a
A
a b a b a b a
b c b c a b a
c a c b a b a
a b a b a b a
A
a b a b a b a
Fig. 2.31 Dissociation of a perfect dislocation AB in a hcp structure into two partial dislocations Aσ and σ B. a Displacement of an atom in the b layer (red) on top of the a layer (blue circles) by Aσ . b Displacement of an atom in the a layer on top of the b layer by σ B. The stacking sequence of the ribbons bounded by the two partial dislocations is illustrated in the bottom
(a)
F
(b)
S
10 nm
Fig. 2.32 a Plan view transmissionelectron micrograph of a pure edge dislocation in wurtzite GaN. S and F mark begin and end of a Burgers cycle which is indicated by open circles. Reprinted c 2000 APS. b Scanning tunneling micrograph of a screw dislocation with permission from [78], c 1998 AVS on the Nface of GaN. Reprinted with permission from [79],
64
2 Structural Properties of Heterostructures
dislocation is most common in GaN layers epitaxially grown on (0001) sapphire or on (111) Si. Screw dislocations can provide a steady source of kinks on a growing crystal surface by producing kink sites and may thereby lead to high growth rates. Figure 2.32b shows an STM image of a pure screw dislocation at a GaN surface (Nface). The measured step heights at the two spiral growth fronts are each one GaN bilayer, yielding a Burgers vector of c[0001] for this dislocation.
2.3.8 Antiphase Domains An antiphase domain, also referred to as inversion domain, is a region in a polar crystal where the atoms are located on regular lattice sites but in the opposite order with respect to the undisturbed crystal. In the domains of zincblende or wurtzite crystals anions occupy cation sites and vice versa. Such a disorder nucleates particularly at the heterointerface of a polar semiconductor grown on a nonpolar semiconductor. Here the antiphase domain is created during growth at monoatomic steps on the nonpolar semiconductor [72]: if growth starts with an anion layer, initial growth on a one monolayer higher region yields an inequivalent crystal orientation as illustrated in Fig. 2.33. Boundaries between domains of reversed orientation correspond to stacking faults and are also termed inversiondomain boundaries (IDBs). At these boundaries bonds among equally charged ions occur, see the bonds across the IDBs marked in green in Fig. 2.33. Inversiondomain boundaries (IDBs) generally create states in the bandgap. They introduce nonradiative carrier recombination and degrade the performance of electronic and optoelectronic devices. The epitaxy of III–V semiconductors on Si is exceedingly interesting, since the integration of a directbandgap III–V device on the indirectbandgap Si combines Si electronics with efficient photonics applications. Growth issues of this demanding interface are reviewed in [73, 74]. In the epitaxy of a zincblende semiconductor on groupIV semiconductor (e.g., InP on (001)oriented Si) the IDBs are inclined to the interface; a second monoatomic step may then induce a second IDB and lead to an annihilation of the inversion domain as illustrated in Fig. 2.33 for IDBs on {111} planes; such an annihilation may also occur with IBDs on {110} planes. IBDs have, however, usually irregular shapes and lie only partly on lowindex planes, making the annihilation process less efficient. The creation of an antiphase domain can be avoided by double steps on the nonpolar semiconductor [72]; this is illustrated at the right in Fig. 2.33, where no disorder in the layer results from the double step of the substrate. On Si(001) substrate such double steps can be formed by applying a ∼6◦ offcut orientation toward a {110} direction for creating singlestep terraces and a subsequent thermal treatment for doublestep formation [75]. Antiphase domains occurring in epitaxial GaN or AlN on Al2 O3 (0001) do not have such a favorable inclination of their boundaries. They have a hexagonal shape
2.3 Dislocations
65
[001] [110] Fig. 2.33 Antiphase domain (shaded region) created at a monoatomic step at the interface of a nonpolar to a polar zincblende semiconductor. The green dashed lines mark inversiondomain boundaries. No such boundary forms at a double step depicted right. The crystal orientations in the nonshaded and shaded regions are invers
¯ side walls being parallel to the (0001) growth direction; they hence with {1010} persist in the entire epitaxial layer [76].
2.3.9 Mosaic Crystal Faults like the line defects considered in the last few pages exist in virtually any crystal. A periodic pattern of dislocations may form an interface between undistorted regions called lowangle grain boundary as depicted in Fig. 2.34. Such a boundary leads to local tilts or twists of crystal planes and separate regions with perfect crystal structure. The tilt angle Θ of a tilt boundary formed from a linear sequence of edge dislocations as shown in Fig. 2.34 is given by their average distance d and the absolute value of their Burgers vector b. From the figure follows tan(Θ/2) = b/(2d) or, since Θ is small, Θ = b/d. There exist also twist boundaries formed from a sequence of screw dislocations. Lowangle grain boundaries are normally composed of a mixture of tilt and twist boundaries. In practice crystals usually consist of a mosaic of small blocks with undistorted structure. The singlecrystalline blocks are typically on the order of a few microns in vertical and lateral dimensions (with respect to the growth plane), and they are randomly slightly misoriented with respect to each other. The finite size of the crystallites limits the coherence of scattered Xray radiation. The dimensions are therefore called vertical and lateral coherence length, respectively. Outofplane rotation perpendicular to the surface leads to a mosaic tilt. Inplane rotation around the surface normal is referred to as mosaic twist. The characteristic parameters of mosaicity are
66
2 Structural Properties of Heterostructures
b
Θ
d Fig. 2.34 Scheme of a lowangle grain tilt boundary inducing a mutual tilt of adjacent crystalline regions by an angle Θ coherence length vertical lateral
tilt
twist
Fig. 2.35 Characteristic parameters of mosaicity in single crystals
illustrated in Fig. 2.35. It should be noted that the distortions are small and the crystal is still considered a single crystal, albeit with some mosaicity. In epitaxial layers with line defects mainly running parallel to the surface normal, the vertical coherence length is commonly related to the layer thickness. The mosaicity observed for ZnSe/GaAs(001) layers is discussed in Sect. 2.4.6. A model of dislocations accounting for the twist found in highly mismatched epilayers such as AlN/Si(111) is reported in [71].
2.4 Structural Characterization Using XRay Diffraction Fig. 2.36 Xray diffraction of two rays at neighboring lattice planes. For constructive interference the path difference of the diffracted waves 2dhkl sin Θ must be equal an integral number of wavelengths
67
θ
θ d hkl
θ
d hkl sin(θ)
2.4 Structural Characterization Using XRay Diffraction Xray diffraction is a powerful tool for investigating the structural properties of epitaxial layers and is employed in virtually any growth laboratory. Interatomic distances in a solid are typically on the order of some angstrom. A diffraction probe of the microscopic structure must hence have a wavelength at least this short. For an electromagnetic wave 1 Å corresponds to a photon energy E = hc/λ = 12.40 keV, a characteristical Xray energy. High resolution Xray diffraction (HRXRD) is the most commonly applied technique for analyzing lattice parameters, strains, and defects in epitaxial heterostructures. The technique is outlined in this section.
2.4.1 Bragg’s Law The periodic arrangement of atoms in the solid leads to an elastic scattering of impinging Xray waves. Diffracted waves have definite phase relations among each other. They interfere constructively, if the phase difference is an integral number n of wavelengths λ. This is depicted in Fig. 2.36 for two rays which are diffracted at two parallel lattice planes spaced a distance dhkl apart. According to this picture the waves behave as being reflected at the lattice planes. The path of the lower ray is 2 × dhkl × sin Θ longer, Θ being the angle of incidence (measured from the diffracting lattice plane). The condition for Xray reflections was concluded by William L. Bragg and his father William H. Bragg in 1913 from characteristic patterns of Xrays reflected from crystalline solids and reads 2dhkl sin Θ = nλ.
(2.39)
n is called the order of the reflection. Note that Bragg’s law (2.39) only defines the direction of a diffracted beam (not the intensity), and that it allows reflections only for λ ≤ 2dhkl . The latticeplane distance dhkl and hence Θ depend on shape and size
68
2 Structural Properties of Heterostructures
Table 2.9 Bragg’s equations for the seven crystal systems Crystal system Cubic Tetragonal Rhombohedral Hexagonal Orthorhombic Monoclinic Triclinic
Angles sin(Θ) of Bragg reflections √ λ 2 2 2 2a h + k + l λ sin(θ ) = 2a h 2 + k 2 + ( ac )2 l 2 (h 2 +k 2 +l 2 ) sin2 α+2(kl+lh+hk)(cos2 α−cos α) λ sin(θ ) = 2a 1−3 cos2 α+2 cos3 α λ 4 2 2 + hk) + ( a )2 l 2 sin(θ ) = 2a (h + k c 3 λ sin(θ ) = 2a h 2 + ( ab )2 k 2 + ( ac )2 l 2 2hl cos β h2 k2 l2 sin(θ ) = λ2 a 2 sin 2 β + b2 + c2 sin2 β − ac sin2 β sin(θ ) = λ2 h 2 a ∗2 + k 2 b∗2 + l 2 c∗2 + 2klb∗ c∗ cos α ∗ + 2lhc∗ a ∗ cos β ∗ + 2hka ∗ b∗ cos γ ∗ ,
sin(θ ) =
cos β cos γ −cos α 1 ∗ D bc sin α, cos α = sin β sin γ c∗ , cos β ∗ , cos γ ∗ correspondingly with
a∗ = b∗ ,
cyclic change of a, b, c, α, β, γ , and D = abc 1 + 2 cos α cos β cos γ − cos2 α − cos2 β − cos2 γ
of the unit cell and on the position of the planes with respect to the axes of the crystal system. They can be calculated for the seven crystal systems listed in Table 2.1 from the lattice vectors a, b, c, the angles α, β, and γ included by them, and the Miller or MillerBravais indices of the lattice planes h, k, l. The result is given in Table 2.9 in terms of Bragg angles sin(Θ) of allowed scattering directions.
2.4.2 The Structure Factor The intensity of the diffracted beam depends on the spatial arrangement of the atoms in the unit cell and their scattering power. The intensity of the wave scattered by all N atoms of the unit cell results from the sum of their individual contributions and their respective phases. This is expressed by the structure factor Fhkl ,
Fhkl =
N
f n exp i2π(hu n + kvn + lwn ) .
(2.40)
n=1
The atomic scattering factor f n expresses the scattering power of the nth atom in the unit cell and is determined by its inner electronic charge distribution. The exponential factor gives the phase relation of the N contributions and depends on the positions of the atoms in the unit cell, expressed by the coordinates u n , vn , and wn . The absolute value of the structure factor Fhkl  yields the amplitude of the diffracted wave, i.e., the amplitude of the wave scattered by all atoms of the unit cell with respect to the amplitude of a wave scattered by a free electron. The intensity Ihkl of the scattered wave is eventually given by its square,
2.4 Structural Characterization Using XRay Diffraction
69
∗ Ihkl ∝ Fhkl 2 = Fhkl Fhkl .
(2.41)
We consider for example the structure factor of a solid with body centered cubic (bcc) structure. The unit cell contains 2 atoms located at 000 and 21 21 21 (in units of the lattice constant a), which are identical ( f 1 = f 2 = f ). From (2.40) we obtain F = f exp i2π(0h + 0k + 0l) + f exp i2π 21 h + 21 k + 21 l = f 1 + exp iπ(h + k + l) , i.e., F = 2 f when h + k + l is even, and F = 0 when h + k + l is odd. For fcc structure we similarly obtain F = 4 f when h, k, l are all even or all odd, and F = 0 when h, k, l are mixed even or odd. In zincblende structure we have two kinds of atoms with atomic form factors f 1 and f 2 (> f 1 ). In this case we find for the structure factor (with n being an integer): h, k, l h, k, l h, k, l h, k, l
all even and h + k + l = 4n, all even and h + k + l = 4n + 2, all odd, are mixed even and odd,
F F F F
= 4( f 1 + f 2 ), = 4( f 1 − f 2 ), 1/2 = 4 f 12 − f 22 , = 0.
Note that all these structures belong to the cubic crystal system. In the hexagonal wurtzite structure the structure factor has the following form: 1/2 , l = 2n and h + 2k = (3m or 3m ± 1), F = 2 f 12 + 2 f 1 f 2 cos(2π ul) + f 22 l = 2n + 1 and h + 2k = 3m, F = 0, √ 1/2 l = 2n + 1 and h + 2k = 3m ± 1, F = 3 f 12 + 2 f 1 f 2 cos(2π ul) + f 22 . n and m are integers and u (≈ 38 c) is the mutual displacement of the anion and cation sublattices. A number of further factors determines the intensity of the scattered wave in addition to the structure factor F which solely considers the geometric structure of the scattering unit cells. They account for the polarization of the scattered wave (polarization factor P ∝ (1 + cos2 2Θ)), deviations from a perfect parallel and monochromatic incident radiation (Lorentz factor L ∝ λ2 / sin2 Θ), the effect of temperature (temperature factor or DebyeWaller factor f T ∝ exp(sin2 Θ/λ)), and absorption corrections depending on the measurement geometry (reflection or transmission setup). They are not included in this brief introduction.
70
2 Structural Properties of Heterostructures
Fig. 2.37 Path difference a + b of Xrays scattered from two atoms separated by r
k0
k
k0 r a
θ0
k
θ b
2.4.3 The Reciprocal Lattice For a detailed description of the scattering geometry the approach formulated by Max von Laue in 1911 is more appropriate than the simplified picture presented in Fig. 2.36. In this framework we regard the crystal as being composed of atoms which reradiate the incident radiation in all directions. Sharp reflections are obtained only in directions for which the rays from all lattice sites interfere constructively. We first consider scattering of only two atoms separated by a vector r, see Fig. 2.37. The incident Xray beam along the direction s0 with wavelength λ has the wave vector k0 = (2π/λ)s0 , s0 being the unit vector k0 /k0 . Constructive interference is obtained along a scattered direction s = k/k, if the path difference of the rays scattered by the two atoms is an integral number of wavelengths. From Fig. 2.37 we read that the path difference is composed by a sum of a = r cos Θ0 = −s0 r and b = r cos Θ = sr, yielding (2.42) (s − s0 )r = nλ. λ = λ0 because the scattering is assumed to be elastic. Multiplying (2.42) by 2π/λ we obtain (2.43) (k − k0 )r = n2π. We now consider many scattering atoms placed at the sites of a Bravais lattice. All lattice sites are displaced from one another by a Bravais lattice vector R. Constructive interference of all scattered rays occurs if condition (2.43) holds simultaneously for all values of r, i.e. (2.44) (k − k0 )R = n2π. Equation (2.44) may be rewritten by introducing the reciprocal lattice. A unique reciprocal lattice can be constructed for each particular Bravais lattice. It is a Bravais lattice for itself, and its reciprocal lattice is the original direct lattice. The base vectors gi of the reciprocal lattice are defined by the condition
2.4 Structural Characterization Using XRay Diffraction
71
gi a j = 2π δi j ,
(2.45)
ai being the base vectors of the corresponding Bravais lattice and Kronnecker’s symbol δi j = 1 for i = j and 0 otherwise. The vector g1 is thus normal to a2 and a3 , and can be calculated from g1 =
a2 × a3 . a1 (a2 × a3 )
(2.46)
The vectors g2 and g3 are obtained from (2.46) by a cyclic permutation of the indices. From the construction of the reciprocal lattice we conclude that each vector Ghkl is normal to a lattice plane of the real lattice with Miller indices (hkl). Furthermore, the distance dhkl of two neighboring parallel lattice planes with Miller indices (hkl) is inverse to the absolute value of the corresponding reciprocal lattice vector Ghkl , dhkl =
2π . Ghkl 
(2.47)
Using the reciprocal lattice vectors defined in (2.45) and a reciprocal lattice vector G built from the base vectors gi we represent (2.44) by the von Laue condition (k − k0 ) = G.
(2.48)
Equation (2.48) means that constructive interference of scattered Xrays occurs if the change in wave vector (referred to as diffraction vector) k = k − k0 is a vector of the reciprocal lattice. Conditions (2.48) and (2.39) are equivalent criteria for constructive interference of Xrays. We may derive Bragg’s law (2.39) from (2.48) by noting that G is an integral multiple of the shortest parallel reciprocal lattice vector, the length of which is 2π/dhkl , i.e., G = n2π/dhkl . G is also related to the Bragg angle Θ. From (2.48) and the triangle built by the vectors k0 , k, and k in Fig. 2.38 we find the relation G = k = 2 × k sin Θ. Putting this together we find k sin θ =
nπ . dhkl
(2.49)
By expressing k in terms of 2π/λ we obtain Bragg’s law from (2.49). We use here the convention, which is common in solid state physics. It should be noted that in crystallography the length of the wave vector is usually defined by k = 1/λ, i.e., without the factor 2π ; the reciprocal lattice spacing is then inverse to the associated latticeplane spacing in real space. The reciprocal lattice defined by (2.45) and (2.46) helps to find allowed Bragg reflections for a given crystal and the corresponding Bravais lattice. Such reflections fulfill the Bragg and von Laue conditions for a set of parameters consisting of latticeplane distance dhkl , angle Θ, and Xray wavelength λ. Methods of Xray
72
2 Structural Properties of Heterostructures [001]
Ewald sphere
006 005 404
204
k
θ θ
004 104 204
404
k
0
k0 [100]
000
sample
[100]
Fig. 2.38 Reciprocal space map of all Bragg reflections accessible for an incident Xray radiation with wave vector of length k0 . The horizontal axis denotes a diffraction vector k along a [100] direction lying in the sample surface, the vertical axis signifies a k normal to the surface. The outer sphere with radius 2k0 refers to a deflection angle 2Θ = 180◦
characterization differ in the parameters varied. They may be well represented using a simple geometric construction introduced by Paul P. Ewald.
2.4.4 The Ewald Construction To represent Xray diffraction using the Ewald construction we first draw the reciprocal lattice, i.e., a collection of points derived from the real (direct) lattice of the crystal structure to be studied using (2.46). Now the incident wave vector k0 is added with the tip pointing to the origin hkl = 000, see Fig. 2.38. An Ewald sphere of radius k0 (= 2π/λ) centered on the origin of k0 is drawn. Scattered wave vectors k (with same length as k0 ) also starting at the center of the sphere satisfy the von Laue condition if and only if their tips end on a reciprocal lattice point, i.e., the lattice points lie on the surface of the sphere. In this case the diffraction vectors k are vectors Ghkl of the reciprocal lattice. Note that each vector Ghkl represents a set of parallel lattice planes of the real crystal with Miller indices hkl. The reciprocal space map shown in Fig. 2.38 is a representation of the real lattice in the reciprocal space. It is fixed with respect to the studied sample and its diffracting Bragg planes. Ewald’s construction therefore provides a good survey of possible reflections for varied angles or wavelengths. For fixed λ and consequently fixed lengths of k0 and k all possible reciprocal lattice points lie within a sphere of radius 2k (corresponding to Bragg scattering with 2Θ = 180◦ ). Some points in the lower part of the map cannot be accessed since either Θ0 < 0 or Θ < 0, i.e., k0 cannot
2.4 Structural Characterization Using XRay Diffraction Fig. 2.39 Ewald’s construction of the von Laue method. The crystal is irradiated with a polychromatic Xray beam
73
k max
k min k 0max
000
k 0min
enter the sample (the incident beam is below the surface) or k cannot emerge from the sample (the diffracted beam is below the surface). If all angles are kept fixed and λ is varied over all possible values we directly obtain an image of the reciprocal lattice. This technique was applied by von Laue and coworkers in 1912 to prove the wave nature of Xrays and is mainly used today to determine the crystallographic orientation of samples with a known structure. Ewald’s construction of the Laue method provides spheres for all wavelengths between λmin (corresponding to kmax ) and λmax . They all have a common touch point at the origin because the crystal is kept stationary and the direction of incidence is hence fixed during data collection, see Fig. 2.39. Variation of λ is performed by using white radiation, i.e., continuum Bremsstrahlung radiation of an Xray tube or not monochromatized synchrotron radiation. The fraction of the reciprocal lattice filled by the shaded area then diffracts simultaneously.
2.4.5 HighResolution Scans in the Reciprocal Space Xray diffractometers are widely employed for nondestructive structural analyses of crystalline samples. Epitaxial structures are usually characterized applying highresolution Xray diffraction (HRXRD). The large natural line width of the generally used Kα1 radiation (λ/λ = 3 × 10−4 for Cu) limits the resolution of a simple singlecrystal diffractometer to Θ/Θ ∼ = 10−2 . Furthermore, the close vicinity to the Kα2 line (1.5443 Å for Cu, with half the intensity of Kα1 at 1.5405 Å) complicates the analysis particularly for multilayer structures. In a modern HRXRD setup the incident Xray radiation is therefore monochromized using Bragg reflections of a primary crystal (commonly a highly perfect Ge or Si crystal with a channel cut for multiple reflections). Such a monochromator improves the resolution to typically 10−5 . Often
74 Fig. 2.40 Highresolution Xray diffractometer for structural analyses of heteroepitaxial structures. The studied sample is symbolized by its diffracting Bragg planes. These are not parallel to the sample surface in case of asymmetric reflections
2 Structural Properties of Heterostructures
detector channelcut analyser source
channelcut monochromator
Xray mirror
2θ θ
sample
also a parabolic shaped multilayer mirror is used to convert the divergent radiation of the Xray tube to an intense quasiparallel beam. Such a beam conditioning reduces the required measuring time significantly. A highresolution Xray setup is illustrated in Fig. 2.40. The setup shown in Fig. 2.40 is also referred to as tripleaxis diffractometer, the three rotation axes being the Bragg angles of the monochromator crystal, of the investigated sample, and of the analyzer crystal. Many other configurations of Xray optics are used, depending on the required resolution. Xray measurements are conveniently described in the reciprocal space illustrated in Fig. 2.38. Various types of scans are used to characterize or map a Bragg reflection. Commonly applied scan directions are depicted in Fig. 2.41. The incident and diffracted wave vectors are denoted ki and kf , respectively. Due to the elastic scattering their absolute values are equal and both given by the applied radiation wavelength, k = 2π/λ. The components of the diffraction vector k = kf − ki are q = k(cos αf − cos αi ), q⊥ = k(sin αf + sin αi ). In the Xray diffractometer the angle of rotation of the sample surface is usually labeled ω, and the angle of the detector rotation is labeled 2Θ. The goniometer angle ω represents the angle of incidence with respect to the sample surface αi , and 2Θ equals the sum of αi and the angle of the diffracted beam with respect to the sample surface αf . The components of the diffraction vector are thus directly measured by scanning ω and Θ. In reciprocal space the ω − 2Θ scan is oriented along the direction of the origin to the studied reciprocallattice point. The direction of k remains fixed, while the length changes. For such a radial scan the sample is rotated by an amount ω and the detector is rotated by 2Θ = 2ω. In the case of a symmetric reflection, i.e., when the Bragg planes are parallel to the sample surface and αi = α f , the relation ω = 2Θ/2 applies. The diffraction vector k is then always normal to the surface as depicted in Fig. 2.38.
2.4 Structural Characterization Using XRay Diffraction
2 θ scan
Fig. 2.41 Scan directions in the reciprocal space commonly applied in highresolution Xray diffraction. ki and kf denote initial and final wave vectors of the monochromatic Xray beams, respectively. Angles α represent angles of the incident and diffracted (final) beams with respect to the sample surface
q
αf αi
ω 2 θ scan
kf
ω scan
∇
k
ki
Xray Intensity (cts)
Fig. 2.42 ω scan of the symmetric (004) reflection of a 7 period AlAs/GaAs superlattice structure grown on (001)oriented GaAs. Data points and the gray curve are measured and simulated diffraction patterns, respectively
75
10
6
10
5
10
4
10
3
10
2
10
1
Cu K
32.8
αi ω
kf
sample
2θ = α i+ α f
q
7 x (AlAs/GaAs) d(GaAs)=93 nm d(AlAs)=115 nm
1
32.9
33.0
33.1
33.2
ω (deg)
The ω scan traces a circle of radius k about the origin and is nearly oriented perpendicular to the ω − 2Θ scan. The sample is rotated (‘rocked’) about the ω axis. The angle 2Θ and hence the length of k remains fixed, while the direction of k changes. Usually no analyzer and no slit is attached to the detector for recording all intensity reflected from the sample. This scan is usually referred to as ‘rocking curve’ measurement, although also the ω − 2Θ scan requires sample rotation. The 2Θ scan traces an arc on the Ewald sphere. The incident angle αi and hence ω is kept fixed, and αf is changed by varying the detector angle 2Θ. Both length and direction of the diffraction vector k change. The ω scan is widely applied for the measurement of composition and layer thickness in coherent heterostructures. Data evaluation then applies Vegard’s law (2.2a)–(2.2c) and a simulation of the intensity based on the dynamical theory of Xray diffraction. In (001)oriented structures of a cubic crystal system often the intense symmetric (004) reflection is used. A measured and simulated diffraction pattern of an AlAs/GaAs superlattice structure is shown in Fig. 2.42.
76
2 Structural Properties of Heterostructures
q
hkl
substrate
Φ relaxed =0
hkl layer
strained relaxation line
=1
hkl layer
000
sample
q
Fig. 2.43 Positions of reciprocallattice points hkl of a fully strained (γ = 1) and fully relaxed (γ = 0) epitaxial layer
2.4.6 ReciprocalSpace Map The analysis of elastically relaxed heteroepitaxial structures requires the measurement of both, vertical and lateral lattice parameters. For the evaluation of lateral components asymmetric reflections must be used. Strain relief in the structure may be quite inhomogeneous as shown in Fig. 2.16. Furthermore, Bragg planes of an epitaxial structure may be tilted with respect to those of the substrate, and mosaicity of layers with tilted and twisted crystallites as illustrated in Sect. 2.3.9 may occur. The analysis of such imperfections is conveniently performed by combining a series of scans in reciprocal space to a map. An analysis of the strain state in a partially relaxed epitaxial layer from reciprocalspace maps is illustrated in Figs. 2.43 and 2.44. For simplicity we assume an equal crystal structure for layer and substrate. Partial relaxation may be described by the relaxation parameter γ (2.29) introduced in Sect. 2.2.8. The reflection hkllayer of a coherently strained pseudomorpic layer (γ = 1) has the same lateral component of the scattering vector as the corresponding reflection of the substrate, because the lateral lattice constant of the layer a adopts the value of the substrate aS . In Fig. 2.43 a layer with a natural (unstrained) lattice constant aL larger than the substrate lattice constant aS is assumed. hkllayer therefore lies below hklsubstrate in the reciprocal space map, i.e. at a smaller q⊥ value. For a completely relaxed layer (γ = 0) the Bragg planes lie parallel to that of the substrate. Consequently the scattering vector k has the same direction for layer and substrate, i.e., hkllayer and hklsubstrate lie on a common line starting at the reciprocal origin 000. Intermediate strain states of the layer lie on a relaxation line bounded by the points for γ = 0 and 1, cf. Fig. 2.43. This line is straight due to the assumed validity of Hook’s law during the relaxation process.
2.4 Structural Characterization Using XRay Diffraction
(a) 4.00
77
(b)
5.00
substrate
substrate
4.99
[00l ]
[00l ]
3.99 4.98
3.98
layer
4.97 layer
3.97 0.01
000
0.00
[hh0]
0.01
0.99
1.00
1.01
[hh0]
Fig. 2.44 Reciprocalspace maps of the symmetrical (004) reflection (left) and the (115) reflection (right) of a 310 nm thick epitaxial ZnSe layer on (001) GaAs substrate. Contour lines refer to scattered Xray intensities on a logarithmic scale with steps of 0.2, coordinates are given in terms of noninteger Miller indices. The straight line in the right map indicates the relaxation line. The dotted lines in the maps indicate sections of Ewald spheres, the streaks along these lines are analyzer c 1994 Elsevier artefacts. Reproduced with permission from [80],
The experimental result given in Fig. 2.44 represents a cut of the reciprocal space using √ the [110] axis of the cubic crystal lattice as azimuth reference: q = [hh0] × 2aS , i.e., h always equals k. The normal reference is q⊥ = [00l] × aS . The measurements show the scattered Xray intensity near the (004) and (115) reflections of an epitaxial ZnSe layer on (001)oriented GaAs substrate [80]. Both materials have zincblende structure. The reciprocallattice points of the layer show a clear broadening with a noncircular shape indicated by triangles. The broadening along the vertical dashdotted line (along the surface normal) demonstrates the coexistence of various strain states in the layer. Small 00l values refer to highly strained parts of the layer (γ → 1), large values to relaxed parts. The distribution is asymmetric. Perpendicular to the scattering vector (i.e., the vertical line) another broadening mechanism originating from mosaicity occurs. The triangular shape of the reciprocallattice point indicates that this mosaicity is related to the strain state: small for large strains (lower triangle corner) and large for relaxed parts. The triangles referring to the (004) and (115) reflections are geometrically similar. The different shapes result from a transformation which depends on the inclination angle φ of the Bragg planes [80]. In the next example the mosaicity of an epitaxial layer is considered. Perturbations in the periodicity of the crystal lattice lead to incoherent scattering of Xrays and consequently to a broadening of reciprocal lattice points. From the broadening the average extension of coherently scattering regions in the crystal (i.e., regions free of
78
2 Structural Properties of Heterostructures
(a) q
(b) q
Φ 000
sample
q
000
sample
q
Fig. 2.45 Scheme of broadened reciprocallattice points due to mosaicity in an epitaxial layer originating predominantly from a finite lateral coherence length and b tilts of mosaic blocks
defects) can be derived. The relation between this socalled coherence length d and the broadening of a reciprocal lattice point due to the finite size of perfect crystallites is expressed by an equation formulated by P. Scherrer [81],
FW H M =
Kλ . d × cos Θ
(2.50)
In the Scherrer equation (2.50) F W H M denotes the full width at half maximum of an Xray reflection scattered from crystallites with average dimension d, and K is the Scherrer constant. K is on the order of unity and usually put to 0.9 for a Gaussian function of the reflection shape. λ and Θ are the Xray wavelength and the Bragg angle, respectively. In addition to finitesize effects in lateral and vertical direction expressed by Scherrer’s formula mutual tilts and twists of the small crystalline blocks building the mosaic of a real crystal (Sect. 2.3.9) contribute to the broadening of reciprocal lattice points. The action of tilts differs from that of a finite size as illustrated in Fig. 2.45. Finite sizes of mosaic blocks along the lateral and vertical directions lead to broadenings along q and q⊥ , respectively. This holds for symmetric and asymmetric reflections of any order in the same way as illustrated in Fig. 2.45a for a limited lateral size. Tilts induce a broadening which linearly increases with the order of the reflection. In symmetric reflections the superimposed broadening contributions due to lateral finite size and tilt can be separated by plotting the F W H M of rocking curves over the respective reflection order, yielding the tilt from the slope and the lateral coherence length from the inverse of the ordinate interceptionpoint. Asymmetric reflections are broadened by pure tilts along an axis inclined by the angle φ which represents the angle between the diffracting Bragg planes and the sample surface. Superimposed finite size effects modify the angle.
2.4 Structural Characterization Using XRay Diffraction
6.06
(a)
6.05
1
q (Å )
Fig. 2.46 Reciprocalspace maps of the asymmetric (10.5) reflection of GaN layers with a 350 nm and b 4200 nm mosaic grains, epitaxially grown on (0001) sapphire substrate. Contour lines refer to equal Xray intensities. Reproduced with permission from [82], c 2003 AIP
79
6.07
(b)
6.06 6.05 6.04 2.26
2.27
2.28
2.29
1
q (Å )
Twists lead to a broadening of reciprocal lattice points in the plane spanned by q and a second independent lateral direction. An evaluation can be obtained from grazing incidence diffraction which uses scattering from Bragg planes lying perpendicular to the sample surface or from measuring the edge of the sample. Also selectedarea electron diffraction of plan view scanning TEM was used to image tilt by broadened diffraction spots [71]. The effect of finite mosaic grain size and tilt on asymmetric reflections is illustrated in Fig. 2.46. The reciprocalspace maps show (10.5) reflections of wurtzite GaN grown on basalplane sapphire [82]. The large lattice mismatch leads to very high dislocation densities in the range of typically 109 cm−2 . The measured reflections have nearly elliptical shape with an inclination of the main axis with respect to the azimuth. The angle depends on the average size of mosaic grains in the epitaxial layer. Small angles are due to a dominant effect of lateral finite size. Pure tilts reproduce the inclination φ with respect to the surface (20.5° for the given reflection).
2.5 Problems Chapter 2 2.1 The stable modification of GaN is the wurtzite (α) structure. Epitaxial layers can also be grown in the metastable cubic zincblende (β) structure. (a) Determine the lattice mismatch f of βGaN on (001)oriented zincblende GaAs at room temperature. (b) Find a suitable ratio of small integers for a coincidence lattice and determine the respective coincidencelattice mismatch.
80
2 Structural Properties of Heterostructures
(c) On (111)oriented GaAs the GaN layer tends to grow in the α phase. What is the wurtzite a lattice parameter of the GaAs(111) plane? Prove that the lattice mismatch of αGaN/GaAs(111) is similar to that of βGaN/GaAs(001), if αGaN is assumed to have the same bond length as βGaN. 2.2 GaN is grown on various substrates due to a lack of well latticematched materials. (a) Calculate the lattice mismatch for growth on the most commonly used relation [0001] basalplane sapphire Al2 O3 in case of an epitaxial GaN
¯ ¯ 10 ¯
2 1 [0001]Al2 O3 and [100]GaN [100]Al2 O3 (or 21¯ 10 GaN Al2 O3 , i.e., a and c axes of substrate and layer are parallel). Compare this value to that often derived from the alternative definition f alternative1 given in the text. The lattice parameters of Al2 O3 are aAl2 O3 = 4.758 Å, cAl2 O3 = 12.991 Å. (b) The a axes of the GaN layer are actually rotated by 30° about the c axis, ¯ Al2 O3 (cf. figure below). What is the yielding the relation [100]GaN [110] lattice mismatch for this epitaxial relation?
(c) The growth of mplane wurtzite GaN (with a nonpolar surface) is often performed on γ LiAlO2 , which has a tetragonal structure with lattice parameters a = b = 5.169 Å and c = 6.268 Å. Compute the lattice mismatch of the two edges of the GaN mplane aligned along the two different axes of γ LiAlO2 , when every second Ga atom along the a axis of the GaN sublattice matches an Al atom along the c axis of the γ LiAlO2 sublattice. (d) An alternative mplane substrate for mplane wurtzite GaN is the readily available 6HSiC polytype with ABC AC B stacking order. What is the lattice mismatch for an equal orientation of the unit cells? It should be noted that the GaN layers tend to grow in a 2H sequence and only partially adopt the 6H sequence (in contrast to AlN layers), yielding a high density of stacking faults. 2.3 (a) How does the Al composition parameter x in the quaternary compound Alx Ga y In1−x−y As depend on the Ga composition parameter y for a layer latticematched to InP according to Vegard’s law? (b) What are the maximum of the Ga composition parameter y and the maximum of the Al composition parameter x?
2.5 Problems Chapter 2
81
(c) Write the relation for a quaternary AlGaInAs layer latticematched to InP in terms of two ternary alloys Xz and Yz−1 which are both latticematched to InP. 2.4 Apply in the following problem linear expansion coefficients (which actually underestimate the thermal expansion at higher temperatures) and a linearly weighted quantity for the alloy. (a) Calculate the lattice mismatch f of a ZnS layer on Si substrate at a growth temperature of 360 °C. (b) Determine the composition parameter x of a ZnS1−x Sex layer for latticematched conditions on Si at growth temperature. (c) Calculate the thermally induced lateral strain of the ZnS1−x Sex layer after cooling the latticematched ZnS1−x Sex layer of (b) from 360 °C to room temperature (23 °C). (d) Which composition parameter x produces a strainfree ZnS1−x Sex layer at room temperature for growth at 360 °C? How large is then the mismatch at growth temperature? 2.5 Consider a pseudomorphic ZnSe layer on (001)oriented GaAs substrate at room temperature. (a) Determine the strain of the ZnSe layer perpendicular to the interface. (b) Calculate the relative change of the unitcell volume induced by the strain. (c) The strain in the layer changes the distance dhkl between nearest lattice planes. In crystal systems with orthogonal axes and lattice vectors of lengths a, b, and c the distance can be expressed by dhkl = ((h/a)2 + (k/b)2 + (l/c)2 )−1/2 . Use this relation to calculate the distances between nearest (111) planes in unstrained ZnSe and √ the pseudomorphically strained ZnSe/GaAs layer. Relate the factor 3 in the unstrained material to the stacking sequence of the zincblende structure. (d) Express the thickness of a 285 Å thick layer in units of monolayers. (e) Calculate the strain energy per unit area of a 285 Å thick layer. Which strain energy per unit area has a 114 nm thick layer? (f) Which strain energy is stored in one unit cell of the pseudomorpic ZnSe layer? 2.6 The strain in pseudomorphic latticemismatched layers is sometimes compensated by inserting additional layers with opposite lattice mismatch, yielding layer stacks which are in total latticematched to a substrate. (a) Determine the thickness of an In0.15 Ga0.85 As layer, which is to be pseudomorphically grown on a 1 monolayer thick (001)oriented GaP layer to obtain a total lateral lattice constant coinciding with that of GaAs. How many monolayers of In0.15 Ga0.85 As correspond to this thickness? The stiffness coefficients of GaP are C11 = 141 GPa, C12 = 62 GPa; use a linearly weighted shear modulus for the In0.15 Ga0.85 As layer determined similar to the unstrained lattice parameter of this layer.
82
2 Structural Properties of Heterostructures
(b) The strain in a pseudomorphic superlattice with 10 Inx Ga1−x As quantum wells separated by GaAs barriers is to be compensated by the additional insertion of a counteracting GaAs1−y P y layer into the center of each of these barriers. The entire layer stack of the straincompensated superlattice should adopt the same lateral lattice parameter as the (001)oriented GaAs substrate. Calculate the composition parameter y for the case that in each of the 20 nm thick barrier layers 12 nm of GaAs is replaced by GaAs1−y P y . The quantum wells have a thickness of 10 nm and a composition of 22% indium. Apply a linearly weighted shear modulus for the wells, but approximate the value for the barriers by that of GaAs (check if such a simplification is justified). 2.7 Determine the energy per unit length for the following perfect misfit dislocations in GaAs within a radius of 300 nm around the dislocation line. A single dislocation with a dislocationcore radius of 13 of the Burgers vector is assumed. (a) Pure screw dislocation. (b) Pure edge dislocation. (c) 60° dislocation. 2.8 The composition parameter x of a (001)oriented alloy layer A x B1−x with diamond structure was approximately adjusted for achieving lattice matching to a substrate with lattice parameter aS = 5.5 Å, yielding a misfit f = 10−3 . (a) Estimate the critical thickness for the introduction of 60° misfit dislocations for a Poisson ratio of the layer ν = 0.25, using the graphical result given in the text. (b) By which factor changes the layer thickness for ν = 0.35? (c) Which misfit must be achieved for extending the critical layer thickness by a factor of 5 for a Poisson ratio ν = 0.25? 2.9 A ZnSe/GaAs(001) layer is characterized by Xray diffraction using CuKα1 radiation. (a) Calculate the separation between the Bragg angles for the (004) reflections of the substrate and the layer for a completely relaxed layer and a pseudomorphically strained layer. (b) Repeat (a) for the asymmetric (115) reflection. (c) The intensity of the scattered radiation is largely determined by the square of the structure factor. Calculate the approximate intensity ratio I (004)/I (115) of the two reflections, if the ratio of the atomic scattering factors f Se / f Zn = 1.17.
2.6 General Reading Chapter 2
83
2.10 An Inx Ga1−x N layer is to be grown latticematched on the basal plane of a ZnO substrate. (a) Find the In composition x1 and the Bragg angle of the (00.2) reflection of a latticematched Inx Ga1−x N layer for CuKα1 radiation. (b) Calculate the In composition x2 of a relaxed (not latticematched) Inx Ga1−x N layer producing the (00.2) reflection at a Bragg angle 400 s below the value of a latticematched layer. Compare this value to the composition x3 of a pseudomorphic Inx Ga1−x N layer, whose (00.2) reflection appears at the same Bragg angle (find x3 by using x2 and interpolation; use for simplicity elastic constants of pure GaN).
2.6 General Reading Chapter 2 J.F. Nye, Physical Properties of Crystals (Clarendon Press, Oxford, 1972) A.S. Saada, Elasticity Theory and Applications (Pergamon Press, New York, 1974) J.P. Hirth, J. Lothe, Theory of Dislocations, 2nd edn. (Wiley, New York, 1982) D. Hull, D.J. Bacon, Introduction to Dislocations, 4th edn. (ButterworthHeinemann, Oxford, 2001) S. Amelinckx, Dislocations in particular structures, in Dislocations in Solids, vol. 2, ed. by F.R.N. Nabarro (NorthHolland, Amsterdam, 1979) J.E. Ayers, T. Kujofsa, P. Rago, J.E. Raphael, Heteroepitaxy of Semiconductors: Theory, Growth, and Characterization, 2nd edn. (CRC Press, Boca Raton, 2017)
References 1. C.Y. Yeh, Z.W. Lu, S. Froyen, A. Zunger, Zincblendewurtzite polytypism in semiconductors. Phys. Rev. B 46, 10086 (1992) 2. O. Ambacher, J. Smart, J.R. Shealy, N.G. Weimann, K. Chu, M. Murphy, W.J. Schaff, L.F. Eastman, R. Dimitrov, L. Wittmer, M. Stutzmann, W. Rieger, J. Hilsenbeck, Twodimensional electron gases induced by spontaneous and piezoelectric polarization charges in N and Gaface AlGaN/GaN heterostructures. J. Appl. Phys. 85, 3222 (1999) 3. H. Ibach, Thermal expansion of silicon and zinc oxide. Phys. Status Solidi 31, 625 (1969) 4. K. Haruna, H. Maeta, K. Ohashi, T. Koike, The negative thermal expansion coefficient of GaP crystal at low temperatures. J. Phys. C 19, 5149 (1986) 5. J.St. John, A.N. Bloch, Quantumdefect electronegativity scale for nontransition elements. Phys. Rev. Lett. 33, 1095 (1974) 6. J.R. Chelikowsky, J.C. Phillips, Quantumdefect theory of heats of formation and structural transition energies of liquid and solid simple metal alloys and compounds. Phys. Rev. B 17, 2453 (1978) 7. S.B. Zhang, M.L. Marvin, Determination of AB crystal structures from atomic properties. Phys. Rev. B 39, 1077 (1989) 8. P. Villars, K. Mathis, F. Hulliger, Environment classification and structural stability maps, in The Structure of Binary Compounds, ed. by F.R. de Boer, D.G. Pettifor (NorthHolland, Amsterdam, 1989) 9. O. Madelung (ed.), SemiconductorsBasic Data, 2nd revised edn. (Springer, Berlin, 1996)
84
2 Structural Properties of Heterostructures
10. G.L. Harris (ed.), Properties of Silicon Carbide. EMIS Datareview Series, vol. 13 (INSPEC, London, 1995) 11. J.H. Edgar (ed.), Properties of Group III Nitrides. EMIS Datareview Series, vol. 11 (INSPEC, London, 1994) 12. L. Vegard, [De]Die Konstitution der Mischkristalle und die Raumfüllung der Atome. Z. Phys. 5, 17 (1921). (in German) 13. M.F. Thorpe, E.J. Garboczi, Elastic properties of centralforce networks with bondlength mismatch. Phys. Rev. B 42, 8405 (1990) 14. W.B. Pearson, A Handbook of Lattice Spacing and Structures of Metals and Alloys, vol. 1 (Pergamon Press, London, 1958) 15. D.R. YoderShort, U. Debska, J.K. Furdyna, Lattice parameters of Zn1−x Mnx Se and tetrahedral II Mn BVI alloys. J. Appl. Phys. 58, 4056 (1985) bond lengths in A1−x x 16. J.C. Mikkelsen Jr., J.B. Boyce, Extended Xray absorption finestructure study of Ga1−x Inx As random solid solutions. Phys. Rev. B 28, 7130 (1983) 17. A. Balzarotti, N. Motta, A. Kisiel, M. ZimnalStarnawska, M.T. Czyzyk, Model of the local structure of random ternary alloys: experiment versus theory. Phys. Rev. B 31, 7526 (1985) 18. J.L. Martins, A. Zunger, Bond lengths around isovalent impurities and in semiconductor solid solutions. Phys. Rev. B 30, 6217 (1984) 19. J.C. Mikkelsen Jr., J.B. Boyce, Atomic scale structure of random solid solutions: extended Xray absorption finestructure study of Ga1−x Inx As. Phys. Rev. Lett. 49, 1412 (1982) 20. T. Fukui, Atomic structure model for Ga1−x Inx As solid solutions. J. Appl. Phys. 57, 5188 (1985) 21. J.F. Nye, Physical Properties of Crystals (Clarendon Press, Oxford, 1972) 22. A.S. Saada, Elasticity Theory and Applications (Pergamon Press, New York, 1974) 23. D.J. Dunstan, Strain and strain relaxation in semiconductors. J. Mater. Sci., Mater. Electron. 8, 337 (1997) 24. K.H. Hellwege, A.M. Hellwege, LandoltBörnstein New Series Group III, vol. 2, Elastic, Piezoelectric, Piezooptic, Electrooptic Constants, and Nonlinear Dielectric Susceptibilities of Crystals, 6th edn. (Springer, Berlin, 1966) 25. K.H. Hellwege, A.M. Hellwege, LandoltBörnstein New Series Group III, vol. 1, Elastic, Piezoelectric, Piezooptic and Electrooptic Constants of Crystals, 6th edn. (Springer, Berlin, 1966) 26. I. Vurgaftman, J.R. Meyer, L.R. RamMohan, Band parameters for IIIV compound semiconductors and their alloys. J. Appl. Phys. 89, 5815 (2001) 27. G. Carlotti, D. Fioretto, G. Socino, E. Verona, Brillouin scattering determination of the whole set of elastic constants of a single transparent film of hexagonal symmetry. J. Phys. Condens. Matter 7, 9147 (1995) 28. R.S. Lakes, Foam structures with a negative Poisson’s ratio. Science 235, 1038 (1987) 29. E. Pasternak, A.V. Dyskin, Architectured materials with inclusions having negative Poisson’s ratio or negative stiffness, in Architectured Materials in Nature and Engineering, ed. by Y. Estrin, Y. Bréchet, J. Dunlop, P. Fratzl (Springer, Cham, 2019) 30. A. Ballato, Poisson’s ratio for tetragonal, hexagonal, and cubic crystals. IEEE Trans. Ultrason. Ferroelectr. Freq. Control 43, 56 (1996) 31. C.G. Van de Walle, R.M. Martin, Theoretical calculation of heterojunction discontinuities in the Si/Ge system. Phys. Rev. B 34, 5621 (1986) 32. L. Kleinman, Deformation potentials in silicon. I. Uniaxial strain. Phys. Rev. 128, 2614 (1962) 33. O.H. Nielsen, R.M. Martin, Stress in semiconductors: ab initio calculations on Si, Ge, and GaAs. Phys. Rev. B 32, 3792 (1985) 34. W.A. Jesser, D. KuhlmannWilsdorf, On the theory of interfacial energy and elastic strain of epitaxial overgrowth in parallel alignment on single crystal substrates. Phys. Status Solidi 19, 95 (1967) 35. F.C. Frank, J.H. van der Merve, Proc. R. Soc. Lond. A 198, 205 (1949) 36. F.C. Frank, J.H. van der Merve, Proc. R. Soc. Lond. A 198, 216 (1949) 37. F.C. Frank, J.H. van der Merve, Proc. R. Soc. Lond. A 200, 125 (1949)
References
85
38. J.H. Van der Merve, Crystal interfaces. Part I. Semiinfinite crystals. J. Appl. Phys. 34, 117 (1963) 39. J.H. Van der Merve, C.A.B. Ball, Energy of interfaces between crystals, in Epitaxial Growth. Part B, ed. by J.W. Matthews (Academic Press, New York, 1975), pp. 493–528 40. C.A.B. Ball, J.H. Van der Merve, The growth of dislocationfree layers, in Dislocations in Solids, vol. 6, ed. by F.R.N. Nabarro (NorthHolland, Amsterdam, 1983) 41. W.A. Jesser, J.H. Van der Merve, An exactly solvable model for calculating critical misfit and thickness in epitaxial superlattices. II. Layers of unequal elastic constants and thicknesses. J. Appl. Phys. 63, 1928 (1988) 42. J.W. Matthews, A.E. Blakeslee, Defects in epitaxial multilayers I. Misfit dislocations. J. Cryst. Growth 27, 118 (1974) 43. J.W. Matthews, S. Mader, T.B. Light, Accommodation of misfit across the interface between crystals of semiconducting elements or compounds. J. Appl. Phys. 41, 3800 (1970) 44. C.A.B. Ball, On bonding and structure of epitaxial bicrystals. Phys. Status Solidi 42, 357 (1970) 45. R. Beanland, D.J. Dunstan, P.J. Goodhew, Plasic relaxation and relaxed buffer layers for semiconductor epitaxy. Adv. Phys. 45, 87 (1996) 46. I. Akasaki, H. Amano, Y. Koide, K. Hiramatsu, N. Sawaki, Effects of a buffer layer on crystallographic structure and on electrical and optical properties of GaN and Ga1−x Alx N (0 0
so
ε xx < 0
Fig. 4.2 Effect of strain on the valence bands and the lowest conduction band (CB) of a zincblendetype semiconductor. hh, lh, and so denote heavyhole, lighthole, and splitoff hole valence bands, 0 is the spinorbit splitting. εx x = ε yy is the inplane strain Table 4.1 Average valenceband energies E v,av and deformation potentials of the valence band av , the conduction band ac , and the gap energy a calculated from the modelsolid theory. 0 and E g denote measured spinorbit splitting and energy gap at 0 K, respectively. All values are given in eV. Data from [10] Solid E v,av av acdir a dir E gdir E cdir acindir a indir E gindir E cindir 0 Si Ge GaP AlAs GaAs InAs ZnS ZnSe
−7.03 −6.35 −7.40 −7.49 −6.92 −6.67 −9.15 −8.37
2.46 1.24 1.70 2.47 1.16 1.00 2.31 1.65
1.98 −8.24 −7.14 −5.64 −7.17 −5.08 −4.09 −4.17
−0.48 −9.48 −8.83 −8.11 −8.33 −6.08 −6.40 −5.82
3.37 0.89 2.90 3.13 1.52 0.41 3.84 2.83
−3.65 4.18 1.72 1.17 −5.36 −1.54 −2.78 0.74 −4.47 3.36 1.56 2.35 −4.27 4.09 1.62 2.23 −5.29 −6.13 −5.29 −5.40
−5.85 −5.51 −5.02 −5.17
0.04 0.30 0.08 0.28 0.34 0.38 0.07 0.43
strained parallel to the interface (x, y) and compressively strained perpendicular (z). According to (2.19a)–(2.19c) the respective strains are εx x = ε yy = 0.046 and εzz = −0.058, leading to a fractional volume increase V /V = 0.035. The change of the volume affects the energy of valence band and conduction band. The band ZnS = −9.07 eV energies of the strained ZnS layer follow from (4.4), yielding E v,av ZnS and E c = −5.43 eV. The deformation potential b of ZnS is −1.25 eV, yielding with (4.7) δ E 001 = 0.26 eV. From (4.6) we finally obtain the energy shifts of the heavy hole, the light hole, and the splitoff hole of the strained ZnS layer ZnS being −0.11 eV, +0.26 eV, and −0.16 eV, respectively. with respect to E v,av The resulting alignment with E v = −0.50 eV and E c = 0.03 eV is depicted in Fig. 4.3.
4.1 Bulk Properties Fig. 4.3 Band alignment of a biaxially strained pseudomorphic ZnS layer on a (001)oriented ZnSe substrate, calculated according to the modelsolid theory using experimental values for gap energies and spinorbit splittings. After [10]
121
E (eV) ZnSe substrate 5
ZnS (unstrained) Ec
Ec
Ec
6 8 9
Ev Ev,av Ev,so
ZnS layer (strained)
Ev
Ev,av Ev,so
Ev
Ev,lh Ev,hh Ev,so
10
Deformation potentials are experimentally obtained from optical spectroscopy. A comparison of the reflectivity and a twophoton absorption spectrum of a ZnSe bulk crystal is shown in Fig. 4.4a. The sharp nonlinear resonances of the 1S exciton allow for a direct measurement of splittings induced by stresses applied along various crystallographic lowindex directions. The deformation potentials a, b, and d are contained in the Hamiltonian of the 1S orthoexciton and are evaluated by assigning the measured energies to the eigenenergies [11]. Results for uniaxial stress along [001] are given in Fig. 4.4b. Application of uniaxial stress to a biaxially strained 5.3 µm thick ZnSe layer on GaAs substrate is shown in Fig. 4.4c. In the lowest spectrum the splitting of lighthole and heavyhole 1S exciton due to pure biaxial strain of the epilayer is seen. Four resonances of the 1S exciton appear when an additional stress is applied along [110]. They are linearly polarized either parallel (π ) or perpendicular (σ ) with respect to the axis of external stress. The stressinduced strain lowers the symmetry to C2v and creates dipoleallowed mixtures of paraexcitons with orthoexcitons, giving rise to 2 × 2 resonances [12]. Experimentally determined deformation potentials for some semiconductors are given in Table 4.2. Wurtzite Crystals We now consider semiconductors with wurtzite structure like the Column III nitrides or ZnO. The unstrained valenceband structure of wurtzite crystals shown in Fig. 4.1b. Due to a weak spinorbit coupling the dispersions of the hh, lh, and chvalencebands are not strongly affected by strain, in contrast to effects in zincblende materials. Under biaxial strain in the basal plane the C6v symmetry of the unit cell is preserved, but the crystalfield splitting changes. For compressive biaxial strain the energy which separates the crystalhole band from the heavyhole and lighthole bands is increased, for tensile strain it is decreased. Uniaxial strain in the basal plane reduces the symmetry to C2v . Under compressive uniaxial strain along the –K direction in
122
4 Electronic Properties of Heterostructures 2.814
(b) 2.812
FII[110] k II[110]
Intensity
Reflectivity
198 96 Reflectivity
Energy (eV)
2.810
(a)
(c)
2.808 2.806
90
2.804
33
2.802
lh
2.800 2.79
2.80
2.81
Energy (eV)
0
30
60
90
120
Stress (MPa)
2.80
0 (MPa)
hh 2.81
2.82
2.83
Energy (eV)
Fig. 4.4 a Twophoton excitation spectrum (solid lines) and reflectivity (dashed) of a ZnSe bulk crystal, recorded at 5 K and 2 K, respectively. b Shift and splitting of twophoton resonances for ¯ and polarizations parallel to [001] uniaxial stress applied along [001], incident light along [110], c 1995 APS. (filled symbols) and [110] (open symbols). Reproduced with permission from [11], (c) Reflectance spectra of a biaxially strained epitaxial ZnSe/GaAs layer under an additional external stress σ applied along [110]. Solid and dotted curves refer to σ and π polarizations, respectively. c 1996 APS Reproduced with permission from [12], Table 4.2 Deformation potentials a, b, and d, experimentally determined for the lowest bandgap E g from optical spectroscopy (exp). Theoretical values (theo) are from the modelsolid theory [10]. Solids denoted in bold have an indirect lowest bandgap. All values are given in eV Solid a exp a theo bexp btheo d exp d theo Si Ge GaP AlAs GaAs InAs ZnS ZnSe
+1.5 ± 0.3a −2.0 ± 0.5b −9.9 ± 0.3c −8.2d −8.5d,e −6.1d −4.56f −4.7 ± 0.2g
+1.72 −2.78 +1.56 +1.62 −8.33 −6.08 −6.40 −5.82
−2.10 ± 0.10a −2.86 ± 0.15b −1.5 ± 0.2c −2.3d −2.0d,e −1.8d −0.75f
−2.35 −2.55
−1.90 −1.55 −1.25 −1.20
−4.85 ± 0.15a −5.28 ± 0.50b −4.6 ± 0.2c −3.4d −4.8d,e −3.6d
−5.32 −5.50
−4.23 −3.10
−6.37 ± 0.07g
a Reference [13], b Reference [8], c Reference [14], d Reference [3], e Reference [15], f Reference [9], g Reference
[11] (factor
√
3/2 in d taken into account)
4.1 Bulk Properties
123
the first Brillouin zone (‘y’ direction) the lh band in this direction and the hh band in the perpendicular lateral x direction move to higher energy. The same effect has a tensile strain along the x direction, and a reverse effect has a tensile strain along the y direction.
4.1.3 Spontaneous Polarization and Piezoelectricity In absence of external electric fields and stress, crystals of low symmetry may show a spontaneous electric polarization. No such effect occurs for zincblende crystals, but spontaneous polarization is observed with wurtzite crystals and structures of lower symmetry [6]. It originates from a mutual shift of positive and negative charges in the unit cell, and in wurtzite structure the main part depends on the deviation of the lattice parameter u listed in Table 2.3 from the ideal value 3/8 c = 0.375 c: a larger u leads to an increase of the spontaneous polarization [16]. The polarization produces charges located at interfaces and surfaces, and the polarization vector PSP points from negative to positive charges. Experimental values of the spontaneous polarization are difficult to measure and scarce; values computed using densityfunctional theory are given in Table 4.4. If stress is applied on a crystal which has no inversion centre in the unit cell, an electric polarization is produced; this effect is referred to as piezoelectricity. The piezoelectric polarization PPE is in first order proportional to the strain, but secondorder piezoelectricity may be relevant for zincblende semiconductors [17]. For crystals showing spontaneous polarization, the total macroscopic polarization P is given by the sum of PSP and PPE . The piezoelectric polarization vector PPE is obtained from the product of the piezoelectric tensor and the strain ε; in the linear regime the components of PPE are given by PPE,i = ei jk ε jk ; (4.9) jk
here ei jk are components (piezoelectric stress constants) of the thirdrank piezoelectric tensor and ε jk are components of the secondrank strain tensor defined in (2.4)1 ; the indices i, j, k stand for the x, y, and z axes of the Cartesian coordinate system. The piezoelectric tensor is commonly written in the matrix representation of the Voigt notation, where the indices j and k are replaced by a single index, yielding for (4.9) the notation
1 The strain components denoted e
jk introduced in (2.3) and applied in (2.4) should not be confused with the piezoelectric tensor components ei jk introduced in (4.9).
124
4 Electronic Properties of Heterostructures
⎛
⎛
PPE
⎞ ⎛ PPE,x e11 e12 e13 e14 e15 = ⎝ PPE,y ⎠ = ⎝ e21 e22 e23 e24 e25 PPE,z e31 e32 e33 e34 e35
εx x ⎞ ⎜ ε yy e16 ⎜ ⎜ εzz e26 ⎠ ⎜ ⎜ ε yz + εzy e36 ⎜ ⎝ εzx + εx z εx y + ε yx
⎞ ⎟ ⎟ ⎟ ⎟. ⎟ ⎟ ⎠
(4.10)
The piezoelectric tensor has 18 independent components only for the lowsymmetry triclinic crystals; for crystals with higher symmetry many components are zero. All ei j = 0 in (4.10) for crystals with inversion symmetry, such as diamond Si and Ge, or rocksalt MgO. For zincblende structure the piezoelectric tensor has only a single independent constant and reads ⎛
⎞ 0 0 0 e14 0 0 ezincblende = ⎝ 0 0 0 0 e14 0 ⎠ ; 0 0 0 0 0 e14
(4.11)
for wurtzite crystals three independent piezoelectric constants exist, yielding ⎛
⎞ 0 0 0 0 e15 0 ewurtzite = ⎝ 0 0 0 e15 0 0 ⎠ . e31 e31 e33 0 0 0
(4.12)
In zincblende crystals only offdiagonal components of the strain tensor produce piezoelectricity, as we note when inserting (4.11) into (4.10). Strain along the cubic axes as, e.g., occurring in biaxially strained quantum wells grown on (001) oriented substrates, have consequently no effect—in contrast to strain in quantum wells on (111) substrates. Piezoelectricity is usually weak in zincblende material, even for growth of heterostructures along [111]; in such strained layers the x component of PPE is given by
PPE,x = e14 ε yz + εzy = 2e14 ε yz . (4.13) The y and z components of PPE result from a cyclic change of x, y, and z. The three offdiagonal strain components are equal, and consequently also those of PPE which √ points in [111] direction; the absolute value of the polarization is hence PPE = 2 3 e14 εx y . The offdiagonal strain components are related to the lattice mismatch f of [111] oriented pseudomorphic layers with ε = f (see (2.20a)) by εx y = −
C11 + 2C12 f. C11 + 2C12 + 4C44
(4.14)
The common zincblende III–V semiconductors have negative components e14 and the II–VI semiconductors positive components (Table 4.3). A [111] compressively strained quantum well in a III–V semiconductor then produces a polarization vector pointing from the cation A face to the anion B face.
4.1 Bulk Properties
125
Table 4.3 Linear e14 and quadratic B coefficients of the piezoelectric tensor for zincblende semiconductors given in C/m2 . Linear coefficients with index calc and quadratic coefficients are calculated values from [19] with 0.05 C/m2 precision unless explicitly indicated, exp denotes experimental values exp calc Semiconductor e14 e14 B114 B124 B156 AlAs AlSb GaP GaAs GaSb
0.157, 0.068 −0.10, −0.15 −0.16 −0.12, −0.126 −0.083 −0.045, −0.12 −0.071, −0.097 0.049 0.028 0.034
InP InAs InSb ZnSe ZnTe CdTe
−0.048 −0.084 −0.131 −0.238 −0.247
−1.5 −0.7 −0.7 −0.4 0.2 ± 0.1
−2.6 −2.2 −3.6 −3.8 −3.2 ± 0.1
−1.2 −0.7 −0.9 −0.7 0.0
0.003 −0.115
−1.1 −0.6 ± 0.1
−3.8 −4.1
−0.5 0.2
−0.159
0.1
−3.5
0.6
The electric field produced by the polarization is given by [18, 19] E PE
√ PPE 2 3 =− =− e14 εx y , εr ε0 εr ε0
(4.15)
where εr is the permittivity of the lowfrequency dielectric constant. Secondorder piezoelectricity may be important for zincblende structures [17]. Considering both linear and quadratic terms in strain we extend (4.9) to
PPE,i =
jk
ei jk ε jk +
1 Bi jkmn ε jk εmn , 2 jkmn
(4.16)
with the indices denoting the Cartesian axes. Bi jkmn is a fifthrank tensor with – for zincblende symmetry – 24 nonzero components comprising three independent ones. In second order the polarization involves both diagonal and offdiagonal components according to [19], ⎛
⎞ ⎛ ⎞ ⎛ ⎛ ⎞ ⎞ 2ε yz 2εx x ε yz 2ε yz (ε yy + εzz ) 4εx z εx y P = e14 ⎝ 2εx z ⎠ + B114 ⎝ 2ε yy εx z ⎠ + B124 ⎝ 2εx z (εzz + εx x ) ⎠ + B156 ⎝ 4ε yz εx y ⎠ . 2εx y (εx x + ε yy ) 2εx y 2εzz εx y 4ε yz εx z
(4.17)
126
4 Electronic Properties of Heterostructures
Layer GaAs InP GaP InAs GaSb GaP InAs GaAs InP InSb Substrate GaP GaP GaAs GaAs GaAs InP InP InAs InAs InAs 2000
Electric field (kV/cm)
1000 0 1000 2000 3000 4000 5000
Fig. 4.5 Calculated electric fields in coherently strained [111] oriented quantum wells of zincblende A/B (A on B substrate) heterostructures produced by linear (green) and linear + quadratic (red) piezoelectricity. Data from [19]
For growth along [111] now also the diagonal strain components appear: εx x = ε yy = εzz =
4C44 f, C11 + 2C12 + 4C44
(4.18)
and (4.16) yields the secondorder polarization (in Voigt notation) √ √ PPE = 2 3e14 ε yz + 2 3 (B114 εx x + 2B124 ε yy )ε yz + 2B156 εx z εx y ,
(4.19)
with the linear first and the quadratic second summand. Firstprinciples calculations indicate that the piezoelectric effect of second order in strain yields important contributions in the studied III–V semiconductors [19], see Fig. 4.5. Data of piezoelectric constants for some zincblende III–V and II–VI semiconductors are given in Table 4.3. Wurtzite heterostructures of the column III nitrides or ZnO show strong piezoelectricity. We consider polarizations along the c axis, i.e., along the common [0001] growth direction. Biaxial strain in the basal plane is expressed by εx x = ε yy = ε = (aL − aL,0 )/aL,0 , and strain along the c axis correspondingly by εzz = ε⊥ = (cL − cL,0 )/cL,0 . The indices L and L,0 denote the actual (strained) and natural lattice parameters of the layer, respectively. Using the relation between ε and ε⊥ (2.19c) we obtain for the z component of the piezoelectric polarization of a biaxially strained wurtzite crystal
4.1 Bulk Properties
127
Table 4.4 Coefficients ei j of the piezoelectric tensor and spontaneous polarization PSP of wurtzite semiconductors. All values are given in C/m2 Semiconductor e15 e31 e33 PSP −0.22 . . . −0.33a −0.48a
GaN AlN InN ZnO a Reference
−0.35 . . . −0.59d [21],
b Reference
−0.35b −0.50b −0.57b −0.35 · · · − 0.62d
1.27b 1.79b 0.97b 0.96 . . . 1.56d
−0.029c −0.081c −0.032c −0.057c
[3], c Reference [16], d Reference [22]
C13 . PPE,z = 2ε e31 − e33 C33
(4.20)
Literature data of piezoelectric tensor components and the spontaneous polarization for some wurtzite semiconductors are given in Table 4.4. According to the sign convention a positive c axis points from the metal cation to the adjacent anion. The semiconductors listed in Table 4.4 show a negative spontaneous polarization. The sign of the straininduced piezoelectricity depends on the sign of strain. For Alx Ga1−x N the bracket in (4.13) yields negative values, and the piezoelectric polarization is positive for compressive strain (ε < 0). The total polarization Pz = PSP,z + PPE,z may then have either sign. For a review on electromechanical phenomena in semiconductor nanostructures see [20]. Piezoelectricity has a substantial effect on the electronic properties of devices made from GaNbased heterostructures. At the interface between two wurtzite semiconductors 1 and 2 the total polarization changes, giving rise to a sheet charge σ determined by the difference in total polarization, σ = (PSP,z1 + PPE,z1 ) − (PSP,z2 + PPE,z2 ). Highelectronmobility transistors based on strained AlGaN/GaN heterostructures achieved very high sheet carrier concentrations in a twodimensional electron gas formed at the interface, enabling devices with excellent performance. The high values could be assigned to an additive effect of spontaneous and piezoelectric polarization in structures with tensely strained AlGaN barriers [23].
128
4 Electronic Properties of Heterostructures
4.1.4 Temperature Dependence of the Bandgap Energies of electronic bands are generally calculated for a temperature T = 0 K. To describe the temperature dependence of the important fundamental bandgap E g a number of approaches was developed. The usually observed decrease of E g for increased temperature originates from a change of both, the electronphonon interaction and the interatomic bond distance. Instead of an explicit derivation from such interactions empirical formula are widely used to express the thermal behavior of E g . Most popular is the empirical Varshni formula [24]
E g (T ) = E g (T = 0) −
αT 2 , T +β
(4.21)
where the three parameters E g (T = 0), α, and β are fitted to experimental data. The dependence describes both, direct and indirect bandgaps. E g (T = 0) is the bandgap energy at 0 K. α is claimed to be related to the Debye temperature but may in certain cases be negative. Moreover, at very low temperatures a rather temperatureindependent behavior of E g was found instead of the quadratic dependence predicted from (4.21). Typical values for α and β are in the range (0.4–0.6) meV/K and (200– 600) K, respectively. The thermal shift of the bandgap energy according to (4.21) is illustrated in Fig. 4.6. A number of better motivated models was developed later, based on the occupation of phonon states and assuming an average phonon energy [25–27]. They particularly improve the description of lowtemperature data but require at least one additional parameter. The physically wellfounded model reported in [27, 29] assumes four parameters to account for the BoseEinstein occupation of phonon modes and for phonon dispersion; it comprises the threeparameter approach of Varshni for the limit of very large phonon dispersion. The analytical fourparameter approximation reads
1.17
Si
1.16
Egg (eV)
Fig. 4.6 Dependence of the indirect bandgap energy of Si on temperature. The gray curve is a fit to Varshni’s formula (4.21), data are from [28]
1.15 1.14 1.13 1.12
0
100
200
T (K)
300
4.1 Bulk Properties
129
1−3Δ2 E g (T ) = E g (T = 0) − αΘ exp(Θ/T )−1 2T 2 3Δ2 −1 2T 3 2 6 π2 + 3Δ2 1 + 3(1+Δ + + 2) Θ 4 Θ
8 3
2T 4 Θ
+
2T 6 Θ
−1
(4.22)
Here Θ is the effective (average) phonon temperature, and Δ is a dispersion coefficient; α is the hightemperature limiting magnitude of the slope of the E g (T ) dependence. The two dispersionrelated parameters Θ and Δ are defined by introducing moments εm = εm · w(ε) dε, m = 1, 2, of the total phonon energy spectrum with a normalized weighting function w(ε) ≥ 0, w(ε) dε = 1, yielding Θ = ε /k,
(4.23)
ε2 − ε 2 / ε ,
(4.24)
α = − d E g /dT T →∞ .
(4.25)
Δ=
The dimensionless dispersion parameter Δ ranges from 0 (small dispersion) to ∼3/4, while a reproduction of values resulting from Varshi’s formula (4.21) require unrealistic large values of ∼1.25 [29]. Table 4.5 lists parameter data for both Varshni’s empirical model and the dispersionrelated approach.
4.1.5 Bandgap of Alloys The bandgap energy of a miscible random alloy of two (or more) semiconductors may continuously be varied by changing the composition. Unlike the lattice constant discussed in Sect. 2.1.10 the bandgap of the alloy is usually not obtained by a linear interpolation. Instead, it can normally be described by a quadratic dependence using a bowing parameter b which is mostly positive [32]. The bandgap energy E g alloy of an alloy A x B1−x from two materials A and B with the same crystal structure and bandgaps E g A and E g B , respectively, is expressed by
E g alloy = x E g
A
+ (1 − x)E g
B
− bx(1 − x),
(4.26a)
x being the molar fraction of A in the alloy (cf. Sect. 2.1.10). The bandgap energy of a (pseudobinary) ternary alloy A x B1−x C from binaries AC and BC is given by the same relation putting E g A and E g B to E g AC and E g BC , respectively. For quaternary compounds of the type A x B y C1−x−y D (i.e., mixing of A, B, C atoms on the cation
130
4 Electronic Properties of Heterostructures
Table 4.5 Parameterized temperature dependence of the bandgap energy E g for various semiconductors according to the empirical Varshi formula and the dispersionrelated model. Varshi parameters of III–V are from [3, 29], II–VI parameters are from [31]; dispersionrelated parameters are from [29] Semiconductor E g (T = 0) Varshi’s parameters Dispersionrelated parameters (lowest band) (eV) α (10−4 β(K) α (10−4 Θ (K) Δ eV/K) eV/K) Si (X ) Ge (L) AlN ( A ) GaN( A ) InN( A ) AlP (X ) GaP(X ) InP () AlAs (X ) GaAs () InAs () AlSb (X ) GaSb () InSb () ZnS () CdS ( A ) ZnSe () CdSe ( A ) ZnTe () CdTe ()
1.170 0.743 6.25 3.510 0.78 2.52 2.35 1.4236 2.24 1.519 0.417 1.696 0.812 0.235 3.91 2.579 2.820 1.84 2.39 1.606
4.73 4.774 17.99 9.09 2.45 3.18 5.771 3.63 7.0 5.405 2.76 3.9 4.17 3.2 10 4.7 5.58 17 5.49 3.10
636 235 1462 830 624 588 372 162 530 204 93 140 140 170 600 230 187 1150 159 108
3.23 4.13 9.1 6.14 2.3
446 253 770 586 590
0.51 0.49 0.34 0.40 0.35
4.77 3.96 3.90 4.77 2.82 3.45 3.87 2.54 5.49 4.10 5.00 4.08 4.68 3.08
355 274 256 252 147 205 205 155 285 166 218 187 170 104
0.60 0.48 0.48 0.43 0.68 0.76 0.44 0.36 0.37 0.47 0.36 0.20 0.37 0.69
sublattice) the bandgaps are described by the weighted sum of the related ternary alloys AB D, AC D, and BC D, yielding [33]
E g alloy = x E g AD + y E g B D + (1 − x − y)E g C D − b AB x y − b AC x(1 − x − y) − b BC y(1 − x − y). (4.26b) Here b AB , b AC and b BC are the three bowing parameters for the ternary alloys A x B1−x D, A x C1−x D, and Bx C1−x D, respectively. The bandgap energy for quaternary alloys of the type A x B1−x C y D1−y (i.e., mixing on the cation and anion
4.1 Bulk Properties
131
Table 4.6 Bowing parameters b of the direct bandgap of alloyed GaAsbased zincblende and GaNbased wurtzite semiconductors. Data from [3] Semiconductor b for alloy with GaAs Semiconductor b for alloy with GaN (eV) (eV) −0.127 + 1.310 × xAl AlN 0.477 InN 0.8
AlAs InAs GaP
1.0 3.0
sublattice) is calculated from the ternary parameters E g E g AB D ,
x(1 − x)[y E g
E g alloy = E g ABC (x) = x E g Eg
AB D (x),
Eg
AC
ABC (x) + (1 −
y)E g
+ (1 − x)E g
AC D (y),
and E g
ABC ,
AB D (x)] + y(1 − y)[x E g x(1 − x) + y(1 − y)
BC
Eg
AB D ,
AC D (y) + (1 −
− b ABC x(1 − x),
BC D (y)
Eg
AC D ,
x)E g
and
BC D (y)]
,
(4.26c)
accordingly.
We note that (4.26a)–(4.26c) are similar to (2.2a)–(2.2c) for b = 0. Bowing parameters for some ternary (pseudobinary) alloys are given in Table 4.6. The value given for Alx Ga1−x As indicates that a constant bowing parameter does not always yield an appropriate description. Bandgap energies for a number of important semiconductors are given in Fig. 4.7. The lines representing the bandgap of alloys in Fig. 4.7 sometimes have a kink. Such features originate from a transition of a direct to an indirect semiconductor due to a crossing of the lowest conduction band and an X or L conduction band (for Si and Ge crossing of indirect X and L bands). The bandgap energy of alloys composed of more than two semiconductors can be illustrated using diagrams with curves of constant energy versus composition parameters. A material of particular importance for optoelectronic devices is the quaternary alloy Gax In1−x As y P1−y . The bandgap of such quaternaries may be chosen independently from the lattice parameter by a proper selection of the two independent composition parameters x and y. For lattice matching conditions on InP substrates one composition parameter is independent and may be used to choose a bandgap energy, while the other parameter is given by x = 0.1896y/(0.4176 − 0.0125y) ≈ 0.47y (0 ≤ y ≤ 1). The diagram Fig. 4.8 shows the variation of the direct bandgap of Gax In1−x As y P1−y in the full range of compositions x and y, along with lattice matching conditions for GaAs and InP substrates.
132
4 Electronic Properties of Heterostructures
Fig. 4.7 Bandgap energy as a function of lattice constant for pure (dots) and alloyed zincblende and diamond semiconductors at room temperature. Blue, red, and green drawing denote direct , indirect X , and indirect L bandgap, respectively
GaAs 1.0
Ga composition x
0.8 0.6 0.4 0.2
2.1
InP
0.0
5
0.
InAs 0.0
GaP
1.6 1 1. 1. .7 8 9 2 .0 1. 1. 5 1.4 GaA 3 s 1. 2
1 1. 1.0 9 0. 0.8 0.7 .6 0
Fig. 4.8 Bandgap energy of the quaternary alloy Gax In1−x As y P1−y in eV at 300 K as a function of compositions x and y. Red and green lines mark compositions which are lattice matched to GaAs and to InP. From [38]
0.2
0.4
0.6
0.8
1.0
InP
P composition 1y
Equations (4.26a)–(4.26c) show that the bandgap energy of an alloy usually deviates from a linear concentrationweighted interpolation by a quadratic term described by the bowing parameter b. It should be noted that the virtualcrystal approximation (Sect. 2.1.11) which describes a lattice parameter variation without bowing also yields such bowing for the bandgap energy [32, 34–36]. The reason is that the eigenvalues produced by bandstructure methods are mostly nonlinear in the potential matrix elements. It was, however, pointed out that a given set of band energies can be fitted by widely different potential parameters in semiempirical models, permitting almost any value of b within the simple VCA approach [37]. The origin of optical bowing is widely associated with disorder in an alloy. The effect of alloy disorder alone may however be insufficient to describe bowing. In a firstprinciples approach evidence was given for three contributions to b in tetrahedrally coordinated compound semiconductors: A modification of the band structure
4.1 Bulk Properties
133
due to the change of the lattice constant, a relaxation of the anioncation bond length in the alloy, and a contribution of chemical electronegativity due to charge exchange in the alloy [37]. Respective calculations provided a good description of bowing parameters experimentally obtained from zinc chalcogenes. Bowing of nitride alloys is reported in [30, 39–41].
4.2 Band Offsets Epitaxy allows to produce a pseudomorphic, atomically sharp transition from one solid to another. The intimate contact of two solids with different electronic properties forms a heterojunction. At the interface the electronic bands of the solids align on a scale of atomic nearestneighbor distances. In addition, transfer of charges from one solid to the other and charge accumulation at the interface may lead to an electrostatic bending of the bands on a larger scale. The band alignment is of basic technological importance, because it controls the transport and confinement of charge carriers and hence the properties and performance of (opto)electronic devices. Calculation and measurement of band offsets (also termed band discontinuities, band lineups or band alignments) are difficult, and a thorough understanding of the physics of semiconductor bandalignment is still missing. In the following we focus on the technologically important contact between two semiconductors. The junction between a semiconductor and a metal is treated in Sect. 10.3. Various types of band alignments may occur at semiconductor junctions, usually labeled type I and type II. In a type I alignment the bandgap of one semiconductor lies completely within the bandgap of the other. If such straddled type I offset is applied to a BAB double heterostructure, electrons and holes can both be confined in material A with the smaller bandgap, see Fig. 4.9a. This feature is often employed in lowdimensional structures like quantum wells to tailor electronic properties, cf. Sect. 4.3. If the offset in the valence band and the conduction band has the same sign for an electron transfer from material A to B the band alignment is referred to as type II. In a BAB double heterostructure with such a staggered band lineup either electrons or holes are confined in material A. In Fig. 4.9b a lower conduction band edge in material A leading to electron confinement is assumed. When the bandgaps of the two semiconductors do not overlap at all a misaligned (or broken gap) configuration occurs. Such alignment appears if in Fig. 4.9 E v A lies above E c B or E c A lies below Ev B . A case analogous to the broken gap configuration occurs if a junction is formed by a semiconductor and a zerogap semiconductor like, e.g., HgTe. This kind of alignment is occasionally referred to as type III. The type of band alignment forming in a semiconductor heterostructure depends on the position of the respective band edges. The prediction of this alignment is not trivial, because there exists no natural common reference energy. Such reference should be a property of a bulk crystal. Much theoretical and experimental work was devoted to predict or measure offsets within the required precision of about 0.1 eV
134
4 Electronic Properties of Heterostructures
(b ) B
A
B Ec Ec
EgB
EgA Ev
Ev
Electron energy
Electron energy
(a)
B
A
B Ec Ec
EgB EgA Ev
Ev
x
x
Fig. 4.9 Alignment of band edges in a type I and b type II double heterostructures built from a smallbandgap semiconductor A with a small extension along the spatial coordinate x and a widebandgap semiconductor B
or better. A comprehensive review as of 1991 was given in [42]. In the following we will consider some rules and more recent theoretical and experimental results.
4.2.1 ElectronAffinity Rule If two semiconductors A and B are combined their Fermi levels E F tend to align by transferring electrons from the solid with higher Fermi energy to the other. In the ideal case the vacuum level E vac is a common reference energy [43, 44]. In the framework of this socalled electronaffinity rule the alignment of the conduction bands follows from their electron affinities eχ = E vac − E c , E c being the band edge of the (lowest) conduction band and e the elementary charge, see Fig. 4.10. The discontinuity of the conduction band at the interface is then E c = e(χ A − χ B ),
(4.27)
and the corresponding offset of the (uppermost) valence band is given by
E v = e(χ A + E g A ) − e(χ B + E g B ),
(4.28)
E g being the bandgap. Theoretical calculations suggest that only a single atomic layer away from the interface the electronic structure in a heterostructure becomes nearly bulklike. The offset can hence be well assumed as being abrupt as illustrated in Fig. 4.10b. This does not apply for the longrange band bending (µm scale) originating from the electron
4.2 Band Offsets
135
(a)
(b) Semiconductor A Semiconductor B
e
e
B
A
EcB Ec
EcA EFA EvA
Evac
Evac
EFB Ev
EvB x
Evac
Electron energy
Electron energy
Evac
e
B
EcB e
A
Ec EcA EFA EvA
EFB EvB Ev x
Fig. 4.10 Band alignment at a heterointerface between two semiconductors in the ideal case in absence of dipoles and interface states. a Before and b after formation of a heterojunction in thermal equilibrium
transfer for aligning E F . Therefore doubleheterostructures with semiconductors of small dimensions (nm scale) embedded in other semiconductors may be represented by flat bands as depicted in Fig. 4.9. The electronaffinity rule outlined above provides in many cases a good estimate of the band alignment of the heterointerface in organic semiconductors; this topic is discussed in Sect. 5.3.1. A drawback of the classical electronaffinity rule is that the reference energy E vac is not a bulk property. The electron affinity eχ is determined by experiments involving the surface. Therefore the structure of the surface and related charges may strongly affect the potential. Consequently the vacuum level is not a reliable reference.
4.2.2 CommonAnion Rule Heterostructures are often fabricated from compound semiconductors like ZnS and ZnSe. In such cases a heuristic rule called commonanion rule has been applied to estimate whether the offset essentially occurs in the valence band or in the conduction band. The rule arises from the evidence that the valenceband states are essentially derived from pstates of the anions in spbonded AB compounds. The energy of the valenceband edge on an absolute scale is therefore expected to be basically determined by the valence electrons of the anions. Consequently the valenceband offset should be governed by the difference in anion electronegativity of the two semiconductors. A heterojunction with a common cation like Zn in a ZnS/ZnSe contact is expected to induce merely a small offset in the conduction band, leaving the majority of the bandgap difference for an offset in the valence band. Early models of band alignments largely complied with the commonanion rule [45, 46]. The models did not include dorbitals of cations. Deviations from the commonanion rule were basically ascribed to contributions of these orbitals to the valence band [47]. It must,
136
4 Electronic Properties of Heterostructures
however, be noted that the rule fails in many cases. A basic shortcoming is the fact that the rule does not pay attention to an interface dipole formed from contributions of both, anions and cations [48].
4.2.3 Model of Deep Impurity Levels Experiments indicate the existence of some “natural” reference potential which adopts the role of the vacuum level in the classical approach. An indication for such a reference is the transitivity rule for the valenceband offset found for some combinations of semiconductors A, B, and C, i.e., E vAC = E vAB + E vBC [49, 50]. Moreover, deep level impurities were found to have similar energy differences in different semiconductors. The observation was used for an empirical description of heterostructure bandoffsets. Transition metals like Fe form localized impurity states in semiconductors. They often possess several charge states separated by a fraction of the energy gap of the host crystal. A change of the impurity’s charge state implies the transfer of a charge carrier from or to the host. This allows to determine the impurity level with respect to the band edges of the host material. Comparing such levels for a series of impurity ground states in various semiconductors yields an apparent similarity of both ordering and relative energy separations, cf. Fig. 4.11. The levels of transitionmetal impurities are not pinned to either band edge like those of shallow impurities used as donors or acceptors (Sect. 10.1). This finding leads to the approach to take these levels within the bulk crystals as a reference for the alignment of the band edges in a heterojunction [51, 52]. The offset of the valence band at the interface E v is then given by the difference in the energy level positions of a given impurity in the two semiconductors forming the heterojunction. The constant separation of deep cationic impurity levels from the vacuum level was attributed to their antibonding character [52]. The energy levels of the transitionmetal impurities depicted in Fig. 4.11 refer to a charge transition of an acceptor from a singly negative charge to the neutral state (−/0). The measured transition energies were vertically shifted, so as to minimize the overall deviations, yielding the relative positions of the valenceband edges [51]. Positions of the conductionband edges were experimentally obtained from lowtemperature energy gaps. It should be noted that the method is restricted to heterojunctions formed by pairs of isovalent compound semiconductors, e.g., among III–V or among II–VI compounds, to ensure an electrically neutral interface without a dipole moment. A comparable universal alignment of deep impurity levels as described above was also reported for hydrogen [53]. By computing the position of the Fermi energy where the stable charge state of interstitial hydrogen changes from the H+ donor state to the H− acceptor state, predictions of band alignments for a wide range of host zincblende and wurtzite compound semiconductors were given.
4.2 Band Offsets
137
Fig. 4.11 Average energy levels of transition metal impurities forming deep acceptor states in GaP, InP, and GaAs, drawn with respect to the GaP valenceband edge. After [51]
conduction bands
2.4
GaP
0.50 eV
2.0
GaAs 0.76 eV
InP
E n e rg y (e V )
1.6
1.2
E(GaP) E(InP)+0.17 eV E(GaAs)+0.33 eV
Cr Fe
0.8
Ni Mn
Co
0.4 0.33 eV 0
0.17 eV valence bands
Cu GaAs InP GaP
4.2.4 InterfaceDipol Theory The dominant role of charge accumulation at the interface rather than the effect of bulk properties was emphasized in the interfacedipol theory for the prediction of heterojunction bandoffsets [54]. The approach was also applied to the theory of Schottky barrier heights at a metalsemiconductor interface [55] considered in Sect. 10.3.2. The initial point of the approach is that the discontinuity at a semiconductor interface induces electronic states in the bandgap of at least one semiconductor. The formation of such states is illustrated in Fig. 4.12 for the artificial case of a band discontinuity created in a homogeneous semiconductor by an external step potential. States lying near the conductionband edge at side A of the interface have exponentially decaying tails into side B. At side B they lie in the gap of the semiconductor. Any state in the gap has a mixture of valence and conductionband character. Occupying such state leads locally to an excess charge, according to its degree of conduction character. Filling a state which lies near the top of the gap gives a large excess charge of almost one electron due to a large conduction character. Leaving that state empty gives an only slight charge deficit. Conversely filling a state near the bottom of the gap at side A results in a slight excess charge in proportion to its little conduction character, while leaving it empty leads to a charge deficit of almost one electron. Changing the band lineup hence induces a net dipole. The external potential assumed to create the potential step in Fig. 4.12 leads to an electron deficit at side B and an electron excess at side A of the interface. The resulting dipole tends to reduce the offset, i.e.,
4 Electronic Properties of Heterostructures
Electron energy
138
A
B +++ +

x Fig. 4.12 Scheme of band alignment at an interface artificially induced in a homogeneous semiconductor. (+) and (−) represent net charges of unoccupied states with electron deficit and occupied states with electron excess, respectively. After [54] Table 4.7 Differences of midgap energies E B,A − E B,B according to the interfacedipol theory and experimental valenceband discontinuities for some semiconductor heterojunctions. Data from [54] Heterojunction E B,A − E B,B (eV) E v,exp (eV) A B Si GaAs GaAs
Ge Ge InAs
0.36 − 0.18 = 0.18 0.70 − 0.18 = 0.52 0.70 − 0.50 = 0.20
0.20 0.53 0.17
the potential step is screened. By the action of the induced local charges the step is reduced by a factor of ε, the bulk dielectric constant. The heterojunction of two different semiconductors is described analogous to the case considered above. Local states in the gap of one or both semiconductors lead to a dipole which screens the potential step and drives the lineup towards a value which minimizes the dipole. The zerodipole lineup condition is not obvious. An effective midgap energy E B for each semiconductor is introduced at which the gap states, on the average, cross over from valence to conduction character [54]. States at E B are nonbonding on the average, the respective position is calculated from the band structure [55]. For a heterojunction E B plays a role in analogy to the Fermi energy in metals: E B is aligned for the respective semiconductors. Results of the interfacedipol theory are given in Table 4.7 for some heterojunctions, calculated values are claimed to be typically accurate to ∼0.1 eV. Extensions of the interfacedipol theory distinguish between the longrange tails of the gap states considered above and polarization of the bonds which form the interface. More recently the approach of branchpoint energies was also applied to zincblendetype nitrides [56, 57].
4.2 Band Offsets
139
4.2.5 ModelSolid Theory The more recently widely applied modelsolid theory emulates the classical electron affinity rule illustrated in Fig. 4.10 by constructing a local reference level and avoiding dipoles. Within this approach the charge density in a semiconductor is composed by a superposition of neutral atoms [58]. The potential outside each such sphere goes exponentially to zero. This zero is taken as reference level. The construction leads to a welldefined electrostatic potential with respect to the vacuum level in each atom. By superposition the average electrostatic potential in a model solid composed of such atoms is hence specified on an absolute energy scale. The electron configuration of an atom in the solid is determined from a tightbinding calculation. This leads for, e.g., one Si atom in a silicon bulk crystal to 1.46s and 2.54 p electrons, meaning that a part of the two s electrons of a Si atom are excited into the p band [58]. The result of the calculation is the position of the valence band on some absolute energy scale, allowing to relate it to the respective value of another semiconductor. For semiconductors with zincblende or diamond structure the value E v,av represents an average of the heavy hole, light hole and splitoff hole valencebands. Spinorbit effects are added a posteriori. Once E v,av values are computed separately for a pair of semiconductors, their band discontinuities can be predicted for an unstrained heterojunction with a perfect interface, i.e., an abrupt change in the type of material without displacements of atoms from their ideal positions. The result of a calculation of the average valenceband energy E v,av on an absolute scale in the framework of the modelsolid theory is given in Fig. 4.13 for some unstrained semiconductors. Data are included in Table 4.1 along with the effect of strain. Data of E v,av for alloys of III–V semiconductors are reported in [59].
4.2.6 Offsets of Some Isovalent Heterostructures For many isovalent combinations of semiconductors with equal valence of the atoms on the two sides of a common junction the contribution of the interface dipole is not very large. In such cases the valenceband energy may be considered a bulk property on either side, and the simple difference of electron affinities (4.28) is a reasonable approximation to evaluate the valenceband offset. Data for a number of technologically important III–V compound semiconductors are summarized in Fig. 4.14. The values do not include effects of strain. Furthermore, the valenceband offset is taken to be independent of temperature, basically due to a lack of reliable data. Valenceband offsets at a junction of two semiconductors of Fig. 4.14 are given by the energy difference of their plotted band positions. The same applies for the offset in the direct conduction band. The direct bandgap energy is represented by the vertical lines and is given for low temperature (0 K). Note that some of the binaries have a smaller indirect bandgap and that the three nitrides usually crystallize in the wurtzite structure.
140
4 Electronic Properties of Heterostructures Si Ge
GaAs InAs GaSb InSb AlP AlAs GaP AlSb InP
ZnSe ZnTe HgTe ZnS CdTe
IVIV
IIIV
IIVI
Energy (eV)
4
Ec 6
Ev,av 8
10
Fig. 4.13 Average valenceband energy E v,av of unstrained semiconductors on an absolute scale resulting from the modelsolid theory. Experimental values of bandgap energies are used to depict the conductionband energy E c , black and gray lines at the bottom of the conduction bands denote direct and indirect conductionband edges, respectively. Data taken from [10] 3
AlN AlP
2
Band offsets (eV)
Fig. 4.14 Valenceband offsets (open circles) of binary semiconductors with zincblende structure, plotted with respect to the valenceband maximum of InSb. Filled circles indicate corresponding offsets of the lowest direct conduction band. From [3]
1
GaAs
GaN
0
AlSb
AlAs
InN
1
GaSb
InSb GaP
InP
InAs
2 Conduction band
3 4 4.0
Valence band
4.5
5.0
5.5
6.0
6.5
Lattice constant (Å)
4.2.7 Band Offset of Heterovalent Interfaces Models considered above in Sects. 4.2.1–4.2.5 considered abrupt interfaces and derived band offsets without detailed knowledge of the atomic interface structure. Theoretical work showed that the valenceband offset may actually depend on the microscopic arrangement of atoms at the interface [60]. A particularly strong effect was experimentally found for heterovalent interfaces, where—in contrast to isovalent systems—the atoms at the two sides of the interface have different chemical valence. We will consider the wellstudied ZnSe/GaAs interface in more detail. The
141
1.6
(a)
ZnSe/GaAs(001)
Ga 3d
R Zn/Se (arb. u.)
Photoemission Intensity (arb. u.)
4.2 Band Offsets
Zn 3d BPR=0.1
(b)
1.2 0.8 Substrate type p+ n+ p n undoped n
0.4
BPR=10 4
2
0
2
4
6
Energy (eV)
8
10
12
0.0
0.6
0.8
1.0
1.2
Ev (eV) E
Fig. 4.15 a Xray photoemission spectra of ZnSe/GaAs heterojunctions grown with different Zn/Se beampressure ratios (BPR). The energy origin was set to the center of the Ga 3d corelevel emission. b Experimental valenceband offsets for ZnSe/GaAs(001) interfaces with different type of substrate doping versus Zn/Se ratio obtained from integrated XPS emission intensities for 0.3 nm thick ZnSe c 1994 APS layers. Reproduced with permission from [66],
same findings were observed in the similar system ZnSe/AlAs [61] and many other heterovalent interfaces. Reviews with an emphasis on theoretical aspects are given in [62, 63]. ZnSe and GaAs have both zincblende structure and are well latticematched with a misfit below 0.5%. Due to the heterovalent nature of the II–VI and the III–V material an abrupt interface builds a strong dipole moment. Calculations indicate that such an abrupt transition at a heterovalent interface is energetically unstable and structures consisting of one or two intermixed layers are more favorable [60, 64, 65]. Experimental evidence for the impact of growth conditions on the band offset of the ZnSe/GaAs interface are given in Fig. 4.15. Using molecular beam epitaxy (Sect. 11.3) ZnSe layers were epitaxially grown on (001)oriented GaAs substrates [66, 67]. Nonstoichiometric growth conditions were applied by controlling the composition via the Zn/Se beampressure ratio (BPR). The valenceband offset at the interface was measured using Xray photoemission (XPS) related to the Ga 3d and the Zn 3d core levels, see Fig. 4.15a. The observed Zn 3d corelevel separation with respect to the ZnSe bulk value (difference between dotted and solid lines in Fig. 4.15a) gives directly the valenceband offset across the heterojunction. The corresponding Zn/Se ratio at the interface RZn/Se was determined from the ratio of the integrated 3d corelevel emission intensities related to those of Zn and Se (Se not shown) for thin ZnSe layers. The measurements given in Fig. 4.15b clearly evidence a monotonous increase of the valenceband offset E v with increasing Zn/Se ratio from 0.58 eV (Serich) to 1.2 eV (Znrich). The apparent dependence of the band offset from the interface stoichiometry can be understood in terms of differently mixed layers formed at the interface for varied growth conditions [65, 66]. Let us consider the sp 3 bonds of a binary zincblende semiconductor like GaAs. Each atom has 4 hybrid orbitals directed to the surrounding
142
4 Electronic Properties of Heterostructures
four nearest neighbors (Fig. 2.4a). Each of these bonds comprises 2 electrons. The primitive unit cell of GaAs contains one cation (Ga) and one anion (As) with a total number of 8 valence electrons: 3 from the Column III element Ga and 5 from the Column V element As. Each atom can be considered to donate one quarter of its valence electrons to its four bond orbitals. The number of valence electrons in one orbital referring to one Ga atom is then 3/4, and the corresponding number per orbital of an As atom is 5/4. One GaAs bond thus contains 3/4 + 5/4 = 2 electrons. The same applies for the II–VI semiconductor ZnSe: One ZnSe bond contains 2/4 + 6/4 = 2 electrons. At the heterovalent interface between GaAs and ZnSe we find GaSe or ZnAs bonds. A GaSe bond contains 3/4 + 6/4 = 2 14 electrons, i.e., it has an excess of a quarter electron. Such a bond acts like a donor. Likewise a ZnAs bond has a quarter electron deficiency and acts like an acceptor. This unbalanced charge generates the dependence of the valence band offset from the stoichiometry at the interface. An abrupt interface contains either solely GaSe bonds or ZnAs bonds. In both cases a strongly localized, twodimensional charge is created at the interface. Such a charge is connected to a high interface energy. Consequently the abrupt interface is thermodynamically unstable against intermixing [65]. Interface layers with a mixture of atoms from both semiconductors contain both kind of bonds; they accumulate less charge and are more stable. Figure 4.16 illustrates two examples of atomic configurations at intermixed heterovalent ZnSe/GaAs interfaces. The total charge of an intermixed interface is reduced by charge transfer from donorlike to acceptorlike bonds. An interface with an equal number of uneven bonds is compensated. There may, however, remain a strong dipol moment at the interface: If the intermixed interface is built by a single layer of 50% Ga and 50% Zn cations (Fig. 4.16a) the acceptorlike ZnAs bonds lie towards the ZnSe and the donorlike GaSe bonds towards the GaAs. Note that the dipole moment is reversed, if such singlelayer interface is formed on the anion sublattice (50% As + 50% Se, not shown in Fig. 4.16): The acceptorlike ZnAs bonds then lie towards the GaAs and the donorlike GaSe bonds towards the ZnSe. The valenceband offset is increased in the first case and decreased in the latter. Calculated values are +1.75 eV and +0.72 eV, respectively, when going from ZnSe to GaAs [65]. Formation of these mixings is favored in more Znrich growth conditions and Serich conditions, respectively, and describes correctly the experimentally observed tendency shown in Fig. 4.15. The average of the two offsets (1.25 eV) is close to the experimental value of 1.22 eV [68]. This indicates the possibility to compensate the dipole moment, namely by interface layers comprising more than a single layer. An interface consisting of an intermixed cation layer and an intermixed anion layer is illustrated in Fig. 4.16b. The Ga atoms and the Se atoms in the interface doublelayer create a quarter charge excess each, while the two AsZn bonds have a quarter charge deficiency each. The dipole moment in this intermixed double layer is hence fully compensated. It should be noted that the dipole moment is also compensated in average if small domains of singlelayer interfaces of both polarities occur in a ratio of 1:1 [65].
4.2 Band Offsets
143
(b)
(a) Ga
As
As
Ga
Ga
As
As
Ga
Ga
As
As
Ga
Ga
As
As
Ga
Ga Zn As Se
Se As Ga Zn
Ga As Se
Se As Ga Zn
Ga Zn As Se
Se As Ga Zn
Ga As Se
Se As Ga Zn
Ga As
As Ga
Ga As
Zn
Ga
Ga Zn
Ga
As Se
As
Zn
Ga
Se As Ga Zn Se As
As Se
As
Ga As
As Se
Se As
Ga As
Ga
Ga Zn Se As Ga Zn Se As
As Se
Ga Zn
[110] [001]
GaAs
inter ZnSe face
GaAs
interface
ZnSe
Fig. 4.16 Schematic arrangement of atoms at the heterovalent ZnSe/GaAs interface, viewed along the [110] direction. Each atom is bond by two bonds in the figure plane and by two bonds, which are directed out of and into the figure plane—the horizontal double lines. a Interface with a single intermixed cation layer comprising 50% Zn and 50% Ga. b Interface with an intermixed double layer containing 75% As and 25% Se anions, and 25% Ga and 75% Zn cations
The ZnSe/GaAs interface is well latticematched. Elastic relaxation as discussed in Sect. 2.2 does hence not play a significant role, and the effect was not considered here. Atomic relaxation does, however, play a crucial role in more mismatched heterostructures like GaN/SiC(001) [69]. Isovalent heterojunctions have, in contrast to the heterovalent interfaces discussed above, band offsets which are almost independent of the local atomic arrangement. This commonly accepted conclusion was initially established for commonion systems, and later generalized [70]. It should be noted that intrinsic defects like antisites may limit the validity of this general statement and must be taken into account in case of low formation energies. The same applies for the formation of heterovalent interlayers at the interface.
4.2.8 Band Offsets of Alloys The observation of a constant energy with respect to the vacuum level of deep transitionatom impurities according to the model of deep impurity levels (Sect. 4.2.3) was also used to measure the change of valenceband energy E v in alloys. Experi
144
0.0
Valenceband offset (eV)
Fig. 4.17 Valenceband offset of alloy semiconductors, plotted with respect to the valenceband maximum of InSb. Vertical lines mark common substrate materials, points signify offsets for binaries and latticematched ternary alloys. From [3]
4 Electronic Properties of Heterostructures
GaAs0.5Sb0.5 GaIn0.47As0.53
GaAs0.08Sb0.92 AlAs0.08Sb0.92
InAs
0.5 GaAs Ga0.51In0.49P
1.0
GaSb AlSb
InAs0.91Sb0.09 InSb0.31P0.69 Al0.48In0.52As
InP
AlAs
1.5
Al0.52In0.48P
5.6
5.8
6.0
6.2
Lattice constant (Å)
ments reveal mostly a linear dependence of the valenceband maximum in the alloy with respect to the deep levels for varied composition x. Studied materials are, e.g., Ga1−x Alx As:Fe [51, 71], Ga1−x Alx As:Cu [72], GaAs1−x Px :Cu [73], In1−x Gax P:Mn [74]. The slope of the linear dependence was found to be largely independent from the impurity. Such linear variation may also be inferred from the interfacedipol theory (Sect. 4.2.4), where the effective midgap energy E B of an alloy was estimated as a linear interpolation from the pure semiconductors [48]. Valenceband offsets of some zincblende semiconductoralloys are summarized in Fig. 4.17 for composition parameters matching the lattice constants of the common substrate materials GaAs, InP, InAs, and GaSb.
4.3 Electronic States in LowDimensional Structures The unique properties of lowdimensional structures originate essentially from the modification of the electronic densityofstates (DOS) produced by the confinement of charge carriers. To track such modification for the reduction of dimensionality from a threedimensional (3D) bulk crystal to a 0D quantum dot we first recall the origin of 3D DOS and then consider the effect of potentials confining the mobility of charge carriers gradually to two, one, and eventually zero dimensions. Electronic properties of the solid are described in the framework of the effectivemass approximation by applying effective carrier masses and the relative permittivity as characteristic parameters.
4.3 Electronic States in LowDimensional Structures
145
4.3.1 Dimensionality of the Electronic DensityofStates We first describe the energy of a single quasifree electron confined in a bulk crystal by a simple square potential W given by the dimensions of the crystal L x , L y , and L z . The periodic potential of the atoms which leads to the band structure is neglected. It may be treated in a second step as a perturbation of W . If we assume W being 0 inside the crystal and a constant W0 > 0 outside we obtain energy and eigenstates of the electron inside the crystal by solving the Schrödinger equation 1 ∂2 1 ∂2 2 1 ∂ 2 + ∗ 2 + ∗ 2 ψ(r) = Eψ(r) (three dimensions). − 2 m ∗x ∂ x 2 my ∂y m z ∂z (4.29) The quantities m ∗ are the electron’s effective masses along the three spatial directions x, y, z. Using periodic boundary conditions like ψ(x ± L x , y, z) = ψ(x, y, z) we obtain the solutions of (4.29) given by plane waves ψk (r) with eigenenergies E k : 1 ψk (r) = √ ei(kx x+k y y+kz z) , V 2 k 2y 2 k z2 2 k x2 Ek = + + . 2m ∗x 2m ∗y 2m ∗z
(4.30) (4.31)
In (4.30) V = L x × L y × L z is the volume of the bulk crystal. If we apply the boundary conditions to (4.30) we yield allowed values for k, 2π n z , n x , n y , n z = 0, ±1, ±2, . . . . Lz (4.32) Each electron state is hence described by discrete values of k as illustrated in the scheme of the reciprocal space depicted in Fig. 4.18a. Each state marked by a dot in the figure is occupied by 2 electrons with opposite spin. The spacing between allowed adjacent values along k x is 2π/L x . Since the crystal dimensions L x , L y , L z are macroscopic quantities, a finite region of kspace contains a very high number of dense lying allowed states. k and likewise E k are therefore quasicontinuous quantities. The number of allowed kvalues per unit volume of k space, i.e., the density of states in k space, is given by the constant quantity V /(2π )3 . The electronic density of states g(E)—expressed in units of m−3 × J−1 or cm−3 × −1 eV —is obtained from the number of electron states d N per unit volume V and per energy interval d E, 1 dN . (4.33) g(E) = 2 × V dE kx =
2π nx , Lx
ky =
2π ny, Ly
kz =
The factor 2 in (4.33) accounts for the spin degeneracy, allowing for a twofold occupancy of each state. We obtain dN from the volume in k space between two planes of constant energy at E and E + d E multiplied by the constant density of
146
4 Electronic Properties of Heterostructures
Fig. 4.18 a Cross section of k space in the k x –k y plane. b Values of E(k x ) which fulfill the boundary condition for a quasifree electron in a solid with finite dimension L x
(a)
ky
k
dk kx
(b)
E(kx)
kx
states in k space. Such a volume is illustrated in Fig. 4.18a by the spherical shell of thickness dk. We note that the volume increases for a given d E (or correspondingly dk) with the same power as the area of a sphere in k space increases as k augments. For a quasifree electron we obtain dN =
V (2π )3
E+d E E
d 3k =
V × 4π k 2 dk. (2π )3
(4.34)
To keep expressions simple we assume an isotropic medium with equal electron masses m ∗ and equal crystal dimensions L in all three spatial directions. We then may put E = (2 /2)(k x2 /m ∗x + k 2y /m ∗y + k z2 /m ∗z ) = (2 /2m ∗ )k 2 . From this we obtain k = √ (2m ∗ /2 )1/2 E and kdk = (m ∗ /2 )d E, yielding for (4.34) V 2m ∗ 3/2 √ dN = Ed E (isotropic medium). 4π 2 2
(4.35)
Inserting (4.35) into the definition (4.33) we obtain the squareroot dependence of the electronic DOS for bulk crystals 1 2m ∗ 3/2 √ g(E) = E (three dimensions). 2π 2 2
(4.36)
4.3 Electronic States in LowDimensional Structures
147
We now consider the twodimensional case by assuming an additional contribution to the potential W (z) which confines the mobility of the electron to the x y plane. Within this twodimensional plane it still moves quasifree. The electron states are now described by the Schrödinger equation 2 1 ∂2 1 ∂2 1 ∂2 + ∗ 2 + ∗ 2 + eW (z) ψ(r) − 2 m ∗x ∂ x 2 my ∂y m z ∂z = Eψ(r) (two dimensions).
(4.37)
Equation (4.37) can be separated into two equations describing movements either within the x y plane or perpendicular by using the approach for the solution 1 ψk (r) = √ ei(kx x+k y y) ϕn (z). V
(4.38)
The planewave term in ψk (r) is analogous to the threedimensional case described by (4.30) and yields correspondingly the eigenvalues Ex y =
2 k 2y 2 k x2 + . 2m ∗x 2m ∗y
(4.39)
For the z direction we obtain −
2 1 ∂ 2 + eW (z) ϕn (z) = E n ϕn (z). 2 m ∗z ∂z 2
(4.40)
The eigenvalues E n depend on the characteristics of the potential W (z). If we assume a square potential with infinite barriers separated by a spacing L z the eigenvalues follow from the condition for allowed waves L z = nλz,n /2, n = 1, 2, 3, . . . . Putting k z,n = 2π/λz,n the eigenvalues are given by
E z,n =
2 nπ 2 , n = 1, 2, 3, . . . . 2m ∗z L z
(4.41)
We note that the energy of the ground state with the quantum number n = 1 is increased by the quantization energy E = E z,1 . The eigenvalues of (4.37) are given by the sum of (4.39) and (4.41), E = E x y + E z,n . The band scheme E(k) along k x and k y therefore consists of a series of parabola, each labeled by a particular value of n. The parabola are also referred to as subbands. The twodimensional electronic DOS follows from the equidistant states in k space similar to the threedimensional case. For an area L x × L y the twodimensional density of states in k space is given by L x L y /(2π )2 . The volume of a spherical shell
148
4 Electronic Properties of Heterostructures
3D
2D
g(E)
g(E)
g(E)
Ec
E
Ec
0D
1D
E
g(E)
Ec
E
E
Fig. 4.19 Electronic density of states g(E) in isotropic semiconductors (red) with different dimensionalities: 3D bulk semiconductor, 2D quantum well, 1D quantum wire, and 0D quantum dot. The environment drawn in blue provides potential barriers for the charge carriers. E C denotes the conductionband edge in the semiconductor
in k space is replaced in 2D by the area of a circular ring bounded by E(k) = const and E + d E = E(k + dk) = const. We assume again an isotropic medium and use the isotropic energy dispersion E(k) = (2 /2m ∗x y )k 2 . In analogy to (4.34) we obtain dN =
L2 (2π )2
E+d E
d 2k =
E
L2 2π kdk (isotropic medium). (2π )2
(4.42)
The general expression for the twodimensional DOS g(E) is obtained by inserting this into the definition (4.33), yielding for the isotropic DOS of the nth subband gn =
m ∗x y π 2
= const (two dimensions).
(4.43)
The twodimensional DOS in (4.43) is expressed in units of cm−2 × eV−1 . The total electronic DOS follows from the sum of all subband contributions, which all have the same magnitude given by (4.43): g(E) = gn . This results in the staircaselike function of the total DOS for a twodimensional (2D) semiconductor illustrated in Fig. 4.19 and expressed by
g(E) =
gn =
m ∗x y π 2
Θ(E − E n ) (two dimensions),
(4.44)
n
Θ(E − E n ) being the unit stepfunction. The subbands are consecutively occupied as the energy is increased.
4.3 Electronic States in LowDimensional Structures
149
The onedimensional case follows from the twodimensional case by an additional confinement W (y). This leads to a quasifree mobility only along the x axis. The energies along the y and z axes are quantized, and the subbands have two corresponding indices l and n. Analogous to (4.39) and (4.41) we may write E = El,n =
2 2 k x2 2 + l 2m ∗x 2m ∗y
π Ly
2 + n2
2 2m ∗z
π Lz
2 (one dimension). (4.45)
The onedimensional electronic DOS is obtained from a onedimensional “volume” element in k space simply given by dk, yielding for the subband l, n gl,n (E) =
m ∗x 1 (one dimension). 2π 2 2 E − El,n
(4.46)
The onedimensional DOS in (4.46) is expressed in units of cm−1 × eV−1 . The total DOS is again given by the sum of all subband contributions, g(E) = l,n gl,n (E). The resulting function of the onedimensional (1D) semiconductor is illustrated in Fig. 4.19. Note that the peaks are not necessarily equidistant since L y and L z are independent. Adding a further confining potential W (x) to the onedimensional semiconductor leads to the zerodimensional case. The mobility is now restricted in all three spatial dimensions. Accordingly the energy is quantized in all directions, and from (4.45) follows
E = E j,l,n =
2 j 2 π 2 l2 n2 (zero dimensions). + + 2 m ∗x L 2x m ∗y L 2y m ∗z L 2z (4.47)
The zerodimensional electronic DOS is a sum of δ functions given by g(E) = 2δ(E − E j,l,n ). The function is shown in Fig. 4.19. Like in the twodimensional case the peaks are not necessarily equidistant.
4.3.2 Characteristic Scale for Size Quantization We considered above the modification of the electronic densityofstates for solids of reduced dimensionality. What is the characteristic scale required for the size quantization to become observable in experiment? Besides the size of the solid it is related to the effective mass of the considered charge carriers and to the temperature. For a
150
4 Electronic Properties of Heterostructures
quasifree charge carrier with effective mass m ∗ size quantization gets distinguishable if the motion is confined √ to a length scale in the range of or below the de Broglie wavelength λ = h/ p = h/ 2m ∗ E. Assuming a room temperature thermal energy E = (3/2)kB T = 26 meV and an effective mass of one tenth of the free electron mass, a typical length is in the 10 nm range. Optical properties of semiconductors are often dominated by excitons. They consist of an electron and a hole in close proximity which attract each other via Coulomb interaction and form hydrogenlike bound states, cf. Sect. 5.1.3 [2]. The relevant length scale of these twoparticle states is the exciton Bohrradius. The exciton Bohrradius is given by
aX =
h 2 εε0 , π μe02
(4.48)
where ε, ε0 , μ, and e0 designate the relative permittivity of the solid and that of vacuum, the reduced mass of the exciton and the electron charge, respectively. The reduced mass of the exciton is defined by 1/μ = 1/m ∗e + 1/m ∗h . The hole mass m ∗h is often much heavier than the electron mass m ∗e , leading to a reduced mass close to m ∗e . The value of the exciton Bohrradius is related to the binding energy (also termed Rydberg constant) of the exciton
EX =
μe04 . 8h 2 (εε0 )2
(4.49)
The product aX × E X is constant for threedimensional excitons. The relation remains a good estimate also for twodimensional excitons [75]. Values for some semiconductors are given in Table 4.8. A typical length to observe size quantization for excitons is also in the 10 nm range. It must be noted that exciton bindingenergy and Bohr radius are significantly modified by a spatial localization [75]. Sizequantization effects were observed at surfaces and in thin layers of both, metals and semiconductors [81]. A review on early work was given in, e.g., [80]. In the following we will focus on semiconductor heterostructures. Clear quantumsize effects are particularly observed in GaAsbased heterostructures. Their electronic properties can be described almost purely quantum mechanically using the effectivemass approximation, with constituent materials represented by a few band parameters.
4.3 Electronic States in LowDimensional Structures
151
Table 4.8 Exciton Bohr radius aX and binding energy E X of excitons in some direct semiconductors with zincblende (ZB) or wurtzite (W) structure. A, B, and C in wurtzite material refer to the three valence bands Semiconductor aX (Å) E X (meV) GaAsa InAsd InPb ZnTec ZnSec ZnSc ZnOd
ZB ZB ZB ZB ZB ZB W
GaNe
W
a Reference
115 494 113 11.5 10.7 10.2
4.7 1.0 5.1 13 19.9 29 60 (A) 57 (B) 21 (A) 21 (B) 23 (C)
[76], b Reference [77], c Reference [1], d Reference [78], e Reference [79]
4.3.3 Quantum Wells A quantum well is made from a thin semiconductor layer with a smaller bandgap energy clad by semiconductors with a larger bandgap forming barriers. Usually the same barrier material is used in such double heterostructure leading to a symmetrical square potential as illustrated in Fig. 4.9. The confinement is given by the band offsets. Since the potential is no longer infinite as assumed to obtain the eigenvalues (4.41) the wave functions of a confined charge carrier now penetrate into the barriers. For finite barrier energy W (z) = W0 the eigenvalues are obtained from a transcendental equation m w E n L 2z m w W0 − E n = tan (4.50a) 22 mb En for even wave functions, i.e. even values of quantum numbers n, and cot
m w E n L 2z 22
=
m w W0 − E n mb En
(4.50b)
for odd wave functions, i.e., odd n [82]. m w and m b are the effective masses of the charge carrier in the well and the barriers, respectively, and L z is the well width. Numerically obtained solutions are given in Fig. 4.20 [83]. Energies in the figure are scaled in units of the groundstate energy E 1 of a well with infinite barriers, cf. (4.41). The gray line signifies the top of the well at E = W0 . Discrete bound states are found for E < W0 , while continuum states exist for E ≥ W0 . We note that the number of bound states of the confined particle decreases as W0 decreases. Furthermore, the
4 Electronic Properties of Heterostructures
2
7
2 2
40
7
6
E (h
E ( h 2 π 2 / (2m* L2z) )
50
/(2m*Lz ))
152
30
2 2
W 0 (h
6
2
/(2m*Lz)
5 5
20
4 10
0 1 10
3 2 1 10 100
4 3 2 1 100 1000
W0 ( h 2 π 2 / (2m* L2z) )
Fig. 4.20 Calculated boundstate energies of a particle in a symmetrical rectangular potential well of finite depth W0 indicated by the gray line. Bars at the righthand side mark energy levels with quantum numbers n for infinitely high barriers. After [84]
level spacing and consequently the energy of the levels decrease. The topmost bound level approaches the top of the well as W0 is gradually reduced. It should be noted that at least one bound level exists in any quantum well. A clear experimental observation of the quantumsize effect in quantum wells requires welldefined sharp interfaces. A vivid demonstration of subband formation was accomplished by imaging the local DOS in InAs/GaSb quantum wells [85]. Growth conditions ensured the formation of smooth InSblike interfaces between InAs and GaSb. The two semiconductors form a misaligned staggered band alignment with the conductionband edge of the InAs quantum well lying below the valenceband edge of the cladding GaSb. This brokengap configuration provides a large confinement potential for electrons in the well. Using the tip of a lowtemperature scanning tunneling microscope the local DOS was probed across the InAs well from the differential conductance d I /d V , cf. Fig. 4.21. The differential conduction given in Fig. 4.21a clearly shows a standingwave pattern originating from electron subbands in the InAs quantum well. The number of maxima increases with energy, i.e. sample bias voltage. The tunneling tip locally probes the probability amplitude of electrons across the well. The experimental result agrees remarkably well with the calculated subband wavefunctions shown in Fig. 4.21b. The twodimensional DOS of the quantum well given in Fig. 4.21c is experimentally deduced from integrating over the local DOS. The contributions of the subbands lead to apparent steps in the DOS being characteristic for a 2D heterostructure, cf. Fig. 4.19.
4.3 Electronic States in LowDimensional Structures
4 3 2 1 0
1.0
(a)
10
20
Position along growth direction (nm)
1.0 0.8 0.6
0.6
0.4
0.4
0.2
0.2
0.0
1
0.0
V = 0.01 V 0
1+2+3+4+5+6 (b)
0.8
0
10
0.2 20
Position along growth direction (nm)
Energy (eV)
V = 0.90 V
LDOS (arb. units)
(dI/dV) / (I/V)
5
Sample bias voltage (V)
InAs
153
(c)
0.8
6
0.6
5
0.4
4
0.2
3
0.0 0.0
2 1 0.5
1.0
Integrated (dI/dV) / (I/V) (arb. u.)
Fig. 4.21 a Experimental scanning tunneling (d I /d V )/(I /V ) spectra locally probed across a 17 nm wide InAs/GaSb quantum well for bias varied from 0.01 to 0.9 V in steps of 0.01 V. b Calculated local densityofstates given as the sum of the squared subband wavefunctions. c Experimental densityofstates obtained from integration of each curve in a over the quantum well. Reproduced c 2007 APS with permission from [85],
Features of both confined electrons and holes are observed in optical spectra. Transitions measured from nearly unstrained GaAs quantum wells with Al0.2 Ga0.8 As barriers and from strained GaAs wells with GaAs0.5 P0.5 barriers on GaAs substrates are shown in Fig. 4.22. The structures consist of multiple wells, i.e. superlattices with barriers sufficiently thick to prevent electronic coupling of the well states. They were grown using molecularbeam epitaxy [86] and metalorganic vaporphase epitaxy [87], respectively. The curves show the intensity of the groundstate emission under excitation at the displayed varied photon energy. The spectra exhibit series of peaks labeled according to the participating levels of the confined electrons and holes. Most intense peaks refer to allowed transitions between electron and hole states of twodimensional excitons with an equal quantum number n. Such exciton states have largest electronhole overlap if strain effects are not dominating. The strongest line labeled E 1h originates from the radiation of an exciton with the electron in the n e = 1 state and the m J = 3/2 hole denoted heavy hole in the n hh = 1 state. The corresponding transition of an electron and an m J = 1/2 light hole in the n lh = 1 state is labeled E 1l . The energy difference E 1l − E 1h reflects the splitting of the m J = 3/2 and 1/2 valence bands due to the biaxial shear strain in the GaAs well arising from the different lattice constants of barriers and well (Sect. 4.1.2). Note that excited states gradually broaden, as indicated in Fig. 4.22 for the heavyhole series labeled E nh . The broadening is described by E n = E 1 × n 2 [86], reflecting a nonconstant well width probed by a gradually increasing exciton diameter. Besides the two series of allowed transitions with n electron = n hole for heavy and light hole there are also forbidden peaks associated with transitions where n electron = n hole : Lines E f1 and E f2 mark transitions E 1e − E 3h and E 2e − E 4h , respectively [86, 88]. The transitions of the more strongly strained GaAs well clad by GaAs0.5 P0.5 barriers shown in Fig. 4.22b exhibit a much larger splitting E 1l − E 1h (44 meV) than observed for Al0.2 Ga0.8 As barriers. Hydrostatic and shearstrain components of εh = 0.008 and εs = 0.014, respectively, were determined from the shift of the groundstate exciton with respect to a GaAs bulk exciton and from the lighthole—
154
4 Electronic Properties of Heterostructures Energy (eV)
(a)
GaAs/AlGaAs pump
E1h E1l
Ef1
E4h
E3h
E2h E2l Ef2 4 meV
E3l 9 meV
16 meV
260 Å
PL Intensity (arb. units)
PL Intensity (arb. units)
1.55
1.60
GaAs/GaAsP E1h E2h E1l
E3h
1.70
E2l E4h
(b)
230 Å 202 Å
0
1.52 1.54 1.56 1.58 1.60 1.62 1.64
1.65
50
100
150
E (meV)
Energy (eV)
Fig. 4.22 Photoluminescence excitation spectra of GaAs quantum wells clad by a Al0.2 Ga0.8 As and b GaAs0.5 P0.5 barriers, recorded at low temperatures and low excitation density. The well width is indicated at the spectra. Labeled energies refer to optical transitions of bound electron states to bound hole states, see text. Absolute energy scale on top of panel (b) refers to upper spectrum, the lower spectrum is shifted in energy to align the E 1h transition. a After [86], b after [87]
Binding energy EX (meV)
15
(a)
GaAs/Al0.40Ga0.60As
lh
10
hh 5
Spatial extension (nm)
Fig. 4.23 a Calculated binding energy and b both lateral (ρex ) and perpendicular (z ex ) spatial extension of an exciton confined in a GaAs/Al0.4 Ga0.6 As quantum well. Solid and dashed lines refer to heavy and lighthole exciton, respectively. Reproduced with permission c 1988 APS from [75],
hh ex
lh 10
zex lh 0
0
(b) 5
10
15
Well width Lz (nm)
20
25
4.3 Electronic States in LowDimensional Structures
155
heavyhole splitting [87]. The quantumsize effect is expressed in Fig. 4.22b by a blue shift of the excitedstate transitions in the thinner quantum well (lower spectrum). The twodimensional confinement changes spatial extension and binding energy of an exciton both within the quantumwell plane and perpendicular [75]. The effect is illustrated in Fig. 4.23 for an exciton confined in a GaAs/Al0.4 Ga0.6 As quantum well. We note a strong increase of the binding energy E X (4.48) in Fig. 4.23a with a maximum for very thin quantum wells near 1 nm. The smaller binding energy of the heavy hole originates from a larger inplane mass of the light hole [75]. The (degenerate) bulk values of the binding energies of lighthole and heavyhole excitons are approached for the limits of zero and infinite well width L z . The binding energy of the excited 2s and 2 p± states of the lh and hh exciton vary similar to that of the 1s ground state shown in Fig. 4.23 [89]. The lateral and perpendicular extensions of the exciton given in Fig. 4.23b show a simultaneous squeezing inverse to the binding energy, according to the rule aX × E X = const. Heterostructure interfaces are usually not abrupt from one single atomic layer to the next layer in growth direction over a macroscopically large lateral scale. The resulting roughness of the interface is probed by excitons confined in a quantum well. Lateral fluctuations of the well thickness (and composition) are averaged within the spatial extent of the exciton which is given by twice the Bohr radius aX . Such an effect leads to the gradual broadening of the exciton series shown in Fig. 4.22. If the fluctuations occur on a scale larger than the exciton diameter discrete transitions may be found. A model for interface roughness due to growth steps with a height of a single monolayer (ML) at both barriers of a quantum well is illustrated in Fig. 4.24. Since a step position at the lower interface is not expected to be reproduced by the upper interface three thicknesses arise from such fluctuations, namely L z , L z + 1 ML, and L z − 1 ML. Interface disorder of the kind illustrated in Fig. 4.24 may be observed particularly in narrow quantum wells. A clear observation in photoluminescence spectra of GaAs/Alx Ga1−x As quantum wells is shown in Fig. 4.25 [90]. In the (001)oriented zincblende material one monolayer corresponds to half a lattice constant: 1 ML = a/2, a being the lattice constant of both materials, the quasiunstrained GaAs well and the Al0.3 Ga0.7 As barriers.
Fig. 4.24 Cross section of a quantum well/barrier doubleheterostructure. Interface roughness by growth steps of single monolayer height is depicted at both barriers of the quantum well
1 ML
Lz1 ML
barrier
Lz
Lz+1 ML
well
barrier
156
Lz+4 a2
EW
PL Intensity (arb. units)
Fig. 4.25 Photoluminescence spectrum of a GaAs/Al0.3 Ga0.7 As heterostructure comprising a superlattice with wells of 50 Å (SL) width and also wells with a width enlarged by additional three monolayers to 58.6 Å (EW). The emission was excited nonresonantly with a low excitation density at low temperature. Arrows at bottom indicate calculated transitions energies referring to L z + n × a/2. After [90]
4 Electronic Properties of Heterostructures
Lz+3 a2
Lz+ a2
1.59
1.60
1.7 K 2 0.1 W/cm
SL
1.61
Lz
1.62
1.63
Energy (eV)
The sample studied in Fig. 4.25 consists of a GaAs/Al0.3 Ga0.7 As superlattice (SL) with L z = 50 Å thick wells and 50 Å thick barriers. After growth of each 14 wells (1400 Å) one enlarged well (EW) with an additional thickness of three monolayers (50 Å + 8.6 Å) was introduced. The photoluminescence shows emissions from heavyhole excitons of the superlattice and the enlarged wells, both split by an amount corresponding to about onethird of their mutual separation. (Corresponding transitions of the lighthole excitons were found in excitation spectra.) This agrees with an expected variation originating from a thickness difference of one monolayer (a/2). The position of the individual peaks matches calculated transitions energies of quantum wells with thicknesses L z + n × a/2, n = 1 to 4, and a = 5.73 Å, if the transition referring to L z of the SL well is taken as a reference. The poor agreement of the leftmost peak is attributed to an increased disorder in the extended well. We note that the peaks corresponding to L z + 2a/2 (middle arrow) is missing. Also no peak is found referring to L z − a/2 (above 1.62 eV, no arrow drawn). These transitions would arise from thinner parts of the enlarged well and the superlattice, respectively. They are not observed due to a negligible thermal occupation at the low measurement temperature of 1.7 K. Sizequantization effects of excited states and interface roughness are frequently observed in quantum wells of various materials systems, albeit usually not as pronounced as in the examples given above.
4.3.4 Quantum Wires Fabrication of a quantum well follows naturally from the twodimensional epitaxy of a double heterostructure. The potential of such a quantum well is basically defined by the well thickness and the (homogeneous) chemical composition of well and barrier
4.3 Electronic States in LowDimensional Structures
157
B
B
B
B B
S Vshaped wire
S
B Ridge wire
S
B
Sidewall wire
B
B
S
Tshaped wire
Fig. 4.26 Crosssection of typical types of epitaxial quantum wires (encircled). B and S signify barrier and substrate materials, respectively
materials, i.e., by the band discontinuities. A further reduction of dimensionality towards a onedimensional quantum wire or a zerodimensional quantum dot requires some patterning to define an additional lateral confinement. The small dimensions needed to obtain respective quantum sizeeffects (Sect. 4.3.2) can usually not be accomplished straightforward by patterning a quantum well structure using, e.g., lithography techniques [91]. The interfacetovolume ratio of 1D and 0D structures increases as compared to 2D quantum wells, and the electronic properties of such structures are largely governed by interface effects. A variety of techniques was developed instead to realize 1D and 0D structures with high optical quality, e.g., by employing growth on corrugated substrates [92], or whisker growth discussed in Sect. 12.2. Most of these techniques lead to complicate confinement potentials, and often an additional quantum well is coupled to the quantum wires or quantum dots. A few examples will be considered in this and the following sections. Much progress in the formation of epitaxial 1D quantum wires was achieved using Vshaped wires or Tshaped wires. A schematic of some typical wire geometries is given in Fig. 4.26. The Vshaped, ridge, and sidewall wires depicted in Fig. 4.26 are fabricated by employing the dependence of the growth rate on crystallographic orientation (Sect. 12.1). Using patterned substrates with various facet orientations thereby a locally enhanced thickness of a wire material clad by barrier materials can be grown. The Tshaped wire depicted in Fig. 4.26 is formed from an overgrowth of the cleaved edge of a quantumwell structure. The fabrication process of lowdimensional structures is described in more detail in Sect. 7.3. Early demonstrations of quantum wires in the late 1980s suffered from thickness fluctuations on a length scale of the exciton Bohr radius, leading to 0D behavior at low temperatures. Clear 1D behavior was proved later using improved structures and also by employing microphotoluminescence on single wires. Photoluminescence (PL) and corresponding excitation (PLE) spectra of V quantum wires are shown in Fig. 4.27 [93]. The given wire thickness refers to the thickest part in the center of the crescentshaped GaAs, which has parabolalike interfaces to the cladding AlGaAs barriers. The wire emission is labeled QWR in Fig. 4.27a, the dominating emission originates from the quantum wells formed at the side walls of the V groove.
158
4 Electronic Properties of Heterostructures Energy (eV) 1.60
1.4
QWR
1.5
1.6
0.0
QW
1.7
AlGaAs barrier
1.8
Energy (eV)
1.9
2.0
2.1
1.68
1.72
2.5 nm QWR
(a) Degree of circular polarization
PL Intensity (arb. units)
2.5 nm QWR 8K
1.64
e1h1 e2h2
0.3
1.76
(b)
e9h9 e h e8h8 e6h67 7 e3h3 e4h4e5h5
0.6
e1h6
1.5 nm QWR (c)
0.2
e2h2
0.0
e1h1
0.2 0.4 0.6 1.56
e3h3 e4h4
e5h5
PL Intensity (arbitrary units)
1.56 0.3
e1h7 1.60
1.64
1.68
1.72
1.76
Energy (eV)
Fig. 4.27 a Photoluminescence of a Vshaped GaAs/Al0.3 Ga0.7 As quantum wire, nonresonantly excited at 2.4 eV with a low excitation density of 25 W/cm2 . b PLE spectra for 2.5 nm and c 1.5 nm thick wires polarized parallel (thin solid line) or perpendicular (dotted line) the [110]oriented wires. Thick solid curves represent the degree of circular polarization. Arrows mark calculated positions c 1997 APS of excitonic en –h m interband transitions. Reproduced with permission from [93],
The PLE spectra given in Fig. 4.27b, c show a number of features also observed with quantum wells, cf. Fig. 4.22. Basically optical transitions with an equal quantum number n of electron and hole states are found. The en –h n transitions shift to the blue as the wire thickness decreases, and their mutual energy spacings increase. The assignment of the peaks to corresponding exciton states is not trivial due to the complicate crescentshaped potential of the wire. The transition energies marked in Fig. 4.27b, c were calculated using a 16band kp model and a potential shape extracted from transmissionelectron micrographs. We note a pronounced oscillator strength of the usually forbidden e1 –h 6 transition in the thicker well. Moreover, no distinction is drawn between contributions of light holes and heavy holes. Calculations reveal a strong mixing of light and heavyhole character in the valenceband states, particularly involved in the mentioned transition. The wave function of the ∼70% lighthole part of the h 6 state has its maximum in the wire center similar to the e1 state, yielding a large overlap [94] (for separate lh and hh assignments cf. [95, 96]). The valenceband mixing also gives rise to the polarization behavior observed in the samples. It should be noted that such mixing and polarization anisotropy may also originate from other sources like structural inhomogeneity, and care was taken to ensure the 1D origin.
4.3 Electronic States in LowDimensional Structures
159
For crescentshaped V groove quantumwires a simple model with infinite barriers and hyperbolic boundaries was considered to obtain approximative energy separations of the subbands in the wires [97]. The assumed potential leads to analytical solutions given by E n,m
√ 2 π αn 2 π 2 n 2 ∼ + (m − 1/2), m, n = 1, 2, 3, . . . , = m ∗ t0 ρ 2m ∗ t02
(4.51)
where m ∗ is the effective chargecarrier mass, t0 is the crescent thickness at its √ center, and ρ = ρlow × ρup is the geometric mean radius of the lower and upper radii of the crescent. The upper curvature ρup is given by ρup = ρlow + αt0 , with α describing the linear increase of the curvature as the wire thickness increases. The second summand in (4.51) describes the energy separation of the 1D subbands due to the lateral confinement. Sizequantization effects of 1D wires are sometimes not well distinguished from those of a 2D well or a 0D dot. The lateral confinement potential of commonly used wire geometries (Fig. 4.26) is typically only on the order of 30–40 meV, giving rise to only 10 meV subband energyseparation [92]. The potential is hence much smaller than that of a quantum well. Furthermore, size fluctuations may give rise to an additional confinement along the wire axis on the same order of magnitude. The potential depth of the lateral confinement in Tshaped GaAs/Alx Ga1−x As quantum wires was evaluated from sample series with varied well widths and Al compositions. Energies of exciton PL peaks related to the T quantum wire (QWR), the stem well QW1 (vertical quantum well in Fig. 4.26), and the arm well QW2 (horizontal) are shown in Fig. 4.28a for varied thickness of QW2 [98]. The exciton energy increases for thinner QW2 also in the quantum wire. Note that the slope of the QWR energy is smaller than that of the QW2 energy. The energy of the wire hence approaches that of QW1 for thinner QW2 and that of QW2 for thicker QW2. The reason is a convergence of QWR states into QW1 for tQW2 tQW1 and vice versa into QW2 for tQW2 tQW1 . The spacings between the QWR PL peak energy and those of the quantum wells QW1 and QW2, i.e., the energy differences between the 1D exciton and the 2D exciton states of the neighboring wells, give directly the effective lateral confinement in the wire for given quantumwell thicknesses. This value includes possible changes of the exciton bindingenergy. The lateral confinement gets maximum for identical thicknesses of QW1 and QW2. For such balanced T quantum wires Fig. 4.28b shows the dependence of the effective lateral confinement on the exciton energy in QW2. The calculated dependence of lateral confinement energy on the recombination energy of wellexcitons given in Fig. 4.28b shows a sublinear increase for finite barrier height. This feature arises from a penetration of the wave function into the wells. The dependence approaches linearity for increasing barriers. At infinite barriers both, QWR energy and QW2 energy scale according to t −2 leading to the linear relation. The strong experimental superlinear increase found for increased barriers (xAl from
160
4 Electronic Properties of Heterostructures
QWR
Energy (eV)
1.62
QW1
QW2 QW1
Lateral confinement energy (meV)
1.64
QW2
(a)
1.60
QWR 1.58
1.56 4.5
5.0
5.5
6.0
QW2 thickness (nm)
50
(b)
infinite barriers
40
500 meV
30 barriers: 20
AlAs Al0.3Ga0.7As
10 0 1.5
355 meV
finite barriers 1.6
245 meV
1.7
1.8
1.9
Energy (eV)
Fig. 4.28 a PL peak energies of excitons confined in a T quantum wire (QWR) and the neighboring stem quantum well (QW1) and arm well (QW2) of a GaAs/Al0.3 Ga0.7 As heterostructure. Dashdotted and dotted vertical lines indicate identical QW1 and QW2 well thicknesses and QW2 thickness at identical QW1 and QW2 exciton energy, respectively. b Calculated lateral confinement energy of electrons in balanced T quantum wires as a function of QW2 exciton energy. Solid and dashed lines refer to energies for infinite and finite barriers as indicated. Crosses and filled circles, respectively, mark calculated and experimental confinement energies extracted from the c 1996 measurement of GaAs/Alx Ga1−x As structures. Reproduced with permission from [98], APS
0.30 to 1.00) is due to the substantial enhancement of Coulomb interaction in 1D excitons [98]. The excitonic absorption of a 1D quantum wire is expected to deviate significantly from that of a 2D quantum well or a 3D bulk crystal. For direct allowed transitions above band edge the intensity ratio of the unbound (continuum) exciton to the free electronhole pair is found to be smaller than unity, in contrast to the 2D and 3D cases [99]. The feature may be understood by considering the eigenenergies of states bound in a bare Coulomb potential for d dimensions (d = 1, 2, 3, . . . ). The analytical solutions of the Schrödinger equation yield in each dimension d energies E nd of eigenstates with s symmetry in form of a Rydberg series [99] E nd
d − 1 −2 = −Ry n + , n = 0, 1, 2, . . . , 2 ∗
(4.52)
4.3 Electronic States in LowDimensional Structures
161
Ry∗ being the effective Rydberg energy. For the threedimensional case (d = 3) we recognize the wellknown Rydberg series of hydrogen. For 1D we note a singularity for the lowest state n = 0, corresponding to infinite binding energy, in contrast to the 3D and 2D case. This suggests the attractive force between electron and hole being stronger in 1D than in 2D or 3D. In a descriptive idea a particle may move around the origin of a Coulomb potential in 2D or 3D, while it moves through the origin in 1D. In fact, the 1/r singularity of the Coulomb potential is removed upon integration in 2D and 3D, but it remains as a logarithmic singularity in 1D. The 1D nature of a quantum wire leads also to a characteristic dynamics of the radiative decay of exciton population after pulse excitation [100]. The population decaytime was found to vary proportional to the square root of sample temperature, in contrast to the linear proportionality observed in quantum wells. The PL hence decays slower at low temperatures and faster at high temperatures in wires compared to wells.
4.3.5 Quantum Dots A quantum dot represents the ultimate limit in chargecarrier confinement, leading to fully quantized electron and hole states like the discrete states in an atom. The most successful approach for the fabrication of dislocationfree semiconductor quantumdots is the selforganized (also referred to as selfassembled) technique of Stranski– Krastanow growth (Sect. 7.3.1). This kind of growth mode may be induced by epitaxy of a highly strained layer, which initially grows twodimensionally and subsequently transforms to threedimensional islands due to elastic strain relaxation. Some part of the layer material does not redistribute but remains as a twodimensional layer, due to a low surface free energy compared to the covered material. Since this layer wets the surface of the material underneath it is referred to as wetting layer. For practical use such islands are covered by a cap layer, which builds an upper barrier in addition to the lower barrier provided by the covered material underneath, cf. Fig. 4.29. It must be noted that a minimum size of a quantum dot exists to allow for confining a charge carrier, in contrast to structures of higher dimensionality. For a dot with spherical shape the minimum diameter Dmin required to confine at least one bound state of a particle is given by [101] Dmin = √
π , 2m ∗ W0
(4.53)
where W0 is the confining potential and m ∗ the effective mass (assumed to be identical in dot and barrier). For a rough estimate of the minimum size to confine a single electron in a spherical InAs/GaAs dot we use an unstrained conduction band offset of ∼0.9 eV for W0 and an effective electron mass in InAs of 0.03 m 0 , yielding Dmin ∼ = 6 Å.
162
4 Electronic Properties of Heterostructures
Fig. 4.29 Crosssection view of a quantum dot grown selforganized in the Stranski–Krastanow mode. Q D, W L, B, and S signify quantum dot, wetting layer, barriers and substrate, respectively
WL QD S
B
B
Quantum dots grown in the Stranski–Krastanow mode often have a shape of a truncated pyramid. Due to the persistence of the wetting layer in the formation process such dots are coupled to a quantum well, similar to the epitaxial quantum wires depicted in Fig. 4.26. Selforganized Stranski–Krastanow growth may be induced by a strong mismatch of the heterostructure. InAs dots on GaAs with 7% mismatch represents the most studied model system. The type I band alignment to GaAs leads to a confinement of both, electrons and holes. The finite barrier height provided by the GaAs matrix allows for only few electronic states to be confined within the dot. Luminescence spectra of single quantum dots detected with high spatial resolution show radiative recombination of correlated electrons and holes, cf. Fig. 4.30. The narrow halfwidth of such confinedexciton recombination reflects the zerodimensional DOS. Various lines from a single QD originate from states differently filled with few particles like, e.g., the negative trion (X− ) formed by two electrons and one hole, or the biexciton (XX) formed by two excitons.
Ec
Intensity (arb. units)
Ev X
XX X

+
X
1.255
+
XX
1.260
1.265
1.270
1.275
Energy (eV) Fig. 4.30 Luminescence of a single quantum dot showing sharp recombination transitions of neutral and charged confined excitons, as depicted above the spectrum. E c and E v denote conduction and c 2005 APS valence band edge, respectively. Spectrum reproduced with permission from [102],
4.3 Electronic States in LowDimensional Structures
163
electrons
holes
0.88 V
1.06 V
1.17 V
1.31 V
Fig. 4.31 Top: Calculated probability densities of electron and hole wavefunctions confined in a pyramidshaped InAs quantum dot in a GaAs matrix. Reproduced with permission from [106], c 1999 APS. Bottom: Lowtemperature STM images of an uncovered InAs quantum dot on GaAs. Left image: Constantcurrent image showing the dot shape. Right four images: Singleelectron densities of different excitation states sampled at different bias voltage. Reproduced with permission c 2003 APS from [104],
The wave functions of the confined states can be calculated by considering realistic size, shape, and composition of the dot, in addition to material properties like dielectric constants, strain tensors and piezoelectric tensors [103]. Results for one electron and one hole confined in an InAs dot with pyramidal shape of 11.3 nm base length and {101} side facets in a GaAs matrix are shown in Fig. 4.31. The isosurfaces encase 65% probability and resemble atomic slike ground states (left column), and p and dlike excited states. Corresponding wave functions of singleelectron states in uncovered InAs/GaAs dots were experimentally imaged using a lowtemperature scanningtunneling microscope. The images were obtained from spatially resolved differential voltagecurrent curves d I /d V taken at different sample voltage [104]. In the same way states of holes confined in InAs quantum dots embedded in GaAs matrix were imaged from cleaved samples [105]. The discrete energies of confined charge carriers sensitively depend on size, shape, and composition of the dot. Since these quantities show some variation among individual dots within an ensemble comprising many dots the eigenenergies vary from dot to dot. Optical spectra detected as a response of the entire ensemble are consequently inhomogeneously broadened due to a superposition of numerous transitions of different energies. The discrete nature of the transitions, i.e. the homogeneous line width, becomes apparent when only a single dot of an ensemble is spatially selected by using, e.g., microphotoluminescence (micro PL) or opaque masks with a small aperture. The luminescence spectra shown in Fig. 4.32 illustrate the effect of a gradually increased spatial selection of the detected or excited area in a planar field of a quantumdot ensemble. The broad luminescence spectrum in Fig. 4.32a measured using a conventional PL setup (macro PL) originates from a large number (∼106 )
164
(a)
macro PL 10 K
Intensity(arbitraryunits)
Fig. 4.32 a, b Luminescence of an InAs/GaAs quantum dot ensemble with ∼108 cm−2 areal density, detected at 10 K using a conventional setup (a) and a setup with a small focus (b). c 10 K electroluminescence of a single dot of the same kind as in a, b, integrated into a diode structure with a currentconfining aperture of submicron diameter. Spectra (b) and (c) adapted from [107]
4 Electronic Properties of Heterostructures
QD ensemble
x1
(b)
micro PL few QDs x 40
(c)
EL with aperture 0.9 nA
single QD
x 20
1.25
1.30
1.35
1.40
Energy(eV)
of dots. The full width at half maximum (FWHM) of an ensemble PL is typically several 10 meV broad. The microPL setup used in Fig. 4.32b probes the photoexcited quantumdot ensemble solely within a small focus, thereby detecting only ρQD × Afocus dots simultaneously, ρQD being the areal dot density. Further selection eventually leads to the detection of a single dot of the ensemble, cf. Figs. 4.32c and 4.30. The homogeneous line width of a singledot emission is extraordinary small. In absence of inhomogeneous contributions (e.g., by spectral diffusion) it is given by the lifetime τ of the excited charge carrier according to the E × τ uncertainty relation. It is typically on the order of µeV and usually below the experimental detection limit. The areal density of a quantumdot ensemble grown using the Stranski–Krastanow mode is typically in the 1–10 × 1010 cm−2 range, cf. Sect. 7.3.1. The number of states to be occupied by charge carriers in a single dot layer (or few dot layers) is much smaller than in bulk or a quantum well. Occupation of quantum dots with more than one exciton or charge carrier hence occurs already at reasonably low optical or electrical excitation. Since the ground state may be occupied with only two charge carriers (of opposite spin) excited states are easily populated. Figure 4.33 shows the strong occupation of excited levels in a quantumdot ensemble at increased excitation density. While at low excitation density only the inhomogeneously broadened emission from the ground state labeled I0 is observed, gradually additional emissions from excited states (I1 to I4) appear on the highenergy side for more intense excitation. The number of excited levels is high in this particular sample, because an Al0.3 Ga0.7 As barrier was placed underneath the dot layer, separated by a 1 nm
4.3 Electronic States in LowDimensional Structures
Log. Intensity (arb. units)
I0
1.08
165
T T=2K = 532 nm ex
1.11
1.14
I1
WL I3
I2
I4
I0 GaAs
1.0
1.1
1.2
1.3
1.4
1.5
Energy (eV) Fig. 4.33 Photoluminescence spectra of an In0.6 Ga0.4 As/GaAs quantumdot ensemble, excited into the GaAs matrix with an excitation density gradually increasing from 0.2 W/cm−2 (bottom) to 5 kW/cm−2 . I0 marks groundstate emission, peaks I2 to I4 originate from excited states. WL and GaAs signify emission from the wetting layer and the GaAs matrix, respectively. Inset: Emission c 2004 Elsevier I0 on a linear scale. Reproduced with permission from [108],
thick GaAs spacer, so as to increase the confinement potential. Taking the degeneracy 2(n + 1) of a lateral harmonic potential as a rough estimate for the exciton occupation in a quantum dot, the maximum overall occupation number of the confined excitonic states is about 30 in the studied case. The approach of an harmonic potential is supported by scanning tunneling spectroscopy [109, 110]. A close look to the energies of the quantumdot emission shows that the increasing occupation of levels with charge carriers is accompanied by a small energy decrease. The groundstate transition, e.g., exhibits a red shift by a total of 35 meV (inset Fig. 4.33). Such behavior cannot be described in a singleparticle picture, because the Coulomb interaction between the confined particles alters the overall energy in the system. The effect is referred to as renormalization of the band gap. The origin was traced back in bulk semiconductors to the exchangecorrelation energy in dense chargecarrier ensembles, being independent on the characteristics of the electronic band structure, i.e., on the material [111]. It is also pronounced in quantumwell structures [112]. In quantum wires [113] and quantum dots [114] such renormalization may be smaller in case of a dominating strong confinement. An ensemble of selforganized quantum dots usually exhibits a single distribution of dot sizes and compositions, leading to a single inhomogeneously broadened ensemble emission. Under certain growth conditions also distributions with several well separated emission maxima are formed. An insight into the interplay between
166
Energy (eV) 0.7
0.8
PL Intensity (arb. units)
4.2 K
0.9
1.0
1.2
InAs/InP
7
1.3
(a)
4
8 6
9
5
7
7K
1.1
8
3
5 6
9
InAs/GaAs
(b)
4 3 2
1.6
e Excitation Energy (eV)
Fig. 4.34 Ensemble emission of a InAs/InP and b InAs/GaAs quantum dots with a multimodal size distribution. Numbers at the peaks refer to a common dot height within a subensemble in units of monolayers. c Combined PL and PLexcitation contour plot of the ensemble measured in b on a logarithmic color scale, abscissa also applies for (b). Horizontal lines mark lighthole (lh) and heavyhole (hh) resonances of the wetting layer, inclined lines indicate resonances of the first and second excited state of the dots and an LO phonon transition. Data in a adapted from [118], data in b and c reproduced with permission from [119], c 2007 Elsevier
4 Electronic Properties of Heterostructures
1.5
GaAs lh hh
1.4 1.3
2. ES
1.2 1. ES
1.1
(c)
LO
1.05
1.10
1.15
1.20
1.25
1.30
1.35
e Detection Energy (eV)
confinedparticle interaction and confinement potential was obtained using dots with a multimodal size distribution, featuring a number of clearly resolved fairly narrow emission peaks of the ensemble [115]. The multiple peaks refer to subensembles (or families) of dots within the ensemble, which differ in height by integral numbers of InAs monolayers. Peak labels given in Fig. 4.34 indicate the height of the dots in the corresponding subensemble in units of monolayers. The assignment was proved by both structural characterization [116] and calculated exciton energies [117], revealing a truncated pyramidal shape of the dots. Spectra shown in Fig. 4.34a, b were excited with a low excitation density to ensure emission solely from the ground state. PL excitation spectra of a multimodal dot ensemble are given in the contour plot Fig. 4.34c: A horizontal cut represents a photoluminescence spectrum at fixed excitation energy, a vertical cut represents an excitation spectrum for the selected detection energy. For large quantum dots with low emission energy an excitation spectrum shows two excited states ES1 and ES2 below the excitation of the dot emission via the wetting layer (labels hh and lh). We note that smaller dots with a
10
Binding energy (meV)
Fig. 4.35 Binding energy of fewparticle complexes confined in InAs/GaAs quantum dots as a function of the neutral exciton emission energy. 0 refers to the neutral exciton recombination energy. X − , X + , and XX refer to negative trion, positive trion, and biexciton. Right ordinate corresponds to the lightgray emission spectrum. Reproduced with permission from [119], c 2007 Elsevier
167 X
0 XX 10 +
X 1.1
1.2
PL Intensity (arbitrary units)
4.3 Electronic States in LowDimensional Structures
1.3
Exciton energy (eV)
height between 5 and 3 monolayers—and correspondingly a higher emission energy between 1.22 eV and 1.32 eV—have only a single excited state. Dots with even higher emission energy (>1.32 eV) have no excited state at all. The welldefined size and shape of multimodal dots was employed to study the renormalization of fewparticle transition energies acting when, e.g., one electron and hole recombine in the presence of additional charge carriers. Figure 4.35 shows relative binding energies of negative trions (consisting of 2 electrons and 1 hole), positive trions (1e, 2h), and biexcitons (2e, 2h) for many singledot spectra recorded all over the inhomogeneously broadened ensemble peak [120]. The binding energy of these fewparticle complexes is given with respect to the (neutral) excitonrecombination energy and the recombination energy of these complexes, i.e. by E X − E complex . The three excitonic complexes show an obvious characteristic trend. The negatively charged exciton labeled X− has always a positive binding energy being almost independent on the neutral excitonrecombination energy. Contrary the binding energies of the positively charged exciton X+ and the biexciton XX clearly decrease for increasing excitonrecombination energy (decreasing dot size). Moreover, for the biexciton a transition from positive to negative binding energies is observed. The nonzero binding energies originate from the Coulomb interaction C between the confined charge carriers. The binding energy of, e.g., X− directly depends on the difference between the two direct Coulomb terms C(e, h) and C(e, e). The wave function of the hole is much stronger localized than that of the electron due to the larger effective mass of the holes, independent on the dot size as shown on top of Fig. 4.36. The absolute value of the Coulomb interaction between two electrons C(e, e) is consequently smaller than that between two holes, and that between an electron and a hole is in between, i.e., C(e, e) < C(e, h) < C(h, h), cf. Fig. 4.36a. All energies increase in smaller dots because the wave functions are slightly squeezed. A negative trion is formed by adding an electron to a dot which is filled with an exciton, thereby adding a repulsive interaction and additionally a
168
4 Electronic Properties of Heterostructures
height base length
13 ML 15.8 nm
3 ML 10.2 nm
electrons holes
ECoulomb (meV)
13
35
9
7
5
(a)
C(h,h) C(e,h) C(e,e)
(b)
Binding energy (meV)
3 height (ML)

X
XX +
X X
(c)

XX +
X
Exciton energy (meV)
Fig. 4.36 Top: Electron and hole wavefunction (65% probability surface) for confinement in a 15 monolayer high (left) and 3 monolayer high (right) InAs/GaAs quantum dot. a Absolute value of the Coulomb energy between two charge carriers confined in a quantum dot. b, c Calculated fewparticle binding energies: b only ground state considered, c additionally 2 excited levels for c 2006 Elsevier both, electrons and holes included. Reproduced with permission from [121],
(larger) attractive interaction. The negative trion has therefore a positive binding energy E X − E X− , while the positive trion has a negative binding energy. The simple picture does not account for the trend of the biexciton XX. Including three instead of one level for both, electron and hole states into the calculation (i.e., considering also effects of correlation) changes the result from a nearly constant negative binding energy (Fig. 4.36b) to a nearly constant positive binding energy (Fig. 4.36c). Figure 4.34c demonstrates that large dots bind more confined levels than small dots. Consequently the degree of correlation decreases as the dot size decreases. We hence start with large dots (small exciton energy) in a case depicted in Fig. 4.36c, and end with small dots in a case similar to Fig. 4.36b. Thereby the XX
4.4 Problems Chapter 4
169
binding energy changes from positive to negative values as found in the experiment Fig. 4.35. A more detailed consideration shows that the number of hole levels plays a major role in correlation [120].
4.4 Problems Chapter 4 4.1 The Ga1−x Inx P alloy is interesting due to its direct large bandgap energy compared to that of GaAs and InP. (a) Calculate the bandgap energy of Inx Ga1−x P at room temperature, assuming a layer which is latticematched on GaAs substrate. Check whether this alloy has a direct or an indirect conductionband minimum. Compare the order of these bandgap energies to that expected from the virtual crystal approximation. Roomtemperature bandgap parameters E Γ , E X , E L (in eV) of GaP are 2.78, 2.27, 2.6, and parameters of InP are 1.34, 2.19, 1.93, respectively. The bowing parameters of the alloy are (in eV) bΓ = 0.65, bX = 0.20, bL = 1.03. (b) Determine the composition parameter x, where unstrained Ga1−x Inx P changes from a direct to an indirect semiconductor. Which bandgap energy exists at the crossing point? 4.2 Consider a latticematched InP/Inx Ga1−x As/InP double heterostructure on (001) InP substrate. Find the offset in the conduction band at 300 K and at 77 K, if the valenceband offset of +0.36 eV from InP to Inx Ga1−x As is assumed temperatureindependent, and effects of thermally induced strain can be neglected. Band parameters E g at 0 K (in eV), α (in meV/K), and β (in K) are for InAs 0.417, 0.276, and 93, for GaAs 1.519, 0.541, and 204, and for InP 1.424, 0.363, and 162, respectively, bInGaAs = 0.48 eV. 4.3 A pseudomorphic hexagonal Al0.2 Ga0.8 N layer grown on a relaxed thick GaN buffer layer produces a sheet chargedensity at the interface induced by piezoelectric polarization. Apply in the following linearly weighted materials parameters. (a) Calculate the sheet carrierconcentration per cm2 of the AlGaN layer originating from the piezoelectric polarization. (b) The piezoelectric polarization adds to the spontaneous polarization of a wurtzite semiconductors, the latter being −0.029 C/m2 for GaN and −0.081 C/m2 for AlN. Determine the lateral strain of the GaN layer required to yield a zero total polarization in the AlGaN layer. What is then the resulting total sheet carrierdensity at the interface? 4.4 (a) Find the offset in the valence band and the conduction band for a transition from a GaAs (001) substrate to a thin pseudomorphic InP layer. Neglect the straininduced splitting between heavy hole and light hole.
170
4 Electronic Properties of Heterostructures
(b) What offsets occur in the inverse heterostructure of a thin pseudomorphic GaAs layer on InP(001) substrate, if the straininduced splitting between heavy hole and light hole is neglected? (c) Compare the energy splitting between the heavyhole valence band and the lighthole valence band of GaAs in case (b) with the band offsets calculated for a neglected splitting. Which exciton has lowest energy? What are the actual band offsets obtained by including the energy splitting between heavy hole and light hole? 4.5 (a) The temperature dependence of the direct bandgap of GaAs is described by the parameters α = 0.54 meV/K and β = 204 K. Which bandgap energy has GaAs at room temperature (300 K) and at the temperature of liquid nitrogen (77 K)? (b) The effective bandgap changes in presence of a confining potential. It is then approximately given by the difference between the groundstate levels of the electron in the conduction band and the hole (with lowest energy) in the valence band. Calculate the effective bandgap of an unstrained GaAs quantum well of 9 nm thickness for infinite barriers at room temperature. Effective electron and hole masses are 0.067m e and 0.082m e , respectively. (c) The thickness of the quantum well in (b) varies by ± one monolayer due to interface roughness. To which variations in the effective bandgap translates this thickness fluctuation?
4.5 General Reading Chapter 4 E.T. Yu, J.O. McCaldin, T.C. McGill, Band offsets in semiconductor heterojunctions, in Solid State Physics, vol. 46, ed. by H. Ehrenreich, D. Turnbull (Academic Press, Boston, 1992), pp. 1–146 P.Y. Yu, M. Cardona, Fundamentals of Semiconductors, Physics and Materials Properties, 4th edn. (Springer, Berlin, 2010) K.W. Böer, U.W. Pohl, Semiconductor Physics (Springer, Cham, 2018)
References 1. P.Y. Yu, M. Cardona, Fundamentals of Semiconductors (Springer, Berlin, 1996) 2. K.W. Böer, U.W. Pohl, Semiconductor Physics (Springer, Cham, 2018) 3. I. Vurgaftman, J.R. Meyer, L.R. RamMohan, Band parameters for IIIV compound semiconductors and their alloys. J. Appl. Phys. 89, 5815 (2001) 4. M. Suzuki, T. Uenoyama, Firstprinciples calculations of effectivemass parameters of AlN and GaN. Phys. Rev. B 52, 8132 (1995) 5. M. Posternak, A. Baldereschi, A. Catellani, Ab initio study of the spontaneous polarization of pyroelectric BeO. Phys. Rev. Lett. 64, 1777 (1990)
References
171
6. G.L. Bir, G.E. Pirkus, Symmetry and StrainInduced Effects in Semiconductors (Wiley, New York, 1974) 7. F.H. Pollak, M. Cardona, Piezoelectroreflectance in Ge, GaAs, and Si. Phys. Rev. 172, 816 (1968) 8. C.G. van de Walle, R.M. Martin, Theoretical calculation of heterojunction discontinuities in the Si/Ge system. Phys. Rev. B 34, 5621 (1986) 9. K. Shahzad, D.J. Olego, C.G. van de Walle, Optical characterization and band offsets in ZnSeZnSx Se1−x strainedlayer superlattices. Phys. Rev. B 38, 1417 (1988) 10. C.G. van de Walle, Band lineups and deformation potentials in the modelsolid theory. Phys. Rev. B 39, 1871 (1989) 11. D. Fröhlich, W. Nieswand, U.W. Pohl, J. Wrzesinski, Twophoton spectroscopy of ZnSe under uniaxial stress. Phys. Rev. B 52, 14652 (1995) 12. F. Kubacki, J. Gutowski, D. Hommel, M. Heuken, U.W. Pohl, Determination of deformation potentials in ZnSe/GaAs strainedlayer heterostructures. Phys. Rev. B 54, 2028 (1996) 13. L.D. Laude, F.H. Pollak, M. Cardona, Effects of uniaxial stress on the indirect exciton spectrum of silicon. Phys. Rev. B 3, 2623 (1971) 14. H. Mathieu, P. Merle, E.L. Ameziane, B. Archilla, J. Camassel, Deformation potentials of the direct and indirect absorption edges of GaP. Phys. Rev. B 19, 2209 (1984) 15. P. Pfeffer, I. Gorczyca, W. Zawadzki, Theory of freeelectron optical absorption in nGaAs. Solid State Commun. 51, 179 (1984) (Table 1 with references therein) 16. F. Bernardini, V. Fiorentini, D. Vanderbilt, Spontaneous polarization and piezoelectric constants of IIIV nitrides. Phys. Rev. B 56, R10024 (1997) 17. G. Bester, X. Wu, D. Vanderbilt, A. Zunger, Importance of secondorder piezoelectric effects in zincblende semiconductors. Phys. Rev. Lett. 96, 187602 (2006) 18. D.L. Smith, Straingenerated electric fields in [111] growth axis strainedlayer superlattices. Sol. State Commun. 57, 919 (1986) 19. A. BeyaWakata, P.Y. Prodhomme, G. Bester, First and secondorder piezoelectricity in IIIV semiconductors. Phys. Rev. B 84, 195207 (2011) 20. L.C. Lew Yan Voon, M. Willatzen, Electromechanical phenomena in semiconductor nanostructures. J. Appl. Phys. 109, 031101 (2011) 21. O. Ambacher, J. Smart, J.R. Shealy, N.G. Weimann, K. Chu, M. Murphy, W.J. Schaff, L.F. Eastman, R. Dimitrov, L. Wittmer, M. Stutzmann, W. Rieger, J. Hilsenbeck, Twodimensional electron gases induced by spontaneous and piezoelectric polarization charges in N and Gaface AlGaN/GaN heterostructures. J. Appl. Phys. 85, 3222 (1999) 22. U. Rössler (ed.), Semiconductor II–VI and I–VII Compounds; Semimagnetic Compounds. LandoltBörnstein III/41B, revised and updated edition of Vols. III/17 and 22 (Springer, Heidelberg, 1999) 23. O. Ambacher, B. Foutz, J. Smart, J.R. Shealy, N.G. Weimann, K. Chu, M. Murphy, A.J. Sierakowski, W.J. Schaff, L.F. Eastman, R. Dimitrov, A. Mitchell, M. Stutzmann, Twodimensional electron gases induced by spontaneous and piezoelectric polarization in undoped and doped AlGaN/GaN heterostructures. J. Appl. Phys. 87, 334 (2000) 24. Y.P. Varshni, Temperature dependence of the energy gap in semiconductors. Physica 34, 149 (1967) 25. L. Viña, S. Logothetidis, M. Cardona, Temperature dependence of the dielectric function of germanium. Phys. Rev. B 30, 1979 (1984) 26. K.P. O’Donnell, X. Chen, Temperature dependence of semiconductor band gaps. Appl. Phys. Lett. 58, 2924 (1991) 27. R. Pässler, Parameter sets due to fittings of the temperature dependencies of fundamental bandgaps in semiconductors. Phys. Status Solidi B 216, 975 (1999) 28. W. Bludau, A. Onton, W. Heinke, Temperature dependence of the band gap of silicon. J. Appl. Phys. 45, 1846 (1974) 29. R. Pässler, Dispersionrelated description of temperature dependencies of band gaps in semiconductors. Phys. Rev. B 66, 085201 (2002)
172
4 Electronic Properties of Heterostructures
30. I. Vurgaftman, J.R. Meyer, Band parameters for nitrogencontaining semiconductors. J. Appl. Phys. 94, 3675 (2003) 31. S. Adachi, Properties of GroupIV, IIIV and IIVI Semiconductors (Wiley, Chichester, 2005) 32. J.A. Van Vechten, T.K. Bergstresser, Electronic structures of semiconductor alloys. Phys. Rev. B 1, 3351 (1970) 33. C.K. Williams, T.H. Glisson, J.R. Hauser, M.A. Littlejohn, Energy bandgap and lattice constant contours of IIIV quaternary alloys of the form A x B y C z D or ABx C y Dz . J. Electron. Mater. 7, 639 (1978) 34. A. Baldereschi, E. Hess, K. Maschke, H. Neumann, K.R. Schulze, K. Unger, Energy band structure of Alx Ga1−x As. J. Phys. C Solid State Phys. 10, 4709 (1977) 35. A.B. Chen, A. Sher, Electronic structure of IIIV semiconductors and alloys using simple orbitals. Phys. Rev. B 22, 3886 (1980) 36. A.B. Chen, A. Sher, Electronic structure of pseudobinary semiconductor alloys Alx Ga1−x As, GaPx As1−x , and Gax In1−x P. Phys. Rev. B 23, 5360 (1981) 37. J.E. Bernard, A. Zunger, Electronic structure of ZnS, ZnSe, ZnTe, and their pseudobinary alloys. Phys. Rev. B 36, 3199 (1987) 38. A.T. Gorelenok, A.G. Dzigasov, P.P. Moskvin, V.S. Sorokin, I.S. Tarasov, Dependence of the band gap on the composition of In1−x Gax As1−y P y solid solutions. Sov. Phys. Semicond. 15, 1400 (1981) 39. M. Ferhat, F. Bechstedt, Firstprinciples calculations of gap bowing in Inx Ga1−x N and Inx Al1−x N alloys: relation to structural and thermodynamic. Phys. Rev. B 65, 075213 (2002) 40. P.G. Moses, M. Miao, Q. Yan, C.G. Van de Walle, Hybrid functional investigations of band gaps and band alignments for AlN, GaN, InN, and InGaN. J. Chem. Phys. 134, 084703 (2011) 41. L. Cláudio de Carvalho, A. Schleife, J. Furthmüller, F. Bechstedt, Distribution of cations in wurtzitic Inx Ga1−x N and Inx Al1−x N alloys: consequences for energetics and quasiparticle electronic structures. Phys. Rev. B 85, 115121 (2012) 42. E.T. Yu, J.O. McCaldin, T.C. McGill, Band offsets in semiconductor heterojunctions, in Solid State Physics, vol. 46 (Academic Press, New York, 1992), pp. 1–146 43. R.L. Anderson, Experiments on GeGaAs heterojunctions. SolidState Electron. 5, 341 (1962) 44. A.G. Milnes, D.L. Feucht, Heterojunctions and MetalSemiconductor Junctions (Academic Press, New York, 1972) 45. W.R. Frensley, H. Kroemer, Theory of the energyband lineup at an abrupt semiconductor heterojunction. Phys. Rev. B 16, 2642 (1977) 46. W.A. Harrison, Elementary theory of heterojunctions. J. Vac. Sci. Technol. 14, 1016 (1977) 47. S.H. Wei, A. Zunger, Role of d orbitals in valenceband offsets of commonanion semiconductors. Phys. Rev. Lett. 59, 144 (1987) 48. J. Tersoff, Band lineups at IIVI heterojunctions: failure of the commonanion rule. Phys. Rev. Lett. 56, 2755 (1986) 49. A.D. Katnani, G. Margaritondo, Empirical rule to predict heterojunction band discontinuities. J. Appl. Phys. 54, 2522 (1983) 50. A.D. Katnani, R.S. Bauer, Commutativity and transitivity of GaAsAlAsGe(100) band offsets. Phys. Rev. B 33, 1106 (1986) 51. J.M. Langer, H. Heinrich, Deeplevel impurities: a possible guide to prediction of bandedge discontinuities in semiconductor heterojunctions. Phys. Rev. Lett. 55, 1414 (1985) 52. A. Zunger, Electronic structure of 3D transitionatom impurities in semiconductors, in Solid State Physics, vol. 39 (Academic Press, New York, 1986), pp. 275–464 53. C.G. van de Walle, J. Neugebauer, Universal alignment of hydrogen levels in semiconductors, insulators and solutions. Nature 423, 626 (2003) 54. J. Tersoff, Theory of semiconductor heterojunctions: the role of quantum dipoles. Phys. Rev. B 30, 4874 (1984) 55. J. Tersoff, Shottky barrier heights and the continuum of gap states. Phys. Rev. Lett. 52, 465 (1984) 56. D. Mourad, Tightbinding branchpoint energies and band offsets for cubic InN, GaN, AlN, and AlGaN alloys. J. Appl. Phys. 113, 123705 (2013)
References
173
57. M. Landmann, E. Rauls, W.G. Schmidt, Understanding band alignments in semiconductor heterostructures: Composition dependence and typeItypeII transition of natural band offsets in nonpolar zincblende Alx Ga1−x N/Al y Ga1−y N composites. Phys. Rev. B 95, 155310 (2017) 58. C.G. van de Walle, R.M. Martin, Theoretical study of band offsets at semiconductor interfaces. Phys. Rev. B 35, 8154 (1987) 59. M.P.C.M. Krijn, Heterojunction band offsets and effective masses in IIIV quaternary alloys. Semicond. Sci. Technol. 6, 27 (1991) 60. R.G. Dandrea, S. Froyen, A. Zunger, Stability and band offsets of heterovalent superlattices: Si/GaP, Ge/GaAs, and Si/GaAs. Phys. Rev. B 42, 3213 (1990) 61. S. Rubini, E. Milocco, L. Sorba, E. Pelucchi, A. Franciosi, A. Garulli, A. Parisini, Y. Zhuang, G. Bauer, Structural and electronic properties of ZnSe/AlAs heterostructures. Phys. Rev. B 63, 155312 (2001) 62. M. Peressi, N. Binggeli, A. Baldereschi, Band engineering at interfaces: theory and numerical experiments. J. Phys. D 31, 1273 (1998) 63. M. Peressi, A. Baldereschi, Ab initio studies of structural and electronic properties, in Characterization of Semiconductor Heterostructures and Nanostructures, 2nd edn., ed. by C. Lamberti, G. Agostini (Elsevier, Amsterdam, 2013), pp. 21–73 64. W.A. Harrison, E.A. Kraut, J.R. Waldrop, R.W. Grant, Polar heterojunction interfaces. Phys. Rev. B 18, 4402 (1978) 65. A. Kley, J. Neugebauer, Atomic and electronic structure of the GaAs/ZnSe (001) interface. Phys. Rev. B 50, 8616 (1994) 66. R. Nicolini, L. Vanzetti, G. Mula, G. Bratina, L. Sorba, A. Franciosi, M. Peressi, S. Baroni, R. Resta, A. Baldereschi, Local interface composition and band discontinuities in heterovalent heterostructures. Phys. Rev. Lett. 72, 294 (1994) 67. A. Bonanni, L. Vanzetti, L. Sorba, A. Franciosi, M. Lomascolo, P. Prete, R. Cingolani, Optimization of interface parameters and bulk properties in ZnSeGaAs heterostructures. Appl. Phys. Lett. 66, 1092 (1995) 68. N. Kobayashi, Single quantum well photoluminescence in ZnSe/GaAs/AlGaAs grown by migrationenhanced epitaxy. Appl. Phys. Lett. 55, 1235 (1989) 69. M. Städele, J.A. Majewski, P. Vogl, Stability and band offsets of polar GaN/SiC(001) and AlN/SiC(001) interfaces. Phys. Rev. B 56, 6911 (1997) 70. F. Bernardini, M. Peressi, V. Fiorentini, Band offsets and stability of BeTe/ZnSe(100) heterojunctions. Phys. Rev. B 62, R16302 (2000) 71. Z.G. Wang, L.Å. Ledebo, H.G. Grimmeis, Optical properties of iron doped Alx Ga1−x As alloys. J. Appl. Phys. 56, 2762 (1984) 72. Z.G. Wang, L.Å. Ledebo, H.G. Grimmeis, Nuovo Cimento 2D, 1718 (1983) 73. L. Samuelson, S. Nilsson, Z.G. Wang, H.G. Grimmeis, Direct evidence for randomalloy splitting of Cu levels in GaAs1−x Px . Phys. Rev. Lett. 53, 1501 (1984) 74. A.A. Reeder, J.M. Chamberlain, Optical study of the deep manganese acceptor in In1−x Gax P: evidence for vacuumlevel pinning. Solid State Commun. 54, 705 (1985) 75. M. Grundmann, D. Bimberg, Anisotropy effects on excitonic properties in realistic quantum wells. Phys. Rev. B 38, 13486 (1988) 76. S. Adachi, GaAs, AlAs and Alx Ga1−x As: material parameters for use in research and device applications. J. Appl. Phys. 58, R1 (1985) 77. S. Adachi, Physical Properties of IIIV Semiconductor Compounds (Wiley, New York, 1992) 78. D.C. Reynolds, D.C. Look, B. Jogai, C.W. Litton, G. Cantwell, W.C. Harsch, Valenceband ordering in ZnO. Phys. Rev. B 60, 2340 (1999) 79. W. Shan, B.D. Little, A.J. Fischer, J.J. Song, B. Goldenberg, W.G. Perry, M.D. Bremser, R.F. Davis, Binding energy for the intrinsic excitons in wurtzite GaN. Phys. Rev. B 54, 16369 (1996) 80. G. Dorda, Surface quantization in semiconductors, in Festkörperprobleme, ed. by H.J. Queisser. Advances in Solid State Physics, vol. 13 (Pergamon/Vieweg, Braunschweig, 1973), p. 215
174
4 Electronic Properties of Heterostructures
81. U.W. Pohl, Lowdimensional semiconductors, in Handbook of Materials Data, 2nd edn., ed. by H. Warlimont, W. Martienssen (Springer, Cham, 2018), pp. 1077–1100 82. G. Bastard, J.A. Brum, Electronic states in semiconductor heterostructures. IEEE J. Quantum Electron. QE22, 1625 (1986) 83. R. Dingle, W. Wiegmann, C.H. Henry, Quantum states of confined carriers in very thin Alx Ga1−x AsGaAsAlx Ga1−x As heterostructures. Phys. Rev. Lett. 33, 827 (1974) 84. R. Dingle, Confined carrier quantum states in ultrathin semiconductor heterostructures, in Festkörperprobleme, ed. by H.J. Queisser. Advances in Solid State Physics, vol. 15 (Pergamon/Vieweg, Braunschweig, 1975), p. 21 85. K. Suzuki, K. Kanisawa, C. Janer, S. Perraud, K. Takashina, T. Fujisawa, Y. Hirayama, Spatial imaging of twodimensional electronic states in semiconductor quantum wells. Phys. Rev. Lett. 98, 136802 (2007) 86. R.C. Miller, D.A. Kleiman, W.A. Nordland Jr., A.C. Gossard, Luminescence studies of optically pumped quantum wells in GaAsAlx Ga1−x As multilayer structures. Phys. Rev. B 22, 863 (1980) 87. P.L. Gourley, R.M. Biefeld, Quantum size effects in GaAs/GaAsx P1−x strainedlayer superlattices. Appl. Phys. Lett. 45, 749 (1984) 88. R.C. Miller, D.A. Kleiman, O. Munteanu, W.T. Tsang, New transitions in the photoluminescence of GaAs quantum wells. Appl. Phys. Lett. 39, 1 (1981) 89. R.L. Greene, K.K. Bajaj, D.E. Phelps, Energy levels of Wannier excitons in GaAsGa1−x Alx As quantumwell structures. Phys. Rev. B 29, 1807 (1984) 90. B. Deveaud, J.Y. Emery, A. Chomette, B. Lambert, M. Baudet, Observation of onemonolayer size fluctuations in a GaAs/GaAlAs superlattice. Appl. Phys. Lett. 45, 1078 (1984) 91. A. Forchel, H. Leier, B.E. Maile, R. Germann, Fabrication and optical spectroscopy of ultra small III–V compound semiconductor structures, in Festkörperprobleme, ed. by U. Rössler. Advances in Solid State Physics, vol. 28 (Pergamon/Vieweg, Braunschweig, 1988), p. 99 92. X.L. Wang, V. Voliotis, Epitaxial growth and optical properties of semiconductor quantum wires. J. Appl. Phys. 99, 121301 (2006) 93. F. Vouilloz, D.Y. Oberli, M.A. Dupertuis, A. Gustafsson, F. Reinhardt, E. Kapon, Polarization anisotropy and valence band mixing in semiconductor quantum wires. Phys. Rev. Lett. 78, 1580 (1997) 94. F. Vouilloz, D.Y. Oberli, M.A. Dupertuis, A. Gustafsson, F. Reinhardt, E. Kapon, Effect of lateral confinement on valenceband mixing and polarization anisotropy in quantum wires. Phys. Rev. B 57, 12378 (1998) 95. Z.Y. Deng, X. Chen, T. Ohji, T. Kobayashi, Subband structures and exciton and impurity states in Vshaped GaAsGa1−x Alx As quantum wires. Phys. Rev. B 61, 15905 (2000) 96. E. Martinet, M.A. Dupertuis, F. Reinhardt, G. Biasiol, E. Kapon, O. Stier, M. Grundmann, D. Bimberg, Separation of strain and quantumconfinement effects in the optical spectra of quantum wires. Phys. Rev. B 61, 4488 (2000) 97. E. Kapon, G. Biasiol, D.M. Hwang, E. Colas, M. Walther, Selfordering mechanism of quantum wires grown on nonplanar substrates. SolidState Electron. 40, 815 (1996) 98. T. Someya, H. Akiyama, H. Sakaki, Enhanced binding energy of onedimensional excitons in quantum wires. Phys. Rev. Lett. 76, 2965 (1996) 99. T. Ogawa, T. Takagahara, An exact treatment of excitonic effects. Phys. Rev. B 44, 8138 (1991) 100. D. Gershoni, M. Katz, W. Wegscheider, L.N. Pfeiffer, R.A. Logan, K. West, Radiative lifetimes of excitons in quantum wires. Phys. Rev. B 50, 8930 (1994) 101. D. Bimberg, M. Grundmann, N.N. Ledentsov, Quantum Dot Heterostructures (Wiley, Chichester, 1999) 102. S. Rodt, A. Schliwa, K. Pötschke, F. Guffarth, D. Bimberg, Correlation and few particle properties of selforganized InAs/GaAs quantum dots. Phys. Rev. B 71, 155325 (2005) 103. A. Schliwa, M. Winkelnkemper, D. Bimberg, Impact of size, shape, and composition on piezoelectric effects and electronic properties of In(Ga)As/GaAs quantum dots. Phys. Rev. B 76, 205324 (2007)
References
175
104. T. Maltezopoulos, A. Bolz, C. Meyer, C. Heyn, W. Hansen, M. Morgenstern, R. Wiesendanger, Wavefunction mapping of InAs quantum dots by scanning tunneling spectroscopy. Phys. Rev. Lett. 91, 196804 (2003) 105. A. Urbieta, B. Grandidier, J.P. Nys, D. Deresmes, D. Stiévenard, A. Lemaître, G. Patriarche, Y.M. Niquet, Scanning tunneling spectroscopy of cleaved InAs/GaAs quantum dots at low temperatures. Phys. Rev. B 77, 155313 (2008) 106. O. Stier, M. Grundmann, D. Bimberg, Electronic and optical properties of strained quantum dots modeled by 8band kp theory. Phys. Rev. B 59, 5688 (1999) 107. M. Scholz, S. Büttner, O. Benson, A.I. Toropov, A.K. Bakarov, A.K. Kalagin, A. Lochmann, E. Stock, O. Schulz, F. Hopfer, V.A. Haisler, D. Bimberg, Nonclassical light emission from a single electrically driven quantum dot. Opt. Express 15, 9107 (2007) 108. F. Guffarth, S. Rodt, A. Schliwa, K. Pötschke, D. Bimberg, Manyparticle effects in selforganized quantum dots. Phys. E 25, 261 (2004) 109. B. Fain, I. RobertPhilip, C. David, Z.Z. Wang, I. Sagnes, J.C. Girard, Discretization of electronic states in large InAsP/InP multilevel quantum dots probed by scanning tunneling spectroscopy. Phys Rev. Lett. 108, 126808 (2012) 110. K. Teichmann, M. Wenderoth, H. Prüser, K. Pierz, H.W. Schumacher, R.G. Ulbrich, Harmonic oscillator wave functions of a selfassembled InAs quantum dot measured by scanning tunneling microscopy. Nano Lett. 13, 3571 (2013) 111. P. Vashishta, R.K. Kalia, Universal behavior of exchangecorrelation energy in electronhole liquid. Phys. Rev. B 25, 6492 (1982) 112. G. Tränkle, E. Lach, A. Forchel, F. Scholz, C. Ell, H. Haug, G. Weimann, G. Griffiths, H. Kroemer, S. Subbanna, General relation between bandgap renormalization and carrier density in twodimensional electronhole plasmas. Phys. Rev. B 36, 6712 (1987) 113. R. Ambigapathy, I. BarJoseph, D.Y. Oberli, S. Haacke, M.J. Brasil, F. Reinhard, E. Kapon, B. Deveaud, Coulomb correlation and band gap renormalization at high carrier densities in quantum wires. Phys. Rev. Lett. 78, 3579 (1997) 114. R. Heitz, F. Guffarth, I. Mukhametzhanov, M. Grundmann, A. Madhukar, D. Bimberg, Manybody effects on the optical spectra of InAs/GaAs quantum dots. Phys. Rev. B 62, 16881 (2000) 115. U.W. Pohl, InAs/GaAs quantum dots with multimodal size distribution, in Selfassembled Quantum Dots, ed. by Z.M. Wang (Springer, New York, 2008), pp. 43–66, Chap. 3 116. U.W. Pohl, K. Pötschke, A. Schliwa, F. Guffarth, D. Bimberg, N.D. Zakharov, P. Werner, M.B. Lifshits, V.A. Shchukin, D.E. Jesson, Evolution of a multimodal distribution of selforganized InAs/GaAs quantum dots. Phys. Rev. B 72, 245332 (2005) 117. R. Heitz, F. Guffarth, K. Pötschke, A. Schliwa, D. Bimberg, N.D. Zakharov, P. Werner, Shelllike formation of selforganized InAs/GaAs quantum dots. Phys. Rev. B 71, 045325 (2005) 118. S. Raymond, S. Studenikin, S.J. Cheng, M. PioroLadrière, M. Ciorga, P.J. Poole, M.D. Robertson, Families of islands in InAs/InP selfassembled quantum dots: a census obtained from magnetophotoluminescence. Semicond. Sci. Technol. 18, 385 (2003) 119. S. Rodt, R. Seguin, A. Schliwa, F. Guffarth, K. Pötschke, U.W. Pohl, D. Bimberg, Sizedependent binding energies and finestructure splitting of excitonic complexes in single InAs/GaAs quantum dots. J. Lumin. 122–123, 735 (2007) 120. S. Rodt, A. Schliwa, K. Pötschke, F. Guffarth, D. Bimberg, Correlation of structural and fewparticle properties of selforganized InAs/GaAs quantum dots. Phys. Rev. B 71, 155325 (2005) 121. U.W. Pohl, R. Seguin, S. Rodt, A. Schliwa, K. Pötschke, D. Bimberg, Control of structural and excitonic properties of selforganized InAs/GaAs quantum dots. Phys. E 35, 285 (2006)
Chapter 5
Electronic Properties of Organic Semiconductors
Abstract The highest occupied und lowest unoccupied molecular orbitals (HOMO and LUMO) form bands in organic semiconductors corresponding to valence and conduction bands of their inorganic counterparts. Organic crystals have comparatively narrow bands and large bandgaps, and they feature strong anisotropies. The Gaussian density of states of HOMO and LUMO supplemented by defect states produces a substantial tailing of the bands into the bandgap. The strong structural and electronic relaxation occurring when a molecule is charged leads to strongly bound Frenkel excitons and to a pronounced polaron character of mobile carriers. The small polaron radius and the high density of defects lead to a prevailing, thermally activated hopping conductance with a relatively low carrier mobility. Band conductance with an increased mobility at low temperature may be found at reduced scattering rates. Molecules at the interfaces between two organic semiconductors have often weak interaction, yielding a band alignment largely described by matching the vacuum levels. Molecular interaction at interfaces to metals is generally strong, creating surface dipoles and an often observed pinning of the Fermi level.
5.1 Band Structure of Organic Crystals Organic semiconductors comprise smallmolecule crystals and polymers. They are employed today in a wide field of applications, e.g., in organic LEDs (OLEDs) and displays, radiofrequency tags, and solar cells; reviews are given in, e.g., [1–5]. The electronic properties of organic crystals show characteristic features usually not observed in inorganic solids, originating from the molecular structure.
© Springer Nature Switzerland AG 2020 U. W. Pohl, Epitaxy of Semiconductors, Graduate Texts in Physics, https://doi.org/10.1007/9783030438692_5
177
178
5 Electronic Properties of Organic Semiconductors
5.1.1 Highest Occupied and Lowest Unoccupied Molecular Orbitals Carriers in Organic and Inorganic Crystals Organic crystals are composed of molecules as building blocks instead of atoms (Sect. 3.1). As a consequence, the periodicity approach used to describe free carriers in the periodic potential of inorganic solids does not apply well for describing the electronic properties of organic solids: while carriers may move well along the backbone of a linear molecule, they experience a substantial energy barrier for the transfer to the adjacent molecule. This barrier originates from the weak intermolecular interaction and the resulting large distance between atoms of neighboring molecules. In addition the strong disorder in organic crystals leads to a Gaussian broadening of the electronic density of states at the band edge with trap states in the bandgap. Transport properties are therefore often rather described by a hopping conductance than by a bandlike conductance. Free carriers in organic crystals differ from those in inorganic solids. The reason is the strong structural relaxation of the lattice occurring when a charge is introduced to an organic molecule. This relaxation accompanies the moving carrier, affecting his effective mass. Such a phonondressed carrier in an organic crystal is conveniently described as a small polaron (Sect. 5.2.1). Lattice polarization by free carriers is also observed in inorganic semiconductors, but the effect is much smaller; their weak electronphonon interaction is described by a large polaron with a small Fröhlich coupling constant α, leading to a merely slight increase of the effective mass. Electronic Levels of Molecules The origin of a band structure in an organic crystal can be illustrated by comparing energy levels of a free molecule with levels of the organic crystal. The simplified level scheme of an isolated single molecule is depicted in Fig. 5.1. The molecule has an even number of electrons if it is electrically neutral and not a radical. The highest occupied molecular orbital (HOMO) in the electronic ground state of the molecule is occupied by 2 electrons with opposite spin. It is hence a singlet state (S 0 in Fig. 5.1) Fig. 5.1 Schematic of the energy levels of a single molecule (gas phase, left) and of a molecule crystal (right); I g , Ag , I c , and Ac denote respectively the ionization energies I and electron affinities A of the molecule in the gas phase and in the crystal; Pn and Pp signify the polarization energies of an electron and a hole in the molecule crystal
E 0
vacuum Ig Ag
Pn
Ic Ac LUMO (CB) S1 exciton
S1
T1 exciton
T1 S0 molecule
S0 HOMO (VB) Pp
crystal
5.1 Band Structure of Organic Crystals
179
with total spin S = 0; the first excited singlet state is S 1 . There exists also a triplet state labelled T 1 with one electron in the HOMO state and one electron in the excited state with parallel spin, yielding a total spin S = 1; the energy of T 1 is larger than that of S 0 . Further excited states S 2 and T 2 may exist with an energy separation to S 0 below the ionization energy I g , but the lifetime of an electron excited to such states is very small compared to the lifetime in the states S 1 and T 1 . These higher excited states of the singlet and triplet manifolds are not shown in Fig. 5.1 for clarity. The ionization energy I g represents the energy required to remove the most weakly bound electron from the ground state of an isolated molecule and is readily accessible in experiment. On the other hand, an energy referred to as electron affinity Ag is released, if an additional electron is bound to an isolated molecule to form a negatively charged molecular ion. If the electron is removed from a molecule in the environment of a crystal lattice, the required energy I c is smaller than I g . Organic molecules are strongly polarized when they are charged; removing an electron from the HOMO forms a positively charged radical with a mobile hole, and atoms in the molecule and in neighboring molecules rearrange. The related polarization energy Pp is large (typically above 1 eV) and represents the difference between the ionization energies: Pp = Ig − Ic . The polarization of the crystal is expressed by a dielectric constant of typically about 3; the reduced ionization energy can hence also be attributed to the effect of the polarizable medium when negative and positive charges are separated. Due to relaxation upon ionization also the electron affinity Ag of an isolated molecule is altered in the crystal; it is increased by a polarization energy Pn to a value Ac . The electron added to the molecule of a crystal is mobile similar to the hole left by a removed electron. The energies of these two transport states are separated by an energy gap E g , which in the case of Pp = Pn ≡ P is given by [6] E g = Ic − Ac = Ig − Ag − 2P = 2Ic − Ig − Ag ;
(5.1)
in (5.1) all quantities are assumed positive (see also Fig. 5.2). E g is the bandgap energy for a single carrier and refers to carrier generation in either the HOMO state or the lowest unoccupied (LUMO) state. The energy gap E g and its position with respect to the vacuum level depend on the spatial extent of the delocalized π electrons or holes in the molecules of the crystal; this dependence is illustrated for acenes (Sect. 3.1.2) in Fig. 5.2. In an anthracene crystal the bandgap energy E g is 4.1 eV; this energy is required to remove an electron from the HOMO level to a quasifree state of the molecule, when the positive charge left in the HOMO is not correlated. The quasifree state is the lowest unoccupied molecular orbital, the LUMO level; in analogy to inorganic semiconductors the LUMO in organic semiconductors is referred to as conduction band, and the HOMO is called valence band. The S 1 state indicated in Fig. 5.1 lies below the LUMO level; in this state the electron is still bound to this positive charge, forming an exciton (Sect. 5.1.3); the excitation energy of the S 1 exciton in anthracene is about 0.5 eV lower than E g . This energy difference represents the
180
5 Electronic Properties of Organic Semiconductors
E (eV)
0
gas solid (?)
Ic Ac Ig Ag
(?)
2
Pn
LUMO (CB)
Eg
4
Pp
6 8
Evac
HOMO (VB)
(?)
10
benzene naphthalene anthracene tetracene
pentacene
Fig. 5.2 Ionization energies of the highest occupied level and binding energies of the lowest unoccupied level for various oligoacenes in the gas phase (horizontal bars left of gray vertical lines, referring to I g and Ag ) and in a crystal (right bars, referring to I c and Ac ). Reproduced with permission from [6], © 1974 Springer Nature
binding energy of the exciton; its value is much larger than values found in inorganic semiconductors. A large binding energy corresponds to a strong spatial localization and a strong structural relaxation of the molecules, both being typical features of excitons in organic crystals.
5.1.2 Bands and Bandgaps in Organic Crystals In organic semiconductors often bandlike conduction similar to that of inorganic semiconductors is observed. The energy of carriers is then well characterized in terms of a band structure. The electronic band structure of an anthracene crystal calculated using the tightbinding approach is given in Fig. 5.3. The dispersions E(k) refer to directions of the monoclinic Brillouin zone shown in the inset; d1 = (½½0) and d2 = (−½½0) are nextneighbor directions in the xy plane. Anthracene has two equivalent molecules with different orientations in the unit cell; both, the LUMO and HOMO levels are composed of symmetrical and asymmetric linear combinations of molecular orbitals of the two molecules, leading to a twofold splitting. The degeneracy of k x and k y at the edge of the Brillouin zone in the xy plane originates from a crystal glideplane symmetry; no such symmetry exists in triclinic crystals like
5.1 Band Structure of Organic Crystals
181 0.005
Anthracene
300
DOS
kc LUMO
Energy (meV)
200
ka
kc
100
kd1
A
0
kb
Z
Y C
ka
ka
kb
100
kb
kd2 200
kc
300
kc
200
Energy (meV)
0.01
ka
HOMO
100
kb
kd1
ka
0
kc 100
kd 2 200
0
0.2
0.4
0.6
DOS
kb 0.8
1
0.005 0.01 0.015
k / kmax Fig. 5.3 Dispersion E(k) and density of states (DOS) of the lowest unoccupied and the highest occupied molecularorbital (LUMO and HOMO) bands for an anthracene crystal. k x to k z signify crystallographic directions of the monoclinic Brillouin zone depicted in the inset of the upper panel, k d1 and k d2 refer to nearestneighbor directions. Reproduced with permission from [7] © 2003 AIP
tetracene and pentacene, where this degeneracy is lifted. Along the nextneighbor directions d1 and d2 there is a substantial overlap of orbitals of adjacent molecules; consequently the dispersions along kd1 and kd2 are quite large. The dispersion along k z is very small, and a large gap occurs between upper and lower band. These features originate in this direction from small interactions of molecules located in adjacent layers and is often found in organic crystals with herringbone packing [7]. The density of states of the LUMO and HOMO bands plotted at the right side of Fig. 5.3 reflects the inverse slope of the contributing dispersion curves. Rubrene crystals also show bandlike conduction; the orthorhombic phase considered in Fig. 5.4 comprises two differently aligned molecule pairs per unit cell in
182
3.0
Rubrene 2.5
LUMO 2.0
Energy (eV)
Fig. 5.4 Electronic dispersion of the LUMO and HOMO bands for a rubrene crystal, calculated using density functional theory and the G0 W 0 approximation; reproduced with permission from [9], © 2013 APS
5 Electronic Properties of Organic Semiconductors
1.5 1.0 0.5
HOMO
0 0.5 1.0
Z
Y
X
Wave vector k
a herringbone packing. The calculated direct bandgap of 2.34 eV agrees reasonably with an experimental optical bandgap of 2.2 eV. The HOMO bands of rubrene show a large dispersion along Y and only minor dispersion along Z, in accordance with angleresolved photoelectronspectroscopy data [8] and the experimental large anisotropy of carrier transport. Width of Electronic Bands The width of the conduction and valence bands in organic semiconductors is generally quite narrow due to the weak intermolecular van der Waals bonds. The intermolecular interaction is usually expressed in terms of a transfer integral outlined in Sect. 5.2.2. In the tightbinding approximation of a onedimensional molecule chain, the total bandwidth equals four times the transfer integral between neighboring molecules. The bandwidth for any molecular packing can be expressed from the amplitude of the transfer integrals between the various interacting units [10]. Data of the lowest unoccupied and the highest occupied molecularorbital (LUMO and HOMO) bands for some organic semiconductors are given in Table 5.1. The bandwidth is maximum at T → 0. At increasing temperature the bandwidth is progressively reduced (Fig. 5.5) by an increased electronphonon coupling and a consequently reduced transfer integral between adjacent molecules [11, 12]. The width of the bands illustrated in Fig. 5.5 is intimately connected with the temperaturedependent effective mass of electrons and holes. The minimum limit at low temperature is obtained from the curvature of the HOMO and LUMO bands resulting from bandstructure calculations. Instead of effective masses generally the mobility is reported for organic semiconductors (Sect. 5.2.2). This quantity is readily
5.1 Band Structure of Organic Crystals Table 5.1 Calculated total bandwidth W of excess electron and hole bands for crystalline organic semiconductors
183
Crystal
Bandwidth W (meV) HOMO (meV)
LUMO
Naphthalenea
409
372
Anthracenea
509
508
Tetracenea
625
502
Pentacenea
738
728
Rubreneb
520
230
96
260
CuPcc a Reference
[7] [9] c Reference [13] b Reference
400
LUMO
300 200
Bandwidth (meV)
Fig. 5.5 Temperaturedependent narrowing of the LUMO and HOMO bands in anthracene and tetracene crystals, calculated from a semiempirical approach employing Buckingham atomatom potentials. Reproduced with permission from [12] © 2004 APS
Tetracene
Anthracene 100 0
HOMO
300
Tetracene 200 100 0
Anthracene 0
50
100
150
200
250
300
Temperature (K)
accessible in experiment and usually much larger for holes than for electrons. Furthermore, it is strongly anisotropic due to the low symmetry of molecules and crystal lattices, and hence the oriental dependence of the transfer integrals. Transport Bandgap and Optical Bandgap The polarization energy P in organic crystals in (5.1) has an electronic and a vibronic component. If an electron is added to a molecule, the neighboring molecules are polarized by the negative charge in their vicinity. The characteristic response time for this electronic polarization is on the order of the oscillation period in an optical transition.
184
5 Electronic Properties of Organic Semiconductors
This time is much shorter than that of a vibronic oscillation; the electronic polarization of the molecular neighborhood thus follows the movement of a quasifree electron, thereby affecting its effective mass. The quasifree electron in the LUMO and its surrounding polarization cloud combined form a negative polaron; correspondingly a positive charge in the HOMO builds a positive polaron. The polaron character of mobile carriers in organic crystals is usually not explicitly considered; in analogy to the quasiparticles of inorganic semiconductors the carriers are simply termed electrons and holes. The vibronic component of the polarization energy is related to a relaxation of the crystal lattice in the environment of the charged molecule. The characteristic response time is given by the period of a phonon oscillation and therefore much longer than the electronic response. Vibronic relaxation provides a contribution on the order of 5–10% to the polarization energy. After ionization of a molecule in a crystal by a photon the ensuing bandgap energy is hence slightly decreased; the adiabatic bandgap resulting from ionization energy, electron affinity, and electronic transport including the vibronic polarization is somewhat larger than the transport gap E g contribution. When an electron is optically excited from the HOMO an onset of absorption is already observed well below the energy of the transport gap. The longwavelength edge of absorption spectra or shortwavelength edge of luminescence spectra originates from S 0 – S 1 transitions of the singlet exciton, see Figs. 5.1 and 5.8. The opt energy of this edge is called optical bandgap E g . The chargeseparation energy, transport opt Eg − E g , is the binding energy E X of the exciton. This quantity is far larger than in inorganic semiconductors [14]. Figure 5.6 shows the transport and optical bandgaps for many organic semiconductors; their difference is given by the separation of the straight line and the dotted line, illustrating an increase of the exciton binding energy for larger bandgap energies. This trend reflects the decrease of the permittivity ε for larger bandgap and the inverse dependence E X ∝ ε−1 [15], which differs from the dependence (4.49) observed for Wannier excitons. The bandgap of organic semiconductors is generally large (typically well above 2 eV). The thermal activation of carriers from HOMO to LUMO states is therefore negligible: pure organic solids are often insulating. Since reliable and robust doping proved difficult for many organic compounds, charge carriers (both, electrons and holes) are generally injected from the contacts into organic semiconductors used for devices. transport can be directly obtained from electron The energy of the transport gap E g spectroscopy: ultraviolet photoelectron spectroscopy (UPS) measures the HOMO energy, and inverse photoelectron spectroscopy (IPES) determines the LUMO energy. Data for some organic semiconductors are given in Table 5.2. It should be noted that energy values reported for organic crystals show a large scatter due to differences in used samples, experimental conditions, or due to assumptions in calculations.
5.1 Band Structure of Organic Crystals Fig. 5.6 Transportbandgap transport energy E g versus opt optical bandgap energy E g for 24 organic semiconductors. Numbers at data points refer to the compounds listed in Table 5.2. The solid line signifies a linear fit to the data, and the dashed straight line represents transport opt Eg = Eg . Reproduced with permission from [16], © 2009 Elsevier
185
8
Eg
transport
(eV)
7
1
Organic Semiconductors
6 2
5 4 3 2 1
3
5 4 7 8
6
9
2
3
4
5
opt E g (eV)
Table 5.2 LUMO and HOMO energies for organic semiconductors measured by photoelectron transport
spectroscopy (IPES and UPS, respectively), transport bandgap E g
= E LUMO −E HOMO , and
opt
measured optical bandgap E g . The numbers in the first column refer to those in Fig. 5.6; data from [16] No
Compound
E LUMO (eV)
E HOMO (eV)
transport
Eg
(eV)
opt
Eg
1
Benzene
−0.4
−7.58
7.2
4.68
2
Naphthalene
−1.1
−6.4
5.3
4.00
3
Anthracene
−1.7
−5.70
4.0
3.25
4
Tetracene
−1.8
−5.10
3.3
2.51
5
Alq3
−1.96
−5.65
3.69
2.75
6
Perylene
−2.5
−5.2
2.7
2.83
7
αHexathiophene
−2.57
−5.3
2.7
2.43
8
CuPc
−4.82
2.17
1.80
9
Pentacene
−4.85
2.1
2.06
2.65 −2.8
(eV)
5.1.3 Excitons in Organic Crystals Excitons are eigenstates of correlated electronhole pairs with energies below the bandgap energy by an amount given by the binding energy of the exciton. In estimating the binding energy, the band structure of valence and conduction bands must be considered, entering into the effective mass and the dielectric function. An exciton can be modeled by an electron and a hole, circling each other much like the electron and proton in a hydrogen atom, except that they have almost the same mass; hence, in a semiclassical model, their center of rotation lies closer to the middle on their interconnecting axis as illustrated in Fig. 5.7. Depending on the reduced exciton mass
186
5 Electronic Properties of Organic Semiconductors
and dielectric constant, we distinguish between Wannier excitons, which extend over many lattice constants, and Frenkel excitons, which have a radius comparable to the interatomic distance. Frenkel excitons become localized and resemble an atomic excited state [17]. The large Wannier excitons are common in inorganic semiconductors; they are well described by a hydrogen model with the proton and electron masses replaced by the effective masses of hole and electron, and a screened Coulomb potential. The screening of the Coulomb potential is appropriately described by the static dielectric constant εstat or, in case of a stronger lattice interaction including the optical dielectric −1 −1 −1 +εstat ) , constant εopt (also named ε∞ ), by an effective dielectric constant ε∗ = (εopt which provides less shielding. Wannier excitons are free to move through the lattice and may be bound to defects or may be confined in quantum structures as described in Sect. 4.3. The binding energy of free excitons is generally small and typically on the order of 10 meV, see Table 4.8. Frenkel excitons [19] are wellknown from ionic crystals with relatively small dielectric constants, large effective masses, and strong carrierlattice coupling resulting in large structural relaxations. These excitons show relatively large binding energies, usually in excess of 0.5 eV; they cannot be described in a simple hydrogenic model. Frenkel excitons are observed particularly in the organic molecular crystals, where the binding forces within the molecule (covalent) are large compared to the binding forces between the molecules (van der Waals interaction, Sect. 3.1.1). Here localized excited states within a molecule are favored. The binding energy increases for larger bandgap energy from about 0.25 eV for 2 eV transport bandgap to 1.5 eV transport = 6 eV, see Fig. 5.6. for E g In contrast to most inorganic semiconductors, the excited states in molecular semiconductors are highly localized, with the charge densities typically confined. The localization of electron and hole on the same molecule leads to a large exchange splitting, generating the distinct states of singlets S (spin 0) and triplets T (spin 1); The energy difference between the respective excited states S 1 and T 1 in organic
(a)
(b)
Fig. 5.7 Schematic model of an exciton. a Wannier exciton in an inorganic semiconductor with a large radius extending over many lattice constants. b Frenkel exciton with a small radius localized at a molecule in an organic crystal. Reproduced with permission from [18], (c) 2018 Springer
5.1 Band Structure of Organic Crystals
(b)
S2 S1 Excitation Singlet emission
S0
T3 T2 T1 Triplet emission
Luminescence intensity (arb. u.)
(a) E
187
S1
Anthracene T = 300 K cw exc. 365 nm
S0 00 T1
S0 x5
400
500
600
700
800
900
Wavelength (nm)
Fig. 5.8 a Singlettriplet exciton schematics with ground state S 0 , excited singlet states S 1 and S 2 , and triplet states T 1 to T 3 ; occupied spin states are indicated beside the electronic levels. b Optical emission spectrum of singletsinglet and singlettriplet excitons in an anthracene crystal, measured at room temperature with excitation at 365 nm. Reproduced with permission from [25], © 2014, Springer Nature
molecules ranges from 50 meV to more than 1 eV [20, 21]. The ground state of neutral molecules is a singlet state—see Fig. 5.8a. In recombination, the singletsinglet transition is allowed, yielding a strong luminescence called fluorescence in organic semiconductors. The tripletsinglet transition is spinforbidden; consequently, the triplet state has a long lifetime, depending on possible tripletsinglet mixing, and a much weaker luminescence referred to as phosphorescence. Such singlet and triplet excitons are common in organic semiconductors [22]. The luminescence of singlet excitons is employed in organic LED (OLED) devices used to create displays for, e.g., mobile phones or TV screens, or for solidstate lighting [23, 24]. The luminescence of molecular singlet and triplet Frenkel excitons is shown in Fig. 5.8. Panel (a) gives the level scheme of organic molecules with an even number of π electrons (i.e., no ions or radicals); the photoluminescence spectrum for anthracene is shown in panel (b). The transition near 678 nm labelled 00 refers to the zerophonon line of the T 1 → S 0 emission; transitions at longer wavelength originate from additional emissions involving molecule and lattice vibrations. The spinforbidden T 1 → S 0 transition is much weaker than the allowed S 1 → S 0 transition with an onset near 380 nm, and its lifetime of 8 ms is correspondingly much longer than the 6 ns of the allowed emission.
5.2 Transport in Organic Semiconductors Organic solids are easily polarized, as evidenced by the large difference between transport gap and optical bandgap pointed out in Sect. 5.1.2. This property leads to a pronounced polaron character of mobile carriers with a low mobility, and to the large binding energy of excitons discussed above. In the following we consider the
188
5 Electronic Properties of Organic Semiconductors
polaron behavior in more detail and consequences for the carrier transport in organic semiconductors.
5.2.1 Polarons In the effectivemass picture of a free carrier its interaction with the induced motion of surrounding lattice atoms is usually neglected. This adiabatic approximation applies well for inorganic semiconductors, particularly for those with a high degree of covalent bonding; the coupling of the carrier to the lattice may then be treated as a small correction to the effective mass. The lattice polarization by the carrier becomes more significant in crystals with a strong ionic character and a large bandgap energy, such as in II–VI semiconductors and IIInitrides; it is especially pronounced in alkali halides. The polarization of the lattice by a free carrier is commonly expressed in terms of an interaction via phonons. The moving carrier is considered a superposition of the moving charge and a phonon cloud, which accounts for the distortion of the surrounding lattice and travels with the carrier. This phonondressed carrier is described as a quasiparticle referred to as polaron. Large Polarons If the radius of the phonon cloud is larger than a lattice constant the carrier is termed a large polaron, in contrast to a small polaron with a strong lattice polarization occurring within a unit cell. The coupling via longitudinal optical phonons is found to be dominant and described by the dimensionless Fröhlich coupling constant 1 e2 α= 4π ε0
1 m∗ 1 , − 2ωLO εopt εstat
(5.2)
with the static and optical dielectric constants εstat and εopt , and the energy of an effective phonon ωLO ; m* denotes the effective mass of the carrier in the rigid lattice without polaron effect. In semiconductors without ionic character of the bonding (Si and Ge) the static and optical dielectric constants are equal, yielding α = 0; in ionic compounds εstat and εopt differ substantially. Semiconductors have typically α values below unity, e.g., GaAs (0.068), GaP (0.201), GaN (0.48) or the II–VI compounds ZnSe (0.43), ZnS (0.63), ZnO (1.19); alkali halides have much stronger coupling: KI (2.50), KBr (3.05), KCl (3.44). The effective mass of a polaron mpol exceeds the effective mass m* of a carrier moving through a rigid lattice. In the framework of Fröhlich coupling the mass of a large polaron is approximately given by
5.2 Transport in Organic Semiconductors
m∗ m pol,large ∼ for α ≤ 1. = 1 − α6
189
(5.3)
With α 1 we note an only small deviation from m*. For stronger coupling 2α 4 ∗ m is used [26]. expressed by α 1 the approximation m pol, large ∼ = 3π Small Polarons When the ion displacement in the environment of the carrier by its Coulomb interaction is very large, the carrier gets trapped in a potential well created by this distortion. The charge is then typically confined to a volume of one unit cell or less, and the quasiparticle is called a small polaron. The strength of the electronlattice interaction is a distinguishing parameter between the selftrapped small and the mobile large polaron: selftrapping is observed when the coupling constant is larger than 5. Small polarons are described by ab initio tightbinding calculations to account for the movement of all atoms in the environment. While the large polaron moves much like a quasifree carrier described by the Boltzmann equation with scattering events, the small polaron moves via hopping between neighboring ions. The effective mass of small polarons is approximately given by [27] m ∗α2 . m pol,small ∼ = 48
(5.4)
Examples for materials with small polarons are generally narrowband semiconductors with large values of α (~10): the band conductivity is usually disturbed by phonon scattering if the bandwidth is narrow. This feature is found in organic crystals (see Sect. 5.1.2), and hopping mechanisms may prevail even if the material has crystalline structure. The bandwidth is maximum at T → 0; at increasing temperature the bandwidth is progressively reduced by an increased electronphonon coupling (Fig. 5.5), and the polaron mass consequently increases. The carriers get more localized over single molecules (or molecule chains), leaving only transport by a thermally activated hopping mechanism. The transport thus gradually changes from coherent bandlike motion at low temperatures to phononassisted hopping transport at high temperature. This transition occurs in oligoacenes at about room temperature [7]. Small polarons occur also in inorganic solids, particularly in oxides such as NiO or BaTiO3 . Following the generally accepted usage the mass of mobile carriers is in the following referred to as effective mass (denoted m*), even if the polaron effect leads to selftrapping and hopping conductance with a low mobility.
190
5 Electronic Properties of Organic Semiconductors
5.2.2 Mobility of Carriers in Organic Semiconductors Band Conductance in Organic Crystals The mobility of mobile carriers is defined by
μ=
q τ, m∗
(5.5)
with the effective mass m* and charge q of the carrier, and a mean time τ between scattering events. In organic crystals the mobility at room temperature is usually below 1 cm2 /(Vs), often orders of magnitude smaller, compared to values of 103 cm2 /(Vs) for inorganic semiconductors. A major reason is the poor structural perfection of organic crystals, which creates trap levels and scattering centers. Other reasons are a pronounced polaron character of carriers, and particularly the weak intermolecular contact in an organic crystal. The filled HOMO and the empty LUMO levels of each molecule are separated from those of neighboring molecules by a potential barrier. The barrier originates from the weak intermolecular van der Waals interaction, leading to a predominant localization of the HOMO and LUMO wave functions in each molecule. If the intermolecular barrier is low, bands similar to those in inorganic semiconductors are created; the stronger coupling is related to a larger overlap of wave functions of adjacent molecules. Higher barriers may still allow for conductivity by phononassisted hopping considered further below. The intermolecular barriers are expressed in terms of intermolecular transfer integrals. These quantities describe the electronic coupling between molecular orbitals of adjacent molecules (HOMOs and LUMOs) and depend sensitively on the spacing and relative orientations of the molecules. For acenes typical values are in the range of some tens of meV [7]. In the regime of band conduction the bands are formed by linear combinations of the orbitals of each molecule, and the transfer integral V affects the effective mass of a mobile carrier moving in a given direction by m∗ =
2 , 2V d 2
(5.6)
where d is the distance of adjacent molecules in the considered direction. In the regime of hopping conduction the transfer integral enters the chargetransfer rate k for hopping transitions between adjacent molecules [28], V 2 k=
λ π exp − . λkT 4kT
(5.7)
In this Marcus expression λ is the is the reorganization energy describing the vibrational relaxation in the vicinity of the mobile charge carrier; this energy is proportional to the electronphonon coupling strength γ and can be described by λ = 2γ 2 ω, with the characteristic phonon mode ω [29].
5.2 Transport in Organic Semiconductors
191
Band conductance is found particularly in smallmolecule crystals. Singlecomponent semiconductors such as the acenes are usually good insulators, but may become photoconductive with sufficient optical excitation and also conduct carriers injected from contacts. They show comparatively high mobilities for electrons and holes, typically in the 10−2 to 10 cm2 /(Vs) range at 300 K; the mobility falls with increasing temperature as discussed below. Twocomponent (chargetransfer) semiconductors include highly conductive compounds and may even show semiconductormetal transitions. The large conductivity originates from an incomplete electron exchange between donors and acceptors and consequently partially filled bands. The resistivity of these semiconductors lies between 102 and 106 cm at room temperature with a transferenergy gap in the 0.1–0.4 eV range [30]. The conductivity is usually highly anisotropic, with the electron transferintegral in the stacking direction typically a factor of 10 larger than in the direction perpendicular to the stacks [31]. The chargetransfer crystals provide an opportunity for fine tuning of the semiconductive properties by replacing TTFtype donors and TCNQtype acceptors (Fig. 3.5) with other similar molecules [32]. Organic molecules show a strong structural relaxation when a charge is introduced. The band structure calculated for a crystal composed of weakly bonded neutral molecules will hence usually not be preserved in the presence of carriers. As a rule of thumb, band conductance occurs despite lattice relaxation if the transfer integral between molecules is sufficiently large: a large transfer integral delocalizes the carrier wavefunction over several molecules. A more quantitative estimate follows from the width W of the energy band for carrier transport. If the mean dwell time of a moving carrier on a molecule is substantially shorter than the characteristic time of a molecule vibration, no significant relaxation and consequential trapping is expected to occur and band conductance may prevail. Taking a characteristic time τ on the order of 10−15 s yields a band width W
, τ
(5.8)
i.e., values exceeding several hundred meV; this condition is reasonably well fulfilled for crystals of acenes and comparable aromatic compounds (Table 5.1). Another approach considers the scattering of a moving carrier. If the mean scattering time τ scatter is in the range or smaller than /W , no wave vector k can be assigned to the carrier. The description in terms of conduction in a band with dispersion E(k) hence requires τ /W . The bands in organic crystals are rather narrow due to a small amount of wavefunction overlap of π electrons (Sect. 5.1.2). With typical bandwidths W in the range of some hundred meV we obtain τ scatter > 10−15 s. Both molecular relaxation and narrow band widths impose limits for bandlike conduction in organic semiconductors. A clear indication for band conduction is provided by the temperature dependence of the mobility. In inorganic semiconductors scattering at acoustic phonons leads to a T −3/2 dependence of the carrier mobility. A comparable decrease of mobility at higher temperature is observed for carriers in organic crystals with band conduction.
192
5 Electronic Properties of Organic Semiconductors
(a)
10
1
β = 1.78
100
β = 2.16
6 kV/cm 20 kV/cm 60 kV/cm
F a F c
µ (cm2 V1 s1)
µ (cm2 V1 s1)
100
(b)
μ1
10 μ2
1
β = 1.47
μ3
β = 1.48 β = 1.48
10
100 T (K)
300
10
100 T (K)
300
Fig. 5.9 Temperature dependence of the electron mobility a in a perylene crystal, and b in a naphthalene crystal. Reproduced with permission from [33, 34], © 1985 and 2001 Springer
The mobility data in Fig. 5.9 show typical features of bandlike transport in organic crystals. The temperature dependence at low electric field is described by a power law μ(T ) = μ0 × (T /T0 )β ,
(5.9)
where μ0 is the mobility at a reference temperature T 0 usually set to 300 K. The exponent β deviates somewhat from the ideal value of −3/2, see Table 5.3. The Table 5.3 Mobility μ in units of cm2 V−1 s−1 for organic crystals at 300 K and exponent β of the temperature dependence according to (5.9) Crystal Naphthalene
Anthracene
Perylene
Direction
Electrons
Holes
μ
β
μ
β
a
0.62
−1.4
0.94
−2.8
b
0.64
−0.55
1.84
−2.5
c
0.44
+0.04
0.32
−2.8
a
1.73
−1.45
1.13
−1.46
b
1.05
−0.84
1.84
−1.26
c
0.39
+0.16
0.32
−1.43
a
2.37
−1.78
b
5.53
−1.72
c
0.78
−2.15
5.2 Transport in Organic Semiconductors
193
lowfield mobilities do not depend on the value of the electric field and show a pronounced anisotropy; the principal axes of the mobility tensor deviate slightly from the crystallograpic crystal axes. Typical mobilities are on the order of 10−2 to 10 cm2 /(Vs). Data for a large number of organic semiconductors are tabulated in [35]; they decrease at higher temperature according to (5.9) with 0 > β > −3. Hopping Conductance in Organic Semiconductors Conductance in organic semiconductors is strongly affected by disorder. Even in perfect smallmolecule crystals the weak intermolecular van der Waals bonds give rise to a phononrelated dynamical disorder which affects the mobility of carriers. In addition, many organic compounds cannot be grown as single crystals and are prepared as paracrystalline thin films by evaporating or spin coating; for a specification of paracrystallinity see (3.7). In these semiconductors the static disorder dominates at most temperatures; their carrier mobility is by orders of magnitudes lower than that of crystalline compounds and increases for increasing temperature: the poor coupling between the molecules in the solid leads to a strong localization of the carriers on single molecules; transport occurs via a sequence of chargetransfer steps from one molecule to another, similar to the hopping between defect states in inorganic semiconductors. The larger mobility at higher temperature is due to the required thermal activation from the localized states. The temperature dependence of such a hopping conductance in organic semiconductors is hence inverse to the band conductance discussed above. Reviews on mobility and other physical data for organic semiconductors are given in [36, 37]. The transport properties are described by the formalism of hopping conductance developed for amorphous inorganic semiconductors: the charge carriers are assumed to hop in a timeindependent disordered energy landscape. In heavily disordered or amorphous inorganic semiconductors defects or deviations from ideal topology lead to a continuous tailing of energy states into the bandgap. Deeper states occur less frequently because the centers which produce such states are less probable. When deep enough, each type of defect center will produce a localized level. Shallower centers are, however, close enough: their levels broaden into bands, and the resulting states are no longer localized. Overlapping levels and narrow bands all merge into the tailing states. Thus, when going from deep tail states to the band states a transition from localized to delocalized states is expected at a critical energy, referred to as the mobility edge. The smooth transition in the density of states of a highly disordered inorganic semiconductor is illustrated in Fig. 5.10a, with a mobility edge indicated for ntype conductivity. Carriers which are thermally activated above the mobility edge contribute to charge transport, while carriers at lower energy are localized in defect states. In Fig. 5.10b the density of states is illustrated for an organic semiconductor with bandlike conductivity, indicating the mobility edge for electrons at the lowenergy band edge of the narrow conduction band. The basic difference between amorphous inorganic semiconductors and disordered organic semiconductors is the shape of the density of states (DOS) g(E). In a disordered inorganic semiconductor the DOS is found to have a mobility edge and a tail of localized states with an exponentially decreasing distribution extending into the band gap. In contrast, the DOS in organic solids has a Gaussian shape:
194
5 Electronic Properties of Organic Semiconductors
(a)
(b)
mobility edge trap extended states states
mobility edge LUMO
g(E)
log g(E)
HOMO
hole traps
Ev
Ec
E
Ev
electron traps
Ec
E
Fig. 5.10 Tailing of states into the bandgap of a a heavily disordered inorganic semiconductor (red solid lines) compared to the density of states g(E) in the crystalline state (dashed), and b an organic semiconductor. Extended and localized states are separated by a mobility edge, indicated for electron conductance by the dotted line
(E − E center )2 G tot g(E) = √ exp , 2σ 2 2π σ
(5.10)
where Gtot is the total DOS, E center is the center of the energy distribution, and σ is the variance of the distribution [38]. Hopping of carriers is determined by both, the energy difference E and the spatial separation d of initial and final states; in addition, hopping is affected by an electric field F. The Gaussian DOS results in a thermally activated mobility [38] √ 2σ 2 σ 2 2 μ = μ0 exp − +C −Σ F , 3kT kT
(5.11)
determined by the spread σ of the energy distribution in the conducting band, the structural disorder parameter Σ, the applied electric field F, and the parameter μ0 representing the mobility of the hypothetic notdisordered semiconductor at high temperature. For a more detailed review of various transport models see [39], a review on experimental techniques for measuring transport properties is given in [40]. The mobility is widely measured using timeofflight experiments. The experimental findings depend on the chemical purity, on the temperature range, and on the electric field; in many cases they can be described by the empirical dependence √ EA ∼ +b F , μ = μ0 exp − kT
(5.12)
5.2 Transport in Organic Semiconductors
195
with the zerofield mobility μ0 and an activation energy E A ; the activation energy corresponds to the difference between the energy of the localized state and the mobility edge. The quantity b is the fieldactivation factor
1 1 − b=B kT kT0
(5.13)
(b)
106
OC1C10PPV
MEHPPV OR1
(
108
R2O
n
1010 1012 1014 1016
µ (cm2 V1 s1)
(a)
c
105
b O
a
OC10C10PPV
1 105 2 105 3 105 4 105
T
2
(
2
(K )
106
300
O
500
700
(
104
(
µ (cm2 V1 s1)
with empirical parameters B and T 0 . Since polymers are stable only in a very limited temperature range, the temperature dependence can often be described in this interval by different relations, such as either (5.11) or (5.12). The hole mobility of the poly(paraphenylene vinylene) (PPV) is shown in Fig. 5.11. Holes dominate the current in many polymers. The polymer PPV is a prominent compound due to its electroluminescence properties; PPV derivatives are soluble and can be spin coated for, e.g., fabrication of organic LEDs. The mobility is reasonably described by a log(μ) ∝ T −2 dependence, although also an Arrhenius dependence log(μ) ∝ T −1 dependence fits well [41]; in the limited temperature range a clear distinction is not possible. The activation energies E A for PPV derivatives (5.12) range between 0.3 and 0.5 eV, and widths σ of the Gaussian DOS according to (5.11) are near 100 meV, with mean separations d of localization sites in the range 1.1–1.7 nm [42]. We note in Fig. 5.11 the comparatively low mobility of disordered organic semiconductors and the characteristic increase at higher temperature.
n
900
√ F (V/cm)
Fig. 5.11 Hole mobility in derivatives of PPV. a Mobility in derivatives with different side groups at zero electric field; OC1 C10 PPV: R1 = CH3 , R2 = C10 H21 ; OC10 C10 PPV: R1 = R2 = C10 H21 ; reproduced with permission from [42], © 2015 ACS. b Dependence of the hole mobility on the electric field F for MEHPPV (R1 = C8 H16 , R2 = CH3 ) prepared without (curve a) and with application of an electric field of 3 and 6 kV/cm for curves b and c; reproduced with permission from [43], © 2006 AIP
196
5 Electronic Properties of Organic Semiconductors
The enhancement of the mobility in an electric field F is shown in Fig. 5.11b, demonstrating the dependence on F 1/2 . This behavior has also been observed from timeofflight measurements in many molecularly doped polymers and amorphous glasses. An electrically induced polarization of MEHPPV during the preparation of films significantly enhances the mobility. The density of states in organic crystals is governed by disorder as noted above. Intrinsic defects (Sect. 3.2) and phonons contribute respectively to static and dynamical structural disorder, and impurities give rise to traps in the bandgap with a broad distribution of states. The density of trap states was experimentally derived from various measurements; results from the evaluation of the spacecharge limited current in transistor structures are shown in Fig. 5.12. We observe a strong tailing from the valenceband edge (mobility edge at E = 0) into the bandgap. Particularly low trap densities have pentacene and rubrene single crystals (sc bulk) and fieldeffect transistors made with such crystals (sc FET ); the increase of the trap density in FET structures is attributed to defects at the interface to the gate dielectric. The comparably low trap density corresponds to the large carrier mobility found in such semiconductors. The defect density in organic smallmolecule transistors is comparable to that in hydrogenated amorphous silicon. Polycrystalline thin films have significantly higher trap densities due to the high density of defects. Distortions in the (para) crystalline regions of a polymer consist, 1022
Trap DOS (states eV1 cm3)
1021 1020 1019 sc
1018
DH
DB FE
6T
TT
T
F
TF
T
αSi:H (holes) Pentacene sc FET Pentacene TFT
1017 αSi:H (electrons)
1016
Rubrene sc FET Pentacene sc bulk Rubrene sc bulk
1015 1014
0.0
0.1
0.2
0.3
0.4
0.5
0.6
0.7
E (eV) Fig. 5.12 Typical trap density in smallmolecule semiconductors (black, red, and blue curves) and hydrogenated amorphous silicon (green curves). Blue curves refer to bulk singlecrystals (sc), red curves to fieldeffect transistors (FET ) made with single crystals; the black curve gives a result of a polycrystalline thinfilm transistor (TFT ). Energy values are relative to the valenceband edge E v (for electrons in αSi:H relative to the conductionband edge E c ). Reproduced with permission from [44], © 2010 APS
Fig. 5.13 Calculated density of states (DOS) of fusedring polythiophene for different degrees of paracrystalline disorder expressed by the paracrystallinity parameter g. The valenceband maximum E v refers to a perfectly crystalline region. Reproduced with permission from [45], © 2011 APS
Trap DOS (states eV1 cm3)
5.2 Transport in Organic Semiconductors
197
1021
S S
S S
1020
n g=8%
1019 g=6%
1018 g=4% g=2%
17
10
0.2
0.0
0.2
0.4
0.6
0.8
E  Ev (eV)
e.g., of random variations in the spacings between the backbone lamella illustrated in Fig. 3.6. Such variations create band tailing into the bandgap comparable to the distortions shown in Fig. 3.8b for molecule shifts in a pentacene crystal. The magnitude of such variations was measured for aligned ribbons of fusedring polythiophene delineated in the inset of Fig. 5.13. By analyzing data of grazing incidence Xray diffraction, the effect on the density of states shown in Fig. 5.13 was calculated using densityfunctional theory [45]. In the calculations the distance between the chains (ideally a) was varied according to a Gaussian distribution with a standard deviation σ , yielding a paracrystallinity g = σ /a, see (3.5). The model predicts an exponential dependence of the distribution of traptailing states within the bandgap, similar to results of disordered inorganic solids depicted in Fig. 5.10. The characteristic energy E 0 in the DOS function g(E) = g0 exp(–E/E 0 ) has values near 10 meV for wellordered and 100 meV for strongly disordered polymers.
5.3 Interfaces in Organic Semiconductors Any semiconductor device comprises heterojunctions between different semiconductor layers and to metal contacts. When two solids are brought into contact, their energy bands at the interface must align with respect to a common reference. This problem is discussed for interfaces between inorganic semiconductors in Sect. 4.2, and for a contact between an inorganic semiconductor and a metal in Sect. 10.3. The alignment leads in both cases to a flow of carriers across the interface, creating a spacecharge region and a corresponding band bending. The basic principles of band alignment outlined for inorganic solids in Sect. 4.2 also apply for organic semiconductors. However, the molecular structure and disorder introduce additional conditions, which complicate the electronic structure of such interfaces. Even though a consistent model to describe organic interfaces is missing, some general rules exist and procedures to control the interface can be identified; for reviews see [46–48].
198
5 Electronic Properties of Organic Semiconductors
5.3.1 OrganicOrganic Heterointerface VacuumLevel Alignment Many organic semiconductors have no intramolecular total dipol moment and have intrinsically low concentrations of free carriers; moreover, the requirement of lattice matching found in inorganic heterointerfaces (Sect. 2.2.5) is largely relaxed for molecular crystals with weak van der Waals bonds (Sect. 3.2.1). A contact between two such solids often does not induce a significant redistribution of charges, i.e., no significant interface dipole is created. In the majority of these cases the classical electronaffinity rule introduced in Sect. 4.2.1 provides a good description of the band alignment at organicorganic semiconductor heterojunctions [49, 50]: the vacuum level E vac of the individual semiconductors represents the common reference level across the interface, and the bands are flat without bending. The electronic properties of organicorganic interfaces are widely measured using photoemission spectroscopy (PS): ultraviolet PS (UPS) yields the ionization energy I for the removal of an electron from the HOMO, and inverse PS (IPES) provides the electron affinity A required to add an electron to the LUMO, see Fig. 5.1. We discussed in Sect. 5.1.2 that organic molecules experience a strong relaxation upon charging; the quantities I and A do hence not yield the HOMO and LUMO levels of the neutral molecule, but the respective related energies of the negative and positive polarons. There exist conditions where the simple rule of vacuumlevel alignment fails. If the organic heterojunction is formed between a strong electron donor and a strong electron acceptor, electrons are transferred from the ntype to the ptype semiconductor and a spacecharge region with accompanying band bending is created. Dipols at the interface or on individual molecules introduce potentials which affect the vacuum level across the interface; in addition, pinning of energy levels may occur. Such conditions are discussed below. Molecular Charge Distribution In a neutral molecule of an organic semiconductors the negative charge of the delocalized π electrons is balanced by the positive charge of the atomic nuclei and their electrons in core and σ orbitals. If we consider the planar pentacene molecule (Fig. 3.10a) the positive charge is located on the backbone built by the nuclei and their electrons, and the negative charges are symmetrically located above and below this plane (comparable to Fig. 3.1). This separation of charges creates two electric dipols, each pointing from the negative to the positive charge distribution. Since both dipols have the same magnitude but opposite orientation their dipol moments cancel, but a quadrupole moment remains. An organic crystal built from these molecules has an electrostatic surface potential, which depends on the orientation of the topmost molecules. Effect of Molecular Orientation In the lyingdown configuration with the molecular plane parallel to the surface (Fig. 3.7) the potential energy for an electron is increased with respect to the vacuum
5.3 Interfaces in Organic Semiconductors
(a)
199
(b)
E crystal
vacuum level
E
surface vacuum
crystal
well
surface vacuum
LUMO level HOMO level
core level
z
z long axis
µ
long axis
Fig. 5.14 Schematic of the potential energy and levels for electrons in an organic crystal made of rodlike molecules near the surface a for a layingdown configuration of the molecules parallel to the surface and b for a standingup configuration. Red dots indicate atom cores, adjacent blue clouds signify π electrons, the green arrow labeled µ is the surface dipol in the layingdown configuration
level further away; the increase results from the terminating dipol layer, which leads to a potential well as illustrated in Fig. 5.14a. The values of the ionization energy I and electron affinity A rise by this potential well. In the standingup configuration depicted in Fig. 3.8a no significant projection of the dipol with respect to the surface normal exists, and the values for I and A are smaller. The orientation of the molecular dipol with respect to the interface plane of a heterojunction affects the electrostatic potential at the interface and consequently the alignment of the bands. This was clearly verified by UPS spectra obtained from perfluoropentacene (PFP) with different inclinations on surfaces. In PFP all 14 hydrogen atoms of pentacene are replaced by strongly electronegative fluorine atoms, which produce intramolecular dipoles in addition to the quadrupol introduced above; the dipol orientations at the ends of the PFP backbone points from the negative ends (comprising two F atoms) toward the molecule center. For PFP the standingup configuration is expected to create a much stronger termination dipol than the layingdown configuration. PFP was prepared in a layingdown configuration of a single monolayer on a clean Au(111) surface, with tilted molecular long axes in a multilayer herringbone configuration, and in a standingup configuration on SiO2 [51]. UPS spectra yield respective ionization energies of 5.80, 6.00, and 6.65 eV, demonstrating the effect of the increasing projection of the terminating dipol on the surface normal. The example also shows that the ionization energy of an organic crystal depends on orientation and is no unique value as for an isolated molecule; this must be considered when using data for a tentative assignment based on vacuumlevel alignment. Top layers at organicorganic interfaces comprising planar molecules typically adopt the orientation of the underlying layer. A review on various heterointerfaces and the orientation dependence of their molecular arrangement is given in [52].
200
5 Electronic Properties of Organic Semiconductors
5.3.2 OrganicMetal Interface The interaction between a clean metal surface and π electrons of organic semiconductors is strong (Sect. 3.2.1), resulting generally in a layingdown configuration of molecules for a single monolayer. If the molecules have a dipol moment p normal to the surface, the work function eφ m of the metal is changed by an amount e φ =
e Np εr ε0
(5.14)
where e, εr , and ε0 are respectively the elementary charge and the permittivities of the solid and vacuum. The areal density N of the dipols gets maximum for a complete monolayer. According to (5.14) the resulting work function e(φ m + φ) of a metal can linearly be varied by the lateral density of a monolayer of dipolar molecules. The surface dipol can also be created by applying molecules which act as electron donors or acceptors. A donor molecule chemisorbed on a metal surface leads to a redistributed electron concentration with a negative charge at the outermost surface, and consequently a dipol oriented towards the surface (acceptor vice versa). The introduction of suitable interlayers allows to control the effective work function of electrodes used as contacts in organic devices [53]. It must be noted that also unintentional surface contaminants like water, oxygen, or hydrocarbons affect the effective work function of metals. This easily leads to discrepancies between energies usually measured in ultrahigh vacuum (10−9 mbar) and those obtained with highvacuum conditions (10−6 mbar) applied for device fabrication; in high vacuum the metal surface is inevitably covered by a monolayer thick chemically inert layer. The organicmetal interaction to an organic semiconductor deposited on top of such a metal is substantially weaker. As a consequence, the energy levels at the contact generally align according to the dependence illustrated in Fig. 5.15. Barriers experienced by carriers at the contact between metal and organic semiconductor are depicted in panel (a); here an ideal
Fig. 5.15 a Work function eφ m , electron injectionbarrier Δe , and hole injectionbarrier Δh at an organicmetal contact without interface dipol. b Slope parameter S of the organicmetal contact for varied work function of the metal
5.3 Interfaces in Organic Semiconductors
201
junction according to the SchottkyMott model (Sect. 10.3.1) without interface dipol is assumed. Electrons injected from the metal to the LUMO have to surmount the electron barrier Δe to reach unoccupied states, and holes injected from the metal to the HOMO experience the barrier Δh . When the work function of the metal eφ m increases, Δe increases and Δh decreases. The slope parameter S=
Δe,h e φm
(5.15)
for the ideal contact is unity. Figure 5.15b shows that such a linear dependence is observed for actual metal electrodes on organic semiconductors only in a limited range. High metal workfunctions above this range are desirable to avoid the hole barrier Δh at ptype contacts, and low metal workfunctions below this range can avoid the electron barrier Δe at ntype contacts. However, there is no change of the injection barriers observed when the metalworkfunction is varied; these ranges with strongly reduced S are referred to Fermilevel pinning. FermiLevel Pinning Fermilevel pinning is wellknown from inorganic semiconductors (Sect. 10.3.2). Gapstate models applied to explain the phenomenon are also used to describe organicmetal contacts, taking characteristic features of organic crystals into account [54–56]. The tailing of the density of states outlined in Sect. 5.2.2 provides localized states in the gap between HOMO and LUMO, which can accommodate carriers transferred across the interface when the contact is made. If a metal with a low work function is applied to fabricate a lowbarrier ntype contact, its Fermi energy will lie in a region where before contact empty states of the organic semiconductor with a lower energy exist; below the LUMO these are empty tail states. When the contact is made and tailing is pronounced, electrons will move from the metal across the barrier into localized states to reestablish equilibrium (Fig. 5.16). They thereby create an interface dipol, which raises the metal workfunction according to (5.14). Similarly a metal with high work function applied to produce a ptype contact leads to a flow of holes across the interface to drain occupied gap states extending from the HOMO, thereby decreasing the work function. Tailing will hence generally reduce the slope parameter S; a nearly ideal dependence of injection barriers on the metal workfunction can only occur in an energy range of negligible density of localized states in the bandgap. Since the degree of disorder and purity of organic semiconductors vary, usually no unique pinning energy is found.
5.4 Problems Chapter 5 5.1 For a neutral anthracene molecule in the gas phase respective ionization and electron affinity energies of 7.42 and 0.58 eV are measured; in an anthracene crystal a ionization energy of 5.77 eV is observed.
202
5 Electronic Properties of Organic Semiconductors
Fig. 5.16 Density of states g(E) and respective occupation (gray shading) at an interface between metal and an organic semiconductor a before and b after contact
(a) Which electron affinity in the crystal results from these data, if the polarization energy upon adding an electron to a neutral molecule of the crystal equals that for removal of an electron? (b) Which binding energy of the singlet exciton is inferred from these data, if the onset of the respective absorption is observed at 382 nm? 5.2 For the mobility of negative carriers in the bandlike conduction of a tetracene crystal values of 0.85 and 25.5 cm2 /(Vs) are found at 300 K and 77 K, respectively. Which mobility results from this data at 0 °C (32 F)? 5.3 Ionization and electronaffinity energies of 5.8 and 3.1 eV are found in photoelectron spectroscopy for Alq3 (Fig. 3.3g). We consider organicorganic interfaces between Alq3 and BCP (4,4 N,N dicarbazolylbiphenyl), PTCDA (Fig. 3.3f), and αNPD (N,N diphenylN,N bis(lnaphthyl)l,l biphenyl4,4 diamine). (a) For a layer of BCP deposited on top of Alq3 a ionization energy of 6.4 eV is measured and an energy difference of 3.1 eV between HOMO and LUMO levels is determined. How do the HOMO and LUMO levels align at this heterojunction if vacuumlevel alignment applies? (b) For the organicorganic interfaces PTCDA/Alq3 and αNPD/Alq3 the vacuumlevel of Alq3 is lower than those of the organic layers in contact. How large is the step of the vacuum level at the PTCDA/Alq3 interface (going from PTCDA toAlq3 ) for a measured PTCDA ionization energy of 6.7 eV, if the LUMO level of PTCDA lies 2.2 eV above the HOMO level and 0.9 eV below the LUMO level of Alq3 ? How do the HOMO levels align? (c) Using the result of (b): How large is the expected step of the vacuum level for a PTCDA/αNPD interface, if a dipol of −0.3 eV is determined for the αNPD/Alq3 interface (going from αNPD toAlq3 ) and a transitivity rule applies?
5.4 Problems Chapter 5
203
5.4 A layer of αNPD is deposited either on Au with 5.2 eV work function or on Mg with 3.8 eV work function, and the position of the Fermi level in αNPD is measured using photoelectron spectroscopy; a ionization energy of 5.4 eV is found for the organic layer. (a) Which Fermi energies (with respect to the HOMO level) would be obtained in αNPD for the two cases if vacuumlevel alignment would apply? (b) Measured values deviate from those obtained assuming vacuumlevel alignment due to the formation of interface dipols, yielding 1.4 eV for Au and 2.0 eV for Mg (above the HOMO level). How large are the dipols at the interfaces to Au and to Mg? Which slope parameter results from these data?
5.5 General Reading Chapter 5 A. Köhler, H. Bässler, Electronic Processes in Organic Semiconductors: An Introduction (WileyVCH Verlag, Weinheim, 2015) M. Schwoerer, H.C. Wolf, Organic Molecular Solids (WileyVCH Verlag, Weinheim, 2007) W.R. Salaneck, K. Seki, A. Kahn, J.J. Pireaux (eds.), Conjugated polymer and molecular interfaces (Marcel Dekker Inc., New York, 2002)
References 1. L.S. Hung, C.H. Chen, Recent progress of molecular organic electroluminescent materials and devices. Mater. Sci. Eng. 39, 143 (2002) 2. M.C. Gather, A. Köhnen, K. Meerholz, White organic lightemitting diodes. Adv. Mater. 23, 233 (2011) 3. A.C. Arias, J.D. MacKenzie, I. McCulloch, J. Rivnay, A. Salleo, Materials and applications for large area electronics: solutionbased approaches. Chem. Rev. 110, 3 (2010) 4. P. Peumans, A. Yakimov, S.R. Forrest, Small molecular weight organic thinfilm photodetectors and solar cells. J. Appl. Phys. 93, 3693 (2003) 5. A.W. Hains, Z. Liang, M.A. Woodhouse, B.A. Gregg, Molecular semiconductors in organic photovoltaic cells. Chem. Rev. 110, 6689 (2010) 6. N. Karl, Organic Semiconductors, in Festkörperprobleme/Advances in Solid State Physics, vol. 14, ed. by H.J. Queisser (Vieweg, Braunschweig, 1974), pp. 261–290 7. Y.C. Cheng, R.J. Silbey, D.A. da Silva Filho, J.P. Calbert, J. Cornil, J.L. Brédas, Threedimensional band structure and bandlike mobility in oligoacene single crystals: a theoretical investigation. J. Chem. Phys. 118, 3764 (2003) 8. S.I. Machida, Y. Nakayama, S. Duhm, Q. Xin, A. Funakoshi, N. Ogawa, S. Kera, N. Ueno, H. Ishii, Highestoccupiedmolecularorbital band dispersion of rubrene single crystals as observed by angleresolved ultraviolet photoelectron spectroscopy. Phys. Rev. Lett. 104, 156401 (2010)
204
5 Electronic Properties of Organic Semiconductors
9. S. Yanagisawa, Y. Morikawa, A. Schindlmayr, HOMO band dispersion of crystalline rubrene: effects of selfenergy corrections within the GW approximation. Phys. Rev. B 88, 115438 (2013) 10. J.L. Brédas, J.P. Calbert, D.A. da Silva Filho, J. Cornil, Organic semiconductors: a theoretical characterization of the basic parameters governing charge transport. Proc. Natl. Acad. Sci. USA 99, 5804 (2002) 11. T. Holstein, Studies of polaron motion part II: the “small” polaron. Ann Phys. (N. Y.) 8, 343 (1959) 12. K. Hannewald, V.M. Stojanovi´c, J.M.T. Schellekens, P.A. Bobbert, G. Kresse, J. Hafner, The theory of polaron bandwidth narrowing in molecular crystals. Phys. Rev. B 69, 075211 (2004) 13. Y. Yang, Y. Yang, F. Wua, Z. Wei, Firstprinciples electronic structure of copper phthalocyanine (CuPc). Solid State Commun. 148, 559 (2008) 14. I.G. Hill, A. Kahn, Z.G. Soos, R.A. Pascal Jr., Chargeseparation energy in films of πconjugated organic molecules. Chem. Phys. Lett. 327, 181 (2000) 15. P.K. Nayak, Exciton binding energy in small organic conjugated molecule. Synth. Met. 174, 42 (2013) 16. P.I. Djurovich, E.I. Mayo, S.R. Forrest, M.E. Thompson, Measurement of the lowest unoccupied molecular orbital energies of molecular organic semiconductors. Org. Electron. 10, 515 (2009) 17. J. Singh, The dynamics of excitons, in Solid State Physics, vol. 38, ed. by H. Ehrenreich, D. Turnbull (Academic Press, Orlando, 1984), pp. 295–370 18. K.W. Böer, U.W. Pohl, Excitons, in Semiconductor Physics (Springer, Cham, 2018) 19. J.I. Frenkel, On the transformation of light into heat in solids II. Phys. Rev. 37, 1276 (1931) 20. G. Klein, R. Voltz, M. Schott, Singlet exciton fission in anthracene and tetracene at 77 degrees K. Chem. Phys. Lett. 19, 391 (1973) 21. H. Uoyama, K. Goushi, K. Shizu, H. Nomura, C. Adachi, Highly efficient organic lightemitting diodes from delayed fluorescence. Nature 492, 234 (2012) 22. M. Pope, C.E. Swenberg, Electronic Processes in Organic Crystals (Oxford University Press, Oxford, UK, 1982) 23. J. Shinar (ed.), Organic LightEmitting Devices: A Survey (Springer, New York, 2004) 24. K.T. Kamtekar, A.P. Monkman, M.R. Bryce, Recent advances in white organic lightemitting materials and devices (WOLEDs). Adv. Mater. 22, 572 (2010) 25. S. Reineke, M.A. Baldo, Room temperature triplet state spectroscopy of organic semiconductors. Sci. Rep. 4, 3797 (2014) 26. R.P. Feynman, Slow electrons in a polar crystal. Phys. Rev. 97, 660 (1955) 27. J. Appel, Polarons, in Solid State Physics, vol. 21, ed. by F. Seitz, D. Turnbull, H. Ehrenreich (Academic Press, New York, 1968), pp. 193–391 28. R.A. Marcus, Electron transfer reactions in chemistry. Theory and experiment. Rev. Mod. Phys. 65, 599 (1993) 29. A. Troisi, Charge transport in high mobility molecular semiconductors: classical models and new theories. Chem. Soc. Rev. 40, 2347 (2011) 30. C.L. Braun, Organic semiconductors, in Handbook on Semiconductors, Vol. 3, Materials Properties and Preparation, ed. by T.S. Moss, S.P. Keller (North Holland Publ, Amsterdam, 1980), pp. 857–873 31. H.J. Keller (ed.), Chemistry and Physics in OneDimensional Metals (Plenum Press, New York, 1977) 32. A.N. Bloch, T.F. Carruthers, T.O. Poehler, D.O. Cowan, The organic metallic state: some physical aspects and chemical trends, in Chemistry and Physics in OneDimensional Metals, ed. by H.J. Keller (Plenum Press, New York, 1977), pp. 47–85 33. W. Warta, R. Stehle, N. Karl, Ultrapure, high mobility organic photoconductors. Appl. Phys. A 36, 163 (1985) 34. N. Karl, Chargecarrier mobility in organic crystals, in Organic Electronic Materials: Conjugated Polymers and Low Molecular Weight Organic Solids, ed. by R. Farchioni, G. Grosso (Springer, Berlin, 2001), pp. 283–326
References
205
35. L.B. Schein, Temperature independent drift mobility along the molecular direction of As2 S3 . Phys. Rev. B 15, 1024 (1977) 36. N. Karl, Organic Semiconductors. LandoldtBörnstein (Springer, Heidelberg, 1984) 37. H. Bässler, A. Köhler, Charge transport in organic semiconductors. Top. Curr. Chem. 312, 1 (2012) 38. H. Bässler, Charge transport in disordered organic photoconductors. Phys. Stat. Solidi B 175, 15 (1993) 39. R. Noriega, A. Salleo, Charge transport theories in organic semiconductors, in Organic Electronics II, ed. by H. Klauk, (WileyVCH, Weinheim, 2012), pp. 67–104 40. V. Coropceanu, J. Cornil, D.A. da Silva Filho, Y. Olivier, R. Silbey, J.L. Bredas, Charge transport in organic semiconductors. Chem. Rev. 107, 926 (2007) 41. P.W.M. Blom, M.J.M. de Jong, M.G. van Munster, Electricfield and temperature dependence of the hole mobility in poly(pphenylene vinylene). Phys. Rev. B 55, R656 (1997) 42. P.W.M. Blom, M.C.J.M. Vissenberg, Charge transport in poly(pphenylene vinylene) lightemitting diodes. Mater. Sci. Eng. 27, 53 (2000) 43. Q. Shi, Y. Hou, J. Lu, H. Jin, Yunbai Li, Yan Li, X. Sun, J. Liu, Enhancement of carrier mobility in MEHPPV film prepared under presence of electric field. Chem. Phys. Lett. 425, 353 (2006) 44. W.L. Kalb, S. Haas, C. Krellner, T. Mathis, B. Batlogg, Trap density of states in smallmolecule organic semiconductors: a quantitative comparison of thinfilm transistors with single crystals. Phys. Rev. B 81, 155315 (2010) 45. J. Rivnay, R. Noriega, J.E. Northrup, R.J. Kline, M.F. Toney, A. Salleo, Structural origin of gap states in semicrystalline polymers and the implications for charge transport. Phys Rev B 83, 121306 (2011) 46. W.R. Salaneck, K. Seki, A. Kahn, J.J. Pireaux (eds.), Conjugated Polymer and Molecular Interfaces (Marcel Dekker Inc., New York, 2002) 47. N. Koch, Electronic structure of interfaces with conjugated organic materials. Phys. Stat. Solidi RRL 6, 277 (2012) 48. K. Akaike, Advanced understanding on electronic structure of molecular semiconductors and their interfaces. Jpn. J. Appl. Phys. 57, 03EA03 (2018) 49. I.G. Hill, D. Milliron, J. Schwartz, A. Kahn, Organic semiconductor interfaces: electronic structure and transport properties. Appl. Surf. Sci. 166, 354 (2000) 50. H. Vázquez, W. Gao, F. Flores, A. Kahn, Energy level alignment at organic heterojunctions: role of the charge neutrality level. Phys. Rev. B 71, 041306 (2005) 51. G. Heimel, I. Salzmann, S. Duhm, N. Koch, Design of organic semiconductors from molecular electrostatics. Chem. Mater. 23, 359 (2011) 52. W. Chen, D.C. Qi, H. Huang, X. Gao, A.T.S. Wee, Organicorganic heterojunction interfaces: effect of molecular orientation. Adv. Funct. Mater. 21, 410 (2011) 53. N. Koch, S. Duhm, J.P. Rabe, A. Vollmer, R.L. Johnson, Optimized hole injection with strong electron acceptors at organicmetal interfaces. Phys. Rev. Lett. 95, 237601 (2005) 54. H. Vázquez, F. Flores, R. Oszwaldowski, J. Ortega, R. Pérez, A. Kahn, Barrier formation at metalorganic interfaces: dipole formation and the charge neutrality level. Appl. Surf. Sci. 234, 107 (2004) 55. J. Hwang, A. Wan, A. Kahn, Energetics of metalorganic interfaces: new experiments and assessment of the field. Mater. Sci. Eng. R 64, 1 (2009) 56. J.P. Yang, F. Bussolotti, S. Kera, N. Ueno, Origin and role of gap states in organic semiconductor studied by UPS: as the nature of organic molecular crystals. J. Phys. D: Appl. Phys. 50, 423002 (2017)
Chapter 6
Thermodynamics of Epitaxial LayerGrowth
Abstract Growth requires some deviation from thermodynamic equilibrium. This chapter outlines the driving force for equilibriumnear growth of a crystal in terms of macroscopic quantities. We consider a thermodynamic description for the transition of a gaseous or liquid phase to the solid phase. The initial stage of layer growth requires a nucleation process. We discuss the energy of a surface and illustrate the nucleation of a layer and the occurrence of different growth modes.
Growth of a crystalline solid represents a transition from one phase, e.g., the vapor phase, to a crystalline phase. Such phase transition is phenomenologically described by thermodynamics using macroscopic quantities. Often the understanding of growth phenomena requires also consideration of the kinetics. A respective description considers transition states on an atomistic scale. Epitaxy may be performed close to thermodynamic equilibrium using, e.g., liquid phase epitaxy (Sect. 11.1). Growth is then well described in terms of thermodynamic properties of the system. Epitaxy far away from equilibrium by applying, e.g., processes occurring during molecular beam epitaxy (Sect. 11.3), may often more appropriately be described in terms of kinetics. In this chapter basics of growth processes employed in epitaxial methods are discussed in terms of thermodynamics.
6.1 Phase Equilibria Thermodynamics studies the effect of changes in, e.g., temperature on a system at a macroscopic scale by analyzing the collective motion of its particles. The term particles comprises both, atoms and molecules, and the term system denominates a large ensemble of particles which is markedoff from environment in some defined manner. The system may either contain a single kind of particles (singlecomponent system) or a mixture of different kind of particles (multicomponent system). If the system is completely homogeneous (regardless of being a single or multicomponent system) it is called to consist of a single phase. Growth occurs in heterogeneous systems which are characterized by interfaces separating different phases within the system. © Springer Nature Switzerland AG 2020 U. W. Pohl, Epitaxy of Semiconductors, Graduate Texts in Physics, https://doi.org/10.1007/9783030438692_6
207
208
6 Thermodynamics of Epitaxial LayerGrowth
6.1.1 Thermodynamic Equilibrium If a system is left undisturbed by outside influences the interacting particles will share energy among themselves and reach a state, where the global statistics are unchanging in time. Parameters describing the system then have ceased to change with time. This allows single parameters like temperature or pressure to be attributed to the whole system. Growth requires a force to drive particles from one phase of a system across the interface towards a solid phase. The crystal grower controls parameters in a way that a more volatile phase of the system is thermodynamically less stable than the crystalline phase, i.e., he adjusts some deviation from equilibrium. There are two kinds of state variables which describe the system: • Intensive parameters like temperature T , pressure P, mole fraction xi of component i, or chemical potential μi are independent on the size of the system. • Extensive parameters like internal energy U , entropy S, volume V , or amount of substance n i do depend on system size. The amount of substance n i designates the number of moles of component i in the system and is given by the mass m i of the substance of component i divided by its mole mass Mi . The corresponding mole fraction xi (also called molar fraction) denotes the number of moles of component i as a proportion of the total number of moles of all components in the system, i.e., ni x i = Nc j=1
nj
=
ni , n
(6.1)
where Nc is the number of components in the system and n is the total number of moles in the system. All thermodynamic properties of a system may be derived from its internal energy U . For a system composed of Nc components this state function is given by
U = TS − PV +
Nc
μi n i .
(6.2)
i=1
S, V , and n i are the proper variables for the internal energy, and μ is the chemical potential introduced in (6.4) below. For crystal growers the direct access to the intensive parameters temperature and pressure is more convenient than control of the extensive parameters entropy and volume. Therefore the state function Gibbs energy G with T , P, and n i as proper variables is introduced,
6.1 Phase Equilibria
209
G = U + PV − TS.
(6.3)
Gibbs energy G—also referred to as Gibbs function or Gibbs free energy—is an extensive function like the internal energy U . The chemical potential of component i in the system is given by the partial derivative of Gibbs energy, μi =
∂G ∂n i
= μi (T, P, x1 , . . . , x Nc ).
(6.4)
T,P,n j=i
Inserting (6.2) into (6.3), Gibbs energy can also be expressed by the Nc amounts of substance n i and their respective chemical potentials,
G=
Nc
μi n i .
(6.5)
i=1
The total chemical potential μ then reads c G = μi xi . n i=1
N
μ=
(6.6)
Thermodynamic equilibrium is characterized by the minimum of Gibbs energy G. Extensive functions of a system are similarly given as the sum of the corresponding quantities for each phase. For a system containing Np phases, G is hence the sum of those for each phase σi , G=
Np
G(σ j ) = G(σ1 ) + G(σ2 ) + · · · + G(σ Np )
j=1
=
Np Nc
μi (σ j )n i (σ j )
(6.7)
j=1 i=1
=
Nc i=1
μi (σ1 )n i (σ1 ) +
Nc i=1
μi (σ2 )n i (σ2 ) + · · · +
Nc i=1
μi (σ Np )n i (σ Np ).
210
6 Thermodynamics of Epitaxial LayerGrowth
The σ j and n i (σ j ) identify the phases and the amount of substance of component i in phase σ j , respectively. If G is minimum at equilibrium, then condition ∂G =0 (6.8) ∂n i (σ j ) T,P,n(σj )j=i must apply for all Nc components and all Np phases of the system. Under given (constant) conditions for T , P, and n i , Gibbs energy G hence assumes a minimum value with respect to any variation of these state parameters. Let us assume a variation of one parameter, namely a transition of component 1 from phase α to phase β. The change is expressed by a variation of n 1 (α) with the condition n 1 (α) + n 1 (β) = constant. Applying condition (6.8) we obtain ∂G ∂(G(α) + G(β) + G(γ ) + · · · ) = ∂n 1 (α) ∂n 1 (α) ∂G(β) ∂G(α) ∂G(β) ∂G(α) + = − = 0. = ∂n 1 (α) ∂n 1 (α) ∂n 1 (α) ∂n 1 (β) In the second fraction all apart from the first two summands are zero for all phases except for α and β due to the assumed transition, and the negative sign of the second summand originates from ∂n 1 (β) = −∂n 1 (α). Inserting (6.4) applied to component 1 yields the equilibrium condition μ1 (α) − μ1 (β) = 0. This condition applies for pairs of all phases and all components. The general conditions for equilibrium hence reads: The chemical potentials μi of all Nc components are equal among each other in each of the Np phases,
μi (σ1 ) = μi (σ2 ) = · · · = μi (Np ), i = 1, . . . , Nc (equilibrium).
(6.9)
Equation (6.9) applies simultaneously for all Nc components of the system, yielding a set of Nc relations in case of an equilibrium between two phases. In equilibrium of a multicomponent system much more phases than two may coexist. For Np coexisting phases a set of (Np − 1) × Nc relations must be fulfilled at equilibrium. The composition of the Np phases is generally not equal at equilibrium to fulfill these conditions, i.e., usually x1 (σ1 ) = x1 (σ2 ) = x1 (σ3 ) = · · · . Figure 6.1 illustrates the equilibrium between phase α and a solid phase β of a threecomponent system. Different species of particles are depicted by different symbols. Note different compositions indicated in phases α and β. The interface between α and β is the surface of the solid. Its structure is thermodynamically less favorable than that of the solid or of the more volatile phase α. The surface hence
6.1 Phase Equilibria
211
Fig. 6.1 Schematic of a threecomponent system with two phases α and β in equilibrium
tends to be thin. In practice, it extends over a few atomic layers. In a thermodynamic description the surface region is usually not regarded as a separate phase and assumed infinitely thin.
6.1.2 Gibbs Phase Rule The number of phases which can coexist at equilibrium is limited. According to (6.4) a set of the variables T, P, and compositions xi of the Nc components specifies a phase of a heterogeneous system. The chemical potential in this phase is fixed when Nc − 1 mole fractions are quoted besides T and P: The last of Nc mole fractions is given by the condition i xi = 1 in each phase. We hence have Np × (Nc − 1) independent mole fractions for a system with Np phases. Therefore a total of Np × (Nc − 1) + 2 intensive variables are sufficient to fix all of the intensive variables of the system. Many of them are dependent, though. Considerations leading to (6.9) show that Nc relations according to μi (α) = μi (β) have to be fulfilled at equilibrium between two coexisting phases. For three coexisting phases 2 × Nc relations, and for Np phases a number of (Np − 1) × Nc relations have to be fulfilled. There remains thus a number Nf of independent intensive variables given by (Np × (Nc − 1) + 2) − ((Np − 1) × Nc ), or
Nf = Nc − Np + 2.
(6.10)
This number of independent intrinsic state parameters may be used to control growth near thermodynamic equilibrium without changing the number of phases Np . Nf is
212
6 Thermodynamics of Epitaxial LayerGrowth
called the number of degrees of freedom for a given thermodynamic condition and specifies how many control variables can be altered while maintaining this condition. This Gibbs phase rule was stated by Josiah Willard Gibbs in the 1870s. In literature the numbers of degrees of freedom, of components, and phases Nf , Nc , and Np , are also labeled as F, C, and π , respectively. Nf may not be negative. Consequently a maximum of Np = 3 phases may coexist in equilibrium of a singlecomponent system (Nc = 1). Since in this case Nf = 0 the variables T and P are fixed in a triple point. In a twophase equilibrium of a singlecomponent system we obtain Nf = 1. We hence can choose one parameter independently (within some limits), say T , while the other, P, adjusts accordingly to accomplish equilibrium. In a singlephase range of a singlecomponent system Nf = 2. T and P may then be varied independently. In a twocomponent system a maximum of 4 phases may coexist, and in a twophase equilibrium still two parameters may be controlled independently.
6.1.3 Gibbs Energy of a SingleComponent System A singlecomponent system has a maximum of three phases in equilibrium (Sect. 6.1.2), and a state is fixed by fixing temperature, pressure, and volume of the system. The equilibrium conditions between the thermodynamically distinct phases are clearly represented in a phase diagram. A simple illustration is the pressuretemperature diagram given in Fig. 6.2. The diagram is a projection of P–V –T space on the P–T plane for a fixed volume and shows the phase boundaries between the three equilibrium phases of solid, liquid, and gas. On a boundary two phases coexist, and in the triple point three phases coexist. Dashed curves near the triple point indicate metastable states (cf. Sect. 6.1.5). The solidliquid phase boundary of most substances has a positive slope. This is due to the solid phase having a higher density than the liquid, so that increasing the pressure increases the melting point. Prominent exceptions are, e.g., water and silicon. To study the behavior of the system at transitions from one phase to another we consider a variation of one of the variables P or T while keeping the other fixed [1]. We first discuss the temperature dependence of Gibbs energy G(T ) P , i.e., G(T ) at constant pressure P, along path 1 drawn in Fig. 6.2. In a second step the pressure dependence G(P)T along path 2 will be discussed. Considering a system consisting of one component yields a descriptive dependence of Gibbs energy G from temperature and pressure. There is only a single chemical potential, μ=
G ∂G = ≡ g (singlecomponent system). ∂n n
The relation shows that the chemical potential is identical to the Gibbs energy per mole g. Both μ and G depend solely on T and P.
6.1 Phase Equilibria
213
Fig. 6.2 P–T phase diagram for a singlecomponent system. Dashed curves near the triple point indicate metastable states. The dependence of Gibbs energy G(P, T ) for variations along paths 1 and 2 is discussed in the text
solid
Pressure
path 2
liquid triple point
path 1
gaseous Temperature
We first consider G(T ) P . The temperature dependence of G is evaluated from the respective dependence of the three summands in (6.3) G = U + PV − TS. The internal energy U (T ) starts at T = 0 K with some constant value U0 which merely represents an offset of all parameters. In the lowtemperature range the increase of U (T ) is essentially determined by the heat capacity of the (solid) system at constant volume, C VS . The slope increases due to an increase of C VS (T ). We may neglect here the small volume change of the solid at constant pressure and the consequential small contribution of U (V (T )). At the melting temperature TSL (index SL for solid → liquid) and also at the boiling temperature TLG (liquid → gaseous) the internal energy U (T ) increases by materialdependent steps USL and ULG , respectively: The bordering phases differ in internal energy. The thermal trend of U in the liquid and gaseous phases is likewise described using the heat capacities C VL (T ) and C VG (T ), respectively. The entire temperature dependence of the first summand of G(T ) in (6.3) is then given by TSL TLG S C V (T ) dT + USL + C VL (T ) dT U (T ) =U0 + 0 TSL (6.11) T + ULG +
TLG
C VG (T ) dT.
For T < TLG thereinafter summands are accordingly omitted. The trend of U (T ) is illustrated in Fig. 6.3.
214
6 Thermodynamics of Epitaxial LayerGrowth
Fig. 6.3 Temperature dependence of Gibbs energy G, internal energy U , enthalpy H , and the energies TS and PV at constant pressure for a singlecomponent system. After [1]
The trend of the second summand of G in (6.3) is given by V (T ) because P is assumed to be constant. Since the thermal expansion coefficients in the solid and liquid phases are very small (typ. of order 10−6 ) we may assume a virtually constant volume. Melting and evaporation lead to a small step VSL and a large step VLG . The dependence in the gas phase is approximated by the ideal gas law V (T ) ∼ = n RT /P, R being the universal molar gas constant. Adding the first two summands of G in (6.3) yields the enthalpy H (T ) = U (T ) + PV (T ). The thermal dependence is similar to that of U (T ) with slightly larger values due to positive values of P and V , cf. Fig. 6.3. The step at the melting point HSL = USL + PVSL is the heat of fusion absorbed during melting at TSL . It is vice versa identical to the heat released during solidification. According to convention a positive sign of H indicates an endothermic reaction, where the system receives heat supplied from the surroundings. Similar considerations apply for evaporation and condensation expressed by HLG . H (T ) may be expressed by a similar relation as (6.11) when U and C V are replaced by H and C P , respectively. The of G in (6.3) increases with T according to the entropy third summand S = C P /T = C P d ln T . S0 is assumed to be zero. During the phase transitions at TSL and TLG the entropy S experiences a steplike increase H/T . It should be noted that these steps have the same height as those in the function H (T ), since H = T S. S may also be expressed by a similar relation as (6.11) when U , C V , and dT are replaced by S, C P , and d ln T , respectively.
6.1 Phase Equilibria
215
We now put the three summands together to obtain Gibbs energy G(T ) according to (6.3). As shown in Fig. 6.3 G(T ) is a monotonously decreasing function with a gradually increasing negative slope. G(T ) is continuous at the phase transitions but experiences a kink. Since μ = G/n we also know the trend of the chemical potential μ(T ). We will consider this in more detail in Sect. 6.1.4. In a second step we address the pressure dependence G(P)T evaluated from the respective dependence of the three summands in (6.3) at constant temperature, cf. Fig. 6.4. Besides steps at phase transitions, U (P) may be considered nearly constant in all phases at constant temperature. The second summand PV (P) is approximately constant at low pressures due to the ideal gas law V ∼ = n RT /P. In the liquid and solid phases V (P) is nearly constant. As P increases PV (P) hence rises approximately linearly, with a larger slope in the liquid phase. The enthalpy H (P) = U (P) + PV (P) reproduces these slopes. The steps HLG and HSL again represent heats of condensation and solidification, respectively. The trend of the third summand of G in (6.3) TS(P) is given by S(P) at constant temperature. To obtain the trend at low pressure (gas phase) we apply the general Maxwell relation (∂ S/∂ P)T = −(∂ V /∂ T ) P and infer from the ideal gas law (∂ V /∂ T ) P ∼ = n R/P. Equalizing and integration yields S(P) ∼ = −n R ln P + S0 , where S0 is an integration constant. In the gas phase the trend decreases monotonously with a steep slope at small pressure due to the term − ln P. In the liquid and solid
Fig. 6.4 Pressure dependence of Gibbs energy G, internal energy U , enthalpy H , and the energies TS and PV at constant temperature for a singlecomponent system. After [1]
216
6 Thermodynamics of Epitaxial LayerGrowth
Fig. 6.5 Chemical potentials μα (T, P) and μβ (T, P) of two phases α and β near their intersection line, where both phases coexist. Dotted vertical lines indicate projection of the intersection line to the P–T plane. After [1]
phases (∂ V /∂ T ) P is quite small due to the small thermal expansion coefficient. S(P) is considered nearly constant in these phases. The sum adds up to the pressure dependence G(P)T illustrated in Fig. 6.4. G(P) is a monotonously increasing function. At phase transitions G(P) is continuous but experiences a kink. The same applies for the chemical potential μ(P) = G(P)/n.
6.1.4 Phases Boundaries in a SingleComponent System We consider the chemical potential μ(T, P) at the boundary between two phases α and β of a singlecomponent system. The characteristics in the P–T phase diagram is obtained from μ(T ) P = G(T ) P /n and μ(P)T = G(P)T /n. We know from Sect. 6.1.3 that μ(P, T ) is a curved plane which in each phase monotonously decreases along T and increases along P. The slopes of μα (T, P) and μβ (T, P) differ in two different phases. The respective planes hence intersect. Along the intersection line the chemical potentials must be equal, μα (T, P) = μβ (T, P). Adjacent to the line of intersection the respective lower plane refers to the stable phase. The stable phases change order upon crossing the section boundary: The respective other phase gets stable. Figure 6.5 illustrates the situation. The projection of the intersection line of the μα (T, P) and μβ (T, P) planes on the P–T plane shown in Fig. 6.5 yields the boundary between phases α and β depicted in Fig. 6.2. The characteristics of this boundary is described by the Clapeyron relation or, if a transition between a condensed (liquid or solid) to a gas phase is involved,
6.1 Phase Equilibria
217
by the ClausiusClapeyron relation, named after B.P. Émile Clapeyron and Rudolf Clausius. The general Clapeyron equation follows from a variation dμ(T, P) of a state on the coexistence line that must fulfill the identity dμα = dμβ , or, by inserting G/n for μ, 1 ∂G α 1 ∂G α 1 ∂G β 1 ∂G β dT + dP = dT + d P. n ∂T P n ∂P T n ∂T P n ∂P T In the relation we may replace (∂G/∂ T ) by −S and (∂G/∂ P) by V . This yields a condition for the proportion of the two variables for a variation along the coexistence line, Sβ − Sα dP = dT. Vβ − Vα The relation gives the slope d P/dT of the coexistence curve. S and V are respectively the change of entropy and volume during a phase transition across the boundary. Since S = H/T we may write S H dP = = . dT V T V
(6.12)
Here H is the latent heat exchanged with the surroundings during the phase transition without change of temperature T . The Clapeyron equation (6.12) explains basic characteristics of the P–T phase diagram Fig. 6.2. A transition from the gaseous phase to the liquid or the solid phase is accompanied by a large volume change V . According to (6.12) the slopes of these two phase boundaries are therefore small. The heat of evaporation H is a positive quantity just as the volume increase V . The slope d P/dT is therefore also positive. Furthermore, the slope increases as P increases due to a decrease of V at higher pressure. Due to a larger heat of sublimation of a solid compared to the heat of evaporation of a liquid the slope of the solidgas boundary is steeper than that of the liquidgas boundary. To obtain an idea of the relation P(T ) for a transition from a condensed phase to the gas phase, we roughly approximate the volume change by the volume of the gas formed, V ∼ = n RT . Inserting the two approximations = Vgas , and put PV gas ∼ into (6.12) and taking H as independent of T , we obtain P(T ) by integration, yielding
P ln P0
−H ∼ = nR
1 1 1 −H 1 ∼ , or P = P0 exp . − − T T0 nR T T0 (6.13)
218
6 Thermodynamics of Epitaxial LayerGrowth
H/n is the molar heat of evaporation or sublimation. We see that for the transition from a condensed to a gas phase the pressure approximately obeys an Arrheniuslike dependence over a limited temperature range. Vapor pressures are often tabled in terms of 2 parameters a and b, obtained from (6.13) by using ln(x) = ln(10) × log(x) and putting b = −H/(n R ln(10)). The relation then reads log(P) = a − b/T , with the parameter a depending on the pressure unit; see Table 11.2. The liquidsolid boundary is generally quite steep in the P–T phase diagram due to a very small volume change V during melting. Since the liquid phase may be more dense or less dense than the solid phase V may have either sign. The slope d P/dT of this boundary may hence be positive or negative.
6.1.5 Driving Force for Crystallization To induce a transition from a stable phase to another the parameters temperature and pressure have to be controlled such that the chemical potential in the target phase is smaller than that in the initial phase. Particles from the initial phase will then cross the phase boundary toward the target phase to allow the system for approaching (the new) equilibrium conditions. For a temperature variation at constant pressure the difference T = T − Te between the controlled temperature T and the equilibrium temperature Te at the given pressure is a measure for the deviation from equilibrium. T is a negative quantity and termed supercooling. In case of a liquidsolid equilibrium Te is the melting temperature. The phase transition may as well be induced by varying the pressure by an amount P = P − Pe at constant temperature. If the initial phase is the gaseous phase P and Pe are called supersaturation and saturation vaporpressure, respectively. The achievement of equilibrium in the target phase via either of the two paths is illustrated in Fig. 6.6.
Fig. 6.6 Crossing the phase boundary from a less stable phase α to a stable phase β induced by supercooling T at constant pressure or by supersaturation P at constant temperature
6.1 Phase Equilibria
219
We consider the phase transition induced by supercooling T = T − Te at constant pressure in more detail. At fixed pressure phase α is above the equilibrium temperature Te more stabile than phase β, i.e. μα (T ) < μβ (T ). Below Te , however, μβ (T ) < μα (T ) due to different slopes of the chemical potentials and their intersection at Te , see Fig. 6.5. Phases α and β may exchange particles via the common phase boundary. Since μβ (T ) < μα (T ) below Te , the system can lower the total enthalpy G = G α + G β = n α μα + n β μβ by transferring particles from phase α to phase β: The amount of substance n β in the stable phase β increases on expense of the amount of substance n α in the less stable phase α. The driving force for this phase transition is the difference in the chemical potential μ ≡ μβ − μα .
(6.14)
μ is called growth affinity, or driving force for crystallization if the stable phase β is a solid phase. μ is a negative quantity, though it must be mentioned that μ is often chosen positive in literature. The relation between the driving force μ and the supercooling T is illustrated in Fig. 6.7. We see that an increase of supercooling raises μ and thereby enhances the rate of substance crossing the phase boundary. It should be noted that the respective instable phases may sometimes be experimentally observed to some extent. Such metastable state of a system is indicated by dashed lines in Fig. 6.7. Wellknown examples are heating of a liquid above the boiling point (bumping) or supersaturated vapor in Wilson’s cloud chamber. The effect is particularly pronounced for undercooled metal melts which may still be liquid some tens of degrees °C below the temperature of solidification. The phenomenon should not be confused with the size effect of melting point depression in nanoscale materials that originates from a high surface to volume ratio.
Fig. 6.7 Temperature dependence of the chemical potential μ of phases α and β. The growth affinity μ designates the difference of the chemical potentials μα and μβ induced by a supercooling T to a temperature T< below the equilibrium temperature Te
220
6 Thermodynamics of Epitaxial LayerGrowth
The driving force (6.14) may likewise be induced by a supersaturation P = P − Pe at constant temperature. For solidification from the liquid phase P must be increased if the liquidsolid boundary has a positive slope d P/dT and decreased otherwise. The driving force increases as P is raised, similar to the dependence in supercooling discussed above. To obtain an explicit relation for the temperature dependence of the driving force μ(T ) we expand the function into a Taylor series at equilibrium temperature T = Te , μ(T ) = μβ − μα ∼ =
2 ∂ μβ ∂ 2 μα (T )2 ∂μβ ∂μα − − T + + ··· . ∂T ∂T ∂T 2 ∂T 2 2
Replacing n(∂μ/∂ T ) P = (∂G/∂ T ) P by −S = −H/T we obtain for the expressions in the second summand 2 ∂ μ 1 ∂S 1 ∂H CP . =− =− =− 2 ∂T P n ∂T P nT ∂ T P nT Insertion into μ yields μ(T ) =
1 Htrans C P − T − (T )2 + · · · . n Te 2Te
(6.15)
In this relation Htrans and C P denote the latent heat exchanged with the surroundings during the phase transition and the difference of the specific heat at both sides of the phase boundary, respectively. We note that the driving force μ is not a linear function of the supersaturation T , particularly for significant deviation from the equilibrium temperature Te and a large difference of the specific heat in phases α and β. In a similar way we obtain an explicit relation for the pressure dependence of the driving force μ(P) by expanding the function into a Taylor series at equilibrium pressure P = Pe , μ(P) = μβ − μα ∼ =
2 ∂μα ∂ μβ ∂ 2 μα (P)2 ∂μβ − P + + ··· . − ∂P ∂P ∂ P2 ∂ P2 2
This approach yields a reasonable description of the transition between condensed phases like, e.g., liquid → solid. We replace n(∂μ/∂ P)T = V and (−1/V )(∂ V /∂ P)T = κ (isothermal expansion coefficient), obtaining μ(P) =
1 Ve P − (Ve,β κe,β − Ve,α κe,α )(P)2 /2 + · · · . n
(6.16)
6.1 Phase Equilibria
221
Ve /n designates the difference of the molar volumes at both sides of the phase boundary at equilibrium pressure Pe . This quantity controls the driving force induced by a supersaturation P as a first approximation. The driving force μ(P) of a pressureinduced transition between a gas phase α and a solid phase β may be obtained by integrating over the pressure. We neglect the much smaller solid molar volume and assume the validity of the ideal gas law,
P
μ(P) =
Pe
∼ =−
∂(μ) dP = ∂P P Pe
P Pe
(Vβ − Vα ) dP ∼ = n
P Pe
−
Vα dP n
RT d P = −RT ln(P/Pe ). P
In this case the driving force for crystallization is approximately proportional to the logarithm of the supersaturation ratio P/Pe of the gas phase α.
6.1.6 TwoComponent System Practical real systems usually comprise more than one component. The treatment of a multicomponent system is quite complex. For simplicity we focus on binary systems, which consist of only two components. Such a system still allows for describing basic phenomena occurring in multicomponent systems. Prominent examples are solidification from a solution, e.g., in liquidphase epitaxy, or the solubility of impurities governing doping of semiconductors. A component in a multicomponent system is a chemically distinct constituent whose concentration may be varied independently in the various phases. The number of components Nc specifies how many substances are (at least) needed to describe the composition of the system in all phases. Thus, pure water (H2 O) forms a singlecomponent system, though some dissociation into hydronium cations (H3 O+ ) and hydroxyl anions (OH− ) occurs; the numbers of anions and cations are contrained to be equal due to charge neutrality and may hence not vary independently. If the substances of a system do not react the number of components Nc is simply given by the number of substances. A system containing two components A and B with substance amounts n A and n B is usually characterized by its composition x. This quantity designates the mole fraction of one of the two components, say x ≡ x A . Often x refers to the solute in a solution, i.e. to the minority component A in the substance formed by adding A to B. The respective remaining composition x B follows from the condition x A + x B = 1, yielding x B = 1 − x. x = 0 and x = 1 then designate the pure components B and A, respectively. Equilibrium of a binary system is described by a minimum of Gibbs energy G = H − T S which depends on three independent variables, namely temperature T ,
222
6 Thermodynamics of Epitaxial LayerGrowth
Pressure P, and composition x. In the following we will consider the molar Gibbs energy g. According to (6.1) and (6.5) g is given by g = G/n = (μ A n A + μ B n B )/(n A + n B ) = μ A x A + μ B x B = μ A x + μ B (1 − x) = (μ A − μ B )x + μ B . We assume a solution of A and B with composition x formed at fixed temperature and pressure in a single phase. If the two components are just put together without intermixing or solving, the molar Gibbs energy is a linear function g of the composition x with the starting and ending vertex given by the chemical potentials μ0,B and μ0,A of the pure components B and A, respectively (Fig. 6.8), g(x) = (μ0,A − μ0,B )x + μ0,B .
(6.17)
If now the two components are mixed their particles interact. This is taken into account by an additive term, the molar Gibbs free energy of mixing gM . In general gM contains contributions of both, a change of molar enthalpy h M and a change of molar entropy sM on mixing, gM = h M − T sM .
(6.18)
A particularly simple case is given by an ideal solution, where the interactions between unlike and like particles in the solution are the same. If the interaction energies in the solution are identical to those in the pure components, mixing will not change the overall enthalpy. No heat is then exchanged with the surroundings on mixing, h M = 0. Due to molecular forces being independent on composition, mixing is not accompanied by a change in molar volume, vM = 0. There is, however, a change in molar entropy sM by mixing. The molar Gibbs energy of an ideal solution is hence given by g(x) = g + gM = g − T sM (ideal solution).
(6.19)
Ideal solutions are completely miscible. For a statistically random distribution of A and B particles the change in molar entropy is sM = −R(x A ln x A + x B ln x B ) = −R x ln x + (1 − x) ln(1 − x) (ideal solution), where R is the molar gas constant. The mixinginduced change of molar entropy sM is a positive quantity, because the ln function yields negative values for x ranging from 0 to 1. The term −T sM in g(x) hence effects a deviation from the linear dependence g towards lower values. This decrease of molar Gibbs energy gets stronger for increased temperature, as illustrated for phase α of a twocomponent system in Fig. 6.8a (gray lines at T1 and T2 > T1 ).
6.1 Phase Equilibria
223
Fig. 6.8 a Compositiondependent molar Gibbs energy of an ideal solution with phases α and β at a low temperature T1 (top) where only phase β is stable, and a higher Temperature T2 where phases α and β coexist in equilibrium. Bottom: T –x phase diagram with phases α and β and a range of coexistence. b Real solution with contribution of an endothermal enthalpy on mixing (top), Gibbs energy of phase β at a critical temperature Tc and a lower temperature T2 . The phase diagram at the bottom shows two stable phases β1 and β2 , an area of metastable compositions between the binodal and spinodal curves, and a range of spontaneous decomposition bounded by the spinodal
Figure 6.8a makes clear how the composition of a twocomponent system changes at a transition from a phase α (e.g., the liquid phase) to phase β (solid). At a low temperature T1 the system is in a solid state β: The molar Gibbs energy of the solid gβ (x) is smaller than gα (x) for any composition x. As the temperature is increased both gα (x) and gβ (x) get smaller, cf. g(T ) depicted in Fig. 6.3. Since the temperature dependence in the liquid phase is stronger than in the solid phase gα (x) decreases
224
6 Thermodynamics of Epitaxial LayerGrowth
faster and will be tangent to gβ (x) at a melting temperature Tmelt,B . (The melting temperature Tmelt,B of component B lies above T1 at the lower left corner of the lensshaped area between phases α and β in Fig. 6.8a (bottom).) At Tmelt,B the pure component with the lower melting point starts melting, say component B. Above Tmelt,B the solid and liquid states will coexist within some concentration range x and temperature range T up to a maximum temperature Tmelt,A , the melting point of pure component A. Above Tmelt,A gα (x) < gβ (x) for any composition x, i.e., the system is entirely in the liquid state α. At an intermediate temperature T2 the liquid (α) and solid (β) phases coexist between the compositions x1 and x2 , see Fig. 6.8a. In this range gβ (x) < gα (x) for smaller x, and gα (x) < gβ (x) for larger x, see g(x) at T2 . For a given composition x between x1 and x2 the system attains lowest molar Gibbs energy with a mole fraction x1 in the liquid phase α and a mole fraction x2 in the solid phase β: g takes an equilibrium value gα (x1 ) = ge,α at x1 in phase α, and in phase β accordingly gβ (x2 ) = ge,β at x2 . The molar Gibbs energy of the twophase state lies on the common tangent (∂gα /∂ x)x1 = (∂gβ /∂ x)x2 at the given composition x. A different composition in two phases α and β of a binary system in equilibrium represents a general feature of multicomponent systems. For an average composition x a mole fraction x1 is in phase α and a mole fraction x2 in phase β. x1 and x2 are fixed for a given temperature for any value of x between x1 and x2 . The fraction of substance in phase α is given by xα = (x2 − x)/(x2 − x1 ), and the fraction of substance in phase β is given by xβ = (x − x1 )/(x2 − x1 ). In the example discussed above and in Fig. 6.8a x1 = 0.50 and x2 = 0.62 at T2 . This means a fraction xα = 17% of A + B is in the liquid phase α and has a composition of 50% of component A in A + B, while xβ = 83% is in the solid phase β which has a composition of 62% of A in A + B. If α and β are respectively the liquid and solid phases, then the line between regions α and α + β is called liquidus curve. It is built from all points x1 as the temperature is varied. The line separating regions α + β and β is then called solidus curve. The quotient k0 ≡ xα /xβ is the equilibrium distributioncoefficient. It controls the solubility of diluted components and is used to describe any mixture, e.g. doping or alloying of crystals. Its value exceeds 1 if the coexistence boundary increases as the concentration of the considered component is increased. In real solutions particle interactions A–A, A–B, and B–B are all different. There is hence an enthalpy change h M = 0 upon mixing which may have either sign. A negative value signifies an exothermal reaction, where heat is generated during mixing due to an attractive interaction among the components. A positive value of h M occurs for an endothermal reaction, where heat from the environment is consumed by the system for mixing. Such behavior indicates a diminishment of binding energy in the mixed system and a consequential tendency towards a separation into immiscible components. Most real solutions are miscible over the entire or a certain range of composition x. If the components of the solution are randomly distributed (in crystalline solid solutions with a random distribution of atoms on lattice sites), then the mixture is termed regular solution. Such real solutions have the same mixtureinduced change
6.1 Phase Equilibria
225
of entropy sM as an ideal solution. Due to a finite h M the Gibbs energy of a regular solution differs from that of an ideal solution, g(x) = g + gM = g + h M − T sM (regular, real solution).
(6.20)
The enthalpy change h M is proportional to the concentrations x and (1 − x) of the components of the system A and B, respectively. It may be described by a parameter Ω characterizing the interaction among the components, h M (x) = Ω x(1 − x) = Ω x − x 2 .
(6.21)
Expression (6.21) represents a quadratic correction to the ideal Gibbs energy (6.19) for regular solutions with a maximum (or—for a negative Ω value—a minimum) at x = 0.5. The function is drawn for positive h M in the top panel of Fig. 6.8b. A negative enthalpy change h M upon mixing—indicative for miscibility—leads to a decrease of Gibbs energy g in addition to that induced by the entropy change. There is then a quantitative change of Gibbs energy g(x), but largely only a minor qualitative change in the shape of the function compared to the ideal case shown in Fig. 6.8a. A positive enthalpy change h M > 0 counteracts the entropy change. A large enthalpy change upon mixing leads to a contribution comparable to the term −T sM in the range of medium composition and at sufficiently low temperature. At low temperature the system is considered to be in the solid phase β. Below a critical temperature Tc , Gibbs energy gβ (x) then has a negative curvature (∂ 2 gβ /∂ x 2 < 0) in this range, leading to two minima b1 and b2 . The function gβ (x) is drawn in Fig. 6.8b for a corresponding low temperature T2 . ∂g The minima b1 and b2 correspond to two chemical potentials μi = ∂ xβ xi at the compositions xi . In equilibrium μ1 = μ2 applies, and the chemical potentials are given by the common tangent drawn in Fig. 6.8b. Analogous to the case of the ideal system with two phases α and β discussed above and in Fig. 6.8a, the lowest Gibbs energy of the solid phase gβ (x) is attained if the system decomposes into two solid phases β1 and β2 with compositions x1 and x2 at T2 , respectively. Such behavior is referred to as spinodal decomposition. The minima b1 and b2 represent points for the given temperature of a curve termed binodal. The minima b1 and b2 are separated by a local maximum in the range of medium composition and two inflection points s1 , s2 . The maximum represents an instable composition of the solid solution. Such a maximum emerges as the temperature is decreased below a critical value Tc . The homogeneous solid phase β then spontaneously separates into two immiscible phases with compositions given by the binodal. The miscibility gap gets wider for lower temperature as illustrated at the bottom of Fig. 6.8b. Cooling of the solid therefore leads to a continuous change in the compositions of the two phases β1 and β2 along the binodal—provided the process is sufficiently slow to allow for establishing a thermal equilibrium. If the kinetics in the solid phase is not fast enough, the compositions of the solid phase β may be
226
6 Thermodynamics of Epitaxial LayerGrowth
preserved in a metastable state below Tc . This feature may be employed in epitaxy to fabricate alloy layers, which cannot be grown using equilibriumnear techniques. Regions of negative curvature of gβ (x) lie within the inflection points of the curve (∂ 2 gβ /∂ x 2 = 0). The points are called the spinodes, and their locus as a function of temperature defines the spinodal curve. For compositions bounded by the spinodal, a homogeneous solution is unstable against infinitesimal fluctuations in composition, and there is no thermodynamic barrier to the decomposition into phases β1 and β2 . For regular solutions the spinodal is given by x(1 − x) = RT /2Ω. Epitaxy of multicomponent systems is often performed at low temperatures, and phase separation leading to compositional fluctuations on a small scale may become an issue. The solid may still be deposited in a metastable state when the kinetics is sufficiently slow. The interaction parameter Ω in (6.21) was assumed independent on composition. Since bond length of alloy constituents usually differ significantly (Fig. 2.8a), a solid solution comprises inherent strain. This leads to a composition dependent Ω(x): it requires more energy to incorporate a large atom A into a small crystal B in the alloy A x B1−x at small x than vice versa at large x, yielding Ω(x = 0) > Ω(x = 1). Calculated values of Ω for zincblende semiconductor alloys are given in Table 6.1. Data for zincblende and wurtzite nitrides are reported in [2, 9] and [3], respectively. It must be noted that spinodal decomposition is significantly affected by elastic strain, which in epitaxial heterostructures is generated by lattice misfit. Experiments demonstrated that strained semiconductor alloys can be grown within the miscibility gap well below the critical temperature Tc [5, 6]. Lowering of Tc and narrowing of the immiscibility range bounded by the spinodal is described by an additive term in the bulk free energy that is proportional to the misfit f (2.20a)–(2.20c) of the inplane lattice parameter parallel to the layersubstrate interface [7–10]. The calculations show that the suppression of phase separation is related to the nonlinearity of the interaction parameter Ω(x). Table 6.1 Calculated interaction parameter Ω of cubic semiconductor alloys at T = 800 K; data are from [4] Alloy Ω(x = 0) Ω(x = 0.5) Ω(x = 1) Alx Ga1−x As Inx Ga1−x As GaAsx P1−x Inx Ga1−x P GaAsx Sb1−x Znx Cd1−x Te Hgx Cd1−x Te Znx Hg1−x Te
0.30 3.56 1.07 4.60 3.78 2.24 0.45 2.13
0.30 2.35 0.86 3.07 3.96 2.29 0.38 1.88
0.30 2.68 0.53 2.92 4.51 2.87 0.31 2.15
6.2 Crystalline Growth
227
6.2 Crystalline Growth Growth of a crystalline layer proceeds by the attachment of particles (atoms, molecules) to the surface. The driving force is provided by the chemical potential treated in the previous section. The growth process is basically described in terms of a structural model and kinetic processes, which an impinging particle experiences until being incorporated into the crystal [11, 12]. In the initial stage of growth the formation of the new phase requires, however, some nucleation: small clusters of the particles forming nuclei of the solid. Once stable nuclei are formed the crystal grows according to conditions controlled by properties of the applied phase transition and adjusted growth parameters. In the following we first consider the initial step in terms of the classical theory of nucleation.
6.2.1 Homogeneous ThreeDimensional Nucleation We discussed in Sect. 6.1 how a driving force may be created by varying temperature or pressure to make a solid phase more stable than a liquid or gas phase. If the system was initially in a homogeneous phase, e.g., entirely liquid, the solid phase is not spontaneously formed when the equilibrium boundary is crossed. Instead, the initial phase remains at first in a metastable state of undercooling (of a liquid below the freezing point) or supersaturation (of a vapor below the condensation point). These states are indicated by dashed lines in Figs. 6.2 and 6.7. The reason for the persistence of the no longer most stable phase is the need to create an interface at the boundaries of the new phase. The formation of such an interface consumes some energy, based on the surface energy of each phase. The stable new phase is only formed at sufficient undercooling or supersaturation. Any disturbance like, e.g., a slight agitation or charge, will reduce to some extent the required deviation from equilibrium. Homogeneous nucleation occurs spontaneously and randomly in a homogeneous initial phase. Nucleation is strongly facilitated in presence of preferential nucleation sites. Such a site is any inhomogeneity in the metastable phase, e.g., a substrate or suspended minute particles. In the case of such heterogeneous nucleation, some energy is released by the partial destruction of the preexisting interface. Nucleation is the onset of the phase transition in small regions called nuclei: regions of the new phase with an interface at the boundaries to the initial phase. If a potential nucleus is too small, the energy that would be released by forming its volume is not enough to create its surface, and nucleation does not proceed. The critical size of a nucleus required for growth in homogeneous nucleation is described by thermodynamics. The creation of a nucleus is accompanied by a change of Gibbs energy G N . This quantity is composed of three contributions. First some amount of substance enters the new stable phase, liberating an energy G V proportional to the volume of the nucleus. This process is favorable for the system, and G V is hence a negative
228
6 Thermodynamics of Epitaxial LayerGrowth
quantity. Secondly the interface between the new stable phase and the metastable surrounding phase must be created, yielding a positive cost G S . This contribution of surface free energy is proportional to the area of the interface. The surface free energy γ may be regarded as reversible work to form a unit area of surface (or interface) at equilibrium with constant system volume and number of components. For a crystal γ is always a positive quantity, because otherwise the crystal phase would not be stable. In a solid the magnitude of the surface energy γ per atom is roughly given by half the heat of melting per atom. This rule of thumb originates from the imagination that melting breaks all bonds of an atom, while only half of the bonds of a surface atom are broken. The surface free energy γ is related to the surface stress tensor γ S with the inplane components γiSj , i, j = 1, 2. The γiSj describe the work per unit area for an elastic strain of the surface and may have either sign. A negative sign for compressive strain indicates that work is released when the surface area decreases. The surface stress γiSj designates the difference used in Hooke’s law (2.10) between the stress field in the bulk of the crystal σibulk j (z) in the region near the surface located at z = 0: and the modified stress field σ i j ) dz. The relation between surface stress γiSj and the surface γiSj = (σi j (z) − σibulk j free energy γ is given by the Shuttleworth relation γiSj = γ δi j +
∂γ
, ∂εi j T,μi
δi j being the Kronecker symbol and εi j the inplane components of the strain tensor [13]. In a liquid the second summand equals zero, because a liquid does not resist to strain: If the surface is increased (e.g. by tilting a halffilled vessel) material just flows from the bulk of the liquid to enlarge the surface. In a liquid surface energy γ and surface stress γ S are equal. A third term G E arises in the change of Gibbs energy G N upon creation of a nucleus if the nucleus is subjected to elastic stress. G E is a positive quantity which counteracts the favorable volume term G V and may even suppress nucleation if G E > G V . The total change of Gibbs energy is given by G N = G V + G S + G E .
(6.22)
We consider an unstrained nucleus and neglect the last term G E to obtain a simple expression for the characteristics of homogeneous nucleation. Strain effects are considered in the next section. As a further simplification we assume an isotropic surface free energy γ expressed by a constant energy per unit surface area. In our approach we consider a nucleus with spherical shape, which is realized for a liquid nucleus in the bulk of a vapor phase. In this case we obtain G S = γ S = γ 4πr 2 and G V = (g/v)(4/3)πr 3 . Here r is the radius of the nucleus and S its surface;
6.2 Crystalline Growth
229
Fig. 6.9 Change of Gibbs energy for creating a spherical nucleus with volume VN in homogeneous nucleation. VN∗ and G ∗N are the critical nucleus size and the critical work of nucleus creation, respectively
v is the mole volume of the new phase and g is the change of Gibbs energy of the system by creating one mole of the new phase. Equation (6.21) then reads G N = G S + G V = 4π γ r 2 + (g/v)r 3 /3 (unstrained spherical nucleus). (6.23) The molar change of Gibbs energy g is negative because the new phase is the stable phase for the set conditions. The sum G N = G V + G S is drawn in Fig. 6.9 as a function of nucleus volume VN . We see from Fig. 6.9 that Gibbs energy initially increases during formation of the stable phase due to the unfavorable creation of the boundary to the initial phase. The favorable volume term counterbalances the energy cost of the phase boundary as the nucleus grows. Since increase of the absolute value of the volume term (∝ r 3 ) preponderates that of the surface term (∝ r 2 ) Gibbs energy change G N passes a maximum at some critical radius r ∗ as the nucleus grows. The volume term eventually prevails over the energy cost of the phase boundary, and Gibbs energy change induced by the creation of the nucleus becomes negative. The critical nucleus size denoted by the critical volume VN∗ follows from the maximum condition of G N in (6.23) and is attained at the critical radius r∗ = −
2vγ . g
(6.24)
v designates the molar volume in the new stable phase and g is the change of molar Gibbs energy for a transition to this phase. Inserting r ∗ into (6.23) yields the corresponding critical work required to create such nucleus, G ∗N = (16/3)π γ 3 (v/g)2 .
(6.25)
230
6 Thermodynamics of Epitaxial LayerGrowth
The critical free energy of nucleation G ∗N represents an activation energy for the formation of stable nuclei. The maximum condition of (6.23) ∂(G N )/∂r = 0 implies that the critical nucleus is in thermodynamic equilibrium with the metastable phase at r = r ∗ . The chemical potential of the nucleus is then identical to that of the surroundings. This equilibrium is labile: Gibbs energy degreases for both a decrease and an increase of nucleus size. Nuclei with a radius smaller than r ∗ are instable and tend to dissolve. Above r ∗ nuclei tend to grow since addition of particles to clusters larger than the critical radius releases, rather than costs, energy. Once G N gets negative the nucleus is stable. Growth is then no longer limited by nucleation, albeit it may still be limited by supply of particles, i.e. by a limited diffusion, or by reaction kinetics. Growth of the stable phase is now more favorable until thermodynamic equilibrium is restored. If we apply (6.24) to supercooling expressed by (6.15) we obtain an approximate expression for the critical radius r ∗ of a nucleus depending on the deviation T = T − Te from the equilibrium temperature Te , yielding r∗ ∼ =
2γ vTe , h trans T
h trans being the change of molar enthalpy by the phase transition, i.e., the molar heat of crystallization. In this relation only the linear term in (6.15) was considered, and we used g = μ for a singlecomponent system. Implicitly we assumed that the properties of the system in the nucleus are identical to those in the macroscopic phase. We similarly may apply (6.24) to supersaturation conditions P = P − Pe described by (6.16), yielding 2γ v . r∗ ∼ = ve P Here ve is the difference of molar volume in the metastable and stable phases, respectively. Homogeneous nucleation induces randomly a spontaneous phase transition in the initial phase. This may, e.g., occur in metalorganic vapor phase epitaxy if instable precursors react in the gas phase before being transported to the substrate. In epitaxy such a situation must generally be avoided to maintain control over growth. Epitaxial growth is therefore performed below the critical supersaturation or supercooling required for homogeneous nucleation.
6.2.2 Heterogeneous ThreeDimensional Nucleation Nuclei form in heterogeneous nucleation at preferential sites. In epitaxy such sites are provided by the crystalline substrate. Due to the presence of a preexisting solid phase the interface area to the ambient metastable phase is reduced. The energy barrier to nucleation G ∗N is therefore substantially smaller. Since a part of the substrate is
6.2 Crystalline Growth
231
Fig. 6.10 Nucleus created on a substrate. The balance of surface energies γ leads to a wetting angle Θ
covered by the nucleus a new interface is created between nucleus and substrate. The total change of Gibbs energy G N in heterogeneous nucleation is described by the sum of volume, surface and stress terms given in (6.22) in the same way as in homogeneous nucleation. We again at first neglect elastic stress term G E in (6.22) and consider its effect at the end of this section. We assume a nucleus with the shape of a spherical cap with radius r on a substrate as depicted in Fig. 6.10. Such a case is realized for a liquid nucleus on a structureless substrate. The balance of interface tensions at the line of contact between the three phases of metastable ambient (index a), nucleus (n), and substrate (s) is given by three quantities which represent the energies needed to create unit area of each of the three interfaces. From the figure we read Young’s relation for the absolute values of tensions in balance γas = γns + γan cos Θ, or cos Θ =
γas − γns . γan
(6.26)
The wetting angle Θ may vary between 0 and 180° depending on the degree of wetting corresponding to the affinity of nucleus and substrate materials. Θ hence determines the shape of the nucleus. The volume of a spherical cap is (4/3)πr 3 × f , where the geometrical factor f depends on Θ according to f = 2 − 3 cos Θ + cos3 Θ /4. The shape factor f reduces the volume of the nucleus with respect to homogeneous nucleation and accordingly the volume term of Gibbs energy change G N , yielding = f × G homo . G hetero V V The surface term G S is now composed of two parts related to the interfaces ambientnucleus and nucleussubstrate. Including the corresponding geometrical factors we ∗ in the same way as in homogeneous nucleation, obtain the critical nucleus size rhetero
232
6 Thermodynamics of Epitaxial LayerGrowth
Fig. 6.11 Change of Gibbs energy G N when creating unstrained spherical nuclei with radius r in heterogeneous (black curve) and homogeneous nucleation (gray). r ∗ is the critical nucleus radius
∗ ∗ leading to rhetero = rhomo given by (6.24). The critical free energy of nucleation G ∗N hetero for (unstrained) heterogeneous nucleation is then
G ∗N hetero =
3 2 v 16π γan f. 3 (g)2
(6.27)
Comparing (6.27) to (6.25) shows that G ∗N hetero is reduced with respect to G ∗N homo by the shape factor f which is controlled by the three surface tensions. Note that there is a smaller amount of substance in the nucleus expressed by f for given r ∗ in heterogeneous nucleation. The relation of Gibbs energy change in hetero and homogeneous nucleation is illustrated in Fig. 6.11. Epitaxy is preferred on substrates which are well wet by the epitaxial layer, so as to obtain a large separation to homogeneous critical supersaturation or undercooling. Furthermore, usually a twodimensional atomically flat layerbylayer growth is intended in epitaxy, favored by such a wetting. Effect of Strain The structureless surface of the substrate assumed above is certainly oversimplified. The surface structure of the substrate provides specific sites for nucleating atoms. On a plane substrate such sites are defined by the potential created by the topmost substrate atoms. Section 2.2 pointed out how layer atoms accommodate to the lateral spacing of the substrate atoms. Such an alignment also applies for nucleation at the initial stage of growth. The nucleus is consequently strained and accumulates a strain energy G E , which is—according to Hooke’s law—proportional to the difference of the lateral equilibrium atom spacings of layer atoms and substrate atoms. The strain ε enters Gibbs energy G N of the nucleus in both the volume term G V and the surface term G S discussed in the previous section for the unstrained case. G V
6.2 Crystalline Growth
233
is reduced by an increased chemical potential in the nucleus originating from the strained atomic bonds. The surface energy G S of the strained nucleus is increased in a complex way due to the anisotropic nature of the strain and the effect of a partial elastic strain relaxation at side faces (compare Fig. 7.35a). As a consequence, the energy G ∗N to form a nucleus of critical size is increased in the presence of strain. A simple explicit expression for the effect of the strain ε on the critical free energy of nucleation G ∗N was derived in [14] for the case of a Kossel crystal with firstneighbor interactions in absence of the Poisson effect, G ∗N hetero,strained
=
G ∗N hetero,unstrained
ε 2 2ε −2 1− 1− . E1 μ
(6.28)
The quantity E 1 is the firstneighbor interaction of the bond between two adjacent atoms, and μ is the supersaturation. We note a singularity in (6.28) for μ equals 2ε. At large strain the term G E in (6.23) which counteracts the favorable (negative) volume term G V in Gibbs energy G N will even suppress nucleation.
6.2.3 Growth Modes The surface energies leading to Young’s relation (6.26) affect the initial stage of layer deposition on a substrate of different material, i.e., in heteroepitaxy. Epitaxy usually aims at depositing a layer with a smooth growth surface. This corresponds to a wetting angle of 0 in Young’s relation, or γas = γns + γan . If this condition applies or γas exceeds the sum of the two other interface energies, we obtain complete wetting of the layer on the substrate surface. The condition implies that layer atoms are more strongly attracted to the substrate than to themselves. Growth may then proceed in an atomically flat layerbylayer mode referred to as FrankVan der Merve growth mode in heteroepitaxy. Figure 6.12 illustrates the initial stages of such twodimensional layer growth for different thickness of deposited material. Nucleation in this case proceeds by the formation of twodimensional islands or step advancement as outlined in Sects. 6.2.5 and 6.2.7. A different surface morphology of the layer is observed if layer atoms are more strongly attracted to each other than to the substrate. This situation is expressed in Young’s relation (6.26) by a wetting angle of π , or γns = γas + γan . If this condition applies or γns is even larger, then the layer does not wet the substrate surface. The surface energy of layer plus substrate is minimized if a maximum of substrate surface (with a low surface energy γas ) is not covered by layer material (which has a large surface energy γan ). This results in a threedimensional growth of the layer referred to as VolmerWeber growth mode in heteroepitaxy. Figure 6.12 shows that the layer material is deposited in form of islands, which for thicker deposits eventually coalesce. Here, nucleation proceeds by 3D nuclei as pointed out in the preceding sections.
234
6 Thermodynamics of Epitaxial LayerGrowth
< 1 ML 1  2 ML 2  3 ML Frank  Van der Merve
Volmer  Weber
Stranski  Krastanow
Fig. 6.12 Schematic of the three growth modes in heteroepitaxy, illustrated as a function of approximately equal coverage given in units of monolayers (ML)
Often an intermediate case is found referred to as StranskiKrastanow growth mode (also termed layerplusisland growth). Here the condition γas ≥ γns + γan for FrankVan der Merve growth applies solely for the first deposited monolayer (or the first few monolayers). After exceeding some critical coverage thickness the growth changes to the VolmerWeber case where γns ≥ γas + γan applies. Such change may be induced by the gradual accumulation of strain in the epitaxial layer (Sect. 2.2.6). The layer material then resumes growth in form of threedimensional islands, leaving a twodimensional wetting layer underneath. It should be noted that the critical thickness pointed out here lies usually below that required for the formation of misfit dislocations treated in Sects. 2.2.6 and 2.3. StranskiKrastanow growth has gained much advertence in recent years, because it may be employed for growth of defectfree quantum dots. We therefore will consider this specific growth mode in more detail separately in Sect. 7.3.1. The three growth modes depicted in Fig. 6.12 arise from a thermodynamic consideration of the interface energies. It should be noted that layerbylayer and threedimensional growth also occur in homoepitaxy, i.e., in growth on a substrate of the same material without a wetting issue. Island growth may here originate from a too high growth rate and a related too short adatom diffusion length; such conditions occur at very low growth temperature or high supersaturation. Furthermore, additional growth modes have been introduced to account for frequently observed surface morphologies. On terraced surfaces stepflow growth may be found under suitable conditions; depending on growth parameters also step bunching may occur (Sect. 7.2.4). In the presence of screw dislocations spiral growth (Sect. 6.2.7) or screwisland growth is observed. Eventually for materials with low surface mobility of adatoms columnar growth may be obtained. Similar to VolmerWeber growth islands nucleate, but they do not merge to continuous layers when growth proceeds. A mosaic crystal composed of numerous slightly tilted and twisted columnar crystallites is formed instead.
6.2 Crystalline Growth
235
6.2.4 Equilibrium Surfaces The StranskiKrastanow growth mode described above indicates that under certain conditions a rough or faceted surface is more stable than a flat surface. The reason is the pronounced dependence of the surface energy γ of crystalline solids on the orientation of the surface. In absence of kinetic effects and defects the macroscopic shape of a solid is determined by a minimum of Gibbs free energy G which includes a term of its surface G surf . The equilibrium shape is therefore given by a minimum of G surf for a given volume (or amount of substance), G surf =
γ (n) d A → minimum,
(6.29)
A
where n is the surface normal of the respective part d A of the surface considered. In liquids γ (n) = γ is isotropic, and the equilibrium shape (in absence of gravity) is consequently a sphere which has minimum surface area. This is illustrated in Fig. 6.13 for a small lead particle annealed slightly below and above the melting point. A spherical shape is observed above the melting point (Fig. 6.13b), whereas the equilibrium shape of solid lead Pb in Fig. 6.13a shows sharp facets of the fcc structure. In crystalline solids γ (n) has pronounced minima for specific faces denoted by their Miller indices (hkl). The equilibrium shape is therefore not given by a minimum surface area but by a minimum of G surf . Such a minimum is attained by a polyhedron built from these particular faces of minimum surface energy. While γ of liquids may be readily obtained from capillary experiments, determination of γ (n) from crystal surfaces is difficult. We employ a simple approach to obtain a qualitative estimate on the orientation dependence of γ . We consider a Kossel crystal which assumes atoms as cubes that are bond by their six faces. Only nextneighbor bonding and only a single species of atoms are presumed. The surface energy is evaluated in the framework of the terracestepkink model (Sect. 7.2.1). According to this model a surface may be classified into the three
Fig. 6.13 Insitu imaged scanning electron micrographs of a small lead particle slightly below (a) and above (b) the melting point. Indices in (a) signify equilibrium facets. Reproduced with permission c 1989 Elsevier from [15],
236
6 Thermodynamics of Epitaxial LayerGrowth
categories singular (i.e., perfectly oriented low index plane), vicinal (i.e., slightly inclined with respect to a singular surface), and rough. Let us first consider a singular (001) surface of a Kossel crystal. The surface energy γ is given by the sum of the energies of all bonds broken to create this surface, i.e. γ =
EB ν. 2
(6.30)
ν is the number of bonds on the surface per unit area, E B is the bond energy and the factor 21 takes into account that 1 bond connects 2 atoms (i.e., actually two surfaces are created when a bulk crystal is cleaved into two parts). E B is related to the sublimation energy HS : Releasing an atom from the bulk requires breaking 6 nextneighbor bonds, leading to the relation HS =
6 1 E B , or E B = HS . 2 3
(6.31)
The number ν of bonds per unit area of a (001) surface with n 1 × n 2 atoms along the two orthogonal lateral directions is just ν = n 1 × n 2 /(n 1 × n 2 × a 2 ) = 1/a 2 . To obtain an expression for the orientation dependence of γ we evaluate a vicinal surface which is inclined by a small angle Θ with respect to the (001) plane. Figure 6.14 shows such a vicinal surface of a Kossel crystal. The surface consists of flat terraces separated by steps. We assume the steps are regularly spaced (i.e., absence of stepstep interactions) and of monoatomic height. The number ν of bonds per unit area of the vicinal surface is larger than that of the singular surface and given by ν=
1 (cos Θ + sin Θ). a2
Inserting this expression into (6.30) and using (6.31) yields γ =
HS (cos Θ + sin Θ). 6a 2
(6.32)
Since the angle dependence in the brackets is always greater than unity, the surface energy of a vicinal surface always exceeds that of the corresponding singular surface.
Fig. 6.14 a Cross section of a Kossel crystal (gray) with a vicinal (016) surface (black, dotted), inclined by a small angle Θ with respect to the singular (001) plane
6.2 Crystalline Growth
237
The excess energy originates from the ledge atoms located at the steps. These atoms have an additional missing bond with respect to atoms located on a terrace site. Relation (6.32) leads to a geometrical construction to represent the surface energy of a solid: the Wulff plot. Equation (6.32) describes a circle (in three dimensions a sphere) with diameter 2r = HS /(6a 2 ). In polar coordinates a circle which passes through the origin is given by γ = 2r cos(Θ − ϕ) = 2r (cos Θ cos ϕ + sin Θ sin ϕ), see Fig. 6.15a. If the origin of the circle lies on a line inclined by ϕ = π/4 with respect to a coordinate axis as illustrated in the figure we obtain an expression like (6.32). Due to the symmetry of the considered cubic crystal the entire threedimensional representation of the surface energy γ (Θ) is actually described by eight interpenetrating spheres, the origins of which are lying on the four 111 axes. Figure 6.15 is a twodimensional cross section of γ (Θ) for an azimuth angle of 0. We note that the surface energy γ has pronounced minima (cusps) on the lowindex 100 axes. The equilibrium shape of the Kossel crystal with nextneighbor bonds is found from the surface energy given in Fig. 6.15a by drawing lines from the origin to all possible crystallographic directions through the γ plot. At a point of intersection with the surface of the plot, a plane is constructed perpendicular to the line. Such Wulff plane has an equal γ as the crystal at the intersection point for the orientation given by the line. The equilibrium shape of the crystal is the inner envelope of all such possible Wulff planes. The construction is called Wulff plot. Figure 6.15b shows the Wulff plot of the Kossel crystal with nextneighbor bonds. Since the surface energy of the {100} faces is much lower than that of all other crystallographic faces, the polyhedron given by the inner envelope of all planes is a cube. This is no longer the case if also secondnext neighbor interactions of the atoms are taken into account. Atoms in the considered cubic Kossel crystal have 12 secondnext neighbor atoms located along the 110 directions. Their bonds are weaker than those of nextneighbor atoms. Consequently their contribution to the surface energy is also weaker. Figure 6.16
Fig. 6.15 a Construction of the surface energy γ (Θ) of a Kossel crystal (blue curves) by circles passing through the origin. b Wulff plot of the equilibrium crystal shape (black lines), constructed from the surface energy given in (a)
238
6 Thermodynamics of Epitaxial LayerGrowth
Fig. 6.16 Surface energy γ = γ1 + γ2 of a cubic Kossel crystal with first (γ1 ) and second (γ2 ) nearest neighbor interactions taken into account. The black polygon represents a cross section of the equilibrium shape of the crystal
shows a twodimensional representation of the first and secondnearest neighbor contributions to γ . The contribution γ2 of the weaker secondnearest neighbor bonds to the surface energy γ is constructed in the same way as that of nearest neighbor bonds γ1 , leading to a smaller γ (Θ) plot with cusps along the 110 bond directions. Consequently the sum γ = γ1 + γ2 has also (local) minima along these directions, and the Wulff plot results in a polyhedron with more faces than obtained in the case with only nextneighbor bonds. The equilibrium crystal shape is generally composed of more crystallographic inequivalent facets if the distance of bonding forces increases. Surfaces of small surface energy γ lead to larger facets. On the other hand the facets referring to surfaces with too large surface energy γ lie far away from the origin in a Wulff plot and can hence not contribute to the equilibrium shape. The condition to appear in the equilibrium crystal shape of a cubic crystal in addition to the {001} facets reads for any surface hkl h +k +l × γ001 . γhkl < √ h2 + k2 + l 2 √ According to this relation e.g. {111} facets appear on a cubic crystal if γ111 < 3γ001 applies. A general expression of the minimum surfaceenergy condition (6.29) may be given in terms of Wulff’s theorem γ2 γ3 γ1 = = = · · · = const. r1 r2 r3
(6.33)
The expression is a concise summarization of Wulff’s construction illustrated above. The indices in (6.33) represent the (hkl) sets of the relevant surfaces, and r is the absolute value of the vectors rhkl parallel to the corresponding surface normals nhkl with rhkl ∝ γhkl .
6.2 Crystalline Growth
239
Table 6.2 Calculated surface energies γ of lowindex surfaces, data are given in J/m2 . Type of reconstruction noted at the listed data indicate the corresponding lowestenergy surface selected from various calculated configurations, (1 × 1) relaxed denotes an unreconstructed cleavage surface Solid (100) (110) (111) Sia
1.41
c (4 × 4)
1.70
Gea
1.00
c (4 × 4)
1.17
GaAsb
∼0.96
β 2(2 × 4)
0.83
InAsc
0.75
β 2(2 × 4)
0.66
InPd
∼0.99
β 2(2 × 4)
0.88
(1 × 1) relaxed (1 × 1) relaxed (1 × 1) relaxed (1 × 1) relaxed (1 × 1) relaxed
1.36
7×7
1.01
c(2 × 8)
0.87
(2 × 2) Ga vacancy (2 × 2) In vacancy (2 × 2) In vacancy
0.67 0.99
References [16–19]
Surface energies γ (n) of solids are difficult to measure. During the 1990s firstprinciples calculations based on slab configurations have reached a maturity to yield sufficient numerical precision. It must be noted that γ (n) for a given orientation depends significantly on the structure of the surface. The equilibrium structure may in turn depend on the chemical potential of the ambient. Data given in Table 6.2 represent the lowest values determined for different reconstructions. In the case of GaAs the reconstruction for the broadest range of the anion potential is given. Calculations of data given for the (100) face assumed ambient conditions μAs = μbulk As − 0.3 eV. Details of surface reconstructions are considered in Chap. 7. The equilibrium crystal shape follows from the surface energies γ (n). Applying Wulff’s construction and using calculated surface energies for Asrich conditions we obtain the equilibrium shape of a GaAs crystal shown in Fig. 6.17a [17]. The polyhedron is composed of lowindex planes reflecting the symmetry of the zincblende ¯ face show a different lattice. It should be noted that the (111) face and the (1¯ 1¯ 1) dependence on the ambient chemical potential and hence vary differently in size as the chemical potential is changed. The cross section of the equilibrium crystal shape shown in Fig. 6.17b demonstrates the dependence on the chemical potential μAs . A high value of μAs corresponds to an Asrich (i.e., Gapoor) ambient. The corresponding shape (black polyhedron) is smaller than that expected for a Garich environment (gray polyhedron): Asterminated surfaces have surfaces energies about 20% smaller than those in a Garich ambient [17]. For equilibrium crystal shapes of wurtzite crystals see [20, 21]. Growth occurs at some deviation from thermodynamic equilibrium as pointed out in Sect. 6.1.5. For a singlecomponent system we obtained homogeneous critical nuclei with radius r ∗ for a given driving force μ. The respective relation (6.24) was derived assuming unstrained spherical nuclei and an isotropic surface energy γ .
240
6 Thermodynamics of Epitaxial LayerGrowth
(a) (011)
(110) (001) (110)
(110) 1
(b)
(111) (101)
(010)
(011) 1) 0.5 (11
(001)
(110) (111) (100)
(11 1)
1
(101)
0.5
0.5
1
(11 1) 0.5 1) (11
Fig. 6.17 a Calculated equilibrium crystal shape of GaAs in Asrich ambient (μAs = μAs(bulk) ). ¯ The polyhedron is constructed from the different surface energies of (100), (110), (111), and (1¯ 1¯ 1) facets. b Cross sections calculated for different chemical potentials: black lines μAs = μAs(bulk) , gray lines μAs = μAs(bulk) − 0.3 eV. Energies are given in J/m2 . After [17]
We now take different surface energies γi of inequivalent facets into account, modifying (6.24) to 2νγi , (6.34) μ = ri where i denotes (hkl) sets of the facets. At equilibrium the chemical potentials of all facets must be equal, leading to constant ratios γi /ri , and consequently to Wulff’s theorem (6.33). Equation (6.34) says that the critical size of stable nuclei decreases with increasing deviation μ from equilibrium. The shape of a growing crystal deviates from the equilibrium crystal shape. From (6.34) we note that the differences to the equilibrium get smaller for large dimensions ri . The driving force to maintain the equilibrium crystal shape therefore gets negligible for macroscopic crystals. Their shape is instead determined by kinetic conditions. Surfaces which grow most slowly eventually build the facets of a crystal, as pointed out below. The consequence of a slow growth rate of a facet is illustrated in Fig. 6.18. We assume slowest growth of {111} facets, and, for simplicity, an equal growth rate of a facet along a given crystallographic direction and ¯ facets. Starting from an initial stage 1 the inverse direction, i.e., for {hkl} and {h¯ k¯ l} with almost spherical crystal shape made from the facets indicated in Fig. 6.18, we note that successively all faster growing facets disappear. At stage 4 only the slowly growing {111} facets remain. Differences in the growth rates of inequivalent facets can be utilized to fabricate faceted structures. This topic is discussed in Sect. 12.1.3. Real crystals may deviate from the ideal growth form discussed above. Local differences in the supersaturation and transport to growing surfaces lead to differences in the growth rate of equivalent facets and consequently to different areas of these facets, i.e., to a parallel displacement of the facets with respect to the ideal form. Moreover, crystal defects may significantly accelerate the growth rate of facets. Particularly screw dislocations build a continuous source of surface steps which facilitate the attachment of particles impinging on the surface and the subsequent incorporation into the crystal. Kinetic processes in the growth at steps are considered in Sect. 7.2.4.
6.2 Crystalline Growth Fig. 6.18 Facets of a growing crystal at successive stages. Different growth rates are assumed along the indicated directions, with a minimum along 111
241 [110]
[221] [111] [112]
12 3
4 [001]
6.2.5 TwoDimensional Nucleation Flat surfaces have generally slow growth rates, because they hardly offer favorable sites like steps for the attachment of atoms from the ambient phase. In absence of terrace steps and defects like screw dislocations, growth of atomically flat surfaces in the layerbylayer mode proceeds by clusters of adsorbed atoms with a sufficient size. They form twodimensional (2D) nuclei which provide preferential sites for the attachment of further atoms at their perimeter. Which mode of nucleation, 2D or 3D, is thermodynamically preferred depends on the difference in interface energies and strain, cf. Sect. 6.2.3. 2D nuclei must exceed a critical size for stable growth in analogy to threedimensional nuclei treated in the previous section. We consider the critical size of a twodimensional nucleus for a onecomponent system. For simplicity we assume a circular shape of the 2D nucleus with radius ρ and monoatomic height as depicted in Fig. 6.19. The formation of a 2D cluster comprising an amount of substance n changes the Gibbs energy due to the transition from the ambient phase to the more stable solid phase by G 2D n = nμ. Since in the assumed onecomponent system the 2D cluster grows on a surface made of atoms of the same kind, no change of the interface energy of the system occurs. There is, however, a contribution G 2D γ originating from the ledge atoms of the cluster. They have fewer neighbors and thus more unsaturated bonds, which add a positive destabilizing boundary free energy to the total free energy of the 2D cluster. The contribution G 2D γ is the 1D analog of the surface free energy, which is generally measured as the surface tension. G 2D γ can hence be considered as a line tension and is proportional to the length of the 2D cluster perimeter 2πρ, ρ being the radius of the nucleus. A specific free step energy γp assumed to be isotropic
Fig. 6.19 Twodimensional nucleus of circular shape with monoatomic height on a flat surface
242
6 Thermodynamics of Epitaxial LayerGrowth
is taken as proportionality factor. If one mole of atoms in a circular 2D island covers an area a, the change of Gibbs energy by the formation of a 2D cluster is given by 2D 2D G 2D N = G n + G γ =
πρ 2 μ + 2πργp . a
(6.35)
The critical 2D nucleus size is obtained similar to the 3D case from the maximum condition of G 2D N , yielding the critical radius of a twodimensional nucleus ρ∗ =
aγp , μ
(6.36)
and the activation energy ∗ G 2D =π N
aγp2 μ
.
(6.37)
a designates the specific area covered by one mole of atoms, and γp the excess energy per length of atoms located at the perimeter of the in 2D nucleus with respect to the energy of atoms located on a flat surface. The prefactor π in (6.37) applies for a circular shape of the 2D nucleus and is to be replaced by another form factor for a different shape (e.g., (1 + α)2 /α for rectangular nuclei, α being the ratio of the side lengths). Relations (6.36), (6.37) are analogous to (6.24) and (6.25) obtained for threedimensional nuclei. We note that the driving force μ enters the 2D activation linearly in the denominator, while a quadratic dependence is found in the 3D case (6.25). For a given small deviation from equilibrium μ the formation energy of a 2D nucleus is hence smaller than in homogeneous 3D nucleation. The shape of 2D nuclei and subsequently growing islands is not necessarily given by the equilibrium crystal shape, due to the required deviation from equilibrium. Furthermore, the shape is affected by the structure of the substrate surface and kinetic effects considered in more detail in Chap. 7. Evidence for such effects are given in Fig. 6.20. The in situ recorded scanning tunneling micrographs show two Si islands growing on a Si(111) substrate [22]. During growth the islands clearly show a triangular shape (Fig. 6.20a). When the growth is interrupted and the temperature is raised, the lateral form gradually turns into a hexagonlike shape (Fig. 6.20b). Here, edges perpendicular to [112] are somewhat shorter than those perpendicular to [112], indicating a lower energy of the latter. When growth is resumed, the islands quickly adopt the initial triangular shape (Fig. 6.20c). To provide some visual evidence for critical 2D nucleus formation, we consider the assembly of CoSi clusters at 400 °C on a Si(111)(7 × 7) surface. High speed scanning tunneling microscopy represents one such cluster as a single bright protrusion, though it probably contains 3 Si atoms and 6 Co atoms [23]. STM images show that the clusters are mobile on the Si surface [24]. Figure 6.21 shows a series of STM scans over 8 × 8 nm2 captured in 5 s frames. We note a steady change of the imaged configuration, until the cluster labeled Y occupies the vacancy visible in Fig. 6.21c.
6.2 Crystalline Growth
243
Fig. 6.20 Scanning tunneling images of twodimensional Si islands on Si(111) substrate, recorded during molecular beam epitaxy at 725 K (a, c) and after 18 min annealing at 775 K (b). The image c 2004 IOP size is 55 × 55 nm2 . Reproduced with permission from [22],
(a)
0 sec
(b)
5 sec
(d)
15 sec
(c)
10 sec
(e)
20 sec
(f)
25 sec
Fig. 6.21 In situ recorded formation of a critical nucleus of CoSi clusters (white protrusions) on a Si(111)(7 × 7) surface. X and Y label two particular clusters. At (d) cluster Y has moved to c complete a ringlike structure consisting of 6 clusters. Reproduced with permission from [24], 2007 RSC Publishing
The ring composed of 6 clusters is fairly stable. Eventually a cluster detaches (arrow in Fig. 6.21f) and the ringstructure decomposes. Studies reported in [24] show that the i = 6 configuration represents a critical nucleus for the studied system. Once one of the 6 clusters moves to occupy the vacant site in the center and a seventh cluster attaches to the ring, a stable nucleus with i = 7 clusters is formed. ∗ (6.37) represents an activation The critical free energy of nucleation G 2D N energy for the formation of 2D nuclei. The rate of formation per unit area of such nuclei is given by the Arrhenius dependence ∗ G 2D N . (6.38) j 2D = j02D exp kT
244
6 Thermodynamics of Epitaxial LayerGrowth
The prefactor j02D follows from kinetic considerations of the nucleation process on an atomic scale.
6.2.6 Island Growth and Coalescence Using j 2D (given in units of m−2 × s−1 ) we obtain the total nucleation rate J 2D on a surface of a given area L × L by the product J 2D = j 2D × L 2 . Twodimensional growth of a layer proceeds by a lateral growth of 2D nuclei, which eventually coalesce and form a complete coverage of the surface by a new monolayer. The 2D nuclei grow by the attachment of atoms at the step formed at their perimeter. The time T required to grow a monolayer thick complete coverage may therefore be expressed in terms of the velocity of step advancement vstep by the relation T ∼ = L/vstep . The number of nuclei N created during the time interval T of one monolayer formation is then given by N∼ = j 2D × L 3 /vstep . = j 2D × L 2 × T ∼ From this relation we may derive an estimate for the velocity R of the growth front along the surface normal. The growth rate R depends on whether only a single nucleus grows and eventually completes a new monolayer on the considered area L 2 , or multinuclear (or even multilayer) growth occurs. In the first case a complete monolayer originates from only a single nucleus, i.e., the number of new forming additional nuclei is N < 1. This condition corresponds to L < 3 vstep /j 2D , i.e., it is favored for a small area. The twodimensional growth of the epilayer proceeds by a formation of a nucleus and its lateral growth until the completion of a monolayer, before the subsequent nucleus is created. The growth rate R is then given by the total nucleation rate J 2D times the thickness d of the 2D nucleus, i.e., R = j 2D L 2 d (N < 1, single nucleus).
(6.39)
Generally the condition N < 1 does not apply, because the area of an epilayer is large (compared to the diffusion length of an atom on the surface) and supersaturation is not thus small to allow only for the creation of just a single nucleus. The more general case N > 1 for the number of nuclei N created during the time interval T of monolayer growth corresponds to L > 3 vstep /j 2D . More than just one nucleus is formed, and all nuclei contribute to the growing layer. In such a multinuclear layerbylayer growth nuclei have a mean time t to grow to 2D islands with a mean radius l before meeting another growing 2D island originating from another nucleus. This time interval is of the order t ∼ l/vstep ∼ = 1/J 2D ∼ = ( j 2D × πl 2 )−1 . The mean radius = 3 2D ∼ may therefore be written l = vstep /(π j ). The growth rate R is in this case given by
2D 2 ∼ 2 πl d d j 2D (N > 1, many nuclei), (6.40) R∼ j = 3 π vstep =
6.2 Crystalline Growth
245
where d is the thickness of the 2D nuclei. If growth is initiated on an flat surface without steps, the first nuclei appear simultaneously. When the isolated nuclei (which subsequently become islands) grow, their total perimeter increases. The total perimeter represents also the total step length. Layer growth proceeds by the overall advancement of this step via the attachment of atoms, which arrive at the surface from the ambient and diffuse laterally. Once the growing islands come into contact, they coalesce and their steps annihilate. The total step length therefore decreases at the onset of island coalescence. If no additional nucleation occurs on top of large and still growing 2D islands, the total step length reaches a minimum (0 without any nucleation) when the layer is completed. The total step length oscillates between a minimum and a maximum. Since the incorporation of atoms into the solid occurs at surface steps, also the growth rate oscillates. The oscillation period corresponds 2 j 2D )−1/3 . Usually after to the growth duration of one monolayer, i.e., T ∼ = (π vstep deposition of a few monolayers there occurs gradually additional nucleation on large and still growing 2D islands, giving rise to growth on various heights. As a result, the oscillations are gradually damped and the growth rate eventually approaches a constant value. Such a behavior is often observed in the intensity of the specular reflectivity of reflection high energy electron diffraction (RHEED) applied during growth in molecularbeam epitaxy (Sect. 8.3): A high diffraction intensity reflected from a smooth completed layer changes periodically with a low intensity reflected from a rough layer composed of many 2D islands. Some of the growth features mentioned above are illustrated in the series of scanning tunneling micrographs Fig. 6.22, which were recorded in situ during homoepitaxial growth of Si/Si(111) [25]. The twodimensional islands have a triangular shape, similar to those shown in Fig. 6.20a, c and those studied in more detail in Sect. 7.2.8. In Fig. 6.22 epitaxy does not proceed in a layerbylayer mode at the given growth conditions. Instead, additional nucleation occurs already before islands start to coalesce (arrow in the middle of the frames). We still observe lateral growth of the islands at their perimeter. Eventually the islands coalescence and the total perimeter decreases (Fig. 6.22d). The left arrow in Fig. 6.22c marks an island, which is rotated by 180° with respect to the other islands. This orientation corresponds to a stacking fault along the [111] growth direction. The chosen growth temperature is significantly
Fig. 6.22 Growth of Si on Si(111) during chemical vapor deposition at 485 °C. The arrows in frames (b) to (d) mark an island which grows by an additional layer each image. The left arrow in (c) designates an island, which is rotated by 180° and represents the onset of a stacking fault. c 1993 Springer The image size is 200 × 180 nm2 . Reproduced with permission from [25],
246 1.0
visible substrate 0.8
Coverage
Fig. 6.23 Buildup of the surface coverage in each layer during epitaxial growth. Distribution of coverages in the first five layers as counted from the Si/Si(111) growth sequence shown in Fig. 6.22. Reproduced with permission c 1993 Springer from [25],
6 Thermodynamics of Epitaxial LayerGrowth
0.6 0.4
layer 1 layer 2
layer 3
0.2
layer 4 0.0 0.0
0.4
0.8
1.2
layer 5 1.6
2.0
2.4
Total coverage (units of layers)
lower than that usually applied in growth of silicon. This leads to structural defects, which are not annealed during further growth. In the case shown in Figs. 6.22c, d an antiphase domain boundary is formed when islands coalesce, cf. the schematics Figs. 2.26 and 2.33. A measure for layerbylayer growth is obtained if the coverage buildup of each layer is plotted as a function of the total coverage or of growth time. The curves in Fig. 6.23 correspond to the simultaneous growth of multiple monolayers visible in the series of Fig. 6.22. We note a set of curves with a slow progression: Even after deposition of 2.4 layers (which actually are bilayers in the stacking AaBbCc of the diamond structure of Si) 40% of the substrate are still not covered. This is a further indicative for a low surface mobility of adatoms due to the low growth temperature applied for in situ characterization.
6.2.7 Growth without Nucleation The nucleation work pointed out in Sects. 6.2.2 and 6.2.5 (3D and 2D nucleation) impose a significant supersaturation required for nucleation and consequential layer growth. This is in remarkable disagreement with frequent experimental findings of growth occurring already at negligible supersaturation. The reason for such apparent discrepancy is found in the fact that growth occurs at steps on the surface, and surfaces without any steps are hardly realized. There are two major sources of persisting monoatomic surface steps: A vicinal orientation of the surface and screw dislocations. Wafer crystals cut with respect to a specific crystallographic orientation always have a slight misorientation. The result of such offcut is the formation of a vicinal surface composed of terraces and steps as illustrated in Fig. 6.14. For a typical offcut of Θ = 0.1 degree the terrace width is l = tan−1 Θ × a ∼ = 2 µm for an assumed
6.2 Crystalline Growth
247
Fig. 6.24 Screw dislocations on the Gaface of a (0001) oriented GaN/sapphire layer with total Burgers vector c[0001]. The image size is 230 × 230 nm2 . Reproduced with permission from [27], c 1998 AVS
30 nm ∼ 0.3 nm of an epitaxial monolayer (for, e.g., zincblende material typical thickness a = a001 = 21 a0 ) and equally spaced steps. Such terrace width is usually well below the mean diffusion length of adatoms, allowing for atoms which arrived from the ambient at the surface to be attached at the terrace step. Consequently there is no need for nucleation to grow on a vicinal surface. The resulting growth proceeds by the advancement of more or less parallel steps and is referred to as stepflow growth. The effect is often designedly applied to facilitate layer growth in epitaxy. For this purpose wafers with a specified offcut in a desired direction to choose the terrace width and the kind of vicinal surface are used. Stepflow growth is discussed in more detail in terms of growth kinetics in Sect. 7.2.3. A second source of steps persisting on a surface during growth is provided by screw dislocations (Sect. 2.3) [26]. It was found that the distance between two neighboring arms of the spiral is directly proportional to the size of a 2D nucleus which depends on the supersaturation. The slope of the growth spiral around the core of the screw dislocation is then direct proportional to the supersaturation. An example of screw dislocations in the metalorganic vaporphase epitaxy of GaN/Al2 O3 is given in Fig. 6.24 [27]. The scanning tunneling micrograph shows two adjacent screw dislocations with Burgers vectors c[0001] pointing in the opposite direction to that of the screw dislocation on an Nface of GaN shown in Fig. 2.32b. Their spirals combine, yielding a doubled Burgers vector. We should note that even perfect crystal surfaces are generally not atomically flat and may intrinsically provide sites for a preferential attachment of atoms. Atomistic details are considered in Sect. 7.2.
6.2.8 Ripening Process After Growth Interruption The interruption of the growth process corresponds to a change of the chemical potential of the surface with respect to that of the ambient. Since growth occurs at a depart
248
6 Thermodynamics of Epitaxial LayerGrowth
Fig. 6.25 Ostwald ripening of 2D Si islands on Si(111). (a) Image scanned during growth at 520 °C, (b) image scanned after a 23 min interruption of the deposition at the same temperature. From [28]
a)
A
b)
A
from thermal equilibrium, a sudden interruption of this process leaves the surface in a nonequilibrium state. An equilibration is therefore initiated comprising diffusion and evaporation–condensation processes. Changes of the surface morphology occurring during equilibration are often described by Ostwald ripening. The term denotes the evolution of an inhomogeneous structure (also in solid or liquid solutions) over time first described by Wilhelm Ostwald in 1896. Generally speaking, large particles (with a lower surface to volume ratio) grow in size, drawing material from smaller particles, which shrink. In the process, many initially formed small particles (or crystals, islands) slowly disappear, except for a few that grow larger, at the expense of the small particles. As a result, the broad size distribution of particles gradually gets more narrow as the mean particle size increases. An example of Ostwald ripening initiated by an interruption of the homoepitaxial chemical vapor deposition of Si is shown in Fig. 6.25 [28]. All small islands with an unfavorable ratio of perimeter over area marked by an arrow in Fig. 6.25a dissolve. Their material feeds the larger islands remaining 23 min later, cf. Fig. 6.25b. In addition, holes in the main terrace tend to close (see, e.g., the hole near label A).
6.3 Problems Chapter 6 6.1 For solid silicon, the molar entropy is 18.8 J/(mol K) and the molar volume is 12.1 cm3 /mol at 1 bar and 298 K. Estimate the change in the chemical potential μ(P, T ) for (a) a decrease in temperature by 5 K at P = 1 bar. (b) an increase in pressure by 5 bar at T = 298 K. 6.2 Differences in the bonding of InN compared to GaN or AlN lead to a large miscibility gap of solid solutions. We consider an unstrained Inx Ga1−x N alloy described by a regular solution with an interaction parameter of 32 kJ/mol. (a) Calculate the molar Gibbs free energy of mixing for an indium composition x = 0.2 at 800 °C and 1200 °C. (b) At which temperature is Gibbs free energy of mixing zero at the given composition?
6.4 General Reading Chapter 6
249
(c) Determine the indium compositions for the locus of the spinodal at 800 °C. 6.3 Construct the cross section of a Wulff plot for GaAs in a {110} plane, using the surface energies given in Table 6.2. Consider only the listed facets, assuming for simplicity equal surface energies for {hkl} faces of different polarity. Verify that × γ011 . the considered facets fulfill the condition γhkl < √hh+k+l 2 +k 2 +l 2 6.4 Consider a rectangular twodimensional silicon island on a flat Si(001) surface, bound by two S A and two S B singlelayer steps with step energies of 0.02 eV/a and 0.1 eV/a, respectively, a being the 1 × 1 surface lattice constant of 3.8 Å. Assume that the shape of the island reflects the ratio of the edge energies, and the length of an Sb side is 1.9 nm. (a) Calculate the free step energy of the island boundary, neglecting the small contribution of the four edges. What would be the free step energy, if the island had the same area, but S B steps also had the step energy of S A steps? (b) In a very simplified description the island of (a) is considered to have a circular shape of equal area bounded by a step with 0.02 eV/3.8 Å step energy. Calculate the number of atoms in the island, if the specific area of a layer is 3 × 104 m2 /mol. Determine the activation energy (in kJ/mol) for the formation of a stable twodimensional nucleus, if the island exceeds the critical radius by a factor of 10. 6.5 The conditions for the epitaxy of (001)oriented GaAs are set to a growth rate of 2 µm/h. (a) Express the growth rate in units of monolayers per second. (b) Estimate the approximate step velocity for layerbylayer growth from multiple nuclei, if the nucleation rate is 1 × 1013 m−2 × s−1 . What is the mean radius of the 2D islands just before coalescence?
6.4 General Reading Chapter 6 T. Nishinaga (Ed.), Handbook of Crystal Growth, vol. I Fundamentals: Part A Thermodynamics and Kinetics, Part B Transport and Stability (Elsevier, Amsterdam 2014) I.V. Markov, Crystal Growth for Beginners,Fundamentals of Nucleation, Crystal Growth, and Epitaxy, 3rd edn., (World Scientific, Singapore, 2017) A.A. Chernov (ed.), Modern Crystallography, vol. III, Crystal Growth. Springer Series Sol. State Sci., vol. 36 (Springer, Berlin, 1985)
References 1. K.Th. Wilke, J. Bohm, Kristallzüchtung (Harry Deutsch, Thun/Frankfurt a. M., 1999). (Crystal Growing, German) 2. I. Ho, G.B. Stringfellow, Solid phase immiscibility in GaInN. Appl. Phys. Lett. 69, 2701 (1996) 3. T. Takayama, Theoretical analysis of unstable twophase region and microscopic structure in wurtzite and zincblende InGaN using modified valence force field model. J. App. Phys. 88, 1104 (2000)
250
6 Thermodynamics of Epitaxial LayerGrowth
4. S.H. Wei, L.G. Ferreira, A. Zunger, Firstprinciples calculation of temperaturecomposition phase diagrams of semiconductor alloys. Phys. Rev. B 41, 8240 (1990) 5. M. Quillec, C. Daguet, J.L. Benchimol, H. Launois, Inx Ga1−x As y P1−y alloy stabilization by the InP substrate inside an unstable region in liquid phase epitaxy. Appl. Phys. Lett. 40, 325 (1982) 6. M.J. Jou, Y.T. Cherng, H.R. Jen, G.B. Stringfellow, Organometallic vapor phase epitaxial growth of a new semiconductor alloy: GaP1−x Sbx . Appl. Phys. Lett. 52, 549 (1988) 7. W.A. Jesser, D. KuhlmannWilsdorf, On the theory of interfacial energy and strain of epitaxial overgrowths in parallel alignment on single crystal substrates. Phys. Status Solidi 19, 95 (1967) 8. D.M. Wood, A. Zunger, Epitaxial effects on coherent phase diagrams of alloys. Phys. Rev. B 40, 4062 (1989) 9. SYu. Karpov, N.I. Podolskaya, I.A. Zhmakin, A.I. Zhmakin, Statistical model of ternary groupIII nitrides. Phys. Rev. B 70, 235203 (2004) 10. SYu. Karpov, Suppression of phase separation in InGaN due to elastic strain. MRS Internet J. Nitride Semicond. Res. 3, 16 (1998) 11. W. Kossel, Zur Theorie des Kristallwachstums. Nachr. Akad. Wiss. Gött. Math.Wiss. Kl. 135–143, (1927). (in German) 12. I.N. Stranski, Zur Theorie des Kristallwachstums. Z. Phys. Chem. 136, 259 (1928). (in German) 13. R. Shuttleworth, The surface tension of solids. Proc. Phys. Soc. A 63, 444 (1950) 14. I.V. Markov, Crystal Growth for Beginners (World Scientific, Singapore, 1995) 15. J.J. Métois, J.C. Heyraud, SEM studies of equilibrium forms: roughening transition and surface melting of indium and lead crystals. Ultramicroscopy 31, 73 (1989) 16. A.A. Stekolnikov, J. Furthmüller, F. Bechstedt, Absolute surface energies of groupIV semiconductors: dependence on orientation and reconstruction. Phys. Rev. B 65, 115318 (2002) 17. N. Moll, A. Kley, E. Pehlke, M. Scheffler, GaAs equilibrium crystal shape from first principles. Phys. Rev. B 54, 8844 (1996) 18. N. Moll, M. Scheffler, E. Pehlke, Influence of stress on the equilibrium shape of strained quantum dots. Phys. Rev. B 58, 4566 (1998) 19. Q.K.K. Liu, N. Moll, M. Scheffler, E. Pehlke, Equilibrium shapes and energies of coherent strained InP islands. Phys. Rev. B 60, 17008 (1999) 20. H. Li, L. Geelhaar, H. Riechert, C. Draxl, Computing equilibrium shapes of wurtzite crystals: the example of GaN. Phys. Rev. Lett. 115, 085503 (2015) 21. B.N. Bryant, A. Hirai, E.C. Young, S. Nakamura, J.S. Speck, Quasiequilibrium crystal shapes and kinetic Wulff plots for gallium nitride grown by hydride vapor phase epitaxy. J. Crystal Growth 369, 14 (2013) 22. B. Voigtländer, M. Kawamura, N. Paul, V. Cherepanov, Formation of Si/Ge nanostructures at surfaces by selforganization. J. Phys. Condens. Matter 16, S1535 (2004) 23. M.A.K. Zilani, Y.Y. Sun, H. Xu, L. Liu, Y.P. Feng, X.S. Wang, A.T.S. We, Reactive Co magic cluster formation on Si(111)7 × 7. Phys. Rev. B 72, 193402 (2005) 24. W.J. Ong, E.S. Tok, Configuration dependent critical nuclei in the self assembly of magic clusters. Phys. Chem. Chem. Phys. 9, 991 (2007) 25. U. Köhler, L. Andersohn, B. Dahlheimer, Timeresolved observation of CVDgrowth of silicon on Si(111) with STM. Appl. Phys. A 57, 491 (1993) 26. W.K. Burton, N. Cabrera, F.C. Frank, The growth of crystals and the equilibrium structure of their surface. Philos. Trans. R. Soc. Lond. A 243, 299 (1951) 27. A.R. Smith, V. Ramachandran, R.M. Feenstra, D.W. Grewe, M.S. Shin, M. Skowronski, J. Neugebauer, J.E. Northrup, Wurtzite GaN surface structures studied by scanning tunneling microscopy and reflection high energy electron diffraction. J. Vac. Sci. Technol. A 16, 1641 (1998) 28. U. Köhler, Kristallwachstum unter dem Rastertunnelmikroskop. Phys. Bl. 51, 843 (1995). (in German)
Chapter 7
Atomistic Aspects of Epitaxial LayerGrowth
Abstract Crystal growth far from thermodynamic equilibrium is affected by kinetic barriers. This chapter describes nucleation and growth in terms of atomistic processes, which are characterized by such energy barriers. We consider the ideal and the real structure of a crystal surface, and discuss kinetic steps occurring during nucleation and growth. At the end of the chapter phenomena of selforganization employed for epitaxial growth of nanostructures are presented.
The description of growth treated in the previous chapter was based on macroscopic quantities: Thermodynamics describes collective motions of particles in terms of a macroscopic growth affinity. It accounts well for the direction a system tends to reach and describes conditions particularly near thermal equilibrium. Crystal growth is actually governed by a competition between kinetic and thermodynamic processes. Growth conditions in epitaxy are sometimes far from equilibrium and processes may largely be determined by kinetics. Particularly on a short time scale a kinetic description of growth on an atomic level may be more appropriate. The kinetics of epitaxial growth can usually be described by only a few categories of atomistic rate processes. Such processes strongly depend on the specific location of an atom on or near the surface. We therefore first consider the surface structure of a solid.
7.1 Surface Structure The equilibrium conditions for surface atoms are different from those of bulk atoms due to the absence of neighboring atoms on one side. Therefore the atomistic structure of the surface does usually not coincide with that of the bulk. This is particularly true for semiconductors, which have pronounced directional bonds. By contrast metals have a chemical bond which is basically not directed, and in many cases the surface lattice corresponds to the bulk lattice. Starting with a simple model we will consider some examples of semiconductorsurface reconstructions to provide a basis for the description of growth on the atomic scale.
© Springer Nature Switzerland AG 2020 U. W. Pohl, Epitaxy of Semiconductors, Graduate Texts in Physics, https://doi.org/10.1007/9783030438692_7
251
252
7 Atomistic Aspects of Epitaxial LayerGrowth
7.1.1 The Kink Site of a Kossel Crystal The Kossel crystal is a simple model which assumes the atoms as cubes (more generally the building blocks which may be atoms, ions, or molecules). In the most simple approach only nearestneighbor interaction is assumed, i.e., only the bond at the face between adjacent cubes. Let us consider a surface with a monoatomic step as shown in Fig. 7.1. Atoms at different positions on the surface have different numbers of neighboring atoms. Consequently these atoms are differently bound to the surface. An atom embedded in the uppermost layer of a flat surface—at position 1 in Fig. 7.1—has 4 lateral bonds and 1 bond to the layer below, leaving just a single unsaturated bond. The atom embedded into the step (site 2) has only 3 lateral bonds and 1 vertical bond, leaving two bonds unsaturated. This atom is hence less tightly bound as that at site 1 and may more easily be detached from the surface. A site of particular importance is position 3, the socalled kink site. We note that 3 bonds are unsaturated and 3 bonds are attached to neighboring atoms of the solid. This means that exactly one half of the bonds is unsaturated. The three saturated bonds attach the atom to a half row of atoms (the row with the atom embedded at site 2), to a half crystal plane (the plane with the atom embedded at site 1), and to a half bulk crystal (the crystal underneath the atom), respectively. The kink position is therefore also referred to as halfcrystal position. Crystal growth basically proceeds via the incorporation of atoms at this site. The work ϕ 21 required to detach an atom from a kink position is just half the work required to detach an atom located in the bulk. We note that an attachment or detachment of an atom at a kink site leaves the number of unsaturated bonds at the surface unchanged: the initial configuration is reproduced. Since the number of unsaturated bonds is associated with the surface energy no change occurs for an occupation of this site. This means that the work required to add or remove a kink atom is equal to the chemical potential of the crystal. This implies that the chemical potential of the atom at a kink site is equal to
1
3 4
2 5
Fig. 7.1 Important sites of an atom on a crystal surface. Numbers signify unsaturated nearestneighbor bonds of atoms located at the marked sites: 1—atom embedded in the uppermost surface layer, 2—atom embedded into a step edge, 3—atom at a kink site, 4—atom attached to a step, 5—atom adsorbed on the surface (adatom)
7.1 Surface Structure
253
that of the crystal. Transferring an atom from the ambient to a kink site of the crystal surface (or vice versa) is therefore equal to the difference of the chemical potentials of the ambient and the crystal. In thermodynamic equilibrium of a (large) crystal with an ambient the probabilities of attachment and detachment of a kink atom are equal. Sites which provide more bonds (like, e.g., a hole in a surface at site 1 in Fig. 7.1) have a larger probability for attachment with respect to detachment. In equilibrium such sites are hence probably occupied. On the other hand sites with less bonds as a kink position like sites 4 and 5 have a smaller probability to be occupied in thermal equilibrium. As a consequence a crystal in thermal equilibrium with an ambient is bounded by flat faces: the equilibrium surfaces discussed in Sect. 6.2.4. It should be noted that perfect atomically flat surfaces do not exist at finite temperatures: The action of entropy always gives rise to some roughening.
7.1.2 Surfaces of a Kossel Crystal Crystal faces of different crystallographic orientation differ in their surface structure. We first consider the lowindex faces of a Kossel crystal. A schematic of this model crystal with {100}, {110}, and {111} faces is given in Fig. 7.2. The figure illustrates that the depicted lowindex planes differ significantly with respect to their roughness on an atomic scale: {100} faces are perfectly flat and {111} faces are rough. Generally crystal surfaces can be classified into three groups, namely flat (F), stepped (S), and kinked (K). Lowindex faces of all groups represent singular faces. The classification follows from a consideration of rows of atoms with a most dense arrangement. The direction of a densely packed row of atoms is referred to as nearestneighbor periodicbondchain. Faces of any lattice which are parallel to at least two nearestneighbor periodicbondchains are called F (flat) faces. Usually these faces have the highest surface density of atoms. In a Kossel crystal closepacked
Fig. 7.2 Kossel crystal with flat (F), stepped (S), and kinked (K) surfaces
F S K
254
7 Atomistic Aspects of Epitaxial LayerGrowth
atoms are aligned along a 100 direction. F faces are therefore {100} faces. Each atom on such a surface offers one unsaturated nearestneighbor bond. Faces which comprise one nearestneighbor periodicbondchain are called S (stepped) faces. S faces of a Kossel crystal with lowest indices are {110} faces like those depicted in Fig. 7.2. Each atom on such an S face offers two unsaturated nearestneighbor bonds. Faces which comprise no nearestneighbor periodicbondchain are called K (kinked) faces. K faces of a Kossel crystal with lowest indices are {111} faces. Each atom of a K face offers three unsaturated nearestneighbor bonds. In Sect. 6.2 we pointed out the importance of a step and, in particular, of a kink for growth of a crystal layer. Obviously, an F face does not offer such sites, and growth requires the formation of stable 2D nuclei. By contrast, the atomically rough K face offers a large number of kink sites. Growth on such a face does not require the presence of 2D nuclei or structural defects. The growth rate is simply expected to increase with supersaturation, without any barrier to be surmounted. For a given supersaturation the growth rate of K faces will therefore be highest. The S face offers kink sites once an atom is attached. The density of kink sites is lower than on F faces, the growth rate will therefore be smaller. F faces will have the smallest growth rate due to the need of nucleation. According to our discussion of the facets of a growing crystal illustrated in Fig. 6.18 we note that K faces are expected to disappear first, followed by S faces, leaving eventually the F faces. A growing Kossel crystal will thus eventually be bounded by {100} faces. The model discussed so far may be extended by taking higherorder interactions into account. If we include also second and thirdnearest neighbor interactions, the detachment energy ϕ 21 from a kink position is given by the sum of the interaction energies E i and their respective coordination numbers Z i , ϕ 21 =
1 (Z 1 E 1 + Z 2 E 2 + Z 3 E 3 ). 2
(7.1)
The coordination number is the number of ith nearest neighbors. A bulk atom in a cubic Kossel crystal has Z 1 = 6 nearest neighbors along 100, Z 2 = 12 secondnearest neighbors along 110, and 8 thirdnearest neighbors along 111. At a kink site half of these neighbors exist, respectively. Our consideration of the halfcrystal site and (7.1) may be applied to extend relation (6.31) between the bond energy (including higher order bonds) and the enthalpy of evaporation, HS ∼ = ϕ 21 .
(7.2)
The considerations above basically also apply for other lattices. The numbers of neighboring atoms of ith order for an atom on a kink site of various lattices are listed in Table 7.1. The directions of the periodicbondchains in the cubic diamond structure differ from those in the simple cubic structure: They are oriented along the six 110 directions and are thus not parallel to the next neighbor bonds. The related zincblende lattice has six periodicbondchains along 110 for each of the two ion types. F faces
7.1 Surface Structure
255
Table 7.1 Numbers of nearest neighbors Z i for an atom on a kink site for some lattices Lattice Z1 Z2 Z3 Simple cubic Diamond Hexagonal closepacked
3 2 6
6 6 3
4 6 1
of the diamond and zincblende structures are {111} faces, while {100} faces and also {110} faces are stepped. K faces are, e.g., {311} faces. Also the diamond structure and the hexagonal closepacked (hcp) structure are related: Both are derived from stacking net planes along a [0001] stacking axis (cf. Sect. 2.1). F faces of the hcp ¯ faces which correspond to the {111} faces structure are hence the (0001) and (0001) of the diamond structure.
7.1.3 Relaxation and Reconstruction The atomic bonds in the uppermost layer of the surface of a solid differ significantly from those in the bulk due to the absence of neighboring atoms on one side. The altered equilibrium conditions for surface atoms lead to shifted atomic positions with respect to the bulk lattice. Two different effects in the rearrangement are to be distinguished: relaxation and reconstruction. Relaxation signifies a pure shift of atoms normal to the surface due to the missing attractive forces above the surface. Usually a compression occurs in the topmost few layers as illustrated in Fig. 7.3a. Relaxation leaves the lateral periodicity of the atom positions unchanged with respect to the bulk, i.e., the 2D surface unit cell corresponds to the unit cell of a truncated bulk crystal. Usually surface atoms tend to restore some of the bonds broken to create the surface. Such rearrangement is accompanied by lateral shifts of atoms, i.e., a shift
abulk
2abulk
(a)
(b) abulk
Fig. 7.3 a Relaxation and b reconstruction of atoms at the surface of a crystalline solid. Blue and red horizontal bars at the side of schematic (a) mark vertical positions of the atomic net planes corresponding to the bulk and the relaxed surface, respectively
256
7 Atomistic Aspects of Epitaxial LayerGrowth
parallel to the surface. This kind of reordering is termed reconstruction. The 2D surface unit cell of a reconstructed surface does not correspond to the lateral part of the bulk 3D unit cell. In most cases the dimension of the surface unit cell differs from the bulk unit cell as depicted in Fig. 7.3b. Reconstruction includes also surface unit cells of unchanged lateral dimensions with a modified lateral order compared to the bulk. The modified order of surfacenear atoms is related to a change of the surface energy. Surface energy may be regarded as the energy difference between an ideal surface without any relaxation and reconstruction, and the actual surface. Vice versa, it is the energy required to rearrange all surfacenear atoms of a relaxed and reconstructed surface to the order of the bulk lattice to form an ideal surface. The ordering of atoms near the surface depends on the kind of bonds and is different for crystalline semiconductors and metals. Semiconductors usually have strongly directed covalent bonds, particularly those with a tetrahedral coordination. Atoms at the surface tend to saturate at least some of the unsaturated bonds to minimize the density of unfavorable dangling bonds. Semiconductors show a large variety of often quite complex reconstructions, some are illustrated below in Sect. 7.1.6. Metals, by contrast, have a delocalized electron gas yielding basically no directed bonds. As a consequence many metal surfaces do not reconstruct. It must be noted that the type of reconstruction does not only depend on the considered solid and (hkl) surface plane, but also to a large extent on preparation conditions. A simple picture on the formation of a reconstructed surface is illustrated in Fig. 7.4. The figure assumes a tetrahedrally coordinated crystal bonded by sp3 hybrides. The ideal surface (Fig. 7.4a) may be considered to be created from a cut of the bulk crystal, leaving halffilled dangling bond orbitals at the surface. Each dangling bond is occupied by one electron. Such ideal surface is not stable, because a dangling bond represents an unfavorable energy state of the surface. The number of dangling bonds can be significantly reduced by the formation of surface dimers (Fig. 7.4b): Two unsaturated bond orbitals form one filled bridgebond orbital parallel to the surface, respectively. The surface energy may be further minimized by a charge redistribution among the remaining dangling bonds. The formation of a morethanhalf filled slike and a less filled plike dangling bond eventually leads to asymmetric dimers (Fig. 7.4c). The electroncharge transfer from the “down” atom to the “up” atom of the dimer changes the covalent bond of the symmetric dimer to a partially ionic bond [1]. Such a relaxation of the dimer bond is referred to as buckling. The vertical shifts of the atoms are accompanied by lateral displacements towards one another.
7.1.4 ElectronCounting Model For tetrahedrally coordinated compound semiconductors such as GaAs a simple electroncounting model has been developed to explain a wide variety of surface reconstructions [2]. This model accounts for the occupation of surface states and
7.1 Surface Structure
(a)
257
1e
(b)
1e
(c)
(1+ )e (1 )e

+
Fig. 7.4 Schematic on the gradual formation of a surface reconstruction from an ideal surface (a) via dimerization with symmetric dimers (b) to relaxed, buckled dimers (c)
assumes no net surface charge for reordered surfaces with minimum energy. Bonding and nonbonding surface states below the Fermi energy must be filled, while the antibonding and nonbonding states above the Fermi energy must be empty. For the given number of available electrons in the surface layer all dangling bonds on the electronegative element will then be full, and all those on the electropositive element of the compound semiconductor will be empty. This rule is generally applicable for any surface of a crystalline solid. Formation and occupation of bond orbitals at the surface is illustrated for GaAs in Fig. 7.5 [3]. In the bulk crystal, bonds oriented towards their nearest neighbors are constructed from sp3 hybrids with energies εh = (3εs + εp )/4 on each atom. The bond energy εb within each bond results from the linear combination of the two hybrids εh (Ga) and εh (As) with lowest energy. Eventually the occupied valence band with maximum E v is formed from linear combinations of these orbitals. Correspondingly, the empty conduction band with minimum E c is built from antibonding linear combinations. At the surface, some hybrid orbitals cannot form bonds, and partially filled dangling bonds remain. Details depend on the considered surface. On (111) surfaces the surface atoms are bonded to three atoms of the layer underneath, yielding three hybrid orbitals used for bonds and one dangling hybrid directed out of the solid. For the electropositive Ga atom the energy of this hybrid lies near the conductionband edge, leading to an empty state (Fig. 7.5). The hybrid of the elec¯ surface (also denoted (111)B surface) lies below tronegative As atoms on a (1¯ 1¯ 1) the valenceband edge and is consequently expected to be occupied. On the (001) surface two of the four sp3 hybrids are used to form bonds to the crystal underneath. Linear combinations of the two remaining danglingbond hybrids with lowest and highest energy yield a pure p state and an sp hybrid [3]. Both, Ga and As p states lie above the conduction band according to Fig. 7.5, leaving the p dangling bond unoccupied. The sphybrid of As lies below the valenceband edge. In a relaxed state this applies also for the sphybrid of the Ga [3]. Any structure obeying the electroncounting model exactly fills the electrons available in the surface layer into all danglingbond states in the valence band, leaving all danglingbond states in the conduction band empty. The surface will then be semiconducting, while partially filled dangling bonds may lead to a metallic surface. The electroncounting rule also assures that no charge accumulates at the surface. The model can successfully explain principal reconstructions on many surfaces. It can, however, not decide among alternatives which fit the model. Moreover, also
258 Fig. 7.5 Energy levels εh of sp3 hybride danglingbond orbitals of GaAs. The hybride energies are derived from the energies εs and εp of the atomic s and p orbitals of Ga and As, respectively. E c and E v denote conduction and valence bands of the GaAs bulk crystal. Data from [3]
7 Atomistic Aspects of Epitaxial LayerGrowth
Energy (eV) 0 5 10 15
a p(Ga) p(As) s(Ga)
h(Ga)
Ec Ev
h(As)
s(As)
b
20 Fig. 7.6 (2 × N ) surface unitcell with a missing dimer on a (001) face of a compound semiconductor with zincblende structure. Electronegative and electropositive elements are dark and bright, respectively. Bonds and dangling bonds are shaded if filled, empty bonds are open. After [2]
N
2
reconstructions may exist which are connected to a surface charge and do not obey the electroncounting rule. We illustrate the application of the electroncounting model for the (Asrich) GaAs(001) surface [2]. Since numerous structures comply with the model, we need some reasonable assumption on the nature of the reconstruction as a starting point, obtained, e.g., from scanning tunneling micrographs. Such images show a surface unit cell in one specific direction being twice as long as the lateral part of the bulk unit cell, originating from the formation of surface dimers as depicted in Fig. 7.4. In the other lateral direction the surface unitcell is a factor of N longer than that of the bulk (Fig. 7.9). This periodicity arises from periodically missing dimers. The reconstruction is termed (2 × N ) and leaves D dimers in one unit cell with D ≤ N , cf. Fig. 7.6. The relation between D and N follows from a balance between the number of electrons required to fill the bonds and that of available electrons. Each As dimer bond requires 2 electrons, and another 2 for the filled dangling bond at each of the two As atoms of the dimer, yielding a total of 6 electrons per dimer, or 6D electrons per unit cell. Furthermore, a total of 8D electrons per unit cell is required to bond all dimer As atoms to the Ga layer underneath. The dangling bonds on the electropositive
7.1 Surface Structure
259
Ga atoms in the second layer are empty. On the other hand, the number of available electrons results from the number of valence electrons Vn of the electronegative element and Vp of the electropositive element. The number of electrons in one unit cell available from the topmost three layers are therefore: 2Vn D 1 2Vp N 2
from the topmost layer comprising the As dimers, and from the second layer comprising Ga atoms, with the factor 21 because half of the total electrons are involved in bonding to the bulk crystal underneath.
To balance the numbers of required and available electrons in a (2 × N ) surfaceunit cell, we thus yield the condition 6D + 8D = 2Vn D + Vp N .
(7.3)
In the case of the studied GaAs surface Vn = 5 and Vp = 3 applies. Inserting these numbers we eventually obtain 4D = 3N (for GaAs). The smallest periodicity fulfilling this condition and D ≤ N is N = 4 and D = 3. This yields a (2 × 4) reconstruction of 3 dimers and one missing dimer in a unit cell (Fig. 7.6). If we consider a (Serich) (001) surface of zincblende ZnSe we have Vn = 6 and Vp = 2. The energies of the hybrid orbitals of the electropositive Zn and that of the electronegative Se lie in the conduction and valence bands of the solid, respectively, similar to the GaAs case [3]. The electron counting model (7.3) yields in this case N = D. We therefore expect a (2 × 1) reconstruction with no missing dimers as a favorable candidate. The Znrich ZnSe(001) surface actually forms a c(2 × 2) reconstruction. Such a reconstruction with Zn dimers is also consistent with the model, since a c(2 × 2) periodicity is formed from a complete layer of Zn dimers if each dimer row is displaced by one spacing in the 2× direction with respect to the previous dimer row [2]. The surface reconstruction of a semiconductor may significantly be modified in the presence of metal adsorbates. Metals then act as an electron reservoir which donates or accepts the right number of electrons, when the surface assumes a specific reconstruction to fulfill the electroncounting model. The model was therefore more recently extended to account also for metalinduced reconstructions [4]. A couple of prominent surface reconstructions assumed by GaAs and Si surfaces are discussed in Sect. 7.1.6. Prior to that we point out the notation used to designate surface unitcells of reconstructions.
7.1.5 Denotation of Surface Reconstructions The surface of a solid represents a threedimensional structure. The symmetry properties may be described by twodimensional operations, though. We therefore con
260
7 Atomistic Aspects of Epitaxial LayerGrowth
Table 7.2 The 4 crystal systems and the 5 Bravais lattices in twodimensional space. a and b are lattice vectors spanning the unit cell, α is the angle between the vectors System Unit cell Bravais lattices Symmetry axes Cubic
a = b, α = 90◦
Cubic
Rectangular
a = b, α = 90◦
Hexagonal
a = b, α = 120◦
Primitive rectangular, centered rectangular Hexagonal
Oblique
a = b, α = 90◦
Oblique
1 fourfold axes of rotation or inversion parallel to a×b 1 twofold axes of rotation or inversion parallel to a × b 1 sixfold axes of rotation or inversion parallel to a × b 1 axes of inversion parallel to a × b
(b) (1x1)
(a) (1x2)
as bs a c
b
c(2x2)
Fig. 7.7 a Unit cells of surface and bulk lattices, defined by their corresponding vectors. b Some unit cells of the surface lattice (black) on the bulk lattice (gray)
sider a twodimensional lattice, which constitutes a 2D translational periodicity, and a basis representing the atomic structure of the recurring surface unitcell. There are only 5 Bravais lattices in two dimensions, which constitute 4 crystal systems of differently shaped surfaceunit cells. Table 7.2 gives the symmetry properties of the 5 twodimensional Bravais lattices. The 2D lattice describing the surface periodicity is related to the 3D lattice of the bulk crystal underneath. The relation is illustrated in Fig. 7.7. The surface lattice vectors as , bs may be expressed in terms of the two vectors a, b which span the surface unit cell of a truncated bulk lattice,
7.1 Surface Structure
261
as bs
a a m 11 m 12 =M = . m 21 m 22 b b
(7.4)
The (2 × 2) matrix M provides an unambiguous relation between the surface and the bulk lattices. Usually the vectors as and bs are multiples of the vectors a, b (by convention as < bs if as = bs ). This leads to more convenient shorthand terms (Wood’s notation), which comprise these multipliers and, if necessary, an angle by which the surface lattice is rotated with respect to the bulk lattice [5]. Let us consider, e.g., the {hkl} surface of a solid X with a surface lattice, which fulfills as = 2a, bs = b. Such a structure may be formed by surface dimers as depicted in Fig. 7.4. The corresponding surface is then described by the shorthand term X {hkl} (2 × 1). Primitive and centered cells are indicated by adding p or c, respectively, and a rotated cell is denoted by adding R and the angle of rotation in units of degrees. Usually the p for a primitive cell is suppressed. The relation between the matrix representation and corresponding shorthand terms is given in Table 7.3. It should be noted that the simplified notation is not always unambiguous. √ A√centered cubic unit cell c(2 × 2) may as well be described by the unit cell ( 2 × 2 )R45◦ .
7.1.6 Reconstructions of the GaAs(001) Surface The electroncounting rule pointed out in Sect. 7.1.4 selects favored structures for a specific surface. The actual reconstruction is further determined by experiments and calculations. Different reconstructions with different surface stoichiometries become thermodynamically stable, when the chemical potential of the ambient is varied. Moreover, different reconstructions may coexist on a given surface due to varied surface preparations and kinetic barriers for a reordering of surface atoms. Table 7.3 Relation between matrix representation and corresponding shorthand terms for some surface lattices
M 10 01 10 02 20 02 1 1 −1 1
Shorthand term (1 × 1) (1 × 2) (2 × 2) c(2 × 2) or √ √ ( 2 × 2 )R45◦
262
TS (°C)
100
(4x1) (3x1) (1x1)
800 700 600
500
400
c(4x4)
(2x4)
(1x3)
(2x1) (2x3)
10
(4x2)
BEPAS4 / BEPGa
Fig. 7.8 Existence range of surface reconstructions forming during the MBE of GaAs for various temperatures TS and beam equivalent pressure (BEP) ratios of the As4 and Ga fluxes. Reproduced with c 1990 permission from [6], Elsevier
7 Atomistic Aspects of Epitaxial LayerGrowth
1
Ga droplets
0.9
1.0
(3x1) (3x6) (4x2) facetting (4x6)
1.1
1.2
1.3
1.4
1.5
(4x1) 1.6
1
3
10 / T (K ) S
As an example we consider the technologically important (001) surface of GaAs, already treated above for illustrating the electroncounting rule. Experimentally, many surface reconstructions were found depending on ambient conditions. Figure 7.8 shows experimental results for a growing GaAs(001) surface composed ¯ As plane as a phase diagram [6]. Here, a vicinal surface tilted by 2◦ toward the (111) was used to facilitate growth. This tilt leads to Asterminated steps. The structure was analyzed by reflection highenergy electron diffraction (RHEED) during molecularbeam epitaxy at a fixed Ga flux corresponding to a growth rate of 0.7 monolayer/sec GaAs. In the experiment the chemical potential was varied by the supplied flux of As4 molecules, expressed in the diagram in terms of the beam equivalent pressure (BEP) ratio with respect to that of the Ga flux. In addition the temperature was varied as an independent basic growth parameter. We note that the conditions do not correspond to equilibrium. The diagram Fig. 7.8 shows 14 different reconstructions which may be distinguished as Asrich surfaces ((2 × 4) or (2 × 1)), as a transition range ((3 × 1) or (1 × 1)), as Garich surfaces ((4 × 1), (4 × 2), (4 × 6), or (3 × 6)), as absorption structures of the type c(4 × 4), (2 × 3), (1 × 3), and surfaces where degradation occurs [6]. The transitions between all regions were found to be reversible and could be described by an Arrhenius law. Within a transition range often a coexistence of adjoining patterns was observed.
7.1 Surface Structure
2(2x4)
c(4x4)
[110]
Fig. 7.9 Filledstate STM image of a the β2(2 × 4) and b the c(4 × 4)β reconstructions of the GaAs(001) surface. In a two AsAs top dimers and an AsAs trench dimer are marked. In b three AsAs top dimers and the c(4 × 4) lattice mesh are marked. Reproduced with permission c 1999 from [7] and [8], and 2004 APS, respectively
263
[110] The periodicity of the surface unit cell is usually readily accessible in MBE from electron diffraction experiments. The arrangement of atoms within the unit cell often poses, however, a tricky problem. A variety of methods such as scanning tunneling microscopy, lowenergy electron diffraction, and angleresolved photoelectron spectroscopy has to be applied to obtain an unequivocal structural model. Two prominent reconstructions of the GaAs(001) surface imaged using highresolution STM are shown in Fig. 7.9. Though many details can be identified on such images, the arrangement of the atoms at the surface may hardly be extracted. Calculations of surface energies for various orientations and reconstructions help substantially to find and to understand the actual atomic structure of the surface unit cell. The stable equilibrium surfacereconstruction is that with the lowest surface free energy γ A. The surface of a compound semiconductor like GaAs may be nonstoichiometric with respect to the number of atoms of different species, and the surface free energy depends on the chemical potential μi for each species i. The surface may exchange atoms with the ambient which acts as a reservoir, and μi is the free energy per particle of species i in the reservoir. In the experiment μi can be varied within the limits given by the bulk chemical potentials of the condensed phases of the species, μi < μi(bulk) , because otherwise the elemental phase of species i will form on the surface. In the case of GaAs this will be bulk As and bulk Ga. Furthermore, in equilibrium the sum of the chemical potentials of the species Ga and As must be equal the bulk energy per GaAs pair [9], μGa + μAs = μGaAs(bulk) = μGa(bulk) + μAs(bulk) + HfGaAs , HfGaAs being the heat of formation of the GaAs bulk crystal. Using this relation the surface energy may be expressed as a function of the As chemical potential μAs . If μAs is varied, different surface stoichiometries and related reconstructions get most stable. A large variety of atomic configurations exists for surface unit cells of each of the reconstruction periodicities shown in Fig. 7.8. Surface structures with low
264
7 Atomistic Aspects of Epitaxial LayerGrowth
1.6
1.4
1.2
γ (J/m2)
Fig. 7.10 Surface energy of different lowenergy GaAs(001) reconstructions, depending on the chemical potential of the arsenic. Dashed lines mark limits of the chemical potential difference μAs − μAs(bulk) . Data from [9]
2(4x2)
(2x4)
1.0 2(2x4) 0.8
0.6
c(4x4)
0.6
0.4
0.2
0.0
µAs  µAs(bulk) (eV)
surface energies within some range of μAs are given in Fig. 7.10. These structures all fulfill the electron counting rule (Sect. 7.1.4) and are semiconducting (filled anion and empty cation dangling bonds). The surface energies shown in Fig. 7.10 are calculated from the total energy E tot according to [9] γ A = E tot − μGaAs NGa − μAs (NAs − NGa ). The stoichiometry of the surface NAs − NGa determines the slope in a linear dependence on the chemical potential μAs . The reconstructions noted in Fig. 7.10 are those with a low surface energy within the indicated allowed limits of μAs . Particular phases of GaAs(001) reconstructions with given periodicity of the unit cell are indicated using a leading label like, e.g., α or β2 [10, 11]. Starting from the Garich β2(4 × 2) reconstruction we note a progressive trend to a negative slope in the sequence towards the most Asrich c(4 × 4) surface for high μAs − μAs(bulk) values. The α(2 × 4) surface is stoichiometric, i.e., NAs = NGa , and does not depend on the chemical potential of As. The lowenergy Asrich β2(2 × 4) and c(4 × 4) surfaces are those generally used in the molecularbeam epitaxy and the metalorganic vaporphase epitaxy of (001)oriented GaAs, respectively. The atomic structure of the four most favorable reconstructions indicated above are shown in Fig. 7.11. Both, GaGa and AsAs dimer bonds occur in the topmost layer of the displayed unit cells. They both have filled bonding and empty antibonding states. The Garich β2(4 × 2) structure consists of two GaGa dimers per unit cell oriented along [110] in the top layer and two missing As atoms in the second layer.
7.1 Surface Structure
265
(b)
[110]
[110]
(a)
[110]
2(4x2)
(2x4)
[110]
c(4x4)
[110]
2(2x4)
[110]
(d)
[110]
(c)
[110]
Fig. 7.11 Models of the four GaAs(001) surface reconstructions considered in Fig. 7.10. The size of the atoms indicates the vertical position, bright and dark atoms represent As and Ga, respectively. Shaded areas indicate the surface unitcells
An electron counting within the unit cell [12] yields a surface stoichiometry of NAs − NGa = − 41 per (1 × 1) unit cell. The stoichiometric α(2 × 4) surface consists of two AsAs toplayer dimers ori¯ ented along [110], adsorbed on a complete Ga monolayer underneath. Two AsAs dimers are missing in the row of toplayer dimers, and two GaGa bonds are formed within the Ga monolayer where one AsAs dimer is missing. It should be noted that another stoichiometric structure with a single AsAs toplayer dimer termed α2(2 × 4) was found with an even lower energy than that depicted here [11, 13, 14]. The more Asrich β2(2 × 4) structure is obtained from the α(2 × 4) structure by removing two Ga atoms in the missing AsAs dimer region, resulting in a stoichiometry of NAs − NGa = 41 per (1 × 1) unit cell. The structure represents the counterpart of β2(4 × 2), with Ga atoms exchanged for As atoms and vice versa. The most Asrich c(4 × 4)β surface represents a doublelayer structure consisting of AsAs dimers oriented along the [110] direction and adsorbed on a full As monolayer, yielding a stoichiometry of NAs − NGa = 45 per (1 × 1) unit cell. The ¯ commonly accepted model comprises a block of three dimers in a row along [110], being interrupted by a dimer vacancy. AsGa heterodimers are assumed to appear in the c(4 × 4) reconstruction as the chemical potential μAs − μAs(bulk) is lowered towards less Asrich conditions and the β2(4 × 2) structure is approached [15]. The c(4 × 4) reconstruction with three AsGa toplayer dimers is referred to as c(4 × 4)α. The reconstructions of the GaAs(001) surface considered above as some typical examples give an impression about the wealth of surface structures. More detailed information on surface reconstructions is found in, e.g., [16, 17].
266
7 Atomistic Aspects of Epitaxial LayerGrowth
7.1.7 The Silicon (111)(7 × 7) Reconstruction Silicon is the most important semiconductor for device technology. Chips for integrated circuits are fabricated from (001)oriented Si wafers. Atoms in the uppermost layer of the unreconstructed {100} surface of the diamond structure have two dangling bonds each. The surface energy is lowered by formation of asymmetric buckled dimers as illustrated in Fig. 7.4c, leading to a Si(001)(2 × 1) reconstruction. Usually Si(001) wafers are chemically treated using a dilute HFetch to remove surface defects. During such a procedure dangling bonds are saturated by hydrogen. The Hterminated surface relaxes but does not reconstruct. Some applications such as electric highpower applications employ the (111) surface of silicon. (111) is the primary cleavage plane of Si. When Si is cleaved ¯ direction, a in vacuum along this plane with a wedge kept parallel to the 112 Si(111)(2 × 1) reconstruction is created. This reconstruction differs from that of the (100) surface by forming long pibonded chains in the first and second surface layers. Annealing above 300 ◦ C converts the structure irreversibly into a (7 × 7) reconstruction, which represents an equilibrium phase. Much effort was spent over more than two decades to unravel the complex structure of this surface. The Si(111)(7 × 7) surface unitcell is 49 times larger than the unit cell of the ideal surface. An unreconstructed cell of this size would have 98 dangling bonds. The formation of the actual (7 × 7) structure comprises an extensive rearrangement of atoms and the addition of adatoms on top. Scanning tunneling micrographs show a pattern of 12 protruding adatoms in a unit cell and vacancies at the deep corner holes, see Fig. 7.12. Each adatom saturates three dangling bonds from the layer underneath and leaves one dangling bond. STM images recorded with a suitable bias show that the rhombic unit cell is composed of two triangular subunits.
1.0V
+1.0V
U F
5 nm Fig. 7.12 Scanning tunneling images of the Si(111)(7 × 7) surface for negative (left, filled states) and positive (right, empty states) sample bias. The orange rhombs mark a unit cell comprising 12 protruding adatoms, U and F denote unfaulted and faulted halfunit cell, respectively. Courtesy of M. Dähne, TU Berlin
7.1 Surface Structure
267
Fig. 7.13 Structure of the Si(111)(7 × 7) surface unitcell according to the dimeradatomstacking fault model. Atoms in layers of decreasing height are represented by decreasing size, dark atoms represent unreconstructed atoms of the uppermost bulk layer underneath the surface layers
The structure of the Si(111)(7 × 7) surface was eventually explained by the generally accepted DAS model derived from a detailed analysis of transmission electron diffraction [18]. The name DAS refers to the basic structural elements: 15 dimers (D), 12 adatoms (A), 1 stacking fault (S). The model has also been confirmed by computation, yielding an energy gain of 60 meV per (1 × 1) unit cell with respect to the (2 × 1) reconstruction [19]. A top view of the unit cell according to the DAS model is given in Fig. 7.13. The uppermost atoms are indicated by largest size, and we recognize the 12 adatoms visible in the STM image Fig. 7.12. We also note the corner holes in the top layer. The model shows an apparent difference in the left and right triangles of the unit cell. In the right half we see the uppermost atoms of the bulk crystal underneath the surface layers drawn with a dark shading. This yields an ABC stacking order with respect to the first two surface layers, thereby continuing the cubic diamond structure of bulk Si. The uppermost bulk atoms are not visible in the left triangle, because they are hidden by the surface layers due to an AB AB stacking order. The left part of the unit cell has consequently a hexagonal order, i.e., the sequence is faulted with respect to the structure of bulk Si. The faulted and nonfaulted triangular subunits are each surrounded by 3 vacancies at the corners and 9 dimers, three of them located at the separating domain boundary, which is oriented along the vertical short diagonal in Fig. 7.13. The DAS model leaves only 19 unsaturated dangling bonds per unit cell: 12 for the adatoms, 6 from threefold coordinated rest atoms lying in the layer below the adatoms, and 1 from the atom below the vacancy at the corner. A number of similar DAS reconstructions in a (2n + 1) × (2n + 1) pattern have also been observed in nonequilibrium conditions, including 5 × 5 and 9 × 9 reconstructions [20]. The
268
7 Atomistic Aspects of Epitaxial LayerGrowth
preference for the (7 × 7) reconstruction is attributed to an optimal balance of charge transfer and stress.
7.2 Kinetic Process Steps in Layer Growth The nonequilibrium process of growth is governed by a competition between kinetics and thermodynamics. As the size of heterostructures approaches the nanometerscale regime, atomiclevel control is becoming crucial. Kinetic growth processes may to a large extend be described by the terracestepkink model already used in Sect. 6.2.4 to characterize surface energies. We will first employ this simplified model to consider growth kinetics, and include the effect of the actually more complex surface structure as described above in a second step.
7.2.1 Kinetics in the TerraceStepKink Model The terracestepkink (TSK) model of a surface [21] (also termed terraceledgekink (TLK) model) is based on the idea that the energy of an atom’s position on a crystal surface is determined by its bonding to neighboring atoms. Processes on an atomistic scale hence involve the counting of broken and formed bonds. In the framework of the TSK model the kinetics of growth is described by rates of transition steps, which atoms undergo on the surface. The complex process of epitaxy is largely determined by only a few categories of such processes. Some processes of particular importance are illustrated for the surface of a Kossel crystal in Fig. 7.14. Growth proceeds by a number of consecutive steps as indicated in Fig. 7.14. Atoms arrive from the ambient and are adsorbed on the surface. They may then diffuse over the surface until they cease to diffuse by one of several processes. Such processes are reevaporation (or resolution in case of a liquid ambient), nucleation of (2D or 3D) islands, attachment to existing islands or to defects like a step on the surface. In the framework of the considered model the adatom diffusion on the surface is described by rates of hopping from one site to an adjacent site. The vibrational
Fig. 7.14 Schematic of atomistic rate processes in epitaxial growth. The stepdown diffusion differs from the indicated lateral diffusion
adsorption nucleation incorporation diffusion
diffusion
7.2 Kinetic Process Steps in Layer Growth
269
motion of an adatom on the surface is regarded as an attempt at such a hop. Since many attempts are required to produce a single hop, a factor is introduced representing the probability per attempt to hop, yielding an effective hopping rate k(T ). The rate may also be expressed in terms of a mean residence time τ (T ) = k −1 (T ). Each thermally activated kinetic process of epitaxy is governed by characteristic parameters entering an Arrhenius dependence with an activation energy E,
τ −1 (T ) = ν0 e
− k ET B
.
(7.5)
E is the barrier which has to be surmounted in the process. The prefactor ν0 represents an attemptrate constant for the given process. Rate equations referring to a few basic processes are used in numeric Monte Carlo simulations to model the dynamics of growth and the evolution of the growth surface. Only the ratelimiting steps are included in the calculations. Faster processes are accounted for in average by using effective kinetic parameters. Parameters to control the supersaturation μ are usually the experimental variables T , the arrival rate of atoms R, and the material parameters of the kinetic processes describing diffusion, reevaporation, and nucleation. The approach does not require a detailed knowledge of the atomic interactions and permits simulations including large time scales. Values for ν0 and E (on the order of 1012 s−1 and 1 eV, respectively) for each process are estimated from, e.g., molecular dynamics, or they are taken as parameters to fit experimental results.
7.2.2 Atomistic Processes in Nucleation and Growth The atomistic processes indicated in Fig. 7.14 are now described in more detail to account for nucleation and growth analogous to the thermodynamic approach discussed in Sect. 6.2. In our simplified approach [22] we neglect surface reconstructions, interdiffusion, and chemical reactions between substrate and deposit material. The assumed processes are indicated in Fig. 7.15. Atoms arriving from the ambient on the surface at an externally controlled flux F (atoms per unit area and per unit time) diffuse on the surface. They either meet other atoms to nucleate, or they are captured at a growing island (also denoted cluster) after a mean time τc , or they reevaporate after a mean adsorption residence time τa . A nucleus will either loose adatoms after a mean time τn , or grows to a critical size comprising i atoms. The critical nucleus also may dissolve or grow to a stable island comprising x > i atoms. Such islands will capture further adatoms but—under growth conditions—hardly loose atoms. We trace an atom which arrives at the surface. At a high temperature the adatom will only stay on the surface for a short residence time τa . This time is determined by the adsorption energy E a and may be written
270
7 Atomistic Aspects of Epitaxial LayerGrowth
F
Fig. 7.15 Processes considered for the kinetic description of growth
arrival
evaporation a
n1 capture c
nucleation
nx
n
ni
growth (dissolution)
critical nucleus τa−1 = νa0 exp −E a /(kB T ) ;
(7.6)
the prefactor νa0 corresponds to an atomic surface vibrationfrequency and represents an attempt rate for desorption. For some materials relation (7.6) is complemented by a factor, which accounts for a dependence of the residence time on the material coverage on the substrate. During τa the adatom migrates in a randomwalk process consisting of a series of jumps to respective adjacent substrate sites. The meansquare displacement of the adatom during a period of duration t depends on the hopping rate (or, mean hopping frequency) νd and is given by 2 λ = νd a 2 t,
(7.7)
a being the mean jump distance. Usually a is the distance of two neighboring lattice sites on the surface. The number of hops during the considered period is νd t. Hopping to a neighboring site requires surmounting a potential barrier, cf. Fig. 7.23. This diffusion barrier E d is surmounted more easily at increased temperature due to an Arrhenius dependence of the hopping rate, νd = νd0 exp −E d /(kB T ) ;
(7.8)
The prefactor νd0 is an attempt rate for a diffusion hop. The ratio of the meansquare displacement (7.7) with respect to the duration of the period is the timeindependent diffusion coefficient (or diffusivity) D, D=
νd a 2 λ2 = , ηt η
(7.9)
7.2 Kinetic Process Steps in Layer Growth
271
where η is the number of neighboring sites reachable by a single jump: For onedimensional diffusion η = 2, while for 2D surface diffusion η = 4 on a square lattice and 6 on a hexagonal lattice. Using Einstein’s relation of the diffusion length, λ = √ Dτ , and (7.9), the displacement (rootmeansquare value) from the arrival site to the site of eventual evaporation or incorporation reads
λ=
√
Dτ = λ0 exp (E a − E d )/(2kB T ) ,
(7.10)
Fig. 7.16 Temperature dependence of the surface diffusion length λ
ln λ
τ being the mean time of surface diffusion (basically τa at high T , τc at lower T ). The preexponential factor√ λ0 is a merged effective elementary jump distance, e.g., for √ τ = τa given by λ0 = νd0 /νa0 × a/ η. Values of νd0 are typically somewhat less than those of the corresponding parameter for adsorption νa0 , but of the same order. The barrier to be surmounted for desorption, E a , is however usually much larger than the diffusion barrier E d , and also several times exceeding thermal energies kB T at typical growth temperatures. The adatom will therefore migrate over a quite long distance λ a before evaporation. For small values of 1/T (in the high temperature range) the surface diffusion length λ increases exponentially with 1/T (or, decreases with T ) as indicated by (7.10) and the straight line in the Arrhenius plot Fig. 7.16. The residence time in this desorption regime is short, and adatoms are likely to evaporate before being incorporated. At large values 1/T (low T ) the slope in the Arrhenius dependence of λ(T ) changes sign. The residence time is large according to (7.6); at low T adatoms are incorporated after diffusion and the competition by desorption gets negligible. Best epitaxial growth is often achieved for large diffusion length. This is obtained just below the onset of significant reevaporation. During surface diffusion the adatom encounters other atoms on the surface. The probability of such a meeting depends on the areal density n 1 of single migrating atoms, and the areal density of clusters containing more than one atom. In our approach we assume the clusters to be stationary, i.e., single adatoms are the only species which are mobile. The clusters on the surface are divided according to their size into subcritical clusters with atom numbers j ≤ i, and stable clusters, j > i, the density of which is summed as
 Ed 2k BT
Ea  Ed 2kBT
1/T
272
7 Atomistic Aspects of Epitaxial LayerGrowth
nx =
∞
nj .
j=i+1
After an initial nucleation of stable clusters the subcritical clusters nucleate and dissolve in an approximate detailed balance. They are therefore not considered further in the evolution due to the local equilibrium condition dn j /dt = 0 for 2 ≤ j ≤ i. In the following we focus on the density of single atoms n 1 and that of stable clusters n x . The density n 1 of the mobile single atoms follows from a balance of processes described by an appropriate rate equation. As we read from Fig. 7.15, atoms arriving on the surface at a rate F increase n 1 , while nucleation (τn ), capture (τc ), and evaporation (τa ) decrease n 1 . Furthermore, when larger stable islands cover a significant fraction Z of the surface, arrival on top of an island is possible, thereby decreasing the part of atoms on the uncovered surface. The evolution of the singleatom density n 1 is therefore described by dn 1 /dt = +F(1 − Z ) − n 1 /τn − n 1 /τc − n 1 /τa = F(1 − Z ) − n 1 /τ,
(7.11)
with τ −1 = τn−1 + τc−1 + τa−1 . The sum may be extended when additional loss processes for diffusing adatoms are to be taken into account. On the other hand, also less processes may be considered. In the limit of high temperature the residence time τa gets very short, and nucleation and capture processes become negligible. Since also Z ∼ = 0 in this case, we obtain dn 1 /dt = F − n 1 /τa . This yields for long times t τa a stationary state (dn 1 /dt = 0) with the solution n 1 = Fτa . The constant density in the high temperature limit reflects the balance of arrival and evaporation without nucleation or growth. Below the high temperature limit loss of adatoms by attachment to growing stable islands is relevant. Once stable islands exist, the term −n 1 /τc in (7.11) is generally much larger than the term −n 1 /τn . Neglecting the nucleation term −n 1 /τn for t τa the solution gets n 1 = F(1 − Z )(1/τa − 1/τc )−1 . The mean time τc of the adatom capture at a stable island depends on their density n x and the diffusional flow, τc−1 = σx Dn x . (7.12) The capture numbers σk of the stable clusters summed to a mean number σx express the local decrease of n 1 (r, t) near a ksized cluster due to capture [23]. They are typically of order 5–10 and may regarded for a first appreciation as slowly varying quantities. The density n x of stable clusters increases by a nucleation rate J involving capture at critical clusters with i atoms. The creation of new stable clusters is proportional to the density n i of the critical clusters with their capture number σi , and the density
7.2 Kinetic Process Steps in Layer Growth
273
of single adatoms n 1 and their diffusivity D, yielding J = σi Dn 1 n i . On the other hand, as growth of a layer proceeds the density will reduce due to an impingement of stable clusters on each other. Such coalescence is accounted for by including a negative term proportional to the temporal change of coverage Z , leading to the rate equation [22] (7.13) dn x /dt = +σi Dn 1 n i − 2n x d Z /dt. To solve the coupled equations (7.11) and (7.13) a relation between Z and n x is needed. If the clusters grow twodimensionally, we may put [22] d Z /dt = Ω 2/3 (i + 1)n 1 /τi + n 1 /τc + F Z ,
(7.14)
where Ω is the atomic volume of the deposit and the stablecluster nucleation rate τi−1 = σi Dn i . The solution of the rate equations leads to the cluster densities schematically shown in Fig. 7.17. Growth on a flat surface starts at coverage Z = 0. At a high temperature T1 we note an initial rise of the singleatom density n 1 ∼ Ft lasting for t < τa , followed by a constant value described by the hightemperature limit. The density of stable clusters n x starts at a negligible value at t = τa , and increases for t > τa as given by the first term in (7.13), i.e., before coalescence. Both, n 1 and n x decrease as coalescence sets in. The condensation coefficient α(t), which denotes the fraction of atomic dose impinging on the surface and being incorporated into the deposit, is initially very small at this high temperature, and so also the total deposit Ftα. At a low temperature T2 no reevaporation occurs, i.e., α = 1. In this temperature range the singleatom density n 1 plotted in Fig. 7.17 increases linearly until capture
T1
nx n1
lo g ( n )
Fig. 7.17 Density of single atoms n 1 , stable clusters n x , and the total number Ftα of atoms condensed on the surface as a function of time t for a high temperature T1 and a low temperature T2 . τa and τc indicate reevaporation and capture times, respectively, the label coal. marks a decrease of n 1 and n x due to coalescence. After [22]
coal.
Ftα T2
τa n1
Ftα
nx τc
log (t)
coal.
274
7 Atomistic Aspects of Epitaxial LayerGrowth
Table 7.4 Parameters p and E of (7.15) for the maximum density n x of stable twodimensional clusters in various regimes of condensation. i is the number of atoms in the critical cluster. From [22] Condensation regime p E Extremely incomplete Initially incomplete Complete
i i/2 i/(i + 2)
E i + (i + 1)E a − E d 1 2 (E i + i E a ) (E i + i E d )/(i + 2)
by previously nucleated clusters sets in, causing n 1 to pass a maximum at the mean capture time τc and to decrease subsequently. The stablecluster density n x increases after a nucleation period and eventually decreases due to coalescence. The maximum density of stable clusters has the general form n x ∼ (F/ν) p exp −E/(kB T ) ,
(7.15)
where the materials parameters p and E lead to different regimes of condensation [22]. Values for the regimes of extremely incomplete condensation, initially incomplete in an intermediate range, and complete condensation are given in Table 7.4. The three regimes refer to the conditions σx Dτa n x Z , Z < σx Dτa n x < 1, and σx Dτa n x 1, respectively, and define the meaning of a high and a low temperature for growth of the considered material. We note from Table 7.4 that the condensation regimes are essentially determined by the relation between the materials parameters E i , which signifies the energy difference between i atoms in the adsorbed state and in stable clusters, the adsorption energy E a , and the critical cluster size i. At extremely incomplete condensation growth is slow due to strong reevaporation and proceeds essentially by direct impingement. In the intermediate, initially incomplete regime stable clusters grow by diffusive capture in the initial state. Direct impingement becomes relevant at large coverage Z , leading to more complete condensation. This regime will often occur in practice. At complete condensation growth is fast, since reevaporation is negligible.
7.2.3 Adatoms on a Terraced Surface Growth of a flat surface proceeds basically by the attachment of adatoms at steps. The steps may originate either from 2D nucleation as discussed above, or from screw dislocations, or from the terrace structure of a vicinal surface inclined with respect to a singular face by a small tilt angle. The rate of layer growth r , which represents the velocity of a parallel displacement of the singular faces, is hence determined by the advancement of steps. To obtain an expression for the velocity of step advance we consider growth conditions with an only minor contribution of nucleation. Such conditions may be found
7.2 Kinetic Process Steps in Layer Growth
275
in stepflow growth of a vicinal surface (Sects. 6.2.7, 7.2.4). This surface consists of terraces of width l which are separated by steps of height a (Fig. 6.14). Let us assume for simplicity that the steps are equidistant and straight. If the steps remain straight all the time, we obtain a onedimensional problem. The steps are assumed perfect sinks for diffusing adatoms arriving from either side and have monoatomic height. Furthermore, the terrace width l is assumed smaller than the mean displacement λ of an adatom after arrival on the surface. If now a constant flux F deposits a low density of adatoms n on the surface (in the previous Sect. 7.2.2 labeled n 1 ), the adatoms will diffuse with some finite probability to an adjacent step where they are incorporated, and we may neglect nucleation on the terrace. For the given conditions the concentration of adatoms on the surface n(x, t) is described by n(x, ˙ t) = Dn
(x, t) −
1 n(x, t) + F, τa
(7.16)
where x is the lateral direction perpendicular to the steps, dot and double primes designate temporal derivative ∂/∂t, and spatial derivative ∂ 2 /∂ x 2 , respectively, D is the surface diffusion coefficient (7.9), and 1/τa denotes the evaporation probability (7.6). The change of the adatom density n expressed by (7.16) is composed of the three terms surface diffusion, loss by evaporation, and deposition by the external flux F. To solve (7.16) we need boundary conditions, which are to be fulfilled by n(x, t). We consider steadystate conditions, where F is constant and n does not change in time, i.e., n(x, ˙ t) = 0. Steps are considered as perfect sinks. A fast incorporation of adatom at steps is fulfilled by the condition that n equals a constant concentration n eq at a step to be reached at thermal equilibrium. Choosing the origin of x at the center of a terrace, the condition reads n(±l/2) = n eq .
(7.17)
The steadystate solution of (7.16) is then given by
n(x) =
cosh(κ x) (n eq − Fτa ) + Fτa . cosh(κl/2)
(7.18)
√ In (7.18) κ is the inverse of the mean displacement, κ = 1/λ = 1/ Dτa . If the residence time τa is long, reevaporation described by the second term in (7.16) becomes negligible. κ is then small. If also κl/2 is small, solution (7.18) can be approximated by a Taylor expansion, yielding n(x) ∼ = n eq + Fτa κ 2 /8 l 2 − 4x 2 = n eq + (F/8D) l 2 − 4x 2 (κl/2 small). (7.19)
276
7 Atomistic Aspects of Epitaxial LayerGrowth
n neq+
Fig. 7.18 Density profile n(x) of adatoms on a terraced surface under steadystate conditions provided by a constant flux F and steps acting as sinks (black curve). Gray curve: n(x) resulting from an uneven capture probability of upsteps and downsteps
neqneq l/2
F
0
+l/2
x
The steadystate solution (7.19) for negligible reevaporation is shown in Fig. 7.18 (black curve). It is a parabola with a maximum centered in the middle of a terrace at x = 0 with values n(±l/2) = n eq . The assumptions made to obtain the simple geometry expressed by (7.16) and the approximate solution (7.19) are quite extensive and may in practice often not be fulfilled. The requirement of a perfect sink may, e.g., be fulfilled by the left step in Fig. 7.18 but less well by the right step, because the latter requires a less probable downstep diffusion for incorporation. An unequal capture probability can be expressed by two equilibrium adatomconcentrations at the steps n eq+ and n eq− , leading to a similar solution as (7.19) with a parabola maximum being displaced from x = 0 by xmax = D/(Fl)(n eq+ − n eq− ). The respective profile n(x) is drawn in Fig. 7.18 in gray; values for n eq+ and n eq− are assumed larger than n eq . The mean adatom density n in steadystate conditions is obtained from (7.19) by integration over n(x), yielding 1 n= l
+l/2
−l/2
n(x) d x = n eq + Fl 2 /(12D).
(7.20)
In case of unequal capture probability at the steps n eq = (n eq+ + n eq− )/2 in the righthand side of (7.20).
7.2.4 Growth by Step Advance We may treat the capture of adatoms at steps similar to the capture at stable clusters of density n x . If we assume the steps acting as strong sinks, i.e., n eq = 0, such a treatment is accomplished by adding a term −n 1 /τs to the right side of (7.11). τs is the mean time of adatom capture at a step. The mean singleadatom density n 1 given by (7.20) then corresponds to Fτs . Capture at steps now compete with capture at stable clusters and nucleation. Capture at a cluster occurs for an adatom arrival within a rootmeansquare distance λc = (Dτc )1/2 . Near a step (ideal sink) nucleation is depressed. This zone on either side of a step is called denuded zone. Its width is
7.2 Kinetic Process Steps in Layer Growth
277
given by λc . This consideration allows to express a condition for the transition from nucleation and 2D island growth at lower temperatures to step flow growth at higher temperatures. For dominating capture at clusters, n 1 is expressed by Fτc with τc given by (7.12). Step flow becomes more dominant than nucleation on a terrace if τs < τc . Inserting n 1 from (7.20) and (7.12), respectively, we see that this condition is met if (7.21) l 2 /(12D) < (σx Dn x )−1 . This inequality may be expressed in terms of the denudedzone width λc with τc from (7.12), yielding l2 1 l 2 σx n x = 2 < 1. (7.22) 12 1 λc 12 According to (7.22) the transition from nucleation to step flow occurs if the width of the denuded zone λc (which increases as the temperature increases) becomes larger than a fraction of about one third of the terrace length l. The surface morphology of homoepitaxial GaAs layers grown at different temperatures is shown in Fig. 7.19. The sample grown in stepflow mode at a high temperature exhibits terraces with steps of atomic height, originating from an offorientation of the substrate with respect to the [001] growth direction. The morphology of the sample grown at decreased temperature shown in Fig. 7.19b exhibits 2D island growth on terraces. The terrace edges are irregular, the large terrace width indicates a small offorientation of the substrate. Note that no islands nucleate close to a step. The transition between island growth to stepflow growth can be studied experimentally using diffraction techniques, see Sect. 8.3. For GaAs(001) surfaces the diffusion length of Ga adatoms in MBE growth was determined from the transition temperature obtained from the onset of RHEED intensity oscillations; the transition was in fact found to depend on the surfacediffusion length with respect to the terrace width [24]. This was also observed for AlN(0001) [25]. A simulation of the molecularbeam epitaxy of GaAs on GaAs(001) in the stepflow growth mode for appropriate growth conditions is given in Fig. 7.20. The growing (001) surface of the GaAs zincblende structure is polar: surfaces with terminations of Ga cations and As anions alternate periodically. For a slow As2 incorporation rate assumed in the simulation, the As coverage (even numbered gray curves) lags behind
Fig. 7.19 Atomicforce micrographs of 0.5 µm thick homoepitaxial GaAs layers grown at a 570 ◦ C, and b 530 ◦ C
278
7 Atomistic Aspects of Epitaxial LayerGrowth
the directly preceding Ga layer coverage (odd numbered black curves) until the near completion of a layer [26]. We note that the Sshaped curves of subsequent (bi)layers overlap: Nucleation of the next layer starts before the layer underneath is completed. Of the first monolayer’s worth of Ga material delivered (at τML ∼ = 0.9/sec) about 95 % goes into the first Ga layer and 5 % into the next for the considered growth conditions. At fast As2 incorporation, coverages of As layers lead the coverage of the preceeding Ga layers [26]; for a comprehensive treatment see [27]. The advancement of a step results from the capture of adatoms from the upper and lower terrace. Let us consider the velocity of lateral advance rstep of the step at the position x = −l/2. We again assume steadystate conditions, i.e., adatoms diffuse much faster than steps move. Furthermore, we again consider terraces of equal width and an equal probability for capture from either terrace. The current density j of adatoms arriving at the step follows from the gradient of the adatom density n(x) at the step position x = −l/2, j (−l/2) = −D
d n(−l/2). dx
(7.23)
Inserting the symmetric adatom density n(x) from (7.18) we obtain j (−l/2) = Dκ(Fτa − n eq ) tanh(−κl/2).
(7.24)
The step velocity rstep results from the (equal) contributions from the upper and the lower terrace separated by the step, rstep = a 2 jupper (−l/2) + jlower (−l/2) = 2a 2 j (−l/2),
1.0 0.8
Coverage
Fig. 7.20 Simulated coverage in the molecularbeam epitaxy of GaAs/GaAs(001) for slow As2 incorporation. Odd and even numbered curves refer to Ga and As layers, respectively. Reproduced with permission from [26], c 1986 APS
(7.25)
1 2
0.6
3 4
5 6
7 8
0.4
9
10
0.2 0.0
0
1
2
3
Growth time (units of
4
) ML
5
7.2 Kinetic Process Steps in Layer Growth
279
a 2 being a unit area of the terrace. The velocity rstep depends on the terrace width, because larger terraces collect more adatoms from the ambient, cf. Fig. 7.21. For small κl/2 (long residence time τa ) (7.24) simplifies to j (−l/2) = D(Fτa − n eq )κ 2 l/2.
(7.26)
The linear relation j ∝ l is reflected in the constant slope of rstep for small terrace width l in Fig. 7.21. We now consider the growth rate r of a flat crystal surface. Growth proceeds essentially by the attachment of adatoms at steps. The steps may either originate from 2D nucleation, or screw dislocations, or from the terrace structure of a vicinal surface inclined with respect to a singular face by a small tilt angle Θ (Fig. 6.14). The advancement of steps therefore determines the rate of layer growth r , which represents the velocity of a parallel displacement of the singular faces. The relation between the lateral advancement of steps and growth rate r is illustrated for a vicinal surface in Fig. 7.22. The figure depicts a cross section of the terraced surface at a time t1 (black lines) and a later time t2 (gray lines). During t2 − t1 the steps are laterally displaced via adatom attachment by some amount s, yielding the velocity rstep = s/(t2 − t1 ). The growth rate r of the singular layer (i.e., the mean vertical displacement of the horizontal terraces in Fig. 7.22a) follows from rstep via the tilt angle Θ of the vicinal layer. For steps of height d and terraces of width l the tilt angle is given by tan Θ = d/l. Since also tan Θ = r/rstep , we obtain r = rstep tan Θ = (d/l)rstep .
(7.27)
Step velocity rstep
The growth rate rvicinal of the vicinal layer (i.e., the velocity of a parallel displacement of the layer indicated by dotted lines in Fig. 7.22) may be read from the enlarged scheme Fig. 7.22b. Since Θ is also the angle between r and rvicinal , the relation is given by
Terrace width l
Fig. 7.21 Steadystate velocity of lateral step advance rstep depending on the terrace width l for equidistant and straight steps
280
7 Atomistic Aspects of Epitaxial LayerGrowth
(a) d
r
l
rstep Θ
(b) r rvicinal rstep Fig. 7.22 a Relation between the lateral growth rate rstep of steps on a vicinal surface and the growth rate r of the related singular layer. Black and gray lines represent cross sections of the surface at two times, the dotted lines indicate the vicinal surface. b Magnified scheme showing the relation between the growth rates of steps, singular surface and vicinal surface
rvicinal = r cos Θ = rstep sin Θ.
(7.28)
7.2.5 The EhrlichSchwoebel Barrier Diffusion of an adatom on a flat or terraced surface is of particular importance in the kinetics of growth. Surface diffusion by a randomwalk process on a flat surface was described by (7.10). Until now we assumed that steps or stable 2D clusters capture adatoms from their top and from their bottom with the same probability. In fact, diffusion across a flat surface generally differs from diffusion across a step, as first pointed out by Ehrlich [28], Schwoebel [29], and coworkers. Adatom capture from the upper and lower terrace at a step hence also differ. Such unequal capture probability causes the asymmetry in the adatom density discussed in Sect. 7.2.3. We consider the diffusion barrier provided by a step and consequences for twodimensional growth. An intuitive picture of the socalled EhrlichSchwoebel barrier of diffusion across a step is given in Fig. 7.23. As an adatom moving on the upper terrace approaches the step it has to overcome a pronounced maximum of the potential to step down. The reason is a fewer number of nearest neighbors in the transitions state of the hop over the ledge compared to that in flatsurface diffusion. We note from Fig. 7.23 that the EhrlichSchwoebel barrier E ES is actually the difference in the activation energy for hopping across the step and hopping across a flat surface. Once the adatom has surmounted the barrier E ES it enters a position at the step edge with an increased binding energy E s . The increase originates from the larger number of nearest neighbors at the lower edge of the step. Step down of an adatom may also occur by another process with a potentially lower barrier: The adatom located at the position on top drawn in Fig. 7.23 pushes the edge atom underneath away to the right and takes its place. This exchange process may provide an efficient parallel channel to the stepdown process discussed above.
7.2 Kinetic Process Steps in Layer Growth
E
281
EES Es
Ed
Fig. 7.23 Cross section of a monoatomic surface step and schematic of the potential associated with the diffusion of an adatom across the surface. Energies E d , E s , and E ES refer to the activation of surface diffusion, binding to a step, and the EhrlichSchwoebel barrier, respectively
Both processes have always higher barriers than diffusion on a flat surface. In the following we focus on the usual EhrlichSchwoebel barrier depicted in Fig. 7.23. We note from Fig. 7.23 a distinct difference for stepdown and stepup diffusion. In the first case the adatom approaches a descending step and experiences a repulsive stepedge barrier of height E ES , which tends to reflect the adatom. By contrast, an adatom approaching an ascending step (i.e., migrating from the right to left towards the step in Fig. 7.23) experiences a trapping potential E s accompanied by a subsequent barrier E ES . Such potential landscape tends to capture the adatom at the step. Incorporation of diffusing adatoms into the crystal was mentioned in Sect. 7.1.1 to occur preferentially at kink positions. For actual incorporation an adatom caught at a step by the binding potential illustrated in Fig. 7.23 needs to diffuse along the step until meeting a kink position. We consider this onedimensional diffusion analogous to the surface diffusion on a terrace. Let us assume a single adatom diffusing along a step towards a kink formed by an additional row of atoms (i.e., a kink with positive sign, cf. Fig. 7.1). To pass the kink site and continue diffusion along the step the adatom has to hop around the kink. Obviously the kink provides a barrier in addition to the activation barrier for the onedimensional diffusion along a straight step, and also in addition to the EhrlichSchwoebel barrier discussed above. Qualitatively, the potential looks like that for twodimensional diffusion across the step depicted in Fig. 7.23. Due to this analogy the barrier is termed the Kink EhrlichSchwoebel barrier, and the constraint of the 1D diffusion by this barrier is referred to as the Kink EhrlichSchwoebel effect. The barriers for diffusion across a step and along a step both affect the morphology of the surface. The first effect may particularly affect the distribution of steps, while the latter may control the structure of a step. Both effects are addressed in the following.
282
7 Atomistic Aspects of Epitaxial LayerGrowth
7.2.6 Effect of the EhrlichSchwoebel Barrier on Surface Steps In the discussion on growth by step advance Sect. 7.2.4 we assumed a terraced surface with equidistant and straight steps. Qualitative arguments show that both conditions may be oversimplified. It has in fact been observed in experiments as well as in computer simulations that the stepflow mode is only metastable. Let us consider stepflow growth of an ideal vicinal surface with equidistant steps, and absence of an EhrlichSchwoebel barrier (Fig. 7.24a). Adatoms from an upper and a lower terrace will then be captured at a step with equal probability, and due to a constant width of all terraces all steps advance with the same velocity rstep . We recall from (7.25) and (7.26) that the velocity is proportional to the widths of upper and lower terrace, rstep ∝ (lupper + llower ). If now one step lags behind its regular position for any reason (e.g., some fluctuation) the area of the lower terrace in front increases and that of the upper terrace behind decreases, see Fig. 7.24b. The lower, wider terrace in front of the step will collect more adatoms, and distributes one half of this surplus to the considered step and the other half to the step ahead. The upper, smaller terrace accordingly collects less adatoms. The lack is equal to the surplus at the lower terrace. Less adatoms are hence supplied from the upper terrace to the considered step and also to that behind. As a consequence, the decreased velocity of the considered step remains unchanged. In addition, the velocity of the step ahead is slightly accelerated, and the velocity of the step behind is slightly delayed. The equidistant arrangement of steps is therefore not stable in absence of an EhrlichSchwoebel barrier. Eventually bunches of steps appear on the surface, cf. Fig. 7.24c. Such a process is termed step bunching. In presence of an EhrlichSchwoebel barrier adatoms are basically captured from the lower terrace at a step. A delayed step will then be supplied with more adatoms from the lower (wider) terrace ahead and its velocity will increase. On the other hand,
Fig. 7.24 a Surface crosssection during stable stepflow growth in presence of EhrlichSchwoebel barriers. b Step delayed behind its regular position (arrow) and c eventually forming bunches of steps in absence of EhrlichSchwoebel barriers
(a)
(b)
(c)
7.2 Kinetic Process Steps in Layer Growth
283
a faster step is supplied less and its speed decreases. The EhrlichSchwoebel barrier therefore stabilizes an equidistant train of steps during stepflow growth. Conditions are reversed if no flux is supplied to the surface. During evaporation of adatoms the EhrlichSchwoebel barrier destabilizes a regularly stepped surface and leads to the formation of step bunches. Steps move in reverse direction due to detachment of atoms and subsequent evaporation. If now a step is delayed, the lower terrace gets more narrow than the upper terrace. The flux of evaporation is then reduced, leading to a further decrease of step velocity. Similar to the transition between island and stepflow growth (Sect. 7.2.4), a transition between stepflow and stepbunching growth depending on sample offcut and growth conditions is found for many semiconductors, e.g., for Si(001) [30], GaAs [31], InP [32], GaN [33], and AlN [25, 34]. The experimental and theoretical studies indicate that the transition also depends on the balance of surface diffusivity and terrace width, where the diffusion can be controlled by supersaturation (or anion/cation ratio) and temperature [31, 34]. Surface steps were by now considered straight and assumed to move during stepflow growth on the hole like a rigid entity. Experiments and theoretical analyses show that such a condition is not stable in practice. A step will generally be perfectly straight only at T = 0 K. At finite temperature the action of entropy produces a roughening addressed in the next section. The overall shape of a step is basically preserved by such change which occurs on a small scale. On a larger scale the shape of a straight step was found to be unstable during stepflow growth, if the adatom attachment from the upper and lower terraces differ. G.S. Bales and A. Zangwill pointed out that surface diffusion in presence of an EhrlichSchwoebel barrier gives rise to a morphological instability of straight steps, leading to a distinct wavy shape [35]. The qualitative reason for the BalesZangwill instability is analogous to that considered above to explain the debunching effect of the EhrlichSchwoebel barrier on a sequence of steps during stepflow growth. We recall from (7.25) that the step velocity rstep is proportional to the sum of the current density of adatoms jupper from the upper terrace to the step and jlower from the lower terrace, rstep = a 2 ( jupper + jlower ). Furthermore, we note that the current density j on either side of the step is proportional to the gradient of the adatom density n near the step, j = −D∂n/∂r. Let us now assume a step deviates at one section from the perfect straight shape and has, say, a warpage in the direction along rstep (like point A in Fig. 7.25). The lines of isoconcentration of the adatom density n on the lower terrace are then more dense in front of the warpage than on the straight parts of the step. The adatom density is even less dense in front of notches (like point B in Fig. 7.25). A high density of isoconcentration lines in front of point A corresponds to an increased current density jlower towards the step at this point. In absence of an EhrlichSchwoebel effect this surplus of adatoms from the lower terrace is exactly balanced by a lack of adatoms from the upper terrace: Behind the warpage on the upper terrace the density of isoconcentration lines of n is decreased, and so jupper . Without an EhrlichSchwoebel effect all parts of the distorted step will travel with the same velocity rstep . The presence of an EhrlichSchwoebel barrier will, however, reduce the compensating contributions from the upper terrace. As a result,
284
7 Atomistic Aspects of Epitaxial LayerGrowth
B A rstep Fig. 7.25 Monoatomic wavy step (solid black line) viewed from top. Light gray and gray shaded area indicate upper and lower terrace, respectively. The dotted lines are isoconcentration lines of adatoms, gray arrows represent adatom fluxes towards the step being proportional to the gradient of adatom concentration. A and B denote respectively points of enhanced and diminished adatom inflow at the step compared to a straight step
the dominating contributions from jlower lead to an increased growth rate at a convex section of the step (point A) and a decreased growth rate a concave section (point B). This positive feedback amplifies perturbations of a straight step. Eventually, the line tension at the step that increases with the step length limits the feedback, and a wavy shape as indicated in Fig. 7.25 develops. The BalesZangwill instability is discussed quantitatively and in more detail in [35, 36]. We confine ourselves to the qualitative arguments given above. A wavy step structure can be recognized in Fig. 7.19; the effect is particularly strong at decreased temperature (Fig. 7.19b), where also low barriers act more effective due to a lowered adatom mobility. It should be noted that a meander pattern of a step may also be induced by a KinkEhrlichSchwoebel effect [37, 38].
7.2.7 Roughening of Surface Steps A surface step will generally be perfectly straight only at T = 0 K. As the temperature is increased, a finite contribution of entropy will decrease Gibbs free energy and kinks separated by straight parts will appear. This roughening provides kink sites for the incorporation of adatoms into the layer during growth. We consider the structure of a straight step of monoatomic height on the (001) surface of a cubic Kossel crystal oriented along the [100] direction [21]. Figure 7.26 shows a top view on a straight step at position (a), where one atom was moved from an embedded step site to a site attached to the step. To evaluate the energy cost of this operation in the framework of the terracestepkink model we count the number of broken and formed nextneighbor bonds. Three bonds with an energy E B each were broken, and one bond for the attachment at the step was formed, yielding a net amount of 2E B . Counting
7.2 Kinetic Process Steps in Layer Growth
285
(a)
(b)
n s
Fig. 7.26 Schematic of monoatomic steps on a Kossel crystal viewed from top, a lighter gray shading indicates higher lying terraces. a Kinks generated by moving one embedded ledge atom of a straight step to a position attached to the step. b Step with kinks of several atom units
of the kinks created yields (from bottom to top in Fig. 7.26 at position (a)) 1+ , 1− , 1− , 1+ , i.e., two positive and two negative kinks. We thus obtain an energy of E B /2 necessary to form a kink. The probability of having a kink or a straight part of the step depends on the energy per kink. Denoting the probabilities for (monoatomic) positive kinks, negative kinks, and straight parts p+ , p− , and p0 , respectively, we obtain [21] E B /2 (1/2)( p+ + p− ) , = exp − p0 kT
p+ + p− + p0 = 1.
(7.29)
The mean distance between kinks is given by y0 = a/( p+ + p− ), a being the unit spacing. Inserting (7.29) yields a y0 = exp 2
E B /2 kB T
a E B /2 + 2 ≈ exp . 2 kB T
(7.30)
The mean distance y0 between kinks decreases as the temperature is raised. Note that at common growth temperatures usually E B kB T applies. Considerations above assumed kinks of a single atom unit and steps without any mutual interaction arising from longrange strain fields. We illustrate the effect of step roughening for the interesting vicinal surface of Si(001). The Si(001) surface reconstructs to a (2 × 1) surface unitcell by forming rows of dimerized atoms. Dimer rows on terraces that are separated by a monoatomic step (or by an odd number of such steps) are perpendicular to each other due to the structure of the diamond lattice (Sect. 2.1.4). If the singular Si(001) surface is tilted by a small angle (below ∼1◦ ) toward a [011] direction, adjacent monoatomic steps are hence not equivalent. It should be mentioned that larger miscuts (2–10◦ ) and heating to typical growth temperatures above 600 ◦ C leads to doublelayer steps, which are not considered here. There exist two kind of monoatomic steps: those labeled S A steps (single A steps) have dimers on the lower terrace directed parallel to the step, while the dimerization direction on the lower terrace at S B steps runs perpendicular
286
7 Atomistic Aspects of Epitaxial LayerGrowth
SA
SB
SA
SB Fig. 7.27 Top view on monoatomic steps of a vicinal Si(001) surface. The height decreases from left to right. On each terrace dark gray dimers and gray atoms lie on the topmost layer and the layer underneath, respectively
to the steps, cf. Fig. 7.27. Calculations show that the formation energy per length of S A steps is much lower (∼0.01 ± 0.01 eV/atom) than that of S B steps (∼0.15 ± 0.03 eV/atom) [39]. This finding was basically confirmed by scanningtunneling microscopy, yielding an upperbound estimate of ∼0.028 ± 0.002 eV/atom for S A steps and ∼0.09 ± 0.01 eV/atom for S B steps [40]. Due to the symmetry of the Si(001) surface each kink must have a length of multiples of 2a, and the same holds for the distance between kinks. We note from Fig. 7.27 that kinks in one type of step are made of segments of the other type of step. The two types of steps have different energies associated with the formation of kinks and consequentially also different morphology: S A steps are smooth and S B steps are rough, see Fig. 7.28. The equilibrium distribution of steps and kinks was analyzed from images like that of Fig. 7.28 [40]. In the analysis a kink is any inside corner followed by an outside corner or vice versa. Separations s and lengths n of kinks are defined as shown in Fig. 7.26. Resulting distributions of kink separations s and kink lengths n of an S B step are displayed in Fig. 7.29. The probability p(s) of finding two adjacent kinks separated by s atoms follows from the probability pk that a kink exists times the probability that no kink (i.e., (1 − pk )) is nearby in a range ±s atoms. The exact relation is given by (7.31) p(s) = pk (1 − pk )s/2−1 .
7.2 Kinetic Process Steps in Layer Growth Fig. 7.28 Scanningtunneling micrograph of a Si(001) surface miscut 0.3◦ towards [100]. The surface was annealed at 600 ◦ C for 5 min prior to quenching to room temperature. Steps are descending from the upper left to the lower right corner. Reproduced with permission c 1990 APS from [40],
287
[110] [110] SA SB
This function is drawn in Fig. 7.29a. In the plot pk equals the number of kinks of S B steps counted from STM images divided by the total number of possible kink sites. We observe that (7.31) describes the measured probability distribution p(s) very well, indicating that kinks may be considered independent in this experiment. The validity of this assumption is also reflected in Fig. 7.29b, showing an exponential dependence of the number N of kinks of length n atoms from the length, i.e., N ∼ exp(−E(n)/(kT )), where E(n) is the energy of a kink of length na. E(n) was shown to be related to the formation energy per length of a step E S according to E(n) = n E S + const [40]. E S corresponds to an S A step for kinks in an S B step (and vice versa) due to the symmetry of the diamond lattice as illustrated in Fig. 7.27. The E(n) offset, i.e., the const = 0.08 ± 0.02 eV, may be considered as an additional energy due to the corner of a kink. The lower formation energy per length E S of S A steps leads to a small kink energy E(n) in S B steps, and consequently according to (7.30) to a smaller mean distance y0 between kinks as compared to S A steps.
7.2.8 Growth of a Si(111)(7 × 7) Surface Surface kinetics considered so far assumed adatoms arriving on the surface to migrate and eventually nucleate islands or being incorporated on a regular lattice site at a step. The nucleation theory outlined above in Sect. 7.2.2 is often successfully applied to describe epitaxy of metals. Metal surfaces often do not reconstruct, and surface diffusion and capture to form a stable nucleus may be the only relevant processes which determine the growth morphology. We know, however, from Sect. 7.1 that the arrangement of surfacenear atoms may strongly deviate from that inside the bulk solid. Such reconstruction is particularly prominent on semiconductor surfaces. Compared to an unreconstructed surface an additional energy barrier must hence be
s (atoms) 0.6
0
4
8
12
16
20
(a) 0.4
0.2
0.0
N(n)
Fig. 7.29 a Probability of two adjacent kinks separated by s atoms depending on their separation for an S B step on Si(001) prepared at 600 ◦ C. The solid line is function (7.31) with pk taken from the measured kink density. b Number of kinks of length n as a function of kink length n. Reproduced with permission from [40], c 1990 APS
7 Atomistic Aspects of Epitaxial LayerGrowth
p(s)
288
10
3
10
2
10
1
10
0
(b)
0
4
8
12
16
20
n (atoms)
surmounted to form a stable nucleus [41]. How are surface atoms rearranged from sites in reconstruction to regular lattice sites during growth? The complexity of surface reconstructions pointed out in Sects. 7.1.6 and 7.1.7 indicate that this question does not have a general answer. Only few studies provide a microscopic insight into the complex growth kinetics of reconstructed semiconductors. We consider sequential growth steps for the two previously treated examples to illustrate the dynamics of surface reconstructions. The (7 × 7) reconstruction of the Si(111) surface is a prominent surface structure. According to the DAS model the complex reconstruction comprises 15 dimers, 12 adatoms, and 1 stacking fault, cf. Fig. 7.13. During growth the atoms of the surface reconstruction have to be rearranged to the bulk structure. We first consider an experimental observation of the epitaxial growth of a twodimensional island. Figure 7.30 shows a sequence of STM images recorded at 575 K during MBE growth on a (7 × 7) reconstructed Si(111) surface [42]. Details of the reconstruction are not resolved in the images. We note a pronounced macro kink at the right edge of the island that gradually moves downwards, thereby eventually completing a laterally enlarged triangular island. Atomically resolved images proved that the fast growing stripe has the width of a (7 × 7) unit cell (27 Å). The stability of the island during the sequence shown in Fig. 7.30 indicates a fast growth of the additional row. This is confirmed by the growth dynamics evaluated from such in situ STM images given in Fig. 7.31 [42]. The lower curve shows the experimentally observed size of a single island expressed in units of half the rhombic (7 × 7) unit cell. We note pronounced plateaus indicating a stable configuration of
7.2 Kinetic Process Steps in Layer Growth
289
Fig. 7.30 Consecutive stages of the homoepitaxial growth of a twodimensional island on a (7 × 7) reconstructed Si(111) surface, recorded at 575 K using scanning tunneling microscopy. The image c 1998 APS size is 500 × 500 Å2 . Reproduced with permission from [42],
150
simulation Island size (HUC)
Fig. 7.31 Evolution of a single island on a Si(111) (7 × 7) surface. Lower and upper curve refer to experimental data and a kinetic Monte Carlo simulation, respectively. The island size is given in numbers of halfunitcells (HUC), gray horizontal lines mark sizes of n 2 HUC. Reproduced with permission c 1998 APS from [42],
100
experiment 50
0
50
100 Time (min)
150
200
the island, and a rapid increase of the island size between the plateaus. These periods of fast growth correspond to the addition of a row like that shown in the sequence of Fig. 7.30. The stable islands occur at triangular “closed shell” configurations, i.e., at sizes of n 2 halfunitcells. At these numbers isosceles triangles appear, cf. Fig. 7.32. The observed island growth is related to the structure of the surface reconstruction. The rhombic (7 × 7) unit cell of the Si(111) (7 × 7) surface is composed of two triangular halfunitcells (HUC): One unfaulted half (UHUC) with a nearsurface layer sequence identical to the bulk underneath, and a faulted half (FHUC) with a stacking fault (the right and left triangles in Fig. 7.13, respectively). During growth the reconstructed atoms have to rearrange toward the bulk structure. In the unfaulted HUC these are the atoms in the uppermost layer. In the faulted HUC the stacking fault must be removed in addition. Atom rearrangement in the faulted half is therefore associated with a higher energy barrier than in the unfaulted half of the (7 × 7) unit cell [43]. A model of the growth sequence is illustrated in Fig. 7.32. A triangular twodimensional island on Si(111) (7 × 7) is surrounded by faulted halfunitcells denoted F in Fig. 7.32 (the initial nucleation is assumed to be favored on an unfaulted unit cell). Growth of the island hence requires the overgrowth of a faulted HUC. Surmounting the unfavorable high energy barrier causes the delay observed in the
290 Fig. 7.32 Arrangement of faulted (F) and unfaulted (U) halfunitcells of a (7 × 7) reconstructed Si(111) surface around a triangular twodimensional Si island (brown)
7 Atomistic Aspects of Epitaxial LayerGrowth
U F U F U F U
F U F U F U F
U F U F U F U
F U F U F U F
U F U F U F U
F U F U F
F
U F U F
U
F U F
F
U F
U
F
F
U F
U
F U F
F
U F U F
U
F U F U F
F
U F U F U F U
F U F U F U F
U F U F U F U
F U F U F U F
U F U F U F U
F U F U F U F
dynamics Fig. 7.31. Once an FHUC nucleates the adjacent UHUC can be overgrown more easily. Overgrowth of the next FHUC is facilitated by the macro kink depicted in Fig. 7.32: The new FHUC has a shorter edge length than the FHUC which nucleated before (1 side instead of 2). Neighboring faulted and unfaulted halfunitcells aside the island are overgrown in a quick succession until an enlarged island comprising n 2 halfunitcells in total is completed. The experimentally observed growth behavior is well reproduced by a kinetic Monte Carlo simulation [42]. The simplified model assumes a honeycomb lattice consisting of alternating F and U sites, and material to be transported towards the island in HUC units. The attachment barrier E is assumed to depend on both, the type of the underlying HUC (F or U), and the number n edge of nearestneighbor HUC already attached to the island, E = E U/F − n edge × E edge . Rates for hopping and attachment are modeled in terms of Arrhenius expressions with energies chosen to yield the best agreement with experimental data. The result shown in Fig. 7.31 features a similar dynamics as the island evolution observed in the experiment. Nucleation of the halfunitcells was addressed in spatially more refined models [44, 45]. Nucleation of a 2D island is considered to proceed in three steps, starting with a small stable cluster in a HUC of the Si(111) (7 × 7) surface. The cluster raises the adatom binding energy in adjacent HUCs, leading to a preferential formation of a second cluster in a neighboring HUC of the same unit cell. Eventually an additional adatom is attached to the cluster pair, and the (7 × 7) reconstruction is locally removed [45]. The species cluster, cluster pair, and 2D island are well reproduced in the STM image Fig. 7.33.
7.2.9 Growth of a GaAs(001) β2(2 × 4) Surface A very detailed scenario of kinetic processes occurring during nucleation and growth of reconstructed surfaces was obtained by combining experimental STM results with kinetic Monte Carlo simulations [46, 47]. Advanced modeling emloyed rates obtained from densityfunctional theory (DFT) calculations [47]. Monte Carlo simulations can bridge the time scales from individual kinetic steps to macroscopic
7.2 Kinetic Process Steps in Layer Growth Fig. 7.33 STM image of a (7 × 7) reconstructed Si(111) surface after deposition of 0.2 bilayers of Si showing clusters, cluster pairs, and 2D islands. The smallest island (circle) has the size of one unit cell. The image size is 425 × 425 Å2 . Reproduced with permission c 2007 APS from [45],
291
single clusters
2D islands
cluster pairs
3
2 1
trench
dimer row
trench
Fig. 7.34 Side and plan views of a β2(2 × 4) reconstructed GaAs(001). The unit cell is indicated by dashed lines, filled and open symbols represent Ga and As atoms, respectively. Numbers label initial growth steps
growth, while DFT calculations yield kinetic parameters from first principles. The studies focus on homoepitaxial growth of GaAs on a Asrich GaAs(001)β2(2 × 4) surface from beams of atomic Ga and As2 molecules. The two species behave quite different on the surface. Ga atoms adsorb with a sticking coefficient of unity on the Asrich surface [48], leading to a growth rate which is controlled by the Ga flux. On the other hand, the chemically rather stable As2 binds only weakly to an Asrich GaAs surface [48, 49]. It adsorbs only after deposition of Ga [50] and diffusion to adjacent sites [47]. Diffusion and incorporation of Ga has thus a strong impact on the adsorption and incorporation of arsenic.
292
7 Atomistic Aspects of Epitaxial LayerGrowth
The β2(2 × 4) reconstructed GaAs(001) surface consists of rows with topmost AsAs dimers, separated by trenches, cf. Fig. 7.34. Diffusion of Ga adatoms is anisotropic with lowest activation energy for hopping processes along the trenches [51]. From calculations it was found that the terminating As2 dimers of the β2(2 × 4) reconstruction, particularly those in the trenches, act as traps for diffusing Ga adatoms: Ga atoms are immobilized for about 10−8 s, much longer than the time scale for hopping of order 10−12 –10−9 s. At such Ga adsorption site a gasphase As2 molecule can readily adsorb by forming one bond to the adsorbed Ga atom and two bonds to Ga atoms with unsaturated bonds that are located at the side walls of the β2(2 × 4) trenches. The new AsAs dimer complex becomes more stable by attaching another diffusing Ga adatom in the trench. Growth on the reconstructed surface hence preferentially nucleates at the side walls of the trench and largely proceeds by partially filling the trenches, followed by island nucleation on surface regions where a filling of the trenches has occurred [52]. The first steps of the mentioned process are depicted in Fig. 7.34. The surface unitcell marked in the figure contains an AsAs dimer in the trench. In one of the favored Ga diffusion channels the bond of these dimers is broken by Ga as depicted at position 1 in the top panel of Fig. 7.34 [51]. The new bonds relax the position of the two As atoms to their bulk position. The Ga atom at position 1 favors a subsequent As2 adsorption at the trench sidewall as indicated at position 2. A dangling bond of As may then be saturated by a further Ga atom in the trench at position 3. The outlined nucleation steps describe the main route occurring at standard conditions of molecular beam epitaxy of GaAs(001) at 800 K. The prevailing processes change when the growth temperature is changed [47]. The examples of homoepitaxial growth on the β2(2 × 4) reconstructed GaAs(001) surface and the (7 × 7) reconstructed Si(111) surface indicated that the classical nucleation theory may sometimes be too simplified for describing the complex processes of semiconductor growth. Still the simple theory provides useful guidelines to interpret growth phenomena and to optimize growth conditions.
7.3 Selforganized Nanostructures The reduction of the dimensionality of a solid leads to a modification of the electronic densityofstates. The effect of size quantization requires characteristic length scales in the range of typically 10 nm defined by the deBroglie wavelength as outlined in Sect. 4.3.2. Fabrication of such small structures with high material quality may hardly be accomplished by lateral patterning of quantum wells. Etching or implantation techniques inevitably introduce defects, which deteriorate the electronic properties of a nanostructure. Therefore a number of techniques were developed particularly in the 1990s employing selforganization phenomena during epitaxial growth. The approaches are based on an anisotropy of surface migration of supplied atoms, originating from a nonuniform driving force like, e.g., strain, that tends to minimize the total energy of the system. Thereby structurally or compositionally nonuniform
7.3 Selforganized Nanostructures
293
Fig. 7.35 Scheme illustrating elastic strain relaxation in a a quantum dot and b a quantum well. Yellow and blue circles represent atoms of sizequantized materials and barrier materials, respectively
crystals with dimensions in the nanometer range may be coherently formed without structural defects. Some of these techniques have attracted much attention for the fabrication of quantum wires or quantum dots, and are outlined in the following.
7.3.1 StranskiKrastanow Island Growth StranskiKrastanow growth is one of the three fundamental growth modes of heteroepitaxy introduced in Sect. 6.2.3. The characteristic feature is a transition of an initially twodimensional layerbylayer growth to threedimensional growth. The size of the threedimensional islands formed by such a transition lies for many semiconductors in the range required for quantum dots (QDs) as expressed by (4.53). The transition of 2D to 3D layer growth may be induced by strain upon depositing a 2D layer on a substrate with a different lateral lattice constant. Since a coherent layer adopts the lateral atomic spacing of the substrate, strain accumulates with increasing thickness. Above a critical layer thickness the strain is relaxed plastically by introduction of misfit dislocations (Sect. 2.2.6). Below this critical thickness under suitable conditions a considerable part of the strain may be relaxed elastically, i.e. without introduction of dislocations, by the formation of threedimensional surface structures. Such reorganization of a flat surface into a structure with tilted facets implies an enlargement of the surface area. The driving force of the StranskiKrastanow growth mode is therefore a minimization of the total strain and surface energy [53]. The elastic strain relaxation in an uncovered 3D island is illustrated in Fig. 7.35a. We note that the strain is inhomogeneous, giving rise to shear deformations in addition to hydrostatic strain components. This feature is in contrast to a strained quantum well depicted in Fig. 7.35b. The quantum well exhibits a constant, homogeneous biaxial strain in the entire layer. Elastic strain relaxation generally leads to an energy decrease of the structure. The contribution of the surface energy upon faceting of a flat surface may, by contrast, be positive or negative. The sign follows from a simple advisement. Consider, e.g., a (001) surface with area A and a surface energy γ001 as illustrated in Fig. 7.36. This surface will gain energy upon a faceting with {110} facets, if the surface energy γ011
294
7 Atomistic Aspects of Epitaxial LayerGrowth
area A [001]
area 2 A
Fig. 7.36 Faceting of a (001) surface with area A to a surface of total area
[011]
√
2 A with {011} facets
L θ0
α
θ
Fig. 7.37 Reorganization of a uniformly strained layer of θ0 monolayers thickness to an island with pyramidal shape on a remaining wettinglayer thickness of θ monolayers. L and α are the base length of the island and the tilt angle of the island facets, respectively
√ √ of these facets fulfills the condition 2γ011 < γ001 . The prefactor 2 is the increase of surface area of a faceted {011} surface with respect to the flat (001) surface. The total energy gain of threedimensional islands with respect to a twodimensional deposition is given by strain and surface energycontributions of both, the reorganized part of the material and the part remaining in the wetting layer after the StranskiKrastanow transition. The wetting layer is a fraction of the deposited strained material of at least one monolayer thickness. This part remains as a twodimensional layer on the substrate and does not migrate to the faceted part due to a lower surface energy of the deposit as discussed in Sect. 6.2.3. We consider the total energy gain per unit volume obtained, if a twodimensional deposit of nominal thickness θ0 (in units of monolayers) reorganizes to a single faceted threedimensional island on a wetting layer (WL) of thickness θ , cf. Fig. 7.37. The contributions sensitively depend on the shape of the island. For simplicity we assume an island with the shape of a pyramid with a quadratic base of length L as often found in experiment. The gain can be expressed as [54] 1 2 γWL (θ ) − γWL (θ0 ) −L , ρ V (7.32) elast elast with the elastic energy densities εisland and εlayer of the island and the uniformly strained layer, respectively. The third term describes the change in surface energy due to the island: γfacet is the surface energy of the island facets, A is their area, and L the island base length. The volume of the pyramidal shaped island V follows from mass conservation and is given by Aγfacet − L 2 γWL (θ0 ) E total elast elast = εisland + − εlayer + V V
7.3 Selforganized Nanostructures
V =
295
1 1 (θ0 − θ )dML = L 3 tan α, ρ 6
where ρ, dML , and α are the areal density of the islands (in units cm−2 ), the thickness of one monolayer, and the tilt angle of the facets. The fourth term in (7.32) accounts for the change of wettinglayer energy as the thickness decreases from θ0 to θ . The relation γWL (θ ) computed for thin reconstructed InAs layers on GaAs substrate is shown in Fig. 7.38a [54]; for similar findings with Ge/Si(001) see [55]. The prefactor (1/ρ − L 2 ) effectuates that this term solely applies for the free surface besides the island (i.e., the area not covered by the island). The sum of all four contributions is given in Fig. 7.38b. Values refer to pyramidal InAs islands with relaxed, but unreconstructed {110} facets and a β2(2 × 4) reconstructed (001) surface of the wetting layer, grown on (001) oriented GaAs. The calculated energy gain per unit volume upon island formation given in Fig. 7.38b shows that major contributions originate from the elastic energy relief, i.e., from the first two terms in (7.32). This negative part scales with the island volume. The surface energy described by the third term in (7.32) is an unfavorable positive energy with a decreasing contribution for larger islands due to a ∝ V 2/3 dependence. The wettinglayer contribution represented by the fourth term in (7.32) is also positive. Besides island volume it depends on island density and the coverage. The importance of facet edges was controversial in literature [53, 56]; the calculation presented in Fig. 7.38b yields an only minor contribution. The total energy density given by the sum of all contributions has an energy minimum for a particular island size as indicated by an arrow in the figure. Such a minimum is important for obtaining a narrow size distribution for an ensemble of islands. It should be noted that a theory considering only the two contributions of elastic relaxation (negative, ∝ V ) and island surfaceenergy (positive, ∝ V 2/3 ) does not yield a finite equilibrium size. For sufficiently high coverages the volume term always prevails and favors steady island growth as previously discussed in nucleation and ripening (Sects. 6.2.1, 6.2.8). StranskiKrastanow growth induced by strain represents a quite universal behavior. Selforganized formation of islands is found for both, compressively and tenselystrained layers in various materials systems and crystal structures. Table 7.5 and Fig. 7.39 give some examples. The mismatch is defined by (2.20a), yielding a negative sign for compressively strained islands. Usually substrate material is also employed for covering the islands after formation. The material is then generally termed matrix. Often the island material is alloyed with matrix material to reduce the strain, yielding a parameter for controlling the transition energy of confined excitons. Selforganized StranskiKrastanow growth was particularly studied for fabricating InAs and In1−x Gax As quantum dots in a GaAs matrix [61]. The InAs lattice constant exceeds that of GaAs by ∼7 %, and the critical thickness for elastic relaxation of such a highly strained 2D InAs layer on a GaAs(001) substrate to 3D islands is only about 1.5 InAs layers. Once this critical layer thickness is exceeded, islands form with a high areal density of typically 1010 − 1011 cm−2 .
296
7 Atomistic Aspects of Epitaxial LayerGrowth
55 51 47 43 0
1
3
2
(meV/Å )
59
WL
2
(b) E/V (meV/Å )
(a)
0
total (1.5 ML)
1 2
2 3 1 coverage θ (ML)
surface WL edge total (1.8 ML)
0
elastic
0.5 1 6 3 V ( x 10 Å )
1.5
Fig. 7.38 a Calculated formation energy of a strained InAs wetting layer on (001)oriented GaAs as a function of coverage θ. b Total energy gain by island formation with various contributions for ρ = 1010 cm−2 areal density and θ0 = 1.8 monolayers InAs layer coverage on GaAs (black lines). The gray line refers to the total energy gain for θ0 = 1.5 monolayers. Arrows mark the minima of the total energy curves, WL denotes the contribution of the wetting layer. Reproduced with permission c 1999 APS from [54], Table 7.5 Some semiconductor materials used for straininduced, selforganized StranskiKrastanow formation of islands Island/matrix Ge/Si InAs/GaAs GaN/AlN PbSe/PbTe Structure Orientation Mismatch (%)
(a)
Diamond (001) −3.6
Zincblende (001) −7
(b)
[100]
Wurtzite (0001) −2.5
(c)
Sodium chloride (111) +5.5
(d)
[110]
[110] Ge / Si
InAs / GaAs
GaN / AlN
PbTe/PbSe
Fig. 7.39 Free standing selforganized islands formed by StranskiKrastanow growth in various strained heteroepitaxial materials: a Ge/Si(001) [57], b InAs/GaAs(001) [58], c GaN/AlN(0001) [59], d PbTe/PbSe(111) [60]. The AFM images are vertically not to scale with respect to the lateral scale
7.3 Selforganized Nanostructures
297
2
Fig. 7.40 Density of selforganized islands formed by StranskiKrastanow growth during molecularbeam epitaxy at 530 ◦ C with a low growth rate of 0.01 ML/s. Reproduced with permission c 1994 APS from [63],
Island density (cm )
The StranskiKrastanow transition from 2D growth of a strained layer to 3D growth of islands occurs quite abrupt, albeit it may be delayed by kinetic barriers constituted by suitable growth conditions. During molecularbeam epitaxy the 2D–3D transition can be monitored in situ using reflection highenergy electron diffraction: The streaky reflection pattern indicating reflection from a flat 2D surface changes to a spotty pattern created by threedimensional surface structures [62], see Fig. 8.7. Atomic force micrographs taken for different coverages of InAs yield virtually no islands below the critical coverage θc , and a sharp increase of the density of islands ρ above θc following a relation ρ ∼ (θ − θc )α [63]. The dependence of island density on InAs coverage θ is shown in Fig. 7.40. The shape of islands created by StranskiKrastanow growth depends on the material system and also on the growth conditions. For uncovered islands in several materials systems the shape is found to undergo a transition upon increase of volume, which increases for thicker coverage. Generally a transition with a continuous introduction of steeper facets at the island edge is expected [64], particularly due to the strain concentrating at the base perimeter. Experimental results for the two most studied materials InAs/GaAs(001) and Ge/Si(001) are given in Fig. 7.41. Small and large islands, referred to as pyramids with shallow facets and domes with steep facets, respectively, were found. The gray scale in the figure indicates the local slope of the facets. Figure 7.41 indicates that islands with distinctly different sizes may coexist. A bimodal size distribution of island ensembles with well separated maxima of the mean sizes is often observed. The finding indicates some departure from thermodynamic equilibrium due to the presence of kinetic barriers in the formation process. Island formation using StranskiKrastanow growth is usually performed at quite low growth temperatures. For quantumdot applications in devices StranskiKrastanow islands are covered by a capping layer. Usually the same material as that underneath the islands is employed. The morphology of the islands is generally strongly modified during the capping procedure, unless special deposition conditions are found to preserve
10
11
10
10
10
9
10
8
10
7
α 1.76 θc = 1.50 ML
no dots
1.2
1.4 1.6 1.8 InAs coverage (ML)
2.0
298
7 Atomistic Aspects of Epitaxial LayerGrowth
(a)
32°
(c) 54°
0°
0° (b)
Pyramid
Dome
Ge/Si(001)
(d)
Pyramid
Dome
InAs/GaAs(001)
Fig. 7.41 Shape of uncapped Ge/Si (a, b) and InAs/GaAs islands (c, d). Steeper facets are marked by a darker gray tone: light gray, gray and dark gray denote {105}, {113}, and {15 3 23} facets for Ge/Si and {137}, {101}, and {111} facets for InAs/GaAs, respectively. Reproduced with permission c 2004 APS from [68],
the initial shape. While strain favors the formation of steep facets in the case of free standing islands, deposition of a mismatched material on top of the islands reverses this trend: Generally the islands tend to become flat during caplayer deposition. Often quantum dots with a shape of truncated pyramids are formed. A microscopic picture of the capping dynamics of InAs/GaAs/(001) islands was obtained from scanning tunneling microscopy [65]. The process is illustrated in Fig. 7.42. Initially the deposited Ga atoms tend to migrate away from the islands’ apex and accumulate at the base due to a better lattice match of the GaAs caplayer material. Indium from the apes starts to alloy with Ga near the base, thereby releasing strain and increasing entropy. Eventually GaAs covers the remaining material of the island, yielding a surface morphology depending on the deposition rate of the cap layer. The effect of caplayer deposition on the island shape is illustrated in Fig. 7.43. The STM images show (110) cross sections of InAs islands in GaAs matrix material grown using MBE under the same conditions as applied for the free standing island shown in Fig. 7.39b. The GaAs cap layer was deposited with a rate of 0.15 ML/s at the same low temperature of 510 ◦ C as the InAs islands after applying 10 s growth interruption. The shape changed from a pyramid with shallow facets to a truncated pyramid with a flat (001) top and steeper side facets [66]. Such a shape was also found for structures grown using MOVPE [67] and is typical for buried InAs/GaAs islands. Often a growth interruption is applied after deposition of the island material and prior to deposition of the cap layer. The interruption intends to equilibrate the ensemble of islands for obtaining a narrow distribution of sizes. Usually the mean
7.3 Selforganized Nanostructures
299
Fig. 7.42 Schematic of the overgrowth process of InAs/GaAs islands. Orange and blue mark In and Ga ColumnIII elements, respectively. Shaded regions indicate intermixed InGaAs materials. Caplayer morphology obtained for a low capping rate is illustrated in (e), for a high capping rate c 2006 APS in (f). Reproduced with permission from [65],
5 nm [110]
2.2 ML
5 nm
2.6 ML
5 nm
3.6 ML
[001] Fig. 7.43 Cross section STM images of small InAs/GaAs(001) islands formed from various InAs coverages and buried by GaAs. The dotted white lines indicate the truncated pyramid shape. Courtesy of M. Dähne, TU Berlin
size of the resulting quantum dots increases as the duration of the growth interruption increases. Such a ripening is a further indicative of kinetic limitations in the usually applied growth procedure.
7.3.2 Thermodynamics Versus Kinetics in Island Formation StranskiKrastanow growth in a regime with a major influence of kinetics sometimes leads to experimental findings which appear inconsistent. Size and density of islands for a given deposition thickness are important parameters which are readily obtained experimentally. At low deposition temperature the diffusion length of adatoms is short and the nucleation rate is high. Consequently small islands form with a high areal density. In this kinetic regime the islands grow larger and the density accordingly decreases for a given deposition thickness as the temperature is increased. Such a trend is usually observed in island formation using StranskiKrastanow growth. On
300
7 Atomistic Aspects of Epitaxial LayerGrowth
the other hand, in the thermodynamic regime at high temperature the size is expected to decrease in favor of a larger areal density as the deposition temperature is increased [69, 70]. Numerical results of corresponding equilibrium calculations are given in the inset of Fig. 7.44a. The maximum of the distribution function shifts to smaller island sizes and broadens as the temperature is increased. The same result is obtained from kinetic Monte Carlo (KMC) simulations shown in the main panel of Fig. 7.44a [71]. In the KMC simulation a long duration for equilibration of the island ensemble (35 s) was assumed. The temporal evolution of the island sizes is displayed in Fig. 7.44b. The KMC simulation was performed on a lattice with 250 × 250 atoms and assumed an initial coverage of 4 %, randomly deposited at a flux of 1 ML/s. Adatoms diffuse by nearest neighbor hopping and may cross island edges by surmounting a Schwoebel barrier. Strain near an island is accounted for by including a positiondependent energy correction in the Arrhenius expression of the hopping rate. In the initial stage we find small islands at low temperature, whereas larger (and fewer) islands are formed at higher temperatures: The mean diffusion length increases at higher temperature, and nucleation of new islands is suppressed. Nucleation is hence the dominating process for a short duration of the evolution, a clear indication for a kinetically controlled growth. Right after deposition the island ensemble begins to equilibrate. At low temperature a slow increase of the mean island size is found. Such ripening proceeds much faster at higher temperature. Eventually the size distribution attains an equilibrium value. We note from Fig. 7.44b that the average island size now decreases as the temperature is increased, in agreement with equilibrium results shown in Fig. 7.44a. The study thus evidences a crossover from an initial kinetically controlled regime to thermodynamic equilibrium after an equilibration period.
Fig. 7.44 a Equilibrium distribution of island sizes for T = 675 K (diamonds), 700 K (circles), 725 K (squares), and 750 K triangles) obtained from Monte Carlo simulations on a 250 × 250 grid. Solid lines are numerical fits. Inset: Results from thermodynamic theory. b Simulated evolution c 2001 of the mean island size for various temperatures. Reproduced with permission from [71], APS
7.3 Selforganized Nanostructures
GaAs AlGaAs
(001)
1) (11 A GaAs
A
Ga
(11 1)
Fig. 7.45 Schematic of GaAs wire formation on a Vshaped patterned substrate with an AlGaAs barrier layer
301
7.3.3 Wire Growth on Nonplanar Surfaces Onedimensional structures in the nanometerscale may be fabricated by employing a variety of growthrelated phenomena [72]. Two different methods are pointed out here. For wire growth employing the vaporliquidsolid mechanism see Sect. 12.2. The realization of quantum wires is a challenging task. A 1D wire has a larger interface/volume ratio than a 2D quantum well and consequently makes high demands for structural quality. Interface fluctuations on a length scale of the exciton Bohr radius easily lead to localization referred to as zerodimensional regime. Progress and true 1D properties of confined carriers was particularly achieved using Vshaped wires fabricated using patterned substrates as depicted in Fig. 4.26. The techniques utilizes the dependence of the Ga surface diffusionlength and GaAs growth rate on the crystallographic orientation of GaAs surfaces. The diffusion length λGa of Ga adatoms is—in a certain temperature range— approximately described by a dependence λGa ∝ exp(−E eff /(kB T )), with an effective activation energy E eff depending on the orientation of the surface. From molecular beam epitaxy of GaAl/AlGaAs superlattices on various GaAs facets grown under ColumnIII limited flux conditions the following order of diffusion lengths was concluded [73]: ¯ λGa (001) ≈ λGa (1¯ 1¯ 3)B
¯ ¯ < λGa (1¯ 1¯ 1)B, λGa (3¯ 3¯ 1)B, λGa (013), λGa (113)A < λGa (159) ≈ λGa (114)A ≈ λGa (111)A < λGa (110). The Ga diffusion length increases in the order of GaAs surfaces related to (001), ¯ (1¯ 1¯ 1)B, (111)A, and (110) orientations. λGa (001) was about 0.5 µm for the investigated growth at 620 ◦ C. On a nonplanar GaAs substrate Ga adatoms migrate towards a surface with the minimum λGa and are incorporated there. The growth rate of facets with a larger diffusion length is therefore decreased. This effect was employed to fabricate Vshaped quantum wires [75] and also ridge quantumwires [76, 77]. Figure 7.45 illustrates the effect of wire formation. Growth is performed on a GaAs substrate with Vshaped grooves fabricated using lithography and anisotropic wet etching. Usually grooves
302 Fig. 7.46 Crosssection transmissionelectron micrograph of a vertically stacked GaAs/Al0.42 Ga0.58 As quantum wires. The white circle marks the radius of curvature of the bottom wire interface. Reproduced with permission from [74], c 1995 AIP
7 Atomistic Aspects of Epitaxial LayerGrowth
VQW
QWR
50 nm
¯ on a GaAs(001) substrate oriented along the [110] direction and composed of two {111}A side walls are used. A lower AlGaAs barrier layer is then grown on the patterned substrate. The adatom diffusionlength during AlGaAs growth is quite short and does not show a pronounced facet formation; the Vgroove bottom therefore remains quite sharp. In the subsequent GaAs growth Ga adatoms impinging on the {111}A side walls tend to migrate with a long diffusion length to facets with a short diffusion length. Thereby the growth rate is enhanced at the bottom of the Vgroove, and a (001) facet and accompanying small {311} facets are generated. Adatom migration towards the center at the Vgroove bottom is supported by an additional capillary effect [78]. Eventually the GaAs layer is capped by an upper AlGaAs barrier, leaving buried regions of an enhanced thickness which act as quantum wires. During growth of the upper AlGaAs layer the diffusion length of Ga adatoms is again quite short. This leads to a sharpening of the Vgroove bottom, and eventually to a shape similar to that existing before the deposition of the GaAs layer. The growth sequence may then be repeated, so as to create a vertical stack of quantum wires as shown in Fig. 7.46. The dark regions in the AlGaAs layers labeled VQW (vertical QW) represent Garich parts with a lower bandgap. Selforganized growth was also applied on nonpatterned substrates to fabricate quantum wires. We consider the use of step bunches which may appear on surfaces as pointed out in Sect. 7.2.6. Quantum wires forming at step bunches were studied for virtually unstrained GaAs/AlGaAs [80], but as well for strained wire/barrier materials such as InGaAs/GaAs [79], InGaAs/InP, and SiGe/Si [81] on various lowindex surfaces. The straininduced interaction among steps in superlattice wirestructures was shown to favor the ordering of step bunching [82], leading to wires with regular
7.3 Selforganized Nanostructures
303
(a)
InGaAs QWR
[001]
(c)
500 nm [110]
(b) (001) 5°
20 nm GaAs step bunch [110]
(d)
InGaAs QWR
InGaAs GaAs GaAs step bunch
Fig. 7.47 Formation of quantum wires from 3 nm thick InGaAs deposition on GaAs (001) misori¯ ented 5◦ towards [110]. a Atomic force micrograph of an In0.1 Ga0.9 As layer grown on the stepped GaAs surface; adopted from [72]. b Magnified schematic of the cross section of image (a). c Crosssection transmissionelectron micrograph and d schematic of an In0.15 Ga0.85 As layer covered by a c 1997 Elsevier thick GaAs barrier layer. Reproduced with permission from [79],
lateral spacing [81]. The formation of wire material at steps of the barrier material may be attributed to the process of stepflow growth (Sect. 7.2.4) and the lower surface energy of the wire material. Furthermore, elastic relaxation of strained wire material is enhanced at step edges. Formation of InGaAs quantum wires on a vicinal GaAs (001) surface misoriented ¯ direction is illustrated in Fig. 7.47. The vicinal GaAs surface by 5◦ towards the [110] forms step bunches of ∼6.1 nm height and 70 nm spacing running along [110]. The terraces correspond to singular (001) faces. Metalorganic vaporphase epitaxy of 3 nm thick InGaAs on this GaAs surface basically reproduces the stepped surface morphology [79]. InGaAs quantum wires form after growth of an upper GaAs barrier layer. The crosssectional TEM image Fig. 7.47c shows ∼6 nm thick quantum wires with a lateral width of ∼25 nm. The thickness of the persisting quantum well on the (001) facets is ∼1.3 nm, yielding a growth enhancement of a factor of 4 at the step edges.
7.4 Problems Chapter 7 7.1 Consider a Kossel crystal with the shape of a cube with edge length n × a, consisting of atom cubes with edge length a. (a) Determine the number of atoms Ni which differ in energy. Assume only nearestneighbor bonds and distinguish between atoms in the bulk, on the faces (but not at corners or edges), at the edges (not at a corner), and at
304
7 Atomistic Aspects of Epitaxial LayerGrowth
corners. Calculate Ni for n equals 10 and 1000, and check that the total number equals n 3 . (b) The number of bonds for the different types of atoms noted in (a) differs. With 1 bond of energy E b shared by 2 neighbored atoms, a bulk atom has an energy E = 6 × E b × 21 = 3E b . Calculate the respective energies for the different types of atoms. The contribution of atoms at the surface (= faces, corners, and edges) to the total energy E tot of all atoms decreases as the size of the crystal increases. Find the fraction of their energy contribution to E tot for n = 101 to 104 in steps by a factor of 10. Compare the result for a large number n to that obtained when only bulk and face atoms are considered. 7.2 The β2(2 × 4) reconstruction of the Asrich GaAs(001) surface contains two As dimers in the 1st (top) layer and one in the 3rd layer. The reconstruction complies with the electroncounting model similar to the missingdimer (2 × 4) surface discussed in the text (cf. Fig. 7.11). (a) Apply electron counting for the β2(2 × 4) reconstruction by listing the required and the available electrons in the topmost 4 layers, assuming dangling Ga bonds empty and dangling As bonds filled. How many electrons are involved? (b) Repeat (a) for the related Garich β2(4 × 2) reconstruction. In this surface the As atoms are exchanged for Ga atoms and vice versa, yielding two Ga dimers in the first and one in the third layer (cf. Fig. 7.11). Does the β2(4 × 2) reconstruction comply with the electroncounting rule? 7.3 The surface diffusion of Ga is the ratedetermining process in the epitaxy of GaAs under excess arsenic pressure. An experiment on the temperaturedependent surfacediffusion length λ yields the following four data points for an Arrhenius plot of λ/cm versus 1000/T/K : 5.3 × 10−6 , 1.00; 7.5 × 10−6 , 1.05; 7.0 × 10−6 , 1.20; 5.5 × 10−6 , 1.25. Assume that the diffusion length of the first two data points in the hightemperature range is solely governed by the diffusion barrier, and the latter data points also reflect a pure exponential behavior which is additionally affected by the adsorption energy. (a) Calculate the energy of the diffusion barrier and the adsorption energy. (b) Find two different temperatures where the diffusion length equals 4.0 × 10−6 cm. 7.4 We consider adatoms on a Si surface. (a) How long is the residence time of an adatom at 1000 ◦ C? Assume 2.0 eV adsorption energy and a typical atomic vibration frequency of 1013 Hz. Find the surface diffusivity, if the mean diffusion length of 4 × 10−5 cm is limited by the residence time. What is the diffusion length at 800 ◦ C, if the diffusion barrier is half the adsorption energy? (b) Stepflow growth occurs, if the surface diffusionlength exceeds well the terrace width. Find the height of a (not reconstructed) single Si(001) monolayer and the angle for a small miscut along [100] required to produce equidistant
7.5 General Reading Chapter 7
305
terraces with 200 nm width and 1 monolayer high steps. Find the rate for the advancement of the step for 1 µm/h growth rate on the Si surface. 7.5 An InAs island of pyramidal shape with 10 nm base length, bound by unreconstructed (110) side facets, is formed on a 1.40 monolayer thick wetting layer on GaAs substrate. The lattice parameter of InAs is approximately 6.1 Å. Neglect the strain in the following assessments. (a) Estimate the number of In and As atoms in the island. (b) Which thickness has the initially deposited twodimensional InAs layer before the formation of the islands, if 4 × 1010 cm−2 islands are generated? (c) What were the thickness of the initially deposited twodimensional InAs layer, if islands of the same areal density as in (b) were generated, but with a shape of a spherical cap? The diameter and contact angle of these islands are assumed to be 10 nm and 45◦ , respectively (compare to Fig. 6.10). How many In and As atoms contains one of these islands?
7.5 General Reading Chapter 7 A. Pimpinellei, J. Villain, Physics of Crystal Growth (Cambridge University Press, Cambridge, 1998) W.K. Burton, N. Cabrera, F.C. Frank, The growth of crystals and the equilibrium structure of their surfaces. Philos. Trans. R. Soc. Lond. A 243, 299–358 (1951) K. Oura, V.G. Lifshits, A.A. Saranin, A.V. Zotov, M. Katayama, Surface Science—An Introduction, 1st edn. (Springer, Berlin, 2003) H. Ibach, Physics of Surfaces and Interfaces (Springer, Berlin, 2006) F. Bechstedt, Principles of Surface Physics (Springer, Berlin 2003)
References 1. D.J. Chadi, Atomic and electronic structures of reconstructed Si(100) surfaces. Phys. Rev. Lett. 43, 43 (1979) 2. M.D. Pashley, Electron counting model and its application to island structures on molecularbeam epitaxy grown GaAs(001) and ZnSe(001). Phys. Rev. B 40, 10481 (1989) 3. W.A. Harrison, Theory of polar semiconductor surfaces. J. Vac. Sci. Technol. 16, 1492 (1979) 4. S. Yuan, L. Zhang, H. Chen, E. Wang, Z. Zhang, Generic principle for the prediction of metalinduced reconstructions of compound semiconductor surfaces. Phys. Rev. B 78, 075305 (2008) 5. E.A. Wood, Vocabulary of surface crystallography. J. Appl. Phys. 35, 1306 (1964) 6. L. Däweritz, R. Hey, Reconstruction and defect structure of vicinal GaAs(001) and and Alx Ga1−x As(001) surfaces during MBE growth. Surf. Sci 236, 15 (1990) 7. V. P. LaBella, H. Yang. D. W. Bullok, P. M. Thibado, P. Kratzer, M. Scheffler, Atomic structure of the GaAs(001)(2 × 4) surface resolved using scanning tunneling microscopy and firstprinciples theory, Phys. Rev. Lett. 83, 29892 (1999) 8. A. Ohtake, P. Kocán, J. Nakamura, A. Natori, N. Koguchi, Kinetics in surface reconstructions on GaAs(001). Phys. Rev. Lett. 92, 236105 (2004)
306
7 Atomistic Aspects of Epitaxial LayerGrowth
9. N. Moll, A. Kley, E. Pehlke, M. Scheffler, GaAs equilibrium crystal shape from first principles. Phys. Rev. B 54, 8844 (1996) 10. J.E. Northrup, S. Froyen, Structure of GaAs(001) surfaces: The role of electrostatic interactions. Phys. Rev. B 50, 2015 (1994) 11. W.G. Schmidt, S. Mirbt, F. Bechstedt, Surface phase diagram of (2 × 4) and (4 × 2) reconstructions of GaAs(001). Phys. Rev. B 62, 8087 (2000) 12. N. Chetty, R.M. Martin, Determination of integrals at surfaces using the bulk crystal symmetry. Phys. Rev. B 44, 5568 (1991) 13. A. Ohtake, Surface reconstructions on GaAs(001). Surf. Sci. Rep. 63, 295 (2008) 14. A.V. Bakulin, S.E. Kulkova, S.V. Eremeev, O.E. Tereshchenko, Abinitio study of new Garich GaAs(001) surface (4 × 4) reconstruction. Surf. Sci. 615, 97 (2013) 15. E. Penev, P. Kratzer, M. Scheffler, Atomic structure of the GaAs(001) surface: firstprinciples evidence for diversity of heterodimer motifs. Phys. Rev. Lett. 93, 146102 (2004) 16. F. Bechstedt, R. Enderlein, Semiconductor Surfaces and Interfaces (Akademie Verlag, Berlin, 1988) 17. K. Oura, V.G. Lifshits, A.A. Saranin, A.V. Zotov, M. Katayama, Surface Science: An Introduction (Springer, Berlin, 2003) 18. K. Takayanagi, Y. Tanishiro, S. Takahashi, M. Takahashi, Structure analysis of Si(111)7 × 7 reconstructed surface by transmission electron diffraction. Surf. Sci. 164, 367 (1985) 19. K.D. Brommer, M. Needels, B.E. Larson, J.D. Joannopoulos, Ab initio theory of the Si(111)(7 × 7) surface reconstruction: a challenge for massively parallel computation. Phys. Rev. Lett. 68, 1355 (1992) 20. R.S. Becker, J.A. Golovchenko, G.S. Higashi, G.S. Swartzentruber, New reconstructions on Silicon (111) surfaces. Phys. Rev. Lett. 57, 1020 (1986) 21. W. K. Burton, N. Cabrera, F. C. Frank, The growth of crystals and the equilibrium structure of their surfaces, Phil. Trans. R. Soc. Lond. A 243, 299 (1951) 22. J.A. Venables, G.D.T. Spiller, M. Hanbrücken, Nucleation and growth of thin films. Rep. Prog. Phys. 47, 399 (1984) 23. J.A. Venables, Rate equation approaches to thin film nucleation kinetics. Phil. Mag. 27, 693 (1973) 24. T. Shitara, T. Nishinaga, Surface diffusion length of gallium during MBE growth on the various misoriented GaAs(001) substrates. Jpn. J. Appl. Phys. 28, 1212 (1989) 25. I. Bryan, Z. Bryan, S. Mita, A. Rice, J. Tweedie, R. Collazo, Z. Sitar, Surface kinetics in AlN growth: A universal model for the control of surface morphology in IIInitrides. J. Crystal Growth 438, 81 (2016) 26. S.V. Ghaisas, A. Madhukar, Role of surface molecular reactions in the growth mechanism and the nature of nonequilibrium surfaces: a Monte Carlo study of molecularbeam epitaxy. Phys. Rev. Lett. 56, 1066 (1986) 27. A. Madhukar, S.V. Ghaisas, The nature of molecular beam epitaxial growth examined via computer simulations, CRC Crit. Rev. Solid State Mater. Sci. 14, 1 (1988) 28. G. Ehrlich, F.G. Hudda, Atomic view of surface selfdiffusion: tungsten on tungsten. J. Chem. Phys. 44, 1039 (1966) 29. R.L. Schwoebel, E.J. Shipsey, Step Motion on Crystal Surfaces. J. Appl. Phys. 37, 3682 (1966) 30. J. Myslivecek, C. Schelling, G. Springholz, F. Schaffler, B. Voigtländer, P. Smilauer, On the origin of the kinetic growth instability of homoepitaxy on Si(001). Mater. Sci. Eng. B 89, 410 (2002) 31. A.L.S. Chua, E. Pelucchi, A. Rudra, B. Dwir, E. Kapon, A. Zangwill, D.D. Vvedensky, Theory and experiment of step bunching on misoriented GaAs(001) during metalorganic vaporphase epitaxy. Appl. Phys. Lett. 92, 013117 (2008) 32. A. Gocalinska, M. Manganaro, E. Pelucchi, D.D. Vvedensky, Surface organization of homoepitaxial InP films grown by metalorganic vaporphase epitaxy. Phys. Rev. B 86, 165307 (2012) 33. X.Q. Shen, H. Okumura, Surface step morphologies of GaN films grown on vicinal sapphire (0001) substrates by RFMBE. J. Crystal Growth 300, 75 (2007)
References
307
34. K. Bellmann, U.W. Pohl, C. Kuhn, T. Wernicke, M. Kneissl, Controlling the morphology transition between stepflow growth and stepbunching growth. J. Crystal Growth 478, 187 (2017) 35. G. S. Bales, A. Zangwill, Morphological instability of a terrace edge during stepflow growth, Phys. Rev. B 41„ 5500 (1990). Erratum referring to one equation cf. G. S. Bales, A. Zangwill, Phys. Rev. B 48, 2024 (1993) 36. A. Pimpinelli, J. Villain, Physics of Crystal Growth (Cambridge University Press, Cambridge, UK, 1998) 37. O. PierreLouis, M.R. D’Orsogna, T.L. Einstein, Edge diffusion during growth: the KinkEhrlichSchwoebel effect and resulting instabilities. Phys. Rev. Lett. 82, 3661 (1999) 38. M. V. Ramana Murty, B. H. Cooper, Instability in molecular beam epitaxy due to fast edge diffusion and corner diffusion barriers, Phys. Rev. Lett. 83, 352 (1999) 39. D.J. Chadi, Stabilities of singlelayer and bilayer steps on Si(001) surfaces. Phys. Rev. Lett. 59, 1691 (1987) 40. B.S. Schwartzentruber, Y.W. Mo, R. Kariotis, M.G. Lagally, M.B. Webb, Direct determination of Step and kink energies on vicinal Si(001). Phys. Rev. Lett. 65, 1913 (1990) 41. R.G.S. Pala, S. Liu, Critical Epinucleation on reconstructured surfaces and firstprinciple calculation of homonucleation on Si(100). Phys. Rev. Lett. 95, 136106 (2005) 42. B. Voigtländer, M. Kästner, P. Smilauer, Magic islands in Si/Si(111) homoepitaxy. Phys. Rev. Lett. 81, 858 (1998) 43. W. Shimada, H. Tochihara, Stepstructure dependent stepflow: models for the homoepitaxial growth at the atomic steps on Si(111)7 × 7. Surf. Sci. 311, 107 (1994) 44. H. Tochihara, W. Shimada, The initial process of molecular beam epitaxial growth of Si on Si(111)7 × 7: a model for the destruction of the 7 × 7 reconstruction. Surf. Sci. 296, 186 (1993) 45. S. Filimonov, V. Cherepanov, Y. Hervieu, B. Voigtländer, Multistage nucleation of twodimensional Si islands on Si(111)7 × 7 homoepitaxy during MBE growth. Phys. Rev. B 76, 035428 (2007) 46. M. Itoh, G.R. Bell, B.A. Joyce, D.D. Vvedensky, Transformation kinetics of homoepitaxial islands on GaAs(001). Surf. Sci. 464, 200 (2000) 47. P. Kratzer, M. Scheffler, Reactionlimited island nucleation in molecular beam epitaxy of compound semiconductors. Phys. Rev. Lett. 88, 036102 (2002) 48. C.T. Foxon, B.A. Joyce, Interaction kinetics of As2 and Ga on 100 GaAs surfaces. Surf. Sci. 64, 293 (1977) 49. P. Kratzer, C.G. Morgan, M. Scheffler, Densityfunctional theory studies on microscopic processes of GaAs growth. Prog. Surf. Sci. 59, 135 (1998) 50. E.S. Tok, J.H. Neave, J. Zhang, B.A. Joyce, T.S. Jones, Arsenic incorporation kinetics in GaAs(001) homoepitaxy revisited. Surf. Sci. 374, 397 (1997) 51. A. Kley, P. Ruggerone, M. Scheffler, Novel diffusion mechanism on the GaAs(001) surface: The role of adatomdimer interaction. Phys. Rev. Lett. 79, 5278 (1997) 52. P. Kratzer, C.G. Morgan, M. Scheffler, Model for the nucleation in GaAs homoepitaxy derived from first principles. Phys. Rev. B 59, 15246 (1999) 53. V.A. Shchukin, N.N. Ledentsov, P.S. Kop’ev, D. Bimberg, Spontaneous ordering of arrays of coherent strained islands. Phys. Rev. Lett. 75, 2968 (1995) 54. L.G. Wang, P. Kratzer, M. Scheffler, N. Moll, Formation and stability of selfassembled coherent islands in highly mismatched heteroepitaxy. Phys. Rev. Lett. 82, 4042 (1999) 55. G.H. Lu, M. Cuma, F. Liu, Firstprinciples study of strain stabilization of Ge(105) facet on Si(001). Phys. Rev. B 72, 125415 (2005) 56. N. Moll, M. Scheffler, E. Pehlke, Influence of surface stress on the equilibrium shape of strained quantum dots. Phys. Rev. B 58, 4566 (1998) 57. A. Rastelli, M. Kummer, H. Von Känel, Reversible shape evolution of Ge islands on Si(001). Phys. Rev. Lett. 87, 256101 (2001) 58. J. Márquez, L. Geelhaar, K. Jacobi, Atomically resolved structure of InAs quantum dots. Appl. Phys. Lett. 78, 2309 (2001)
308
7 Atomistic Aspects of Epitaxial LayerGrowth
59. T. Xu, L. Zhou, Y. Wang, A.S. Özcan, K.F. Ludwig, GaN quantum dot superlattices grown by molecular beam epitaxy at high temperature. J. Appl. Phys. 102, 073517 (2007) 60. M. Pinczolits, G. Springholz, G. Bauer, Direct formation of selfassembled quantum dots under tensile strain by heteroepitaxy of PbSe on PbTe (111). Appl. Phys. Lett. 73, 250 (1998) 61. S. Ruvimov, P. Werner, K. Scheerschmidt, U. Gösele, J. Heydenreich, U. Richter, N.N. Ledentsov, M. Grundmann, D. Bimberg, V.M. Ustinov, AYu. Egorov, P.S. Kop’ev, ZhI Alferov, Phys. Rev. B 51, 14766 (1995) 62. Y. Nabetani, T. Ishikawa, S. Noda, A. Sasaki, Initial growth stage and optical properties of a threedimensional InAs structure on GaAs. J. Appl. Phys. 76, 347 (1994) 63. D. Leonard, K. Pond, P.M. Petroff, Critical layer thickness for selfassembled InAs islands on GaAs. Phys. Rev. B 50, 11687 (1994) 64. I. Daruka, J. Tersoff, A.L. Barabási, Shape transition in growth of strained islands. Phys. Rev. Lett. 82, 2753 (1999) 65. G. Costantini, A. Rastelli, C. Manzano, P. AcostaDiaz, R. Songmuang, G. Katsaros, O.G. Schmidt, K. Kern, Interplay between thermodynamics and kinetics of InAs/GaAs(001) quantum dots. Phys. Rev. Lett. 96, 226106 (2006) 66. H. Eisele, A. Lenz, R. Heitz, R. Timm. M. Dähne, Y. Temko, T. Suzuki, K. Jacobi, Change of InAs/GaAs quantum dot shape and composition during capping, J. Appl. Phys. 104, 124301 (2008) 67. U.W. Pohl, K. Pötschke, A. Schliwa, F. Guffarth, D. Bimberg, N.D. Zakharov, P. Werner, M.B. Lifshits, V.A. Shchukin, D.E. Jesson, Evolution of a multimodal distribution of selforganized InAs/GaAs quantum dots. Phys. Rev. B 72, 245332 (2005) 68. G. Costantini, A. Rastelli, C. Manzano, R. Songmuang, O.G. Schmidt, K. Kern, H. von Känel, Universal shapes of selforganized semiconductor quantum dots: Striking similarities between InAs/GaAs(001) and Ge/Si(001). Appl. Phys. Lett. 85, 5674 (2004) 69. V.A. Shchukin N.N. Ledentsov, D. Bimberg, Entropy effects in selforganized formation of nanostructures, in NATO Advanced Workshop on Atomistic Aspects of Epitaxial Growth, ed. by M. Kortla et al. (Kluwer, Dordrecht, 2002) 70. V.A. Shchukin, N.N. Ledentsov, D. Bimberg, Epitaxy of Nanostructures (Springer, Berlin, 2004) 71. M. Meixner, E. Schöll, V.A. Shchukin, D. Bimberg, Selfassembled quantum dots: Crossover from kinetically controlled to thermodynamically limited growth. Phys. Rev. Lett. 87, 236101 (2001) 72. X.L. Wang, V. Voliotis, Epitaxial growth and optical properties of semiconductor quantum wires. J. Appl. Phys. 99, 121301 (2006) 73. T. Takebe, M. Fujii, Y. Yamamoto, K. Fujita, T. Watanabe, Orientationdependent Ga surface diffusion in molecular beam epitaxy of GaAs on GaAs patterned substrates. J. Appl. Phys. 81, 7273 (1997) 74. A. Gustafsson, F. Reinhardt, G. Biasiol, E. Kapon, Lowpressure organometallic chemical vapor deposition of quantum wires on Vgrooved substrates. Appl. Phys. Lett. 67, 3673 (1995) 75. R. Bhat, E. Kapon, D.M. Hwang, M.A. Koza, C.P. Yun, Patterned quantum well heterostructures grown by OMCVD on nonplanar substrates: Applications to extremely narrow SQW lasers. J. Crystal Growth 93, 850 (1988) 76. S. Koshiba, N. Noge, H. Akiyama, T. Inoshita, Y. Nakamura, A. Shimizu, Y. Nagamune, M. Tsuchiya, H. Kano, H. Sasaki, Formation of GaAs ridge quantum wire structures by molecular beam epitaxy on patterned substrates. Appl. Phys. Lett. 64, 363 (1994) 77. T. Sato, I. Tamai, H. Hasegawa, Growth kinetics and modeling of selective molecular beam epitaxial growth of GaAs ridge quantum wires on prepatterned nonplanar substrates. J. Vac. Sci. Technol. B 22, 2266 (2004) 78. G. Biasiol, A. Gustafsson, K. Leifer, E. Kapon, Mechanisms of selfordering in nonplanar epitaxy of semiconductor nanostructures. Phys. Rev. B. 65, 205306 (2002) 79. S. Hara, J. Motohisa, T. Fukui, Formation and characterization of InGaAs strained quantum wires on GaAs multiatomic steps grown by metalorganic vapor phase epitaxy. J. Crystal Growth 170, 579 (1997)
References
309
80. S. Hara, J. Motohisa, T. Fukui, H. Hasegawa, Quantum well wire fabrication method using selforganized multiatomic steps on vicinal (001) GaAs surfaces by metalorganic vapor phase epitaxy. Jpn. J. Appl. Phys. 34, 4401 (1995) 81. K. Brunner, Si/Ge nanostructures. Rep. Progr. Phys. 65, 27 (2002) 82. L. Bai, J. Tersoff, F. Liu, Selforganized quantumwire lattice via step flow growth of a shortperiod superlattice. Phys. Rev. Lett. 92, 225503 (2004)
Chapter 8
In Situ Growth Analysis
Abstract Sensors to analyse layer structures already during epitaxial growth provide valuable information for developing device structures and for ensuring the reproducibility of runtorun conditions. Most analytical online tools are applicable to all major growth techniques. Today a variety of probes is routinely integrated into growth systems for monitoring in situ sample temperature, growth rate, layer thickness, composition, strain, and other parameters of the growth process. Sensors measure either the ambient in the vicinity of the growing sample or the sample surface. Ambient analysis comprises mass spectrometry and optical probes; they provide information about the mass transport, the kind and density of species, their temperature, and potential mutual reactions. Surface probes include diffraction techniques and various optical tools. Surface sensitivity for diffraction is achieved by applying grazingincidence angles, and the diffracted electron and Xray beams disclose the surface morphology and reconstructions. Optical probes are widely applied in gaseous growth ambient. The selectivity for the surface may strongly be enhanced by taking advantages of symmetryrelated surface properties, and several optical probes can resolve the growth of single monolayers. The chapter describes prominent techniques for in situ analysis of epitaxy. After discussing ambient analysis using mass spectrometry and optical spectroscopy, surface probes are considered. Structural analysis by reflection highenergy electron diffraction and by Xray diffraction is outlined, and optical probes by pyrometry and deflectometry yielding data on temperature and strain are presented. The text then focuses on reflectometry, ellipsometry, and reflectancedifference spectroscopy (reflectanceanisotropy spectroscopy); these techniques provide both chemical and structural information.
8.1 Surface and Ambient Probing Semiconductor devices consist of many epitaxial layers with different composition. The demand to control the perfection of growth in situ, i.e., already during epitaxy, led to the development of various analytical tools. Some of these sensors are today routinely integrated into commercial growth systems and allow for online monitoring
© Springer Nature Switzerland AG 2020 U. W. Pohl, Epitaxy of Semiconductors, Graduate Texts in Physics, https://doi.org/10.1007/9783030438692_8
311
312
8 In situ Growth Analysis
of sample temperature, composition, growth rate, strain, and other parameters of the growth process. There are mainly two different kinds of probes for in situ monitoring: electrons and photons. Using these probes either the ambient near the sample or the sample surface is monitored during growth. To achieve sufficient sensitivity for the small interaction volume of the probe with the surface, the penetration depth into the sample should be small. This condition is well fulfilled for electrons with a low energy as depicted in Fig. 8.1a; the given mean free path λ is largely independent of the material; a least squares analysis of data in Fig. 8.1a shows that the measurements for energies below 15 eV are described by a power law near E −2 and those above 75 eV by E 1/2 , the solid line is a fit to λi = ai E −2 + bi E 1/2 . The universal behavior makes electron diffraction an ideal tool for obtaining structural information on the surface. This is routinely applied in vacuumbased deposition techniques (Sect. 8.3.1). In the environment of vaporphase deposition electron probes cannot be used due to absorption in the gas phase, but photons in the visible spectral range can penetrate the gas phase. A drawback of light is its comparably large penetration depth as illustrated in Fig. 8.1b, yielding a dominant contribution from the bulk when simple optical techniques like reflectometry are applied. Surface sensivity can be preserved when polarization effects or specific properties of the surface are utilized. Such optical probes are discussed in Sect. 8.4. In addition to electrons or photons also other in situ probes are applied. A prominent technique is mass spectrometry, mainly used for analysing vacuum conditions. Direct information on surface morphology is obtained from in situ scanning probe microscopy, implemented in a specially designed growth setup. In situ probing techniques were generally developed for ex situ analyses, and often the application in a growth apparatus requires some modification to provide access
Electrons
Photons ZnSe
GaAs
Energy (eV)
(b) Light penetration depth (nm)
Inelastic mean free path (nm)
(a)
Energy (eV)
Fig. 8.1 a Inelastic mean free path of electrons in solids. b Penetration depth of light in GaAs and ZnSe. Reproduced with permission from [1, 2], © 1979 Wiley and 1996 Springer, respectively
8.1 Surface and Ambient Probing
313
to the sample surface or its environment. Still most of the widely applied probes have negligible impact on the growth process; a survey of in situ probes is given in Table 8.1. The instrumentation of a growth apparatus with in situ sensors depends on the growth method and the material to be grown. Virtually any chamber for molecular beam epitaxy is equipped with RHEED and QMS, often also with pyrometry and reflectometry. Vaporphase methods like MOVPE usually employ reflectometry and pyrometry. Pyrometers in commercial MOVPE reactors are today integrated into a closedloop temperature control, and reflectometry is often applied for online correction of the growth rate. In the epitaxy of nitrides additionally deflectometry is routinely applied. In situ sensors employed in production of devices also monitor the compliance with specifications within certain tolerance levels, thereby increasing yield and reducing down times; often a fingerprint record of the sensor signal is sufficient to keep constant runtorun growth conditions. On the other hand, growth Table 8.1 Techniques for in situ analyses of epitaxial growth Probes
Acronym
Information
RHEED
Surface geometry
Probes using electrons Reflection high energy electron diffraction Probes using photons Deflectometry
Strain, composition
Pyrometry
Surface temperature
Reflectometry
Growth rate, layer thickness, optical constants, composition
Spectroscopic ellipsometry
SE
Optical constants, strain, layer thickness, composition
Reflectance difference/anisotropy spectroscopy
RDS, RAS
Surface and interface anisotropy, reconstructions
Raman scattering, coherent antiStokes Raman scattering
RS, CARS
Species, strain
Grazing incidence Xray scattering/reflection
GIXS, GIXR
Surface structure, layer thickness
Surface photo absorption, ppolarized reflectance spectroscopy
SPA, PRS
Surface coverage
Laser light scattering
LLS
Macroscopic surface irregularities
Second harmonic generation
SHG
Surface symmetry
Laserinduced fluorescence (LIF), LIF spectroscopy
LIF, LIFS
Ambient species, partial pressure
Quadrupole mass spectrometry
QMS
Ambient species, partial pressure
Scanning tunneling microscopy
STM
Surface structure
Atomic force microscopy
AFM
Surface structure
Other probes
314
8 In situ Growth Analysis
systems used in research are often equipped with additional and specialized sensors, and the signals are carefully analyzed to achieve an insight into the growth process.
8.2 In Situ Ambient Analysis Sensors measure either the (surfacenear) sample ambient or the sample surface. In the following we discuss some widely applied methods for ambient monitoring. Analysis of the ambient in the vicinity of the growing sample provides information about the mass transport, i.e., about the species moving toward the surface and those desorbing into the ambient. Besides the identification of the species and their density also their temperature, hydrodynamics, and potential reactions may be disclosed, thereby offering valuable insights into the growth process.
8.2.1 Quadrupole Mass Spectrometry Mass spectrometry is routinely employed in vacuum systems for detecting leakage and contaminations. The application in ambient monitoring requires a high resolution of masses to distinguish fragments of species, detection up to high masses, and differential pumping to provide the high vacuum for the detector; generally quadrupole mass spectrometry (QMS) is employed ambient analysis by QMS was applied in both molecular beam epitaxy (MBE) and (metalorganic) vapor phase epitaxy (VPE, MOVPE); studies focusing on desorption are also referred to as desorption mass spectrometry. Mass spectrometry in MBE benefits from the UHV conditions in the growth chamber. By applying a lineofsight configuration the mass spectrometer is sensitive only to particles emitted from the sample surface; this is achieved by appropriate apertures with cryopumping walls, such that the line of sight is established only between a small patch on the sample surface and the ionization volume in the QMS [3, 4]. The flux of species incident on the surface can be identified and monitored as well; for this purpose an inert surface is used, or the experimental surface is made inert. The number of particles within the ionization volume of lineofsight QMS is small due to the geometry with two apertures defining the line of flight; this requires the use of a secondary electron multiplier within the mass spectrometer. An example for the application of QMS to the MBE of GaN is given in Fig. 8.2. The UHV conditions of MBE leads to GaN growth in a thermodynamically metastable regime; deposition must hence overcompensate desorption. Figure 8.2a shows the temperature dependence of Ga desorbing from a GaN (0001) surface in vacuum [5]. Preceding calibration was performed by measuring the 69 Ga partial pressure for various Ga fluxes evaporated onto sapphire, which was kept at very high temperature to ensure that all impinging Ga desorbs; this yields a linear relation of 2.53×10−10 mbar/monolayer s−1 [6], used to scale Ga desorption in units of 1 nm/min; the measured Ga flux provides directly the GaN decomposition rate due to congruent
8.2 In Situ Ambient Analysis
315 T (°C)
GaN (0001) Vacuum
Desorbing Ga flux (nm/min)
4
805°C
(a)
3
2
780°C 760°C
1 740°C
GaN decomposition rate (nm/min)
820
800
780
760
740
720
(b) EA= 3.1 eV
QMS RHEED
720°C 0
0
400 t (s)
800 1/(kB T ) (eV)
Fig. 8.2 a Ga flux desorbing from heated GaN in vacuum at various temperatures. b Decomposition rate of GaN as derived from the data in (a) and additional RHEED measurements as a function of T −1 ; reproduced with permission from [5], © 2008 AIP
decomposition of GaN in vacuum. The Arrhenius plot Fig. 8.2b of the measured flux data for the GaN decomposition yields an activation energy of (3.1 ± 0.1) eV, also obtained from the simultaneously measured RHEED oscillations originating from a layerbylayer decomposition in this experiment. The same QMS technique was applied to confirm experimentally [6] the theoretically predicted existence of a Ga double layer on a Gapolar (0001) face forming under Garich conditions [7]. This metallic surface proved to be important for the epitaxy of smooth GaN layers [8]. Mass spectrometry in MOVPE is more demanding due to the high ambient pressure (typically 20–100 mbar from the carrier gas) and the large number of different species. Analysis of the gas composition behind the reactor yields results from a gas composition, which is not representative for the hot zone at the sample due to reactions during cooling. Therefor a gas probe is ingested in vicinity of the sample surface by a capillary [9, 10] or, in an early experiment, via a small orifice in the sample susceptor [11]; the latter arrangement yields a short sample path length, so that shortlived reactive species like free radicals are not removed by wall reactions and gasphase recombination reactions. This provides the most realistic pattern of the growth ambient. In the 1990s mass spectrometry and gasphase spectroscopy were important means to study the pyrolysis reactions of MOVPE sources in the ambient, taking the frequently coupled pyrolysis pathways for both the cation and anion precursor molecules in the MOVPE of compound semiconductors into account [12, 13]. Since implementation of mass spectrometry in a MOVPE reactor requires a major modification, most of these studies were performed in an ersatz reactor, i.e., a thin heated flow tube, which
316
8 In situ Growth Analysis
quite roughly represents the hot zone of the reactor and neglected transport phenomena of a MOVPE reactor; they still helped finding the standard precursors routinely used today. Mass spectrometry of tertiarybutylphosphine (TBP, (C4 H9 )PH2 ) in D2 flowtube ambient is shown in Fig. 8.3a; the standard H2 carrier gas was replaced by D2 in order to label the products and to distinguish reactions among reactants and those with the ambient [14]. We observe the decrease of TBP as the temperature or the partial pressure increases, accompanied by the production of C4 H8 , C4 H10 , H2 , and PH3 from the pyrolysis. At higher TBP partialpressure the ratio of isobutene C4 H8 and isobutane C4 H10 is reversed; this indicates a prevailing transition from a unimolecular pyrolysis by bond cleavage (C4 H9 )PH2 → (C4 H9 )• + •PH2 and (C4 H9 )• → (C4 H8 ) + H• at low partial TBP pressure, to a bimolecular reaction (C4 H9 )• + (C4 H9 )PH2 → HC4 H9 + (C4 H9 )PH at high pressure, where a tertiarybutyl radical (C4 H9 )• removes a H from TBP [13, 14]. Pyrolysis of the nitrogen sources tertiarybutylhydrazine (TBHy, (C4 H9 )NNH2 ) and dimethylhydrazine (DMHy, (CH3 )2 NNH2 ) in a flow tube is shown in Fig. 8.3b; the given mass peak intensities of the undecomposed molecules (TBHy+ , DMHy+ ) decrease at increasing temperature under production of products indicating a dominating N–N bond cleavage for both molecules; some detected masses such as (a) TBP
6
(b) TBHy a
TBP 7.6 mbar
7
+ +
H22NNH m32 H NNH22 m32
C 4H8
Partial pressure (mbar)
H2
3
PH3
2 C4H10
1
HD
0
1E8
TBP 42.4 mbar
40 TBP
30
1E9
20 10 0 350
DMHy b ++ H H22CN CN m28 m28 +
Mol DMHy++m60 m60
++
NH m17 NH33 m17
NH NH22+ m16 m16 + m44 (CH (CH33))22NN+m44 +
+ m32 H2NNH H 2 2 m32 2NNH H2
450
+
NH2+ m16 NH 2 m16 + + TBHy/CH Mol/CH3 3
x8
CH++ m13 m13 CH
PH3 400
Mol TBHy+m88 m88
C 4H8
C4H10
+
+ (CH CNH22 (CH33))32CNH
+
4
Ion Count count Rate rate (arb. units) Ion (arb. units)
5
+
+ NH NH33 m17 m17
x0.5
500
Temperature (°C)
HD 550
0
0
100
200
300
400
500
Temperature (°C)
Fig. 8.3 a Temperaturedependent partial pressure of TBP and pyrolysis products measured using mass spectrometry. b Peak intensities in the temperaturedependent mass spectra of TBHy and DMHy. Reproduced with permission from [14, 15], © 1989 Springer and 1999 Elsevier, respectively
8.2 In Situ Ambient Analysis
80 TBAs m134
TBAs 1.7 103 mbar
Intensity (arb. units)
Fig. 8.4 Decomposition of TBAs measured using iontrap mass spectrometry. Reproduced with permission from [10], © 2018 Springer Nature
317
•C4H9 m57
10
C4H10 m58
1 C4H8 m56 100
300 200 Temperature (°C)
400
500
H2 NNH2 + or TBHy/CH3 + , which follow the abundance of the mol peak, originate from fragmentation in the mass spectrometer [15]. In a more recent study of tertiarybutylarsine (TBAs, (C4 H9 )AsH2 ) pyrolysis a sensitive iontrap mass spectrometer was fed by a nozzle in an MOVPE reactor to probe the gas phase in an epitaxial environment and largely avoid fragmentation by ionization [10]. The results given in Fig. 8.4. provide evidence for the •C4 H9 production by both thermal TBAs decomposition and some fragmentation. The production of C4 H10 preceding that of C4 H8 similar to the finding with TBP indicates the existence of two pathways of TBAs decomposition: a free radical process generating C4 H10 and a βH elimination process producing C4 H8 [11, 16, 17].
8.2.2 Optical Ambient Probing Optical characterization of the environment near the growing sample is of particular importance in gaseous ambient due to the strong interaction of particles in the gas phase and related reactions. Such interactions do not occur in molecular beams of vacuumbased epitaxy such as MBE and related techniques, where the growth species are given by the flux emitted from the source cells; they can be well measured using mass spectrometry. Optical access to the reaction zone is generally provided by windows or fibre ports, purged by carrier gas or inert gas to prevent deposition. An important aspect of gasphase growth is hydrodynamics in the reactor. In the early days of reactor development in the 1980s laser doppler anemometry (LDA) was
318
8 In situ Growth Analysis
used to measure the velocity of gaseous particles. In these studies the actual molecules were replaced by micrometersized particles (TiO2 ), and the Doppler shift of laser radiation scattered from the focus by Mie scattering was measured. An introduction to LDA is given in [18], application to MOVPE reactors is reviewed in [2]; for a visualization of the particle flow see Fig. 11.16a. Today a realistic insight into transport phenomena in the reaction zone (including major chemical reactions) is achieved by advanced modelling, and LDA measurements in MOVPE reactors were recently no longer applied. Optical spectroscopy of molecules and atoms in the gas phase may identify species and roughly respective concentrations by observing electronic or vibronic transitions. Electronic transitions mostly occur in the ultraviolet and visible spectral range and can be probed by absorption or fluorescence spectroscopy. Vibrational excitations are either measured using Raman or infrared spectroscopy. The analysis is usually limited by the sensitivity for the detection of species with low concentration. Most optical in situ studies of the growth ambient were made in the 1980s and 1990s, when MOVPE was established as growth technique for mass production of (opto) electronic devices. We briefly point out some features of these investigations. Absorption spectroscopy requires a comparably simple setup. Electronic transitions may be observed using a single pass through the growth ambient, while the smaller absorption constants of vibrational transitions usually require a multipass configuration. Ultraviolet absorption spectroscopy was most popular for measuring gasphase concentrations, with an emphasis on alkyl and hydride precursors used in the MOVPE of arsenides [19, 20], phosphides [21], and nitrides [22]. Applying Beer’s law I /I0 = exp(−σ cl),
(8.1)
with the absorption coefficient σ , the concentration c, and the absorption pathlength l, the partial pressure of the species can be measured. In a multicomponent mixture the spectrally broad absorption bands must carefully be analyzed to obtain pure component partial pressures. Spectral selection is more convenient in the IR range, and the photon energies are too low to cause photolysis. Monitoring the IR absorption of In, Ga, Al akyls, and AsH3 near 2 … 3 μm in an ersatz reactor, effects of gas dynamics and chemistry were monitored online [23]. Measurement of species concentrations yielded precursor decomposition and reaction products, and transients measured velocities and diffusion effects. Besides conventional absorption spectroscopy also Fourier transform IR spectroscopy was applied, achieving reasonably low detection limits [24]. Most metalorganic precursors comprise C–H bonds; the stretching oscillation of this bond produces an absorption peak near 3.4 μm. Using this absorption also simple singlechannel (i.e., nondispersive) spectroscopy was applied for monitoring gas concentrations [25], albeit also other frequencies were used, e.g., for monitoring biscyclopentadienyl magnesium (Cp2 Mg), the standard ptype dopant source for GaN [26].
8.2 In Situ Ambient Analysis
319
Raman spectroscopy benefits from a high spatial resolution, and signals from vibrational modes are specific for each species; in addition, the temperature of molecules is directly obtained from the occupation of rotational states. A drawback is the low sensitivity of the technique to species with low partial pressure such as decomposition products. The decomposition of trimethylindium (TMIn, In(CH3 )3 ) with products of monomethylindium and indium, measured using Raman spectroscopy, is shown in Fig. 8.5. When approaching the heated susceptor (decreasing distance d) we observe a decrease of the TMIn signal, accompanied by increasing signals of In and monomethylindium; the latter decreases at smaller distances (spectra not shown in the figure). Laserinduced fluorescence (LIF or LIFS, LIF spectroscopy) is a further optical technique for ambient measurement. A tunable laser selectively excites electronic transitions of molecules or atoms in the gasphase, and the resulting fluorescence is analyzed. The method provides a high spatial, spectral, and (for pulsed excitation) temporal resolution. It is very sensitive for the detection of small molecules or atoms with a high quantum yield, while large molecules produce substantially smaller yield due to nonradiative relaxation or photo dissociation. Laserinduced fluorescence was widely used for monitoring processes in chemical vapor deposition (CVD) and etching [28]; there are, however, only few reports on applications in epitaxy, e.g. [29, 30]. Fig. 8.5 Decomposition of trimethylindium measured using Raman spectroscopy. Reproduced with permission from [27], © 2002 RSC Publishing
T (°C) 488
0.03
330 InCH3
214
120
70
In(CH3)3 d
In
(mm) 2.9
Mole fraction (arb. units)
3.9
In
4.9
400
0.02
InCH3
450 500 2200 Raman shift (cm1)
2230
In(CH3)3
0.01
0.00 0
8 2 4 6 Distance d from susceptor (mm)
10
320
8 In situ Growth Analysis
8.3 SurfaceSensitive Diffraction Techniques The structure of the surface during epitaxial growth can be best characterized by applying diffraction techniques. Waves of electrons and Xrays yield minimum perturbation of growth conditions and provide informations on the arrangement of atoms. Conditions for the diffraction of Xrays were discussed in Sect. 2.5; they also apply for electron diffraction, which is more widely used in vacuumbased growth. While the description in Sect. 2.5 focused on bulk diffraction, in situ monitoring of growth requires probes sensitive only to the structure of the surface. This sensivity is obtained for electrons by either using low energies (cf. Fig. 8.1a) or by applying grazing angles of incidence; the latter technique also allows for using Xrays, which otherwise have a large penetration depth in solids. The diffraction of electrons with low energies yields precise informations on the surface structure. Low energy electron diffraction (LEED) is a powerful standard technique in surface science [31]. A serious drawback of the somewhat bulky LEED setup is, however, the mounting in front of the sample; thereby the path for molecular beams in MBE is blocked. LEED is therefor not applied in MBE and related vacuumbased epitaxy, and we focus on the deployed methods based on grazing incidence.
8.3.1 Reflection HighEnergy Electron Diffraction (RHEED) The diffraction of electrons with a very shallow (grazing) incidence angle is a standard method in any MBE apparatus, and is also well established in sample preparation for surface studies [32, 33]. The technique is compatible with vacuum, nonintrusive, and simple. Moreover, in MBE the RHEED assembly does not disturb the arrangement of the Knudsen cells opposite to the wafer, see Fig. 11.21. Electrons with an energy of 5–50 keV are directed to the surface at a low angle ( 0.20, and the initially varied slope of the x = 0.36 trajectory reveals that the target composition in this deposition is only reached after growing 15 Å of AlGaAs.
8.4.4 ReflectanceDifference Spectroscopy Reflectancedifference spectroscopy (RDS), also referred to as reflectanceanisotropy spectroscopy (RAS), measures the difference of normalincidence reflectivity with polarizations oriented along two principal axes. In solids with optically isotropic bulk this technique is very surface sensitive, because light reflected in normal incidence from such a bulk can basically not depend on polarization, i.e., the light probes the anisotropy of the surface. This anisotropy originates essentially from surface reconstructions, which usually form dimer bonds along specific directions to minimize the total energy (Sects. 7.1.3 and 7.1.4). An anisotropic surface geometry leads to an anisotropic probability for optical transitions involving electronic surface states, and consequently to a response in the difference of respective RDS reflectivities. The technique was introduced in the 1980s [68] and is widely applied for in situ monitoring of the epitaxial growth of cubic semiconductors, such as zincblende III–V and II–VI compound semiconductors; for reviews see [60, 69]. For zincblende semiconductors the two principal polarization axes x and y of a (001) surface are ¯ given by the 110 and [110] directions. There are various configurations of RDS systems discussed in more detail in [60]; the schematic of a phasemodulated RDS setup is given in Fig. 8.16. The beam of a white light source is linearly polarized by a polarizer and directed onto the sample at near normal incidence. The reflected light is generally elliptically polarized; its state of polarization is analyzed by a photoelastic modulator with a high modulation frequency (typ. 50 kHz) and an analyzer, which converts the phase modulation generated by the modulator into an intensity modulation. This light is dispersed in a monochromator and detected. The optical response of the sample can be described by introducing an anisotropic surface layer (overlayer) with a surface dielectric constant εo in addition to the bulk dielectric constant εb . The normalincidence RDS response is then given by [70] r˜x − r˜y ˜r do ε˜ o,x − ε˜ o,y = = 2πi , r˜ (˜r x + r˜y )/2 λ/2 ε˜ b − 1
(8.24)
336
8 In situ Growth Analysis
[110]
Analyzer 45°
Monochromator and detector
45°
Photoelastic modulator
[110] 45°
Sampl e
State of polarization
0° Polarizer
Light source Fig. 8.16 Schematic of a setup for reflectancedifference spectroscopy on the (001) surface of a sample with cubic crystal structure
where i is the imaginary unit and do λ is the thickness of the anisotropic overlayer. The actually measured quantity is the real part of (8.24), i.e., for zincblende semi , which is often simply written conductors Re 2 r˜[110 ¯ ] − r˜[110] / r˜[110 ¯ ] + r˜[110] r/r; the imaginary part is usually not measured. Typical RDS signals are on the order of 10−3 . The interpretation of RDS spectra is complicated by the fact that the bulk also contributes to the RDS response. This occurs not only due to buried interfaces within the penetration depth of the light or due to imperfections such as an unbalanced density of α and β 60° dislocations and their related strain [71] or alloy ordering in the bulk [72]. Even in the ideal case transitions between surfaceperturbed bulk states contribute strongly to RDS spectra near criticalpoint energies of the band structure as shown by calculated spectra given in Fig. 8.17. The spectra were obtained from DFT calculations in the local density approximation [73]; note that in this scheme the transition energies are underestimated due to neglected selfenergy effects. Contributions from bulkrelated states to the RDS response appear in the spectra of Fig. 8.17 particularly near the E 1 and E 0 /E 2 critical points. Surface contributions are pronounced near 1.2 eV and near 3.4 eV, particularly for the c(4 × 4) reconstruction; these transitions are related to states of As dimers in this Asrich surface. Since layers in different depth beneath the surface provide different contributions to the spectra, also layerbylayer decomposition of the RAS signal were computed to unravel the complex response [74]. Experimental RDS spectra of GaAs(001) surfaces for various reconstructions are given in Fig. 8.18. The spectra are typical fingerprints of the respective surfaces and do basically not depend on the growth method. Samples prepared using either MBE or MOVPE yield similar RDS response [75]; RHEED studies of MBE samples and comparative GIXD measurements on MOVPE samples reported in [76] confirmed the formation of similar wellordered reconstructed surfaces in MOVPE despite the high ambient pressure.
8.4 Optical in Situ Surface Probes , E0 E2
E1
(a)
337
0.005
Bulk
Surface
β2(2 4)
0
1
2 3 Energy (eV)
4
c(4 4)
Re{(r[110] –r[110])/ r }
Re{(r[110] –r[110])/ r }
c(4 4)
Surface + Bulk 0.005 β2(2 4)
0
5
, E0 E2
E1
(b)
1
2 3 Energy (eV)
4
5
Fig. 8.17 RDS spectra of GaAs(001) with c(4 × 4) and β2(2 × 4) surface reconstructions, calculated using DFTLDA. a Separate contributions of bulk and surface, b total RDS response. Dotted lines indicate transition energies of critical points. Reproduced with permission from [73], © 2001 Wiley
3 GaAs (001)
Re{(r[110] –r[110])/ r } (103)
Fig. 8.18 Experimental RDS spectra of GaAs(001) surfaces with different reconstructions. Reproduced with permission from [77], © 1996 Elsevier
2
β2(2 4) α2(2 4)
1
(2 6) 0
c(4 4)
1
2
2
3 Energy (eV)
4
5
Today RDS is established as a valuable standard tool for monitoring metalorganic vaporphase epitaxy, where RHEED is not applicable. Its excellent surface sensivity is widely employed to obtain information on the state of the surface, or simply to ensure the reproducibility of runtorun conditions. Usually RDS transients at a selected fixed photon energy are recorded to trace the response during removal of the native oxide prior to deposition, to monitor the subsequent formation of a reconstructed surface [78], and to track the numerous subsequent process steps during epitaxy of heterostructures [79, 80]. Thereby layer thicknesses, compositions of alloyed layers and doping levels (typically those above mid 1017 cm−3 ) can be determined already during growth of the semiconductor structures.
8 In situ Growth Analysis
0 InGaAs/GaAs(001) T = 485 °C h = 2.6 eV
1 ML
1 2 3
GaAs
Re{(r[110] –r[110])/ r } (103)
338
In0.15Ga0.85As 0
10
20
30 Time (s)
GaAs 40
50
Fig. 8.19 Transient RDS response at 2.6 eV recorded during metalorganic vaporphase epitaxy of In0.15 Ga0.85 As/GaAs(001) layers at a rate of 0.4 monolayers/second. Reproduced with permission from [82], © 2004 Elsevier
The high surface sensivity of RDS is proved by the obervation of monolayer oscillations during layerbylayer island growth [42], analogous to the respective response of RHEED and GIXD discussed in Sects. 8.3.1 and 8.3.2. Oscillations of the RDS response during deposition of an InGaAs/GaAs layer are shown in Fig. 8.19. The Origin of RDS oscillations is less obvious than those of the morphologyrelated responses of RHEED and GIXD, which are due to longrange order; RDS studies for GaAs at two energies 2.6 and 1.9 eV, which according to calculations are respectively characteristic of dimers of As and Ga, indicate that oscillations are related to the periodic change of dimer orientations particularly near step edges [42]. More recent reports also emphasize the importance of the periodic modulation of orthorhombic surface strain associated to surface reconstruction [81]. Oscillations of RDS are generally well observed under lowtemperatures conditions that are Aslean compared to standard growth conditions. But even at typical growth conditions the RDS response of nanometerthick layers may provide valuable informations; without monolayeroscillations the response recorded during quantumwell growth could be well related to the emission energy of this quantum structure [79].
8.5 Problems Chapter 8 8.1 A heated and not stabilized cplane GaN surface decomposes in vacuum. Losses of 3.3 monolayers/minute (ML/min) at 760 °C sample temperature and 6.5 ML/min at 780 °C are measured by the desorbing Ga flux (≡ GaN flux) using calibrated mass spectrometry. Note: 1 ML corresponds to c/2 of GaN. (a) Determine the activation energy E d resulting from this measurement, if the thermally activated desorption follows an Arrhenius dependence.
8.5 Problems Chapter 8
339
(b) Calculate the Ga flux (expressed in ML/min), which is expected at 800 °C. (c) How many Ga atoms per cm2 of the surface desorb in one minute at 780 °C? 8.2 The electron gun of a RHEED setup is operated with 10 kV. (a) Calculate the fraction of relativistic correction of the electron momentum with respect to the classical calculation. How large is this fraction at 50 kV? (b) How many times larger is the Ewald sphere of the electrons at 10 kV compared to the unit cell of GaAs? 8.3 The calibration of a pyrometer yields a signal of 1.00 nA at the surface temperature of 577 °C with a real reflectance of 0.89 at a wavelength of 930 nm. (a) Determine the pyrometer signal at 800 °C, if the reflectance did not change. To which temperature corresponds this pyrometer signal, if the reflectance changed to 0.85? Calculate the actual pyrometer signal for 800 °C and a reflectance of 0.85. (b) Find the temperature of the surface, if a pyrometer signal of 1051.8 nA and a reflectance of 0.70 are measured. 8.4 A 2 μm thick (0001) oriented GaN layer is grown at 1050 °C on 0.45 mm thick basal plane sapphire. A (negligibly thin) properly recrystallized GaN nucleation layer on sapphire has provided an effective substrate for the GaN epitaxy with a relaxed lateral GaN lattice constant at 1050 °C but with elastic properties of sapphire; these are given by a thermal expansion coefficient of 8.2 × 10−6 K−1 and an inplane biaxial elastic modulus of 607 GPa. (a) Find the thermally induced lattice mismatch between the effective substrate and the GaN layer, when the temperature is lowered to 620 °C (a typical temperature for growing InGaN on top). (b) Calculate the biaxial elastic modulus of the GaN layer. How large is the stress in the layer at 620 °C? (c) Determine the curvature of the wafer resulting from the stressed layer. Calculate the corresponding curvature radius. 8.5 The real reflectance recorded during growth of a layer is described by the fit function R ∼ = 0.4 + 0.2 × exp(−1.8 × 10−3 s −1 t) × cos(2.0 × 10−2 s −1 t). (a) Find the reflectance measured at t = 0 and after 2.5 and 10 min according to the fit. Calculate the reflectance attained at an infinite thick layer. (b) Determine the approximate the period of the oscillating reflectance. When is the amplitude of the oscillation reduced to 10% of its initial value? (c) Calculate approximated values of the real reflective index and the extinction coefficient of the layer. (d) Determine the growth rate for a recording wavelength of 830 nm.
340
8 In situ Growth Analysis
8.6 General Reading Chapter 8 G. Bauer, W. Richter, Optical Characterization of Epitaxial Semiconductor Layers (Springer, Berlin, 1996) M.A. Hermann, W. Richter, H. Sitter, Epitaxy (Springer, Berlin, 2004)
References 1. M.P. Seah, W.A. Dench, Quantitative electron spectroscopy of surfaces: a standard data base for electron inelastic mean free paths in solids. Surf. Interface Anal. 1, 2 (1979) 2. W. Richter, D. Zahn, Analysis of epitaxial growth, in Optical Characterization of Epitaxial Semiconductor Layers, ed. by G. Bauer, W. Richter (Springer, Berlin, 1996), pp. 12–67 3. A.S.Y. Chan, M.P. Skegg, R.G. Jones, Line of sight techniques: providing an inventory of all species arriving at and departing from a surface. J. Vac. Sci. Technol., A 19, 2007 (2001) 4. S.G. Hessey, R.G. Jones, Lineofsight mass spectrometry: principles and practice. Surf. Interface Anal. 47, 587 (2015) 5. S. FernándezGarrido, G. Koblmüller, E. Calleja, J.S. Speck, In situ GaN decomposition analysis by quadrupole mass spectrometry and reflection highenergy electron diffraction. J. Appl. Phys. 104, 033541 (2008) 6. G. Koblmüller, R. Averbeck, H. Riechert, P. Pongratz, Direct observation of different equilib¯ surfaces. rium Ga adlayer coverages and their desorption kinetics on GaN (0001) and (0001) Phys. Rev. B 69, 035325 (2004) 7. J.E. Northrup, J. Neugebauer, R.M. Feenstra, A.R. Smith, Structure of GaN(0001): the laterally contracted Ga bilayer model. Phys. Rev. B 61, 9932 (2000) 8. J. Neugebauer, T.K. Zywietz, M. Scheffler, J.E. Northrup, H. Chen, R.M. Feenstra, Adatom kinetics on and below the surface: the existence of a new diffusion channel. Phys. Rev. Lett. 90, 056101 (2003) 9. M. Yoshida, H. Watanabe, F. Uesugi, Mass spectrometric study of Ga(CH3 )3 and Ga(C2 H5 )3 decomposition reaction in H2 and N2 . J. Electrochem. Soc. 132, 677 (1985) 10. L. Nattermann, O. Maßmeyer, E. Sterzer, V. Derpmann, H.Y. Chung, W. Stolz, K. Volz, An experimental approach for real time mass spectrometric CVD gas phase investigations. Sci. Rep. 8, 319 (2018) 11. P.W. Lee, T.R. Omstead, D.R. McKenna, K.F. Jensen, In situ mass spectroscopy and thermogravimetric studies of GaAs MOCVD gas phase and surface reactions. J. Cryst. Growth 85, 165 (1987) 12. G.B. Stringfellow, Alternate sources and growth chemistry for OMVPE and CBE processes. J. Cryst. Growth 105, 260 (1990) 13. G.B. Stringfellow, Organometallic VaporPhase Epitaxy, 2nd edn. (Academic Press, San Diego, 1999) 14. S.H. Li, C.A. Larsen, N.I. Buchan, G.B. Stringfellow, Pyrolysis of tertiarybutylphosphine. J. Electron. Mater. 18, 457 (1989) 15. U.W. Pohl, C. Möller, K. Knorr, W. Richter, J. Gottfriedsen, H. Schumann, A. Fielicke, K. Rademann, Tertiarybutylhydrazine: a new precursor for the MOVPE of III nitrides. Mater. Sci. Engin. B 59, 20 (1999) 16. C.A. Larsen, S.H. Li, N.J. Buchan, G.B. Stringfellow, Mechanisms of GaAs growth using tertiarybutylarsine and trimethylgallium. J. Cryst. Growth 94, 673 (1989) 17. A. Stegmüller, R.A. Tonner, Quantum chemical descriptor for CVD precursor design: predicting decomposition rates of TBP and TBAs isomers and derivatives. Chem. Vap. Depos. 21, 161 (2015)
References
341
18. F. Durst, A. Melling, J.H. Whitelaw, Principles and Practice of LaserDoppler Anemometry, 2nd edn. (Academic Press, London, 1981) 19. G.A. Hebner, K.P. Killeen, R.M. Biefeld, In situ measurement of the metalorganic and hydride partial pressures in a MOCVD reactor using ultraviolet absorption spectroscopy. J. Cryst. Growth 98, 293 (1989) 20. H. Itoh, M. Watanabe, S. Mukai, H. Yajima, Ultraviolet absorption spectra of metalorganic molecules diluted in hydrogen gas. J. Cryst. Growth 93, 165 (1988) 21. R.F. Karlicek, B. Hammarlund, J. Ginocchio, UV absorption spectroscopy for monitoring hydride vaporphase epitaxy of InGaAsP alloys. J. Appl. Phys. 60, 794 (1986) 22. M.C. Johnson, K. Poochinda, N.L. Ricker, J.W. Rogers Jr., T.P. Pearsall, In situ monitoring and control of multicomponent gasphase streams for growth of GaN via MOCVD. J. Cryst. Growth 212, 11 (2000) 23. J.E. Butler, N. Bottka, R.S. Sillmon, D.K. Gaskill, In situ, realtime diagnostics of OMVPE using IRdiode laser spectroscopy. J. Cryst. Growth 77, 163 (1986) 24. S. Salim, C.A. Wang, R.D. Driver, K.F. Jensen, In situ concentration monitoring in a vertical OMVPE reactor by fiberopticsbased Fourier transform infrared spectroscopy. J. Cryst. Growth 169, 443 (1996) 25. S.P. Watkins, T. Pinnington, J. Hu, P. Yeo, M. Kluth, N.J. Mason, R.J. Nicholas, P.J. Walker, Infrared single wavelength gas composition monitoring for metalorganic vapourphase epitaxy. J. Cryst. Growth 221, 166 (2000) 26. D. Hayashi, A. Teraoka, Y. Sakaguchi, M. Minami, H. Nishizato, Realtime measurement of Cp2 Mg vapor concentration using the nondispersive infrared spectroscopy. J. Cryst. Growth 453, 54 (2016) 27. C. Park, W.S. Jung, Z. Huang, T.J. Anderson, In situ Raman spectroscopic studies of trimethylindium pyrolysis in an OMVPE reactor. J. Mater. Chem. 12, 356 (2002) 28. I.P. Herman, Optical Diagnostics for Thin Film Processing, Chapter 7 Laserinduced fluorescence (Academic Press, New York 1996) 29. B. Zhou, X. Li, T.L. Tansley, K.S.A. Butcher, Growth mechanisms in excimer laser photolytic deposition of gallium nitride at 500 °C. J. Cryst. Growth 160, 201 (1996) 30. V.M. Donnelly, R.F. Karlicek, Development of laser diagnostic probes for chemical vapor deposition of InP/InGaAsP epitaxial layers. J. Applied Physics 53, 6399 (1982) 31. M.A. Van Hove, W.H. Weinberg, C.M. Chan, LowEnergy Electron Diffraction (Springer, Berlin 1986) 32. A. Ichimiya, P.I. Cohen, Reflection High Energy Electron Diffraction (Cambridge University Press, Campridge, 2004) 33. W. Braun, Applied RHEED, Reflection HighEnergy Electron Diffraction During Crystal Growth (Springer, Berlin, 1999) 34. Y. Ma, S. Lordi, J.A. Eades, Dynamical analysis of a RHEED pattern from the Si(111)7 × 7 surface. Surf. Sci. 313, 317 (1994) 35. Y. Nabetani, T. Ishikawa, S. Noda, A. Sasaki, Initial growth stage and optical properties of a threedimensional InAs structure on GaAs. J. Appl. Phys. 76, 347 (1994) 36. T. Sakamoto, H. Funabashi, K. Ohta, T. Nakagawa, N.J. Kawai, T. Kojima, Y. Bando, Well defined superlattice structures made by phaselocked epitaxy using RHEED intensity oscillations. Superlattices Microstruct. 1, 347 (1985) 37. D.W. Kisker, G.B. Stephenson, P.H. Fuoss, S. Brennan, Characterization of vapor phase growth using Xray techniques. J. Cryst. Growth 146, 104 (1995) 38. G. Ju, M.J. Highland, A. YanguasGil, C. Thompson, J.A. Eastman, H. Zhou, S.M. Brennan, G.B. Stephenson, P.H. Fuoss, An instrument for in situ coherent Xray studies of metalorganic vapor phase epitaxy of IIInitrides. Rev. Sci. Instrum. 88, 035113 (2017) 39. B. Jenichen, W. Braun, V.M. Kaganer, A.G. Shtukenberg, L. Däweritz, C.G. Schulz, K.H. Ploog, A. Erko, Combined molecular beam epitaxy and diffractometer system for in situ Xray studies of crystal growth. Rev. Sci. Instrum. 74, 1267 (2003) 40. G. Ju, S. Fuchi, M. Tabuchi, H. Amano, Y. Takeda, Continuous in situ Xray reflectivity investigation on epitaxial growth of InGaN by metalorganic vapor phase epitaxy. J. Cryst. Growth 407, 68 (2014)
342
8 In situ Growth Analysis
41. G. Ju, M. Tabuchi, Y. Takeda, H. Amano, Role of threading dislocations in strain relaxation during GaInN growth monitored by realtime Xray reflectivity. Appl. Phys. Lett. 110, 262105 (2017) 42. I. Kamiya, L. Mantese, D.E. Aspnes, D.W. Kisker, P.H. Fuoss, G.B. Stephenson, S. Brennan, Optical characterization of surfaces during epitaxial growth using RDS and GIXS. J. Cryst. Growth 163, 67 (1996) 43. W. Braun, B. Jenichen, V.M. Kaganer, A.G. Shtukenberg, L. Däweritz, K.H. Ploog, Layerbylayer growth of GaAs(001) studied by in situ synchrotron Xray diffraction. Surf. Sci. 525, 126 (2003) 44. D.W. Kisker, G.B. Stephenson, P.H. Fuoss, F.J. Lamelas, S. Brennan, Atomic scale characterization of organometallic vapor phase epitaxial growth using insitu grazing incidence Xray scattering. J. Cryst. Growth 124, 1 (1992) 45. D.W. Kisker, G.B. Stephenson, J. Tersoff, P.H. Fuoss, S. Brennan, Atomic scale studies of epitaxial growth processes using Xray techniques. J. Cryst. Growth 163, 54 (1996) 46. W.G. Breiland, Reflectancecorrecting pyrometry in thin film deposition applications, Technical Report, Sandia National Laboratories, Albuquerque, NM 87185, SAND20031868 47. K. Haberland, J.T. Mullins, T. Schenk, T. Trepk, L. Considine, A. Pakes, A. Taylor, J.T. Zettler, First realtime true wafer temperature and growth rate measurements in a closedcoupled showerhead MOVPE reactor during growth of InGa(AsP). In International Conference on InP and Related Materials. Santa Barbara, CA, USA (2003) 48. J.A. Floro, E. Chason, S.R. Lee, Real time measurement of epilayer strain using a simplified wafer curvature technique. Mat. Res. Soc. Symp. Proc. 405, 381 (1996) 49. S. Terao, M. Iwaya, R. Nakamura, S. Kamiyama, H. Amano, I. Akasaki, Fracture of Alx Ga1−x N/GaN heterostructure—compositional and impurity dependence. Jpn. J. Appl. Phys. 40, L195 (2001) 50. A. Krost, A. Dadgar, G. Strassburger, R. Clos, GaNbased epitaxy on silicon: stress measurements. Phys. Stat. Sol. A 200, 26 (2003) 51. F. Brunner, V. Hoffmann, A. Knauer, E. Steimetz, T. Schenk, J.T. Zettler, M. Weyers, Growth optimization during IIInitride multiwafer MOVPE using realtime curvature, reflectance and true temperature measurements. J. Cryst. Growth 298, 202 (2007) 52. G. Stoney, The tension of metallic films deposited by electrolysis. Proc. R. Soc. London A 82, 172 (1909) 53. L.B. Freund, J.A. Floro, E. Chason, Extensions of the Stoney formula for substrate curvature to configurations with thin substrates or large deformations. Appl. Phys. Lett. 74, 1987 (1999) 54. C.A. Klein, How accurate are Stoney’s equation and recent modifications. J. Appl. Phys. 88, 5487 (2000) 55. C. Kisielowski, J. Krüger, S. Ruvimov, T. Suski, J.W. Ager III, E. Jones, Z. LilientalWeber, M. Rubin, E.R. Weber, M.D. Bremser, R.F. Davis, Strainrelated phenomena in GaN thin films. Phys. Rev. B 54, 17745 (1996) 56. F. Brunner, A. Knauer, T. Schenk, M. Weyers, J.T. Zettler, Quantitative analysis of in situ wafer bowing measurements for IIInitride growth on sapphire. J. Cryst. Growth 310, 2432 (2008) 57. S. Hearne, E. Chason, J. Han, J.A. Floro, J. Figiel, J. Hunter, H. Amano, I.S.T. Tsong, Stress evolution during metalorganic chemical vapor deposition of GaN. Appl. Phys. Lett. 74, 356 (1999) 58. D.E. Aspnes, Minimaldata approaches for determining outerlayer dielectric responses of films from kinetic reflectometric and ellipsometric measurements. J. Opt. Soc. Am. A 10, 974 (1993) 59. D.E. Aspnes, Optical approaches to determine nearsurface compositions during epitaxy. J. Vac. Sci. Technol., A 14, 960 (1996) 60. J.T. Zettler, Characterization of epitaxial semiconductor growth by reflectance anisotropy spectroscopy and ellipsometry. Prog. Cryst. Growth Charact. 35, 27 (1997) 61. F.K. Urban III, M.F. Tabet, Virtual interface method for in situ ellipsometry of films grown on unknown substrates. J. Vac. Sci. Technol., A 11, 976 (1993)
References
343
62. W.G. Breiland, K.P. Killeen, A virtual interface method for extracting growth rates and high temperature optical constants from thin semiconductor films using in situ normal incidence reflectance. J. Appl. Phys. 78, 6726 (1995) 63. R.M.A. Azzam, N.M. Bashara, Ellipsometty and Polarized Light (North Holland, New York, 1987) 64. W.G. Breiland, H.Q. Hou, H.C. Chui, B.E. Hammons, In situ pregrowth calibration using reflectance as a control strategy for MOCVD fabrication of device structures. J. Cryst. Growth 174, 564 (1997) 65. C. Pickering, In situ optical studies of epitaxial growth, in Handbook of Crystal Growth 3, Part B: Thin Films and Epitaxy, Growth Mechanisms and Dynamics, ed. by D. Hurle (Elsevier, Amsterdam, 1994), pp. 819–878 66. R.W. Collins, I. An, H. Nguyen, Y. Li, Y. Lu, Realtime spectroscopic ellipsometry studies of the nucleation, growth, and optical functions of thin films, Part I: Tetrahedrally bonded materials, in Optical Characterization of Real Surfaces and Films, ed. by K. Vedam (Academic Press, Orlando, 1994), pp. 49–125 67. D.E. Aspnes, W.E. Quinn, S. Gregory, Application of ellipsometry to crystal growth by organometallic molecular beam epitaxy. Appl. Phys. Lett. 56, 2569 (1990) 68. D.E. Aspnes, Abovebandgap optical anisotropies in cubic semiconductors: a visible—near ultraviolet probe of surfaces. J. Vacuum Sci. Technol. B 3, 1498 (1985) 69. W.G. Schmidt, Calculation of reflectance anisotropy for semiconductor surface exploration. Phys. Stat. Sol. B 242, 2751 (2005) 70. K. Hingerl, D.E. Aspnes, I. Kamiya, L.T. Florez, Relationship among reflectancedifference spectroscopy, surface photoabsorption, and spectroellipsometry. Appl. Phys. Lett. 63, 885 (1993) 71. L.F. LastrasMartínez, A. LastrasMartínez, Reflectance anisotropy of GaAs(100): Dislocationinduced piezooptic effects. Phys. Rev. B 54, 10726 (1996) 72. M. Zorn, P. Kurpas, A.I. Shkrebtii, B. Junno, A. Bhattacharya, K. Knorr, M. Weyers, L. Samuelson, J.T. Zettler, W. Richter, Correlation of InGaP(001) surface structure during growth and bulk ordering. Phys. Rev. B 60, 8185 (1999) 73. W.G. Schmidt, F. Bechstedt, K. Fleischer, C. Cobet, N. Esser, W. Richter, J. Bernholc, G. Onida, GaAs(001): Surface structure and optical properties. Phys. Stat. Sol A 188, 1401 (2001) 74. C. Hogan, R. Del Sole, Optical properties of the GaAs(001)c(4 × 4) surface: direct analysis of the surface dielectric function. Phys. Stat. Sol B 242, 3040 (2005) 75. I. Kamiya, D.E. Aspnes, H. Tanaka, L.T. Florez, J.P. Harbison, R. Bhat, Surface science at atmospheric pressure: Reconstructions on (001) GaAs in organometallic chemical vapor deposition. Phys. Rev. Lett. 68, 627 (1992) 76. D.W. Kisker, G.B. Stephenson, I. Kamiya, P.H. Fuoss, D.E. Aspnes, L. Mantese, S. Brennan, Investigation of the relationship between reflectance difference spectroscopy and surface structure using grazing incidence Xray scattering. Phys. Stat. Sol. A 152, 9 (1995) 77. W. Richter, J.T. Zettler, Realtime analysis of IIIVsemiconductor epitaxial growth, Appl. Surf. Sci. 100/101, 465 (1996) 78. C. Kaspari, M. Pristovsek, W. Richter, Deoxidation of (001) III–V semiconductors in metalorganic vapour phase epitaxy. J. Appl. Phys. 120, 085701 (2016) 79. M. Zorn, M. Weyers, Application of reflectance anisotropy spectroscopy to laser diode growth in MOVPE. J. Cryst. Growth 276, 29 (2005) 80. N.A. Kalyuzhnyy, V.V. Evstropov, V.M. Lantratov, S.A. Mintairov, M.A. Mintairov, A.S. Gudovskikh, A. Luque, V.M. Andreev, Characterization of the manufacturing processes to grow triplejunction solar cells, Int. J. Photoenergy 2014, 836284 (2014) 81. J. OrtegaGallegos, L.E. GuevaraMacías, A.D. ArizaFlores, R. CastroGarcía, L.F. LastrasMartínez, R.E. BalderasNavarro, R.E. LópezEstopier, A. LastrasMartínez, On the origin of reflectanceanisotropy oscillations during GaAs (001) homoepitaxy. Appl. Surf. Sci. 439, 963 (2018) 82. U.W. Pohl, K. Pötschke, I. Kaiander, J.T. Zettler, D. Bimberg, Realtime control of quantum dot laser growth using reflectance anisotropy spectroscopy. J. Crystal Growth 272, 143 (2004)
Chapter 9
Application of Surfactants
Abstract Surfaceactive species referred to as surfactants modify the surface energy in semiconductor epitaxy. Applying an appropriate combination of surfactant and semiconductor materials, the threedimensional island growth occurring during heteroepitaxy can be suppressed, and the layer grows smoothly in a twodimensional layerbylayer mode. In this process the surfactant layer floats on the semiconductor layer during growth without significant incorporation. The effect is well established for many layer/substrate materials and particularly well studied for surfactantmediated epitaxy of Ge layers on Si substrate: twodimensional growth is maintained far beyond the critical thickness for the usually observed Stranski–Krastanow island formation with Sb or Bi acting as surfactant. The surfactant is found to substantially alter adatom diffusivity and nucleation rate. In addition, different processes for strain relaxation in the epitaxial layer are found. Similar findings are obtained with compound semiconductors. Both thermodynamic and prevailing kinetic effects account for the experimental observations. Generally accepted models consider a kinetically retarded approach to an equilibrium state of the layer comprising threedimensional islands. Modelling of adatom diffusion processes on the bare surface without surfactant and on the surfactantcovered surface indicate the prominent role of the passivation of step edges at nucleating monolayer islands. The passivation is connected to a suppression of deexcitation processes with atoms below the surfactant layer reexchanging with surfactant atoms. Exchange pathways of adatoms and surfactant atoms with low activation energy were identified for specific surfaces and participating species using ab initio calculations.
9.1 The Surfactant Effect 9.1.1 Concept of SurfactantMediated Growth Most device structures grown by epitaxy need sharp interfaces, a requirement usually met by growing with a smooth surface in a layerbylayer growth mode (Frank– Van der Merve mode in heteroepitaxy). Such twodimensional (2D) growth is often prevented in the epitaxy of a layer A on another material B (referred to here as © Springer Nature Switzerland AG 2020 U. W. Pohl, Epitaxy of Semiconductors, Graduate Texts in Physics, https://doi.org/10.1007/9783030438692_9
345
346
9 Application of Surfactants
substrate): if the surface energy of B is smaller than the sum of the surface energy of A and the interface energy of A/B, the layer does not wet the substate surface. This leads to 3D island growth in the Volmer–Weber mode pointed out in Sect. 6.2.3. Moreover, layer A is generally strained by structural or thermal mismatch to B. Thus, even if a wetting layer is formed, strain easily induces the 3D Stranski–Krastanow island growth as shown in Figs. 6.12 and 7.39. These conditions leads to a fundamental obstacle for the growth of a B/A/B heterostructure such as a quantum well. One of the two solids A or B must have a lower surface energy. We disregard here the interface energy, since it refers to both A/B and B/A structures. If A with a lower surface energy grows on B in the Frank–Van der Merve or Stranski–Krastanow mode, then B tends to grow on A in the Volmer–Weber mode [1]. Hence, when an embedded layer is grown, either the growth mode of this layer or that of the capping layer tends to Volmer–Weber, i.e., a 3D growth with immediate islanding leading to a rough interface. Any growth of a quantum well or a superlattice must overcome this limitation. This is generally achieved by limiting the growth kinetics, using a decreased growth temperature or an increased growth rate. Since such means may also reduce the epitaxial quality, an alternative is desirable. Early investigations indicated that the growth mode can be altered in the presence of impurities, see, e.g., [2]. Such an effect of contaminants was observed with many layers A on substrates B and discussed in an early review in terms of metastable layers [3]. Surfactantmediated growth implies a controlled modification of the surface energy. A third material C is introduced which lowers the surface energy of both A and B: a thin film of a surfactant C is deposited on B before growing layer A on B. With an appropriate choice of material C it will float on top of A during growth without significant incorporation into layer A. Growth of A may now proceed in the layerbylayer (Frank–Van der Merve) mode. This applies as well for the subsequent deposition of material B on layer A. By using a surfactant the formation of 3D islands can be avoided, and a 2D layerbylayer growth can be maintained for layer thicknesses much beyond those obtained without the surfactant. It must be noted that the strain introduced in the heteroepitaxy is still present, even if the 3D growth is suppressed. Similar to the growth without surfactant the strain is relieved by misfit dislocations for layers exceeding a critical thickness. The mechanism and the kind of misfit introduction may, however, differ significantly. The term surfactant signifies the application of a surfaceactive species. The term is widely used in semiconductor growth, but its meaning differs substantially from that commonly used in chemistry. For semiconductors it describes the effect of an adsorbate layer on the growth of a layer deposited on a substrate, while in chemistry it usually denotes a material which improves emulsifying, dispersing, wetting, or other surface properties of liquids. The surfactant effect is also found in the epitaxy of metals on metals [4, 5]. B/A/Btype layer structures with a monolayer (ML) of a highsurfaceenergy transition metal (Ni, Fe, Co) and a lowsurfaceenergy noble metal (Au, Ag, Cu) are basic building blocks for a broad category of magnetic multilayers; these tend to grow with rough and intermixed interfaces, but smoothly in a layerbylayer mode with the addition
9.1 The Surfactant Effect
347
of a surfactant like Pb or Bi. Still the effect differs from that observed for semiconductors. In metal growth a small fraction of an adsorbate monolayer may change the surface kinetics, leading to modified nucleation rates and stepedge barriers [6]. In semiconductor growth typically an entire monolayer is required to produce the surfactant effect. This chapter focuses on the effect observed for semiconductors.
9.1.2 Evidence for the Surfactant Effect The surfactant effect was demonstrated for many different semiconductor heterostructures. Most studies were made with groupIV layers on groupIV substrates, particularly with Ge on Si; in this system the investigations focused on (001) and (111) surfaces and employed various surfactants, mainly groupIII elements (Ga, In) or groupV elements (As, Sb, Bi). Ge and Si both crystallize in diamond structure, with the lattice constant of Ge (5.6576 Å) exceeding that of Si by 4.2%, see Sect. 2.1. Epitaxial growth of Ge/Si(001) proceeds in the Stranski–Krastanow mode (Figs. 7.39a and 9.1a) with a typically ~3 monolayers thick wetting layer [7] and a maximum thickness of 2D layerbylayer growth of six monolayers [8]. In the 3D Stranski–Krastanow growth coalescence of the islands produces inevitably a highly defective Ge layer. Si grows on Ge and on Ge/Si in the 3D Volmer–Weber mode [9]. Growth of a Si/Ge/Si quantum well structures hence shows strong islanding and interdiffusion effects [10]. Growth of Ge on Si and Si on Ge/Si was found to be completely altered, if one monolayer of As is deposited on a Si(001) surface prior to the Ge deposition [1, 11]. With As as a surfactant, thick Ge layers can be grown in a clear layerbylayer mode, see Figs. 9.1b and 9.2. Furthermore, Si deposited on a thin pseudomorphic Ge/Si(001) layer—and hence not undergoing significant strain—is also found to grow Fig. 9.1 a Cross sectional TEM micrograph of 8 ML Ge/Si(001) grown without surfactant; Ge forms pseudomorphic Stranski–Krastanow islands. b 50 ML Ge/Si(001) grown in a layerbylayer mode with 1 ML As surfactant; the arrow marks a Vshaped defect. Reproduced with permission from [12], © 1990 APS
(a) Ge
Si 3.1 Å
Ge
(b)
Si 10 nm
348
20 Å Si n ML Ge Si(001)
1 ML As
3 ML Ge
Surface Buried As Ge
random channeled
Backscatter yield (arb. units)
Fig. 9.2 He+ ion backscattering spectra of Ge layers on Si(001) substrate, buried underneath a 20 Å thick Si cap layer; one monolayer of As was deposited before growth of the Ge layer and floates on the surface during Ge and Si depositions. Blue circles denote randomly scattered He+ ions, green dots denote backscattered channeled ions of 100keV He+ incident in the 111¯ direction. Reproduced with permission from [11], © 1990 APS
9 Application of Surfactants
8 ML Ge
15 ML Ge
85
90 95 Energy (keV)
100
as a smooth layer in the presence of As, while clear indications for island formation is observed if no As is layer is applied. In this study no As was incorporated in the Ge or Si layers within the resolution of 1%; instead, As was found to constantly segregate to the surface during growth [11]. The findings summarized above were first concluded from ion backscattering spectra given in Fig. 9.2, accompanied by photoemission and electron microscopy studies [11]. In these ion backscattering experiments He+ ions accelerated to 100 keV ¯ direction of the sample—leading to channelwere either impinged along the [111] ing—or some degrees off for random spectra; the energy of backscattered ions was analyzed with high resolution. The spectra for Ge layers embedded in Si show a peak at 96 keV due to backscattering from As at the surface, and a lowerenergy peak for the buried Ge. The Ge peak increases for thicker Ge layers but remains at lower energy; the continuous increase of signal without saturation at thicknesses well above Stranski–Krastanow island formation indicates that no such islands formed, and the persisting lower energy of the peak indicates a continuous Si layer on top [11]. The strongly diminished channeling signal of the Ge peak results from the overlying Si cap and indicates that both Ge and Si are epitaxial. When islands are formed (typically after depositing 3 ML Ge), the ratio of channeled to random signals increases significantly [8]; this is not observed with As surfactant. Channeling and
9.1 The Surfactant Effect
349
random spectra of the As peak are identical, because there is no shadowing cap layer on top. The conclusions drawn from the backscattering spectra were confirmed by electron micrographs and by corelevel photoemission spectra, where the Asrelated lines did not diminish as the Ge layer thickness increases [11].
9.1.3 SurfactantMediated Ge/Si Epitaxy The surfactant effect of Ge/Si on a (001) substrate described above is also found for [111] oriented heterostructures and for many other surfactant elements. These are elements of group I (H), III (Ga, In), IV (Sn, Pb), V (As, Sb, Bi), VI (Te), or noble metals with a low surface energy such as Au. A comprehensive review is given in [13]. The initial publication of surfactantmediated Ge/Si(001) growth [1] was followed by many experimental studies with Ge/Si confirming the early results and providing indications for the origin of the pronounced effects. In a simple view it might be assumed that a surfactant passivates the surface by saturating dangling bonds, leading to an increased diffusion length of adatoms. Such enhanced adatom diffusivity was observed for group III and IV surfactants with a consequential 3D islanding in Ge/Si epitaxy, while group V and VI surfactants reduce the diffusivity with a suppression of islanding. The diffusion length can be determined by studying the surface morphology: near the edge of a growing island or that of an advancing step no stable nuclei can be formed, because the adatom density is reduced due to incorporation at the edge (denuded zone, see Sect. 7.2.3). The mean distance between 2D islands or likewise the width of the depleted zone at step edges is hence a measure for the diffusion length, and for 2D island √ growth this distance R is related to the areal density of islands N by R = 1/ N . Based on this context the diffusion length of adatoms in the homoepitaxy of Si/Si(111) and changes in the respective surfactantmediated homoepitaxy was investigated by scanning tunneling microscopy (STM) [14]. Figure 9.3a shows the effect of the surfactants on the density of 2D islands and the related island distance for a submonolayer Si coverage; at increased substrate temperature the density decreases and the distance increases due to a higher adatom diffusivity in all studied cases. The dependence is well described by an Arrhenius law, yielding various barriers for adatom diffusion deviating from the Si/Si reference. A similar behavior is obtained from the width of the denuded zone depleted of islands at step edges shown in Fig. 9.3b. These results lead to a factor g for the adatom diffusionlength in presence of a surfactant with respect to that of the pure Si/Si epitaxy at a given temperature. A factor g ≥ 1 is found for Ga, In (group III), and Sn (group IV). The increased diffusion length supports lateral mass transport; such transport is required for the formation of large Stranski–Krastanow islands in the heteroepitaxy of Ge/Si. From the similar chemical nature of Si and Ge also a favored adatom diffusion of Ge on Si
350
9 Application of Surfactants T (K)
T (K) 700
600
(a)
900
(111) Si/Sb/Si
Si/As/Si
1011
Si/Si
100 nm 500 Si/In/Si
1010 1.0
1.4 1/T (103 K1)
1.6
1.8
700
1000 (111)
600
Si/In/Si Si/Si Si/Ga/Si
100
1000 1.2
800
(b)
100
Island distance (Å)
Island density (cm2)
1012
800
Depleated zone (Å)
900
10 1.0
Si/Sb/Si
Si/As/Si
1.2
1.4
1 μm 1.6
1.8
1/T (103 K1)
Fig. 9.3 a Density of 2D islands in the homoepitaxy of Si on Si(111) grown with and without surfactants as indicated at the curves. Inset: STM image of Si/Si grown at 500 °C. b Width of depleated zone at the step edge in Si on Si(111) epitaxy. Inset: STM image of Si/Ga/Si grown at 630 °C. Reproduced with permission from [14], © 1995 APS
was suggested, and in fact for these surfactants island formation is observed in Ge/Si epitaxy. On the other hand g < 1 is found for Sb and As (group V) surfactants, and the 3D island formation for Ge/Si is suppressed [14]. This led to the conclusion that the surfactantmediated layerbylayer growth originates from a kinetically reduced mass transport; in fact, in the surfactantinduced 2D growth of Ge/Sb/Si(111) a temperature increase leads to the reappearance of 3D growth [15, 16]. An alternative interpretation of the experimental findings was suggested by considering a passivation effect of a surfactant on the island edges [17]; such a passivation was actually confirmed for Ascovered Si(111) [18]. If a surfactant passivates the island edges, they do not act as sinks for adatoms diffusing on the surface (Sect. 7.2.3). Consequently the width of depleted zones is reduced. We consider this model in more detail below in Sect. 9.2.3. Strain relaxation is required also in the surfactantmediated 2D heteroepitaxy. The relief of strain in the pure Ge/Si epitaxy with the formation of 3D Stranski– Krastanow islands differs for growth on (111) and (001) surfaces [19]. On both surfaces the 2D → 3D transition is preceded by the formation of surface structures with a decreased layer density and a related partial strain relaxation, and after island formation strain is elastically more efficiently relieved by a bending of the lattice in the islands; misfit dislocations are introduced from island edges when the thickness is increased and when islands coalesce (at ~100 ML Ge coverage with ~1012 cm−2 threading dislocations). If the elastic 3D relaxation mechanism is disabled by a surfactantmediated 2D growth, misfit dislocations must accommodate the strain accumulated in the 2D layers. Antimony is a preferred surfactant for the epitaxy. Sb forms on Si(111) √Ge/Si(111) √ ◦ 3 × 3 30 reconstruction comprising a selflimiting coverage of 1 ML with a Sb trimers; each Sb is bonded with one electron to a Si top atom and with two electrons to the two neighboring Sb atoms, leaving the remaining two electrons in a lonepair orbital [20]. The efficient segregation of Sb on the growing Ge layer was
9.1 The Surfactant Effect
351
proved, yielding an upper limit for Sb incorporation into the Ge bulk below 2 × 1019 cm−3 by XPS [21] and below 2 × 1018 /cm3 by SIMS [15]. Using antimony as surfactant for the Ge/Si(111) epitaxy, surface studies applying STM and LEED show successive stages for strain relief as the Ge coverage is increased. Up to a thickness of 8 ML Ge grows smooth and defectfree. Above 8 ML thickness, the analysis of LEED patterns recorded in situ during deposition shows the onset of a periodic dislocation network; near 8 ML 70% of the lattice mismatch of the Ge layer is immediately relaxed by dislocations with an average distance of ~15 nm [21]. After 10 ML additional Ge coverage the average distance attains its final value of 10.4 nm, leaving a completely strainrelieved Ge layer with bulk lattice constant. The satellite structure of the LEED spots indicates a relief by 60° dislocations. In the 3D growth of pure Ge/Si, dislocations nucleate at the edge of the islands above a critical thickness of about 6 ML [8, 22]; they glide as Shockley partial dislocations (SPDs) and thread to the surface when the islands coalesce. The surfactantmediated 2D epitaxy constrains the nucleation of strainrelieving dislocations; this extends the critical thickness for dislocation formation to about 8 ML. Since no sources for dislocation nucleation exist at the interface, they must nucleate at the surface. A detailed TEM investigation shows a quite complex relaxation mechanism proceeding in two steps [20, 23]: In the first step an SPD nucleates at the surface and glides down to the interface, where it cross slips laterally along the interface; this creates stacking faults in the layer and at the interface. In the second step at thicker layers (with increased strain) another SPD nucleates at the surface at the same location where the first SPD intersects the surface; it glides on the same plane to the interface, eliminating the portion of the first SPD’s stacking fault that threads through the epilayer. Such a restoring of the perfect lattice is very unlikely in presence of 3D islands due to the numerous lowenergy nucleation sites at the island edges; if the dislocations are not at exactly the same plane, they leave a high density of stacking faults. The crossslip process at the interface leads to an edge dislocation, which can climb to the surface by absorbing atoms of the Ge layer. As a result shown in Fig. 9.4, this relaxation mechanism creates a defectfree relaxed Ge(111) layer on Si(111) with a dense array of dislocations confined in the (111) plane of the interface. The structure of the periodic defect array at the Ge/Si interface was also revealed in the TEM study [23]. The honeycomb pattern shown in Fig. 9.4b is composed of alternating faulted and unfaulted regions. The small faulted regions with a size below 5 nm can be described by dislocation lines oriented along the three 110 directions of ¯ the (111) interface plane indicated in Fig. 9.5. There are three dislocations of a2 110 type with Burgers vectors in the interface plane (required to be glissile there), and each is equivalent to a sum of two partial dislocations D1 (90° edge dislocation) and D2 (30° dislocation), see Sect. 2.3.3. For the imaging condition of Fig. 9.4b with diffraction vector g = 022¯ all dislocations fulfilling g · b = 0 are invisible, e.g., a ¯ ¯ 1¯ = a 011¯ . In the 211 ; visible are, e.g., the partial dislocations a6 112¯ + a6 12 6 2 network we hence observe two sets of dislocations 81 Å apart and one set of dislocations 40.5 Å apart. The dissociation of the perfect dislocation into two Shockley
352
9 Application of Surfactants
(a)
(b)
Ge
IF
IF 8.1 nm
Si D1
D2
D1
D2
g = [022]
0.31 nm
¯ of 50 ML Ge grown with Sb surfactant on Fig. 9.4 a Highresolution TEM image along 110 Si(111). D1 and D2 denote alternating partial dislocations, the interface is marked by IF. b Planview weakbeam darkfield image showing a honeycomb array of small dislocations. Reproduced with permission from [23], © 1991 APS
g = [022]
81 Å
D2 16 [121] D1 16 [112] D1 1 [211] 6
D2 1 [112] 6
D2 1 [211] 6
40.5 Å
D1 1 [121] 6
Fig. 9.5 Schematic of a strainrelieving dislocation array with a symmetry like that in Fig. 9.4b. Blue and green lines signify respective dislocation lines of 90° (D1) and 30° (D2) partial dislocations at the interface with Burgers vectors specified at the labels, shaded areas mark faulted regions delineated by the same type of dislocations. After [23]
partials creates a stackingfault ribbon in between like that shown in Fig. 2.23. In Fig. 9.5 triangular faulted areas formed by the same type of bordering partial dislocations are indicated by shading. The spacing in the dislocation network corresponds to one plane less in the Ge layer every 25 planes of the Si substrate, yielding the relaxed Ge bulk lattice constant. The relaxed Ge films can be grown further to arbitrary thickness. Sb sticks still at the surface, though; it may be desorbed at high temperature (≥720 °C), but such a
9.1 The Surfactant Effect
353
treatment leads to the reappearance of Ge islands. This effect may arise from a straininduced Ge–Si intermixing at the interface and subsequent glide of dislocations to the surface [21].
9.1.4 SurfactantMediated Epitaxy of III–V Semiconductors
(aInAs  aGaAs) / aGaAs (%)
The surfactant effect described above for the Ge/Si model system was also observed for compound semiconductors and particularly studied for III–V layers on III–V substrates. While the effect has clearly been demonstrated, modelling of the results is much more complex. The presence of anions and cations leads to a larger variety of surface reconstructions, which in addition to temperature also depend on partial pressures. Also the dynamics of growth is more complex even without surfactant. Still some basic correlations could be identified. InAs on GaAs(001) has a lattice mismatch of about −7% and is well known to grow in the Stranski–Krastanow mode with a critical thickness of 1.5 ML for the 2D → 3D transition [24], see also Fig. 8.7. This property is widely employed for the fabrication of quantum dots, see Sect. 7.3.1. When the GaAs surface is covered with 1 ML Te prior to InAs deposition, the coherent 2D growth can be maintained up to a thickness of 6 ML [25]. The in situ measurement of the lateral lattice constant aInAs of InAs by RHEED given in Fig. 9.6 shows coherent 2D growth up to 1.5 ML without Te and up to 6 ML with Te acting as surfactant (the mismatch is given here according to (2.20b)). Accompanying XPS analysis proved the respective 3D and 2D growth mode and a floating of the Te layer on top of the InAs surface.
T = 400°C
6 InAs/GaAs InAs/Te/GaAs 4 1.5 ML
6 ML
2
0 0
2
4
6 8 InAs thickness (ML)
10
12
Fig. 9.6 Normalized difference of inplane lattice parameters a of InAs and GaAs, measured in situ during growth of InAs on GaAs(001) without (blue circles) and with Te surfactant (green diamonds); the onset of plastic lattice relaxation is indicated by arrows. Reproduced with permission from [25], © 1992 APS
354
9 Application of Surfactants
The effect of Te on the diffusion of adatoms was studied by monitoring the specular beam intensity of RHEED oscillations during homoepitaxial growth of GaAs: the oscillations disappear at increased temperature when the 2D islandnucleation growth mode changes to stepflow growth, see Sect. 8.3.1. This transition temperature is 580 °C for GaAs standard MBE on GaAs(001) 5° off toward (111)A; the offcut is used to obtain a terrassed surface [26]. For Teassisted growth the transition occurs at 600 °C, proving the reduced diffusion length at a given temperature in presence of the Te surfactant. √ A reduced diffusion length λ = Dτ may also be obtained by growth without surfactant; λ decreases if either the diffusion coefficient D or the average dwelling time τ are diminished. A surfactant reduces D by introducing energy barriers. A reduced diffusivity is also obtained at decreased temperature, as experimentally demonstrated by a persistent 2D growth mode of Inx Ga1−x As/GaAs(001) at low substrate temperature [27]; however, such procedure has generally a detrimental effect on the material quality. Also the residence time τ can be altered by growth conditions; an increase of the supersaturation leads to an increased growth rate, i.e., a reduced τ . The 2D growth mode of Inx Ga1−x As/GaAs(001) was in fact maintained up to twice the critical thickness tc for epitaxy at increased growth rate [28]; here strain and tc depend on the In composition x, and the extension of tc disappears as x approaches unity. For III–V epitaxy also the V/III ratio applied during growth affects the adatom surfacediffusion and consequently the growth mode. Changing from anionrich (V/III > 1) to cationrich conditions, island formation of InAs/GaAs(001) is suppressed as well—an effect originating from a reduced diffusion length of the growthlimiting As species [29]. For InAs/GaAs(001) different types of surfactants were found, similar to the findings for Ge/Si; Te is shown above to decrease the diffusion length, while Pb increases the diffusion length, and the critical thickness for the 2D → 3D transition is correspondingly decreased. The different behavior was interpreted in terms of socalled reactive and nonreactive surfactants, respectively [26]. The surfactant effect may in fact differ from that of Ge/Si epitaxy: a large concentration of incorporated Te corresponding to ½ ML was found at the interface of Temediated InAs/GaAs(001) epitaxy [30]. Similar results were observed with thallium as surfactant [31]. Such a high local density of impurities is expected to affect the relaxation mechanism. InGaAs on InP(001) can be grown lattice matched with 47% Ga composition on the cation sublattice; this applies as well for InAlAs with 48% Al and the quaternary Alx Ga0.48−x In0.52 As. Such layers are interesting for optoelectronic devices operating at 1.5 µm telecom wavelength and for highelectronmobility transistors. Surfactantmediated growth was studied using Bi in MBE of InGaAs/InP [32]; at sufficiently high growth temperature (450 °C) Bi acts as a surfactant; it may change the growth mode from 3D to 2D and improve surface smoothness. This was employed for fabricating highly strained InGaAs/InP quantum wells [33] for lasers with improved performance [34]. At lower growth temperature Bi is rapidly incorporated into InGaAs by forming an InGaAsBi alloy [32, 35]. Such a behavior is in contrast to that of Sb [36]; Sb on InP(001) forms at elevated temperature (>300 °C) a relaxed InSb layer with 1 ML Sb coverage, while 1 ML Sb deposition at room temperature leads to
9.1 The Surfactant Effect
355
an epitaxial Sb terminated surface [37], which could be employed for surfactantmediated 2D growth of Ge/InP(001) up to 5 ML (instead of only 2 ML without Sb [38]). GaN on AlN(0001) has an inplane lattice mismatch f = −2.3%. Epitaxy is often performed on basalplane sapphire covered with thick relaxed buffer layers as pseudosubstrates. Growth at sufficiently high temperature and usual Nrich conditions proceeds in the Stranski–Krastanow mode with a GaN thickness of ~2 ML for the 2D → 3D transition. Similar to the findings for InAs/GaAs(001), 3D growth is suppressed at decreased temperature. Furthermore, 2D growth is maintained at low V/III ratio, i.e., under Garich conditions [39]. Indium has a surfactant effect on the cationpolar basal plane of GaN and AlN [40, 41]. The change from Ga to N rich conditions in the epitaxy of GaN(0001) leads to a rough surface morphology; the smoothtorough transition shifts to much higher V/III ratios when In is added [42]. For AlN/GaN(0001) the AlN layer is tensely strained, and strain relief often occurs by cracks, see Fig. 9.7a. Supplying In as a surfactant during deposition of the AlN layer, stepflow growth evolves around the typical threading cores of screw dislocations—an effect attributed to an increased adatom diffusion length [43]. In the superlattice AlN/GaN structure shown in Fig. 9.7b an In incorporation below 2% was observed. Indium is also an important component in InGaN quantum wells, where an Inrich composition is intended. Applying Sb as surfactant during growth of InGaN layers, an abrupt increase in the In content is observed above a threshold concentration of ~1% Sb [44]. This effect is accompanied by a change of surface morphology; above threshold an increased density of smaller island is found. In the homoepitaxy of GaN(0001), Sb is expected to increase the effective diffusion length of N. Calculations based on density functional theory indicate that the presence of Sb leads to the formation of SbN intermediates, which are much more mobile than atomic N; since N diffusion is the ratelimiting step in the overall GaN growth process, such increased diffusivity favors a smooth surface morphology and an improved N incorporation during growth [45]. Fig. 9.7 Atomic force micrographs of the 30 nm thick cap layer of a AlN on 30 periods of (1.8 nm GaN wells/2 nm AlN barriers) and b Al(In)N on a similar superlattice with Al(In)N barriers. Reproduced with permission from [43], © 2006 AIP
(a)
(b)
500 nm
500 nm
356
9 Application of Surfactants
9.2 Models of SurfactantAssisted Epitaxy There are some common observations in the applications of surfactants to various materials A and B. Introduction of the surfactant leads generally to an increased nucleation rate. This means that the density of 2D islands nucleating on a surface becomes larger and their size becomes smaller. This finding is connected to a decrease of the adatom diffusion length. The surfactant layer removes the typical reconstruction of the pure surface. The surfactantrelated reconstruction is usually passivated, i.e., dangling bonds are filled and the surface becomes chemically more inert. The new reconstruction is often more simple; e.g., the (7 × 7) reconstruction of Si(111) changes to a (1 × 1) reconstruction when As is applied as surfactant. The combination of Ge and Si is a model system for the study of surfactants. This choice has several reasons. Compound semiconductors consist of (at least) two species with different chemical identity. This leads to complicated surface reconstructions, which depend on the cation/anion ratio and on temperature (see Fig. 7.8). Anions are typically not provided as monomers during growth; e.g., in the MBE of GaAs the As species are dimers As2 or tetramers As4 . Growth hence requires a decomposition of these species, making the dynamics quite complex. Studies such as those presented in Sect. 9.1 show that the surfactant changes both the thermodynamics and the kinetics of the involved processes. Several models were developed, emphasizing either a prevalence of the thermodynamic or the kinetic aspect. In the following we discuss approaches explaining the surfactant effect on semiconductors emphasizing these two aspects.
9.2.1 Thermodynamic Considerations The basic assumption of a thermodynamic approach is that the equilibrium state of a layer in presence of the surfactant is a smooth twodimensional surface. Such a state is formed if the equilibrium shape of a 3D crystal of material A, accommodated epitaxially on a misfit substrate B, has a vanishing aspect ratio of height h over lateral extension l [46]. This Kern–Müller criterion may be fulfilled by introducing a surfactant, which reduces surface stress and surface energy and consequently leads to a wetting of A on B that otherwise may not form. We consider the change of free energy during the epitaxial deposition of a small island A on the substrate B at constant temperature and vapor pressure PA ; the process is illustrated in Fig. 9.8 [46]. In terms of simple cubic Kossel crystals A and B with a mismatch f according to (2.20a) there are two bulk and three surface terms contributing to the total change of free energy F for the formation of the A island on substrate B. In the first step of Fig. 9.8a to b chemical work is gained by forming the solid A with all its faces from the gas phase of A species. This creates the negative bulk contribution F 1 and the positive surface contribution F 2 containing the
9.2 Models of SurfactantAssisted Epitaxy S A+ A
a
A B
357 a(1νf )
a
A
b = a(1+f ) AB
b
B (a)
(b)
(c)
(d)
Fig. 9.8 Thermodynamical process for the formation of a small crystal A on a substrate B: a supersaturated gas phase of A species, b formation of the crystal and all crystal surfaces, c accommodation of A to B and corresponding deformation of crystal A surfaces, d adhesion of A to B
surface free energy γ A . In the next step to Fig. 9.8c the (initially relaxed) crystal A is elastically strained for a coherent fit to substrate B. The deformation energy of the corresponding bulk contribution F 3 contains the misfit f, Young’s modulus, and Poisson’s ratio of A. A surface contribution F 4 accounts for the simultaneously occurring deformation of the surfaces and the resulting surface stress γ AS of the basal and side surfaces. In the last step to Fig. 9.8d the crystal A adheres to the substate B; the related contribution F 5 contains the adhesion energy γ AB . The apect ratio h/l for a 3D crystal A on B in equilibrium is now considered for the case without elastic relaxation. The contributions Fi mentioned above lead to a fraction for h/l with the numerator given by the socalled wetting factor [46] 2γ A − γ AB + 4 f γ AS − γ A ;
(9.1)
this is the Kern–Müller criterion for 2D layerbylayer growth, obtained from the Bauer criterion [47] (first two summands) by adding a strain term containing the misfit f. A decreasing ratio h/l, i.e., a 3D → 2D transition, is obtained when the adhesion energy γ AB increases or if the surface energy γ A decreases. The surface stress γ AS may drive the system away from or towards to the 3D → 2D transition. By introducing a surfactant the wetting factor (9.1) is complemented by two additional summands, which respectively decrease the surface free energy γ A and account for a differently stressed surface of A when some quantity of the surfactant is adsorbed on A; the adhesion energy γ AB is not affected by the surfactant, which by definition floats on A [46]. The new summands depend both on the mismatch f and the quantity of surfactant Γ . For f > 0 (i.e., lattice constant b > a) the system can be driven from 3D to 2D growth by increasing the surfactant coverage Γ ; for negative f this applies only for special parameter values within this model. The equilibrium model discussed so far may well indicate whether a surfactant species drives the system into the right direction to suppress island formation. However, it does not account for the Stranski–Krastanow growth mode, where the layer A wets the surface B and still proceeds with 3D growth. Moreover, the effect of elastic strain relaxation of A islands is not included. This contribution is negative and
358
9 Application of Surfactants
proportional to the island volume; it is known to substantially reduce the cost of 3D island formation [48, 49]. Today it is generally accepted that the surfactant effect is not of purely thermodynamic origin, and most approaches assume a prevailing kinetic effect. The models consider atomistic processes, often with some influence of thermodynamics.
9.2.2 Kinetic Approach A kinetic model assumes that the equilibrium state of a layer is a threedimensional surface even in presence of the surfactant. The surfactant leads to layerbylayer growth by kinetically prolonging the approach to equilibrium beyond the time scale of fabricating the structure. We first discuss a thermodynamically motivated atomistic model including kinetic contributions. A generally accepted kinetic description is outlined in Sect. 9.2.3. The Markov Model The commonly observed increase of nucleation rate and decreased adatom diffusion length for surfactantmediated growth is described in a simple atomistic model of homoepitaxial nucleation, including both thermodynamic and kinetic aspects [50, 51]; accounting for strain would introduce an additional term into the work of nucleus formation G containing the wetting factor (9.1). We consider the nucleation of a 2D cluster according to the process illustrated in Fig. 9.9 [52]. The process implies the isothermal and reversible evaporation of all surfactant atoms from the crystal surface, then producing a cluster with i crystal atoms on the surface, and finally condensing back the surfactant atoms. If we assume a cubic Kossel crystal and a surface cluster with a square shape and edge length l, the work for cluster formation on the surfactantfree surface (Fig. 9.9b) reads G 0 = −i μ + 4 l γc ;
(a)
(b)
(9.2)
(c)
Fig. 9.9 Process for evaluating the Gibbs free energy change by the formation of a homoepitaxial small nucleus on a surface covered with a surfactant monolayer: a the surfactant atoms (filled circles) are evaporated, b the nucleus is formed, c the surfactant layer is condensed back
9.2 Models of SurfactantAssisted Epitaxy
359
here μ is the supersaturation, i.e., the chemical potential difference between the ambient and the new phase, and γc is the edge energy per length of crystal atoms (index c) at the perimeter of the cluster. For a 2D cluster this is the energy of the dangling bonds of the perimeter atoms, and for the cluster on top of the Kossel crystal it is simply the number of dangling bond times half the bond energy between crystal atoms. When in the step of Fig. 9.9c the surfactant atoms are condensed back, the surfactant atoms beside the edge of the cluster saturate the dangling bonds, gaining an energy −4lsγc ; the parameter s is introduced as a measure for the energy efficiency of this process. Additionally an edge energy per length +4lγs must be paid for the surfactant atoms (index s) on top of the cluster at the edge. The total work for the formation of the cluster hence reads G = G 0 − 4 l s γc + 4 l γs .
(9.3)
The parameter s for the surfactant efficiency is obtained from s =1−
1 (E cc 2
+ E ss ) − E sc 1 E 2 cc
;
(9.4)
here E cc is the bond energy between two crystal atoms, E ss that between surfactant atoms, and E sc that between a crystal atom and a surfactant atom; for the factor ½ see (6.30). In the fraction of (9.4) the numerator is the energy of a dangling bond saturated by a surfactant, and the denominator that of an unsaturated dangling bond. Without surfactant E ss = E sc = 0 and s = 0; on the other hand, for perfectly efficient saturation of dangling bonds E cc + E ss = E sc + E sc = 2E sc and s = 1. s must be positive and below unity to cause floating of the surfactant on the surface. s represents the energy parameter for the mixing of two species; for s > 1 alloying of surfactant and crystal atoms occurs [52]. The work G for surfactantmediated cluster formation (9.3) contains two counteracting terms added to the work on the pure surface G 0 . The first term −4lsγc is the edge energy of the cluster with saturated lateral dangling bonds, and the second term +4lγs is the edge energy of the surfactant atoms on top of the cluster. These terms produce a dependence of the Gibbs energy change for cluster formation on the surfactant efficiency s. This dependence is shown in Fig. 9.10 for parameters corresponding to cluster formation on the (111) surface of a metallic fcc crystal with constant supersaturation μ and a bondstrength ratio EEccss = 0.2. The model of small surface clusters consisting of individual atoms turns the smooth curve of the capillary theory in Fig. 6.9 to the curve with s = 0.0 composed of straight lines depicted in Fig. 9.10. G is maximum at the critical nucleus, which for s = 0 is also considered in Sect. 7.2.2. This maximum is the critical work G ∗ to create the critical nucleus, which contains i = i ∗ atoms; without surfactant these are only two atoms for the assumed parameters of an fcc metal surface. As the efficiency of the surfactant s increases, both G ∗ and the critical nucleus size i ∗ decrease. There is an exception for a very small efficiency s = 0.05; in such a case the edge energy of the surfactant cluster on top of the crystal cluster 4lγs is
9 Application of Surfactants
Fig. 9.10 Change of Gibbs free energy G per energy of bond strength E cc for the formation of a small cluster on the fcc(111) surface of equal crystal atoms. G/E cc depends on the efficiency s of the applied surfactant given at the curves. The insets depict the structures of the critical nuclei with blue filled circles denoting cluster atoms, the red open circles indicate atoms which convert the critical nuclei into smallest stable clusters. Reproduced with permission from [52], © 2010 Springer
Gibbs energy change ΔG / bond energy E cc
360 4
fcc lattice Δµ = 1.1E cc 2
s = 0.05 0.0 0.3 0 0.7
2
0
5 10 Number of cluster atoms
15
larger than the edge energy of the crystal cluster with inefficiently saturated dangling bonds 4lsγc . G ∗ and critical nucleus size i ∗ consequently increase. It should be noted that all these changes induced by the surfactant occur at otherwise constant growth conditions. The usually smaller critical cluster size and decreased work for critical nucleus formation leads also to a higher nucleation rate and an increased saturation nucleusdensity Ns in the presence of a surfactant. For the density Ns of surfactantmediated nucleation the relation Es Ns = Ns,0 exp −c kT
(9.5)
holds, with c = 1/(i ∗ + 2) if no significant stepedge barrier impedes the incorporation of adatoms into the nucleus (diffusionlimited case), and c = 2/(i ∗ + 3) if such a barrier exists (kinetically limited case) [51]. The energy E s contains all contributions introduced by the surfactant, ∗ − i ∗ (E de−exc − E exc ) − E d,bare − E d ; E s = −4lsγc + 4lγs + E exc
(9.6)
here the first two terms are given by the thermodynamic aspects discussed above, while the two following terms are purely kinetic ∗ barriers. They refer to the processes , exchange (E exc ) and deexchange of exchange at the edge of the nucleus E exc (E de−exc) far from the nucleus, and diffusion on the surfactantfree crystal surface E d,bare and on top of the surfactant monolayer (E d ). Since two terms are positive and two are negative, E s may have either sign. E s < 0 stimulates nucleation and promotes growth by 2D nucleation; in addition, the larger density of smaller nuclei favors layerbylayer growth and hampers secondlayer nucleation.
9.2 Models of SurfactantAssisted Epitaxy
361
9.2.3 The Diffusion—Deexchange—Passivation (DDP) Model Adatom Diffusion With DeExchange Processes The importance of adatom diffusion is emphazised in most models on surfactants. In early work the reduced adatom diffusionlength discussed for surfactantmediated epitaxy of Ge/Si in Sect. 9.1.3 was considered the reason for the suppression of 3D growth. The argument was the following: epitaxy in presence of a surfactant layer requires a site exchange of an adatom and a surfactant atom to allow for crystal growth beneath the floating surfactant layer. The energy barrier for this exchange E exc was assumed to be smaller than the barrier E d for adatom diffusion on top of the surfactant layer. The diffusion length is then quite small and limited by the exchange process: underneath the surfactant layer the atom cannot diffuse. The short diffusion length leads to a high density of nucleating 2D islands. Consequently these islands coalesce before secondlayer islands nucleate. Thereby growth proceeds layerbylayer, and 3D growth is suppressed. While this explanation appears reasonable it was found to be incomplete. It turned out that also the reverse process—the deexchange—is important for describing experimental findings. The energy barrier E de  exc for a crystal atom on the topmost crystal layer to become an adatom on top of the surfactant layer is significantly larger than E exc and E d . Still a rough estimate shows that such a process can affect the growth process [17]. Analogous to (7.6) the time scale corresponding to a kinetic process with energy barrier E is given by ν −1 exp(−E/(kT )), where ν is the attempt rate, here typically on the order of 1013 s−1 . E de  exc = 1.6 eV at a typical growth temperature T = 600 °C yields a characteristic time of 0.2 ms; this time is much shorter than the growth rate for a monolayer, being typically larger than one second. A deexchange process therefore usually occurs before another crystal atom binds the buried atom permanently to the growing layer. The description of surfactantmediated epitaxy including the deexchange process is referred to as diffusion—deexchange—passivation (DDP) model. The combination of exchange and deexchange processes makes the effective diffusion of adatoms more complex. The effective diffusion coefficient Deff is related to the diffusion coefficient Dbare and the related energy barrier E d,bare for bare adatom diffusion without surfactant by [13]
Deff
exp (E d,bare − E d )/(kT ) . = Dbare 1 + exp((E de  exc − E exc )/(kT ))
(9.7)
The ratio of E d and E exc does hence not provide an information whether Deff is smaller than Dbare or larger. If the surfactant passivates the surface, then E d,bare > E d and E de  exc > E exc ; which of the energy differences in (9.7) is larger cannot be decided a priori. First principles DFT calculations for surfactantcovered Si(111) yield E de  exc − E exc = 0.8 eV, while the difference of E d,bare − E d is much smaller
362
9 Application of Surfactants
[13]; this results in Dbare Deff , and hence a decreased diffusivity in presence of the surfactant. It should be noted that a less efficient passivation of the surface may reverse the ratios and the diffusion length could be increased; since a decreased diffusivity in presence of the surfactant may also occur for E exc > E d , a surfactant can simultaneously increase the diffusivity on top of a surfactant layer and decrease the effective diffusivity. Passivation of Island Edges Kinetic MonteCarlo simulations in the DDP model indicate that the effective diffusion expressed by the coefficient Deff is actually not the relevant process for inducing either 2D or 3D growth: two different surfactants leading to the same value of Deff may induce different growth modes [13, 17]. These studies show that the crucial effect of a surfactant is the passivation of step edges. These edges occur at terraces of vicinal surfaces (Fig. 7.22) and also at the perimeter of nucleated 2D islands, see Sect. 7.2. The passivation of a step edge can be accounted for by an increased energy barrier E det for the detachment of an atom, which after an exchange process has been attached to a 2D island underneath the surfactant layer. The detachment requires the breaking of lateral bonds; in the simulation described below this process is allowed if only a single lateral bond has to be broken. The result of such a kinetic MonteCarlo simulation for different detachment energies in homoepitaxy is shown in Fig. 9.11; for simplicity a simple cubic lattice is assumed. The simulations have equal parameters determining the adatom diffusion and differ only in the detachment energy. If the detachment process is suppressed by a respective high barrier (Fig. 9.11a) deposition of 0.15 monolayer leads to a high density of islands, and rough edges are formed at the islands. When the detachment is enabled the island density is substantially decreased and the island edges are faceted (Fig. 9.11b). In Fig. 9.11a, b E d < E exc was assumed. It must be noted that similar results may be obtained for a parameter set with E d > E exc and appropriately chosen E de  exc and E det [13]: island densities and shapes are not significantly affected. The results of homoepitaxy simulation are in agreement with experimental observations. Surfactants which suppress 3D growth increase the island density; also rough island edges and an increase of island density at the expense of their size at lower temperature are observed for Si homoepitaxy [14]. In the simulation the increased island density does not originate from a reduced diffusivity, but from the ability for adatoms to detach again from an island edge and subsequently nucleate on a flat part of the surface. In heteroepitaxy strain is more efficiently elastically relaxed in 3D growth than in 2D growth, yielding a driving force for the formation of 3D islands. For 3D growth atoms must get detached from the island edge and migrate to the top of the island. If this detachment is suppressed by the presence of surfactant atoms the islands will grow wide and flat, i.e., in the layerbylayer mode. Still strain affects growth; its effect is included in the simulation of Fig. 9.11c, d by assuming an altered bond strength in the strained islands. Consequently also the activation energy for the detachment of atoms from island edges is affected by strain; the other barriers are less affected and kept constant. For the detachment energy a dependence on the island
9.2 Models of SurfactantAssisted Epitaxy
363
(a)
(b)
(c)
(d)
Fig. 9.11 Shape of 2D islands according to kinetic MonteCarlo simulations of surfactantmediated epitaxy with (a, c) and without (b, d) a passivation of the island edges; the initially flat substrate surface is white. a Homoepitaxy at 600 °C with activation energies E d = 0.5eV, E exc = 0.8eV, E de−exc = 1.6eV, and edge passivation enforced by E det = 3.0eV. b Same as a but with E det = 1.6eV to enable atom detachment at edges. c Heteroepitaxy of 1 ML at 300 °C with same energies as in a but f = 4%. d Same as c but with E det as in b; colors indicate different surface heights; blue, yellow, and green indicate 1, 2, and 3 ML height. Reproduced with permission from [13], © 2000 Academic Press
size was assumed, according to the elastic strain energy of rectangular islands with lateral lengths l1 and l2 [53]: E det = ε0 + ε1
ln l1 ln l2 ; + l1 l2
(9.8)
here ε0 = E de  exc for surfactants passivating island edges and ε0 = 0 without such passivation; ε1 is set to 3.0 eV in the simulations of Fig. 9.11c, d. The simulation without islandedge passivation Fig. 9.11d shows 3D growth with islands up to 7 ML height after deposition of 1 ML and still large uncovered areas of the substrate, while islanding is suppressed for passivated island edges (Fig. 9.11c); the latter surface is covered with 1 ML of the deposit, with some small holes (white) and some small 1 ML high islands (yellow) on top. Similar to homoepitaxy no
364
9 Application of Surfactants
significant changes occur when a parameter set with E d > E exc is applied instead of E d < E exc . The simulated surfactantmediated 2D growth at low temperature changes quite abruptly to 3D growth at higher temperature with a transition around 400 °C for the given parameters; such a transition is experimentally observed for Sbmediated Ge/Si(111) epitaxy [15, 16] and was studied in detail for Bimediated Ge/Si(111) epitaxy [54]. The size of islands nucleating during epitaxy usually follows a distribution function with a single peak at the mean island size [55]; in addition a denuded zone is found near step edges where hardly any island nucleates. Such distributions were measured for Si islands grown by Bimediated epitaxy on Si(111) and also for Ge islands, the latter, however, only at sufficiently high temperature (480 °C) [54]; at lower temperature (440 °C) a monotonously decreasing distribution function with a maximum at very small islands is observed, and correspondingly no pronounced denuded zone is found. These findings obtained from scanning tunneling microscopy of submonolayer depositions are well described by kinetic MonteCarlo simulations based on the DDP model [54]. The temperature threshold for the Ge growth marks a transition from epitaxy limited by surface diffusion at high temperature to epitaxy limited by attachment kinetics at lower temperature, where the adatom distribution between step edges becomes uniform [56]. An analysis based on rate equations indicates that the transition originates from adatom exchange and deexchange processes [57].
9.2.4 Exchange Pathways in SurfactantMediated Epitaxy How does an adatom diffusing on a complete floating monolayer of surfactant atoms manage to exchange its site with a surfactant atom to incorporate below the surfactant? Such exchange pathways can hardly be observed experimentally and are generally studied using ab initio calculations, mostly by density functional theory in the local density approximation (DFTLDA). The atomic configurations and related activation energies are specific for any surface, participating species, and pathways. Exchange paths are quite complex and consist of sections with higherenergy saddle points and local energy minima. We consider examples of the (111) and (001) surfaces of the Ge/Si model system. For Ge/Si(001) epitaxy mediated by Sb or Bi surfactants, DFTLDA calculations identified lowenergy exchange processes where surfactant dimers are broken by adsorbed Ge atoms [58]. Most stable adsorption sites for a Ge dimer on the Si(001) surface covered with Sb dimers are illustrated in Fig. 9.12a, b, where the latter has a lower energy; the Ge dimer initially adsorbed above the trench (panel a) can move to the position above the Sb dimers below by breaking the bonds indicated by the crosses in Fig. 9.12a and rolling over to the position above the lower Sb dimer row. The Ge dimer there buckles (Fig. 9.12b) and—in a complex process—exchanges with two Sb atoms, yielding the configuration of Fig. 9.12c below an uplifted Sb dimer. There is a saddlepoint energy of 0.78 eV between the sites of panels a and b,
9.2 Models of SurfactantAssisted Epitaxy
(a)
365
(b)
(c)
Si Sb Ge
Fig. 9.12 Plan view on a Si(001) surface covered with Sb surfactant atoms (green circles) and a Ge dimer (red circles) adsorbed a above the horizontal trench between Sb dimers and b on a row of Sb dimers. c Final configuration with Ge atoms exchanged with surfactant atoms; atom sizes indicate the height above the surface. After [58]
and an exchange barrier of 1.05 eV with two local maxima between the sites of panels b and c; the total energy gain is 0.9 and 0.47 eV for a → b and b → c, respectively; for the Bi surfactant a different pathway a → c is favorable with somewhat smaller energies [58]. Diffusion and exchange processes of surfactantmediated Ge/Si(111) epitaxy were studied using ab initio molecular dynamic calculations [59] and DFTLDA [13]. A lowenergy diffusion path of a Ge adatom on Si(111) covered with 1 ML of As surfactant proceeds from a minimum position above site H3 (position Gead in Fig. 9.13) to a saddle point above a neighboring T4 site and further to a position above
T4 H3
H3 Si
Ge ad
Ge dim
Ge sub
As ad
As Fig. 9.13 Plan view on a Si(111) surface without (left part, gray lines indicate Si bonds) and with As surfactant atoms (green circles, right part); atom sizes indicate the height above the surface. The exchange process of a Ge adatom (red, Gead ) with an As surfactant atom is illustrated at the bottom right; it yields Ge on a substitutional site (Gesub ) and As on an adatom site (Asad ). After [59]
366
9 Application of Surfactants
the next H3 site (path not shown in Fig. 9.13). On the saddle point the energy is 0.25 eV higher than at position Gead ; this difference represents the barrier for diffusion E d . The path given in Fig. 9.13 illustrates an exchange process, where a Ge adatom gets incorporated under the As layer [59]: the Ge adatom approaches a saddlepoint site and then moves downwards, pushing the As adatom located on a substitutional site (above Gesub ) away. It then proceeds to the Gedim site where it forms a dimer bond to the moved As atom. Finally the Ge atom moves to a substitutional site Gesub and the As atom moves upwards to an adatom site Asad . The complex exchange path from Gead to Gesub comprises local energy maxima and minima; the highest saddle point occurs in the last step and represents the exchange energy barrier E exc = 0.7 eV [59]. Since E exc is substantially larger than E d the Ge adatom performs many diffusion steps before getting incorporated under the As layer. The large exchange barrier originates basically from strain, while the diffusion barrier is not significantly affected by strain; calculations of exchange barriers in surfactantmediated homoepitaxy Si/As/Si(111) and Ge/As/Ge(111) yield small E exc of 0.3 and 0.4 eV, respectively [59, 60]. The exchange processes for an entire Ge double layer (=1 ML) in Sbmediated Ge/Si(111) epitaxy were studied in [13]. The modelled pathway implies a concerted exchange of Ge dimers on a floating Sb monolayer as illustrated in Fig. 9.14. In the initial configuration shown in panel a the Ge layer is only threefold coordinated and the layer of the pentavalent Sb is fourfold coordinated. Arrows indicate the movement of atoms via the intermediate configuration b to the final configuration c, where all atoms are coordinated properly: Ge fourfold, and Sb threefold. Consequently the energy of this state is lower than that of the initial and of the metastable intermediate Fig. 9.14 Pathway for a concerted exchange that brings a Ge layer (red circles) on top of an Sb surfactant layer (green) on Si(111) beneath the surfactant, for a crosssectional view along ¯ . After [13] 110
Ge
(a)
As Si
(b)
(c)
9.2 Models of SurfactantAssisted Epitaxy
367
symmetry, where only half of the Ge atoms has exchanged site. The intermediate configuration is separated by saddlepoint energies from the start and end configurations, and the activation energy for such a concerted exchange was found to be only 0.8 eV [13]. This model considers a final configuration, which is ready for the deposition of the next Ge layer; the growth process can hence proceed with similar steps. The model thus provides an idea of surfactantmediated epitaxy, even if detailed studies of single exchange events may be physically more realistic.
9.3 Conclusion The beneficial effect of a surfactant on smooth epitaxial growth is evident, and also a useful effect on doping (not discussed in this chapter) was reported [61– 63]. Sill surfactants are hardly employed in device fabrication. A rare example is a Ge pchannel MOSFET fabricated on Si(111) substrate using Sbmediated MBE; the device showed a quite high channel drift mobility of 430 cm2 /Vs [64]. One reason preventing the wide application of surfactants in device production is the finite incorporation of surfactant species into the layer structure. The concentration is usually in the range of 10−3 to 10−4 , but may be substantially lower; for Sbmediated Ge/Si(111) epitaxy an incorporation below the SIMS detection limit of 2 × 1017 cm−3 was reported [65].
9.4 Problems Chapter 9 9.1 In the surfactantmediated epitaxy of Ge on Si(111) a triangular network of dislocations confined to the interface is formed, see Figs. 9.4b and 9.5. (a) Compute the lattice mismatch of Ge on Si and the remaining mismatch, if a coincident lattice with 25 planes in the Si substrate corresponds to one plane less of the Ge layer. ¯ type with Burgers vectors in the interface (b) The three dislocations of a2 110 plane dissociate in three sums of two partial dislocations D1 and D2 each, labelled in Fig. 9.5. Which of these dislocations are visible for the imaging conditions of Fig. 9.4b and which not? Which dislocations are consequently observed 81 Å apart, which are observed 40.5 Å apart? 9.2 The diffusion length of adatoms is usually decreased in presence of a surfactant; the change is described by the ratio of the diffusion coefficients for adatom diffusion on the bare surface (without surfactant) and on the surfactant layer. (a) Consider a single diffusion step of a Ge adatom on an As covered Si(111) surface along the path H3 → T4 → H3 of Fig. 9.13 with a barrier of 0.25 eV. Calculate the length ahop of one diffusion hop and the diffusion constant
368
9 Application of Surfactants
D0 for a diffusion along this path at an attempt rate of 1013 s−1 . How many diffusion hops occur in 10 ns at a temperature of 400 °C, and how long is the path for diffusion of this kind in this time? (b) For a diffusion without deexchange process the diffusion length of an adatom on a surfactant layer is limited by the (first) exchange process with a surfactant atom. Assuming Ge adatom diffusion only along the path and at the temperature given above, which diffusion length λ results for an exchange barrier of 0.7 eV? How many hops does the adatom perform on this path? (c) If deexchange processes occur, a dependence on the respective energy for deexchange enters the effective diffusion coefficient. Given the quantities above and a diffusion barrier of 0.35 eV on the bare surface (without surfactant), compute the ratio of the effective diffusion coefficient with respect to the coefficient of bare diffusion for a deexchange barrier of 1.1 eV. (d) Assume the above given values for barriers for diffusion on the bare surface and on the surfactant, and for the exchange process; compute the energy barrier for deexcitation required to obtain an effective diffusion coefficient twice as large as the coefficient of bare diffusion. 9.3 (a) Determine the approximate activation energy for Si adatom diffusion on the bare Si(111) surface and on the Sbcovered surface from the Arrhenius plot Fig. 9.3b. (b) Taking the width of the depleated zone plotted in Fig. 9.3b as the characteristic diffusion length and the activation energies determined above, calculate the diffusion length of Si on the bare Si(111) surface at 850 K and the factor g by which the diffusion length is changed when the Sb surfactant layer is introduced; calculate the temperatures for a diffusion length of 100 nm on the bare Si(111) surface and on the Sbcovered surface. 9.4 We consider a cubic Kossel model of an Sbcovered “Si(001)” surface and assume a Si–Si binding energy of 1.7 eV and corresponding Sb–Sb energy of 0.7 eV. (a) Compute the Sb–Si binding energy for a surfactant efficiency expressed by a parameter of 0.85. How much is the energy of an unsaturated dangling Si bond lowered by surfactant saturation? (b) Determine the total energy gain by surfactant passivation at the edge of a nucleus containing just a single crystal atom. Which gain results if the nucleus contains two atoms? 9.5 Application of a Te surfactant prolongates the onset of plastic relaxation of InAs on GaAs(001) as shown in Fig. 9.6. By which factor has the relaxed lattice parameter of InAs increased from 300 K to 400 °C? Which normalized lattice parameter (aInAs − aGaAs )/aGaAs has the completely relaxed InAs layer at 400 °C (in linear approximation)? Determine the actual normalized lateral
9.4 Problems Chapter 9
369
lattice parameters of InAs/GaAs and of InAs/Te/GaAs for saturated relaxation from Fig. 9.6 and compute the respective lateral strains in InAs.
9.5 General Reading Chapter 9 I.V. Markov, Crystal Growth for Beginners, 3rd edn. (World Scientific, New Jersey, 2017)
References 1. M. Copel, M.C. Reuter, E. Kaxiras, R.M. Tromp, Surfactants in epitaxial growth. Phys. Rev. Lett. 63, 632 (1989) 2. J.W. Matthews, E. Grünbaum, The need for contaminants in the epitaxial growth of gold on rocksalt. Appl. Phys. Lett. 5, 106 (1964) 3. R. Kern, G. Le Lay, J.J. Metois, Basic mechanisms in the early stages of epitaxy, in Current Topics in Materials Science, vol. 3, ed. by E. Kaldis (North Holland Publ. Co., Amsterdam, 1979), pp. 130–419, Sect. 9 4. J. Camarero, T. Graf, J.J. de Miguel, R. Miranda, W. Kuch, M. Zharnikov, A. Dittschar, C.M. Schneider, J. Kirschner, Surfactantmediated modification of the magnetic properties of Co/Cu(111) thin films and superlattices. Phys. Rev. Lett. 76, 4428 (1996) 5. J.J. de Miguel, R. Miranda, Atomic aspects in the epitaxial growth of metallic superlattices and nanostructures. J. Phys.: Condens. Matter 14, R1063 (2002) 6. Z. Zhang, M.G. Lagally, Atomicscale mechanisms for surfactantmediated layerbylayer growth in homoepitaxy. Phys. Rev. Lett. 72, 693 (1994) 7. A. Rastelli, M. Kummer, H. von Känel, Reversible shape evolution of Ge islands on Si(001). Phys. Rev. Lett. 87, 256101 (2001) 8. J. Bevk, J.P. Mannaerts, L.C. Feldman, B.A. Davidson, A. Ourmazd, GeSi layered structures: artificial crystals and complex cell ordered superlattices. Appl. Phys. Lett. 49, 286 (1986) 9. P.M.J. Marée, K. Nakagawa, F.M. Mulders, J.F. Van der Veen, K.L. Kavanagh, Thin epitaxial GeSi (111) films: study and control of morphology. Surf. Sci. 191, 305 (1987) 10. E. Kasper, H. Jorke, Growth kinetics of molecular beam epitaxy, in Chemistry and Physics of Solid, Surfaces, vol. VII, ed. by R. Vanselow, R.F. Howe (Springer, Berlin, 1988), pp. 557–582 11. M. Copel, M.C. Reuter, M. Horn von Hoegen, R.M. Tromp, Influence of surfactants in Ge and Si epitaxy on Si(001). Phys. Rev. B 42, 11682 (1990) 12. F.K. LeGoues, M. Copel, R.M. Tromp, Microstructure and strain relief of Ge films grown layer by layer on Si(001). Phys. Rev. B 42, 11690 (1990) 13. D. Kandel, E. Kaxiras, The surfactant effect in semiconductor thinfilm growth, in Solid State Physics, vol. 54, ed. by H. Ehrenreich F. Spaepen (Academic Press, San Diego, 2000), pp. 219– 262 14. B. Voigtländer, A. Zinner, T. Weber, H.P. Bonzel, Modification of growth kinetics in surfactantmediated epitaxy. Phys. Rev. B 51, 7583 (1995) 15. B. Voigtländer, A. Zinner, Surfactantmediated epitaxy of Ge on Si(111): the role of kinetics and characterization of the Ge layers. J. Vac. Sci. Technol. A 12, 1932 (1994) 16. I. Portavoce, A. Berbezier, Ronda, Sbsurfactantmediated growth of Si and Ge nanostructures. Phys. Rev. B 69, 155416 (2004) 17. D. Kandel, E. Kaxiras, Surfactant mediated crystal growth of semiconductors. Phys. Rev. Lett. 75, 2742 (1995)
370
9 Application of Surfactants
18. A. Antons, R. Berger, K. Schroeder, B. Voigtländer, Structure of steps on Aspassivated Si(111): ab initio calculations and scanning tunneling microscopy. Phys. Rev. B 73, 125327 (2006) 19. S.A. Teys, Different growth mechanisms of Ge by StranskiKrastanow on Si (111) and (001) surfaces: an STM study. Appl. Surf. Sci. 392, 1017 (2017) 20. M. Hornvon Hoegen, F.K. LeGoues, M. Copel, M. C. Reuter, R. M. Tromp, Defect selfannihilation in surfactantmediated epitaxial growth. Phys. Rev. Lett. 67, 1130 (1991) 21. M. Hornvon Hoegen, Surfactants: perfect heteroepitaxy of Ge on Si(111). Appl. Phys. A 59, 503 (1994) 22. M. Kammler, M. Hornvon Hoegen, Transition in growth mode by competing strain relaxation mechanisms: surfactant mediated epitaxy of SiGe alloys on Si. Appl. Phys. Lett. 85, 3056 (2004) 23. F.K. LeGoues, M. Hornvon Hoegen, M. Copel, R.M. Tromp, Strainrelief mechanism in surfactantgrown epitaxial germanium films on Si(111). Phys. Rev. B 44, 12894 (1991) 24. D. Leonard, K. Pond, P.M. Petroff, Critical layer thickness for selfassembled InAs islands on GaAs. Phys. Rev. B 50, 11687 (1994) 25. N. Grandjean, J. Massies, V.H. Etgens, Delayed relaxation by surfactant action in highly strained IIIV semiconductor epitaxial layers. Phys. Rev. Lett. 69, 796 (1992) 26. J. Massies, N. Grandjean, Surfactant effect on the surface diffusion length in epitaxial growth. Phys. Rev. B 48, 8502 (1993) 27. G.L. Price, Criticalthickness and growthmode transitions in highly strained Inx Ga1−x As films. Phys. Rev. Lett. 66, 469 (1991) 28. N. Grandjean, J. Massies, Epitaxial growth of highly strained Inx Ga1−x As on GaAs(001): the role of surface diffusion length. J. Crystal Growth 134, 51 (1993) 29. E. Tournié, A. Trampert, K.H. Ploog, Interplay between surface stabilization, growth mode and strain relaxation during molecularbeam epitaxy of highly mismatched IIIV semiconductor layers. Europhys. Lett. 25, 663 (1994) 30. W.N. Rodrigues, V.H. Etgens, M. SauvageSimkin, G. Rossid, F. Sirotti, R. Pinchaux, F. Rochet, Heteroepitaxial growth of InAs on GaAs(100) mediated by Te at the interface. Solid State Commun. 95, 873 (1995) 31. D.F. Storm, M.D. Lange, T.L. Cole, Surfactant effects of thallium in the epitaxial growth of indium arsenide on gallium arsenide(001). J. Appl. Phys. 85, 6838 (1999) 32. G. Feng, K. Oe, M. Yoshimoto, Temperature dependence of Bi behavior in MBE growth of InGaAs/InP. J. Crys. Growth 301, 121 (2007) 33. Y. Gu, Y.G. Zhang, X.Y. Chen, S.P. Xi, B. Du, Y.J. Ma, Effect of bismuth surfactant on InPbased highly strained InAs/InGaAs triangular quantum wells. Appl. Phys. Lett. 107, 212104 (2015) 34. W.Y. Ji, Y. Gu, Y.G. Zhang, Y.J. Ma, X.Y. Chen, Q. Gong, B. Du, Y.H. Shi, InPbased pseudomorphic InAs/InGaAs triangular quantum well lasers with bismuth surfactant. Appl. Opt. 56, H10 (2017) 35. Y. Zhong, P.B. Dongmo, J.P. Petropoulos, J.M.O. Zide, Effects of molecular beam epitaxy growth conditions on composition and optical properties of Inx Ga1−x Biy As1−y . Appl. Phys. Lett. 100, 112110 (2012) 36. D. Rioux, H. Höchst, Sb/InP(100) interface: a precursor to surfactantmediated Ge epitaxy. Phys. Rev. B 46, 6857 (1992) 37. R.R. Wixom, N.A. Modine, G.B. Stringfellow, Theory of surfactant (Sb) induced reconstructions on InP(001). Phys. Rev. B 67, 115309 (2003) 38. D. Rioux, H. Höchst, Enhanced structural and electronic properties of strained Ge(100) films grown by molecularbeam epitaxy with a Sb surfactant layer. J. Vac. Sci. Technol. A 10, 759 (1992) 39. G. Mula, C. Adelmann, S. Moehl, J. Oullier, B. Daudin, Surfactant effect of gallium during molecularbeam epitaxy of GaN on AlN (0001). Phys. Rev. B 64, 195406 (2001) 40. J.E. Northrup, C.G. Van de Walle, Indium versus hydrogenterminated GaN(0001) surfaces: Surfactant effect of indium in a chemical vapor deposition environment. Appl. Phys. Lett. 84, 4322 (2004)
References
371
41. Q. Zhuang, W. Lin, J. Kang, Effect of Inadlayer on AlN (0001) and (0001) polar surfaces. J. Phys. Chem. C 113, 10185 (2009) 42. H. Chen, R.M. Feenstra, J.E. Northrup, T. Zywietz, J. Neugebauer, D.W. Greve, Surface structures and growth kinetics of InGaN(0001) grown by molecular beam epitaxy. J. Vac. Sci. Technol. B 18, 2284 (2000) 43. S. Nicolay, E. Feltin, J.F. Carlin, M. Mosca, L. Nevou, M. Tchernycheva, F.H. Julien, M. Ilegems, N. Grandjean, Indium surfactant effect on AlN/GaN heterostructures grown by metalorganic vaporphase epitaxy: applications to intersubband transitions. Appl. Phys. Lett. 88, 151902 (2006) 44. J.L. Merrell, F. Liu, G.B. Stringfellow, Effect of surfactant Sb on In incorporation and thin film morphology of InGaN layers grown by organometallic vapor phase epitaxy. J. Cryst. Growth 375, 90 (2013) 45. A.A. Gokhale, T.F. Kuech, M. Mavrikakis, A theoretical comparative study of the surfactant effect of Sb and Bi on GaN growth. J. Cryst. Growth 303, 493 (2007) 46. R. Kern, P. Müller, Threedimensional towards twodimensional coherent epitaxy initiated by surfactants. J. Cryst. Growth 146, 193 (1995) 47. E. Bauer, Phänomenologische Theorie der Kristallabscheidung an Oberflächen. Z. Krist. 110, 372 (1958) (Theory of crystalline deposition on surfaces, in German) 48. L.G. Wang, P. Kratzer, N. Moll, M. Scheffler, Size, shape, and stability of InAs quantum dots on the GaAs(001) substrate. Phys. Rev. B 62, 1897 (2000) 49. J.E. Prieto, I. Markov, StranskiKrastanov mechanism of growth and the effect of misfit sign on quantum dots nucleation. Surf. Sci. 664, 172 (2017) 50. I.V. Markov, Kinetics of nucleation in surfactantmediated epitaxy. Phys. Rev. B 53, 4148 (1996) 51. I.V. Markov, Influence of surface active species on kinetics of epitaxial nucleation and growth. Mater. Chem. Phys. 49, 93 (1997) 52. I.V. Markov, Nucleation at surfaces, in Handbook of Crystal Growth, ed. by G. Dhanaraj, K. Byrappa, V. Prasad, M. Dudley (Springer, Berlin, 2010), pp. 17–52 53. J. Tersoff, R.M. Tromp, Shape transition in growth of strained islands: spontaneous formation of quantum wires. Phys. Rev. Lett. 70, 2782 (1993) 54. V. Cherepanov, S. Filimonov, J. Mysliveˇcek, B. Voigtländer, Scaling of submonolayer island sizes in surfactantmediated epitaxy of semiconductors. Phys. Rev. B 70, 085401 (2004) 55. M.C. Bartelt, J.W. Evans, Scaling analysis of diffusionmediated island growth in surface adsorption processes. Phys. Rev. B 46, 12675 (1992) 56. I.V. Markov, Nucleation and stepflow growth in surfactant mediated homoepitaxy with exchange/deexchange kinetics. Surf. Sci. 429, 102 (1999) 57. D. Wang, Z. Ding, X. Sun, Nucleation transition and nucleus density scaling in surfactantmediated epitaxy. Phys. Rev. B 72, 115419 (2005) 58. E.Z. Liu, C.Y. Wang, J.T. Wang, Dimerbreakingassisted exchange mechanism in surfactantmediated epitaxial growth of Ge on Si(001): ab initio total energy calculations. Phys. Rev. B 76, 193301 (2007) 59. K. Schroeder, A. Antons, R. Berger, S. Blügel, Surfactant mediated heteroepitaxy versus homoepitaxy: kinetics for groupIV adatoms on Aspassivated Si(111) and Ge(111). Phys. Rev. Lett. 88, 046101 (2002) 60. K. Schroeder, B. Engels, P. Richard, S. Blügel, Reexchange controlled diffusion in surfactantmediated epitaxial growth: Si on Asterminated Si(111). Phys. Rev. Lett. 80, 2873 (1998) 61. A.D. Howard, G.B. Stringfellow, Effects of low surfactant Sb coverage on Zn and C incorporation in GaP. J. Appl. Phys. 102, 074920 (2007) 62. J. Zhu, F. Liu, G.B. Stringfellow, Enhanced cationsubstituted ptype doping in GaP from dual surfactant effects. J. Cryst. Growth 312, 174 (2010) 63. L.B. Karlina, A.S. Vlasov, B.Y. Ber, D.Y. Kazantsev, Diffusion of zinc in gallium arsenide with the participation isovalent impurities. J. Cryst. Growth 432, 133 (2015)
372
9 Application of Surfactants
64. D. Reinking, M. Kammler, N. Hoffmann, M. Hornvon Hoegen, K.R. Hofmann, Fabrication of highmobility Ge pchannel MOSFETs on Si substrates. Electron. Lett. 35, 503 (1999) 65. D. Reinking, M. Kammler, M. Hornvon Hoegen, K.R. Hofmann, High electron mobilities in surfactantgrown Ge on Si substrates. Jpn. J. Appl. Phys. 36, L1082 (1997)
Chapter 10
Doping, Diffusion, and Contacts
Abstract The ability to control the conductivity is an essential feature of semiconductors. This chapter points out the basics for the control of the free carrier concentration and discusses the nature of limiting factors. The integrity of doping profiles and of interfaces in heterostructures depends on the stability of atoms against a change of lattice site. We briefly consider fundamentals of diffusion and discuss some basic mechanisms governing the diffusivity of atoms in a crystal. The chapter concludes with concepts for ohmic metalsemiconductor contacts.
Device applications of semiconductors require control of the free carrier concentration and application of ohmic contacts for carrier injection or extraction. The conductivity of a semiconductor can be varied over a wide range from semiinsulating to semimetallic by the introduction of impurities. The substitutional replacement of a semiconductor atom by, e.g., a dopant atom with a chemical valence incremented by one introduces an additional electron and a positive charge at the ion core. For suitable dopant species the electron may thermally be released at room temperature due to a small binding energy, allowing for adjusting the conductivity via the concentration of impurities. The same applies for the creation of free holes by substitutional dopants with a lower chemical valence. The simple concept works particularly well for low doping levels and many semiconductors with a bandgap below about 2 eV. Section 10.1 points out the essentials for conductivity control, limits imposed by thermodynamics, and the nature of limiting factors. Doping profiles are often created via diffusion by providing a concentration gradient of the doping species. Diffusion phenomena also control the abruptness of semiconductor interfaces. The underlying concepts are treated in Sect. 10.2. Ohmic contacts are usually fabricated by evaporation of a contact metal on heavily doped semiconductor layers. Besides such nonepitaxial techniques also epitaxial contact structures may provide a solution in special cases. Basic concepts for ohmic metalsemiconductor contacts are discussed in Sect. 10.3.
© Springer Nature Switzerland AG 2020 U. W. Pohl, Epitaxy of Semiconductors, Graduate Texts in Physics, https://doi.org/10.1007/9783030438692_10
373
374
10 Doping, Diffusion, and Contacts
10.1 Doping of Semiconductors The use of semiconductors in electronic and optoelectronic devices requires the reliable control of unipolar or bipolar conductivity. Typical concentrations of impurities employed for doping are in the 1015 –1020 cm−3 range, compared to about 5 × 1022 atoms/cm3 of the host semiconductor. Doping of shallow impurities for both, donors and acceptors is usually well achieved for semiconductors with a sufficiently small bandgap energy such as Si. In contrast, widebandgap semiconductors with a gap energy above ∼2 eV like, e.g., many II–VI compounds and groupIII nitrides can typically be doped either ntype or ptype, but not both. It is exceedingly difficult to achieve ntype conductivity in ZnTe or ptype conductivity in ZnO. Fundamental problems arise from various origins. The solubility of dopants imposes limits for incorporation, a large ionization energy may hamper activation, native defects may compensate an intentional doping, dopants may change their character depending on the incorporation site or lattice relaxation, and eventually hydrogen may passivate dopants. Many of these processes are related to the bandgap energy, and are hence particularly pronounced in wide bandgap semiconductors. The effect is illustrated in Fig. 10.1 for the compensation of ptype doping by a native donor defect. The intentional ptype doping moves the Fermi level E F to the valenceband edge E v . The creation of a point defect made of host atoms like, e.g., an interstitial atom consumes some formation energy, but the transfer of the electron from its occupied donor level E defect near the conduction band E c to the Fermi level may recoup this energy. Since the energy gained by such a compensation is on the order of the bandgap energy, the tendency for native defect compensation increases as the bandgap increases. Dopant incorporation during epitaxial growth may occur far from thermal equilibrium, potentially allowing to achieve a net doping which cannot be achieved under equilibriumnear conditions. In the following we treat basic concepts to obtain conductivity control.
Fig. 10.1 Compensation of ptype doping by a native donor defect, which introduces an occupied level E defect near the conduction band
E Ec Edefect
EF Ev
10.1 Doping of Semiconductors
375
10.1.1 Thermal Equilibrium CarrierDensities The density of electrons n in the conduction band at temperature T is given by the FermiDirac distribution function f n and depends on the density of energy levels in the conduction band Dc (E) and the value of the Fermi energy E F , n=
∞ Ec
Dc (E)
1 d E. e(E−EF )/kB T + 1
(10.1)
The Fermi energy E F of charge carriers is also referred to as chemical potential μ. A similar expression as (10.1) holds for the density of holes p in the valence band with densityofstates Dv and a distribution function f h = 1 − f n , p=
Ev
−∞
Dv (E) 1 −
1 e(E−EF )/kB T + 1
d E.
(10.2)
Equations (10.1) and (10.2) are simplified, if the position of the chemical potential is not in the vicinity of one of the band edges, i.e., if conditions E c − E F kB T or E F − E v kB T hold, respectively. Such semiconductors are called nondegenerate. The Fermi distribution may then be replaced by the Boltzmann distribution by omitting the term “+1” in the denominator. Due to the exponential factors in the simplified integrals only energies within kB T at the band edges give significant contributions. The band edges are then well described by a quadratic approximation, yielding the density of states √ ∗ 3/2 2m e,h E − E c,v  (10.3) Dc,v (E) = 3 π 2 with the effective masses of electrons m ∗e and holes m ∗h . The effective masses include potentially occurring degeneracy and anisotropy. For Si, e.g., the conduction band is 6fold degenerate and comprises longitudinal and transversal mass components, yielding m ∗e = 62/3 × (m 2t × m l )1/3 . Similarly, the hole mass includes heavyhole and lighthole contributions (the splitoff hole is usually not occupied), yielding 3/2 3/2 m ∗h = (m hh + m lh )2/3 . Using the density of states (10.3), (10.1) and (10.2) for the carrier densities read m ∗e kB T 3/2 −(Ec −EF )/kB T n=2 e = Dceff e−(Ec −EF )/kB T , 2π 2 ∗ m h kB T 3/2 −(EF −Ev )/kB T e = Dveff e−(EF −Ev )/kB T . p=2 2π 2
(10.4a) (10.4b)
The prefactors of the exponential functions in (10.4a), (10.4b) are the effective densities of states at the edges of conduction and valence bands Dceff and Dveff , respectively. The dependence on the until now unknown position of the chemical potential disappears from the product of the carrier densities,
376
10 Doping, Diffusion, and Contacts
kB T n×p=4 2π 2
3 3/2 ∗ ∗ me mh e−Eg /kB T ,
(10.5)
where E g = E c − E v is the bandgap energy. This relation is called the law of mass action and applies for nondegenerate semiconductors. It means that at a given temperature the density of one carrier type is given by the density of the other. The position of the Fermi energy E F within the bandgap follows from (10.4a), (10.4b). If we resolve (10.4a) for E c − E F we obtain Dceff . E c − E F = kB T ln n
(10.5a)
In devices the electron density n, and consequently E F , is controlled by doping and basically given by the density of ionized donors ND and acceptors NA , i.e., n ≈ ND − NA . But also in an undoped semiconductor the Fermi level is not fixed. If in a pure crystal the contribution of impurity donors or acceptors to the carrier densities is negligible, the semiconductor is called intrinsic. In this case each electron in the conduction band originates from the valence band, n = p ≡ n i . The value of the intrinsic carrier density n i at any temperature is given by the square root of (10.5). We note that the intrinsic carrier concentration decreases exponentially as the bandgap increases. At T = 300 K we find values of, e.g., Ge (E g = 0.67 eV, n i ≈ 1013 cm−3 ), Si (1.12 eV, ∼1010 cm−3 ), GaAs (1.43 eV, ∼106 cm−3 ), and GaP (2.26 eV, ∼100 cm−3 ), illustrating the trend. In the intrinsic case the position of the chemical potential, E F , follows from the charge neutrality condition n = p and (10.1), (10.2), yielding EF = Ev +
∗ Eg 3 mh (intrinsic case). + kB T ln 2 4 m ∗e
(10.6)
At T = 0 the chemical potential lies in the middle of the energy gap. Since m ∗h is typically less than an order of magnitude larger than m ∗e , the last term in (10.6) is of order kB T . This is usually much less than E g , leading to a near midgap position of E F at finite temperatures. To control conductivity impurities are introduced in the crystal as sources of free carriers. The semiconductor is then called extrinsic. For efficient doping the energy level introduced by a dopant should lie in the bandgap near the band edge to allow for thermal activation at the intended operating temperature. Such impurities are referred to as shallow impurities. In a nondegenerate semiconductor the density of band states Dv (E) or Dc (E) is not considerably altered by doping. Shallow donor impurities are well described in analogy to a hydrogen atom. A substitutional donor has a higher chemical valence than the replaced host atom. A single donor introduces a positive charge at the ion core and an additional electron. The binding energy of the electron is strongly reduced compared to the Rydberg energy R∞ = 13.6 eV of hydrogen due to the electron motion in the medium of the semiconductor with a dielectric constant εr . Replacing in the hydrogen problem ε0
10.1 Doping of Semiconductors
377
by ε = εr ε0 , εr being the (relative) permittivity of the semiconductor, and the free electron mass m 0 by the effective mass m ∗e , we obtain the binding energy of the donor electron in the ground state
E Db =
m ∗e 1 × R∞ . m 0 εr2
(10.7)
E Db is also referred to as donor Rydberg energy or donor ionization energy. The position of the donor energy in the bandgap is E D = E g − E Db . Taking typical values m ∗e ≈ m 0 /10 and εr ≈ 10 we obtain binding energies of the order 10 meV. Donors which fulfill the approximation (10.7) are referred to as effectivemass donors. The effectivemass and dielectric constant corrections lead to a donor Bohr radius aB∗ =
εr m ∗e × aB , m0
(10.8)
with the hydrogen Bohr radius aB = 0.53 Å. Inserting typical values noted above yields an order of 50 Å. The electron orbit hence extends over many lattice constants. In such a case the description of a donor Coulomb potential screened by the effective dielectric constant εr is a good approximation. The usually small differences found for different shallow donors, termed chemical shift, are accounted for by a centralcell correction to the Coulomb potential. An acceptor impurity has a lower chemical valence than a host atom. The missing electron is represented by a hole, which is bound to the excess negative charge of the acceptor core. An application of the hydrogen analogy to a shallow acceptor impurity must account for the more complicated structure of the valence band (Sect. 4.1). The dispersion of holes near the center of the Brillouin zone of semiconductors with zincblende or diamond structure is often described by the Luttinger parameters γ1 , γ2 , and γ3 [1]. 1/γ1 is a multiplying factor (of order 10−1 ) in the acceptor bindingenergy E Ab described analogous to (10.7) for the light and heavy holes. To obtain the acceptor ionizationenergy an additional multiplication by a function f (γ1 , γ2 , γ3 ) is required, f covering values between 1 and 5. A more detailed treatment is given, e.g., in [2]. Rydberg energies of some dopants in semiconductors are given in Table 10.1. We restrict ourselves to ntype doping with shallow donors to discuss the effect of doping. Electrons in the conduction band originate either from ionized donors or from the valence band, n = ND+ + p. ND+ denotes the density of positively charged donors, which lost their electron by thermal activation. The value follows from the total density of donors ND and an electron occupation of donors depending on the activation energy E Db . Furthermore, the degeneracy g for the occupation of the donor groundstate must be included in the Fermi distributionfunction, yielding ND+ = ND 1 −
1 1 (E D −E F )/kB T e g
+1
(only donors).
(10.9)
378
10 Doping, Diffusion, and Contacts
Table 10.1 Binding energies of donors (E Db ) and acceptors (E Ab ) in Si, GaAs (donor data from [3], CGa and acceptors from [4]), GaN (donor data from [5], acceptor data from [6], lowdoping limits), and ZnSe (donor data from [7], acceptor data from [8], Lii from [9]) Host Bandgap E g Donor Rydberg E Db (meV) Acceptor Rydberg E Ab (meV) (eV) Si
1.12
GaAs
1.42
GaN ZnSe
3.42 2.67
PSi AsSi SbSi SAs TeAs SnGa CGa SiGa AlZn GaZn InZn Lii
45 49 39 5.9 5.8 5.8 5.9 ∼22 25.7 27.5 28.2 ∼26
BSi AlSi GaSi BeGa MgGa ZnGa CAs MgGa NSe PSe AsSe LiZn
45 5745 65 28 29 31 27 ∼208 ∼110 ∼87 ∼105 ∼114
For effectivemass donors g = 2 due to an occupation with an electron of either spin (up or down). We now consider the semiconductor at low temperature and neglect the small intrinsic contribution of p electrons, i.e., n i ND+ , yielding n = ND+ (low temperature).
(10.10)
At low temperature most donors are not ionized, and the occupation of the conduction band is described by Boltzmann statistics used in (10.4a). We hence may express the chemical potential in (10.9) by e EF /kB T = n/Dceff e Ec /kB T .
(10.11)
This leads to a quadratic equation for the free carrier concentration n2 + with the solution
1 eff −EDb /kB T 1 b D e n − Dceff e−ED /kB T ND = 0 g c g
n = 2ND 1 +
ND b 1 + 4g eff e ED /kB T Dc
−1
.
(10.12)
(10.13)
In the limit of very low temperatures the condition 4g(ND /Dceff )e ED /kB T 1 applies. Equation (10.13) then simplifies to b
10.1 Doping of Semiconductors
n∼ =
379
b (1/g)ND Dceff e−ED /2kB T (ionization regime).
(10.14)
In this lowtemperature range sufficient donors still have their electron and may be ionized if the temperature is increased. The ionization energy can be derived from the slope of an Arrhenius plot of the carrier density versus reciprocal temperature, see Fig. 10.2. From (10.14) we obtain E Db = −2kB d(ln n)/d(1/T ). Once all donors are ionized, the carrier density saturates. n is given by the donor concentration and remains constant, independent on temperature, n = ND+ = ND (saturation regime).
(10.15)
As the temperature is further increased the carrier concentration again raises due to a thermal activation of electrons from the valence band. The intrinsic carrier concentration increases with a much steeper slope −E g /2kB in the Arrhenius plot given in Fig. 10.2. In this hightemperature range we hence find n ∝ e−Eg /(2kB T ) (intrinsic regime).
(10.16)
Fig. 10.2 Arrhenius plot of the carrier concentration n in the conduction band of an uncompensated ntype semiconductor. n i denotes the contribution of intrinsic carriers
Carrier concentration log(n)
Pure doping of solely one kind of carriers does hardly occur. In practice dopant atoms of one kind are partially compensated by a smaller number of dopants of the other kind. Let us assume donors with a concentration ND being partially compensated by residual acceptors with concentration NA . Since acceptors provide lowenergy states for donor electrons, even at lowest temperatures all acceptors are ionized, i.e. NA− = NA . Consequently the number of donors which may release their electron to the conduction band is reduced by this number, yielding instead of (10.10) now n = ND+ − NA− . The most evident change in the free carrier concentration n is given by a decrease of the plateau in the saturation regime to the value n = ND − NA . Furthermore, for a given carrier concentration the mobility is reduced in a compen
Intrinsic regime n
exp(Eg/(2kBT ))
Saturation regime
Ionisation regime n
exp(EDb /(2kBT ))
ni
Reciprocal temperature 1/T
380
10 Doping, Diffusion, and Contacts
sated semiconductor due to additional scattering at ionized dopants. An additional effect is the appearance of a second ionization regime with a slope −E Db /kB instead of −E Db /2kB in the Arrhenius plot at the lowtemperature end.
10.1.2 Solubility of Dopants Doping of a semiconductor host with impurities requires a sufficiently high solubility for the introduction on the intended lattice site. The solubility of a dopant is inherently connected to the dissociation of the impurity atom into an ionized state and a carrier, and is therefore associated with the Fermi level [10]. If, e.g. a donor atom is introduced, energy is gained by incorporating the electron of the donor at the Fermi level. The energy gain decreases at higher doping concentration, because the Fermi level increases by doping. A comparable situation occurs for acceptors. Low dopant concentrations are therefore more readily achieved than high concentrations, and the problem gets increasingly severe as the bandgap energy increases. Incorporation of the dopant at other sites than intended may then get more favorable, and even the formation of phases composed of impurity and host atoms with a configuration deviating from that of the semiconductor may occur. The creation of a defect is generally connected to the incorporation or removal of atoms from other parts of the crystal, its surface, or the environment. Since this finding and the treatment below apply for both, impurities and native defects, we will just denote them defects in the following. The creation—or annihilation—of a defect is considered by a coupling to subsystems or reservoirs, which donate or accept atoms and, in case of charged defects, also electrons. The equilibrium is described by respective chemical potentials. We consider the introduction of an impurity by connecting the semiconductor to a reservoir of dopant atoms. The probability of incorporation is related to the formation energy of a respective defect in the crystal. In thermal equilibrium the concentration [Di ] of the dopant (or any defect) in the semiconductor is given by
q
q E form (Di ) q . Di = N exp − kB T
(10.17)
E form (Di ) is the formation energy of the defect Di in the charge state q. N is the number of sites where the defect can form, e.g., the number of substitutional cation A sites of an AB compound semiconductor in case of dopant incorporation of this site. The defectformation energy depends on the chemical potential of the species involved in the creation of the defect and the change of Gibbs free energy required to create the defect. An additional term accounts for the charge of the defect. The general expression reads
10.1 Doping of Semiconductors
381
q q E form Di = G form Di + n j μ j (reservoir) + q E F ,
(10.18)
j
where q is the charge state (e.g., −1) and E F is the Fermi energy with respect to the valenceband edge E v . The index j in the sum of (10.18) goes over all chemical species involved in the defect creation. The number n j of species j is positive if an atom is removed from the semiconductor and negative if it is added. μ j are the respective chemical potentials. The energy to substitute, e.g., a negatively charged Li acceptor for Zn in a ZnSe semiconductor reads − E form Li− Zn = G form LiZn + μZn − μLi − E F . q
The change of Gibbs free energy G form (Di ) is given by q G form Di = E 0 − T S + PV,
(10.19)
E 0 being the difference between the electronic groundstate energy of the system with and without the defect. Correspondingly S and V are the respective entropy and volume changes due to the creation of the defect. The contributions related to a volume change and the entropy change are usually expected to yield only minor corrections and are not considered. A positive sign of G form denotes an energy cost to create the defect. The charge state of the defect will be that with lowest formation energy. Depending on E F the defect may be in different charge states. The energy where the defect changes the charge state from q to q is referred to as chargetransfer energy E q/q . Figure 10.3 illustrates how the formation energy depends on the charge state q and the Fermi energy E F , which is varied between valence and conduction band. In the example given in Fig. 10.3 the defect is negatively charged if E F lies above E 0/− , because in this range E f or m (D − ) < E form (D 0 ). Below E 0/− the defect is in its neutral charge state. The level in the bandgap E 0/− is the value of the Fermi energy at which the two charge states E form (D 0 ) and E form (D − ) have the same energy. The quantities noted in the equations above are accessible by firstprinciples calculations. The electrical interaction of the defect is treated analogous to the chemical interaction of atoms with their atomic reservoirs: The defect donates or accepts elec
Fig. 10.3 Formation energy of a defect in a neutral and a negative charge state. The Fermi level E F is varied between the energy of the valence band E v and the conduction band E c
Eform
q=0 q = 1 Ev
E
0/–
E c EF
382
10 Doping, Diffusion, and Contacts
trons from the electron reservoir of the semiconductor. A negative charge denotes that the defect accepts q electrons. The position of the Fermi energy is calculated selfconsistently by applying (10.18) for all relevant defects and accounting for the condition of charge neutrality net charge = 0 = p − n −
q n ielectron Di .
(10.20)
i
p and n are the hole and electron densities, and n ielectron is the number of excess q electrons in the defect Di . Details of the computational approach are given in [11] for the example of ZnSe doping. Within this framework performed in a supercell geometry the change of Gibbs free energy G form in (10.18) is the total energy of a supercell containing the defect minus the energy of a supercell of the pure bulk semiconductor. For an elementary semiconductor like Si the chemical potential, μSi , is fixed, while for an AB compound semiconductor this applies for the sum of the constituents μ AB = μ A + μ B , leaving an individual summand variable. Bounds on chemical potentials arise from the phases that can be formed by the constituents. For the host atoms the upper bound is given by formation of the respective elements. In ZnSe, e.g., μmax Zn = μZn(bulk) : Further increase above this level will preferentially lead to the formation of Zn metal. The same applies for μmax Se . A lower bound is imposed by the heat of formation Hform of the semiconductor and the fixed sum of the chemical potentials noted above. For our example we obtain μZnSe = μZn(bulk) + μSe(bulk) + Hform (ZnSe), yielding μmin Zn = μZn(bulk) + Hform (ZnSe). Note that Hform < 0 for the stable semiconductor. For the dopant the various compounds which the impurity can form including host atoms must be considered. For the example of a ptype doping of ZnSe using Li the most stringent bound is found to be given by the formation of the LiSe2 compound [12], yielding the constraint on the chemical potential 2μLi + μSe = μLi2 Se = 2μLi(bulk) + μSe(bulk) + Hform (Li2 Se). To obtain the solubility and doping effect of a dopant we have to include all relevant configurations and charge states of the impurity as expressed by (10.18). To be specific we continue to analyze the Li acceptor in ZnSe [12]. Besides the substitutional site Li− Zn where Li acts as an acceptor we particularly find two interstitial were it acts as a shallow donor. Calculations show that the tetrahedral site sites Li+ i surrounded by Se is by 0.2 eV more favorable than the respective site with Zn atoms. The substitutional Se site may be excluded due to a very large formation energy. Results of firstprinciples calculations for Li doping of ZnSe are displayed in Fig. 10.4 [12]. The contour plot Fig. 10.4a shows the total concentration of Li in ZnSe at an equilibrium temperature of 600 K, corresponding to the typical low growth temperature of ZnSe. Figure 10.4b gives the resulting Fermi energy. In Fig. 10.4a the bounds of the chemical potentials of Zn and Li are indicated by straight gray lines. The formation of the Li2 Se compound leads to the bound for μLi with a slope of 2 due to the dependence of μLi2 Se from μLi noted above. Li2 Se islands were actually found to form during molecular beam epitaxy of heavily
10.1 Doping of Semiconductors
(a) max µ Zn
383
(b)
6
max µ Zn
0.80
µ
0.40
µ Zn
µ Zn
10
min Zn
1.00
14
18
µ Li
22
0.60
µ
0.20
min Zn
µ Li
Fig. 10.4 a Total Li concentration log10 [Li] in a ZnSe:Li semiconductor doped at 600 K. Values depend on the chemical potentials of Li and Zn, and are given in cm−3 . b Fermi level resulting from the Li doping shown in (a). Values are given in eV and refer to the top of the valence band. c 1993 APS Reproduced with permission from [12],
doped ZnSe:Li [13]. The calculated maximum of Li concentration of ZnSe:Li is slightly above 1018 cm−3 [12]. The coinciding slope of the contour lines near the Li2 Serelated bound is accidental and originates from the incorporation of two Li atoms (one substitutional, one interstitial) for the removal of one Zn atom. The highest Li concentration (1.7 × 1019 cm−3 ) is obtained at the crossover point of a minimum accessible Zn chemical potential μmin Zn and a maximum accessible Li chemical potential before formation of Li2 Se. At this point the calculation yields fewer than 3% of the introduced Li atoms on an interstitial site and the most abundant native ZnSe defect of the Se antisite Se2+ Zn (a donor) with two orders of magnitude concentration below that of Li. Native defect concentrations become sizeable only below the physically meaningful limit μmin Zn and lead to a bending of the contour lines. If the equilibrium temperature is lowered the concentrations of all defects reduce. Reduction factors of about 5, 101 , and 102 for substitutional Li, interstitial Li, and the Se antisite, respectively, are found as the temperature decreases by 100 ◦ C [12]. The Fermi energy resulting from the Li concentration of Fig. 10.4a is shown in Fig. 10.4b. We note that the Fermi level decreases at fixed μLi as the Zn chemical potential is lowered. This trend results from the increasingly favored incorporation of Li on a Zn site and is also reflected in the Li concentration of Fig. 10.4a. If μLi is increased at fixed μZn we note from Fig. 10.4b that the decrease of the Fermi level tends to saturate despite the further increase of the total Li concentration shown in Fig. 10.4a. The reason is a steady increase by compensating interstitial Li donors that limits the hole concentration. The effect is minimized by decreasing the Zn chemical potential. Results outlined above for the specific case of Li exemplify the general behavior of dopant impurities. For any dopant limits of the solubility are imposed by the compounds that can be formed by the participating atoms. The relevant bound of the dopant chemical potential is imposed by the phase with minimum heat of formation.
384
10 Doping, Diffusion, and Contacts
Saturation of the Fermilevel position occurs when compensating species are formed. Such species are extrinsic species of amphoteric dopants or intrinsic native defects and are addressed in the following sections. In addition to isolated point defects treated above basically also complexes may affect the electrical properties. The concentration of a given complex (e.g., a pair of + substitutional and an interstitial Li denoted (Li− Zn , Lii )) gets significant if the binding energy exceeds the larger of the two formation energies of the individual defects out of which the complex is formed [12]. This makes it less likely that complexes have a significant influence, since complexes with a low binding energy tend to dissociate at growth temperatures.
10.1.3 Amphoteric Dopants An amphoteric dopant is one that can act as either a donor or an acceptor. The word “amphoteric” originates from the Greek word amphoteroi (amfoteroi) and means “having two characters”. Amphoteric behavior can occur if the dopant occupies different lattice sites like lithium in ZnSe as illustrated above. Prominent examples are groupIV impurities (C, Si, Ge, Sn) in III–V semiconductors that form donors on groupIII sites and acceptors on groupV sites. Obviously incorporation of an undesired site limits the intended doping effect. Such a compensation due to the same chemical species is referred to as autocompensation. The discussion of the amphoteric behavior of Li in the preceding section indicates that the degree of compensation depends on the applied equilibrium conditions. Anionpoor conditions applied during doping of III–V semiconductors by groupIV impurities favor incorporation on an anion site, while anionrich conditions favor incorporation on a cation site. This behavior is demonstrated in Fig. 10.5a for the incorporation of carbon in GaAs during metalorganic vaporphase epitaxy [14]. C doping originates from the organic CH3 ligands of the Ga source trimethylgallium Ga(CH3 )3 . A low V/III ratio in the gas phase of the applied arsenic source AsH3 with respect to Ga(CH3 )3 leads preferentially to CAs acceptors, while a high ratio favors CGa donors. Ge is an impurity with a pronounced amphoteric character in III–V semiconductors. Both n and ptype conductivity can hence be obtained depending on growth conditions. Besides the V/III ratio incorporation is also strongly affected by kinetics on the growth surface. GaAs surfaces stabilized by As favor incorporation on a Ga site yielding a GeGa donor. This represents the usual case of molecular beam epitaxy on (001) GaAs surfaces at temperatures below 630 ◦ C, i.e., below the congruent sublimation temperature of GaAs. Above this temperature Garich surfaces occur leading to GeAs acceptors. Even below 630 ◦ C a gradual increase of the concentration of Ge on As is observed as the temperature is raised [15]. This behavior is shown in Fig. 10.5b. Temperature increase leads to a gradual reevaporation of As from the
10
Temperature (°C) 600 550 500
18
(a)
10
10
GaAs:C
17
ptype
10
385
[GeAs] / [GeGa]
3
Carrier concentration (cm )
10.1 Doping of Semiconductors
ntype
(b)
As4
GaAs:Ge
As2 10
1
As4 grown As2 grown 2
10
16
10
0
0
1
10 Ratio AsH3/Ga(CH3)3
10
2
1.15
1.20 1.25 1 1000 / T (K )
Fig. 10.5 a Doping of GaAs with C from organic ligands in metalorganic vaporphase epitaxy for a varied ratio of arsenic and gallium sources in the gas phase. Data points are from [14]. b Autocompensation ratio of the doping of GaAs with Ge in molecular beam epitaxy at varied c 1982 Springer temperature for different arsenic species. Reproduced with permission from [15],
surface and hence increased occupation of Ge on As sites, i.e., to compensating acceptors. The more reactive As2 species are expected to yield a higher As coverage of the surface and hence a smaller compensation ratio. Amphoteric behavior may also occur for a defect on a given lattice site, i.e., without occupation of different inequivalent sites. If the defect has several levels in the bandgap like, e.g., Au in Ge, its character depends on the position of the Fermi level. We illustrate such a behavior below for a native defect pair.
10.1.4 Compensation by Native Defects Native defects represent an equilibrium phenomenon and occur in any solid. The abundance of intrinsic charged point defects has a strong impact on the electronic properties of semiconductors. Such defects comprise vacancies, interstitial atoms, and, in case of compound semiconductors, antisites. In compound semiconductors the abundance of native defects is particularly sensitive to a deviation from stoichiometry. With about 5 × 1022 cm−3 atomic sites even a slight deviation from perfect stoichiometry as small as 10−4 leads to a defect concentration in the range 1018 cm−3 . Generally native defects which accommodate deviation from stoichiometry are those that compensate majority carriers. Since the energy gained by such a compensation increases as the bandgap energy increases, early work on widegap semiconductors focused particularly on selfcompensation by native defects [16]. Certainly the effect contributes significantly to doping problems, albeit autocompensation and solubility may impose more rigorous limits.
386 Fig. 10.6 Calculated formation energies of defects in GaAs. a Isolated interstitial Ga atom Gai at a tetrahedral site with 4 nearest As atoms, b isolated vacancy at the Ga site VGa , and c a vacancyinterstitial pair Gai + VGa . Defect energies in (a) and (b) are arbitrarily normalized. The origin of the Fermienergy scale is set to the maximum of the valence band E v . After [17]
10 Doping, Diffusion, and Contacts
T
Gai d
VGa
T
Gai d + VGa
We study the effect of a native defect for the vacancyinterstitial pair in GaAs created by a Ga atom which moved from a regular lattice site to an interstitial position. The pair formation is described by the reaction 0 ↔ Gai + VGa . Calculated energies are given in Fig. 10.6 [17]. The ionization levels are in qualitative agreement with more recent calculations [18, 19]. Both isolated defects of the vacancyinterstitial pair have several chargetransfer energies in the band gap. For a Fermi level near the valenceband edge in ptype GaAs, the interstitial Gai defect with threefold positive charge has lowest formation energy. The defect hence traps holes, thereby compensating the extrinsic doping. As the Fermi level is increased, less holes are trapped by Gai due to an increased formation energy and gradually more electrons are trapped by the vacancy VGa defect. As a result, the charge state of the vacancyinterstitial pair gets more negative. We note that the formation energy depicted in Fig. 10.6c decreases for either high doping. Both, ptype and ntype doping are hence compensated by the vacancyinterstitial pair. The equilibrium concentration of intrinsic defects is given by (10.17) which was also used to describe extrinsic defects. The abundance of native defects hence depends on temperature, doping level, and the deviation from ideal stoichiometry. The dependence on the doping level, i.e., on the electron chemical potential, is illustrated in Fig. 10.6. We now turn toward the dependence on the chemical potentials of the atoms. Limits for the stoichiometry are imposed by thermodynamics. We express these bounds by applying the approach discussed in Sect. 10.1.2 for impurity doping of
10.1 Doping of Semiconductors
387
ZnSe. The chemical potentials of the constituents Ga and As may not exceed their max respective bulk values, i.e., μmax Ga = μGa(bulk) , μAs = μAs(bulk) , and their sum equals the chemical potential of bulk GaAs, μGa + μAs = μGaAs . The difference of the chemical potentials μ = μGa − μAs − (μGa(bulk) − μAs(bulk) ) is then limited by the heat of formation Hform (GaAs) of bulk GaAs from elemental Ga and As, μ ≤ Hform , with Hform  = μGaAs − μGa(bulk) − μAs(bulk) . We recall that Hform < 0, because GaAs is a stable compound. Garich and Asrich bounds of μ are given by μ = +Hform  and μ = −Hform , respectively. We consider some native defects in GaAs for a fixed doping level and temperature. Figure 10.7a shows the concentration of the Ga vacancy VGa and the Ga antisite GaAs in ntype GaAs [20]. For high doping VGa is triply negatively charged as shown in 3− is the dominant defect with a concentration of about Fig. 10.6. In the Asrich limit VGa 1/3 of the effective doping level Nd [20]. Under these conditions the formation energy is so low that about one such defect is formed for every three electrons introduced by 3− abundance by more than 10 orders of doping. We find a strong decrease of the VGa magnitude as μ is increased toward Garich conditions. Two reasons account for this finding. First, the formation energy of VGa increases. This effect is accompanied by a decrease of the electron chemical potential that further increases the formation 3− [20]. Second, Asrich conditions provide an effective sink for removed energy of VGa Ga atoms at the surface. This counteracts thermal equilibrium for Ga interstitial atoms and consequently, by the law of mass action, enhances the concentration of vacancies. 3− in Garich ntype GaAs is accompanied by an increase of The decrease of VGa the antisite GaAs , the formation energy of which linearly decreases as μ is raised. It becomes the dominat defect in the Garich limit and acts also as a compensating electron trap under these conditions.
10
18 2
Ga As 10
(a)
14 3
V Ga
3
Concentration (cm )
Fig. 10.7 a Calculated equilibrium concentration of the Ga vacancy and the Ga antisite as a function of the difference of the chemical potentials of Ga and As atoms under ntype conditions at 827 ◦ C. b Concentration of the Ga interstitial and the As antisite for ptype conditions at 827 ◦ C. Reproduced with permission from [20], c 1991 APS
10
10 10
10
N d =+10
6
18
cm
3
20 2+
As Ga 10 10
(b)
16 3+
Ga i 12
I H I Asrich
N d =10
20
µ
cm
3
I HI Garich
388
10 Doping, Diffusion, and Contacts
Ec Nd=+10
Fermi energy EF
Fig. 10.8 Calculated position of the Fermi energy in GaAs as a function of the difference of the chemical potentials of Ga and As atoms for three fixed doping levels Nd = ND+ − NA− . Reproduced with permission c 1991 APS from [20],
18
3
cm
T = 580°C
Nd= 0
Ev
Nd=10
18
3
cm
I H I Asrich
µ
I HI Garich
In strongly ptype doped GaAs the dominant native defect under Garich conditions is the interstitial Ga atom Gai at a tetrahedral site with 4 nearest As atoms. At this doping level it acts as a triple hole trap. Below 1017 cm−3 ptype doping it mainly appears in the singly charged state [20]. Decreasing μ toward Asrich conditions leads to a decrease of the Ga3+ i abundance, accompanied by an increase , which also acts as a hole trap. of the As antisite As2+ Ga Charged native defects have an influence on the position of the Fermi level due to the charge neutrality condition (10.20). The effect on E F becomes obvious by explicitly expressing the hole and electron densities in terms of Boltzmann statistics, Nd = ND+ − NA− = Dceff exp −(E c − E F )/kB T − Dveff exp −(E F − E v )/kB T
q + (10.21) n ielectron Di . i q
Here [Di ] is the concentration of a native defect, and Dceff and Dveff are the effective conductionband and valenceband densities of states defined in (10.4a)–(10.4b). Figure 10.8 shows the calculated dependence of the Fermilevel position on native defects created by a variation of the stoichiometry [20]. We note significant variations of E F for fixed concentrations of excess free charge carriers. The strong decrease for Garich conditions in ntype GaAs (Nd = +1018 cm−3 ) originates from charge compensation by the antisite defect Ga2− As , the slight increase on the Asrich side 3− . originates essentially from the vacancy VGa
10.1.5 Hydrogen Compensation and Passivation Hydrogen is easily incorporated in semiconductors, particularly in MOVPE and related gassource techniques. Due to its generally high reactivity and diffusivity it has a strong effect on electronic properties. Interstitial hydrogen is amphoteric and
10.1 Doping of Semiconductors
389
assumes the positive charge state H+ in ptype and the negative state H− in ntype semiconductors [21]. It thereby counteracts the prevailing conductivity: an acceptor dopant has a negative charge state A− if it has created a free hole in the valence band; hydrogen then acts as a donor according H0 → H+ + e. Vice versa it acts as an acceptor if donors create ntype material according to H0 + e → H− . Hydrogen hence tends to compensate doping. The position of the Fermi level where hydrogen changes directly from the H+ donor state to the H− acceptor state depends on the band structure of a semiconductor on an absolute energy scale (cf. Sect. 4.2.3) and lies for most semiconductors and insulators in the bandgap. For many solids this energy was determined by firstprinciples calculations based on densityfunctional theory and ab initio pseudo potentials [21]. The positively charged, highly mobile H+ in ptype material is attracted by the Coulomb field of the negatively charged ionized acceptor. This may easily lead to the formation of a neutral (AH)0 complex, a process referred to as passivation. A similar process may occur in ntype material with ionized donors D + and H− , yielding a neutral (DH)0 complex. Passivation and compensation both reduce the density of free carriers, but the effects are actually different. In a Hall measurement the creation of neutral complexes leads to a reduced ionizedimpurity scattering and hence an increased freecarrier mobility by passivation; in compensation, however, ionized hydrogen and dopants are located at different (random) positions and both contribute to ionizedimpurity scattering—the mobility is hence decreased. Passivation of shallow dopants by hydrogen is known for many technologically important semiconductors. Often the effect is stronger for ptype doping than for ntype doping. Prominent examples are pGaN:Mg [22], pGaAs:Zn [23], pSi:B and nSi:P [24], 6H pSiC:Al, pSiC:B and nSiC:N [25].
10.1.6 DX Centers A number of impurities introduce levels in the bandgap that are far away from the conductionband and valenceband edges. Due to their large ionization energy they are able to trap free charge carriers, thereby increasing the resistivity of a semiconductor. Prominent examples are transition metals like Cr or Fe in GaAs or InP. According to the position of the chargetransfer level in the bandgap they are classified into donorlike or acceptorlike centers. A common feature is a strong localization of their wavefunction compared to that of shallow impurities. Deep centers affect many properties of semiconductors, e.g., they compensate doping, reduce minoritycarrier lifetime and diffusion length, and lead to a reduced carrier mobility. There exists a large variety of different kind of centers introducing deep levels in semiconductors. We focus here on a specific kind of deep centers related to a structural instability of impurities. The motivation to emphasize these socalled DX centers is their amphoteric character, which converts an intentional shallow dopant to a deeplevel impurity. The label DX refers to a complex of a donor D and an unknown (at the time of discovery) intrinsic defect X. A comparable case for acceptors is referred to as AX
10 Doping, Diffusion, and Contacts
Electronic + vibronic energy
390
(a) (b)
E D0+eE DX 
[111]
E opt E cap
[010] E emi
QD Q DX Configuration coordinate
Q
[001] [100]
Fig. 10.9 a Configurationcoordinate diagram representing the total energy of a DX center and a substitutional donor. b Structural model of a DX center. The dotted line indicates the bond which breaks when the tetrahedrally coordinated impurity (red) is displaced along a 111 direction to a position depicted by the transparent atom
center. Experiments found a large energy difference between the optical and thermal ionization energies, indicating that the deep state is strongly coupled to the crystal lattice [26]. The generally accepted model of a DX center in a tetrahedrally coordinated compound semiconductor is illustrated in Fig. 10.9. The donor has two configurations: A substitutional site where it acts as a shallow donor, and a relaxed site where one of the four bonds with two electrons is broken and the impurity is displaced along one of the 111 directions [27]. The broken bond creates two dangling bonds which may be occupied by up to four electrons. The (neutral) donor thus can hold its own extra electron and accept an additional electron according to the reaction D0 + e− → DX− . Since the ionization of a shallow donor is described by D0 → D+ + e− , an electron transfer between the donors is given by the sum of the two reactions, yielding 2D0 → D+ + DX− .
(10.22)
The two donors do not need to be in close proximity to each other. Reaction (10.22) indicates that one half of all donor atoms may exist in the brokenbond configuration and compensates thereby the free electrons released from the other half in the substitutional shallow configuration. Donor centers which yield an exothermic reaction according to (10.22) are also referred to as negativeU centers. U denotes the effective electronelectron correlation energy of the two centers. A negative correlation energy is obtained if the energy gained by the lattice distortion is larger than the energy cost for the electron repulsion.
10.1 Doping of Semiconductors
391
The instability of specific dopants against formation of DX centers is assigned to a large JahnTeller distortion of the highly symmetric substitutional site. The strength of the effect depends on the bonding character and hence on both, the dopant and the host crystal. Ga, e.g., forms a stable substitutional donor on a Zn site in ZnSe, but is instable against formation of a DX center in ZnTe [28]. For a (metastable) Garelated DX center in ZnSe the corresponding parabola (E DX− ) in the configurationcoordinate diagram has a minimum at Q DX with a higher energy than the minimum of the parabola (E D0 +e− ) at Q D . Substitutional Si in GaAs forms a stable donor on a Ga site, while it builds a wellstudied DX center in Alx Ga1−x As for compositions x > 0.22 (below this value the DX level lies in the conduction band) [26]. Electron capture into the DX center is thermally activated with a compositiondependent energy barrier E cap (>0.2 eV) as depicted in Fig. 10.9a. The barrier E emi for thermal emission of carriers from the DX center is larger (∼0.4 eV). Carriers may as well be released by optical absorption with a large photon energy E opt (>1 eV). Optically released carriers remain in the conduction band (for days) due to a very low recapture rate and generate a persistent photoconductivity. Other donors like, e.g., Te, Se, and Sn show similar DX characteristics. The model outlined in Fig. 10.9 accounts well for the experimental findings.
10.1.7 FermiLevel Stabilization Model The amphoteric character of intrinsic defects and the formation of related deep levels illustrated above leads to a phenomenological model to account for the widely differing doping ability of semiconductors. The Fermilevel stabilization model, also termed amphoteric defect model or doping pinning rule, points out trends for intrinsic limitations to account for, e.g., the difficulties for achieving ntype ZnTe or ptype ZnO. The model ties in with the empirical rule of naturally fixed energy levels of transitionmetal impurities in different semiconductors (Sect. 4.2.3). Similarly, clear evidence for the localized nature of native defects is found. The Fermilevel stabilization model therefore assumes that doping limitations reflect the absolute position of the valence and conduction band edges with respect to a fixed reference energy like, e.g., the vacuum level. Doping restrictions are hence not assigned to the size of the bandgap per se or to properties of particular dopants. The reference level for the natural alignment of the band edges with respect to the ability of doping is termed Fermilevel stabilization energy E FS . Indication for such an internal reference was concluded from semiconductors, which were heavily damaged with gamma rays or electrons [29]. For a high density of damage, where material properties are controlled by native defects, the Fermi level was found to stabilize at a certain energy and becomes insensitive to further damage. This energy E FS is located at an energy of about 4.9 eV below the vacuum level for the studied tetrahedrally bonded semiconductors [30]. The internal reference E FS allows
392
10 Doping, Diffusion, and Contacts
GaP Si Ge
InP
GaAs GaSb ZnSe ZnTe InAs GaInAs
Ec
E c  E FS
E FS Ev
E FS  E v
1 eV
IV
IIIV
IIVI
Fig. 10.10 Valence band maxima and conduction band minima of various semiconductors aligned with respect to their internal Fermilevel stabilization energy E FS . Data from [31]
to arrange the bands of all semiconductors on a common energy scale. Figure 10.10 shows the band alignment of some tetrahedrally coordinated semiconductors. The position of E FS with respect to the band edges depicted in Fig. 10.10 affects the ability to achieve high carrier concentration of a given type. The formation energy of compensating native defects depends on the difference between the Fermi energy and the stabilization energy E FS . If E FS lies close to the valence band, the Fermi level should easily be moved into the valence band by ptype doping without significant formation of compensating defects. Consequently high ptype carrier concentration is expected. On the other hand, a large energy difference to the conduction band will lead to a high abundance of compensating defects if E F is raised by ntype doping, resulting in solely poor ntype carrier concentration. The asymmetry of p and ntype doping increases as the bandgap increases. Experimental data of maximum carrier concentrations achieved are given in Fig. 10.11. Electron and hole concentrations are normalized by the effective density of states Dceff and Dveff , respectively. Normalized values are used, because electron concentrations are given by n = Dceff × F1/2 [(E F − E c )/kB T ] and hole concentrations p accordingly with Dveff and (E v − E F ), where F1/2 is the Fermi integral. Figure 10.11 clearly shows that the achieved normalized doping levels decrease as the energy separation between the stabilization energy E FS and the band edges E c or E v increase. The data can be roughly described by the empirical relation [31] ccmax /D eff = a × exp bE FS − E band edge  .
10.1 Doping of Semiconductors
393
Fig. 10.11 Experimental maximum carrier concentrations for ntype (black circles) and ptype semiconductors (gray circles) as a function of the energy difference between E FS and either the conductionband edge E c , or the valenceband edge E v , respectively. The solid lines are fits. Data taken from [31]
3
Normalized carrier concentration n/Dc
eff
p/Dv
eff
10
10
2
Si GaAs
Ge
10
1
10
InP Si
GaAs
GaSb
GaSb
Ge
10
n type p type
ZnSe GaP
InP
GaP
1
ZnSe
2
0
0.2 0.4 0.6 0.8 1.0 1.2 1.4 1.6 1.8
IEc  EFSI (eV)
IEFS  EvI (eV)
Here, ccmax is the maximum carrier concentration n or p with the related effective density of states and the related bandedge energies E c or E v , and the parameters are an = 2.7 × 103 , bn = −5.5 eV−1 , a p = 4.0 × 102 , b p = −6.1 eV−1 . The maximum carrier concentrations achieved in experiments can be expressed ( p) (n) and E pin of the Fermi energy in ntype and ptype in terms of pinning energies E pin semiconductors, respectively. In the approximation of single parabolic bands the maximum net free carrier concentration ccmax is given by [32] ccmax =
(2m ∗(n/ p) )3/2 2π 2
√
∞ 0
exp((E −
E dE
(n/ p) E pin )/k B T )
+1
. ( p)
(n) The equation is inverted to obtain the pinning energies E pin and E pin from the experimental ccmax data. The resulting pinning energies are given in Fig. 10.12 for various III–V and II–VI compound semiconductors. We note a fairly small scatter in the pinning energy, if the bands are aligned with respect to an absolute reference energy.
10.1.8 Delta Doping and Modulation Doping Epitaxial growth allows for fabricating highly doped buried layers with a very small thickness in the range of atomic monolayers referred to as delta doping (δ doping) [33, 34]. The spacially inhomogeneous doping profile provides free carriers and an electrical potential which differs from that of the conventional homogeneous doping.
394
10 Doping, Diffusion, and Contacts E (eV) AlP 3.0
GaSb ZnS AlAs InAs GaP ZnTe CdSe CdTe ZnSe CdS AlSb InSb GaAs InP (n )
E pin
(n ) E pin 2.0
1.0
E
(p) pin
(p)
E pin
0.0 1.0
IIVI
IIIV
Fig. 10.12 Pinning energies (black bars) calculated from experimental maximum carrier concentrations. Dotted lines are averaged pinning energies. Bands are aligned with respect to calculated offsets, zero is set at the valence band edge of GaAs for III–V and that of ZnSe for II–VI compounds. Data are from [32]
Many characteristics of semiconductor structures related to potential fluctuations like, e.g., free carrier mobility of luminescence linewidth, perform better applying delta doping. The most prominent application is the enhancement of conductivity in a layer, where the carriers are not subjected to impurity scattering at the ionized dopant cores. The mobility of carriers in this layer is strongly increased, similar to the modulationdoping technique based on band bending at heterojunctions. The effect of delta doping requires a confinement of the doping atoms within a layer thickness well below a relevant length scale, which usually is given by the de Broglie wavelength of free carriers. In practice doping profiles with a width of 3 nm and below can be considered like a delta function. Note that this width corresponds to only five lattice constants. To achieve such narrow profiles, impurity redistribution processes like diffusion or segregation must largely be suppressed. This usually implies deposition at lowered temperature to avoid thermally activated diffusion. The doping procedure basically proceeds by an initial interruption of the epitaxy of the undoped semiconductor, followed by the deposition of the highly doped layer. Eventually the growth of the undoped material is resumed. Growth parameters like temperature, partial pressures and material supply have to be adjusted such that the doping profile is preserved. Due to the twodimensional character of the doping layer it is often referred to as doping sheet. The profile of delta doping is described by two parameters: The location of the dopand sheet z 2D and the areal density of doping atoms in the sheet n 2D or p2D . To be specific we consider donor dopants and a complete ionization. The 2D donor density n 2D may be estimated from growth parameters used to obtain a 3D bulk carrier concentration n by scaling with the thickness r × t of the doping sheet, n 2D = nr t.
10.1 Doping of Semiconductors
395
Here r is the growth rate and t the duration of the dopingsheet deposition. The relation applies well if the incorporation efficiency of dopants is not affected by the preceding growth interruption. The effective 3D concentration of donors n 3D is obtained from n 2D of a homogeneously doped sheet by considering the mean distance between donors in the sheet (n 2D )−1/2 and assuming the same mean distance in 3D bulk, yielding (10.23) n 3D = (n 2D )3/2 . In semiconductors with delta doping the concentration of dopants varies strongly over short distances. The free carrier concentration is then spread much further than the profile of doping atoms. This feature is different to a slowly varying doping concentration, where the freecarrier profile follows the doping profile. Let us assume in a first approximation that all (ionized) doping atoms are located within a single atomic layer in the x y plane located at z = z 2D with a density n 2D . The doping profile is then described by n(z) = n 2D δ(z − z 2D ), δ being the delta function. The twodimensional charge e × n 2D of the doping sheet creates a onedimensional electric potential V (z) which is calculated using Poisson’s equation, en(z) ∂2V . =− ∂z 2 ε
(10.24)
ε = εr ε0 is the permittivity of the semiconductor. Twofold integration yields the potential en(z) z − z 2D . (10.25) V (z) = 2ε We note that V is a linear and symmetric function of z and is Vshaped with V (z 2D ) = 0. For an interaction with negative free carriers V ≤ 0. The slope of the potential V (z) represents the electric field created by the ionized impurity atoms in the doping sheet, E = −∂ V /∂z = const. It depends on the doping density and the permittivity, yielding typical values exceeding 106 V/m. Such strong fields lead to a strong attractive interaction with free carriers: The potential V (z) forms a narrow well with a width on the order of the de Broglie wavelength. Similar to the narrow square potential treated in Sect. 4.3 we obtain size quantization with discrete energy levels. We should note that the shape of the potential actually deviates from a simple V. The deltadoped semiconductor is neutral, because the charge of the doping sheet is balanced by the opposite charge of the released free carriers. The electric field therefore approaches 0 at some distance from the sheet. Figure 10.13 depicts a selfconsistent solution of an effectivemass calculation of carriers confined in a potential which is created by delta doping [35]. The calculation assumes data of GaAs with an electron mass m ∗ = 0.067m 0 . The donordoping profile n(z) illustrated in Fig. 10.13a creates a local bending of the conductionband edge E c that confines free electrons to discrete energies E i . For the parameters assumed in the calculation four energy levels E 0 to E 3 are occupied with fractions of 61%, 24%, 11%, and 4%, respectively. We note a steep and nearly
396 Doping n (z)
(a)
Depth z
(b)
EF
E3 E2
150
Energy (meV)
Fig. 10.13 a Schematic of deltadoping profile. b Calculated effectivefield potential well (E c ) and confined carrier distribution ψ2 of an ntype deltadoping sheet with 2 Å thickness and 5 × 1012 cm−2 density. E F denotes the Fermi energy. Reproduced with permission from [35], c 1990 AIP
10 Doping, Diffusion, and Contacts
E1 100
2
E0 50
Ec
0 0
200
400
600
800
1000
1200
Depth ( Å )
constant slope of the confining potential in a close vicinity to the doping sheet, and an approach to a constant value at some distance. The spatial extent of the carrier wavefunction is much wider than the thickness of the doping sheet (∼50 Å in the ground state vs. 2 Å, even more in the excited states). This finding leads to a more precise condition for delta doping: The distribution of doping atoms must be significantly more narrow than the spatial extent of carriers confined in the ground state. Obviously a factor 10 thicker doping sheet will lead to quite similar results in the present example. The effect of delta doping on the Hall mobility of free carriers is illustrated in Fig. 10.14 [36]. The mobility μ of a carrier with drift velocity v (at low electric field E) is generally given by v = μ E, and is limited by scattering processes (see, e.g., [37]). The 2D mobility was measured using the twodimensional electron gas created in the channel of a GaAs fieldeffect transistor [38]. Bulk values of the donor concentration n 3D corresponding to the 2D values of the deltadoping sheet were calculated from (10.23) and used in the abscissa of Fig. 10.14. The 2D mobility μ2D is related to the dopingdependent mobility of bulk GaAs which is taken from the empirical expression μ3D = μL (1 + (n 3D /1017 cm−3 )1/2 )−1 , μL = 104 cm2 /(Vs) being the mobility limit due to lattice scattering [42]. Figure 10.14 shows that the mobility of free carriers in the twodimensional electron gas significantly exceeds that of bulk free carriers at high doping concentrations n 3D . The increase of mobility is assigned to various features of the 2D carriers. From an only weak dependence of the mobility μ2D on temperature a reduced scattering at ionized impurities was concluded [36]. The carriers in the 2D electron gas have a high degeneracy on their energy levels E i , connected to high kinetic energies parallel to the
10.1 Doping of Semiconductors
2D
/ µ 3D
4
µ
Fig. 10.14 Relative mobility enhancement of deltadoped ntype GaAs with respect to homogeneously doped ntype GaAs measured at 300 K. Data from [36]
397
3 2 1 10
15
17
10 n3D (cm3)
10
19
plane of the doping sheet. Carriers with energies close to the Fermi surface are most sensitive to scattering. Their energies E F − E i exceed well the thermal energy kB T , leading to a reduced temperaturedependent impurity scattering. A further contribution originates from a decreased overlap of oddnumbered carrier wavefunctions with the deltadoping plane of impurities. Wave functions ψ1 , ψ3 , . . . have a node at the position of the doping sheet (cf. Fig. 10.13b) and hence experience much less impurity scattering. Also the overlap of symmetric evennumbered excited wave functions ψ2 , ψ4 , . . . is much smaller than that of the ground state ψ0 , and even the spatial extent of the ground state is significantly larger than the thickness of the doping sheet. A drawback of the deltadoping technique discussed above is that the mobile electrons are bound to the doping plane, where the statistically distributed donors provide a fluctuating potential; the electrons hence experience substantial impurity scattering. This disadvantage can be avoided if the donors are separated from the mobile electrons by confining them in a separate potential. This is achieved by introducing a heterointerface to confine the electrons, and placing the donor sheet at some distance away by inserting an undoped spacer layer; using such a spacer layer also a homogeneous doping can be applied, yielding a modulationdoped structure [39]. Band bending at the heterointerface creates a triangular confinement potential with discrete energies (along growth direction z) in the semiconductor with smaller bandgap as illustrated in Fig. 10.15 [43]. A similar potential can also be created at the oxide/semiconductor interface of a MOSFET device [40]. The electrons provided by the remote doping are free to move in the lateral (x, y) directions and form a twodimensional electron gas (2DEG) with a high mobility, particularly at low temperature [41]. The low impurity scattering is utilized in modulationdoped fieldeffect transistors (MODFET, also termed HEMT, high electronmobility transistor); it can be further reduced by delta doping. In a conventional MODFET a homogeneously doped widebandgap layer (usually AlGaAs) provides free carriers, which are trapped at the heterojunction to an adjacent undoped layer with a smaller bandgap (GaAs), see Fig. 10.15. Employing delta doping instead of homogeneous doping allows for a large and welldefined separation between free carriers and doping impurities [2].
398
10 Doping, Diffusion, and Contacts
Fig. 10.15 Energyband diagram of a modulationdoped AlGaAs/GaAs heterostructure with a metal gate contact, creating a 2D electron gas located at the interface; occupied energy level E 1 and an undoped spacer layer of thickness ds are indicated
E ds
Ec EF E1 Ev
metal
AlGaAs
GaAs
z
10.2 Diffusion Atoms in a crystal may not stay fixed on their site. In presence of a concentration gradient and at sufficiently high temperature atoms redistribute by diffusion, thereby changing the interface abruptness in heterostructures and the spatial distribution of defects. The effect is utilized, e.g., for the indiffusion of dopants into semiconductors via the surface, but may also be detrimental for epitaxial nanostructures. Atoms diffuse via different mechanisms, which are controlled by temperature, partial pressure, and material composition. Since various diffusion paths usually act simultaneously and diffusivity may depend on defect concentration, diffusion is a complex subject. We will outline basic phenomena and illustrate some examples.
10.2.1 Diffusion Equations The diffusion of an atom incorporated in a crystal is described similar to the surface diffusion of an adatom considered in Sect. 7.2.2. Each jump of the atom to an adjacent site is the result of an attempt to leave the actual site and of the success to surmount the potential barrier E which tends to keep the atom at its site. The diffusion coefficient D is likewise given by the product of the mean square value of the displacement λ2 and the rate of successful jumps ν, yielding D = λ2 ν = λ2 ν0 exp −E/(kB T ) = D0 exp −E/(kB T ) .
(10.26)
10.2 Diffusion
399
The diffusion constant D0 = λ2 ν0 has usually an only small temperature dependence compared to the exponential term and is often assumed constant with respect to temperature. Note that D0 may still vary spatially in an inhomogeneous solid. To obtain an expression for the motion of a diffusing atom we first consider a macroscopic view of the diffusion of impurities in a solid; an atomistic approach is discussed below in Sect. 10.2.2. We assume an impurity concentration c which varies only along a single coordinate z and a random diffusion of an impurity which is not affected by other impurities. In this case the net flux of impurities j per unit area and unit time also varies only along z and is given by Fick’s first law, j (z) = −D
d c(z). dz
(10.27)
The flux of impurities j (z) is proportional to the gradient of the impurity concentration c(z) and directed toward the lowconcentration region (cf. the negative sign). Since the atoms move in such a way as to even the gradient up, the onedimensional form of Fick’s law is sufficient to describe the flux. We note that there is no net flux if the impurity concentration is constant. The diffusion coefficient D depends in a simple case not on the impurity concentration c and also not on the spatial position z (but still on the temperature). This case describes a linear Fick diffusion. A dependence D(c, z) due to experimental conditions leads to a nonlinear Fick diffusion also described by (10.27). The impurity flux must comply with the continuity condition. The net flow into any volume element equals the increase of impurity concentration per unit time in this volume element, ∂ ∂ j (z) = − c(z, t). (10.28) ∂z ∂t Inserting (10.27) into the onedimensional continuity equation (10.28) yields the diffusion equation known as Fick’s second law, ∂c(z, t) ∂c(z, t) ∂ D = . ∂z ∂z ∂t
(10.29)
If the diffusion coefficient D is constant with respect to z, then (10.29) simplifies to D
∂ 2 c(z, t) ∂c(z, t) . = 2 ∂z ∂t
(10.30)
The solution to Fick’s second law depends on the boundary conditions which are given by the experiment. We consider some solutions of the onedimensional diffusion equation in the form of (10.30) for different experimental conditions; a more comprehensive treatment is given in [44]. The first example is the indiffusion of impurities from the surface with a surface concentration kept constant at a value c0 . Such a condition may be given by
400
10 Doping, Diffusion, and Contacts
applying an external constant vapor pressure of impurity atoms on the surface. The impurity concentration in the solid depends only on the distance z from the surface, which is assumed to be located at z = 0. The resulting boundary conditions read c(z = 0, t) = c0 for all t, and c(z, t) = 0 for z > 0 and t = 0. The solution of the diffusion equation (10.30) for these conditions is z , c(z, t) = c0 erfc √ 2 Dt where erfc is the complementary error function. The diffusion profile c(z, t) depends on the diffusion coefficient D(T ) and the duration of the indiffusion process t. Profiles for varied values of the product Dt are shown in Fig. 10.16a. The concentration profiles c(z) show a progressive indiffusion of impurities for increasing process time t. The material is constantly supplied from the external vapor phase via the surface, such that c(z = 0, t) = c0 during the entire process. In our second example the source of impurities is assumed to be located within the solid. We consider a solid being doped with impurities with an (initially) constant concentration cd in a range z < 0 up to an interface located at z = 0. Beyond the interface at z > 0 the solid is assumed to be undoped. The boundary conditions are now c(z) = cd for z < 0 and c(z) = 0 for z > 0 for t = 0.
1.0
1.0
0.1 0.3 1
Dt 0.5 2
1 0.1 0.0
0
5
c(z) / cd
c(z) / c0
(a)
10
(b) Dt
0.5
3 10
0.5 1
2
3
4
Distance from surface z
5
0.0
4
2
0
2
4
Distance from interface z
Fig. 10.16 Solutions of the onedimensional diffusion equation for two different boundary conditions. Concentration profiles c(z) are given for varied values of the quantity Dt as indicated on the curves. a Impurity distribution in an initially (at Dt = 0) undoped solid for a surface concentration kept constant at a value c0 . b Distribution for a solid being initially homogeneously doped with an impurity concentration cd at z < 0 and undoped at z > 0
10.2 Diffusion
401
The solution of the diffusion equation (10.30) in this case is given by z cd . erfc √ c(z, t) = 2 2 Dt The result is quite similar to the first case. In contrast to the first example the total amount of impurities diffusing in the solid now is constant. Impurities diffusing across the interface hence increase the concentration c at z > 0 on expense of c at z < 0. The initial stepfunctionlike profile gradually smoothens and has the shape of the complementary error function as shown in Fig. 10.16b. The impurity concentration at the interface remains fixed at c(z = 0, t) = cd /2. The example resembles the first one as long as the doped √ part can be considered semiinfinite thick with respect to the diffusion length Dt. In our third example a deltadoping sheet within an undoped solid is assumed to represent the source of impurities. The total impurity concentration c2D is initially (at t = 0) located in the twodimensional (x y)plane at z = 0. The boundary conditions are in this case ∞ c(z, t) = c2D = const for all t > 0. c(z, t) = c2D δ(z) for t = 0, and z=−∞
The solution of the diffusion equation (10.30) for this geometry is given by c2D z2 . c(z, t) = √ exp − 4Dt 2 π Dt The total amount of impurities diffusing in the solid is constant like in the previous example. The initial δfunctionlike profile gradually broadens to a Gaussian distribution as illustrated in Fig. 10.17. The broadening is characterized by the increasing √ standard deviation of the distribution σ = 2Dt. 1.0
0.1
0.8
c(z) / c2D
Fig. 10.17 Impurity concentrationprofiles for a doping sheet located at z = 0 initially (at Dt = 0) described by a δfunctionlike profile. Numbers on the curves signify respective values of Dt
0.2
0.6
0.5 1 2 Dt 5
0.4 0.2 0.0
4
2 0 2 Distance from doping sheet z
4
402
10 Doping, Diffusion, and Contacts
10.2.2 Diffusion Mechanisms The diffusion of atoms in a crystal depends on many experimental parameters in addition to the temperature, such as the material composition, the position of the Fermi level, or the concentration of point defects. An understanding of these dependences requires a microscopic view on the diffusion mechanisms. We consider some important mechanisms separately, even though usually a combination of these diffusion paths occurs in practice. Often the dominant mechanism provides a reasonable description of the diffusion process at least in some limited temperature range. In a perfect crystal which does not contain point or line defects, the only mechanisms for atom diffusion on lattice sites are the exchange and ring mechanisms illustrated in Fig. 10.18a. Since many bonds need to be broken simultaneously in these collective mechanisms, they are associated with a very high activation energy for the migration and do not play a significant role in practice. Mechanisms involving defects are much more effective for both, diffusion of impurities and selfdiffusion of crystal species. We focus on the effect of point defects and do not include phenomena in the presence of line defects. Vacancy mechanism: Any crystal at finite temperature contains vacant lattice sites, which provide an efficient path of diffusion via substitutional sites. The elementary jump of an atom into a neighboring vacancy is depicted in Fig. 10.18b. Diffusion of substitutionally dissolved impurities or selfdiffusion via this path is still slow compared to other mechanisms. Examples of slow impurity diffusors are the common Column III and Column V dopants in silicon as shown below in Fig. 10.19. Interstitial mechanism: If atoms exist on interstitial sites, they can migrate by jumping from one interstitial site to another as illustrated in Fig. 10.18c. This mechanism is particularly favorable for small impurity atoms, which do not need to greatly displace crystal atoms from their regular lattice site. The mechanism is very efficient. Prominent fast diffusors are interstitially dissolved Cu, Li, H, or Fe in silicon [45]. Their large diffusivities are shown in Fig. 10.19.
(a)
(b)
(c)
(d)
(e)
Fig. 10.18 Schematic illustration of diffusion mechanisms. a Top: exchange mechanism, bottom: ring mechanism. b Vacancy mechanism. c Interstitial mechanism. d Interstitialcy mechanism. e Substitutionalinterstitial mechanisms, top: FrankTurnbull mechanism, bottom: kickout mechanism
10.2 Diffusion
403
1400 1200 1000 4
2 1
Ni
Pt Au
8
DA (cm s )
Cu
H
10
600°C
800
10
S
Li Fe
Zn
Ge 12
10
Ga
Al C Sb B As P
Si 16
10
0.6
O
0.7
0.8
0.9 3
1.0
1.1
1.2
1
10 / T(K ) Fig. 10.19 Diffusion coefficients D A of impurities A in Si. Black lines refer to elements which mainly dissolve substitutionally and diffuse via the vacancy or interstitialcy mechanism. Gray lines represent data of hybride elements which diffuse via the substitutionalinterstitial mechanism. Light gray lines give data of elements diffusing via the direct interstitial mechanism. The dotted line represents Si selfdiffusion. Data from [51], Li, Fe, and Ga from [52]
Interstitialcy or indirect interstitial mechanism: This path is more likely for impurities with a similar size as lattice atoms or for selfdiffusion. The mechanism implies a cooperative motion of two atoms as shown in Fig. 10.18d. An interstitial atom moves into a lattice site by pushing an atom, which originally occupied this site, to a neighboring interstitial site. Substitutionalinterstitial mechanism: This effective diffusion mechanism in semiconductors may apply for impurity atoms A which can be incorporated on both a substitutional site As and an interstitial site Ai (hybrid solutes). Such impurities can diffuse via one of the two types of this mechanism depicted in Fig. 10.18e. The FrankTurnbull (or, dissociative) mechanism involves vacancies V according to the reaction [46] (10.31) Ai + V ↔ As . The kickout mechanism involves selfinterstitials I (interstitials of crystal species) according to the reaction [47, 48] Ai ↔ As + I.
(10.32)
404
10 Doping, Diffusion, and Contacts
The diffusivity of Ai is generally much larger than that of As , while the solubility and hence also the equilibrium concentration ci on interstitial sites is much less than on lattice sites cs . An efficient incorporation of impurities A may then proceed by a fast interstitial diffusion for many consecutive jumps, eventually followed by the occupation of a regular lattice site. This process differs from the interstitialcy mechanism, where the atom in the interstitial position remains there for only a single step. The FrankTurnbull and kickout mechanisms are prevailing diffusion paths for many substitutionally dissolved fast diffusing elements in ColumnIV and III–V semiconductors. Well established examples are the diffusion of Cu, Ag, and Au in Ge via the FrankTurnbull mechanism and that of Au, Zn, Pt, and S in Si via the kickout mechanism.
10.2.3 Effective Diffusion Coefficients Usually several of the diffusion mechanisms outlined above act simultaneously. Since diffusion coefficients vary over many orders of magnitude depending on experimental conditions, the dominating path may already provide a reasonable description. We illustrate some dependences of the diffusivity for the important diffusion mechanisms with participating point defects. In compound semiconductors single point defects are vacancies, interstitials, and antisites. Their equilibrium concentrations depend on the parameters temperature, partial pressures, and composition, which are mutually related by the phase diagram. In this section we assume the concentrations Cdefect as given quantities to point out their effect on diffusivity. Vacancy mechanism: One diffusion jump of this mechanism requires the presence of one vacancy V . The diffusion coefficient D of the migrating species is therefore proportional to the concentration of vacancies C V . An atom with no adjacent vacancy can also move, if first a vacancy diffuses to a neighboring lattice site. The diffusion coefficient D is therefore also proportional to the diffusion coefficient DV of the vacancies, eventually yielding D ∝ C V DV
(vacancy mechanism).
Substitutionalinterstitial mechanism: There are two types of this mechanism as outlined in the previous section. In the FrankTurnbull mechanism (Fig. 10.18e, top) the diffusivity of the impurity A is essentially given by the (large) diffusivity Di of the (small) fraction Ai dissolved on interstitial sites. The marginal contribution of substitutional impurities As , which either diffuse directly via the vacancy mechanism or interact with selfinterstitials, is neglected. According to (10.31) the diffusion mechanism involves the three species Ai , As , and vacancies V . The diffusivity of As depends on the incorporation rate of impurities A on a lattice site. It is determined by the slower process of either supplying interstitials Ai or vacancies V from the sample surface. If the supply of interstitials limits the process due to experimental conditions eq eq (i.e., Ci Di C V DV ), the effective diffusivity of the FrankTurnbull mechanism is given by [45, 49]
10.2 Diffusion
405
eq Ci = eq eq Di C + Cs eqi eq ≈ Ci /Cs Di (FrankTurnbull, limited by interstitials).
lim(i) Deff
eq
eq
Ci and Cs are the local equilibrium concentrations of Ai and As , respectively. The index lim(i) denotes the limitation by the supply with interstitials. If the supply of eq eq vacancies limits the process (i.e., C V DV Ci Di ), the local equilibrium conceneq tration of vacancies C V controls the effective diffusivity according to eq lim(V ) = C V /Cseq DV (FrankTurnbull, vacancylimited). Deff The kickout type of the substitutionalinterstitial mechanism involves the species Ai , As , and selfinterstitials I according to (10.32). Now the diffusivity of As depends on the rate of indiffusion of Ai and the outdiffusion of selfinterstitials. When a eq eq slow indiffusion of Ai controls the process, Ci Di C I D I holds and the diffusion lim(i) of the FrankTurnbull mechanism noted above. If coefficient is identical to Deff the outdiffusion of selfinterstitials limits the process, the diffusivity becomes [45] 2 lim(I ) ∼ eq Deff = C I /Cseq Cseq /Cs D I (kickout, selfinterstitiallimited), eq
where C I is the local equilibrium concentration of selfinterstitials I and Cs = Cs (r) is the actual local concentration of substitutional impurities As . A simultaneous operation of diffusion mediated by selfinterstitials and vacancies leads for eq eq eq Ci Di (C I D I + C V DV ) to a combined effective diffusivity composed of both lim(I ) lim(V ) parts, i.e. Deff = Deff + Deff . Using such effective diffusivities the diffusion via the various substitutionalinterstitial mechanisms can be described by a single effective process using Fick’s diffusion equation (10.29). Effect of charge: The diffusivity of a point defect Ddefect depends strongly on its charge state. Since defects in semiconductors are usually charged, this property must be included into the terms discussed above. A stable charged point defect must possess an electronic level in the fundamental energy gap [48]. If a charged defect has several charge states, the thermal equilibrium concentrations of the differently charged defects depend on the position of the Fermi level. This feature is related to the dependence of the defect formation energy as illustrated in Fig. 10.6 for some native point defects in GaAs. The substitutionalinterstitial mechanism represents the diffusion of an impuritydefect complex. The interaction of the impurity and the defect depends on the charge state of the defect and the impurity, and so also the diffusivity of the complex. The FrankTurnbull reaction (10.31) of an interstitial impurity Al+ i with charge l+, an with mfold negatively charged vacancy V m− , and a substitutional impurity An− s charge n− reads [45] m− ↔ An− Al+ s + (l − m + n)h. i +V
406
10 Doping, Diffusion, and Contacts
h denotes the holes created or consumed in this reaction due to the charge balance condition, and l, m, n are integers. In compound semiconductors the vacancy is here assumed to be located on the same sublattice in which the substitutional impurity As is dissolved. Charged species were introduced in literature to describe the diffusion − + of Zn in GaAs according to the reaction Zn+ i + VGa ↔ Zns + 2h , and since then the FrankTurnbull process involving charged species is also referred to Longini mechanism [50]. For the kickout mechanism the relation is given by n− m+ + (l − m + n)h. Al+ i ↔ As + I
Diffusivities following from the chargeincluding reactions depend on the supply of the charged defects similar to the reactions without charge discussed above. If the supply of interstitials Ai limits the process, we obtain [45] Cieq (Cseq ) Cs n±l = n + 1 Di eq eq Cs Cs (FrankTurnbull with charged defects, interstitiallimited).
lim(i) Deff
A positive sign in the exponent applies for substitutional acceptors, a negative for substitutional donors. The reaction does not depend on the charge m of the vacancy. The equation accounts for a (possibly) locally varying electron or hole concentration, eq yielding an also locally varying concentration Ci of charged interstitials Al+ i . Similar to the uncharged case the same equation applies to the kickout mechanism when a slow indiffusion of Ai limits the incorporation rate of As . If the incorporation rate of As in the FrankTurnbull process with charged defects is limited by the supply of vacancies, then the effective diffusivity of As impurities is described by [45] eq ±m−n C Veq (Cseq ) Cs = n + 1 DV eq Cs Cs (FrankTurnbull with charged defects, vacancylimited).
lim(V ) Deff
When in the kickout mechanism with charged defects the incorporation of As is limited by the supply of selfinterstitials, the effective diffusivity is analogously given by eq ±m−n−2 C Ieq (Cseq ) Cs = n + 1 DI eq Cs Cs (kickout with charged defects, selfinterstitiallimited).
lim(I ) Deff
If the diffusion coefficient of each charged complex is independent of that of other complexes, the resulting effective diffusion coefficient is given by a linear combination of the diffusivities of all complexes. This leads eventually to an effective diffusion coefficient, which in the general case is composed of the effective diffusion coef
10.2 Diffusion
407
ficients of all defect complexes with all occurring charge states. We abbreviate the notation for effective diffusivities of the two substitutionalinterstitial mechanisms (10.31) and (10.32) by Deff (AV ) for the FrankTurnbull type and Deff (AI ) for the kickout type, and include the various charge states of vacancies V 0 , V − , V 2− , . . . , V + , V 2+ , . . . and the same for selfinterstitials I . We then may write for the general case
z V,max
Deff =
z V,min
z I,max Deff AV z V + Deff AI z I . z I,min
In the sums the charge states of the native defects characterized by the integers z V and z I start at the most negative values z V,min and z I,min occurring in the considered semiconductor, and end at the corresponding most positive values. The relations discussed in this section point up the complexity of diffusion phenomena in semiconductors. A clear description is usually restricted to specific elements and a limited temperature range. Diffusivities of some impurity atoms in silicon are shown in Fig. 10.19. The diffusion coefficients shown in the Arrhenius plot are described by the relation (10.26) and vary over many orders of magnitude. We note the very high diffusivity of the elements moving via the interstitial mechanism (light gray lines, except for O) and the slowly moving substitutional impurities diffusing via the vacancy mechanism or the interstitialcy mechanism (black lines). Such elements are favorable for fabricating stable doping profiles.
10.2.4 Disordering of Heterointerfaces Epitaxial growth procedures have proved their ability to fabricate atomically sharp heterointerfaces. Such interfaces provide strong gradients in the distribution of different atom species and hence a driving force for disordering by diffusion. There may even exist growth conditions which counteract the formation of atomically sharp interfaces. Furthermore, also the preservation of sharp interfaces is important, e.g., during device processing of heterostructures. On the other hand, a welldirected locally enhanced layer disordering was employed for both studying diffusion mechanisms and defining lateral confinement for photons and charge carriers in optoelectronic devices. We consider disordering of heterointerfaces in more detail for Alx Ga1−x Asbased heterostructures to illustrate the effect of experimental conditions on the diffusivity outlined in the previous section. The selfdiffusion of Ga in GaAs was found to be quite low under intrinsic conditions. A similar diffusivity was found for Ga selfdiffusion DGa (n i ) and GaAl interdiffusion DAlGa (n i ) obtained from AlGaAs/GaAs heterostructures, both being
10 Doping, Diffusion, and Contacts
Alx Ga1x As/GaAs QW 12
8
Energy E (meV)
2 1
16
19
Diffusion coefficient D AlGa (10
Fig. 10.20 Energy shift E of the photoluminescence from an Al0.25 Ga0.75 As/GaAs quantum well annealed for 25 h at 825 ◦ C at various values of the As4 ambient pressure (gray squares). The black circles are corresponding calculated diffusion coefficients of the AlGa interdiffusion. Dashed lines are guides to the eye. From [54]
cm s )
408
100 4
0 2 10
60 20 1
10
0
10
1
10
Pressure As4 (atm)
well described by (10.26) with a diffusion constant D0 = 2.9 × 108 cm2 /s and a ∼ fairly high √ activation energy E = 6 eV [53]. Such values correspond to a diffusion length Dt of 1 nm for 30 h diffusion at 1100 K. Since the self and interdiffusion on the Column III sublattice must proceed through native defects of the crystal, the diffusivity depends on the As pressure applied during the annealing at elevated temperature. Pressuredepending interdiffusion coefficients were derived from an evaluation of the photoluminescence energyshift measured for annealed Al0.25 Ga0.75 As/GaAs quantum well samples [54]. The diffusion of Al and Ga across the heterointerfaces of the 13 nm thick quantum well leads to a change of the confinement potential, resulting in a blueshift of the energy levels. Figure 10.20 shows that both, a high and a low As4 ambient pressure applied during annealing leads to an enhanced DAlGa interdiffusion coefficient. The increase of DAlGa is generated by the change of the native defect concentration via the sample surface. Six single pointdefect species may occur in GaAs. A shift of the crystal stoichiometry to the Aspoor side favors the creation of As vacancies VAs , Ga interstitials IGa , and Ga antisites GaAs . Asrich point defects are Ga vacancies VGa , As interstitials IAs , and As antisites AsGa . Corresponding defects apply for Al which occupies the same sublattice as Ga, leading to the more general notation for Column III defects, e.g., Column III vacancies VIII . A consistent description including also Fermilevel effects was obtained by considering the Column III selfdiffusion as being due to neutral and singly ionized Column III vacancies VIII and Column III interstitials IIII [55]. A creation of such a defect pair can occur according to the reaction 0 ↔ IIII + VIII and CIIII CVIII = k1 . The second equation expresses the law of mass action with the concentrations C of the participating defects and a temperaturedependent constant k1 . Under Asrich conditions the crystal surface can act as a sink for the interstitials IIII , thereby increas
10.2 Diffusion
409
ing the concentration of vacancies C VIII . Under Aspoor conditions, evaporation of As at the surface leads to a local excess of Ga atoms, which can diffuse into the crystal and increase the concentration of interstitials C IIII according to the reaction 1 vapor 1/4 0 ↔ IIII + As4 and C IIII PAs4 = k2 . 4 Both VIII and IIII can lead to Column III selfdiffusion, yielding a diffusivity 1/4
−1/4
DIII = c1 C VIII DVIII + c2 C IIII D IIII = c3 PAs4 DVIII + c4 PAs4 D IIII . The ci are constants containing the temperaturedependent constants k j . In the second equation we used the law of mass action involving k2 . The equation describes the trend of the pressuredependent diffusivity shown in Fig. 10.20. Under Aspoor conditions the diffusivity is increased by Column III interstitials IIII , while under Asrich conditions Column III vacancies VIII enhance the diffusivity. The diffusivity is also affected by doping. A shift of the Fermi level from the intrinsic position can increase the selfdiffusion by orders of magnitude. Evidence for a combined effect of doping and ambient pressure on heterointerfaces applied during annealing is given in Fig. 10.21. The TEM images show cross sections of ntype (left, n = 1018 cm−3 ) and ptype (right, p = 8 × 1018 cm−3 ) AlGaAs/GaAs superlattices, which were annealed for 10 h at elevated temperature [56]. The ntype structure shows some interdiffusion for an anneal under Aspoor conditions, and a much stronger layer intermixing in Asrich ambient. In contrast, the ptype structure shows a complete intermixing for Aspoor conditions, while the superlattice remains stable in Asrich ambient. Experiments with compensated doping (i.e., simultaneous doping with donors and acceptors) confirmed that the enhancement of the interdiffusivity is controlled by the position of the Fermi level and not by the presence of impurity atoms [57]. The experimental results point to the participation of charged defects in the effective diffusivity DIII . Their equilibrium concentration depends on their energy position in the bandgap with respect to the Fermi level. Considering only neutral and singly ionized vacancies VIII and interstitials IIII yields for the donorlike interstitials IIII the relation C IIII+ /C IIII0 = exp((E D − E F )/(kB T )), and for the acceptorlike vacancies VIII the ratio C VIII− /C VIII0 = exp((E F − E A )/(kB T )) [55]. The difference of the ionization energy and the Fermi level in the exponential terms represents the energy gain when the native defect is charged, cf. Fig. 10.1 and Sect. 10.1.2. If the Fermi level is decreased by extrinsic ptype doping, the donorlike interstitials IIII are positively charged and attain an increased solubility and corresponding high concentration C IIII+ . In ntype heterostructures the solubility and thereby concentration of acceptorlike − is increased. Introducing respective diffusivities of the charged charged vacancies VIII native defects, the effective diffusion constant for Column III selfdiffusion noted above only for undoped defects is extended and reads [55]
410
10 Doping, Diffusion, and Contacts Al0.4Ga0.6As/GaAs:Si
Al0.4Ga0.6As/GaAs:Mg
002 g 320 Å
as grown
002 g 290 Å
800 °C (10 h) 800 °C (10 h) Aspoor Asrich
as grown
815 °C (10 h) 815 °C (10 h) Aspoor Asrich
Fig. 10.21 Transmissionelectron micrographs of cross sections of Sidoped (left) and a Mgdoped (right) Al0.4 Ga0.6 As/GaAs superlattices. The images show the asgrown structures and the structures after annealing for 10 h under either Aspoor or Asrich conditions. Reproduced with permisc 1988 MRS sion from [56],
1/4 DIII = c5 PAs4 DVIII0 + DVIII− exp (E F − E A )/(kB T ) −1/4 + c6 PAs4 D IIII0 + D IIII+ exp (E D − E F )/(kB T ) . According to this relation the diffusivity increases when ptype AlGaAs heterostructures are annealed in an Aspoor ambient, because both effects increase the concentration of interstitials IIII . The diffusivity increases also when ntype structures are annealed in an Asrich ambient. In this case both effects increase the concentration of vacancies VIII . The effect of the Fermilevel position on the effective diffusivity is more pronounced for multiple charged defects. A cubic dependence of DIII on the electron 3− [53]. concentration, e.g., points to the participation of a triply charged defect VIII A definite assignment to a specific charged defect is difficult though, because both the enthalpy of formation and the enthalpy of migration enter the effective diffusivity, and both quantities change if the charge state of a defect changes due to a shift of the Fermilevel [55]. The spatially selective modification of heterostructure interfaces by layer disordering was also employed for device fabrication. By applying masks on the surface, a laterally selective intermixing of quantumwell heterostructures is obtained. The corresponding change of the bandgap and the refractive index with respect to the not intermixed regions can be used to locally confine charge carriers and photons. If, e.g., a sample containing a quantum well is exposed to intermixing conditions except along a stripe, the lateral regions adjacent to the stripe have a larger bandgap and a lower refractive index. These effects were used to fabricate, e.g., indexguided edgeemitting lasers of III–V [58, 59] and II–VI [60] semiconductors. Techniques employed for selective intermixing comprise impurityinduced layer disordering (IILD) by introducing dopants [61], impurityfree vacancy disordering (IFVD) by supplying vacancies [58], and ionimplantationinduced composition disordering (IID).
10.3 MetalSemiconductor Contact
411
10.3 MetalSemiconductor Contact Any electronic semiconductor device requires an electric contact between the semiconductor and a metal. A metalsemiconductor junction may have either rectifying or ohmic characteristics, depending on the two materials which are brought into contact. The problem is closely related to the band alignment of a semiconductor heterostructure treated in Sect. 4.2. We will introduce the characteristics of a classical ideal metalsemiconductor contact, nonideal effects, and some approaches to fabricate ohmic junctions.
10.3.1 Ideal Schottky Contact We consider a rectifying metalsemiconductor contact in the framework of the model introduced by Schottky [62] and Mott [63]. According to the simple SchottkyMott model the properties of the junction are determined by the work function eφm of the metal and that of the semiconductor eφsc . Since φm may be larger or smaller than φsc and the latter depends on the type of semiconductor (n or p), we have to distinguish four cases. We first consider a metal—ntype semiconductor junction with φm > φsc . Figure 10.22a shows the energyband diagram of the two solids before contact, taking the vacuum level E vac as reference energy. Since the work functions of the metal and the semiconductor differ, electrons will flow from the side with a high Fermi energy to that with a lower Fermi energy for equilibration if a contact is made. The difference φm − φsc is referred to as contact potential. In the case depicted in Fig. 10.22a electrons are transferred to the metal, leaving positively charged donors without a balancing negative charge in the ntype semiconductor. A positive space charge is thereby built up in the interfacenear region of the semiconductor, leading to a bending of the band edges over a width w, which is depleted from free electrons. Outside the depletion layer the semiconductor is neutral. The positive space charge in the semiconductor is balanced by an equal negative charge at the metal surface. The dipole potential equilibrates the contact potential. In thermal equilibrium these quantities are equal and the Fermi energy is constant through the junction. We note from Fig. 10.22b that now a barrier eφBn exists at the junction. The height of this Schottky barrier is given by the band bending eVbi , the socalled builtin potential barrier, and the energy spacing between the Fermi level and the conductionband edge in the semiconductor, eφBn = e(Vbi + φsc − χ ) = e(φm − χ ),
(10.33)
eχ being the electron affinity of the semiconductor as depicted in Fig. 10.22a. Equation (10.33) shows that the builtin potential equals the contact potential,
412
10 Doping, Diffusion, and Contacts
(a) E
(b) E Evac
Evac e
e
sc
Evac
e
Evac Ec EF
m
EF
e
EF
Ev
eVbi
Bn
w
Ec EF Ev
Metal
x Semiconductor
Metal
Semiconductor
x
Fig. 10.22 Energyband diagram of an ideal junction between a metal with a large work function eφm and an ntype semiconductor with a smaller work function eφsc . a Before contact, b in contact without an external bias. eφm and w denote the height of the Schottky barrier and the width of the spacecharge region, respectively. Gray shadings indicate occupied bands
Vbi = φm − φsc . Values of work functions and electron affinities for some solids are given in Table 10.2. The width of the spacecharge region w may be calculated in the SchottkyMott model under the abrupt approximation, i.e., assuming that the charge density in this region is given by the constant concentration of the donors, ρ = en D . Outside the spacecharge region the semiconductor is neutral and ρ = 0. The potential in the semiconductor is obtained from the onedimensional Poisson equation ρ d2V =− , dx2 ε where ε = εr × ε0 is the permittivity. Taking the location of the junction along x and E c in the bulk of the semiconductor as origin, integration leads to V (x) =
1 en D wx − x 2 − Vbi . ε 2
(10.34)
The width of the depletion region w is obtained from the condition V (x = w) = 0, yielding w=
2εVbi en D
1/2 .
(10.35)
In (10.35) we assumed a complete ionization of donors in the spacecharge region and a zero bias across the junction. If the thermal distribution of the majority carriers is taken into account, the charge density ρ = en D is replaced by ρ =
10.3 MetalSemiconductor Contact
413
Table 10.2 Work functions φ m of some metals and electron affinities χ of some semiconductors. Metal data from [64], semiconductors from [65] Metal eφm (eV) Semiconductor eχ (eV) Al Au Ni Pd Pt Ti W
4.28 5.10 5.15 5.12 5.65 4.31 4.54
Ge Si SiC (4H) GaAs InP GaN ZnSe
4.00 4.05 4.05 4.07 4.38 4.10 4.09
en D (1 − exp[eV (x)/(kB T )]). Vbi in (10.35) is then replaced by (Vbi − kB T /e). If an external bias Vext is applied to the metalsemiconductor junction, this quantity is also added. The more complete expression then reads
2ε(Vbi − Vext − kB T /e) 1/2 w= en D (external bias and thermal carrier distribution included).
(10.36)
Application of an external bias Vext such that the semiconductor is negative with respect to the metal (forward bias) lowers the barrier to e(Vbi − Vext − kB T /e), while a reverse bias leaves the barrier eφBn , in this firstorder model, unaffected. The Schottky barrier hence represents an asymmetric resistance for the current across the junction. The junction has a rectifying character, it represents a Schottky diode. The treatment above refers to a metal—ntype semiconductor junction. We now compare the four basic cases of φm > φsc , φm < φsc , and contacts to either an ntype or a ptype semiconductor. If the junction to the ntype semiconductor is made using a metal with a smaller work function φm < φsc , electrons will flow from the metal to the semiconductor for equilibration. In thermal equilibrium (without external bias), when the Fermi energy is constant across the junction, a negative space charge in the semiconductor balances an equal positive charge at the junction in the metal. Figure 10.23b depicts the resulting band bending in the semiconductor. There exits no barrier for an electron flow from the ntype semiconductor to the metal, and a small barrier e(φsc − χ ) for the reverse direction. Such a contact has nearly ohmic character. A comparable case is the metal— ptype semiconductor junction for a larger work function of the metal φm > φsc depicted in Fig. 10.23c. When the contact is made, electrons flow from the semiconductor to the metal to equilibrate the Fermi level E F . The band bending in the semiconductor originating from the space charge of the positively ionized donors is qualitatively similar to the case assumed in Fig. 10.23a, but now there exists no barrier for an electron flow from the metal to the ptype
414
10 Doping, Diffusion, and Contacts
(a) E
m
>
(b) E
sc
m
x
Metal
nSemiconductor
(d) E
sc
m